Crystallography and Crystal Defects Second Edition
Kelly_ffirs.indd i
11/29/2011 4:19:54 PM
Crystallography and Crys...

This content was uploaded by our users and we assume good faith they have the permission to share this book. If you own the copyright to this book and it is wrongfully on our website, we offer a simple DMCA procedure to remove your content from our site. Start by pressing the button below!

Crystallography and Crystal Defects Second Edition

Kelly_ffirs.indd i

11/29/2011 4:19:54 PM

Crystallography and Crystal Defects Second Edition

ANTHONY KELLY Fellow of Churchill College

and

KEVIN M. KNOWLES Fellow of Churchill College

Department of Materials Science and Metallurgy University of Cambridge

Kelly_ffirs.indd iii

11/29/2011 4:19:54 PM

This edition first published 2012 © 2012 John Wiley & Sons, Ltd Registered Office John Wiley & Sons, Ltd, The Atrium, Southern Gate, Chichester, West Sussex, PO19 8SQ, United Kingdom For details of our global editorial offices, for customer services and for information about how to apply for permission to reuse the copyright material in this book please see our website at www.wiley.com. The right of the author to be identified as the author of this work has been asserted in accordance with the Copyright, Designs and Patents Act 1988. All rights reserved. No part of this publication may be reproduced, stored in a retrieval system, or transmitted, in any form or by any means, electronic, mechanical, photocopying, recording or otherwise, except as permitted by the UK Copyright, Designs and Patents Act 1988, without the prior permission of the publisher. Wiley also publishes its books in a variety of electronic formats. Some content that appears in print may not be available in electronic books. Designations used by companies to distinguish their products are often claimed as trademarks. All brand names and product names used in this book are trade names, service marks, trademarks or registered trademarks of their respective owners. The publisher is not associated with any product or vendor mentioned in this book. This publication is designed to provide accurate and authoritative information in regard to the subject matter covered. It is sold on the understanding that the publisher is not engaged in rendering professional services. If professional advice or other expert assistance is required, the services of a competent professional should be sought. The publisher and the author make no representations or warranties with respect to the accuracy or completeness of the contents of this work and specifically disclaim all warranties, including without limitation any implied warranties of fitness for a particular purpose. This work is sold with the understanding that the publisher is not engaged in rendering professional services. The advice and strategies contained herein may not be suitable for every situation. In view of ongoing research, equipment modifications, changes in governmental regulations, and the constant flow of information relating to the use of experimental reagents, equipment, and devices, the reader is urged to review and evaluate the information provided in the package insert or instructions for each chemical, piece of equipment, reagent, or device for, among other things, any changes in the instructions or indication of usage and for added warnings and precautions. The fact that an organization or Website is referred to in this work as a citation and/or a potential source of further information does not mean that the author or the publisher endorses the information the organization or Website may provide or recommendations it may make. Further, readers should be aware that Internet Websites listed in this work may have changed or disappeared between when this work was written and when it is read. No warranty may be created or extended by any promotional statements for this work. Neither the publisher nor the author shall be liable for any damages arising herefrom. Library of Congress Cataloging-in-Publication Data Kelly, A. (Anthony) Crystallography and crystal defects / Anthony Kelly and Kevin M. Knowles. – 2nd ed. p. cm. Includes bibliographical references and index. ISBN 978-0-470-75015-5 (cloth) – ISBN 978-0-470-75014-8 (pbk.) 1. Crystallography. 2. Crystals–Defects. I. Knowles, Kevin M. II. Title. QD931.K4 2012 548′.8–dc23 2011034130 A catalogue record for this book is available from the British Library. HB ISBN: 9780470750155 PB ISBN: 9780470750148 Set in 10/12pt Times by SPi Publisher Services, Pondicherry, India

Kelly_ffirs.indd iv

11/29/2011 4:19:54 PM

Contents Preface to the Second Edition Part I

Perfect Crystals

xiii 1

1 Lattice Geometry 1.1 The Unit Cell 1.2 Lattice Planes and Directions 1.3 The Weiss Zone Law 1.4 Symmetry Elements 1.4.1 Translational Symmetry 1.4.2 Rotational Symmetry 1.4.3 Reflection Symmetry 1.5 Restrictions on Symmetry Elements 1.6 Possible Combinations of Rotational Symmetries 1.7 Crystal Systems 1.8 Space Lattices (Bravais Lattices) Problems Suggestions for Further Reading References

3 3 7 11 14 15 15 16 16 21 26 26 37 40 41

2 Point Groups and Space Groups 2.1 Macroscopic Symmetry Elements 2.2 Orthorhombic System 2.3 Tetragonal System 2.4 Cubic System 2.5 Hexagonal System 2.6 Trigonal System 2.7 Monoclinic System 2.8 Triclinic System 2.9 Special Forms in the Crystal Classes 2.10 Enantiomorphous Crystal Classes 2.11 Laue Groups 2.12 Space Groups 2.13 Nomenclature for Point Groups and Space Groups 2.14 Groups, Subgroups and Supergroups 2.15 An Example of a Three-Dimensional Space Group

43 43 49 52 53 56 59 63 65 67 68 69 69 78 79 79

Kelly_ftoc.indd v

11/14/2011 12:14:28 PM

vi

Contents

Problems Suggestions for Further Reading References

Kelly_ftoc.indd vi

82 84 84

3 Crystal Structures 3.1 Introduction 3.2 Common Metallic Structures – 3.2.1 Cubic Close-Packed (Fm3m) 3.2.2 Hexagonal Close-Packed (P63 /mmc) 3.2.3 Double Hexagonal Close-Packed (P63 /mmc) – 3.2.4 Body-Centred Cubic (Im3m) 3.3 Related Metallic Structures 3.3.1 Indium (I4/mmm) – 3.3.2 Mercury (R3m) 3.3.3 b-Sn (I41/amd) 3.4 Other Elements and Related Compounds – 3.4.1 Diamond (Fd3m) 3.4.2 Graphite (P63 /mmc) 3.4.3 Hexagonal Boron Nitride (P63 /mmc) – 3.4.4 Arsenic, Antimony and Bismuth (R3m) 3.5 Simple MX and MX2 Compounds – 3.5.1 Sodium Chloride, NaCl (Fm3m) – 3.5.2 Caesium Chloride, CsCl (Pm3m) – 3.5.3 Sphalerite, a-ZnS (F43m) 3.5.4 Wurtzite, b-ZnS (P63mc) 3.5.5 Nickel Arsenide, NiAs (P63/mmc) – 3.5.6 Calcium Fluoride, CaF2 (Fm3m) 3.5.7 Rutile, TiO2 (P42/mnm) 3.6 Other Inorganic Compounds – 3.6.1 Perovskite (Pm3m) – – 3.6.2 a-Al2O3 (R3c), FeTiO3 (R3) and LiNbO3 (R3c) – 3.6.3 Spinel (Fd3m), Inverse Spinel and Related Structures – 3.6.4 Garnet (Ia3d) – 3.6.5 Calcite, CaCO3 (R3c) 3.7 Interatomic Distances 3.8 Solid Solutions 3.9 Polymers 3.10 Additional Crystal Structures and their Designation Problems Suggestions for Further Reading References

85 85 86 86 90 92 92 93 93 94 94 95 95 95 97 97 98 98 99 100 101 101 102 103 104 104 105 106 107 109 110 110 113 116 119 121 122

4 Amorphous Materials and Special Types of Crystal–Solid Aggregates 4.1 Introduction 4.2 Amorphous Materials 4.3 Liquid Crystals

123 123 123 126

11/14/2011 12:14:28 PM

Contents

4.4 4.5 4.6 4.7 4.8

4.3.1 Nematic Phases 4.3.2 Cholesteric Phases 4.3.3 Smectic Phases Geometry of Polyhedra Icosahedral Packing Quasicrystals 4.6.1 A Little Recent History and a New Definition Incommensurate Structures Foams, Porous Materials and Cellular Materials Problems Suggestions for Further Reading References

vii

127 129 129 129 134 135 136 137 137 139 139 140

5 Tensors 5.1 Nature of a Tensor 5.2 Transformation of Components of a Vector 5.3 Dummy Suffix Notation 5.4 Transformation of Components of a Second-Rank Tensor 5.5 Definition of a Tensor of the Second Rank 5.6 Tensor of the Second Rank Referred to Principal Axes 5.7 Limitations Imposed by Crystal Symmetry for Second-Rank Tensors 5.8 Representation Quadric 5.9 Radius–Normal Property of the Representation Quadric 5.10 Third- and Fourth-Rank Tensors Problems Suggestions for Further Reading References

141 141 142 145 146 148 149 153 155 159 161 161 163 163

6 Strain, Stress, Piezoelectricity and Elasticity 6.1 Strain: Introduction 6.2 Infinitesimal Strain 6.3 Stress 6.4 Piezoelectricity 6.4.1 Class 2 6.4.2 Class 222 6.4.3 Class 23 6.4.4 Class 432 6.4.5 The Converse Effect 6.5 Elasticity of Crystals – 6.5.1 Class 1 6.5.2 Class 2 6.5.3 Class 222 6.5.4 Class 23 Problems Suggestions for Further Reading References

165 165 166 170 177 179 179 180 180 181 181 184 185 185 186 193 196 196

Kelly_ftoc.indd vii

11/14/2011 12:14:28 PM

viii

Contents

Part II

Imperfect Crystals

7 Glide and Texture 7.1 Translation Glide 7.2 Glide Elements 7.3 Independent Slip Systems 7.4 Large Strains of Single Crystals: The Choice of Glide System 7.5 Large Strains: The Change in the Orientation of the Lattice During Glide 7.6 Texture Problems Suggestions for Further Reading References

199 199 203 208 218

8 Dislocations 8.1 Introduction 8.2 Dislocation Motion 8.3 The Force on a Dislocation 8.4 The Distortion in a Dislocated Crystal 8.5 Atom Positions Close to a Dislocation 8.6 The Interaction of Dislocations with One Another Problems Suggestions for Further Reading References

241 241 247 249 253 258 261 265 266 267

9 Dislocations in Crystals 9.1 The Strain Energy of a Dislocation 9.2 Stacking Faults and Partial Dislocations 9.3 Dislocations in C.C.P. Metals 9.4 Dislocations in the Rock Salt Structure 9.5 Dislocations in Hexagonal Metals 9.6 Dislocations in B.C.C. Crystals 9.7 Dislocations in Some Covalent Solids 9.8 Dislocations in Other Crystal Structures Problems Suggestions for Further Reading References

269 269 277 280 288 290 295 297 301 301 303 303

10 Point Defects 10.1 Introduction 10.2 Point Defects in Ionic Crystals 10.3 Point Defect Aggregates 10.4 Point Defect Configurations 10.5 Experiments on Point Defects in Equilibrium 10.6 Experiments on Quenched Metals 10.7 Radiation Damage

Kelly_ftoc.indd viii

197

222 228 235 237 237

305 305 309 310 312 317 321 324

11/14/2011 12:14:28 PM

Contents

10.8

Anelasticity and Point Defect Symmetry Problems Suggestions for Further Reading References

ix

326 329 331 331

11

Twinning 11.1 Introduction 11.2 Description of Deformation Twinning 11.3 Examples of Twin Structures 11.3.1 C.C.P. Metals 11.3.2 B.C.C. Metals 11.3.3 Sphalerite (Zinc Blende) 11.3.4 Calcite 11.3.5 Hexagonal Metals 11.3.6 Graphite 11.4 Twinning Elements 11.5 The Morphology of Deformation Twinning Problems Suggestions for Further Reading References

335 335 337 342 342 342 344 345 346 346 350 354 358 360 360

12

Martensitic Transformations 12.1 Introduction 12.2 General Crystallographic Features 12.3 Transformation in Cobalt 12.4 Transformation in Zirconium 12.5 Transformation of Indium–Thallium Alloys 12.6 Transformations in Steels 12.7 Transformations in Copper Alloys 12.8 Transformations in Ni–Ti-Based Alloys 12.9 Transformations in Nonmetals 12.10 Crystallographic Aspects of Nucleation and Growth Problems Suggestions for Further Reading References

363 363 364 366 369 374 379 382 383 384 385 387 388 389

13

Crystal Interfaces 13.1 The Structure of Surfaces and Surface Free Energy 13.2 Structure and Energy of Grain Boundaries 13.3 Interface Junctions 13.4 The Shapes of Crystals and Grains 13.5 Boundaries between Different Phases 13.6 Strained Layer Epitaxy of Semiconductors Problems Suggestions for Further Reading References

391 391 397 409 414 420 424 429 431 431

Kelly_ftoc.indd ix

11/14/2011 12:14:28 PM

x

Kelly_ftoc.indd x

Contents

Appendix 1 Crystallographic Calculations A1.1 Vector Algebra A1.1.1 The Scalar Product A1.1.2 The Vector Product A1.2 The Reciprocal Lattice A1.3 Matrices A1.4 Rotation Matrices and Unit Quaternions References

435 435 436 438 440 443 448 449

Appendix 2 The Stereographic Projection A2.1 Principles A2.2 Constructions A2.2.1 To Construct a Small Circle A2.2.2 To Find the Opposite of a Pole A2.2.3 To Draw a Great Circle through Two Poles A2.2.4 To Find the Pole of a Great Circle A2.2.5 To Measure the Angle between two Poles on an inclined Great Circle A2.3 Constructions with the Wulff Net A2.3.1 Two-Surface Analysis A2.4 Proof of the Properties of the Stereographic Projection References

451 451 455 455 458 458 459

Appendix 3 Interplanar Spacings and Interplanar Angles A3.1 Interplanar Spacings A3.1.1 Triclinic A3.1.2 Monoclinic A3.1.3 Orthorhombic A3.1.4 Trigonal A3.1.5 Tetragonal A3.1.6 Hexagonal A3.1.7 Cubic A3.2 Interplanar Angles A3.2.1 Orthorhombic A3.2.2 Hexagonal A3.2.3 Cubic

469 469 470 470 470 471 471 471 471 472 472 472 472

Appendix 4 Transformation of Indices Following a Change of Unit Cell A4.1 Change of Indices of Directions A4.2 Change of Indices of Planes A4.3 Example 1: Interchange of Hexagonal and Orthorhombic Indices for Hexagonal Crystals A4.4 Example 2: Interchange of Rhombohedral and Hexagonal Indices

473 473 475

460 460 464 465 468

476 477

11/14/2011 12:14:29 PM

Contents

Appendix 5 Slip Systems in C.C.P. and B.C.C. Crystals A5.1 Independent Glide Systems in C.C.P. Metals – A5.1.1 Example: Slip Along [110] on the (111) Slip Plane A5.1.2 Number of Independent Glide Systems A5.2 Diehl’s Rule and the OILS Rule – A5.2.1 Use of Diehl’s Rule for {111} Slip (Such as C.C.P. Metals) – A5.2.2 Use of Diehl’s Rule for {110} Slip (Such as B.C.C. Metals) A5.2.3 The OILS Rule A5.3 Proof of Diehl’s Rule and the OILS Rule References

xi

481 481 481 482 483 484 484 484 485 486

Appendix 6 Homogeneous Strain A6.1 Simple Extension A6.2 Simple Shear A6.3 Pure Shear A6.4 The Relationship between Pure Shear and Simple Shear

487 488 488 489 489

Appendix 7 Crystal Structure Data A7.1 Crystal Structures of the Elements, Interatomic Distances and Six-Fold Coordination-Number Ionic Radii A7.2 Crystals with the Sodium Chloride Structure A7.3 Crystals with the Caesium Chloride Structure A7.4 Crystals with the Sphalerite Structure A7.5 Crystals with the Wurtzite Structure A7.6 Crystals with the Nickel Arsenide Structure A7.7 Crystals with the Fluorite Structure A7.8 Crystals with the Rutile Structure

491 491 495 496 497 497 497 498 498

Appendix 8 Further Resources A8.1 Useful Web Sites A8.2 Computer Software Packages

499 499 499

Brief Solutions to Selected Problems

501

Index

509

Kelly_ftoc.indd xi

11/14/2011 12:14:29 PM

Preface to the Second Edition This fully revised and updated edition has been prepared by a very active worker in the field, who has used previous editions extensively both in teaching and in research, together with one of the original authors. Since the first edition, written in the late 1960s, understanding of crystal defects such as dislocations, stacking faults, twin, grain and interphase boundaries and of their effect on the mechanical and electrical properties of materials has grown enormously and has been accompanied by a total change in style of the way in which both research and teaching are carried out through the use of the fast digital computer. This edition takes account of this change. It provides a fully updated account of basic crystallography and of structural imperfections in materials, while ensuring that it remains accessible to both undergraduate and postgraduate students and to others wishing to have a basic understanding of crystallography and why this subject is important when dealing with real (i.e. imperfect) materials. This edition has discussions of a number of new topics not covered in previous editions such as piezoelectricity, groups, subgroups and supergroups, liquid crystals, incommensurate materials and the structure of foamed and amorphous materials, and martensitic transformations in nickel–titanium shape memory alloys and zirconia ceramics. The topic of quasicrystalline materials, covered briefly in the revised edition published in 2000, has been rewritten and linked to discussions of icosahedral packing and the understanding of topologically close-packed structures. Constructions involving the stereographic projection have been moved to an appendix. It is now usual to produce stereographic projections via proprietary software packages. Accounts of three-dimensional coordinate geometry and spherical trigonometry have been rewritten using vector algebra, matrix algebra and quaternions. Such algebra is also amenable to the use of spreadsheets. Tables of data and references in previous editions have been meticulously checked and updated. Numbered references are listed in full at the end of each chapter, together with suggestions for further reading. The problems at the end of each chapter have been reviewed and updated. Brief solutions to these are given after the appendices. More detailed worked solutions are available on the password protected Wiley Web page accompanying this book at http://booksupport.wiley.com. Lists of websites and computer software packages relevant to the topics we have covered here are given in a new appendix. The authors are extremely grateful to those who have helped to foster our interest in crystallography. AK would like to thank in particular the late Geoffrey Groves, co-author of the first edition, as well as Patricia Kidd, co-author of the revised edition published in 2000; KMK would like to thank the late David Smith, his DPhil supervisor at Oxford, and also a former PhD student of AK.

Kelly_fpref.indd xiii

11/29/2011 3:40:26 PM

xiv

Preface

We are both grateful to James Elliott for his great help with preparing diagrams of polymer crystals and to other colleagues from both of our departments at Cambridge and at Churchill College, Cambridge for their advice and encouragement. In attempting to strike a balance between general background knowledge, specialist research knowledge and succinctness of description, we have inevitably had to make compromises in every chapter; each could have been a separate volume. We hope the reader whose understanding of crystallography and crystal defects goes well beyond what we have described here will nevertheless find parts where we have enriched his or her knowledge. Finally, we hope that all readers will enjoy reading this book as much as we have enjoyed both its writing and its revision. Anthony Kelly Kevin M. Knowles

Kelly_fpref.indd xiv

11/29/2011 3:40:27 PM

Part I Perfect Crystals

Kelly_p01.indd 1

11/29/2011 4:12:52 PM

1 Lattice Geometry

1.1 The Unit Cell Crystals are solid materials in which the atoms are regularly arranged with respect to one another. This regularity of arrangement can be described in terms of symmetry elements; these elements determine the symmetry of the physical properties of a crystal. For example, the symmetry elements show in which directions the electrical resistance of a crystal will be the same. Many naturally occurring crystals, such as halite (sodium chloride), quartz (silica) and calcite (calcium carbonate), have very well-developed external faces. These faces show regular arrangements at a macroscopic level, which indicate the regular arrangements of the atoms at an atomic level. Historically, such crystals are of great importance because the laws of crystal symmetry were deduced from measurements of the interfacial angles in them; measurements were first carried out in the seventeenth century. Even today, the study of such crystals still possesses some heuristic advantages in learning about symmetry. Nowadays the atomic pattern within a crystal can be studied directly by techniques such as high-resolution transmission electron microscopy. This atomic pattern is the fundamental pattern described by the symmetry elements and we shall begin with it. In a crystal of graphite the carbon atoms are joined together in sheets. These sheets are only loosely bound to one another by van der Waals forces. A single sheet of such atoms provides an example of a two-dimensional crystal; indeed, recent research has shown that such sheets can actually be isolated and their properties examined. These single sheets are now termed ‘graphene’. The arrangement of the atoms within a sheet of graphene is shown in Figure 1.1a. In this representation of the atomic pattern, the centre of each atom is represented by a small dot, and lines joining adjacent dots represent bonds between atoms. All of the atoms in this sheet are identical. Each atom possesses three nearest neighbours. Crystallography and Crystal Defects, Second Edition. Anthony Kelly and Kevin M. Knowles. © 2012 John Wiley & Sons, Ltd. Published 2012 by John Wiley & Sons, Ltd.

Kelly_c01.indd 3

11/30/2011 6:13:52 PM

4

Crystallography and Crystal Defects (a)

(b)

S R y

M

Y O´

O N

A

P

B

H

X Q

x

T

(c)

y b g a

x

Figure 1.1

We describe this by saying that the coordination number is 3. In this case the coordination number is the same for all the atoms. It is the same for the two atoms marked A and B. However, atoms A and B have different environments: the orientation of the neighbours is different at A and B. Atoms in a similar situation to those at A are found at N and Q; there is a similar situation to B at M and at P. It is obvious that we can describe the whole arrangement of atoms and interatomic bonds shown in Figure 1.1a by choosing a small unit such as OXAY, describing the arrangement of the atoms and bonds within it, then moving the unit so that it occupies the position NQXO and repeating the description and then moving it to ROYS and so on, until we have

Kelly_c01.indd 4

11/30/2011 6:13:53 PM

Lattice Geometry

5

filled all space with identical units and described the whole pattern. If the repetition of the unit is understood to occur automatically, then to describe the crystal we need only describe the arrangement of the atoms and interatomic bonds within one unit. The unit chosen we would call the ‘unit parallelogram’ in two dimensions (in three dimensions, the ‘unit cell’). In choosing the unit we always choose a parallelogram in two dimensions or a parallelepiped in three dimensions. The reason for this will become clear later. Having chosen the unit, we describe the positions of the atoms inside it by choosing an origin O and taking axes Ox and Oy parallel to the sides, so that the angle between Ox and Oy is ≥ 90°. We state the lengths of the sides a and b, taking a equal to the distance OX and b equal to the distance OY (Figure 1.1a), and we give the angle g between Ox and Oy. In this case a = b = 2.45 Å1 (at 25 °C) and g = 120°. To describe the positions of the atoms within the unit parallelogram, we note that there is one at each corner and one wholly inside the cell. The atoms at O, X, A, Y all have identical surroundings.2 In describing the positions of the atoms we take the sides of the parallelogram, a and b, as units of length. Then the coordinates of the atom at O are (0, 0); those at X (1, 0); those at Y (0, 1); and those at A (1, 1). The coordinates of the atom at O′ are obtained by drawing lines through O′ parallel to the axes Ox and Oy. The coordinates of O′ are therefore 13 , 23 . To describe the contents fully inside the unit parallelogram – that is, to describe the positions of the atoms – we need only give the coordinates of the atom at the origin, (0, 0), and those of the atom at O′. The reason is that the atoms at X, A and Y have identical surroundings to those at O and an atom such as O, X, A or Y is shared between the four cells meeting at these points. The number of atoms contained within the area OXAY is two. O′ is within the area, giving one atom. O, Y, A, X provide four atoms each shared between four unit cells, giving an additional 4 × 14 = 1. A second way of arriving at the same result is to move the origin of the unit cell slightly away from the centre of the atom at O so that the coordinate of the O atom is (ε1, ε2) and the coordinate of the O′ atom is 13 + ε1 , 23 + ε 2 , where 0 < ε1, ε2 90°. Close examination of the proposed structure shows that it has a monoclinic I lattice. Specify a more conventional description of the lattice type and describe the relationship of the sides of the unit cell for this new lattice type in terms of the monoclinic I unit cell.

Kelly_c01.indd 38

11/30/2011 6:15:23 PM

Lattice Geometry

39

1.5 The spinel MgAl2O4 has a = b = c = 8.11 Å and a = b = g = 90°. Crystals show – – – ––– the faces (111), (111), (111) and (111) and the faces parallel to these, namely (11 1), –– – – –– (111 ), (111) and (1 1 1 1). Such crystals look like regular or distorted octahedra. –– (a) Find the zone axis symbol (indices) of the zone containing (111) and (1 1 1). Which of the other faces listed above also lie in this zone? –– (b) Show that the zone containing (111) and (11 1) also contains (001) and (110). (c) Sketch the projection of the lattice on (001). Draw in the trace of the (110) lattice plane and the normal to the plane through the origin. Find the perpendicular distance of the first plane of this set from the origin in terms of the cell side. (d) Draw the section of the lattice through the origin which contains the normal to (110) and the normal to (001). Mark in on this section the traces of the (111), –– ––– – (11 1), (11 1) and (111) planes. Measure the angles between adjacent planes. 1.6 Find the angle between [111] and the normal to (111) in (a) a cubic crystal and (b) a tetragonal one with a = 5.67 Å, c = 12.70 Å. – 1.7 Show that the faces (111), (231) and (12 4) all lie in a zone. (a) Find the zone symbol (indices) of this zone and (b) calculate the angle between this zone and the zone [100] in the cubic system. –– 1.8 In a tetragonal crystal CuFeS2, the angle between (111) and (11 1) is 108.67°. Calculate (a) the ratio of the axial lengths and (b) the interzone angle [236]∧[001]. 1.9 Following the method of Section 1.6, determine the angles between the rotational axes in the axial combinations of (a) two triads and a diad and (b) a tetrad, a triad and a diad. Draw a sketch to show the arrangement of the symmetry elements in each case. 1.10 Show that (a) successive combinations of rotations about two different tetrad axes are unable to be expressed as a rotation about a single triad axis in crystals, and (b) successive combinations of rotations about two different triad axes are unable to be expressed as a rotation about a single tetrad axis in crystals. 1.11 The unit cell of a two-dimensional lattice has a = b, g = 120°. Dispose three atoms about each lattice point in different ways so that the two-dimensional crystal can show the following symmetries in turn: (a) a six-fold axis with mirror planes parallel to it, (b) a three-fold axis, (c) a diad axis at the intersection of two mirror planes, (d) a two-fold axis and (e) a one-fold axis. 1.12 CdI2 and CdCl2 both belong to the trigonal crystal system. The former has a primitive hexagonal lattice and the latter a rhombohedral lattice. The coordinates of the atoms associated with each lattice point are given below, using a hexagonal unit cell for both crystals: CdI 2 Cd: 0, 0, 0 I: ±

(

2 1 1 3 3 4

, ,

)

CdCl 2 Cd: 0, 0, 0 Cl: ±

( 23 , 13 , 121 )

Draw plans of the two structures on (001) and outline on your diagram for CdCl2 the projections of the cell edges of the true rhombohedral primitive unit cell.

Kelly_c01.indd 39

11/30/2011 6:15:32 PM

40

Crystallography and Crystal Defects

1.13 Show that there are three cubic lattices by following the procedure used in Section 1.8 and finding the conditions for which in Figure 1.28 triad axes lie normal to (010), (100) and (001) of the rhombohedral primitive unit cell. Hint: find the condition under which successive planes project along their normal so that the lattice points in one lie at the centroids of triangles of lattice points in that below it. 1.14 A two-dimensional crystal possesses four-fold rotational symmetry. Sketch the net. Position four atoms of an element at the net points so that the arrangement is consistent with (a) just four-fold symmetry and (b) four-fold symmetry with mirror planes parallel to the four-fold symmetry axis. Are two different arrangements of mirror planes possible in (b)? 1.15 Specify the directions of a*, b* and c* in a hexagonal crystal relative to the lattice vectors a, b and c. What is the angle between a* and b*? Determine the magnitudes of a*, b* and c* in terms of the lattice parameters a and c. Using the formula |t*hkℓ| = 1/dhkℓ, show that the interplanar spacing of the hkl planes in an hexagonal crystal is given by the formula: 1 dhk 2

= (h2 + k 2 + hk )

4 3a 2

+

l2 c2

Hence show that the planes (hkl), (h,−(h+k),l) and (k,−(h+k),l) have the same interplanar spacing. 1.16 Show that in a triclinic crystal the vector [uvw] is parallel to the normal to the plane (hkl) if: ⎛ h⎞ ⎛ a 2 ab cos γ ⎜ ⎟ ⎜ b2 ⎜ k ⎟ = ⎜ ab cos γ ⎜ ⎟ ⎜ ⎜⎝ l ⎟⎠ ⎝ ac cos β bc cos α

ac cos β ⎞ ⎟ bc cos α ⎟ c 2 ⎟⎠

⎛ u⎞ ⎜ ⎟ ⎜ v⎟ ⎜ ⎟ ⎜⎝ w⎟⎠

Determine u, v and w in terms of h, k, l, a, b and g . Hint: it is useful to define an orthonormal set of vectors with respect to which the basis vectors a, b and c of the triclinic crystal are defined. 1.17 Using the hint in Problem 1.16, or otherwise, confirm that the volume, V, of the unit cell of a triclinic crystal with cell dimensions a, b, c, a, b and γ is given by the formula: V = abc 1 − cos2 α − cos2 β − cos2 γ + 2 cos α cos β cos γ

Suggestions for Further Reading S.M. Allen and E.L. Thomas (1999) The Structure of Materials, John Wiley and Sons, New York. M.J. Buerger (1963) Elementary Crystallography, John Wiley and Sons, New York. M.J. Buerger (1970) Contemporary Crystallography, McGraw-Hill, New York.

Kelly_c01.indd 40

11/30/2011 6:15:33 PM

Lattice Geometry

41

C. Giacovazzo (ed.) (2011) Fundamentals of Crystallography (International Union of Crystallography Texts on Crystallography – 15), 3rd Edition, Oxford University Press, Oxford. C. Hammond (2009) The Basics of Crystallography and Diffraction (International Union of Crystallography Texts on Crystallography – 12), 3rd Edition, Oxford University Press, Oxford. F.C. Phillips (1971) Introduction to Crystallography, 4th Edition, Oliver & Boyd, Edinburgh. J.-J. Rousseau (1998) Basic Crystallography, John Wiley and Sons, Chichester.

References [1] M.J. Buerger (1963) Elementary Crystallography, John Wiley and Sons, New York, pp. 35–45. [2] M.J. Buerger (1970) Contemporary Crystallography, McGraw-Hill, New York, pp. 24–27. [3] H. Grimmer (1974) Disorientations and coincidence rotations for cubic lattices, Acta Crystall. A, 30, 685–688. [4] S.L. Altmann (1986) Rotations, Quaternions and Double Groups, Clarendon Press, Oxford. [5] J.B. Kuipers (1999) Quaternions and Rotation Sequences, Princeton University Press, Princeton. [6] T. Hahn and A. Looijenga-Vos (2002) International Tables for Crystallography (ed. Theo Hahn), 5th, Revised Edition, Vol. A: Space-Group Symmetry, published for the International Union of Crystallography by Kluwer Academic Publishers, Dordrecht, pp. 14–16.

Kelly_c01.indd 41

11/30/2011 6:15:37 PM

2 Point Groups and Space Groups 2.1

Macroscopic Symmetry Elements

The macroscopically measured properties of a crystal, such as electrical resistance, thermal expansion, optical properties, magnetic susceptibility and the elastic constants, show a symmetry which can be defined and understood without reference to the translational symmetry elements defined by the lattice. If the translational symmetry of the crystal is disregarded, the remaining symmetry elements (such as axes of rotational symmetry, mirror planes and any centre of inversion), themselves consistent with the translational symmetry of the lattice, can be arranged into 32 consistent groups. These are the 32 crystallographic point groups. They are so called because they are consistent with translational symmetry and because all of the symmetry elements in a group pass through a single point and the operation of these elements leaves just one point unmoved – the point through which they pass. Other point groups, such as the point group symmetry of the icosahedron, which we shall consider in Chapter 4 when discussing the point group symmetries exhibited by quasicrystals, are not compatible with translational symmetry. The axes of rotational symmetry, the mirror plane and the centre of inversion are all called macroscopic symmetry elements because their presence or absence in a given crystal can be decided in principle by macroscopic tests, such as etching of the crystal, the arrangement of the external faces or the symmetry of the physical properties, without any reference to the atomic structure of the crystal. The macroscopic symmetry elements are of two kinds. A symmetry operation of the first kind, such as a pure rotation axis, when operating on a righthanded object (say) produces a right-handed object from it, and all subsequent repetitions of this object are also right-handed. A symmetry operation of the second kind repeats an enantiomorphous object from an original object. The left and right hands of the ideal external form of the human body are enantiomorphously related. The operation of reflection illustrated in Figure 1.12 is an example of a symmetry operation of the second kind since a left-handed object is repeated from an original right-handed object. Subsequent operation of the same Crystallography and Crystal Defects, Second Edition. Anthony Kelly and Kevin M. Knowles. © 2012 John Wiley & Sons, Ltd. Published 2012 by John Wiley & Sons, Ltd.

Kelly_c02.indd 43

11/30/2011 7:32:17 PM

44

Crystallography and Crystal Defects

3⫻

2p 4

2⫻ 3

2p 4

2 4

1 2p 4⫻ 4

2p 4

Figure 2.1

1

2

3

4

6

Figure 2.2

symmetry element would produce a right-handed object again and then a left-handed object, and so forth. A symmetry operation of the second kind thus involves a reversal of sense in the operation of repetition. Inversion through a centre is also an operation of the second kind. In developing the 32 crystallographic point groups it is convenient to have all the macroscopic symmetry elements represented by axes and to do this we define what are called improper rotations. These produce repetition by a combination of a rotation and an operation of inversion. We shall use rotoinversion axes. These involve rotation coupled with inversion through a centre.1 A pure rotation axis is said to produce a proper rotation. The basic operation of repetition by a rotation axis is shown schematically in Figure 2.1. An n-fold axis repeats an object by successive rotations through an angle of 2p/n. In the example shown in Figure 2.1, the axis is one of four-fold symmetry. The operation of monad, diad, triad, tetrad and hexad pure rotation axes on a single initial pole is shown in Figure 2.2. These diagrams are stereograms (see Appendix 2) with the pole of the axis at 1 It is also possible to use rotoreflection axes [1], pp. 23–30, also termed alternating axes [2], p. 117, in developing the point groups. These repeat an object by rotation coupled with reflection in a plane normal to the axis. One-fold, two-fold, three-fold, ~ ~ ~ ~ ~ ~ four-fold and six-fold rotoreflection axes are possible, usually denoted 1 (pronounced ‘one tilde’), 2 , 3 , 4 and 6 respectively. 1 is clearly equivalent to a mirror plane.

Kelly_c02.indd 44

11/30/2011 7:32:18 PM

Point Groups and Space Groups (a)

(b)

m

45

(c)

m

Centre

Figure 2.3

Figure 2.4

1 (≡ centre)

2 (≡ m)

3 (≡ 3 plus centre)

4

6 (≡ 3 m)

Figure 2.5

the centre of the primitive circle. Dots are used to represent poles in the northern hemisphere of projection related to one another by the rotation axis. The numbers below the stereograms give the shorthand labels for the axes 1, 2, 3, 4 and 6, indicating a one-fold, two-fold, three-fold, four-fold and six-fold axis, respectively. The repetition of an object by a mirror plane, symbol m, and by a centre of symmetry (or centre of inversion) is shown in Figure 2.3. In Figure 2.3a the mirror plane lies normal to the primitive circle. It is denoted by a strong vertical line | coinciding with the mirror in the stereographic projection. In Figure 2.3b the mirror coincides with the primitive; the dot representing the pole in the northern hemisphere has as its mirror image the circle shown in the southern hemisphere. In Figure 2.3c the centre of inversion is at the centre of the sphere of projection. The one-fold inversion axis is a centre of symmetry. The operation of the other rotoinversion axes is explained in Figures 2.4 and 2.5. The twofold rotation–inversion axis 2¯ shown

Kelly_c02.indd 45

11/30/2011 7:32:18 PM

46

Crystallography and Crystal Defects The 32 three-dimensional point groups Triclinic

Monoclinic (1st setting)

Tetragonal

X 1

2

4

m ( = 2)

4

2 ⁄m

4 ⁄m

X (even)

X (even) plus centre and

X (odd)

1 Monoclinic (2nd setting)

Orthorhombic

2

222

422

m

2mm

4mm

X2

Xm

X2 (even) or

Xm (even)

42m

X2 or

Xm plus centre and

Xm (odd)

2 ⁄m

mmm

4 ⁄mmm

Figure 2.6 Stereograms of the poles of equivalent general directions and of the symmetry elements of each of the 32 point groups. The z-axis is normal to the paper. (Taken from the International Tables for X-ray Crystallography, Vol. 1 [4] and adapted to conform to current notation for the two centrosymmetric point groups in the cubic crystal system.)

Kelly_c02.indd 46

11/30/2011 7:32:19 PM

Point Groups and Space Groups Trigonal

Hexagonal

47

Cubic

X 3

6

23

X

(even)

6 X

(even) plus centre and

3

X

6 ⁄m

m3

(odd)

X2 32

622

432

Xm 3m

6mm X2

(even)

or Xm

6m2

43m

(even)

X2 or

Xm

plus centre and

3m

6 ⁄mmm

Figure 2.6

Kelly_c02.indd 47

m3m

Xm

(odd)

(continued)

11/30/2011 7:32:19 PM

48

Crystallography and Crystal Defects

in Figure 2.4 repeats an object by rotation through 180° (360°/2) to give the dotted circle, – followed by inversion to give the full circle. Similarly, the threefold inversion axis 3 involves rotation through 360°/3 = 120° coupled with an inversion. In general, an n-fold rotoinversion axis n– involves rotation through an angle of 2p/n coupled with inversion through a centre. The rotation and inversion are both part of the operation of repetition and must not be considered as separate operations. The operation of the various rotoinversion axes that can occur in crystals on a single initial pole is shown in Figure 2.5, with the pole of the rotoinversion axis at the centre of the primitive circle. The following symbols are – – – used: inversion monad, 1, symbol ; inversion diad, 2, symbol ; inversion triad, 3, – – symbol ; inversion tetrad, 4 , symbol ; inversion hexad, 6, symbol . Inspection of – – Figures 2.2–2.4 shows that 1 is identical to a centre of symmetry, 2 is identical to a mirror – plane normal to the inversion diad, 3 is identical to a triad axis plus a centre of symmetry – and 6 is identical to a triad axis normal to a mirror plane (symbol 3/m, the sign ‘/m’ indicat– ing a mirror plane normal to an axis of symmetry).2 Only 4 is unique. The operation of – repetition described by 4 cannot be reproduced by any combination of a proper rotation axis and a mirror plane or a centre of symmetry. – – – – The various different combinations of 1, 2, 3, 4 and 6 pure rotation axes and 1, 2, 3, 4 and – 6 rotoinversion axes constitute the 32 point groups or crystal classes. These 32 classes are grouped into systems according to the presence of defining symmetry elements (see Table 1.3). Stereograms of each of the 32 point groups or crystal classes are given in Figure 2.6, following the current conventions of the International Tables for Crystallography [3]. With the exception of the two triclinic point groups, each point group is depicted by two stereograms. The first stereogram shows how a single initial pole is repeated by the operations of the point group and the second stereogram shows all of the symmetry elements present. The nomenclature for describing the crystal classes is as follows. X indicates a rotation axis – and X an inversion axis. X/m is a rotation axis normal to a mirror plane, Xm a rotation axis with a mirror plane parallel to it and X2 a rotation axis with a diad normal to it. X/mm indi– cates a rotation axis with a mirror plane normal to it and another parallel to it. Xm is an inversion axis with a parallel plane of symmetry. A plane of symmetry is an alternative description of a mirror plane. We shall describe each of the classes in Sections 2.2–2.8. A derivation of the 32 classes follows by noting from Sections 1.5 and 1.6 that the rotation axes consistent with translational symmetry are 1, 2, 3, 4 and 6. Individually, these give in total five crystal classes. Their consistent combinations give another six (see Table 1.2): 222, 322, 422, 622, 332 and 432, thus totalling 11. All of these 11 involve only operations of the first kind. A lattice is inherently centrosymmetric (Section 1.4) and so each of the rotation axes could be replaced by the corresponding rotoinversion axis, thus giving another five – – – – – classes: 1, 2, 3, 4 and 6. The remaining sixteen can be described as combinations of the proper and improper rotation axes. It is convenient to begin first with the three crystal systems where the angles between the axes are all 90°, then to consider the hexagonal and trigonal crystal systems, before finally turning our attention to the monoclinic and triclinic systems.

2

Our symbols are identical to those used in the International Tables for Crystallography [3], with the exception of ‘ ’, which in the International Tables is always indicated by the symbol for a mirror plane.

Kelly_c02.indd 48

11/30/2011 7:32:19 PM

Point Groups and Space Groups

2.2

49

Orthorhombic System

A crystal in this system contains three diads, which must be at right angles to one another. In Figure 2.6 they are the crystal axes. From Table 1.3 and Figures 1.19d–g, the lattice parameters may be all unequal. The point group containing just three diad axes at right angles is shown in Figure 2.6 and is designated 222. In general, a pole in a crystal belonging to this point group is repeated four times. If the indices of the initial pole are (hkl), where there is no special relationship between h, k and l, the operation of all of the symmetry elements of the point group on this –– –– –– one initial pole produces three other poles. These are (h k l), (hk l ) and (h kl ) (Figure 2.7). The assemblage of crystal faces produced by repetition of an initial crystal face with indices (hkl) is called the form hkl and is given the symbol {hkl}.3 If the assemblage of faces encloses space, the form is said to be closed; otherwise it is open. In this case {hkl} is closed. The symbol {hkl} with curly brackets means all faces of the form hkl, in this case, –– –– – – for the point group 222, (hkl), (h k l), (hk l ) and (h kl ). The form {hkl} is said to show a multiplicity of four. Then {hkl} would be said to be a general form; that is, a form that bears no special relationship to the symmetry elements of the point group. Special forms in this crystal class would be {100}, {010} and {001}; each of these forms – gives just two faces: for {100}, these would be the faces (100) and (1 0 0) (Figure 2.7). These forms are all open ones. They are easily recognized as special forms since their mul– 100 – hk0

––

hk0

––

– – – h0l h0l

hkl

– 010

– 0kl

–– hkl

001

z

–– 0kl

0kl – 0kl

– 001

––

hkl

h0l

– h0l

– hk0

010

y

hkl

hk0 100 x

Figure 2.7 A stereogram of an orthorhombic crystal of point group 222 centred on 001. The diad axes are parallel to the x-, y- and z-axes. 3

All the individual faces of the form {hkl} are crystallographically identical. In a similar way, if a single direction is given, say [uvw], then all the directions produced if the repetition operations of the point group are carried out on the initial direction are called the family of directions of the type uvw and are given the symbol 〈uvw〉.

Kelly_c02.indd 49

11/30/2011 7:32:20 PM

50

Crystallography and Crystal Defects

tiplicity is less than that of the general form. Forms such as {hk0}, {h0l} and {0kl} which have one index zero and no special relationship between the other two would also be described as special, even though, as is evident from Figure 2.7, the multiplicity of each is four, as for the general form in this crystal class. One reason for this is that these poles lie normal to a diad axis. This is a special position with respect to this axis and has the result that if a crystal grew with faces parallel only to the planes of indices {hk0}, {h0l} and {0kl}, it would appear to show mirror symmetry as well as the three diad axes. A second reason is that each of the {hk0}, {h0l} and {0kl} forms is open, while the general {hkl} form is closed. Special forms usually correspond to poles lying normal to or on an axis of symmetry, and normal to or on mirror planes, and sometimes to poles lying midway between two axes of symmetry. However, the best definition of a special form is as follows: a form is special if the development of the complete form shows a symmetry of arrangement of the poles which is higher than the one the crystal actually possesses. Special forms in all of the crystal classes are listed later, in Table 2.1. The orthorhombic system also contains the classes 2mm and mmm (Figure 2.6). The former contains two mirror planes, which must be at right angles. Two mirror planes at right angles automatically show diad symmetry along the line of intersection (Figure 2.6). – –– Since m ≡ 2, this group could be designated 2 2 2, and this is why it appears in the orthorhombic system, which is defined as possessing three diad axes. This crystal class could simply be designated mm since the diad is automatically present. However, mm2 is usually used for the later development of space groups (see Section 2.12). A crystal containing three diad axes can also contain mirrors normal to all of these without an axis of higher symmetry. Such a point group is designated mmm, or could be designated 2/mm. As can be seen from Figure 2.6, the multiplicity of the general form is now eight. The special forms {hk0}, {h0l} and {0kl} now show a lower multiplicity than the general one. The point group mmm shows the highest symmetry in the orthorhombic system. The point group showing the highest symmetry in a particular crystal system is said to be the holosymmetric class. To plot a stereogram of an orthorhombic crystal centred on 001 if given the lattice parameters a, b and c, we proceed as shown in Figure 2.8. In Figure 2.8a the poles of the (001), (010) and (100) planes are immediately inserted at the centre of the primitive and where the x- and y-axes cut the primitive, respectively. A pole (hk0) can be inserted at an angle q along the primitive to (100), as shown in Figure 2.8a, by noting from Figure 2.8b (which is a section of the crystal parallel to (001) showing the intersection of the plane (hk0) with the crystal axes) that the pole of (100) lies along OM, that (hk0) makes intercepts on the crystal axes of a/h along the x axis and b/k along the y axis, and that q is the angle between the normal to (hk0) and the normal to (100). From Figure 2.8b we have: tan θ = cot (90° − θ ) =

a /h a k = b/k b h

That is: tan (100) ^ (hk 0) = ( a / b)(k / h)

Kelly_c02.indd 50

(2.1a)

11/30/2011 7:32:20 PM

Point Groups and Space Groups

51

(a)

(b) 90°–q 001

010

y

–b k

0

N

q

Trace of (hk0)

q

hk0 –a h

q

Normal to (hk0)

90°–q 100 x

M

(d)

(c)

001 h0l

0kl

010

001

011

010

hkl hk0 311

100

100

310

Figure 2.8

where (100)∧(hk0) means the angle between the (100) and (hk0) planes; that is, the angle between the pole of (100) and the pole of (hk0). Similarly, if the lattice parameters are given, we can locate (0kl) and (h0l), since: tan (001) ^ (0 kl ) = (c / b)(k / l )

(2.1b)

tan (001) ^ (h0l ) = (c / a)(h / l )

(2.1c)

and:

These relations can be seen immediately by drawing diagrams similar to Figure 2.8b but looking along the x- and y-axes, respectively. When poles such as (h0l), (0kl) and (hk0) have been inserted on the stereogram, we can insert a pole such as (hkl) immediately by use of the zone addition rule, given in Section 1.3, Equation 1.20. If two poles (h1k1l1), (h2k2l2) both lie in the same zone with the indices [uvw] then so does the pole of the plane (mh1 + nh2, mk1 + nk2, ml1 + nl2); that is, any plane whose indices can

Kelly_c02.indd 51

11/30/2011 7:32:23 PM

52

Crystallography and Crystal Defects

be formed by taking linear combinations of the indices of two planes in a given zone can provide the indices of a further plane in that same zone (Section 1.3). In general, m and n can be positive or negative, but if m and n are both positive then the pole of the plane under consideration must lie on the great circle between the poles of (h1k1l1) and (h2k2l2): this simple result can be extremely useful when locating poles on stereographic projections such as Figure 2.7. In Figure 2.8c, after (001), (010), (100) and (hk0), (h0l), (0kl) are plotted, then to plot, say, (hkl), we note that (hkl) must lie in the zone containing (001) and (hk0), since if we multiply (001) by the number l and add the indices (00l) and (hk0) we obtain (hkl). It then follows that (hkl) lies somewhere on the great circle between (001) and (hk0). Similarly, (hkl) lies in the zone containing (0kl) and (100), since h times (100) gives (h00) and this added to (0kl) gives (hkl). Again, it is true that (hkl) lies somewhere on the great circle between (0kl) and (100), but we can now rationalise that (hkl) must lie at the intersection of the two great circles we have considered. We then draw the great circle (or zone) containing (001) and (hk0) and that containing (001) and (0kl) and we know that (hkl) is situated where these intersect. A particular example may make the procedure clear. Suppose we wish to locate (311) after plotting (001), (010) and (100) (Figure 2.8d). One way to proceed would be to locate (011) using Equation 2.1b, setting k = 1 and l = 1 and using the known lattice parameters. We then find (310), on the primitive, by finding the angle between (100) and (310) from Equation 2.1a, setting h = 3 and k = 1. Finally, we note that (311) lies in the zone containing (001) and (310), since (001) plus (310) yields (311). Also, (311) lies in the zone containing (100) and (011) since three times (100) plus (011) yields (311). The pole of (311) is then immediately located by drawing the great circle through (001) and (310) and that through (011) and (100); (311) is located where these great circles meet. Using the above procedure for locating poles is usually the quickest way to draw an accurate stereogram when key poles have been located either by calculation or through the use of a computer software package. It must be strongly emphasized that, although we have chosen the orthorhombic system as an example, the use of Equation 1.20 to locate poles applies to any crystal system and does not depend on the crystal axes being at any particular angle to one another. The utility of Equation 1.20 is one of the great advantages of the Miller index for denoting crystal planes, and arises naturally from the properties of a space lattice. Equations such as Equation (2.1) can of course be used to find the ratio of the lattice parameters – the axial ratios – from measurements of the angles between poles.

2.3 Tetragonal System The tetrad axis is always taken parallel to the z-axis. The lattice parameters a and b are equal. The holosymmetric point group is 4/mmm, showing three mutually perpendicular mirror planes with a tetrad normal to one of them (Figure 2.6). If a single pole is repeated according to the presence of these symmetry elements it will be found that diad axes are necessarily present normal to the mirrors and that, in addition, a second pair of diad axes also

Kelly_c02.indd 52

11/30/2011 7:32:25 PM

Point Groups and Space Groups

53

normal to mirror planes automatically arises. One of the pairs of mutually perpendicular diads is chosen as defining the directions of the x- and y-axes. The general form is {hkl}, with a multiplicity of 16. Special forms are {001}, {100}, {110}, {hk0}, {h0l} and {hhl}. The last of these, {hhl}, indicates a face making equal intercepts on the x- and y-axes. The point group 422 could be specified simply as 42 since if 4 and 2 are present at right angles a second pair of diad axes arises and one of these pairs is chosen to define the x- and – – y-axes. The group 4 2m can be developed as 4 m. It is then found that diad axes automatically arise at 45° to the two, mutually perpendicular, mirror planes. The pair of diad axes is taken – to define the x- and y-axes. The four other tetragonal point groups, 4, 4 , 4/m and 4mm, are straightforward and no diad axes arise. The angles between poles on a stereogram and the ratio of the lattice parameters (i.e. the ratio a : c in this crystal system) are easily related by using equations such as Equation 2.1 with a = b.

2.4

Cubic System

Cubic crystals possess four triad axes as a minimum symmetry requirement. These are arranged as in Figure 1.30 and are always taken to lie along the type directions of the unit cell, which is a cube, so a = b = c. This is the only crystal system in which the direction [uvw] necessarily coincides with the normal to the plane (uvw) for all u, v, w. If we put four triad axes to coincide with the 〈111〉 directions on a stereogram and allow these to operate on a single pole, as in Figure 2.9, we find that diad axes automatically arise along the crystal axes. The presence of the diads also follows from Table 1.2, with the row starting 233. The point group symbol used to describe the combination of a diad and two triads, shown in Table 1.2, is just 23. This is the cubic point group of lowest symmetry. The multiplicity of the general form for this point group is 12 (Figure 2.9). A feature of the – symbols for describing point groups in the cubic system is that the symbol 3 or 3, even though it indicates the defining axis for the system, is never placed first because the triads,

Figure 2.9

Kelly_c02.indd 53

11/30/2011 7:32:26 PM

54

Crystallography and Crystal Defects (a)

(b) m

m m

Figure 2.10

or inverse triads, are always at 54.74° (cos −1 (1/ 3)) to the crystal axes. (In all other systems the defining axis comes first in the symbol – the presence of the diads or inverse diads parallel to at least two axes must be stated to distinguish orthorhombic point groups from monoclinic point groups.) – The figure 3 (or 3) always occurs second in the symbol for cubic point groups, and this enables a point group in the cubic system to be distinguished from those in all other crystal systems. In a cubic crystal mirror planes can run either parallel to {1 0 0} planes, as in Figure 2.10a, or else parallel to {1 1 0} planes, as in Figure 2.10b. The first alternative is – – described by putting the symbol m before 3 (to give m3) and the second by placing m after – – – the 3 (or 3) to give X3m or X3m, where X is an axis other than 3 or 3. If we add mirror planes parallel to {100} to the class 23 we obtain 2/m3, conventionally – denoted m3. (Prior to the most recent revision of the International Tables for Crystallography in 1995 this point group was denoted m3; older textbooks will use this terminology as well.) As is evident from Figure 2.6, this contains a centre of symmetry in addition to the three diads at the intersection of three mutually perpendicular mirror planes – and the four triads. The triads therefore become inversion triads, 3. The multiplicity of the general form {hkl} is 24. It is worth noting from Table 2.3 (see below) that when there are no diads along 〈110〉 nor mirrors parallel to {110}, {hk0} and {kh0} are separate special – forms. This occurs in the classes 23 and m3. Replacement of the diads in 23 by tetrads gives 43. Here we notice that diads automatically arise along the 〈110〉 directions, as tabulated in Table 1.2. This class is denoted 432 to indicate the diads because of later development of space groups (see Section 2.11). However, 43 is sufficient to identify it. – Replacement of 2 by 4 in 23 will be found to produce mirror planes automatically parallel to the {110} planes, and hence passing through the triads. Correspondingly, if mirrors – parallel to {110} are added to 23 then the diad axes along the directions become 4 axes. If we have mirror planes passing through the triad axes then parallel to the crystal – – – axes we can have either 4 or 4. The first of these classes is 4 3m and the second m3m. (This latter point group was known as m3m conventionally prior to the 1995 revision of the International Tables for Crystallography.) In 4¯ 3m there is no centre of symmetry and there are no additional symmetry elements, other than those indicated in the symbol.

Kelly_c02.indd 54

11/30/2011 7:32:26 PM

Point Groups and Space Groups

55

100 210

]

210

[0

12

[02

[0 2 1

1]

12

[0

]

]

110

110 321

[1 02 ]

132

[20

312

312 201

] 321

[111

0]

121

111

231

221 211 [1 10 ] [ 1 321 11]

[21

0]

120

110

0]

1]

[01

[12

110

[12

212

101

122

]

211

112

]

01

[1

132

[111

221

212

]

111

231

11

]

213

213

010

[100]

[0

02

[1

102

112

122

121

1]

021

011

123

123

132

[10

132

012

001

121

122 123

012

011

[1 [111] 10 ]

112

102

123

021

1]

213

213

[010]

]

0]

112

122

120

231

111

212

212

111

[201

[21

221

101

121

120

211 312

312

231

010

201

211

221 120

321

210

210 100

Figure 2.11

Stereogram of a cubic crystal. (From [5], p. 82. Copyright 1959.)

– – The multiplicity of the general form is 24. In 4 3m (as in 23), {111} and {111} are separate special forms: each shows four planes parallel to the surfaces of a regular tetrahedron. – Class m3m has mirror planes parallel to {100} and to {110}; thus nine are present in all. There are six diads, three tetrads, a centre and of course the four triads. All of these can be produced by putting mirrors parallel to both {110} and {100}, coupled with the four triads. – Hence the symbol m3m is used to describe this point group, which is the cubic holosym– metric class. In full notation this would be 4/m 3 2/m, to denote the point group symmetry – elements as 4/m along the directions, 3 along the directions and 2/m along the directions. The general form has 48 faces. A stereogram of a cubic crystal with the poles of a number of faces indicated, along with the zones in which they lie, is shown in Figure 2.11. Additional poles are easily located on a stereogram, such as that in Figure 2.11, by use of the zone addition rule explained in Section 1.3 (Equation 1.20 and following) and used to plot poles in Section 2.2.

Kelly_c02.indd 55

11/30/2011 7:32:27 PM

56

2.5

Crystallography and Crystal Defects

Hexagonal System

Crystals possessing a hexad axis have a Bravais lattice, as illustrated in Figure 1.19j in Section 1.8. The x- and y-axes are at 120° to one another and perpendicular to the hexagonal axis along z. The holosymmetric class of this system, 6/mmm, possesses a hexad at the intersection of two sets of three vertical planes of symmetry, two sets of three diad axes normal to these, a plane of symmetry normal to the hexad axis and a centre of symmetry (Figure 2.6). These symmetry elements are shown in Figure 2.12a. Diad axes at 120° to one another are taken as the crystal axes. If this is done, the indices of a number of faces are as marked in Figure 2.12b. The plane of index (100) is repeated by the hexad axis to give – – – – (010), (110), (100), (010), (110). All of these are identical crystallographic planes and yet – their Miller indices appear different: note (010) and (110). To avoid the possibility of confusion from having planes of the same form with quite different indices, it is customary in materials science and metallurgy to employ Miller–Bravais indices for the hexagonal system. To do this, we choose a third crystal axis u normal to the hexagonal axis and at 120° to both the x- and the y-axes. The lattice repeat distance u along u is equal to a (= b) from Figure 1.19j. To state the Miller–Bravais indices of a plane we then take the intercepts along all three axes, x, y and u, express these in terms of the lattice parameters and proceed exactly as in Section 1.2. The result is that a plane always has four indices (hkil), where i is the intercept along the u-axis. It is obvious that there is a necessary relationship between h, k and i since the u-axis is a redundant third axis normal to the hexagonal axis. This can be deduced from Figure 2.13 and is: i = − (h + k ) (a)

(2.2)

u

(b)

110 1120

100 1010

210 2110

010 0110

y

110 1100 001

120 1210

120 1210

0001

110 1100

y

010 0110

210 2110

x

100 1010

110 1120

x

Figure 2.12

Kelly_c02.indd 56

11/30/2011 7:32:28 PM

Point Groups and Space Groups

57

i.e. the third index is always the negative of the sum of the first two. The indices of a number of poles are given in both Miller–Bravais and Miller indices in Figure 2.12b. The hexagonal symmetry is then apparent in the former from the indices of planes of the same form. A Miller–Bravais system is also used to specify directions in hexagonal crystals so that the index appears as [uvtw] instead of [uvw]. When this is done, a little care is needed in relating the results to those obtained using a three-index notation. To enable directions of a given family to have indices of similar appearance, the directions are specified by taking steps along all three axes and arranging it so that the step along the u-axis is of such length that the number of unit repeat vectors moved along this direction, t, is equal to the negative of (u + v). –– The direction corresponding to the x-axis in Figure 2.14 is then [21 1 0] in the four-index –– notation and [100] in the three-index system; the magnitude of [21 10] is three times that of [100], so therefore [100] in the three-index system is equivalent in magnitude to the fourindex vector 13 [2 1 1 0] . Likewise, [010] in the three-index system is equivalent in magnitude to the four-index vector 13 [1 2 1 0] and [110] to 13 [1 1 2 0] . It should be noted that the Miller–Bravais index cannot easily be immediately written down from the first two indices of the three-index triplet, as is the case for a plane, although knowing the four-index vectors equivalent in magnitude and direction to the three-index vectors [100] and [010] enables more general three-index vectors [uvw] to be transformed into their four-index equivalent vectors relatively easily prior to the clearing of fractions to specify four-index zones or directions. Some indices of direction specified in both ways are given in Figure 2.14. In relating planes and zone axes using Equation 1.6, it is usually best to work entirely in the three-index

u

O

a k

B

y

Trace of (hkil )

a 120° h –a i X A

x

Figure 2.13

Kelly_c02.indd 57

11/30/2011 7:32:29 PM

58

Crystallography and Crystal Defects [011] [1213]

[001] [0001]

u

y

2 [0110] [120] –1 –1 [2110] [100]

[1120] [110]

x

Figure 2.14

notation for both planes and directions and to translate the three-index notation for a direction into the four-index system at the end of the calculation. It is also useful to note that the condition needed for a four-index vector [uvtw] to lie in a four-index plane (hkil) is: hu + kv + it + lw = 0

(2.3)

Other point groups besides 6/mmm in the hexagonal system are shown in Figure 2.6. We – note that 6 (≡ 3/m) is placed in this system because of the use of rotoinversion axes to – describe symmetry operations of the second sort; 6, 6, 6/m and 6mm show no diad axes, just like their counterparts in the tetragonal system. The crystal axes for 6mm are usually cho– sen to be perpendicular to one set of mirrors (they then lie in the other set) and 6 m2 could – be developed as 6 m (≡ 3/mm). The diads automatically arise and are chosen as crystallographic axes. Of course, 622 contains diads. It could be developed as 62, since the second set of diads arises automatically (e.g. see Table 1.2). The axes are chosen parallel to one set of diads. Only 6/m and 6/mmm are centrosymmetric in this system. It is apparent from the stereogram in Figure 2.12b that stereograms with 0001 at the centre showing {hki0} poles are straightforward to plot. To plot more general poles on a stereogram with 0001 at the centre, it is apparent that the c/a ratio has to be used. Thus, for

Kelly_c02.indd 58

11/30/2011 7:32:33 PM

Point Groups and Space Groups

59

Normal to (0001)

Normal to (hh2hl)

c l q a h

a h

y

a 2h 90º 30º

x

Figure 2.15

example, this has to be used to determine the angle between faces such as (0001) and – (hh2hl), for example (1121). It is convenient to choose a (hh2hl) plane because such a plane is equally inclined to the x- and the y-axes. From Figure 2.15, the angle q between the (0001) pole and the (hh2hl) pole is seen to be given by: tan θ =

c 2h a l

(2.4)

– Similarly, the angle q between (0001) and (h0h l) is: tan θ =

c 2h a 3l

(2.5)

– – An example of a stereogram centred at (0001) with poles of the forms {1121}, {1011} and – {1231} indicated for a hexagonal cell is shown in Section 2.6 in connection with crystals of the trigonal system. The special forms in the various classes of the hexagonal system are listed in Table 2.1.

2.6 Trigonal System This crystal system is defined by the possession of a single triad axis. It is closely related to the hexagonal system. The possession of a single triad axis by a crystal does not, by itself, indicate whether the lattice considered as a set of points is truly hexagonal, or

Kelly_c02.indd 59

11/30/2011 7:32:34 PM

60

Crystallography and Crystal Defects 211 101

110

214

112

241

z

001

010

124

011

121

100

111

010

y 142

011

001 100

121 120

421

x

210

412

112 102

201

110

101 211

– Figure 2.16 A stereogram of a trigonal crystal of class 3m with a rhombohedral unit cell. When poles in the upper and lower hemispheres coincide in projection, the indices shown refer to the poles in the upper hemisphere

whether it is based on the staggered stacking of triequiangular nets. When the lattice is rhombohedral, a cell of the shape of Figure 1.19k can be used. The cell in Figure 1.19k is a rhombohedron and the angle a (< 120°) is characteristic of the substance. When the lattice of a trigonal crystal is hexagonal, it is not appropriate to use a rhombohedral unit cell. – The symmetry elements in the holosymmetric class 3m are shown in Figure 2.6 and the repetition of a single pole in accordance with this symmetry is also demonstrated. In this – class, three diad axes arise automatically from the presence of 3 and the three mirrors lying – parallel to 3. These diad axes, which intersect in the inverse triad axis, do not lie in the mirror planes. If the rhombohedral cell is used for such a crystal then the axes cannot be chosen parallel to prominent axes of symmetry. A stereogram of a trigonal crystal indexed according to a rhombohedral unit cell is shown in Figure 2.16. The value of a is 98°. The x-, y- and z-axes are taken to lie in the mirror planes and the inverse triad is a body diagonal of the cell, therefore lying along the direction [111], which, from the geometry of the rhombohedral unit cell, is also parallel to the normal to the (111) plane. It is clear that the x-, y- and z-axes – that is, the directions [100], [010] and [001] – do not lie normal to the (100), (010) and (001) planes, respectively. However, these directions are easily located. For example, the z-axis, [001], is the pole of the zone – – containing (110), (010), (100) and (110), shown as a great circle in Figure 2.16. Likewise,

Kelly_c02.indd 60

11/30/2011 7:32:37 PM

Point Groups and Space Groups u

1010 2110

1120

2111 1011

1121

0110

1100

1101

0111 1211

1210

0001

1211

3211

1011 1121

2111 3121

y

1231

0110

2131

2110 x

1210

0111

1101

1100

61

1120 1010

Figure 2.17 The same crystal as in Figure 2.16 indexed using a hexagonal cell. When poles in the upper and lower hemispheres superpose in projection, the indices refer to poles in the upper hemisphere

– – the y-axis is the pole of the zone containing (101), (100), (001) and (101), and the x-axis is – – the pole of the zone containing (011), (001), (010) and (011). In plotting a stereogram of a trigonal crystal with a rhombohedral unit cell from a given value of the angle a, it is useful to note that the angle g between any of the crystal axes and the unique triad axis is given by: sin γ =

2 3

sin α /2

(2.6)

(see Problem 2.2). For many purposes it is more convenient to use a hexagonal cell when dealing with trigonal crystals, irrespective of whether the lattice of the trigonal crystal is primitive hexagonal or rhombohedral. The shape of the cell chosen is the same as for hexagonal crystals (Figure 1.19j) and, since it is chosen without reference to the lattice, may or may not be primitive. The value c/a is characteristic of the substance. – A stereogram of a trigonal crystal of the point group 3m with planes indexed according to the Miller–Bravais scheme is shown in Figure 2.17. This is the same crystal as that in Figure 2.16 (c/a = 1.02). When using the hexagonal cell, the x-, y- and u-axes are chosen – parallel to the diads in 3m.

Kelly_c02.indd 61

11/30/2011 7:32:37 PM

62

Crystallography and Crystal Defects

The relationship between the indices in the two stereograms can be easily worked out using the zone addition rule and the Weiss zone law, Equation 1.6, from the orientation relationship of the rhombohedral and hexagonal cells. In Figures 2.16 and 2.17 this is – – –– (0001)⏐⏐(111)4 and (1011)⏐⏐(100). The plane (1010) in Figure 2.17 then has indices (211 ) –– –– in Figure 2.16. The indices (211 ) could be deduced by noting that the plane (211 ) contains –– the [111] direction (and so the pole of (211) must lie on the primitive if [111] is at the centre of the stereogram), is equally inclined to the y- and z-axes, and lies in the zone containing (111) and (100). The plotting of a stereogram and the determination of axial ratios for a trigonal crystal referred to hexagonal axes then proceed as for the hexagonal system.5 – In the class 3m, special forms lie (i) normal to the triad: {0001}, (ii) parallel to the triad: – {hki0}, (iii) normal to mirror planes: {h0h l}, and (iv) equally inclined to two diads: – – {hh2hl}. The six faces in the form {h0h l} make a rhombohedron; {1012} would be an – – – – – – – –– example, consisting of the planes (1012), (1102), (0112), (1012), (1102) and (011 2). This form is similar in appearance to {0hh¯l}, which is also a rhombohedron, rotated 60° with respect to the first one. – – – The relationship between {h0h l} and {0hh l} (or, equivalently, {0kk l}) is shown in Figure 2.18. They are actually quite separate forms and each one is a special form. We – – therefore need to add {0hh l} to the list of special forms, in addition to {h0h l}. It is apparent – – from Figure 2.16 that when using the rhombohedral cell the two forms {1011} and {0111} – have different indices, since the face above (001) in the projection in Figure 2.16 would – have indices (221). – The other trigonal point groups are shown in Figure 2.6. In 3 and in 3 there are neither mirrors nor diads. The class 3m has three mirrors intersecting in the triad axis; the x-, y- and u-axes of the hexagonal cell are taken to lie perpendicular to the mirror planes. The point group 32 contains diads normal to 3 (consistent with the geometry for permissible combinations of rotational symmetry operations in Table 1.2), which are taken as the crystallo– graphic axes. If three mirror planes intersect in an inversion triad, as in 3m, then diads automatically arise normal to the mirror planes; the diads are chosen as the x-, y- and u-axes. Finally, we note that the class 3/m is not specified as a point group in the trigonal system: it is placed in the hexagonal system because it is equivalent to 6¯.

(1011)

y

(1101)

y

(1011)

(0111)

Figure 2.18 The symbol ⏐⏐ means ‘parallel to’. The relationship between the two cells used in Figures 2.16 and 2.17 is shown in Figure A4.2a, where general methods of transforming the indices of planes and directions, when different unit cells are chosen for the same crystal, are considered. 4 5

Kelly_c02.indd 62

11/30/2011 7:32:39 PM

Point Groups and Space Groups

2.7

63

Monoclinic System

Crystals in the monoclinic system possess a single two-fold axis. Since a mirror plane is – equivalent to an inverse diad, the class m (≡ 2) is put into this system. Two settings are shown in Figure 2.6 for the monoclinic point groups, depending on whether the stereogram is centred on the two-fold axis (the 1st setting) or whether the two-fold axis is lying in the equatorial plane of the stereogram (the 2nd setting). With respect to the convention for choosing x-, y- and z-axes for stereograms centred on the normal to the 001 planes for orthorhombic, tetragonal and cubic crystals, the two-fold axis is along the z-axis in the 1st setting, so that the angle g between the x- and y-axes is obtuse (as for hexagonal crystals, where g is fixed to be 120°), while a = b = 90°. In the 2nd setting, the two-fold axis is along the y-axis, so that the angle b between the x- and z-axes is obtuse, while a = g = 90°. Somewhat confusingly, both conventions are used in the scientific literature to describe the unit cells of monoclinic crystals, but it is much more common in materials science and metallurgy for the 2nd setting to be used, as we have chosen to do in Table 1.3 and Figures 1.19b and c. Irrespective of the choice of 1st or 2nd setting, the sides of the unit cells of crystals belonging to the monoclinic system are in general all unequal to one another. The symmetry elements in the holosymmetric point group 2/m are shown in Figure 2.19 for the 2nd setting. The pole of (010) and the y-axis coincide on the stereogram. In this m 100

hk0

hk0

x h0l hkl

hkl

0kl

0kl z

010

010

b – 90° 001

0kl

hkl

y

0kl

f

hkl h0l

hk0

+x

hk0

b – 90° 100 m

Figure 2.19

Kelly_c02.indd 63

Monoclinic stereogram centred on [001] for the 2nd setting

11/30/2011 7:32:39 PM

64

Crystallography and Crystal Defects z

(hk0)

b

b k

90° f

Normal to 010

b – 90° 90° a h

y

Normal to hk0

x

Figure 2.20 A diagram from which the angle f in Figure 2.19 between 010 and hk0 can be derived

figure, [001], the z-axis, is chosen to be at the centre of the primitive and so (100) lies on the primitive 90° from (010). The x-axis, the direction [100], which makes the obtuse angle b with [001], is necessarily in the lower hemisphere. The angle between [001] and (001) is (b − 90°), which is of course equal to the angle between (100) and [100]. Poles such as {hk0} lie around the primitive because [100] lies in {hk0} planes (Weiss zone law, Equation 1.6). A pole such as (hk0) lies at angle j to (010), given by: cot ϕ =

(a / h) sin β (b / k )

(2.7a)

(see Figure 2.20), or equivalently (Section A3.2): cos ϕ =

Kelly_c02.indd 64

k b ⎛ h2 k2 ⎞ ⎜ a 2 sin 2 β + b2 ⎟ ⎝ ⎠

1/2

(2.7b)

11/30/2011 7:32:39 PM

Point Groups and Space Groups

65

The factor sin b arises because the normals to (hk0) and (010) and the x-axis do not lie in the same plane. In the point group 2/m the only special form besides {010} is {h0l}, with – – a multiplicity of two – the planes (h0l) and (h 0l ). It is apparent that the two faces in this latter form are parallel, both lying normal to the mirror plane and parallel to the diad axis. The general form is {hkl}, with a multiplicity of four (see Figure 2.19). {hk0} and {0kl} are also general forms. The remaining point groups in the monoclinic system are 2 and m. Again, {h0l} is a special form in both and so is {010}. However, 2 does not possess a centre and so for this – point group {010} and {010} must each be listed as separate special forms.

2.8 Triclinic System There are no special forms in either of the point groups in this system. The unit cell is a general parallelepiped and the geometry is more complicated than even for the monoclinic system. The drawing of a stereogram whose centre is taken to be the z-axis, [001], can be carried out with the aid of Figures 2.21a and b. The two diagrams here are completely general and can be specialized to apply to any crystal system more symmetric than the triclinic by setting one or more of the axial angles to particular values and by setting two or more of the lattice parameters to be equal. The choice of the centre of the stereogram as the z-axis in Figure 2.21a means that all planes of the general form (hk0) lie on the primitive of the stereogram, just as for the monoclinic stereogram in Figure 2.19. However, for triclinic crystals there is no good reason to have the 010 pole located on the right-hand side of the horizontal axis of the stereogram, and so here it is deliberately rotated around the primitive away from this position. The great circle passing through 001 and 010 is the [100] zone, containing planes of the general form (0kl). Therefore, the angle between this zone and the primitive must be the angle between [100] and [001], b, as shown in Figure 2.21a. This is because the stereographic projection is a conformal projection (see Appendix 2); that is, one for which angles are faithfully reproduced. Similarly, a and g can be specified on Figure 2.21a from the triclinic system geometry. Angles between poles can be determined using Equation A3.18. Once the position of the 010 pole (or any other pole of the form hk0) has been chosen, geometry determines the positions of the remaining poles on the stereogram. Thus, for example, the position of the 001 pole is fixed knowing that it lies in the [100] zone, which has to make an angle of b with the primitive, and that 001 is a given angle from 010, determined for example using Equation A3.4. Likewise, the position of a pole 0kl lying in the [100] zone can be determined, as can the positions of the poles 100, h0l, hk0 and hkl. While stereographic projections can now be produced routinely via proprietary software packages, it is still instructive to consider further aspects of the geometry of the part of the triclinic stereogram shown in Figure 2.21a in order to gain a full appreciation of the richness of information displayed on stereograms. An (hkl) plane of a triclinic crystal is shown in Figure 2.21b. The six angles f1–f6 in Figure 2.21b are the same as those marked in Figure 2.21a. Thus, for example, f1 in Figure 2.21b is an angle lying in the (001) plane. It is the angle – between the y-axis and the vector [k h0] common to (hkl) and (001); that is, the angle

Kelly_c02.indd 65

11/30/2011 7:32:42 PM

66

Crystallography and Crystal Defects (a) b

z

010 f3

001 y

0kl

f2

f1

f4

hkl h0l hk0

f6 a

f5

100 z

(b)

f5 f4 (010)

a

b g f3 f2

a h

(100)

c l

f6

b k f1

y

hkl (001)

x

Figure 2.21 Diagrams relevant to drawing stereograms of triclinic crystals. The centre of the stereogram in (a) is the z-axis, [001]

between the zone containing (001), (h0l) and (100) and the zone containing (001), (hkl) and (hk0). We can therefore mark f1 on the stereogram. Similarly, f5 in Figure 2.21b is an angle – lying in the (100) plane. It is the angle between the z-axis and the vector [0 l k] common to (hkl) and (100); that is, the angle between the zone containing (100), (hk0) and (010) and the zone containing (100), (hkl) and (0kl). f5 can therefore also be marked on the

Kelly_c02.indd 66

11/30/2011 7:32:42 PM

Point Groups and Space Groups

67

stereogram. Proceeding in this way, we can identify all of the angles f1–f6. We have, from the geometry in Figure 2.21b:

α + φ5 + φ6 = 180° β + φ3 + φ4 = 180° γ + φ1 + φ 2 = 180°

(2.8)

Furthermore, from the triangle on the (001) face in Figure 2.21b we have, using the sine rule: a/h b/k = sin φ1 sin φ2

(2.9)

a / h sin φ1 = b / k sin φ2

(2.10a)

c / l sin φ6 = b / k sin φ5

(2.10b)

a / h sin φ4 = c / l sin φ3

(2.10c)

Therefore:

and similarly:

and:

As an aside, we note that Equations 2.10a–c are also of use in finding axial ratios and axial angles from measured angles between planes on single crystal specimens of crystals belonging to the triclinic crystal system; such crystals tend to be minerals or organic materials, rather than metals, the crystal structures of which rarely tend to belong to either the monoclinic or the triclinic systems.

2.9

Special Forms in the Crystal Classes

A summary of the special forms in the various crystal classes for the various crystal systems is given in Table 2.1. The orientation of the axes is that used in this chapter. Monoclinic crystals are in the 2nd setting of Figure 2.6 and trigonal crystals are referred to hexagonal axes. There are no special forms in the triclinic system.

Kelly_c02.indd 67

11/30/2011 7:32:42 PM

68

Crystallography and Crystal Defects

Table 2.1

Special forms in the crystal classes

2

32

6mm

– {0 1 0}, {0 1 0}, {h 0 l}

– {0 –0 –0 1}, {1 0 –1 0}, {2 1 1 0}, {1 1 –2 0}, {h k i 0}, {h 0 h l}, {0 k k l}, {h h 2h l}, {2h h h l}

– – {0 0 0 1}, {0 0 0 1}, {1 0 1 0}, – {1 1 2 0}, {h k i 0}, {h 0 h l}, {h h 2h l}

m and 2/m

4

{0 1 0}, {h 0 l}

– {0 0 1}, {0 0 1}, {h k 0}

mm2

– 4 and 4/m

– {0 0 1}, {0 0 1}, {1 0 0}, {0 1 0}, {h k 0}, {h 0 l}, {0 k l}

{0 0 1}, {h k 0}

622 and 6/mmm – – {0 0 0 1}, {1 0 1 0}, {1 1 2 0}, {h k i 0}, {h 0 h l}, {h h 2h l}

222 and mmm

4mm

23

– {0 0 1}, {0 0 1}, {1 0 0}, {1 1 0}, {h k 0}, {h 0 l}, {h h l} – 4 2m

{1 0 0}, {1 1 – 0}, {h k 0}, {k– h 0}, {1 1 1}, {1 1 1}, {h l l}, {h l l}, {h h l}, {h h l} – m3

{0 0 1}, {1 0 0}, {1 1 0}, {h k 0}, {h 0 l}, {h h l}, {h h l}

{1 0 0}, {1 1 0}, {h k 0}, {k h 0}, {1 1 1}, {h l l}, {h h l}

42 and 4/mmm

432

{0 0 0 1}, {h k i 0}

{0 0 1}, {1 0 0}, {1 1 0}, {h k 0}, {h 0 l}, {h h l}

3m

6

{1 0 0}, {1 1 0}, {h k 0}, {1 1 1}, {h l l}, {h h l} – 4 3m

– – {0 0 0 – 1}, {0 0 0– 1}, {1 0 1 0}, {0 1 1 0}, {1 1 2 0}, {h k i 0}, {h 0 h l} {0 k k l}, {h h 2h l} – 3m – – {0 0 0 1}, {1 0 1 0}, {1 1 2 0}, {h k i 0}, {h 0 h l}, {0 k k l}, {h h 2h l}

– {0 0 0 1}, {0 0 0 1}, {h k i 0}

{1 0 0}, {0 1 0}, {0 0 1}, {h k 0}, {h 0 l}, {0 k l} 3 – {0 0 0 1}, {0 0 0 1}, {h k i 0} – 3

2.10

– 6 and 6/m {0 0 0 1}, {h k i 0}

– 6 m2 – – {0 0 0 – 1}, {1 0 1 0}, {0 1 1 0}, {1 1 2 0}, {h k i 0}, {h 0 h l}, {0 k k l}, {h h 2h l}

{1 0 – 0}, {1 1 0}, {h– k 0}, {1 1 1}, {1 1 1}, {h l l}, {h l l}, {h h l}, {h h l} – m3m {1 0 0}, {1 1 0}, {h k 0}, {1 1 1}, {h l l}, {h h l}

Enantiomorphous Crystal Classes

In some crystal classes the possibility exists of crystals being found in either a right-handed or a left-handed modification with the two not being superposable, in the sense that the right hand of the body cannot be superposed upon the left hand. This occurs if the crystal only

Kelly_c02.indd 68

11/30/2011 7:32:48 PM

Point Groups and Space Groups Table 2.2

69

Laue groups

System Cubic Hexagonal Tetragonal Trigonal Orthorhombic Monoclinic Triclinic

Class – – 432, 4–3m, m3m 23, m3 ¯ 622, – 6mm, 6m2, 6/mmm 6, 6, 6/m – 422, – 4mm, 4 m2, 4/mmm 4, 4 , 4/m– 32,– 3m, 3m 3, 3 222, 2mm, mmm 2, m, – 2/m 1, 1

Laue group – m3 –m m3 6/mmm 6/m 4/mmm 4/m – 3 –m 3 mmm 2/m – 1

possesses simple rotation symmetry operations; that is, no symmetry operation of the second kind. Therefore, mirror planes and rotoinversion axes of any degree do not appear in such crystal classes. There are 11 such classes: 1, 2, 3, 4, 6, 23, 222, 32, 422, 622 and 432.

2.11

Laue Groups

Some physical methods of examination of crystals cannot determine whether or not there is a centre of symmetry present, such as, for example, when stationary single crystals are illuminated by a continuous distribution of X-ray wavelengths (known as ‘white radiation’) to produce Laue diffraction patterns. This is known as the Laue method. Such diffraction patterns are used for symmetry determination and for the accurate alignment of crystals; they are also useful for time-resolved macromolecular crystallography using synchrotron radiation. The Laue group is the crystal class to which a particular crystal belongs if a centre of symmetry is added to the symmetry elements already present. The 11 Laue groups are shown in Table 2.2. The loss of symmetry information in time-resolved macromolecular crystallography is more than compensated for by the ability to capture structural information over subnanosecond timescales in fast chemical reactions such as enzyme reactions.

2.12

Space Groups

We showed in Section 1.4 that repetition of an object (e.g. an atom or group of atoms) in a crystal is carried out by operations of rotation, reflection (or inversion) and translation. We have also described in this chapter the consistent combinations of rotations and inversions that can occur in crystals, and in Section 1.8 we described the possible translations that can occur in crystals to produce the 14 Bravais lattices, or space lattices. However, we have so far not made any attempt to combine the operations of rotation (and inversion) with translation, except briefly in Section 1.5, where it was shown that only one-, two-, three-, four- and six-fold rotation axes are compatible with translational symmetry. A full description of the symmetry of a crystal involves a description of the way in

Kelly_c02.indd 69

11/30/2011 7:32:48 PM

70

Crystallography and Crystal Defects (a)

(b)

(c)

t 2 180º

t 2

180º

t 2

180º 180º

2

21

Figure 2.22 (a) A two-fold rotation axis. (b) A 21 screw axis. (c) A glide plane normal to the surface of the paper

which all of the symmetry elements are distributed in space. This is called the space group. There are 230 different crystallographic space groups and each one gives the fullest description of the symmetry elements present in a crystal possessing that group. The rotation axes and rotoinversion axes possible in crystals were discussed in Section 2.1 and the possible translations in Section 1.8. An enumeration of the way these axes can be consistently combined with the translation is therefore an enumeration of the possible space groups. Space groups are most important in the solution of crystal structures. They are also very useful when establishing symmetry hierarchies in phase transitions in perovskites [6–8]. When an attempt is made to combine the operations of rotation and translation, the possibility arises naturally of what is called a screw axis. This involves repetition by rotation about an axis, together with translation parallel to that axis. Similarly, a repetition by reflection in a mirror plane may be combined with a translational component parallel to that plane to produce a glide plane. If, for example, a two-fold rotational axis occurs in a crystal, then this means some structural unit or motif is arranged about this direction so that it is repeated by a rotation of 180° about the axis. The repetition shown in Figure 2.22a corresponds to a pure rotational diad axis. However, the rotation of 180° could be coupled with a translation of one-half of the lattice repeat distance, t, in the direction of the axis to give the screw diad axis shown in Figure 2.22b, denoted by the symbol 21. The translation t/2 will be of a length of the order of the lattice parameters of the crystal and hence of the order of a few Ångstrom units (1 Å = 10−10 m), and so quite undetected by the naked eye. The operation of glide plane repetition is shown in Figure 2.22c. Again, the magnitude of the translation will be of the

Kelly_c02.indd 70

11/30/2011 7:32:48 PM

Point Groups and Space Groups

71

order of the lattice parameters. Macroscopically, the crystal containing a 21 axis would then show diad symmetry about that axis in the symmetry of its external faces or of its physical properties. Similarly, the glide plane in Figure 2.22c would show itself macroscopically as a mirror plane. Although the presence of a screw axis, say a screw diad as in Figure 2.22b, indicates the presence of identical atomic motifs arranged about it so that they are related by a rotation plus translation, the screw axis must not be thought of as translating the translation vectors of the lattice. A screw axis and a pure rotation axis of the same order n repeat a translation in the same way. It follows that the rotational components of screw axes can only be 2p/1, 2p/2, 2p/3, 2p/4, 2p/6 and that an n-fold screw and an n-fold pure rotation axis must have similar locations with respect to a similar set of translations. The angles between screws and between screws and rotations must therefore be the same as the permissible combinations listed in Table 1.2. When we combine the operations of rotation with translation and look for the possible consistent combinations we can start with the point group and associate its symmetry elements with each lattice point of the lattices consistent with it. From the number of Bravais lattices and number of point groups detailed in Figures 1.19 and 2.6 it might be expected that 66 space groups could be obtained (2 triclinic, 6 monoclinic, 12 orthorhombic, 14 tetragonal, 5 trigonal with a rhombohedral lattice, 5 trigonal with a hexagonal lattice, 7 hexagonal and 15 cubic). Seven additional ones arise because of cases in which the glide planes or screw axes automatically arising are different for different orientations of the – – point group with respect to the lattice; for example, in the tetragonal system I4 m2 and I4 2m are distinct space groups. The 14 space groups for which this consideration is relevant are – – – – – – Cmm2, Amm2 (≡ C2mm), P4 2m, P4 m2, I4 2m, I4 m2, P6 m2, P6 2m, P312, P321, P3m1, – – P31m, P3m1 and P31m. Therefore, there are 73 such space groups, referred to as arithmetic crystal classes in Section 8.2.3 of the fifth edition of the International Tables for Crystallography [3]. When the possibilities of introducing screw axes to replace pure rotational axes and glide planes to replace mirror planes are taken into consideration, the result is to produce a total of 230 different space groups [3]. Of particular note are the space groups in the trigonal crystal system. Of the 25 trigonal space groups, only seven have a – – – rhombohedral unit cell (R3, R3, R32, R3m, R3c, R3m, R3c); the majority have a primitive hexagonal unit cell. Buerger [1] argues that ‘to refer one crystal of the trigonal class to rhombohedral axes, and another to hexagonal axes, because the lattice types are R and P respectively, leads to confusion’ (p. 106) and discourages the use of rhombohedral axes for this reason. It is certainly the case in the scientific literature that the use of rhombohedral axes for crystals where the space group is one of the seven rhombohedral space groups is markedly less prevalent than the use of hexagonal axes. The various kinds of screw axis possible are shown in Table 2.3. An nN-fold screw axis involves repetition by rotation through 360°/n with a translation of tN/n, where t is a lattice repeat vector parallel to the axis. There are five types of screw hexad; for example, 61 involves rotation through 60° and translation of t/6, while 65 involves rotation through 60° and translation of 5t/6. By drawing a diagram showing the repetition of objects by these axes, it is easily seen that 61 is a screw of opposite hand to 65, 41 to 43, and 62 to 64. A diagram to show this for 31 and 32 is given in Figure 2.23. In this figure, A and A′ are lattice points. The operation of 31 is straightforward, as shown in Figure 2.23a. When repeating an object according to 32, note that the object at height 43 must also occur at height 13 , since

Kelly_c02.indd 71

11/30/2011 7:32:49 PM

72

Crystallography and Crystal Defects

Table 2.3

Screw axes in crystals

Name

Symbol

Screw diad

21

Screw triads

31 32

Screw tetrads

41 42 43

Screw hexads

61 62 63 64 65

Graphical symbol

Right-handed screw translation along the axis in units of the lattice parameter 1 2 1 3 2 3 1 4 2 1 4=2 3 4 1 6 2 1 6=3 3= 6 4 6= 5 6

1 2 2 3

A and A′ are both lattice points and the pattern is infinitely long parallel to AA′. It should also be noted that axes 42 and 63 include the pure rotation axes 2 and 3 respectively in the lattice. 62 and 64 also contain two-fold rotation axes. Glide planes are described as axial glide planes if the translation parallel to the mirror is parallel to a single axis of the unit cell and equal to one-half of the lattice parameter in that direction. Such glide planes are given the symbols a, b or c, corresponding to the directions of the glide translations. A diagonal glide plane involves a translation of one-half of a face diagonal or one-half of a body diagonal (the latter in the tetragonal and cubic systems), given the symbol n, and a diamond glide plane involves a translation of one-quarter of a face diagonal, given the symbol d. The diamond glide plane involves a translation of one-quarter of a body diagonal in the tetragonal and cubic systems. In centred cells, the possibility of a ‘double’ glide plane arises, given the symbol e. In this symmetry operation, recognised officially in the most recent edition of the International Tables for Crystallography and incorporated into the conventional space group symbols of five space groups [3], two glide reflections occur through the plane under consideration, with glide vectors perpendicular to one another. The conventional space group symbol shows that the space groups have been built up by placing a point group at each of the lattice points of the appropriate Bravais lattice. Thus, – – for example, Fm3m (in full, F 4/m 3 2/m) means the cubic face-centred lattice with the – point group m3m associated with each lattice point and P63/mmc (in full, P 63/m 2/m 2/c) is a hexagonal primitive lattice derived from P6/mmm by replacing the six-fold rotation axis

Kelly_c02.indd 72

11/30/2011 7:32:49 PM

Point Groups and Space Groups (a)

73

(b)

A⬘

A⬘

2t 3

A

t 3

120º 31

A

120º

120º 32

Figure 2.23 Screw axes 31 and 32: these are screw axes of opposite hand, as shown by the symbols at the top

by 63 and one of the mirror planes by a c-axis glide plane. P63/mmc and P6/mmm share the same point group symmetry. The point group symmetry of any crystal is derived immediately from the space group symbol by replacing screw axes by the appropriate rotational axes and glide planes by mirror planes in the space group symbol. The arrangements of all of the symmetry elements in the 230 space groups are listed in the various editions of the International Tables for Crystallography. Of particular interest to most materials scientists are the coordinates of general and special positions within each unit cell and diagrams showing the symmetry elements. More recent editions have extensive descriptions of space groups, which also include listings of maximal subgroups and minimal supergroups; these concepts will be discussed in general terms in Sections 2.14 and 2.15. For our purposes in this section, the essential elements of how the assignment of a crystal structure to a particular space group imposes restrictions on the possible general and special positions of atoms or ions within a particular unit cell can be illustrated by considering the 17 two-dimensional space groups (or plane groups). These space groups are shown in Figure 2.24 in the same way they are depicted in the International Tables for

Kelly_c02.indd 73

11/30/2011 7:32:50 PM

No. 1 p1

1 Parallelogram

Origin on 1 Coordinates of equivalent positions 1 1 x, y

No. 3 pm ,

m Rectangular ,

,

No. 2 p2

2 Parallelogram

Origin at 2 Coordinates of equivalent positions 2 1 x, y ; x–, y– 1 2 21– , 12– 1 2 12– , 0 1 1 2 0, 2– 1 2 0, 0 m Rectangular No. 4 pg ,

,

,

Origin on m Coordinates of equivalent positions – y 2 1 x, y ; x, 1, 1 m 2 y 1 m 0, y

Origin on g Coordinates of equivalent positions 2 1 x, y ; x–, 1–2 + y

No. 5 cm ,

No. 6 pmm , ,

m Rectangular ,

mm Rectangular , ,

, ,

,

, ,

Origin on m Coordinates of equivalent positions (0, 0 ) +; ( 1–2, 1–2 ) + 4 1 x, y ; x–, y 2 m 0, y

, ,

Origin at 2mm Coordinates of equivalent positions 4 1 x, y ; x–, y ; x–, y– ; x, y– 2 m –12 , y ; 12–, y– 2 m 0, y ; 0, y– m x, –12 ; x–, 12– 2 m x, 0; x–, 0 2 1 mm 21– , 12– 1 mm 12– , 0 1 mm 0, 1–2 1 mm 0, 0

Figure 2.24 The 17 two-dimensional space groups arranged following the International Tables for Crystallography [3]. The headings for each figure read, from left to right, Number, Short Symbol (see Table 2.4), Point Group, Net. Below each figure the columns give the number of equivalent positions, the point group symmetry at those positions and the coordinates of the equivalent positions. The coordinates of positions x, y are expressed in units equal to the cell edge length in these two directions.

Kelly_c02.indd 74

11/30/2011 7:32:50 PM

No. 7 pmg

No. 8 pgg

mm Rectangular

,

mm Rectangular

,

,

,

,

,

Origin at 2 Coordinates of equivalent positions 4 1 x, y; x, y; 1–2 + x, y; 12– – x, y 2 m 1–4, y; –43, y

Origin at 2 Coordinates of equivalent positions 4 1 x, y; x–, –y; 1–2 + x, 1–2 – y; 21– – x, 2 2 12–, 0; 0, 12–

2 2

2

0, 21–; 12–, 1–2 0, 0; 21–, 0

2 2

No. 9 cmm

+y

1– 2

No. 10 p4

mm Rectangular

,

1

0, 0; 2–,

2

1– 2

4 Square

,

,

, , , ,

,

,

,

Origin at 2mm Coordinates of equivalent positions (0, 0) +; (12–, 1–2 ( + 8 1 x, y; x, y; x, y; x, y m 0, y; 0, y 4 m x, 0; x, 0 4 4 2 14–, 1–4; 14–, 3–4 2 mm 0, 1–2 2 mm 0, 0

Origin at 4 Coordinates of equivalent positions 4 1 x, y; x, y; y, x; y, x 2 2 1–2, 0; 0, 12– 1 4 1–2, 1–2 1 4 0, 0

No. 11 p4m , , , ,

No. 12 p4g

4 mm Square , , , ,

4 mm Square

,

, , , ,

, ,

, ,

, ,

Origin at 4mm Coordinates of equivalent positions 8 1 x, y; x, y; y, x; y, x; x, y; x, y; y, x; y, x m x, x; x, x; x, x; x, x 4 1 1 1 m x, –2; x; –2; –2, x; –12, x 4 m x, 0; x; 0; 0, x; 0, x 4 1 1 mm 2–, 0; 0, 2– 2 1– 1– 1 4mm 2, 2 1 4mm 0, 0

Figure 2.24

Kelly_c02.indd 75

,

Origin at 4 Coordinates of equivalent positions 1 1 1 1 8 1 x, y; y, x; –2 – x, –2 + y; –2 – y, –2 – x; 1– 1– 1– 1– x, y; y, x; 2 + x, 2 – y; 2 + y, 2 + x m x, 1–2 + x; x, 1–2 – x; 1–2 + x, x, 1–2 – x, x 4 2 mm 2

4

1– 2,

0; 0, 1–2

0, 0; 1–2 ,

1– 2

(continued)

11/30/2011 7:32:50 PM

No. 13 p3

No. 14 p3m1

3 Triequiangular

3 m Triequiangular

,

, ,

,

,

,

, ,

,

,

,

,

Origin at 3 Coordinates of equivalent positions 3 1 x, y; y, x − y; y − x, x 1 3 3–2, 13– 1 3 13– , 23– 1 3 0, 0

Origin at 3m Coordinates of equivalent positions 6 1 x, y; y, x − y; y − x, x; x, x − y; y − x, y; y, x m x, x; x, 2x; 2x, x 3 1 3m –32, 13– 1 3m 1–3, 2–3 1 3m 0, 0

No. 15 p31m

No. 16 p6

3 m Triequiangular

,

6 Triequiangular

,

, ,

,

,

,

, ,

,

,

,

Origin at 31m Coordinates of equivalent positions 6 1 x, y; y, x – y; y − x, x; y, x; x, y − x; x − y, y 3 m x, 0; 0, x; x, x 2 3 13–, –23; –23, 13– 1 3m 0, 0

Origin at 6 Coordinates of equivalent positions 6 1 x, y; y, x – y; y − x, x; x, y; y, y – x; x – y, x 3 2 –12 , 0; 0, –12; –12, –12 2 3 13– , –32; –23, 1–3 1 6 0, 0

No. 17 p6m 6 mm Triequiangular , , , , , , , , , , , ,

,

, ,

,

, , ,

,

, ,

, ,

Origin at 6mm Coordinates of equivalent positions 1 x, y; y, x – y; y – x, x–; y, x; x–, y – x; 12 x – y, y– ; x–, y– ; y, y – x ; x – y, x ; y– , x–; x, x – y; y – x, y m x, x–; x, 2x; 2x–, x– ; x–, x; x–, 2x–; 2x, x 6 m x, 0; 0, x; x–, x–; x–, 0; 0, x–; x, x 6 3 mm 12– , 0; 0, 12– ; 12– , 12– 3m –13, –32; –23, 1–3 2 1 6mm 0, 0

Figure 2.24 (continued)

Kelly_c02.indd 76

11/30/2011 7:32:51 PM

Point Groups and Space Groups

77

Table 2.4 Two-dimensional lattices, point groups and space groups System and lattice symbol

Parallelogram p (primitive) Rectangular p and c (centred)

Point group

1 2 m 2mm

Square p

4 4mm

Triequiangular (hexagonal) p

3 3m 6 6mm

Space group symbols Full

Short

p1 p211 p1m1 p1g1 c1m1 p2mm p2mg p2gg c2mm p4 p4mm p4gm p3 p3m1 p31m p6 p6mm

p1 p2 pm pg cm pmm pmg pgg cmm p4 p4m p4g p3 p3m1 p31m p6 p6m

Space group number

1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17

Note: The two distinct space groups p3m1 and p31m correspond to different orientations of the point group relative to the lattice. This does not lead to distinct groups in any other case.

Crystallography [3]. If the plane groups are understood, the essential elements of the threedimensional space group tables in the International Tables can be understood without difficulty. Space groups are obtained by the application of point group symmetry to finite lattices, the possibility of translation symmetry being taken into account. There are five lattices or nets in two dimensions, shown in Figure 1.14. Following the convention in the International Tables for Crystallography, we shall give them the symbol p for primitive and c for centred. The symbols for two-fold, three-fold, four-fold and six-fold axes and for the mirror plane are as in Section 2.1. The only additional symmetry element in two dimensions is the glide reflection line: symbol g and denoted by a dashed line in Figure 2.24. It involves reflection and a translation of one-half of the repeat distance parallel to the line. The two-dimensional lattices and the two-dimensional point groups are combined in Table 2.4 to show the space groups that can arise, which are shown in Figure 2.24. In all the diagrams, the x-axis runs down the page and the y-axis runs across the page, the positive y-direction being towards the right. In each of the diagrams the left-hand one shows the equivalent general positions of the space group; that is, the complete set of positions produced by the operation of the symmetry elements of the space group upon one initial position chosen at random. The total number of general positions is the number falling within the cell, but surrounding positions are also shown to illustrate the symmetry. The righthand diagram is that of the group of spatially distributed symmetry operators; that is, the true space (plane) group.

Kelly_c02.indd 77

11/30/2011 7:32:51 PM

78

Crystallography and Crystal Defects

Below each of the diagrams in Figure 2.24, the equivalent general positions and special positions are also indicated. Special positions are positions located on at least one symmetry operator so that repetition of an initial point produces fewer equivalent positions than in the general case. The symmetry at each special position is also given. The group p1 is obtained by combining the parallelogram net and a one-fold axis of rotational symmetry. There are no special positions in the cell. The group p2 arises by combining the parallelogram net and a diad. A mirror plane requires the rectangular net (Section 1.5) and if this net is combined with a single mirror, the space group pm, No. 3, results. Points , are in mirror relationship to one another. If the mirror in pm is replaced by a glide and reflection line, the space group pg results. In No. 4 the glide reflection line runs normal to the x-axis. The centred rectangular lattice necessarily shows a glide reflection line as in cm, No. 5, but only one of these need be present, corresponding to the plane point group m. Since, in this case, the net is multiply primitive, the motif associated with the lattice point at ( 12 , 12 ) is the same as that at (0, 0). Hence the coordinates of equivalent positions, if added to ( 12 , 12 ) , give additional equivalent positions. If two mirror planes at right angles (point group mm) are combined with the rectangular lattice we get diads at the intersections of the mirrors as in pmm, No. 6. If one or both of the mirrors is replaced by g, the diads no longer lie at the intersections (see pmg, No. 7 and pgg, No. 8). The group cmm, No. 9, necessarily involves the presence of two sets of glide reflection lines, while p4, No. 10, denotes the square lattice and point group 4, which together necessarily involve the presence of diads. However, mirror planes are not required. If 4 lies at the intersection of two sets of mirrors we have p4m, No. 11, the diagonal glide reflection line necessarily being present. However, 4 can also lie at the intersection of two sets of glide reflection lines, in which case again two sets of mirrors arise but the mirrors intersect in diads, giving point group symmetry mm at these points (No. 12). The triequiangular net and point group 3 give the space group p3 (No. 13). If mirror planes are combined with the triad axis – the combination of the point group 3m and the triequiangular net – it is found that the mirrors can be arranged in two different ways with respect to the points of the net, yielding p31m and p3m1 (Nos. 14 and 15). With the hexagonal point group 6mm, which necessarily has two sets of mirrors, this duality does not arise and the two space groups are p6 and p6mm (Nos. 16 and 17).

2.13

Nomenclature for Point Groups and Space Groups

The nomenclature we have introduced in this chapter to describe point groups and space groups conforms to a notation known as the Hermann–Mauguin notation arising from the work of Carl Hermann [9] and Charles-Victor Mauguin [10] and used in the Internationale Tabellen zur Bestimmung von Kristallstrukturen, edited by Hermann and published in 1935. However, another notation for describing point group and space group symmetry is also in common use. This second notation, known as the Schoenflies notation, is named after Arthur Moritz Schoenflies [11]. This latter notation is used in particular in physical chemistry in connection with molecular symmetry and molecular spectroscopy [12], and it is also useful when considering group theoretical aspects of point groups and space groups [13]. The equivalence between the Hermann–Mauguin notation and the Schoenflies notation is discussed in detail by Hans Burzlaff and Helmut Zimmerman in Chapter 12 of

Kelly_c02.indd 78

11/30/2011 7:32:51 PM

Point Groups and Space Groups

79

International Tables for Crystallography [3]. The reason why the Hermann–Mauguin notation might be preferred over the Schoenflies notation is neatly summarized by Phillips [2]: ‘each space group symbol [in the Hermann–Mauguin notation] conveys all the essential information, whereas we must always have a catalogue at hand to follow an arbitrary serial numbering such as that of Schoenflies’ (p. 340).

2.14

Groups, Subgroups and Supergroups

It is evident from the discussion in this chapter on point groups and space groups that each point group and space group consists of a self-consistent finite set of symmetry operations. Therefore, point groups and space groups can be described in the formalism of group theory [13–15]. A group G is a set of elements g1, g2, g3 … gn which conform to the following four conditions [15]: 1. The product gigj of any two group elements must be another element within the group. 2. Group multiplication is associative: (gigj)gk = gi(gjgk). 3. There is a unique group element I called the identity element belonging to G so that its operation on a member of the group gi is such that Igi = giI = gi. 4. Each element within the group has a unique inverse; that is, for each gi there is a unique element gi−1 so that gigi−1 = gi−1 gi = I. Thus, for example, following the example of the point group mmm used by de Jong [5], p. 20, the eight group elements within this point group are: the identity, I; three 180° rotations about the x-, y- and z-axes; three reflections in the (100), (010) and (001) planes; and a centre of symmetry. A subgroup of these symmetry elements is found in 2mm: the identity, a 180° rotation about the x-axis and two reflections in the (010) and (001) planes. – Other subgroups are the point groups 222, 2/m, m, 2, 1 and 1. Conversely, the point group mmm is clearly a supergroup for 2mm and 222. Similar principles apply to subgroups and supergroups of space groups. Thus, for example, following Hans Wondratschek in Chapter 8 of International Tables for Crystallography – [3], the space group P6 2m is one member of the group whose minimal nonisomorphic – supergroup is P63/mcm; it has as maximal nonisomorphous subgroups P6 , P321, P31m and Pm2m. (Groups are termed isomorphic if they have an equivalent group multiplication structure but differ in the nature of the elements constituting them [15]. Thus, for example, the point groups 2/m, 222 and 2mm are isomorphic: all three have four elements within the group and the same multiplication structure within them.)

2.15 An Example of a Three-Dimensional Space Group To illustrate the principles we have outlined in Sections 2.12–2.14, an example of an entry in the most recent edition of the International Tables for Crystallography is shown in Figure 2.25. It is apparent from the Hermann–Mauguin notation of this space group, Pnma, No. 62, that crystals with this space group symmetry belong to the orthorhombic crystal 16 system, point group mmm. The Schoenflies notation D2h indicates that the space group is dihedral (or two-sided; from the ‘D’), that it has a 2-fold rotation axis (from the ‘2’), that

Kelly_c02.indd 79

11/30/2011 7:32:54 PM

Crystallography and Crystal Defects

80

D16 2h

Pnma No. 62

Orthorhombic

mmm

Patterson symmetry P m m m

P 21/n 21/m 21/a 21 21 21 P– – –a nm 1 4

1 4

1 4

1 4

2 21 21 P n–1 – – am

1 4

1 4

1 4

2 2 2 P –1 –1 –1 b n m

21 21 21 Pm – –n –b

1 4

1 4

1 4

2 2 2 P –1 –1 –1 cm n 1 4

1 4

1 4

1 4 –

,

–

2 2 2 P –1 –1 –1 mc n

+

+

–

,

,

+

, 1+ 1 +

1+ 2

2

2

, 1–

, 1 – 1– 2 2 –

,

– +

1 4

1 4

2

+

–

,

,

+

1 4

– Origin at 1 on 1211 Asymmetric unit 0 ≤ x ≤ 12 ; 0 ≤ y ≤ 14 ; 0 ≤ z ≤1 Symmetry operations (2) 2 (0,0, 12 )

(1) 1 –

(5) 1 0,0,0

(6) a x,y, 14

1 4 ,0,z

(3) 2(0, 12 ,0) 0,y,0

(4) 2( 12,0,0) x,41 , 41

(7) m x, 14, z

(8) n(0, 12 , 12 ) 14 ,y,z

Figure 2.25 An example of a space group. (Taken from [3].)

there is in addition a mirror plane perpendicular to this 2-fold axis (from the ‘h’ subscript) 1 28 and that it is the 16th of 28 such space groups D2h … D2h (space groups 47–74 inclusive), all of which are space groups derived from the mmm point group. The full Hermann–Mauguin notation for this space group is P21/n 21/m 21/a, showing that there are three mutually perpendicular sets of screw diads in addition to the mirror, m, and the diagonal, n, and axial, a, glide planes. The diagrams of the symmetry elements of the group follow the principles in Figure 2.24, with the use of standard graphical symbols for n (parallel to (100) ) and a (parallel to (001) ). The projections in the top left-hand corner and the bottom right-hand corner are both down [001], the one in the top right-hand corner down [010] and the one in the bottom left-hand corner down [100]. The asymmetric unit is ‘a (simply) connected smallest part of space from which, by application of all symmetry operations of the space group, the whole of space is filled

Kelly_c02.indd 80

11/30/2011 7:32:54 PM

Point Groups and Space Groups CONTINUED

No. 62

81

Pnma

Generators selected (1); t(1,0,0); t(0,1,0); t(0,0,1); (2); (3); ( 5) Positions Multiplicity, Wyckoff letter, Site symmetry 8

4 4 4

d

c b a

1

Coordinates

Reﬂection conditions General:

(1) x, y, z

– z + –1 (2) x– + –12 , y, 2

– y + –1 , z– (3) x, 2

y + –12 , –z + –12 (4) x + –12 , –

– –y, –z (5) x,

–12 ,

y, –z + –12

(7) x, –y + –12 , z

(8) x– + –12 , y + –12 , z + –12

(6) x +

m

x, –14 , z

x– + –12 , –34 , z + –12

– 1 – 1

0, 0, –12

–12 , 0, 0

0, 0, 0

–12 ,

0, –12

Symmetry of special projections Along [001] p2gm a' = –12 a b' = b Origin at 0, 0, z Maximal non-isomorphic subgroups I

[2] Pn21a (Pna21, 33) [2] Pnm21 (Pmn21, 31) [2] P21ma (Pmc21, 26) [2] P212121 (19) [2] P1 1 21/a (P21/c, 14) [2] P21/n11 (P21/c, 14) [2] P121/m1 (P21/m, 11)

IIa IIb

none none

– –3 , –z x, 4

x + –12 , –14 , –z + –12

0kl : k + l = 2n hk0 : h = 2n h00 : h = 2n 0k0 : k = 2n 00l : l = 2n Special: as above, plus no extra conditions

1 – 1 0, – 2, 2

–12 , –12 , 0

hkl : h + l, k = 2n

1 0, –2 ,

–12 , –12 , –12

hkl : h + l, k = 2n

0

Along [010] p2gg a' = c b' = a Origin at 0, y, 0

Along [100] c2mm a' = b b' = c Origin at x, –14 , –14

1; 3; 6; 8 1; 2; 7; 8 1; 4; 6; 7 1; 2; 3; 4 1; 2; 5; 6 1; 4; 5; 8 1; 3; 5; 7

Maximal isomorphic subgroups of lowest index IIc [3] Pnma (a' = 3a) (62); [3] Pnma (b' = 3b) (62) ;[3] Pnma (c' = 3c) (62) Minimal non-isomorphic supergroups I none [2] Amma (Cmcm, 63); [2] Bbmm (Cmcm, 63); [2] Ccme (Cmce, 64); [2] Imma (74); [2] Pcma (b' = –12 b) (Pbam, 55); II [2] Pbma (c' = –12 c) (Pbcm, 57); [2] Pnmm (a' = –12 a) (Pmmn, 59)

Figure 2.25

(continued)

exactly’ [3]. The listing under the heading ‘Symmetry Operations’ in Figure 2.25 is a summary of the various geometric descriptions of each of the eight symmetry operations in the

(

1

)

1

space group, numbered (1)–(8). Thus, for example, here the second of these, 2 0,0, 2 4 , 0, z, 1 defines the screw diad parallel to [001] intersecting the x–y plane at ( 4 , 0). The ‘Generators Selected’ define the order in which the coordinates of the symmetrically equivalent positions are produced; for example, the coordinates related by symmetry to the general position x, y, z in the space group. (1) is the identity operation, showing that in this case integral lattice translations produce the equivalent point in adjacent unit cells. After the ‘Positions’, which follow the protocol described in Section 2.12, and the ‘Symmetry of

Kelly_c02.indd 81

11/30/2011 7:32:54 PM

82

Crystallography and Crystal Defects

Special Projections’, which are self-explanatory, a summary is given of subgroups and supergroups related to the space group under consideration, following the methodology set out in Chapter 2 of International Tables for Crystallography [3]. Finally, the reflection conditions listed under ‘Positions’ specify the systematic absences which occur under kinematical diffraction conditions, such as X-ray diffraction.

Problems Material in Appendices 1 and 2 may be useful; in Problem 2.12 the material in Appendix 4 may also be useful. 2.1 Using Figure 2.13, confirm that in the four-index notation for a plane with indices (hkil): i = −(h + k ) (Equation 2.2.) Confirm also that the condition for a four-index vector [uvtw] to lie in a four-index plane (hkil) is: hu + kv + it + lw = 0 2.2 Show that the angle g between any of the crystal axes and the unique triad axis in a trigonal crystal is given by: sin γ =

2 sin α /2 3

2.3 The corners of a wooden model of a cube are cut off to make equal faces of the form – – – – {111}. The first four new faces are cut in positions (111), (111), (1 11) and (111 ), in that order. Draw sketch stereograms to show the symmetry elements shown by the model after each new face is formed. What is the crystal system of the model in each case? 2.4 (a) Sketch stereograms showing the operation of the undermentioned symmetry elements on two distinct poles, each in a general position, and insert the symmetry elements themselves, except the centre of symmetry: centre of symmetry vertical plane of symmetry horizontal plane of symmetry vertical axes 2, 3, 4, 6 – – – – vertical inversion axes 2, 3, 4 , 6 horizontal axes 2, 4 – horizontal inversion axis 4 . – (b) The symbol X /m is not used in conventional point group notation. Draw sketch stereograms of the poles of one general form for each possible value of X and hence derive the conventional symbols that are actually used. – – 2.5 (a) In which of the trigonal classes 3, 3, 3m, 32, 3m does a rhombohedron occur as a special form? In what class is the rhombohedron the general form? – – (b) Which of the tetragonal classes 4, 4 , 4/m, 422, 4mm, 4 2m, 4/mmm have closed forms as their general forms?

Kelly_c02.indd 82

11/30/2011 7:32:58 PM

Point Groups and Space Groups

83

– – – (c) To which of the cubic classes 23, m3, 432, 4 3m and m3m could a crystal belong which had the shape of (i) an octahedron, (ii) a tetrahedron or (iii) an icositetrahedron? (The icositetrahedron is the name given to the {112} form with 24 faces.) 2.6 In a holosymmetric cubic crystal the angle between (110) and a face P which lies in the zone [010] is 53.97°. Find the indices of P and calculate the angle between P and – the face P′ related to P by the mirror plane parallel to (110). Determine the indices – [uvw] of the zone containing P and P′ and calculate the interzone angle [uvw]∧[110]. – 2.7 (a) Calculate the angle between [0001] and [1123] in beryllium (hexagonal, a = 2.28 Å, – – c = 3.57 Å). What face lies at the intersection of the zones [1123] and [2113]? (b) In a crystal of calcite (trigonal; c/a = 0.8543), a face lies in the zone – – – between (1011) and (1101) at an angle of 16.50° from (1011). Determine the indices of this face. 2.8 In an orthorhombic crystal (topaz) with axial ratios a:b:c = 0.529:1:0.477, the following angles were measured to the face P of the general form: (100)∧P = 67.85°, (010)∧P = 66.5°. Determine the indices of P. 2.9 Calculate the axial ratios a : b : c and the axial angle b for a monoclinic crystal – – – (gypsum) given that (110)∧(110) = 68.5°, (001)∧(110) = 82.3° and (001)∧(101) = 33.1°. – – 2.10 (a) In a hexagonal zeolite crystal the angle (1010)∧(1011) is found to be 37.2°. Calculate the axial ratio c/a and specify the indices of the zone containing both faces in (i) conventional three-dimensional indices and (ii) the Miller–Bravais 4-index notation. – (b) Show that (0001)∧(1122) = 48.8°. Hence, construct a stereogram centred on 0001 – – – – showing all the poles of the form {1010}, {1011}, {1120} and {1122} for this zeolite. 2.11 a-sulphur forms orthorhombic holosymmetric crystals with a = 10.48 Å, b = 12.92 Å and c = 24.55 Å. (a) Draw a sketch stereogram showing the symmetry elements shown by a-sulphur. (b) Calculate the angles (001)∧(011) and (100)∧(110). Insert these poles on a stereogram. (c) Hence, draw an accurate stereogram of sulphur showing all the faces of the forms {100}, {010}, {001}, {101}, {110}, {111}, {011} and {113}. Index all the faces in the upper hemisphere. Which of these are general and which are special forms? 2.12 In dealing with some imperfect crystals with a cubic face-centred lattice it is convenient to use a hexagonal unit cell. The cubic face-centred lattice can be referred to a hexagonal cell where the z-axis is parallel to [111] and of magnitude 3a , where a is the lattice parameter of the conventional cubic unit cell and the x- and y-axes are parallel to the 〈1 0 1〉 directions perpendicular to [111] and of magnitude a / 2 . (a) Draw a diagram showing the relation between the two unit cells. (b) Write the hexagonal lattice vectors in terms of the cubic lattice vectors. Hence, derive the matrix for transforming the indices of lattice planes.

Kelly_c02.indd 83

11/30/2011 7:33:01 PM

84

Crystallography and Crystal Defects

(c) Find the ratio of the volumes of the two unit cells by the matrix method and check by direct calculation. How many lattice points does each contain? – (d) Obtain the hexagonal indices of the planes with indices (112), (100) and (110) referred to the conventional cubic cell.

Suggestions for Further Reading See the suggestions for Chapter 1 as well as the following: T. Janssen (1973) Crystallographic Groups, North-Holland, Amsterdam. W.A. Wooster (1973) Tensors and Group Theory for the Physical Properties of Crystals, Clarendon Press, Oxford.

References [1] M.J. Buerger (1963) Elementary Crystallography, John Wiley and Sons, New York. [2] F.C. Phillips (1971) Introduction to Crystallography, 4th Edition, Oliver & Boyd, Edinburgh. [3] T. Hahn (ed.) (2002) International Tables for Crystallography, 5th, Revised Edition, Vol. A: Space-Group Symmetry, published for the International Union of Crystallography by Kluwer Academic Publishers, Dordrecht. [4] N.F.M. Henry and K. Lonsdale (eds.) (1952) International Tables for X-Ray Crystallography, Volume I, International Union for Crystallography–Kynoch Press, Birmingham, England. [5] W.F. de Jong (1959) General Crystallography: A Brief Compendium, W.H. Freeman, New York. [6] M.A. Carpenter and C.J. Howard (2009) Symmetry rules and strain/order-parameter relationships for coupling between octahedral tilting and cooperative Jahn–Teller transitions in ABX3 perovskites. I. Theory, Acta Crystall. B, 65, 134–146. [7] M.A. Carpenter and C.J. Howard (2009) Symmetry rules and strain/order-parameter relationships for coupling between octahedral tilting and cooperative Jahn–Teller transitions in ABX3 perovskites. II. Application, Acta Crystall. B, 65, 147–159. [8] C.J. Howard and M.A. Carpenter (2010) Octahedral tilting in cation-ordered Jahn–Teller distorted perovskites – a group-theoretical analysis, Acta Crystall. B, 66, 40–50. [9] C. Hermann (1928) Zur systematischen Strukturtheorie I. Eine neue Raumgruppensymbolik, Z. Kristall., 68, 257–287. [10] C. Mauguin (1931) Sur le symbolisme des groupes de répétition ou de symétrie des assemblages cristallins, Z. Kristall., 76, 542–558. [11] A. Schoenflies (1891) Krystallsysteme und Krystallstructur, B.G. Teubner, Leipzig. [12] P.W. Atkins and J. De Paula (2009) Atkins’ Physical Chemistry, 9th Edition, Oxford University Press, Oxford. [13] G. Burns and A.M. Glazer (1990) Space Groups for Solid State Scientists, 2nd Edition, Academic Press, New York. [14] J. Mathews and R.L. Walker (1970) Mathematical Methods of Physics, 2nd Edition, Addison-Wesley, Reading, MA. [15] K.F. Riley, M.P. Hobson and S.J. Bence (2006) Mathematical Methods for Physics and Engineering, 3rd Edition, Cambridge University Press, Cambridge.

Kelly_c02.indd 84

11/30/2011 7:33:04 PM

3 Crystal Structures 3.1

Introduction

The relative positions of the atoms in crystals can be deduced from measurements of the relative intensities of the diffraction spectra using X-rays, electrons or neutrons. X-rays are most useful in this regard because the intensities of the diffracted waves are not as affected by crystalline perfection as are those obtained with electrons. Neutron diffraction is a more specialised technique than X-ray diffraction or electron diffraction, but has distinct advantages when determining the crystal structures of low-atomic-number materials and when locating the atomic positions of elements such as hydrogen in a material. Careful measurements of the spectra enable the electron density to be found throughout the unit cell of a crystal. Since only the outermost electrons are involved in binding the atoms together in a crystal, most of the electrons in the crystal reside in orbits that are the same as those in an isolated atom. The crystal structure can therefore be described by stating the relative positions of atoms within the unit cell. In many crystals of both elements and compounds the charge distribution of the outermost electrons, which are not involved in the chemical binding, are more or less spherically symmetric and therefore the crystal structure is sometimes regarded as being composed of spheres of the same size (if the crystal structure of an element is being considered) or of different sizes (corresponding to the different atoms in a chemical compound) packed together. The crystal structures of the stable elements and of most simple compounds are now well established. These are listed in the Suggestions for Further Reading given at the end of this chapter. We shall now describe a number of the structures, emphasizing the geometrical features of the relative arrangement of the atoms. The imperfections in these crystals, such as point defects, dislocations and grain boundaries, will be described in Part II. When describing each crystal structure we shall state the space group in the style given in the International Tables for Crystallography [1] because from this symbol the Bravais lattice

Crystallography and Crystal Defects, Second Edition. Anthony Kelly and Kevin M. Knowles. © 2012 John Wiley & Sons, Ltd. Published 2012 by John Wiley & Sons, Ltd.

Kelly_c03.indd 85

11/30/2011 4:07:02 PM

86

Crystallography and Crystal Defects

and the point group of the crystal are immediately known (see Section 2.12). Other ways of describing crystal structures are described in Section 3.10. We shall first describe the structures of some of the elements and then those of simple compounds. In many cases a given element or compound possesses more than one crystal structure, each being the thermodynamically stable form in a given regime of temperature and pressure. When this is the case, an element is said to show allotropy and a compound is spoken of as polymorphous. In describing the crystal structures of some compounds we shall sometimes refer to the chemical formulae as being of the type MX, M denoting a metal ion or atom and X an electro-negative element, such as O, F, Cl and so on. Crystal structures can be described by stating the lattice and the coordinates of the atoms in terms of the cell sides as units of length, referred to the lattice point at the origin. In multiply primitive unit cells the same arrangement of atoms must, of course, occur around every lattice point.

3.2

Common Metallic Structures

The vast majority of the elements are metallic. With notable exceptions such as manganese (Mn), gallium (Ga), indium (In), tin (Sn), mercury (Hg), polonium (Po), protoactinium (Pa), uranium (U) and plutonium (Pu) (see Appendix 7), the metallic elements all possess one of four structures: either the cubic close-packed (c.c.p.), hexagonal close-packed (h.c.p.), double hexagonal close-packed (double h.c.p.) or body-centred cubic (b.c.c.). The c.c.p. structure is also frequently referred to as face-centred cubic (f.c.c.); however, we will use the designation c.c.p. here to distinguish clearly between the face-centred cubic1 Bravais lattice and the c.c.p. crystal structure. 3.2.1

– Cubic Close-Packed (Fm3m)

The noble metals (Cu, Ag, Au), the metals of higher valence (Al and Pb), the later transition metals (Ni, Rh, Pd, Ir, Pt) and the inert gases (Ne, Ar, Kr, Xe) when in the solid state all possess this structure (see Appendix 7), as does Fe between 912 and 1394 °C and Co above 420 °C. The lattice is face-centred cubic and there is one atom associated with each lattice point. A conventional unit cell of the structure with lattice parameter a is shown in Figure 3.1a. The conventional unit cell has four lattice points, and therefore four atoms, per unit cell. The relationship of this unit cell to the primitive rhombohedral unit cell for this crystal structure is shown in Figure 3.1b. The coordinates of the atoms in the conventional unit cell are therefore (0, 0, 0), ( 12 , 12 , 0) ,

( 12 , 0, 12 ) and (0, 12 , 12 ) . Each atom possesses 12 nearest neighbours at a distance of a /

2 . The coordination number is thus 12. This structure is the one obtained if equal spheres are placed in contact at the lattice points of a face-centred cubic lattice. A diagram illustrating this is shown in Figure 3.2a. An alternative packing arrangement of equal spheres which produces the hexagonal close-packed structure is shown in Figure 3.2b (Section 3.2.2). If the radius of the spheres is R then R = a / (2 2). The proportion of space filled by the spheres in the c.c.p.

1

Kelly_c03.indd 86

Also known as a cubic face-centred lattice; the two terms are identical.

11/30/2011 4:07:03 PM

Crystal Structures (a)

87

(b)

a

Figure 3.1 (a) The conventional unit cell of the c.c.p. crystal structure. (b) The primitive unit cell of the c.c.p. crystal structure shown within the conventional unit cell (a)

(b)

Figure 3.2 Close packing of equal spheres. (a) Cubic close-packed (c.c.p.). The close-packed layers are parallel to the darker balls. (b) Hexagonal close-packed (h.c.p.). The close-packed layers are horizontal. (After Bragg and Claringbull [9].)

crystal structure is π / (3 2) or 74%. This is described by saying that the packing fraction is 0.74. A packing fraction of 0.74 is the closest packing of equal spheres that can be achieved [2–8], and is the closest packing that can be achieved with equal spheres at the lattice points of a Bravais lattice (see Section 3.6). Rows of spheres are in contact along the line joining their centres. These lines are 〈1 1 0〉 directions in the lattice. Such directions are the closest packed and are termed close-packed directions. There are 12 such directions in all, if account is taken of change in sign. Taking the atomic centres to be at the lattice points, it is apparent from Figure 1.27 that in the {1 1 1} planes, which lie normal to triad axes, the atom centres form a triequiangular net of points. If the atoms are spheres of radius a /2 2 , the appearance of a {1 1 1} plane is

Kelly_c03.indd 87

11/30/2011 4:07:09 PM

88

Crystallography and Crystal Defects

A

A C

C

B A

1] a [121] 6

B A

C

C

a [01 2

B

B A

a [112] 6

A

A C

B

B A

A

B A

Figure 3.3

shown by the full circles in Figure 3.3. Each sphere is in contact with six equidistant spheres with centres in the plane. Since the arrangement shown in Figure 3.3 is the closest packing of circles in a plane, the {111} planes are spoken of as being closest packed, or close-packed. There are eight such planes in the lattice if distinction is drawn between parallel normals of – – – opposite sense (so that, for example, (11 1) and (1 11) are counted separately) and each contains six close-packed directions. The spacing of the {111} planes is a / 3 = 2 2/3 R and so is equal to 2/3 of the atomic spacing in the {111} planes. The centres of the atoms in a particular (111) plane occupy points such as A in Figure 3.3. If the positions of the centres of the atoms in adjacent (111) planes are projected on to this (111) plane, they occupy positions such as those marked B or C in Figure 3.3. The projections of the spheres centred on points B are shown dotted in the figure. A given crystal can be considered to be made up by stacking, one above the other, successive planar rafts of closest-packed spheres so that proceeding in the [111] direction the centres of the atoms in adjacent rafts follow the sequence ABCABCABC… (Figure 3.4a). The same crystal structure, but in a different orientation, would be described by the sequence of rafts ACBACBACB… Any atom in a c.c.p. crystal has 12 nearest neighbours along < 110 > directions at a distance of a / 2 (= 2R), 6 second-nearest along < 100 > directions at a (= 2 2 R) , 24 third-nearest along < 211 > directions at 3/2 a(= 2 3 R) and 12 fourth-nearest along < 110 > directions at

Kelly_c03.indd 88

2 a( = 2 4 R ) .

11/30/2011 4:07:12 PM

Crystal Structures

89

A

(a) A

A A

(b)

C

A

A

C C

A B

B B B

B B

A

A A

A

A A

Figure 3.4 The stacking of closest-packed planes in (a) the c.c.p. structure and (b) the h.c.p. structure

When the c.c.p. crystal structure is regarded as being made up of spheres in contact, the size of the interstices between spheres is important, because many other crystal structures contain at least one set of atoms in either a c.c.p. arrangement or a very close approxima-

tion to it. The largest interstice occurs at positions in the unit cell with coordinates ( 12 , 12 , 12 ) and equivalent positions ( i.e. 0, 12 , 0; 0, 0, 12 and 12 0, 0 ). There are four of these interstice s per unit cell and, hence, one per lattice point; one is illustrated in Figure 3.5. The largest sphere which can be placed in this position without disturbing the arrangement of spheres at the lattice points has radius r = ( 2 − 1) R = 0.414 R. This sphere would have octahedral coordination with six nearest neighbours (Figure 3.5); for this reason these interstices are commonly referred to as octahedral interstices. The sites of these octahedral interstices by themselves form a face-centred cubic lattice.

The second largest interstice occurs at points with coordinates ( 14 , 14 , 14 ) and equivalent positions (Figure 3.6). The largest sphere which can be placed here has radius r = ( 3/2 − 1) R = 0.225 R and possesses tetrahedral coordination; for this reason these interstices are commonly referred to as tetrahedral interstices. There are eight such points in the unit cell and hence two per lattice point. If the atoms in the c.c.p. crystal structure are ignored, the sites of the tetrahedral interstices can be seen to lie on a primitive cubic lattice.

Kelly_c03.indd 89

11/30/2011 4:07:19 PM

90

Crystallography and Crystal Defects

x

Figure 3.5 The largest interstice in the c.c.p. structure: the octahedral interstice

x

Figure 3.6 The second largest interstice in the c.c.p. structure: the tetrahedral interstice

3.2.2

Hexagonal Close-Packed (P63 /mmc)

This structure is exhibited by the early transition metals Sc, Ti, Y and Zr, by the divalent metals Be, Mg, Zn and Cd, and by a number of the rare earth metals (see Appendix 7). The hexagonal primitive unit cell contains two atoms with coordinates (0, 0, 0) and ( 23 , 13 , 21 ) (Figure 3.7). Hence, there are two atoms associated with each lattice point. There is no pure rotational hexagonal axis, but instead 63 axes located at 00z; that is, at the origin of the unit cell (and equivalent sites) running parallel to the z-axis. This structure can be produced by packing together equal spheres, as shown in Figure 3.2b. If each sphere has 12 nearest neighbours equally far away from it, the axial ratio c/a must equal 8/3 = 1.633 . The packing fraction is then 0.74, as in the c.c.p. structure.

Kelly_c03.indd 90

11/30/2011 4:07:25 PM

Crystal Structures

91

c

y

x

a

Figure 3.7 The unit cell of the h.c.p. structure Table 3.1 Axial ratios at room temperature of some metals with an h.c.p. crystal structure Metal Cd Zn Co Mg Re

c/a

Metal

c/a

1.886 1.857 1.625 1.624 1.615

Sc Zr Ti Y Be

1.597 1.593 1.587 1.571 1.568

Values of the axial ratio for a number of metals with this structure are given in Table 3.1. Cobalt has an axial ratio very close to the ideal. It is noteworthy that there are significant departures from the ideal axial ratio: Ti and Zn, for example. If the atomic centres are projected on to a plane parallel to (0001), the basal plane, the structure can be regarded as being made up by stacking rafts of spheres in the sequence ABABAB or ACACAC (Figures 3.3 and 3.4b). If c/a is equal to or greater than the ideal value for sphere packing, there are six – directions of the type 〈1 1 2 0〉 in the basal plane along which atoms touch, and these are the only close-packed directions. If c/a is less than the ideal value, spheres will not touch along these directions, but will be sufficiently close to one another that they can to all intents be regarded as close-packed directions. Octahedral interstices in the h.c.p. crystal structure have coordinates ( 13 , 23 , 14 ) and ( 13 , 23 , 43 ) (Figure 3.8a). There are two such interstices per unit cell and hence one per atom. If c/a = 8/3 then the largest sphere that can be inserted without disturbing the spheres of radius R packed in contact has radius r = 0.414R, just as in the c.c.p. crystal structure. The second-largest interstices, the tetrahedral interstices, lie at 0, 0, 83 , 0, 0, 85 , ( 23 , 13 , 81 ) and ( 23 , 13 , 87 ) (Figure 3.8b). There are four such interstices per cell and hence two per

(

atom. If c/a =

Kelly_c03.indd 91

) (

)

8/3 these have r/R = 0.225, again, just as in the c.c.p. crystal structure.

11/30/2011 4:07:28 PM

92

Crystallography and Crystal Defects (a)

(b)

X

X y

y

x

x

Figure 3.8 Interstices in the h.c.p. arrangement. The octahedral interstices in (a) are denoted by X and the tetrahedral interstices in (b) by open circles

3.2.3

Double Hexagonal Close-Packed (P63 /mmc)

In the eight rare earth metals La, Pr, Nd, Pm, Am, Cm, Bk and Cf, the hexagonal close packing is a four-layer repeat, ABAC. This crystal structure is often referred to as the double h.c.p. structure. The axial ratios characteristic of these metals vary between 3.192 for Pm and 3.262 for Cf, so that in each case they are just below the ideal value of 2 8/3 = 3.266. There are four atoms per unit cell, one octahedral interstice per atom and two tetrahedral interstices per atom. 3.2.4

– Body-Centred Cubic (Im3m)

This structure is shown by the alkali metals Li, Na, K, Rb and Cs, and by the transition metals V, Cr, Fe, Nb, Mo, Ta and W. It is also shown by Ti and Zr at high temperature. The lattice is b.c.c. with one atom at each lattice point, so the atomic coordinates are (0, 0, 0) and ( 12 , 12 , 12 ) (Figure 3.9). Each atom has eight nearest neighbours along 〈111〉 directions at a separation of 3a /2, where a is the lattice parameter. These eight 〈111〉 directions are close-packed directions. Unlike in the c.c.p. and h.c.p. structures, none of the nearest neighbours of one particular atom are nearest neighbours of each other. If the b.c.c structure is presumed to be made up with spheres of equal size, these each have radius R = 3a /4. The packing fraction is π 3 /8 = 0.68. The second-nearest neighbours of an atom are closer than in the c.c.p. structure. There are six second-nearest neighbours along directions at a distance 4 R / 3 = 2.309R (in c.c.p., second-nearest neighbours are at 2 2R = 2.828R) and 12 third-nearest along directions at 4 2 R / 3. There are no closest-packed planes of atoms in this structure. This structure has its largest interstices at coordinates ( 12 , 14 , 0 ) and equivalent positions (Figure 3.10). There are 12 such positions per cell: six per lattice point, and therefore six per atom. The largest sphere fitting in such an interstice has radius r = 5/3 − 1 R = 0.291R. This interstice is therefore significantly smaller than the largest one in c.c.p. It has four nearest neighbours equidistant from it, and so it is a tetrahedral interstice, but the tetrahedron

(

Kelly_c03.indd 92

)

11/30/2011 4:07:41 PM

Crystal Structures

93

a

Figure 3.9 The b.c.c crystal structure

X

O

O = 1, 1, 0 2 2 X = 12 , 14 , 0

Figure 3.10 Tetrahedral (X) and octahedral (O) interstices in the b.c.c crystal structure

that these neighbours form is not regular. The second-largest interstice is at ( 12 , 12 , 0) and equivalent positions (Figure 3.10). There are six such sites per cell ( 6 × 12 at the centres of cube faces and 12 × 14 at the midpoints of cube edges) and so three per lattice point. Each can accommodate a sphere of radius r = (2/ 3 − 1) R = 0.155R; such a sphere is at the centre of a distorted octahedron, and so these interstices are distorted octahedral interstices.

3.3 3.3.1

Related Metallic Structures Indium (I4 /mmm)

The crystal structure of indium is very similar to the c.c.p. structure. It is body-centred tetragonal with c/a = 1.521. This axial ratio is such that, if referred to a face-centred tetragonal lattice instead of the conventional body-centred one, the axial ratio c/a = 1.076.

Kelly_c03.indd 93

11/30/2011 4:07:55 PM

94

Crystallography and Crystal Defects

Therefore, the structure can be described as face-centred tetragonal (F4/mmm), with one atom at each lattice point and an axial ratio of 1.076. 3.3.2

– Mercury (R3m)

Mercury also has a structure that can be described as distorted c.c.p. The primitive unit cell has a rhombohedral lattice with one atom at each lattice point (Figure 3.11). The axial angle a is 70.74° and a = 2.992 Å at 78 K. The primitive unit cell of a c.c.p. crystal has a = 60° (Figure 3.1b). Thus the mercury structure can be derived from the c.c.p. crystal structure by compressing it along a body diagonal of the cell. The atoms in the (111) planes of mercury are therefore arranged to form a triequiangular net but the spacing of these planes is too small to allow closest packing of spherical atoms. The nearest neighbours of any one atom are in adjacent (111) planes. The closest-packed directions are 〈100〉 of the primitive rhombohedral cell of side a (Figure 3.11). There are six nearest neighbours at a distance a. Mercury can, of course, also be referred to a rhombohedral face-centred cell containing four atoms to emphasize the relationship to the conventional cell of an c.c.p. crystal. This larger cell for Hg has a′ = 4.577 Å and axial angle a ′ = 98.36° at 78 K (see Problem 3.4). 3.3.3

b-Sn (I41/amd)

b-Sn, also known as white tin, is the form of tin that is stable at room temperature. It has a body-centred tetragonal lattice with two atoms associated with each lattice point: one at the lattice point and the other at 0, 12 , 14 . The value of c/a at room temperature is 0.546. Each atom has four nearest neighbours at the vertices of an irregular tetrahedron and two more at a slightly greater distance (see Problem 3.5). The structure is a distorted form

(

)

a

a

Figure 3.11 The crystal structure of mercury, showing the primitive rhombohedral unit cell

Kelly_c03.indd 94

11/30/2011 4:08:00 PM

Crystal Structures

95

of the diamond structure (Section 3.4.), which is taken by the form of tin stable below room temperature known as a-Sn or grey tin.

3.4 3.4.1

Other Elements and Related Compounds – Diamond (Fd3m)

The elements Si, Ge, a-Sn (the low-temperature allotrope of tin) and crystalline carbon stable at high temperature and pressure (diamond) all have the structure shown in Figure 3.12. The Bravais lattice is face-centred cubic and there are two atoms associated with each lattice point. The coordinates of these atoms can be taken to be (0, 0, 0) and ( 14 , 14 , 14 ) , or, if the origin is taken to be at a centre of symmetry, ± 81 , 81 , 81 . The coordination number is 4, with the nearest neighbours at a distance 3a /4 arranged at the corners of a regular tetrahedron, outlined in Figure 3.12. The atom centres lie at the corners of triequiangular nets in {111} planes. If these are projected on to (111) the stacking sequence of successive (111) planes can be described as CA AB BC CA AB BC. Successive planes are not equally separated from one another (Figure 3.13). The structure is very loosely packed. If equal spheres in contact have their centres at the atom centres, the packing fraction is only π 3 /16 = 0.34. The diamond crystal structure can be regarded as a special case of the sphalerite crystal structure (sub-section 3.5.3), in which the atoms at (0, 0, 0) and ( 14 , 14 , 14 ) are of different types. For this reason, Figure 3.13 can also be used to show the stacking sequence of the sphalerite crystal structure. In – sphalerite, there are no longer centres of symmetry, so the space group symmetry is F43m (Section 3.5).

(

3.4.2

)

Graphite (P63 /mmc)

The thermodynamically stable crystal structure of carbon at room temperature is graphite, shown in Figure 3.14a. The lattice is hexagonal with four atoms per unit cell, with coordinates

y x

a

Figure 3.12 The crystal structure of diamond

Kelly_c03.indd 95

11/30/2011 4:08:01 PM

96

Crystallography and Crystal Defects

[111]

[112] C b

C B a 4 3

B A

B a

A C

A g

C B

C b

B A

a 3

A C

B a A g

Figure 3.13 The stacking of (111) planes in the diamond and sphalerite structures. The atomic positions are projected onto (110). In diamond, the filled and open circles represent the same type of atom. The sequence of triequiangular nets is described for diamond on the left-hand side and for sphalerite (zinc blende) on the right-hand side

(

)(

)

2 1 1 1 2 , , 0 and ( , , ) . At room temperature a = 2.46 Å and c = 6.71 Å; (0, 0, 0), 0, 0, 12 3 3 2 3 3 thus c/a = 2.72 is large. The atoms in one (0001) plane are arranged at the corners of regular hexagons. The x- and y-axes of the unit cell are shown in Figure 1.1. The structure can be built up by stacking successive hexagonal sheets of atoms one above the other along the z-axis so that the hexagons are in the same orientation, but with half the corners of the hexagons in one plane lying in the centres of the hexagons in adjacent planes (Figure 3.14a). If the atomic centres are all projected on to (0001), the stacking sequence can be described as ABABAB or ACACAC, where it must be remembered that the letters A, B and C refer to sheets of atoms arranged at the corners of hexagons, rather than at the vertices of equilateral triangles, as in the h.c.p. crystal structure, for example. Each atom has three nearest neighbours at a separation of a / 3 in the basal plane. Half of the atoms in any one hexagonal layer have atoms directly above and below them at a distance of c/2. The separation of the nearest neighbours in the (0001) planes is only 1.42 Å (compared with 1.54 Å in diamond) and this is much smaller than the separation of the hexagonal sheets – 3.35 Å. Graphite is therefore said to possess a layer structure because the atoms are strongly bonded within a sheet, and the sheets are only weakly bound to one another through van der Waals forces. If graphite crystals are ground or otherwise severely deformed at low temperature, another form of graphite can be detected in which the atomic hexagons are arranged in the sequence ABCABCABC or alternatively CBACBACBA. This crystal structure has a rhom– bohedral Bravais lattice (space group R3m). The primitive rhombohedral cell has a = 3.635 Å

Kelly_c03.indd 96

11/30/2011 4:08:08 PM

Crystal Structures (a)

97

(b)

y

x Graphite

BN

Figure 3.14 (a) The crystal structure of graphite. (b) The crystal structure of hexagonal boron nitride

and a = 39.5° at room temperature. There are two atoms per unit cell with coordinates ±(u, u, u) where u = 61 (= 0.167). 3.4.3

Hexagonal Boron Nitride (P63 /mmc)

The structure of hexagonal boron nitride thermodynamically stable at room temperature is closely related to that of graphite (Figure 3.14b). The atoms occur in hexagonal sheets, but the sheets are stacked directly above one another along [0001] so that the stacking sequence is described as AAAAA…, with unlike atoms above one another in consecutive layers (see Figure 3.14b). In any one sheet there are equal numbers of B and N atoms arranged so that B and N alternate around any one atomic hexagon. At room temperature the B–N separation in the sheets is 1.45 Å and the separation of the sheets is 3.33 Å. – 3.4.4 Arsenic, Antimony and Bismuth (R3m) The structures of As, Sb and Bi are also based on a primitive rhombohedral Bravais lattice, with two atoms associated with each lattice point. The structure is shown in Figure 3.15. The coordinates of the atoms in the rhombohedral unit cell are ±(u, u, u); u is a little less than 14 and a somewhat less than 60° (see Table 3.2). The structure is easily visualized as being made up of sheets of atoms lying perpendicular to [111]. Within each sheet the atoms are arranged at the corners of triequiangular nets. Referring to Figure 3.15 and noting the values of u, the stacking sequence of these nets along [111] is BA CB AC BA… If u is 14 , the spacing of adjacent nets will be regular. In fact, each atom in any one sheet has three nearest neighbours in the closest adjacent sheet at d1 (see Table 3.2) and three at a slightly greater distance in the sheet on the other side at d2. The possession of three nearest neighbours fits with the positions of As, Sb and Bi in the periodic table, since each atom is

Kelly_c03.indd 97

11/30/2011 4:08:12 PM

98

Crystallography and Crystal Defects

A C A C C

C

B C B

B

B A B

A

Figure 3.15 The crystal structure of As, Sb and Bi Table 3.2

As Sb Bi

Cell dimensions of As, Sb and Bi

a (Å)

a (deg)

u

d1 (Å)

d2 (Å)

4.132 4.507 4.746

54.13 57.11 57.23

0.227 0.233 0.234

2.517 2.908 3.071

3.120 3.355 3.529

expected to form three covalent bonds. If a = 60° and u = 14 in this structure, each atom has six closest neighbours and the arrangement of the atoms is at the points of a simple cubic lattice.

3.5

Simple MX and MX2 Compounds – Sodium Chloride, NaCl (Fm3m)

3.5.1

One-third of all compounds of the type MX crystallize in the sodium chloride (halite) – structure (Fm3m), shown in Figure 3.16. In such compounds the metal atom or ion M is usually smaller than the electronegative element, X. The lattice is face-centred cubic with two different atoms associated with each lattice point: one, say X, at (0, 0, 0) and the other, M, at 0, 0, 12 . Each of the two types of atom, considered in isolation, lies upon a facecentred cubic lattice, and each lies at the largest interstice of the other’s face-centred cubic lattice. From the diagram in Figure 3.5 and from inspection of Figure 3.16, it is then clear that each atom has a coordination number of 6, the neighbours being at the vertices of a regular octahedron. There are four formula units per conventional unit cell but there is clearly no trace of the formation of a molecule of MX in this structure.

(

Kelly_c03.indd 98

)

11/30/2011 4:08:16 PM

Crystal Structures

99

Figure 3.16 The crystal structure of sodium chloride, NaCl

Each {111} lattice plane specifies a double sheet of atoms, each of the sheets consisting entirely of atoms of one kind arranged at the points of a triequiangular net. If we denote sheets of atoms of one kind with a Greek letter and those of the other with a Roman letter, then the stacking sequence along a [111] direction can be described as A g B a C b A g B a C b … The spacing of the sheets of atoms denoted by letters from the same alphabet is a / 3 , where a is the lattice parameter. All of the alkali halides, with the exception of CsCl, CsBr and CsI, crystallize with this crystal structure, as do many of the sulfides, selenides and tellurides of Mg, Ca, Sr, Ba, Pb and Mn, as well as the oxides of formula MO of Mg, Ca, Sr, Ba, Cd, Ti, Zr, Mn, Fe, Co, Ni and U and some transition metal carbides and nitrides such as TiC, TiN, TaC, ZrC, ZrN, UN and UC (see Section A7.2 in Appendix 7). When the metallic ion is of variable valence, crystals with this structure often form with some ion positions unoccupied. For example, FeO crystals would be perfect if they contained only divalent iron, Fe2+. If some Fe3+ ions are present then for every two Fe3+ ions, one of the sites on the iron sublattice must be empty. Such a structure is called a defect structure (see Section 10.1). 3.5.2

– Caesium Chloride, CsCl (Pm3m)

CsCl, CsBr, CsI, as well as many intermetallic compounds such as CuBe, CuZn, AgCd, AgMg – and FeAl (see Section A7.3 in Appendix 7), show the caesium chloride structure (Pm3m), which has a primitive cubic lattice with one atom of each kind associated with each lattice point, one, say X, at (0, 0, 0) and the other, M, at ( 12 , 12 , 12 ) (Figure 3.17). The coordination number is 8 for each atom, the nearest neighbours being at

Kelly_c03.indd 99

3a /2 , where a is the lattice parameter.

11/30/2011 4:08:19 PM

Crystallography and Crystal Defects

100

a 90°

90°

90°

a

a

Figure 3.17 The crystal structure of caesium chloride, CsCl

(a)

(b)

c

y a

a x

Figure 3.18 The crystal structures of (a) sphalerite (a-ZnS) and (b) wurtzite (b-ZnS)

3.5.3

– Sphalerite, a-ZnS (F43m)

– The cubic form of ZnS, designated a-ZnS, shows the sphalerite structure2 (F43m) shown in Figure 3.18. This is also exhibited by the sulphides, selenides and tellurides of Be, Zn, Cd and Hg and the halides of Cu and AgI: see Section A7.4 of Appendix 7 for a tabulation of selected crystals with the sphalerite structure. The lattice is face-centred cubic with one atom of each kind associated with each lattice point, one at (0, 0, 0) and the other at ( 14 , 14 , 14 ) , so the relationship to the structure of diamond (Section 3.4) is very close (Figure 3.13). Each type of atom considered in isolation from the other lies at the lattice points of a face-centred cubic lattice and each lies in the second largest interstice of the close-packed crystal structure

2

Kelly_c03.indd 100

Sometimes called zinc blende.

11/30/2011 4:08:23 PM

Crystal Structures

101

Table 3.3 Axial ratios at room temperature of some materials with the wurtzite crystal structure Material NH4F a-AgI BeO ZnO b-ZnS

c/a

Material

c/a

1.61 1.63 1.63 1.60 1.63

b-CdS CdSe AlN SiC TaN

1.62 1.63 1.60 1.65 1.62

of the other. The coordination number is 4, the nearest neighbours being atoms of the other kind at a distance 3a /4 arranged at the vertices of a regular tetrahedron. The sequence of (111) planes is stacked at the same intervals as in diamond (Figure 3.12), but alternate planes are occupied by atoms of different chemical species. Thus, following the same nomenclature as for NaCl, the stacking sequence is g A a B b C g A … (Figure 3.13). 3.5.4 Wurtzite, b-ZnS (P63mc) The sphalerite structure is derived from the c.c.p. structure by placing atoms of a different kind to those at the lattice points at every other tetrahedrally coordinated interstice. A related structure, also shown by ZnS, is obtained by filling alternate tetrahedrally coordinated interstices in the h.c.p. structure. This is the b-ZnS or wurtzite structure (P63mc). The lattice is hexagonal with atoms of one kind at (0, 0, 0) and ( 23 , 13 , 21 ) and those of the other kind at (0, 0, u) and 23 , 13 , 21 + u (Figure 3.18b). The value of u is very close to 0.375, i.e. 83 ; however, it is not constrained by symmetry to be exactly 0.375. From Figure 3.8b the relationship to the h.c.p. structure is obvious. Each atom is, of course, tetrahedrally coordinated with four of the opposite kind. The stacking of planes of atoms parallel to (0001) using the same nomenclature as for NaCl and a-ZnS is then A a B b A a B… or equivalently A a C g A a C g A … This structure is shown by a number of compounds (Table 3.3). The axial ratios shown in Table 3.3 and Section A7.5 of Appendix 7 are quite close to the ideal, 1.633, for hexagonal close packing of one type of ion with the other in the tetrahedral interstices.

(

3.5.5

)

Nickel Arsenide, NiAs (P63/mmc)

We described the sodium chloride structure as being derived from the c.c.p. structure by placing a second set of atoms in the octahedrally coordinated largest interstices of the structure. It is not surprising therefore that a structure exists in which atoms of a different kind are placed in the octahedral interstices of the h.c.p. structure. This is the nickel arsenide (nickeline)3 structure (P63/mmc) (Figure 3.19). The lattice is hexagonal, with atoms of one kind at (0,0,0) and 0, 0, 12 and those of the other kind at ( 23 , 13 , 14 ) and ( 13 , 23 , 34 ). For both kinds of atom the coordination number is 6, but while the sites occupied by one kind of atom, those denoted by open circles in Figure 3.19, lie in positions corresponding to a

(

3

)

Also known as niccolite.

Kelly_c03.indd 101

11/30/2011 4:08:24 PM

102

Crystallography and Crystal Defects

= As = Ni c

y a x

Figure 3.19 The crystal structure of nickel arsenide, NiAs

Table 3.4 Axial ratios at room temperature of some materials with the nickel arsenide structure Material NiAs CrS FeS

c/a

Material

c/a

1.40 1.64 1.66

CoS NiS

1.52 1.55

close-packed hexagonal arrangement (As), the others (Ni) lie at the lattice points of a primitive hexagonal lattice (if the As atoms are ignored), with a repeat distance in the c direction half that of the lattice parameter of the NiAs crystal structure. This difference in stacking of the M and X atoms is obvious from Figure 3.8a and also by stating the stacking sequence of the planes of atoms along [0001] following the procedure for NaCl. The stacking sequence is A b A g A b A g … The atoms denoted by Greek letters lie in the centre of a trigonal prism of atoms denoted by Roman letters, while the atoms denoted by Roman letters are octahedrally coordinated. The axial ratios of some crystals of sulphides with this structure are listed in Table 3.4; the selenides, tellurides and antimonides of the metals listed often have the same structure: see Section A7.6 of Appendix 7. The values of c/a at room temperature depart from the ideal for hexagonal close packing of one type of ion. Usually the metal atom is situated in the type of site occupied by Ni in NiAs, but in PtB the ‘anti-NiAs’ structure is shown. 3.5.6

– Calcium Fluoride, CaF2 (Fm3m)

If all of the tetrahedral interstices in the c.c.p. crystal structure are filled with atoms of a different kind from those in the c.c.p. crystal structure, we obtain the calcium fluoride – (CaF2) or fluorite structure (Fm3m) (Figure 3.20). The lattice is face-centred cubic with

Kelly_c03.indd 102

11/30/2011 4:08:33 PM

Crystal Structures

103

=F = Ca

a

Figure 3.20 The crystal structure of calcium fluoride, CaF2

atoms of one kind, for example Ca, at (0, 0, 0) and equivalent positions, and with F atoms at ( 14 , 14 , 14 ) and ( 14 , 43 , 14 ) and equivalent positions. There are clearly four formula units per unit cell. The coordination number of Ca is 8, with the nearest neighbours being atoms of F arranged at the corners of a cube. If the calcium atoms are ignored, it is apparent that the fluorine atoms lie at the lattice points of a primitive cubic lattice. Each F atom has tetrahedral coordination with four Ca atoms. The centres of atoms of one kind all form triequiangular nets of points parallel to {111} lattice planes. The separation of the atoms in these places is the same for the two types of atom. The stacking sequence of these planes along [111] can therefore be described as … aBg bCa g Ab aBg bCa … The planes of atoms denoted by successive Roman letters are regularly spaced from one another; the same is true of the planes of atoms denoted by Greek letters. This structure is shown by the fluorides of Ca, Sr and Ba and by the oxides of Zr, Th, Hf and U. Oxides and sulfides of alkali metals also show this structure; in these cases it is sometimes called the antifluorite structure. A tabulation of crystals with the flourite structure is given in Section A7.7 of Appendix 7. 3.5.7

Rutile, TiO2 (P42/mnm)

A common structure of compounds with the formula AX2, besides that of fluorite, is the rutile (TiO2) structure (P42/mnm) (Figure 3.21a). It is also sometimes called the cassiterite (SnO2) structure. A number of dioxides and fluorides have this crystals structure, such as those tabulated in Section A7.8 of Appendix 7. The lattice is primitive tetragonal with c/a about 0.65. There are titanium atoms at (0, 0, 0) and ( 12 , 12 , 12 ) and oxygen atoms at ± (u, u, 0) and ± (u + 12 , 12 − u, 12 ) , where u is close to 0.30 in all examples of the structure. Thus, there are two formula units per cell. A plan of the structure is shown in Figure 3.21b, projected down [001]. Each Ti atom is surrounded by six O atoms, but the octahedron of O atoms is not a regular octahedron. It is apparent that the crystal structure of rutile can be described in terms of how these Ti octahedra pack together. This leads conceptually to the more general geometry of the packing of polyhedra, which will be

Kelly_c03.indd 103

11/30/2011 4:08:33 PM

104

Crystallography and Crystal Defects

(a)

(b) y Ti 0

Ti 0 0.5 0

O 0.5 Ti

c

O

0

O

a

0 Ti

TiO2

= Ti

0.5

O

0 Ti

x

=O

Figure 3.21 (a) The crystal structure of rutile, TiO2. (b) The rutile crystal structure projected down [001]. The numbers indicate the z-coordinates of the atoms

discussed in Section 4.4 in the context of the packing of atoms or ions within very complicated crystal structures.

3.6

Other Inorganic Compounds

As we have seen in the descriptions of simple crystal structures in Sections 3.2–3.5, the concept of the packing of spheres into arrangements that are close-packed is of great practical use. It is also useful for circumstances where there are departures from the most close-packed ideal arrangement shown by c.c.p. crystal structures or h.c.p. crystal structures where c/a = 8 / 3, so that a ‘close-packed’ arrangement of one type of atom or ion (not necessarily in contact) occurs, with the interstices filled or partly filled with smaller atoms (or ions). Simple examples of such structures have already been considered in Section 3.5. In this section we consider other examples where the chemistry is less simple, or where the packing departs significantly from the ideal close-packed arrangement. 3.6.1

– Perovskite (Pm3m)

This primitive cubic crystal structure is a very common structure of crystals of compounds of the type MM′X3. It is named after the mineral perovskite, CaTiO3, which has this crystal structure above 900 °C; at room temperature, CaTiO3 has an orthorhombic crystal structure belonging to the space group Pnma (see Section 2.15).4 In this crystal structure, the calcium (M) and oxygen (X) ions taken together form a c.c.p. arrangement with the titanium (M′) ions in the octahedral voids (Figure 3.22). The coordination number of Ca is 12, that of 4

Kelly_c03.indd 104

SrTiO3 has this crystal structure at room temperature.

11/30/2011 4:08:38 PM

Crystal Structures

O

Ca

105

Ti

– Figure 3.22 The crystal structure of perovskite, Pm3m

Ti is 6 and that of O is 2. The atomic coordinates in the primitive unit cell are Ti ( 12 , 12 , 12 ) , Ca (0, 0, 0) and O 12 , 12 ,0 , 0, 12 , 12 , 12 , 0, 12 . The description of the perovskite crystal structure in terms of the packing of titanium octahedra will be deferred to Section 4.4. There are many slightly distorted forms of the perovskite structure that are important in solid-state devices. At room temperature, barium titanate, BaTiO3 (P4mm), has a crystal – structure that is a tetragonally distorted form of the Pm3m high-temperature structure. At lower temperatures, further distortions convert this into an orthorhombic crystal structure (Amm2) and a rhombohedral crystal structure (R3m) [10]. Pb(Zr1−xTix)O3, in which the Zr and Ti ions both occupy the M′ position, has two different rhombohedral (R3m and R3c) crystal structures [11] and a tetragonal (P4mm) form at room temperature, dependent on the value of x. The high-temperature superconducting oxide YBa2Cu3O7−d , where d is a small fraction 0 ⎝ ⎠

(4.8)

Hence, it follows that if m = n, they can both only take the value 3; integers 4 or greater would not satisfy this inequality. If m = 3, possible values of n which satisfy Equation 4.7 for integer E are 3, 4 and 5, giving E = 6, 12 or 30: the tetrahedron, the cube and the dodecahedron, respectively. If n = 3, solutions for m are 3, 4 or 5, giving the tetrahedron, the octahedron and the icosahedron, respectively. Many examples where use was made of the first three Platonic solids are discussed in Chapter 3 in order to describe a crystal structure; for example, the tetrahedron was used for the diamond structure and the cube for the sodium chloride structure. The description of crystal structures given in Chapter 3 is useful, but its formality, based as it is on the Bravais lattice, often fails to indicate the way in which the solid crystal is bound by the forces between the component atoms. For this reason, it is often useful to describe crystal structures in terms of an assemblage of polyhedra linked in various ways. This approach can help to simplify the description of the structures and bring out the crystal chemistry or explain why a crystal possesses a desirable physical property. Thus, for example, the rutile structure, MX2 (sub-Section 3.5.7), can be described either as a complex assemblage of oxygen ions, with the titanium ions occupying one-half of the octahedral cavities, or alternatively, and more powerfully, as an assemblage of slightly distorted TiO6 octahedra linked by their corners and edges. The perovskite structure, MM′X3 (sub-Section 3.6.1), can be regarded as a framework of M′X6 octahedra linked by their corners, each X being shared by two octahedra. The result is a three-dimensional assemblage of

Kelly_c04.indd 133

11/29/2011 7:06:00 PM

134

Crystallography and Crystal Defects

octahedra whose tetragonal axes coincide with those of the unit cell. When the relative dimensions of the octahedra of M′ ions are incompatible with this configuration, the structure becomes slightly distorted, causing a lowering in symmetry. –– The regular dodecahedron, the fourth Platonic solid, has m3 5 point group symmetry. It has 12 five-fold axes, 20 triads and 30 diads and mirror planes. The 12 five-fold axes are at an angle to one another of tan−1 2 = 63.43°. Seen in projection looking down one of the five-fold axes, the other five adjacent five-fold axes are all at 72° to one another. Sets of rods (or fibres) aligned normal to the faces of a regular dodecahedron can produce an elastically isotropic solid; this requires that the cross-sections of the rods have specific shapes and that these be arranged to meet each other in specified ways [12].

4.5

Icosahedral Packing

Regular dodecahedral packing has not so far been shown to be of great use in the description and understanding of complicated crystal structures, in contrast to the icosahedron. This also –– has m3 5 point group symmetry, with 12 five-fold rotation axes, 20 triads and 30 diads and mirror planes. The importance of the icosahedron arises because of its close relationship with cubic close packing. In the cubic close-packed (c.c.p) assembly of equal spheres, each sphere is surrounded by a first coordination polyhedron of 12 identical spheres (Section 3.2). Each neighbouring sphere is situated at a vertex of a cubo-octahedron (see Figure 13.28a). This 14-sided figure has eight hexagonal faces and six square faces and can be formed by suitably truncating a cube with planar slices at the eight vertices to form the eight equilateral triangular faces. At each new vertex produced, exactly halfway along the edges of the original cube, two hexagonal faces and two square faces meet. A second layer of spheres packed similarly over the first layer will be found to require 42 spheres to complete it. In general, it may be shown that if the structure of spheres is continued, the nth layer will consist of (10n2 + 2) spheres [13]. The cubo-octahedron can be transformed into a regular icosahedron by compression of some 5% along the line joining the vertices to the centre and allowing the square faces to become rhombs, and each to split into two triangular faces. This movement is easily illustrated on a stereogram (Problem 4.5). When an icosahedron of 12 spheres about a central sphere is surrounded by a second icosahedral sphere, the second shell will also contain 42 spheres. The second shell will lie over the first, so that spheres will be in contact along the six five-fold axes of symmetry. These spheres will not be close-packed. The packing density of such an icosahedral shell packing is less than that of the c.c.p. structure, 0.74, but nonetheless can be quite high; close to 0.69, which is a higher packing fraction than is found in body-centred cubic (b.c.c.) (0.68) [13]. The packing fraction in this icosahedron shell packing can be calculated by noting that within the solid icosahedron the unit that is repeated is a distorted tetrahedron; 20 of these make up the solid icosahedron. An icosahedral packing of equal spheres is shown in Figure 4.6. On each triangular face, the layers of spheres succeed each other, just as in the c.c.p. sequence. Each of these spheres touches just six neighbours, three above and three below, and is separated by a distance of 5% of its radius from its six neighbours in the plane of the icosahedron. Icosahedral packing is extremely useful for describing structures containing many types of atom of very different sizes. The polyhedra within a given structure can have various

Kelly_c04.indd 134

11/29/2011 7:06:02 PM

Amorphous Materials and Special Types of Crystal–Solid Aggregates

135

Figure 4.6 Packing of equal-sized spheres into an icosahedral arrangement. The diagram shows the third layer of spheres. (After Mackay [13].)

shapes in order to accommodate atoms or ions of different sizes. They are often referred to as topologically close-packed (TCP) structures or Frank–Kasper phases [14,15]. TCP structures enable a closer packing of atoms to arise than is found in the geometrically closepacked structures (c.c.p. and hexagonal close-packed, h.c.p.). There are many examples in the literature of metallic alloys with TCP structures containing three or more types of atom. In general, TCP structures are made up of clusters of polyhedra, with the symmetry of the whole crystal being less than that of the individual clusters. Icosahedral coordination frequently occurs in TCP structures, as do clusters containing 55 or more atoms. Examples of icosahedral coordination can be found in compounds such as MoAl12 (Figure 4.7), WAl12 – and Mn0.5Cr0.5Al12 [16]. The space group of these compounds is now designated Im3. Some of the triads and diads from the icosahedral arrangement of the Al atoms are retained in the crystal, but the five-fold rotational axes of the individual MoAl12 units are lost.

4.6

Quasicrystals

The perovskite example is one where, in order to maintain the essential packing of the ions, the deviation from ideal symmetry is towards a lower symmetry (Sections 3.6 and 4.4). In some cases, particularly where the packing is based on clumps of atoms with nearly close packing, the point symmetry may be greatly increased, so that it exceeds that compatible with repetition at the points of a Bravais lattice. The famous first report of five-fold rotational symmetry in a solid occurred in 1984, in a paper whose title amply describes the effect: ‘Metallic phase with long-range orientational order and no translational symmetry’ [17]. For this discovery, the first author of the paper, Daniel Shechtman, was awarded the 2011 Nobel Prize for Chemistry. The compositions of

Kelly_c04.indd 135

11/29/2011 7:06:03 PM

136

Crystallography and Crystal Defects

Figure 4.7 The crystal structure of MoAl12. This figure is derived from Figure 1 of [16]. Molybdenum (Mo) atoms (heavily shaded) are found at the corners and centre of the unit cell. Each Mo is surrounded by 12 aluminium atoms (lightly shaded) arranged at the 12 vertices of a regular icosahedron

the alloys investigated were relatively simple: Al with 10–14 wt% of Mn, Fe or Cr. Since these initial observations, many examples have been found in related alloy systems of metallic phases without translational symmetry in two or three dimensions. These can show a number of ‘forbidden’ rotational symmetries (e.g. 5-, 8-, 10- or 12-fold symmetry), which are completely incompatible with the possession of a Bravais lattice as defined so far in this book. Such structures are best described in terms of the regular or slightly irregular (distorted) polyhedra, often icosahedra. Phases with icosahedral symmetry are often referred to as i-phases. Useful reviews of quasicrystals can be found in [18] and [19]. The first quasicrystals were produced by rapid cooling from the melt. Although this is still a common way of producing quasicrystalline phases, quasicrystalline phases of suitable compositions can now be produced in centimetre sizes by conventional crystal growth methods, such as in i-Al–Mn–Pd. It is common for i-phases to be formed over a range of compositions, such as in i-Mg–Al–Zn alloys [18]. There is often a quasicrystalline phase and a crystalline phase of the same composition in the same alloy. Three typical alloys readily showing both crystal and quasicrystal behaviour are α-Al–Mn–Si, Mg32(Al,Zn)49 and Al5.6Li2.9Cu. In such alloys, it is usual for the crystalline phase to have a relatively large unit cell, and to be referred to as an approximant (of the quasicrystal). A notable feature of quasicrystals is that they can be almost free of defects: this can be deduced directly from the contrast seen in transmission electron microscopy of individual icosahedral grains, but also from the extreme sharpness of the X-ray diffraction peaks – which are often as sharp as those found from very carefully prepared silicon crystals. 4.6.1 A Little Recent History and a New Definition As we have noted above, the history of quasicrystals began in 1984 with their discovery by Shechtman and his coauthors. Since then, hundreds of quasicrystals have been discovered. Very recently, evidence has been produced that quasicrystals might form naturally in Al–Cu–Fe minerals, producing the Al65Cu24Fe13 phase [20]. Following these many discoveries, the International Union of Crystallography has amended its definition of a

Kelly_c04.indd 136

11/29/2011 7:06:03 PM

Amorphous Materials and Special Types of Crystal–Solid Aggregates

137

crystal so as to include ordering of the atoms in either a periodic or an aperiodic manner. Nowadays those symmetries compatible with translational symmetry are defined as crystallographic. This leaves room for ‘noncrystallographic symmetries’. Hence crystals can be divided into two main classes: those with crystallographic point group symmetry, to which all of the structures described in this book other than in this section belong, and those with noncrystallographic symmetry, to which the quasicrystals described in this section and the incommensurate structures described in Section 4.7 belong.

4.7

Incommensurate Structures

In addition to quasicrystals, there are other types of aperiodic structures. The first incommensurate phases were discovered in the 1970s [21]. A good example of an incommensurate phase is a magnetic system in which the magnetization has a helical structure with a pitch that does not have a rational relation to the underlying lattice [21,22]. Expressed mathematically, two periodicities q1 and q2 in the same direction in a lattice are incommensurate if their ratio cannot be expressed as a ratio of two integers M and N. That is: q1 M ≠ M , N = 1,2,3… q2 N Many materials are now known which display two or more periodicities that are incommensurate with each other. A well-known example of an incommensurate structure is the modulated structure which appears over a narrow 1.3 K temperature range in the high ↔ low phase transition in quartz [23]. A second example can be found in the mineral calaverite [24].

4.8

Foams, Porous Materials and Cellular Materials

While the emphasis in this book is on the arrangements of atoms in single crystals, there are a number of sections, such as those concerned with crystalline textures and interfaces, in which we note that most materials are usually arranged in polycrystalline aggregates. The interfaces between the individual crystals, known as grain boundaries or interphase boundaries (Chapter 13), are usually just a few atoms wide. These boundaries form a continuous skeleton within which the individual crystals are contained. If we imagine a solid metal or ceramic consisting only of these intercrystalline regions, with the material of the individual crystals removed, we should have a material with the geometry of a foam. An example of the microstructure of a solid foam is shown in Figure 4.8 [25,26]. The foam is an important type of porous solid, which itself is a class of cellular solids [27]. Polymer foams such as those of polyurethane and polystyrene have been known for many years, and there are natural cellular materials, such as zeolites and sponges – the term ‘sponge’ usually denotes a very flexible foam. Recent technical advances in techniques for foaming metal and ceramic have led to intense research into such materials. The nomenclature for describing the architecture of foams and other forms of porous solids is not completely consistent. The terms ‘three-dimensional meshes’ and ‘lattice structures’ are also used to describe foamed materials. The International Union of Pure and Applied Chemistry (IUPAC) recommendations for the characterization of porous solids [28] describe pore diameters of less than 2 nm as micro; between 2 and 50 nm as meso and

Kelly_c04.indd 137

11/29/2011 7:06:03 PM

138

Crystallography and Crystal Defects

5 mm

Figure 4.8 The microstructure of a foam made from an Al −9 wt% Si alloy containing 10 vol% of silicon carbide particulates [25,26]. Pretreated titanium dihydride, TiH2, was used as the foaming agent

greater than 50 nm as macro, but these definitions are not consistently maintained. These authors of the IUPAC recommendations had in mind catalysts, absorbents and membranes primarily. They define materials as constitutively porous if their final structure depends mainly on the original structure, such as pores in zeolites or amorphous carbon. Materials made porous by a subtractive processing route have material removed from them: chemically etched porous silicon is an example of such a material. The volume fraction of porosity is the fraction of the total volume occupied by pores; that is, Vp/V, where Vp is the total volume of pores and V the total volume of specimen. Pores are open if accessible by the particular probe used, and closed if they are not: the definition depends on the type of probe employed. Open pores are interconnected; the same range of sizes micro, meso and macro may be used to define the diameter of the connecting channels. It is also possible to have mesopores with micro-connectivity or mesopores with meso-connectivity. The term porous metal or porous ceramic usually suggests a porosity range of 15–75%. This range of porosity is shown by metals used in filtration, fluid flow control, self-lubricating bearings and battery electrodes. True foams have high porosities, such as 80–90%, and it is these that provide a distinct advantage for energy and sound absorption, vibration suppression and thermal management. A special form of closed-cell foam is a syntactic foam consisting of small spheres, which are stuck together (Greek: συνταξις – arrangement). If the pores are hollow and the interstices are completely filled, the maximum porosity is about 65%. To a first approximation, most porous structures can be regarded as equiaxed, although it is possible to obtain porous metals and ceramics with elongated structures, the so-called lotus structures; anodized aluminium is a particularly good example. The properties of porous materials are governed by three main factors: 1. The properties of the solid forming the walls of the foam. 2. The topology (connectivity) and shape of the faces and edges of the individual cells. 3. The relative density rf /rs of the foam, where rf is the overall density of the foam, and rs that of the solid material within it. When estimating the mechanical properties of cellular materials, reference is often made to lattice structures, which in this case refers to a connected set of struts, rather than the term used elsewhere in this book. In this context, a lattice, truss or space frame means an array of struts pin-jointed or rigidly bonded at their connections. Foams are like the trusses and frames of space structures, and so are made up of a connected array of struts or plates. They

Kelly_c04.indd 138

11/29/2011 7:06:04 PM

Amorphous Materials and Special Types of Crystal–Solid Aggregates

139

are characterized by a typical ‘unit cell’ with symmetry elements, even though most foams do not show translational symmetry. However, these lattices, cellular materials and foams differ from the lattices of the engineer in one very important regard: that of scale of size. The unit cell of a cellular material is one on the scale of micrometres–millimetres, or sometimes less, so allowing it to be viewed both as structure and as material. Although a foam may not show translational symmetry, the identification of a typical (or average) ‘unit cell’ is very important for describing the overall symmetry of the physical properties, such as elastic properties. This same procedure is used with composite materials – the best known of which, and presently the most useful, are the fibre composites, consisting of stiff fibres arranged in a soft and yielding matrix. Here, the ‘unit cell’ is termed the representative volume element. We shall revisit similar structures in Chapter 13.

Problems 4.1 Determine the shape of the polyhedron which represents the Voronoi polyhedron for a c.c.p. arrangement of spheres. What is the name of this polyhedron? 4.2 Construct the Schlegel figure for the rhombic dodecahedron. 4.3 Describe a solid having five vertices and six triangular faces. 4.4 Draw a stereogram of each of the Platonic solids and insert all of the symmetry elements; make the primitive of the stereogram parallel to the chosen plane of the relevant Schlegel diagram. 4.5 By placing a triad axis of the cubo-octahedron at the centre of the primitive, draw a stereogram to illustrate the distortion of a cubo-octahedron, so as to form a regular icosahedron. 4.6 Show that in c.c.p., the nth layer packed over the layers below is the surface of a cubooctahedron on which there are (n + 1) spheres along each of its edges. Hence show that the nth layer consists of (10n2 + 2) spheres. Explain why in an icosahedrally-packed assembly of equal spheres the nth layer packed over the layers must also consist of (10n2 + 2) spheres. 4.7 Giving your reasons, explain whether MoAl12 has crystallographic point group symmetry or noncrystallographic point group symmetry. 4.8 Give a logical reason why the porosity limit of a syntactic foam is very close to Bernal’s packing fraction for a liquid.

Suggestions for Further Reading S.M. Allen and E.L. Thomas (1999) The Structure of Materials, John Wiley and Sons, New York. A.M. Donald, A.H. Windle and S. Hanna (2006) Liquid Crystalline Polymers, 2nd Edition, Cambridge University Press, Cambridge. L.J. Gibson and M.F. Ashby (1997) Cellular Solids: Structure and properties, 2nd Edition, Cambridge University Press, Cambridge. C. Janot (1994) Quasicrystals: A Primer, 2nd Edition, Clarendon Press, Oxford. F.R.N. Nabarro (ed.) (1992) Dislocations in Solids, Vol. 9. Dislocations and Disclinations, North Holland, Amsterdam.

Kelly_c04.indd 139

11/29/2011 7:06:04 PM

140

Crystallography and Crystal Defects

References [1] J.D. Bernal (1959) A geometrical approach to the structure of liquids, Nature, 183, 141–147. [2] J.A. Elliott, A. Kelly and A.H. Windle (2002) Recursive packing of dense particle mixtures, J. Mater. Sci. Lett., 21, 1249–1251. [3] G.F. Voronoï (1908) Nouvelles applications des paramètres continus à la théorie des formes quadratiques. Deuxième mémoire. Recherches sur les parallélloèdres primitifs, J. reine angew. Math. (Crelle’s Journal), 134, 198–287. [4] B. Valenti and M.L. Sartirana (1984) Mesophase formation in lyotropic polymers, Il Nuovo Cimento, 3, 104–120. [5] F. Reinitzer (1888) Beiträge zur Kenntniss des Cholesterins, Monatshefte für Chemie, 9, 421–441. [6] O. Lehmann (1889) Über fliessende Krystalle, Z. Phys. Chem., 4, 462–472. [7] G. Friedel (1922) Les états mésomorphes de la matière, Ann. Physique, 18, 273–474. [8] F.R.N. Nabarro (1987) Theory of Crystal Dislocations, Dover Publications, New York. [9] F.C. Frank (1958) On the theory of liquid crystals, Disc. Faraday Soc., 25, 19–28. [10] H.S.M. Coxeter (1961) Introduction to Geometry, John Wiley and Sons, New York. [11] V. Schlegel (1883) Theorie der homogen zusammengesetzten Raumgebilde, Nova Acta Academiae Caesareae Leopoldino-Carolinae Germanicae Naturae Curiosorum, 44, 343–459. [12] J.G. Parkhouse and A. Kelly (1998) The regular packing of fibres in three dimensions, Proc. Roy. Soc. Lond. A, 454, 1889–1909. [13] A.L. Mackay (1962) A dense non-crystallographic packing of equal spheres, Acta Crystall., 15, 916–918. [14] F.C. Frank and J.S. Kasper (1958) Complex alloy structures regarded as sphere packings. I. Definitions and basic principles, Acta Crystall., 11, 184–190. [15] F.C. Frank and J.S. Kasper (1959) Complex alloy structures regarded as sphere packings. II. Analysis and classification of representative structures, Acta Crystall., 12, 483–499. [16] J. Adam and J.B. Rich (1954) The crystal structure of WAl12, MoAl12 and (Mn, Cr)Al12, Acta Crystall., 7, 813–816. [17] D. Shechtman, I. Blech, D. Gratias and J.W. Cahn (1984) Metallic phase with long-range orientational order and no translational symmetry, Phys. Rev. Lett., 53, 1951–1953. [18] A.I. Goldman and K.F. Kelton (1993) Quasicrystals and crystalline approximants, Rev. Mod. Phys., 65, 213–230; erratum 579. [19] W. Steurer (2004) Twenty years of structure research on quasicrystals. Part I. Pentagonal, octagonal, decagonal and dodecagonal quasicrystals, Z. Kristall., 219, 391–446. [20] L. Bindi, P.J. Steinhardt, N. Yao and P.J. Lu (2009) Natural quasicrystals, Science, 324, 1306–1309. [21] P. Bak (1982) Commensurate phases, incommensurate phases and the devil’s staircase, Rep. Prog. Phys., 45, 587–629. [22] M. Habenschuss, C. Stassis, S.K. Sinha, H.W. Deckman and F.H. Spedding (1974) Neutron diffraction study of the magnetic structure of erbium, Phys. Rev. B, 10, 1020–1026. [23] A. Putnis (1992) Introduction to Mineral Sciences, Section 12.3, Cambridge University Press, Cambridge. [24] W.J. Schutte and J.L. de Boer (1988) Valence fluctuations in the incommensurately modulated structure of calaverite AuTe2, Acta Crystall. B, 44, 486–494. [25] V. Gergely, D.C. Curran and T.W. Clyne (2003) The FOAMCARP process: foaming of aluminium MMCs by the chalk-aluminium reaction in precursors, Comp. Sci. Tech., 63, 2301–2310. [26] V. Gergely and T.W. Clyne (2000) The FORMGRIP process: foaming of reinforced metals by gas release in precursors, Adv. Engng. Mater., 2, 175–178. [27] L.J. Gibson and M.F. Ashby (1997) Cellular Solids: Structure and properties, 2nd Edition, Cambridge University Press, Cambridge. [28] J. Rouquerol, D. Avnir, C.W. Fairbridge, D.H. Everett, J.H. Haynes, N. Pernicone, J.D.F. Ramsay, K.S.W. Sing and K.K. Unger (1994) Recommendations for the characterization of porous solids, Pure & Appl. Chem., 66, 1739–1758.

Kelly_c04.indd 140

11/29/2011 7:06:04 PM

5 Tensors 5.1

Nature of a Tensor

There are a number of ways to introduce tensors. We shall begin by considering tensors of zero, first and second rank, before extending our discussion to tensors of third and fourth rank. Scalar quantities are examples of tensors of zero rank; these simply have magnitude. Vectors are tensors of the first rank. These have both direction and magnitude and represent a definite physical quantity. Tensors of the second rank are quantities that relate two vectors. Suppose we wish to know the relationship between the electric field in a crystal, represented by the vector E, and the current density (i.e. current per unit area of cross-section perpendicular to the current), represented by the vector J.1 In general, in a crystal the components of J referred to three mutually perpendicular axes (Ox1, Ox2, Ox3), which we can call J1, J2 and J3, will be related to the components of E, referred to the same set of axes in such a way that they each depend linearly on all three of the components E1, E2 and E3. It is usual to write this in the following way: J1 = σ 11 E1 + σ 12 E2 + σ 13 E3 J 2 = σ 21 E1 + σ 22 E2 + σ 23 E3 J 3 = σ 31 E1 + σ 32 E2 + σ 33 E3

(5.1)

The nine quantities s11, s12, s13, s21, s22, s23, s31, s32, s33 are called the components of the conductivity tensor. The electrical conductivity tensor relates the vectors J and E. If we write all of the relations (5.1) in the shorthand form: J=σ E

(5.2)

1

It is conventional to denote current density by j, as in Section A1.3 and in [1]. However, j is used in this chapter to denote a unit vector along Ox2.

Crystallography and Crystal Defects, Second Edition. Anthony Kelly and Kevin M. Knowles. © 2012 John Wiley & Sons, Ltd. Published 2012 by John Wiley & Sons, Ltd.

Kelly_c05.indd 141

11/30/2011 7:18:26 PM

142

Crystallography and Crystal Defects

Table 5.1

Properties represented by second-rank tensors

Tensor Electrical conductivity Thermal conductivity Diffusivity Permittivity Dielectric susceptibility Permeability Magnetic susceptibility

Vectors related Electric field Thermal gradient (negative) Concentration gradient (negative) Electric field Electric field Magnetic field Magnetic field

Current density Thermal current density Flux of atoms Dielectric displacement Dielectric polarization Magnetic induction Intensity of magnetization

we see that s is a quantity that multiplies the vector E in order to obtain the vector J. When a tensor relates two vectors in this way it is called a tensor of the second rank or second order. Many physical properties are represented by tensors like the electrical conductivity tensor. Such tensors are called matter tensors. Some examples are given in Table 5.1. In addition there are field tensors, of which two second-rank tensors are very important, namely stress and strain. The stress tensor relates the vector traction (force per unit area) and the orientation of an element of area in a stressed body. The strain tensor relates the displacement of a point in a strained body and the position of the point (see Chapter 6).

5.2 Transformation of Components of a Vector If we know the components of a vector, say p, referred to a set of orthogonal axes (Ox1, Ox2, Ox3), each of unit length – that is, orthonormal axes (Appendix 1) – it is often necessary to know the components of the same vector referred to a different set of axes (Ox′1, Ox′2, Ox′3), which are again orthonormal and have the same origin as Ox1, Ox2 and Ox3 (Figure 5.1). We must first define how the two sets of axes are related to one another. We do this by setting down a table of the cosines of the angles between each new axis and the three of the old set. The table will appear as: x1 New

x1′ a11 x2′ a21 x3′ a31

Old x2 x3 a12 a22 a32

a13 a23 a33

(5.3)

Here, a32, for example, is the cosine of the angle between the new axis 3 and the old axis 2; that is, the angle x′3Ox2 in Figure 5.1. Similarly, a11 is the cosine of the angle between Ox′1 and Ox1, and so on. In an array of the type of Equation 5.3 it should be noted that the sum of the squares of any row or column of the array is equal to one, because both sets of axes are orthonormal. Therefore, for example, a112+ a212+ a312 = 1 and a212+ a222+ a232 = 1, and so on. It is evident that the elements aij constitute the elements of a rotation matrix (Section A1.4). If we call this matrix A, the inverse of this matrix, A−1, is equal to its transpose, Ã (Section A1.4).

Kelly_c05.indd 142

11/30/2011 7:18:30 PM

Tensors

143

x3 x2′ x3′

cos–1 a21

P

cos–1 a23

k¢ k O

i

cos–1 a22

j¢ j

x2

i¢

x1 x1′

Figure 5.1

Now let p have components p1, p2, p3 along the old axes so that: p = p1i + p2 j + p3 k

(5.4)

where i, j, k are unit vectors along Ox1, Ox2, Ox3, respectively. The component of p along the new axis Ox′1 can be found by resolving the three old components, p1i, p2 j and p3k, along the new axis Ox′1 and adding up the projections, thus obtaining: p1′ = a11 p1 + a12 p2 + a13 p3

(5.5a)

Similarly, we find the new components of p along Ox′2 and Ox′3, p′2 and p′3 respectively, to be: p2′ = a21 p1 + a22 p2 + a23 p3

(5.5b)

p3′ = a31 p1 + a32 p2 + a33 p3

(5.5c)

and

The vector p has the same magnitude and direction referred to any set of axes. If i′, j′, k′ are unit vectors along Ox′1, Ox′2, Ox′3 then: p1i + p2 j + p3 k = p1′ i′ + p2′ j′ + p3′ k ′

(5.6)

From Equation 5.3 we can also write:

Kelly_c05.indd 143

11/30/2011 7:18:31 PM

144

Crystallography and Crystal Defects

i′ = a11i + a12 j + a13 k j′ = a21i + a22 j + a23 k k ′ = a31i + a32 j + a32 k

(5.7)

and, conversely, since the elements aij constitute the elements of a rotation matrix: i = a11i′ + a21 j′ + a31k ′ j = a12 i′ + a22 j′ + a32 k ′ k = a13 i′ + a23 j′ + a33 k ′

(5.8)

Equations 5.5a–c could also be deduced by using Equation 5.8 to express i, j and k each in terms of i′, j′ and k′ and then substituting in Equation 5.4, noting that p′1 is the coefficient of the unit vector i′, and so on. It is a useful exercise to write out the substitution in full. Proceeding in the same way, we can also obtain expressions for the old components of the vector p, [p1, p2, p3], in terms of the new components by substituting for i′, j′, k′ in terms of i, j, k (using Equations 5.7) on the right-hand side of Equation 5.6 and subsequently comparing terms on the two sides of the equation. Doing this, we find: p1 = a11 p1′ + a21 p2′ + a31 p3′ p2 = a12 p1′ + a22 p2′ + a32 p3′ p3 = a13 p1′ + a23 p2′ + a33 p3′

(5.9)

Relations (5.9) are the converse of Equations 5.5a–c. We are now in a position to relate these results on the transformation of the components of a vector to a relation such as Equation 5.2. A tensor of the second rank is a quantity that multiplies one vector to give another, generally nonparallel, vector of a different magnitude. If we return to our example of electrical conductivity in Section 5.1, we note that we could state Equations 5.1 in the following way:

J1i = (σ 11 E1 + σ 12 E2 + σ 13 E3 ) i J 2 j = (σ 21 E1 + σ 22 E2 + σ 23 E3 ) j J 3 k = (σ 31 E1 + σ 32 E2 + σ 33 E3 ) k

(5.10)

Having done this, let us add up these three equations and express the right-hand side in a new form so that the equation reads: J1i + J 2 j + J 3 k = [σ 11ii + σ 12 ij + σ 13 ik + σ 21 ji + σ 22 jj + σ 23 jk + σ 31ki + σ 32 kj + σ 33 kk ] .( E1i + E2 j + E3 k )

(5.11)

The quantity in square brackets is to be regarded as an operator, which operates on vector E in order to obtain the vector J from E. The form in which the operator is written here is the one that is appropriate to the orthogonal axes defined by the unit vectors i, j and k.2 We let the operator inside the square brackets ‘multiply’ the vector 2

Kelly_c05.indd 144

Note that inside the square brackets we do not have i . i (which equals one), but ii.

11/30/2011 7:18:37 PM

Tensors

145

E (= E1i + E2 j + E3k), as if we were forming the scalar (or dot) product of vector multiplication (Appendix 1). To understand Equation 5.11, it is best to write out the right-hand side term by term. The first term is s11ii · E1i = s11E1ii · i = s11E1i, since i · i = 1. The next term is s11ii · E2j = 0, since i · j = 0 because the i and j axes are orthogonal. Similarly, s11ii · E3k = 0 and s12ij · E1i = 0, but the fifth term is s12ij · E2j = s12E2i, since j · j = 1. If all terms are written out and similar ones collected, we finally obtain just Equations 5.10, which can also be represented as in Equations 5.1. Equation 5.11 is the expanded form of Equation 5.2, or, put another way, the most succinct expression of Equation 5.11 is Equation 5.2. Equation 5.11 contains the components of the conductivity tensor s11, s12, s13, …, s33 referred to the axes (Ox1, Ox2, Ox3), defined by the unit vectors i, j and k. We have seen how to transform the components of a vector, so we can also transform the components of this second-rank tensor. If we take new axes represented by the unit vectors i′, j′, k′, the components of the conductivity tensor s will be different and we can find what they are by substituting for i, j, k in Equation 5.11 the values of i′, j′, k′ referred to the new axes, using Equations 5.7. We would also have to substitute for E1, E2, E3 the components of E along the new axes – E′1, E′2, E′3 – so that the new components of the tensor s11′ , s12′ , s13′ ,…, s 33 ′ , multiplied by the new components of E in a form such as Equation 5.9, yield the components of the vector J, also referred to the new set of axes. This is very lengthy to write out and so we shall first introduce a convenient short notation.

5.3

Dummy Suffix Notation

The tensor T relates the vector p with components p1, p2 and p3 to the vector q with components q1, q2 and q3 so that: p1 = T11q1 + T12 q2 + T13q3 p2 = T21q1 + T22 q2 + T23q3 p3 = T31q1 + T32 q2 + T33q3

(5.12)

These three equations can be written as: j =3

p1 = ∑ T1 j q j , j =1

j =3

p2 = ∑ T2 j q j , j =1

j =3

p3 = ∑ T3 j q j

(5.13)

j =1

or, even more succinctly, as: j =3

pi = ∑ Ti j q j j =1

( i = 1, 2 , 3)

(5.14)

We now leave out the summation sign and introduce the Einstein summation convention [2]: if a suffix occurs twice in the same term, summation with respect to that suffix is

Kelly_c05.indd 145

11/30/2011 7:18:43 PM

146

Crystallography and Crystal Defects

automatically implied. In what follows, the summation will always run over the values 1, 2 and 3 for both i and j. Equations 5.12 can then be written as: pi = Tij q j

(5.15)

Here j is called a dummy suffix, because it does not matter which letter except i is taken to represent it. Equation 5.11 could equally well read: pi = Tik qk using k as the dummy suffix. If we apply this notation to Equations 5.5a–c, all three are contained in the single expression: pi′ = aij p j

(5.16)

Note that the dummy suffix occurs in neighbouring places in Equation 5.16. If we apply the same notation to Equations 5.9 we obtain: pi = (a −1 )ij p′j = (a )ij p′j = a ji p′j

(5.17)

so that when writing the ‘old’ components in terms of the ‘new’, the dummy suffixes are separated because, as we have noted in Section 5.2, the elements aij constitute the elements of a rotation matrix, and so the elements of the inverse of this matrix, [a−1]ij, are simply the transpose of this matrix. When first learning this notation it is best to write out the sums term by term. Thus p′i = aij pj gives, on expansion: p1′ = a1 j p j p2′ = a2 j p j p3′ = a3 j p j

(5.18)

These three sums can then be expanded without fear of making an error.

5.4 Transformation of Components of a Second-Rank Tensor Let two vectors p = [p1 p2 p3] and q = [q1 q2 q3] be related by the tensor Tij for a specific choice of the axes i, j, k. The components of Tij relate the components of q to those of p according to Equation 5.12, or, more succinctly, according to Equation 5.15: pi = Tij q j Now, the components of the two vectors depend upon the choice of axes, because this choice determines the values [p1 p2 p3] and [q1 q2 q3]. The vectors p and q themselves do not change. When the axes are changed, and hence the components of p and q change, the components Tij will also change. If now we choose new axes i′, j′, k′ so that: pi′ = Tij′q′j

Kelly_c05.indd 146

(5.19)

11/30/2011 7:18:47 PM

Tensors

147

we will wish to find the relation between the nine components Tij′ and the nine components Tij. We can find these directly by writing Equation 5.15 in the operational form of Equation 5.11: p1i + p2 j + p3 k = [T11ii + T12 ij + T13 ik + T21 ji + T22 jj + T23 jk + T31ki + T32 kj + T33 kk ] ⋅ (q1i + q2 j + q3 k )

(5.20)

We can now substitute for i, j and k in this equation the values of these quantities in terms of i′, j′ and k′ according to Equations 5.8. The substitution in the left-hand side yields p′1i′ + p′2 j′ + p′3k′, directly from Equation 5.6. Likewise, the term in round brackets on the right-hand side of Equation 5.20 becomes q′1i′ + q′2 j′ + q′3k′. The tensor operator in square brackets is treated in the same way and substitution is made for i, j and k in terms of i′, j′ and k′ from Equations 5.8. There will be 81 terms in total in this square bracket, but these can be grouped together in nine separate new terms. If all those containing (say) the vectors j′k′ are collected, there will be nine of these and the coefficient of j′k′ will be the new component T 23′ . If we write out the expression for T 23 ′ , it is: T23′ = (a21a31T11 + a21a32T12 + a21a33T13 + a22 a31T21 + a22 a32T22 + a22 a33T23 + a23 a31T31 + a23 a32T32 + a23 a33T33 )

(5.21)

Using the summation convention, this can be written succinctly in the form: ′ = a2 k a3l Tkl T23

(5.22)

Similarly, the other eight components of T ij′ may be found by collecting the terms in i′i′, i′j′, i′ k′, j′i′, j′ j′, k′ i′, k′ j′ and k′k′, respectively. Using the summation convention, the full relationship can be written in the form: Tij′ = aik a jl Tkl

(5.23)

For each value of i and j, the sum is to be taken over both k and l. To confirm Equation 5.23 is correct, it is helpful to write out the expansion summing over each of these separately. For example, if i = 2 and j = 3, Equation 5.21 is the expanded version of Equation 5.23. An alternative, and more elegant, method to establish the relationship between Tij′ and Tij is to perform the following mathematical operations with suitable dummy suffices to determine the nine components of T′ij: 1. Write p′ in terms of p: p′i = aik pk (using Equation 5.16). 2. Write p in terms of q: pk = Tkl ql (using Equation 5.15). 3. Write q in terms of q′: ql = ajl q′j (using Equation 5.17). When we combine these three operations we have: pi′ = aik pk = aik Tkl ql = aik Tkl a jl q′j

Kelly_c05.indd 147

(5.24)

11/30/2011 7:18:55 PM

148

Crystallography and Crystal Defects

or: pi′ = aik Tkl a jl q′j

(5.25)

This is of the form of Equation 5.19. Therefore, by comparing Equations 5.19 and 5.26, we have the important result: Tij′ = aik Tkl a jl

(5.26)

which is Equation 5.23, because the order in which a product is written on the right-hand side of this equation does not matter when the dummy suffix notation is used. The relationship between T′ij and Tij is most easy to remember in the form: Tij′ = aik a jl Tkl

(5.27)

The reverse transformation to Equation 5.27 – that is, the transformation giving the components of the tensor Tij in terms of those of the new components T′ij – can be accomplished in exactly the same way. This will lead to: Tij = aki alj Tkl′

(5.28)

It is a useful exercise to prove this.

5.5

Definition of a Tensor of the Second Rank

If the operator T relates two vectors p and q, so that T may be written in the form of the operator given in Equation 5.20, then T is known as a dyadic or tensor of the second rank. Alternatively, we can define a tensor of the second rank as a physical quantity which, with respect to a set of axes xi, has nine components which transform according to Equation 5.27 when the axes of reference are changed.3 A tensor of the second rank, Tij, is said to be symmetric if Tij = Tji, and to be skew symmetric or antisymmetric if Tij = −Tji. Thus the tensor with components: ⎡ 9 −4 ⎢ −4 7 ⎢ ⎣⎢ 1 2

1⎤ 2 ⎥⎥ 6 ⎥⎦

(5.29)

is symmetric. An antisymmetric tensor necessarily has all the diagonal terms Tij equal to zero, such as the tensor:

Generalizing this definition, a scalar is a tensor of zero rank, because it transforms according to the law r′ = r when the axes are changed. A vector is a tensor of the first rank, because when the axes are changed, its components transform according to the rule pi′ = aij pj (Equation 5.16). Sometimes, the word ‘order’ is used instead of rank to describe the number of suffixes appropriate to a tensor quantity. 3

Kelly_c05.indd 148

11/30/2011 7:19:01 PM

Tensors

β⎤ ⎡ 0 −γ ⎢ γ 0 −α ⎥⎥ ⎢ ⎢⎣ − β α 0 ⎥⎦

149

(5.30)

Whether or not a tensor is symmetric or antisymmetric is independent of the choice of axes. The condition for two tensors to be equal is that each component of one be equal to the corresponding component of the other. Any second-rank tensor may be expressed as the sum of a symmetric tensor and of an antisymmetric tensor. This is because any component Tij can always be written as: Tij = 12 (Tij + T ji ) + 12 (Tij − T ji )

(5.31)

The first term then gives the component of a symmetric second-rank tensor and the second term that of an antisymmetric second-rank tensor. Any symmetric tensor Sij can be transformed by a suitable choice of axes so that it takes on the simple form: 0 0⎤ ⎡ S11 ⎢ 0 S 0 ⎥⎥ 22 ⎢ ⎢⎣ 0 0 S33 ⎥⎦

(5.32)

That is, all Sij = 0 unless i = j. Such a tensor when expressed in this form is said to be referred to its principal axes. When referred to its principal axes, the components S11, S22, S33 are called the principal components and are often written simply as S1, S2, S3, respectively. This second-rank tensor can be written in the form: S1ii + S2 jj + S3 kk

(5.33)

We shall not prove any of the above statements. Proofs can be found in the books listed at the end of this chapter.

5.6 Tensor of the Second Rank Referred to Principal Axes When referred to its principal axes, the symmetric tensor Sij relating vectors p and q only has its diagonal components S11, S22 and S33 as possible non-zero components. Under these circumstances, the equations: pi = Sij q j

(5.34)

p1 = S11q1 , p2 = S22 q2 , p3 = S33q3

(5.35)

reduce to:

Now let us return to the simple example of electrical conductivity. The conductivity tensor sij is symmetric. When referred to its principal axes, all the sij are zero except s11, s22 and s33.

Kelly_c05.indd 149

11/30/2011 7:19:07 PM

150

Crystallography and Crystal Defects x2

J J2 E2

O

E

x1

E1 J1

Figure 5.2

If the crystal under consideration is orthorhombic, monoclinic or triclinic, there is no symmetry requirement that two or more of s11, s22 and s33 have to be equal. For our purposes here we shall assume that none of s11, s22 and s33 are equal. Suppose we apply an electrical field E in the x1–x2 plane with components [E1, E2, 0] along these principal axes. Then: J1 = σ 11 E1 + σ 12 E2 + σ 13 E3 = σ 11 E1

(5.36)

because s12 and s13 are both zero. Similarly, J2 = s22E2. However, J3 = 0 because E3 = 0. We can represent this relationship between J and E on a diagram such as Figure 5.2. This diagram can be constructed by drawing E, finding E1 and E2, and multiplying E1 by s11 to get J1 and E2 by s22 to get J2. We then construct J from its components along the axes; that is, J1 and J2. It should be noted carefully that, in general, J and E are not parallel. If E were directed along Ox1, we would have J1 = s11E1 because then both J2 and J3 would be zero. Likewise, if E were directed along Ox2, J would be parallel to E; J will only be parallel to E if E is directed along a principal axis. When we speak of the conductivity in a particular direction, what we actually mean in practice is that if E is applied in that direction and the current density is measured in the same direction, to give a value Jǁ, the conductivity in this direction is Jǁ divided by the magnitude of E; that is, Jǁ/uEu. We can find an expression for this by resolving J parallel to E. Suppose E is applied in a direction so that its direction cosines with respect to the principal axes of the conductivity tensor are cosa, cosb and cosg. Then we have:

Kelly_c05.indd 150

11/30/2011 7:19:14 PM

Tensors

151

x2 J||

E cos b

22

a os 2

Ec

11

s

s

s22 E cos b

Ec os 2

b

E

O

E cos a

x1

s11 E cos a

Figure 5.3 Derivation of the magnitude of the conductivity in a particular direction. The figure is drawn for s11 = 250 and s22 = 75 (ohm−1 m)−1, so that s22 = 0.3s11

J1 = σ 11 E1 = σ 11 E cosα J 2 = σ 22 E2 = σ 22 E cosβ J 3 = σ 33 E3 = σ 33 E cosγ

(5.37)

where E is the magnitude of E (i.e. uEu). Then, a unit vector nˆ parallel to E is simply the vector [cosa, cosb, cosg ], since cos2a + cos2b + cos2g = 1. Resolving J parallel to E produces a vector parallel to E of magnitude Jǁ = J.nˆ . Hence: J|| = J1 cos α + J 2 cos β + J 3 cos γ = E (σ 11 cos2 α + σ 22 cos2 β + σ 33 cos2 γ ) (5.38) Therefore the conductivity in the direction parallel to E is: σ = J|| / E = σ 11 cos2 α + σ 22 cos2 β + σ 33 cos2 γ

(5.39)

The steps in deriving Equation 5.39 are illustrated diagrammatically in Figure 5.3 for the simple case where E is normal to the principal axis Ox3 of the conductivity tensor, so that cosg = 0. It is instructive to derive the result given in Equation 5.39 in a different way. Suppose we consider the meaning of the component s 11 ′ of the conductivity tensor irrespective of whether it is referred to principal axes. The component s 11 ′ relates the electric field along axis Ox′1 to the component of the current along the same axis Ox′1. If, therefore, we wish to find the value of the conductivity in a particular direction, having been given the components of the conductivity tensor referred to its principal axes, we can proceed as follows: Choose a new set of axes such that Ox′1 is along the direction of interest. Then the component s 11′ of the conductivity tensor referred to this new set of axes gives us the

Kelly_c05.indd 151

11/30/2011 7:19:16 PM

152

Crystallography and Crystal Defects

conductivity along this particular direction – the Jǁ/E. We are only interested in s11′ , so in writing out the array of the aij for this transformation we only need to know the values of the cosines of the angles between Ox′1 and the principal axes of the conductivity tensor, Ox1, Ox2 and Ox3. Following the scheme of the expressions in Equation 5.3, we therefore only need to know a11, a12 and a13. These quantities are cosa, cosb and cosg, respectively. Using the transformation formula in Equation 5.27, we have: σ ij′ = aik a jl σ kl

(5.40)

σ11 ′ = a1k a1l σ kl

(5.41)

and so when i = 1 and j = 1:

Since sij is defined relative to its principal axes, the only non-zero terms within this conductivity tensor are s11, s22 and s33. Therefore: σ11 ′ = a11a11σ 11 + a12 a12σ 22 + a13 a13σ 33

(5.42)

Substituting for a11, a12, a13, we obtain: 2 2 2 σ 11 ′ = σ 11 cos α + σ 22 cos β + σ 33 cos γ

(5.43)

in agreement with Equation 5.39. It is clear that we could have proceeded in exactly the same way to find the conductivity in a particular direction even if the values of the components of sij, the conductivity tensor, had not been given to us referred to principal axes. In that case there would have been, in general, nine terms in the expansion of Equation 5.40. This transformation formula clearly holds irrespective of whether the sij are referred to principal axes. Therefore, we can state that to find the value of a property of a crystal in a particular direction we proceed as follows: Let the components of the tensor representing this property be given as Tij referred to axes (Ox1, Ox2, Ox3). Choose an axis along the direction of interest and call this Ox 1′. Let this axis have direction cosines referred to (Ox1, Ox2, Ox3) of a11, a12, a13, respectively. Then the value of the property T11′ in the direction we are interested in is given by: T11′ = a1i a1 j Tij

(5.44)

This relation holds for all second-rank tensors, whether or not they are symmetrical. This equation can be written in a convenient shorthand notation by removing the dash and the ‘1’ subscripts in Equation 5.44, so that the property T along the direction of interest is: T = li l j Tij

(5.45)

where the relevant direction cosines are now defined as l1, l2 and l3 to conform to the notation used by Nye [1].

Kelly_c05.indd 152

11/30/2011 7:19:20 PM

Tensors

5.7

153

Limitations Imposed by Crystal Symmetry for Second-Rank Tensors

The discussion in this section applies to tensors used to represent physical properties of crystals, and strictly only to perfect single crystals; that is, ones without defects. Suppose two vector quantities p and q are related by the tensor Tij in a crystal so that this tensor represents a property of the crystal. The crystal then determines the relationship between components of p and those of q and we choose to represent this relationship by means of the tensor Tij. We state the components of Tij with respect to certain axes. If we now take a different set of axes in the crystal, the components of p and of q along these new axes will in general be different and, furthermore, the relationship between the components of p and those of q along the new axes will alter because the tensor T′ij referred to these new axes will in general be different from Tij. However, if we select new axes in the crystal which are related to the old ones by some symmetry operation, the values of the components of p and of q with respect to the new set of axes will be different from the values of those referred to the old ones, but the relationship between the components of p and those of q will be the same, so that: Tij′ = Tij This is because the properties of the crystal are the same along the new axes as along the old ones. In order for this to be true for particular symmetry elements, limitations are imposed upon the components of Tij when representing a property of a crystal. The same general type of argument will also impose restrictions upon the components of tensors of the third and higher orders; examples occur in Sections 6.4 and 6.5. The fact that physical properties of crystals should remain the same when the system of coordinates to which the properties are referred are rotated to a new set of coordinates by a symmetry operation was first appreciated by Franz Neumann, who applied this principle to elastic coefficients of crystals in a course in elasticity at the University of Königsberg in 1873/4 [3,4]. While this is one way [5] of defining what has now come to be known as Neumann’s principle, it is nowadays more usual to state the principle in the form: The symmetry elements of a physical property of a crystal must include the symmetry elements of the point group of the crystal [1(p. 20),6,7].

It is important to appreciate that the principle does not state that the symmetry of the physical property is the same as that of the point group: the symmetry of physical properties is often higher than that of the point group. Physical properties characterized by a second-order tensor are necessarily invariant with respect to the operation of a centre of symmetry. This is implicit in the linear relations: pi = Tij q j because if we substitute −pi for pi and −qj for qj (i.e. we reverse the directions of p and of q), the relation is still satisfied by the same values of Tij. In terms of applying Neumann’s principle, this means that physical properties represented by second-order tensors for all

Kelly_c05.indd 153

11/30/2011 7:19:27 PM

154

Crystallography and Crystal Defects

crystals must include the symmetry of 1¯; this will be true even for crystals belonging to noncentrosymmetric point groups. It will assist in understanding what follows if we look at the centre-of-symmetry statement in another way. Suppose that for one set of axes (Ox1, Ox2, Ox3) the relation between the pi and the qj is given by Tij. If we now reverse the axes of reference, leaving p and q the same as before, this corresponds to choosing a new set of axes such that the array of the aij relating the axes is:

x1 New

Old x2 x3

x1′ −1 0 x2′ 0 −1 x3′ 0 0

0 0

(5.46)

−1

Here, all aij are equal to zero unless i = j. We now apply the transformation formula, Equation 5.27: Tij′ = aik a jl Tkl Therefore: Tij′ = aii a jj Tij = Tij since a11 = a22 = a33 = −1

(5.47)

What we have done here is to leave the measured quantities p and q the same and to imagine the crystal inverted through a centre-of-symmetry operation. We have obtained the same result as if we had reversed the directions of p and q. Now suppose the crystal contains a diad axis of symmetry. If we measure a certain property along a certain direction with respect to this axis, and then rotate the crystal 180° about this axis and remeasure the property, we will get the same value as before by Neumann’s principle. This imposes restrictions on the values of the components of any symmetric second-rank tensor Sij which represents this property. In this context, it is relevant that the tensors of the second rank in which we will be interested will all be symmetric. To see what these restrictions are, take axes (Ox1, Ox2, Ox3) and suppose there is a diad axis along Ox2, such as might arise in a material with monoclinic symmetry. Initially, we assume the tensor Sij is symmetric, so that it has six independent components. Now, if we take new axes related to the old by a rotation of 180° about Ox2, the physical property must remain the same as before. The new axes are related to the old by the array of aij as: Old x1 x2 x3 New

Kelly_c05.indd 154

x1′ −1 0 0 x2′ 0 1 0 x3′ 0 0 −1

(5.48)

11/30/2011 7:19:30 PM

Tensors

155

The components of the tensor with respect to the new axes, S′ij, are given in terms of the old components, Sij, by: Sij′ = aik a jl Skl

(5.49)

and we must have S′ij = Sij for all i and j. If we work out the components S′ij one by one, we find: ′ = a11a11S11 = S11 , S11 ′ = a33 a33 S33 = S33 , S33

′ = a22 a22 S22 = S22 , S22 ′ = a11a33 S13 = S13 S13

(5.50)

but: ′ = a22 a33 S23 = −S23 S23

and

′ = a11a22 S12 = −S12 S12

(5.51)

However, we must also have S′23 = S23 and S′12 = S12. Therefore, S23 = S12 = 0. Hence, a symmetrical second-rank tensor representing a physical property of a crystal with a twofold axis of rotational symmetry must have the components S23 and S12 equal to zero when referred to axes so that Ox2 corresponds to the diad axis. The limitations on the components of a symmetrical second-rank tensor representing a physical property of a crystal are summarized in Table 5.2 for each of the seven crystal systems. The derivation of this table is dealt with in Section 5.8 by a rapid method. However, we could deduce part of it using the procedure we have just outlined for a diad axis and applying this to the defining symmetry elements of each of the crystal classes. The constraints listed in Table 5.2 apply to any of the physical properties of a crystal listed in Table 5.1 (see Footnote 4 in this chapter).

5.8

Representation Quadric

The discussion in Section 5.6 demonstrated that the measured value of a property that can be represented by a second-order tensor will vary with the direction of measurement and that this variation can be found by the procedure of that section, leading to Equation 5.45, which is: T = li l j Tij If we expand this equation, we obtain: T = li (l1Ti1 + l2Ti 2 + l3Ti 3 ) (5.52) = l12T11 + l1l2T12 + l1l3T13 + l2l1T21 + l22T22 + l2l3T23 + l3l1T31 + l3l2T32 + l32T33 Here, l1, l2 and l3 are the direction cosines of the direction we are considering with respect to the same axes to which Tij is referred. We shall now restrict our discussion to symmetrical second-rank tensors, so that Tij = Tji. When second-order tensors are used to represent physical properties, in nearly every case the tensor can be shown to be symmetrical (a proof

Kelly_c05.indd 155

11/30/2011 7:19:34 PM

156

Crystallography and Crystal Defects

Table 5.2 Number of independent components of physical properties represented by second-rank (order) tensors Crystal system

Orientation of principal axes with respect to the crystal axes

Form of tensor

Number of independent components

Cubic

Any; representation quadric is a sphere

⎡ S 0 0⎤ ⎢0 S 0 ⎥ ⎢ ⎥ ⎣0 0 S ⎦

1

Tetragonal Hexagonal Trigonala

x3 parallel to 4, 6, 3 or 3¯

⎡ S1 0 0 ⎤ ⎢ ⎥ ⎢ 0 S1 0 ⎥ ⎢⎣ 0 0 S3 ⎥⎦

2

Orthorhombic

x1, x2, x3 parallel to the diads along the x-, y- and z-axes

⎡ S1 0 0 ⎤ ⎢0 S 0 ⎥ 2 ⎢ ⎥ ⎣⎢ 0 0 S3 ⎦⎥

3

Monoclinic

x2 parallel to the diad along the y-axis

⎡ S11 0 S13 ⎤ ⎢0 S 0 ⎥ 22 ⎢ ⎥ ⎢⎣ S13 0 S33 ⎥⎦

4

Triclinic

Not fixed

⎡ S11 S12 S13 ⎤ ⎢S S S ⎥ ⎢ 12 22 23 ⎥ ⎣⎢ S13 S23 S33 ⎥⎦

6

a

A hexagonal cell is used here for trigonal crystals.

always involves thermodynamic considerations).4 We shall show in Chapter 6 that when second-rank tensors are used to represent stresses and small strains, they too are always symmetric. When the tensor is symmetric, terms such as a1a2T12 and a2a1T21 are clearly equal. If we denote the tensor now by Sij, S being chosen to remind ourselves that it is symmetric, we have, from Equation 5.52: S = l12 S11 + l22 S22 + l32 S33 + 2l1l2 S12 + 2l1l3 S13 + 2l2 l3 S23

(5.53)

If Sij were referred to principal axes as well as being symmetric, Equation 5.52 would reduce to: 4 All of the properties listed in Table 5.1 can be shown to be represented by symmetric second-rank tensors [1]. However, in the case of the transport properties in materials, such as electrical or thermal conductivity and diffusion, appeal to experiment is necessary to complete the proof. In some cases, the tensor is definitely not symmetric; examples are the tracer mixing tensor and the antisymmetric stirring tensor, both of which are used in models of ocean circulation behaviour [8].

Kelly_c05.indd 156

11/30/2011 7:19:40 PM

Tensors

S = S1l12 + S2 l22 + S3l32

157

(5.54)

because S12 = S13 = S23 = 0. In Equation 5.54 we have also chosen to use an abbreviated notation, so that the principal axis coefficients are written S1, S2 and S3, rather than S11, S22 and S33. Equation 5.53 is of the same form as the equation to the general surface of the second degree (called a quadric) written in polar coordinates and referred to its centre as the origin. The general equation of a quadric is: 1 r2

= A cos2 α + B cos2 β + C cos2 γ + 2 D cos α cos β + 2 E cos α cos γ + 2 F cos β cos γ

(5.55)

where r is the radius vector and cosa, cosb and cosg are the direction cosines of r with respect to a set of orthogonal axes. When the general surface of the second degree is referred to its principal axes, it takes the form: 1 r2

= A cos2 α + B cos2 β + C cos2 γ

(5.56)

which is of the same form as Equation 5.54. When the axes, to which a general surface of the second degree is referred, are altered, the coefficients in Equation 5.55 transform in the same way as do the components of a symmetrical second-rank tensor. Because of this, the variation of a given property of a crystal with direction, given by Equations 5.53 and 5.54, can be represented by a figure in three-dimensional space, which gives the variation of the property S with direction. The general surface of the second degree can be an ellipsoid or a hyperboloid of one or two sheets. To explain the procedure for representing the variation of the property S with direction in a crystal, we shall confine ourselves to the case where the values of S1, S2 and S3 in Equation 5.54 and A, B and C in Equation 5.56 are all positive. In this case, the second-degree surface, which we shall call the representation quadric, is an ellipsoid.5 Fixing attention on Equations 5.54 and 5.56, we see that if we construct an ellipsoid of semiprincipal axes 1/ S1 , 1/ S2 , 1/ S3 , as in Figure 5.4, so that a general point on the ellipsoid satisfies the equation: S1 x12 + S2 x22 + S3 x32 = 1

(5.57)

then the length r of any radius vector of the ellipsoid (representation quadric) is equal to the reciprocal of the square root of the magnitude of the property S in that direction. Thus, if we return to the example of electrical conductivity, and we know the values s1, s2 and s3 of the components of the electrical conductivity referred to principal axes, then we can construct the conductivity quadric (which, if the sii are all positive, will be an ellipsoid). If now a field E is applied in any direction, the magnitude of the conductivity in that 5 If two of the coefficients S1, S2, S3 are positive and the other one is negative, the quadric is a hyperboloid of one sheet; if two are negative and the other is positive, it is a hyperboloid of two sheets. If all three values are negative, the quadric is an imaginary ellipsoid [1].

Kelly_c05.indd 157

11/30/2011 7:19:48 PM

158

Crystallography and Crystal Defects x3

1 √S3

1 √s3 r

g b

O a 1 √S1

1 √s2

1 √s11′

1 √S2

1 √s1

x2

x1

Figure 5.4 The representation ellipsoid

direction can be found by drawing a radius vector r in the direction of E, measuring the value of r and taking the reciprocal of the square root of r to find the conductivity in that direction. We are now in a position to deal rapidly with the limitations imposed by crystal symmetry on any physical property of a crystal which can be described by a symmetric second-rank tensor. The number of independent coefficients in the equation of the representation surface (Equation 5.55) equals the number of independent components of the tensor representing the physical property (Equation 5.53). If we look for the symmetry of the representation quadric of a property of a crystal belonging to each of the Laue groups,6 we find that the symmetry of the representation quadric for a symmetrical second-rank tensor is governed only by the symmetry of the crystal system. The results are collected in Table 5.2. A cubic crystal must possess four triad axes. The representation quadric is then a sphere, and so the axes, to which the symmetrical second-rank tensor representing any of the properties shown in Table 5.1 is referred, are then of no consequence. The crystal is isotropic with regard to this property. Hexagonal, trigonal and tetragonal crystals have two independent components for the properties indicated in Table 5.1. This is because the representation quadric must be a surface of revolution about the hexad, triad or tetrad, respectively. A general quadric shows three mutually perpendicular diad axes. In the orthorhombic system these must lie along the crystal diads. There are then just three independent 6 The Laue groups are important here because we showed in Section 5.7 that all properties represented by a second-rank tensor are necessarily invariant upon the operation of a centre of symmetry.

Kelly_c05.indd 158

11/30/2011 7:19:54 PM

Tensors

159

p

q Q O

Figure 5.5 The radius–normal property of a representation ellipsoid

components of the tensor necessary to describe the physical property. In the monoclinic system, one of the diad axes of the quadric must lie parallel to the crystallographic diad. There are four independent components of the symmetrical second-rank tensor describing a property. These can be thought of as three necessary to specify the length of the semi-axes of the quadric and one to fix the angle in the plane, normal to the crystal diad, between a crystal axis and a principal axis of the quadric. In the triclinic system there are six independent components possible for any property that may be represented by a symmetrical second-rank tensor – a symmetrical second-rank tensor has to be invariant upon a centrosymmetric operation and the holosymmetric class in this system, 1¯, possesses just a centre of symmetry.

5.9

Radius–Normal Property of the Representation Quadric

The representation ellipsoid has a further very useful property known as the radius–normal property. It can be stated as follows: if Sij are the components of a symmetrical second-rank tensor relating the vectors p and q so that pi = Sijqj then the direction of p for a given q can be found by drawing a radius vector OQ of the representation quadric parallel to q and finding the normal to the quadric at Q. This is shown in two dimensions in Figure 5.5. A proof of this property can be undertaken straightforwardly using the principles of vector calculus applied to surfaces [9]. From Equation 5.57, the equation of the ellipsoid with respect to the principal axes of Sij takes the form: S1 x12 + S2 x22 + S3 x32 = 1, Suppose a unit vector parallel to q has direction cosines l1, l2 and l3 with respect to the three mutually perpendicular principal axes (Ox1, Ox2, Ox3). The vector p in Figure 5.5 will be parallel to the vector [S1l1, S2l2, S3l3]. We wish to determine the normal to the representation ellipsoid at a point such as Q, so that OQ is in the direction of q and is the vector y = [x1, x2, x3] = [rl1, rl2, rl3], where the reciprocal of the square root of r is the property of the tensor Sij in that direction (Section 5.8).

Kelly_c05.indd 159

11/30/2011 7:19:54 PM

160

Crystallography and Crystal Defects

In general from Equation 5.57 we can solve for x3 so that: x3 =

1 − S1 x12 − S2 x22 S3

(5.58)

and: ⎡ y = ⎢ x1 , x2, ⎢⎣

1 − S1 x12 − S2 x22 ⎤ ⎥ S3 ⎥⎦

(5.59)

We can now determine the gradients ∂y/∂x1 and ∂y/∂x2. Since the surface of the representation ellipsoid is smooth, these two gradients define the tangent plane at the point of interest [9]. A vector normal to this tangent plane will be parallel to the vector: n=

∂y ∂x1

×

∂y ∂x2

(5.60)

It is evident from Equation 5.59 that: ⎡ ⎤ ⎡ S1 x1 Sx ⎤ ⎥ = ⎢1, 0, − 1 1 ⎥ = ⎢1, 0, − ∂x1 ⎢ S3 x3 ⎦ S3 1 − S1 x12 − S2 x22 ⎥⎦ ⎣ ⎣ ⎡ ⎤ ⎡ S2 x 2 S x ⎤ ∂y ⎥ = ⎢1, 0, − 2 2 ⎥ = ⎢0, 1, − 2 2 ∂x2 ⎢ S3 x3 ⎦ S3 1 − S1 x1 − S2 x2 ⎥⎦ ⎣ ⎣ ∂y

(5.61)

so that:

i

j

k ⎡S x S x ⎤ Sx n = 1 0 − 1 1 = ⎢ 1 1 , 2 2 , 1⎥ S3 x3 ⎣ S3 x3 S3 x3 ⎦ S x 0 1 − 2 2 S3 x3

(5.62)

That is, n is parallel to the vector: n = [ S1 x1 , S2 x2 , S3 x3 ] = r [ S1l1 , S2 l2 , S3l3 ]

(5.63)

Hence, n is parallel to the vector p. Finally, we note that we could have solved Equation ∂y ∂y 5.57 for either x1 or x2, rather than x3, and then defined n by either n = or × ∂ ∂ x x3 ∂y ∂y 2 n= × as appropriate; we would still have obtained the same result for n. ∂x3 ∂x1

Kelly_c05.indd 160

11/30/2011 7:19:57 PM

Tensors

161

5.10 Third- and Fourth-Rank Tensors Just as a second-rank tensor relates two vectors, so a third-rank tensor relates a second-rank tensor and a vector, and a fourth-rank tensor relates two second-rank tensors, and so on. Thus, for a tensor of the third rank, Tijk, we can envisage a relationship between a secondrank tensor sjk and a vector pi so that, for example: pi = Tijk s jk

(5.64)

Equally, relationships could be of the general form: sij = Tijk pk

(5.65)

where we require the tensor of the third rank to transform as: T ′ijk = ail a jm aknTlmn

(5.66)

generalizing the result in Section 5.4 for a tensor of the second rank. Likewise, a tensor of the fourth rank, Tijkl, can relate two tensors of the second rank, sij and gkl, through an equation of the form: sij = Tijkl gkl

(5.67)

T ′ijkl = aim a jn akp alqTmnpq

(5.68)

where Tijkl transforms as:

We shall consider third- and fourth-rank tensors in more detail in Chapter 6, once we have introduced the two important field tensors of stress and strain.

Problems 5.1 Define a tensor of the second rank. Write down two physical properties of crystals that can be represented by a second-rank tensor, and for each state the two physical quantities that are related by the tensor. For one of your examples, write down in full the equations relating the components of the two physical quantities and explain your notation. Explain the physical significance of the tensor component D12, where D is the diffusivity tensor. 5.2 Explain why the array of the aij in Equation 5.3 does not represent the components of a second-rank tensor. 5.3 Express the following tensor as the sum of a symmetric tensor and an antisymmetric tensor: ⎛ 12 6 0⎞ ⎜ 4 7 0⎟ ⎜ ⎟ ⎝ 0 0 3⎠

Kelly_c05.indd 161

11/30/2011 7:20:06 PM

162

Crystallography and Crystal Defects

5.4 If s is a symmetric dyadic and n and b are vectors, show that: (σ ⋅ n) ⋅ b = (σ ⋅ b) ⋅ n 5.5 A crystal possesses a single four-fold rotational axis of symmetry parallel to the z-axis. Find the necessary relations between the components of a second-rank tensor representing a physical property of the crystal when the tensor is referred to axes parallel to the crystal axes. How can this result be reconciled with the entry for tetragonal crystals in Table 5.2? 5.6 Prove that whether a tensor is symmetric or antisymmetric is independent of the choice of axes. Hint: show that if Tij = Tji then T′ij = T′ji. 5.7 The electrical conductivity of an orthorhombic crystal, with lattice parameters a = 10.2 Å, b = 7.8 Å and c = 6.3 Å, is found in general to be anisotropic. However, in a (hk0) plane whose normal is 52° to the [010] axis, the electrical conductivity is isotropic. In a separate experiment on the same crystal, it was found that the magnitude of the electrical conductivity in the [001] direction was 4 × 107 Ω−1m−1 and that the electrical conductivity in the [010] direction was three times that in the [100] direction. (a) Determine the electrical conductivity tensor of the crystal with respect to the crystallographic axes of the orthorhombic crystal. (b) Determine the electrical conductivity in the [110] direction. 5.8 (a) The electrical conductivity tensor of a crystal has the components: ⎛ 18.25 − 3 × 2.25 0⎞ ⎜ ⎟ σ ij = ⎜ − 3 × 2.25 22.75 0⎟ × 108 Ω −1m −1 ⎜ 0 0 9⎟⎠ ⎝ Take new axes rotated 60° about x3 in a clockwise direction looking along negative x3 and write down a table of the direction cosines between the new and old axes as in Section 5.2. Check that the sum of the squares of the aij in each row and column equals 1. (b) Write down the components of the conductivity tensor referred to the new axes. Check that sij has not altered. The tensor is now referred to principal axes. (c) Draw a section of the representation quadric (i.e. the conductivity ellipsoid in this case) in the plane x′3 = 0. Draw radius vectors of the resulting ellipse at angles of 30° and 60° to x′1 and hence find the conductivity in these directions. (d) Check your results in (c) by direct calculations. (e) Suppose an electric field E of 100 Vm−1 is established in a direction at 60° to x′1 in the plane x′3 = 0. Write down the components of this electric field along x′1 and x′2 and hence find the electric current densities in these two directions. Finally, find the component of the resultant current density along E and hence the electrical conductivity in this direction. (f) Find the direction of the resultant current vector J in (e). (g) Draw the direction of the resultant current density vector on your diagram prepared in (c) and confirm that J is parallel to the normal to the surface of the representation quadric at the point where a vector from the origin parallel to E meets the representation quadric.

Kelly_c05.indd 162

11/30/2011 7:20:13 PM

Tensors

163

Suggestions for Further Reading D.R. Lovett (1999) Tensor Properties of Crystals, 2nd Edition, Adam Hilger, Bristol and Philadelphia. J.F. Nye (1985) Physical Properties of Crystals, Clarendon Press, Oxford. D.E. Sands (1982) Vectors and Tensors in Crystallography, Addison-Wesley, Reading, Massachusetts and London. W.A. Wooster (1973) Tensors and Group Theory for the Physical Properties of Crystals, Clarendon Press, Oxford.

References [1] J.F. Nye (1985) Physical Properties of Crystals, Clarendon Press, Oxford. [2] A. Einstein (1916) Die Grundlage der allgemeinen Relativitätstheorie, Annalen der Physik, 49, 769–822. [3] F. Neumann (1885) Elasticität krystallinischer Stoffe, Chapter 12 in O.E. Meyer and B.G. Teubner (eds) Vorlesungen über die Theorie der Elasticität der festen Körper und des Lichtäthers, Leipzig, pp. 164–202. [4] S. Katzir (2004) The emergence of the principle of symmetry in physics, Historical Studies in the Physical and Biological Sciences, 35, 35–65. [5] W.A. Wooster (1973) Tensors and Group Theory for the Physical Properties of Crystals, Clarendon Press, Oxford, p. 15. [6] P. Gay (1972) The Crystalline State, Oliver and Boyd, Edinburgh, p. 259. [7] D.R. Lovett (1999) Tensor Properties of Crystals, 2nd Edition, Adam Hilger, Bristol and Philadelphia, p. 31. [8] S.M. Griffies (1998) The Gent–McWilliams skew flux, J. Phys. Oceanogr., 28, 831–841. [9] K.F. Riley, M.P. Hobson and S.J. Bence (2006) Mathematical Methods for Physics and Engineering, 3rd Edition, Cambridge University Press, Cambridge, pp. 345–347.

Kelly_c05.indd 163

11/30/2011 7:20:16 PM

6 Strain, Stress, Piezoelectricity and Elasticity 6.1

Strain: Introduction

When forces are applied to crystals or when imperfections are formed inside them the atoms change their relative positions. This change in the relative positions is called strain, and in this section we describe a way of specifying it. The basic ideas of strain are those of extension and shear. The first is easily understood. Consider a very thin rod of length l (Figure 6.1a). Let the rod be stretched so that l′ is its length in the strained state. Then the extension, e, is defined as: e=

l′ − l l

(6.1)

That is: l ′ = l (1 + e) Thus e is the ratio of the change in length to the original length. It is positive in tension and negative in compression. Shear is a measure of the change in angle between two lines in a body when the body is distorted. It is defined as follows (Figure 6.1b). If OP, OR are two perpendicular straight lines in the unstrained state and O′P′, O′R′ are the positions of the corresponding lines in the strained state then the (engineering) shear strain g associated with these two directions at the point O is defined as: γ = tan

⎛ π − θ⎞ ⎝2 ⎠

(6.2)

Crystallography and Crystal Defects, Second Edition. Anthony Kelly and Kevin M. Knowles. © 2012 John Wiley & Sons, Ltd. Published 2012 by John Wiley & Sons, Ltd.

Kelly_c06.indd 165

11/30/2011 7:08:07 PM

166

Crystallography and Crystal Defects (a)

(b) P

l

P′

tan–1γ

l′ θ

R′

O′

l′ l

O

Figure 6.1

R

(a) Definition of extension. (b) Definition of shear

where q is the angle between O′P′ and O′R′ in the strained state. The description of general distortions, involving both extensions and shears, can be very complicated. We shall consider two important special cases: 1. Infinitesimal strain, where it is assumed that the quantities e and g are so small that their squares and products can be neglected. For elastic strains within a crystal, this assumption is a good one, except at points which are only a very few atomic distances from a defect. 2. Homogeneous strain, where every part of the strained region suffers the same distortion. Large homogeneous strains will be encountered in Chapters 7, 11 and 12. In this chapter we will restrict our attention to infinitesimal strains, because these are relevant for a description of how elastic strains affect perfect crystals when considering piezoelectricity and elasticity. Homogeneous strains are considered in Appendix 6. The discussion of homogeneous strains in the context of slip, twinning and martensitic transformations will be deferred to the relevant chapters later in the book.

6.2

Infinitesimal Strain

The distortion of a body can be described by giving the displacement of each point from its location in the undistorted state. Any displacements which do not correspond to a translation or rotation of the body as a whole will produce a strain. We now confine ourselves to two dimensions and choose an origin fixed in space such as O in Figure 6.2. Let P be a point with coordinates (x1, x2) in the unstrained state, which after distortion of the body moves to the point P′. (Then the displacement of the point P is the vector PP′.) Let the coordinates of P′ be (x1 + u1, x2 + u2). Now consider a point Q with coordinates (x1 + dx1, x2 + dx2) lying infinitesimally close to P in the unstrained state. After deformation, Q moves to Q′. Now, in a strained body, the displacement of Q will not be exactly the same as that of P. The displacement of Q to Q′ has components (u1 + du1, u2 + du2). We can write: du1 =

Kelly_c06.indd 166

∂u1 ∂x1

dx1 +

∂u1 ∂x2

dx2

(6.3)

11/30/2011 7:08:08 PM

Strain, Stress, Piezoelectricity and Elasticity

167

Q′

x2 P′

Q P

x1

O

Figure 6.2

and: ∂u2

du2 =

dx1 +

∂x1

∂u2 ∂x2

dx2

(6.4)

Defining the four quantities at the point P: e11 =

∂u1 ∂x1

,

e12 =

∂u1 ∂x2

e22 =

,

∂u2 ∂x2

,

e21 =

∂u2 ∂x2

,

(6.5)

Equations 6.3 and 6.4 can be compactly written as: dui = eij dx j

( j = 1,2)

(6.6)

Since dui and dxj are vectors, according to the definition given in Chapter 5, eij is a tensor, which we can term the relative displacement tensor. We shall now demonstrate the physical meaning of the various eij when each is very small compared to unity. Let us take two special positions of the vector PQ: first parallel to Ox1 (PQ1) and then parallel to Ox2 (PQ2), and find out how a rectangular element at P is distorted (Figure 6.3). For PQ1 we put dx2 = 0 and obtain: du1 = du2 =

∂u1 ∂x1 ∂u2 ∂x1

dx1 = e11 dx1

(6.7)

dx1 = e21 dx1

(6.8)

From Figure 6.3 it is clear that e11 measures the extension per unit length of PQ1 resolved along Ox1, while e21 measures the anticlockwise rotation of PQ1, provided that e11 and e21 are small. Similarly, e22 measures the change in length per unit length of PQ2, resolved along Ox2, and e12 measures the small clockwise rotation of PQ2. This relative displacement tensor eij is not completely satisfactory as a measure of strain, because it is possible to have non-zero components of eij without there being any distortion of the body. Thus, consider a rigid-body rotation through a small angle w, illustrated in

Kelly_c06.indd 167

11/30/2011 7:08:08 PM

168

Crystallography and Crystal Defects x2

Q′2

Q′1

Q2 P′

dx1

P

du2 dx1 + du1

Q1 x1

O

Figure 6.3

x2

Q'2

Q2 w Q'1 P

w Q1

O

x1

Figure 6.4

Figure 6.4. Evidently we have e11 = e22 = 0, but e12 = −w and e21 = w (since for small angles, tan w = w − O(w3) ≅ w, neglecting the higher-order terms because we are considering infinitesimal relative displacements). To remove the component of rotation from a general eij we express it as the sum of a symmetrical tensor, eij, and an antisymmetrical tensor, wij, so that: eij = ε ij + ω ij = 1 (eij + e ji ) + 1 (eij − e ji ) 2

ε ij =

1 2

2

(eij + e ji ) is then defined as the pure strain and ω ij =

1 2

(6.9)

(eij − e ji ) measures the rota-

tion (as in Figure 6.4). The geometrical interpretation of Equation 6.9 is shown in Figure 6.5. It should be noted that the change in angle between the two lines originally at right angles in Figure 6.5 is 2e12. Therefore, the shear component of the pure strain tensor e12 is half the engineering shear strain g defined in Equation 6.2. In specifying infinitesimal strain in three dimensions, the method is the same as for two dimensions. The variation of displacement u (= u1, u2, u3) with variation in position x (= x1, x2, x3) is used to define nine components of a relative displacement tensor eij:

Kelly_c06.indd 168

11/30/2011 7:08:08 PM

Strain, Stress, Piezoelectricity and Elasticity 1 2

e12

1 2

(e12+e21)

=

169

(e12–e21)

+

e21 e12

e12

=

+

w12

Figure 6.5

eij =

∂ui

(i, j = 1, 2, 3)

∂x j

(6.10)

The strain tensor eij is then defined as the symmetrical part of eij: ε ij = 1 (eij + e ji )

2

(6.11)

In full: ⎡ ε11 ⎢ ⎢ ε12 ⎢⎣ ε13

ε12 ε 22 ε 23

1 (e + e ) 1 (e + e ) ⎤ ⎡ e11 21 31 2 12 2 13 ⎢ ⎥ ⎥ 1 (e + e ) ⎥ e22 ε 23 ⎥ = ⎢ 1 (e21 + e12 ) 32 ⎥ 2 23 ⎢2 ε 33 ⎥⎦ ⎢ 1 ⎥ 1 (e + e13 ) (e + e23 ) e33 2 32 ⎣⎢ 2 31 ⎦⎥ ε13 ⎤

(6.12)

The diagonal components of eij are the changes in length per unit length of lines parallel to the axes and are called the tensile strains. The off-diagonal components measure shear strains so that, for instance, e13 is one-half the change in angle between two lines originally parallel to the Ox1 and Ox3 axes. Since pure strain is a symmetrical second-rank tensor, it can be referred to principal axes (Chapter 5). Under these circumstances, the shear components vanish and we have: ⎡ ε1 ε = ⎢⎢ 0 ⎢⎣ 0

0 ε2

0

0⎤ 0 ⎥⎥ ε 3 ⎥⎦

(6.13)

The geometrical meanings of the principal strains e1, e2 and e3 are shown in Figure 6.6, which shows that a unit cube whose edges are parallel to the principal axes is changed into a rectangular-sided figure with edges (1 + e1), (1 + e2) and (1 + e3). The change in volume per unit volume is called the dilatation, and is given by: Δ = (1 + ε1 ) (1 + ε 2 ) (1 + ε 3 ) − 1 = ε1 + ε 2 + ε 3

(6.14)

where terms such as e1e2 and e1e2e3 have been neglected, since the strains are infinitesimal. When the strain is referred to any other axes, the dilatation is always given by the invariant

Kelly_c06.indd 169

11/30/2011 7:08:09 PM

170

Crystallography and Crystal Defects (l + e ) 1

x2

l l

(l + e2)

l

(l +

O

e 3)

x1

x3

Figure 6.6

sum of the trace of the strain matrix, (e11 + e22 + e33). (This is a general result for symmetrical tensors of the second rank, the proof of which follows from the properties of similarity transformations and can be found in references [1–4] of Appendix 1.) The components of either eij or eij can be transformed to new axes by means of the standard transformation rule for second-rank tensors (Chapter 5). In a number of books on elasticity, the strain is described by the quantities: ⎡ εx ⎢ ⎢γ xy ⎢ ⎣⎢γ zx

γ xy

γ zx ⎤

εy

γ yz ⎥

γ yz

⎥

⎥ ε z ⎦⎥

(6.15)

We then see that, for instance, gxy ≡ 2e12. The g values are usually called shear strains or engineering shear strains, and it should be noted that they are equal to twice the corresponding tensor shear strains defined in this book. This array of the values of e and g does not form a tensor.

6.3

Stress

When atoms in a crystal are displaced relative to one another, forces act on them, tending to restore their normal spatial relationship. If a plane is passed through a strained region of crystal, it will be found that the atoms on one side of the plane are exerting forces upon the atoms on the other side. At any point on the plane, the force acting per unit area of plane is defined as the traction on the plane at that point. The force is customarily resolved into components normal and parallel to the plane, fn and fs, respectively, and corresponding normal and shear stress components, sn and t, are defined as follows: fn σ n = δ Lt (6.16) A→ 0 δA τ = δ Lt A→ 0

fs δA

(6.17)

The area d A is shown in Figure 6.7; it surrounds the point P, so that by finding the limit of the series of average stresses f/d A as d A decreases, the stress at the point itself can be

Kelly_c06.indd 170

11/30/2011 7:08:09 PM

Strain, Stress, Piezoelectricity and Elasticity ƒn

171

ƒ

ƒs

P dA

Figure 6.7 x3 (z)

(a)

s31 (τzx)

s33 (z)

s13 (τxz)

(x)

(x)

s12 (τxy)

s21 (τyx)

sz

z

szr

szq s32 (τzy) srq

s23 (τyz)

s11 x1

(b)

sq r

sr

sq

srz

s22 (sy)

sq z x2 (y)

q

Figure 6.8 Definition of stress components (a) in Cartesian coordinates and (b) in cylindrical polar coordinates

defined. For this definition to be meaningful, the force at P must not be changing too sharply on an atomic scale. The procedure outlined above could be repeated for any plane passing through the point P. To define the stress at P completely, it is sufficient to specify the stresses acting on three mutually perpendicular planes passing through P. It is then possible to calculate the stress acting on any other plane by means of a force balance. The stresses acting on the faces of an infinitesimal cube located at P are shown in Figure 6.8a, using two alternative notations. In the numerical suffix notation, the stress component sij is the component in the direction of the xj-axis of the traction acting on the face whose normal is parallel to xi.1 The sign convention is that a stress is positive if the force component and the outward-going 1 Nye [1] and Lovett [2] use a notation where sij is the component in the direction of the xi-axis of the traction acting on the face whose normal is parallel to xj. The notation we have chosen is that used elsewhere, such as [3–6], but, irrespective of which notation is used, sij = sji in equilibrium. There is no single ‘correct’ notation.

Kelly_c06.indd 171

11/30/2011 7:08:09 PM

172

Crystallography and Crystal Defects x3 C P s11

B

x2

s21 s22 O s 23

s31 s33 A

Figure 6.9

x1

Calculation of the stress acting on the plane ABC

normal of the face on which it acts have the same sense, relative to the axes to which they are respectively parallel. The letter suffix notation follows the same pattern, except that shear stresses are distinguished by the letter t. It is sometimes convenient to work with cylindrical polar coordinates instead of Cartesian coordinates, and the stress components for this case are shown in Figure 6.8b. As the cube in Figure 6.8a is supposed to be infinitesimally small, the forces acting on opposite faces must be equal and opposite. If the cube were of side d, the shear stresses txy and tyx would produce a couple (txy − tyx) d 3, tending to rotate the cube about the z-axis. Since the moment of inertia of the cube varies as d 5, it vanishes as d → 0 more rapidly than does the couple (txy − tyx) d 3, so that, to avoid an infinite angular acceleration: τ xy = τ yx

and in general in equilibrium: σ ij = σ ji

(6.18)

In order to calculate the stress acting upon any given plane at P, an infinitesimal body is constructed having one face, ABC, parallel to the given plane and all its other faces parallel to the cube faces (Figure 6.9). A balance of the forces acting on the tetrahedron ABCO then determines the required stress. Let P = [P1P2P3] be the traction exerted on the face ABC by the material outside the tetrahedron. Setting the sum of forces in the Ox1 direction equal to zero: P1 ( ABC ) = σ 11 ( BOC ) + σ 21 ( AOC ) + σ 31 ( AOB)

(6.19)

Now, the volume of a tetrahedron is (area of base × perpendicular height)/3. If we specify the perpendicular from O to ABC to be d then evidently: d. (ABC ) = OA.( BOC ) = OB.( AOC ) = OC.( AOB)

Kelly_c06.indd 172

(6.20)

11/30/2011 7:08:10 PM

Strain, Stress, Piezoelectricity and Elasticity

173

and so: d d d ( BOC ) ( AOC ) ( AOB) = = l1 ; = = l2 ; = = l3 ( ABC ) OA ( ABC ) OB ( ABC ) OC

(6.21)

where l1 is the cosine of the angle between the normal to ABC and Ox1, and so on for l2 and l3. Hence: P1 = σ 11l1 + σ 21l2 + σ 31l3

(6.22)

where li are the direction cosines of the normal to the plane ABC. We obtain similar equations for P2 and P3, and all three equations can be written compactly as: Pi = σ ji l j

(6.23)2

Resolving P into two components, one normal and one parallel to ABC, we can obtain the normal stress sn and shear stress t, where sn is given by the sum of the components Pi, each resolved normal to ABC: σ n = Pl i i

Therefore, from Equation 6.23: σ n = σ ji l j li

(6.24)

By resolving the forces: τ = ⎡⎣ P 2 − σ n2 ⎤⎦

1/2

(6.25)

where P is the magnitude of P. It is apparent from Equation 6.23 that the components of the vector P representing the traction on a plane are linearly related to those of the unit vector which is normal to that plane. It follows that the relating coefficients sij form a tensor of the second rank. When the axes of reference are rotated, the components of a given stress transform according to the general transformation law: σ ij = aik a jl σ kl

(6.26)

where aij is the cosine of the angle between the new Oxi-axis and the old Oxj-axis (Chapter 5). Because the stress tensor is symmetrical (sij = sji), it is always possible to find a set of axes, the principal axes, so that a cube with its edges parallel to them has no shear stresses acting upon its faces. Referred to the principal axes, the stress takes the form: ⎛ σ1 0 ⎜0 σ 2 ⎜ ⎝0 0

2

0⎞ 0⎟ ⎟ σ3 ⎠

(6.27)

It is evident that this equation is written Pi = sijlj in the notation used by Nye [1] and Lovett [2].

Kelly_c06.indd 173

11/30/2011 7:08:10 PM

174

Crystallography and Crystal Defects

where s1, s2 and s3 are called the principal stresses. In very special cases, a body may be under a homogeneous stress; that is, the stress may be the same at every point. If the stress is homogeneous, parallel cubes of any size and at any location have the same tractions on their faces. Such a condition obtains in the tensile test of a uniform rod, the stress at every point being: ⎛ F/A 0 0⎞ ⎜ ⎟ 0 0⎟ ⎜ 0 ⎜ 0 0 0 ⎟⎠ ⎝

(6.28)

where F is the tensile force and A is the cross-sectional area of the rod, and the tensile axis is parallel to Ox1. More generally, the stress in a body varies from point to point. However, the different components of stress cannot vary in an entirely arbitrary way, independently of one another. The variations in the different stress components must be related in such a way that there is a balance of the forces acting on any internal body (assuming that the body as a whole is in static equilibrium). One face of a cube of side 2d in a varying stress field is shown in Figure 6.10. By setting the sum of forces in the Ox1 direction equal to zero, we obtain: ∂σ 11 ∂x1

+

∂σ 21 ∂x2

+

∂σ 31 ∂x3

+ f1 = 0

(6.29)

where f1 is the component of body force per unit volume (e.g. due to gravity) acting in the Ox1 direction. Two similar equations are obtained with respect to the Ox2 and Ox3 directions, and all three equations of equilibrium can be written compactly as: ∂σ ij ∂xi

+ fj = 0

(6.30)

The repetition of the suffix i in Equation 6.30 implies the summation of the differential coefficients obtained by setting i = 1, 2 and 3 in turn. We shall now mention some important types of stress. A pure shear stress is of the form s12 = S, with all other sij zero, or: ⎛ 0 S 0⎞ ⎜ ⎟ ⎜S 0 0⎟ ⎜ 0 0 0⎟ ⎝ ⎠

(6.31)

When the axes of reference are rotated through 45° about Ox3, in an anticlockwise sense, the stress components transform to: ⎛S 0 0⎞ ⎜ ⎟ ⎜ 0 −S 0 ⎟ ⎜ 0 0 0⎟ ⎝ ⎠

Kelly_c06.indd 174

(6.32)

11/30/2011 7:08:10 PM

Strain, Stress, Piezoelectricity and Elasticity (s22 +

⭸s22 d) ⭸x2

(s12 +

(s11

⭸s12 d) ⭸x2

(s12 +

⭸s11 d) ⭸x1 P (s12

⭸s12 d) ⭸x1

(s11 +

⭸s12 d) ⭸x1

(s12

175

⭸s11 d) ⭸x1

⭸s12 d) ⭸x2 (s22

⭸s22 d) ⭸ x2

Figure 6.10

S

S

S S

P

P

Figure 6.11 A shear stress at the point P

The principal stresses of a pure shear are therefore equal tensile and compressive stresses acting on planes at 45° to those on which the shear stress acts alone (Figure 6.11). In a general state of stress, shear stress components exist on all planes other than those normal to the principal axes. It can be shown that the largest shear stress occurs on the plane which bisects the angle between the planes on which the greatest and least of the principal stresses act (Figure 6.12). If s1 < s2 < s3, the magnitude of the largest shear stress is 12 (σ 3 − σ 1 ) . A hydrostatic pressure p takes the form: 0 ⎞ ⎛−p 0 ⎜ ⎟ 0 − p 0 ⎟ ⎜ ⎜ 0 0 − p ⎟⎠ ⎝

Kelly_c06.indd 175

(6.33)

11/30/2011 7:08:10 PM

176

Crystallography and Crystal Defects s3 tmax

tmax

s1

Figure 6.12 If σ3 is the largest principal stress and σ1 is the smallest, the largest shear stress acts in the direction shown, on a plane that is normal to the plane of the figure

which remains the same no matter what axes of reference are chosen. In other words, a hydrostatic pressure produces no shear stress anywhere. It is possible to produce any state of stress by superimposing a hydrostatic pressure or tension upon three pure shear stresses. To prove this, we note that a general stress can be written as the sum of a hydrostatic component and a component called the deviatoric stress. Referred to principal axes, the stress can be written as: ⎛ σ1 0 ⎜0 σ 2 ⎜ 0 0 ⎝

0⎞ ⎛ σ ii 1⎜ ⎟ 0 = 0 ⎟ 3⎜ σ3 ⎠ ⎝ 0

0 σ ii

0

⎛σ − 1 σ 0 ⎞ ⎜ 1 3 ii 0⎟ +⎜ 0 ⎟ ⎜ σ ii ⎠ ⎜ 0 ⎝

0

⎞ ⎟ ⎟ 0 ⎟ (6.34) 1 σ 3 − σ ii ⎟⎠ 3 0

σ 2 − 1 σ ii

3

0

where sii = s1 + s2 + s3. The hydrostatic component 13 σ ii is invariant, because the sum (s11 + s22 + s33) remains the same whatever axes of reference are chosen, since, just like strain tensors (Section 6.2), stress tensors are symmetrical second-rank tensors. The deviatoric stress can be expressed as the sum of three pure shear stresses, as follows: ⎛ σ 1 − 1 σ ii 3 ⎜ ⎜ 0 ⎜ ⎜ 0 ⎝ ⎛ σ1 − σ 3 1 + ⎜ 0 3⎜ ⎝ 0

Kelly_c06.indd 176

0 σ 2 − 1 σ ii 3

0

⎞ ⎛ σ1 − σ 2 ⎟ 1⎜ ⎟ 0 = 0 ⎟ 3⎜ 0 ⎝ σ 3 − 1 σ ii ⎟⎠ 3 0

0 σ 2 − σ1 0

0 0 ⎞ 0 0 ⎞ ⎛0 1 0 0 ⎟ + ⎜ 0 σ2 − σ3 0 ⎟ ⎟ 3⎜ ⎟ 0 σ 3 − σ1 ⎠ 0 σ3 − σ2 ⎠ ⎝0

0⎞ 0⎟ ⎟ 0⎠ (6.35)

11/30/2011 7:08:10 PM

Strain, Stress, Piezoelectricity and Elasticity 3

177

1'

2' 2

1

3' 'New' set of axes

'Old' set of axes

Figure 6.13

6.4

Piezoelectricity

When some single crystals are stressed in uniaxial tension, an electric polarization, P, can occur within the crystal, the magnitude of which increases linearly with the magnitude of the stress. This manifests itself through the development of electrical charges on the surfaces of the crystals. P is a vector describing the electric dipole moment per unit volume, or equivalently, the surface charge developed per unit area [1,7]. Conversely, the application of an electric field, E, to these single crystals produces a strain within the crystals, and again there is a linear relationship between the magnitude of the electric field and the magnitude of the strain produced. This phenomenon is known as piezoelectricity and was first discovered by Pierre and Jacques Curie in 1880 [7]. The piezoelectric tensor, dijk, is a tensor of the third rank which relates the stress applied, sjk, to the polarization produced, Pi: Pi = dijk σ jk

(6.36)

Reversing the sign of sjk reverses the sign of Pi. As we will now demonstrate, it is straightforward to show that this means that centrosymmetric crystals cannot exhibit piezoelectricity using Neumann’s principle (Section 5.7). From Equation 5.66, tensors of the third rank transform as: T ′ijk = ail a jm aknTlmn If a crystal has a centre of symmetry at the origin, the direction [uvw] maps exactly on to –] for all u, v and w. We can examine what happens to the d specified the direction [u– –v w ijk relative to an ‘old’ orthonormal set 1, 2 and 3 if we then choose new orthonormal axes 1′, 2′ and 3′ related to 1, 2 and 3 by the centre of symmetry (Figure 6.13). Under these circumstances, aij = − dij, where dij is the Kronecker delta, since the angle between the ith ‘old’ axis and the jth ‘new’ axis is either 90 or 180°. Hence, the elements of the tensor dijk produce transformed moduli so that: dijk ′ = ail a jm akn dlmn = − δ il δ jm δ kn dlmn = − dijk

(6.37)

However, if the crystal has a centre of symmetry, and we have performed this centre-ofsymmetry operation, the transformed modulus d′ijk defined with respect to the ‘new’ axis set must be equal to the modulus dijk defined with respect to the ‘old’ axis set. That is, we require:

Kelly_c06.indd 177

11/30/2011 7:08:11 PM

178

Crystallography and Crystal Defects

′ = dijk dijk

(6.38)

for all i, j and k. For Equations 6.37 and 6.38 to be compatible, it follows that dijk = 0 for all i, j and k, so that we can conclude that materials with a centre of symmetry have zero piezoelectric moduli, and are not therefore piezoelectric. Of the 32 crystal classes, 21 are noncentrosymmetric (Chapter 2); a necessary (but not sufficient) condition for a crystal to exhibit piezoelectricity is that it belongs to a noncentrosymmetric crystal class. In principle, we might expect the tensor dijk to have 27 independent components. However, the fact that for a shear stress, skj = sjk, irrespective of body torques being present [8], means in turn that dikj = dijk and so there are actually at most 18 independent coefficients of dijk. At this stage, it becomes possible to introduce a contracted notation in which two suffixes are replaced by one, both in sjk and in dijk. The notation for the stress sij is contracted as follows: ⎛ σ 11 σ 12 ⎜σ σ 22 ⎜ 12 ⎝ σ 13 σ 23

σ 13 ⎞

⎛ σ1

σ 23 ⎟ → ⎜ σ 6

⎟ σ 33 ⎠

⎜ ⎝σ5

σ6 σ2 σ4

σ5 ⎞

σ4 ⎟

⎟ σ3 ⎠

(6.39)

A similar procedure applies to dijk, but in this case it is necessary to introduce factors of into the contracted form of dijk: dijk → dmn for n = 1, 2 and 3 dijk →

1 dmn for n = 4, 5 and 6 2

1 2

(6.40a) (6.40b)

The new dmn form a 3 × 6 matrix of 3 rows and 6 columns, but are not tensors. It is instructive to see why the factors of 12 arise by examining one component of Equation 6.36. For example, when i = 2: P2 = d211σ 11 + d212σ 12 + d213σ 13 + d221σ 21 + d222σ 22 + d223σ 23 + d231σ 31 + d232σ 32 + d233σ 33 from which it is evident that the two terms d212s12 and d221s21 in the full notation become together d26s6 in the contracted notation only if the factor of 12 is included. Similar considerations apply to the other terms for n = 5 and 6 in this equation. The zero and non-zero dij for a particular crystal class can be represented conveniently using a matrix notation introduced by van Dyke in 1950 [9]. In this notation, and the variation used by Nye [1], non-zero dij are represented by large filled dots, •, zero dij are represented by either small dots or a space, numerically equivalent dij are joined by lines, and rings denote values which are the negative of •. A complete presentation of the piezoelectric moduli in this form for each crystal class is given in Appendix E of Nye [1]. Here, we will restrict our attention to consideration of determining the non-zero dij of a few noncentrosymmetic crystal classes.

Kelly_c06.indd 178

11/30/2011 7:08:11 PM

Strain, Stress, Piezoelectricity and Elasticity

179

3 1'

2

2'

1 3' 'Old' set of axes

Figure 6.14

6.4.1

'New' set of axes

180° rotation about [010]

Class 2

In this crystal class there is a single 180° rotation axis. Let this be about x2 in a crystal. ‘Old’ and ‘new’ axes can be defined as in Figure 6.14. The only non-zero aij are a11 = −1, a22 = 1 and a33 = −1. Hence, for example: d113' = a11a11a33 d113 = − d113 ; d112' = a11a11a22 d112 = d112

(6.41)

However, because of the diad axis, d113 ′ must be equal to d113 and d112 ′ must be equal to d112. Hence, we conclude that d113 = 0 but d112 ≠ 0. Thus, if in the transformation from dijk to d′ijk the sign is +1, the modulus is non-zero, but if the sign is −1, the modulus is zero. Clearly, only those dijk with either a single ‘2’ or three ‘2’s survive. Hence the non-zero moduli are the eight in bold in the array: d111

d112 d122

d113 d123 d133

d 211

d212 d 222

d 213 d223 d 233

d311

d312 d322

d313 d323 d333

(6.42)

which then become the eight dots in the corresponding matrix representation: ⎛ ⋅ ⋅ ⋅ • ⋅ •⎞ ⎜ ⎟ ⎜• • • ⋅ • ⋅ ⎟ ⎜ ⋅ ⋅ ⋅ • ⋅ •⎟ ⎝ ⎠ 6.4.2

(6.43)

Class 222

Here, the occurrence of two mutually perpendicular diads forces the third one to occur (Section 1.6). Of the eight non-zero dij in Class 2, only d14, d25 and d36 are non-zero for Class 222 (Problem 6.9), so that the matrix representation is the following: ⎛⋅ ⋅ ⋅ • ⋅ ⋅ ⎞ ⎜ ⎟ ⎜⋅ ⋅ ⋅ ⋅ • ⋅ ⎟ ⎜⋅ ⋅ ⋅ ⋅ ⋅ •⎟ ⎝ ⎠

Kelly_c06.indd 179

(6.44)

11/30/2011 7:08:11 PM

Crystallography and Crystal Defects

180

3

2'

2

3'

1 'Old' set of axes

Figure 6.15

6.4.3

1'

'New' set of axes

120° rotation about [111]

Class 23

Crystal Class 23 has three mutually perpendicular diads and four triad axes along and belongs to the cubic crystal system. Clearly, from the above consideration of Class 222, we know that there are at most three independent dij in Class 23 before we consider the effect of the triad axes. Suppose we examine the effect of a 120° anticlockwise rotation about [111]. In terms of the ‘old’ axes, this is 1 → 2, 2 → 3 and 3 → 1 (Figure 6.15). The only non-zero aij are a12 = 1, a23 = 1 and a31 = 1. Thus, for example: d123′ = a11a22 a33 d123 + a11a23 a32 d132 + a12 a21a33 d213 + a12 a23 a31d231 + a13 a21a32 d312 + a13 a22 a31d321 reduces to: d123′ = a12 a23 a31d231 = d231

(6.45)

and likewise d231′ = d312 and d312′ = d123. Thus, in the dij terminology, d14 = d25 = d36. That is:

(6.46)

Further rotations of 120° about the three other triad axes leave this result unchanged. This result is also true for class 4¯3m: the effect of a shear stress s12 acting in the (001) plane of – a crystal such as sphalerite is to produce a polarization, P3, in the [001] direction by displacing tetrahedrally coordinated zinc ions relative to the centre of mass of the four surrounding sulphur ions (Problem 6.12). (By convention, the direction of polarization of a vector from the centre of the negative charge to the centre of the positive charge determines the sense of a dipole.) 6.4.4

Class 432

Here we have 90° symmetry operations to superimpose upon the ‘basic’ symmetry elements of Class 23. Consider the effect of a 90° anticlockwise symmetry operation about x3 on the surviving moduli of Class 23; that is, d123 = d213 = d312. The non-zero aij are a12 = 1,

Kelly_c06.indd 180

11/30/2011 7:08:11 PM

Strain, Stress, Piezoelectricity and Elasticity

181

a21 = −1 and a33 = 1. Hence, d213′ = a21a12a33d123 = −d123, d123′ = a12a21a33d213 = − d213 and d321′ = a33a21a12d312 = −d312. However, since we must also have d123 = d213 = d312, it follows that d123 = d213 = d312 = 0, and so for Class 432 all the piezoelectric moduli vanish. Thus, even though 432 is not centrosymmetric, crystals belonging to Class 432 are not piezoelectric. This is the only noncentrosymmetic class for which all the piezoelectric moduli vanish; the remaining 20 crystal classes have at least one nonvanishing piezoelectric modulus [1]. 6.4.5 The Converse Effect In the converse piezeoelectric effect, the relevant tensor equation is: ejk = dijkEi

(6.47)

where the dijk are the same as in Equation 6.36 [1]. When Equation 6.47 is expressed in the contracted form: ej = dijEi

(6.48)

the ejk transform as: ⎛ ε11 ⎜ ε12 ⎜⎝ ε 13

ε12 ε 22 ε 23

⎛ ε1 ε13 ⎞ ⎜ ε 23 ⎟ → ⎜ 1 ε 6 2 ⎜1 ε 33 ⎟⎠ ⎜⎝ ε 5 2

1ε 2 6 ε2

1ε 2 4

1ε ⎞ 2 5 1 ε ⎟⎟ 2 4 ⎟ ε 3 ⎟⎠

(6.49)

(Problem 6.13). Note that the contracted shear strains e4, e5 and e6 are engineering shear strains (g ), as defined in Section 6.2, and not tensor shear strains.

6.5

Elasticity of Crystals

In a strained crystal, the stress at any point is linearly related to the strain at that point, provided that the strain is very small. This relationship is known as Hooke’s law. The physical basis for Hooke’s law is merely that at small strains the relative displacements of the atoms are small, so that the interatomic force–separation relationship operates over such a small range as to be sensibly linear. In most solids, strains do in fact remain small (e.g. 2 / 3 that on the {110} planes, slip only on the [111] – (101) slip system would occur for all initial crystal orientations within this stereographic triangle [36,37]. From Table 7.1, it is worth noting that, in crystals of the NaCl structure slipping on – {110} k110l, at least two slip systems are always equally stressed. C.c.p. metal crystals have been very intensively studied. Even for crystals with the position of F near to the centre of the unit triangle, small amounts of glide on systems other than the most highly stressed one are observed. Since the slip plane of a glide system is easily observed, these slip systems are usually identified by reference to the glide plane alone. The slip plane of the most highly stressed system is called the primary glide plane; the names given to this and the others are shown in Figure 7.16.

Kelly_c07.indd 220

11/30/2011 8:24:53 AM

Glide and Texture

221

[0001]

I

I

[1100]

[1010]

[2110]

Figure 7.14 A unit triangle of the standard stereogram of a hexagonal crystal of point group – 6/mmm which glides on (0001) in k1120l, showing the slip direction of maximum resolved shear stress

111

[111] (211) [111] (101) [111] (112) 001

011

– Figure 7.15 The 001–011–111 stereographic triangle for a b.c.c. metal crystal which glides – – on {11 0} in k111l and on {112 } in k111l, showing the regions within this triangle where the resolved shear stresses on the various slip systems are greatest for a situation where the – – critically resolved shear stress is the same on the {11 0} and {112 } planes. The dashed line is – – the boundary between the two possible k111l {112} systems if slip did not occur on {110}

– In cubic crystals slipping on {111} k11 0l, a simple rule has been given by Diehl [40] to identify the primary glide system when the direction of F lies in any of the unit triangles shown in Figure 7.13. This states: ‘Reflect the k110l pole of the triangle in question in the opposite side of the triangle to find the glide direction, and reflect the {111} pole of the triangle in the opposite side to find the glide plane normal.’ An equivalent rule to this is the OILS rule devised by Hutchings [41] as a nongraphical method for deducing the slip

Kelly_c07.indd 221

11/30/2011 8:24:56 AM

222

Crystallography and Crystal Defects [101] (111) Critical

(111) Conjugate

F (001)

[011]

(111) Primary

(111) Cross

Figure 7.16

system with the highest Schmid factor. A mathematical proof of the validity of these two rules is given in Appendix 5.

7.5 Large Strains: The Change in the Orientation of the Lattice During Glide Returning to Figure 7.12, if a small amount of glide, dg, occurs on the slip system shown, the crystal will increase in length by dl in the direction of F where: dl = l cos φ 0 cos λ 0 dγ

(7.30)

where dg is the increment of crystallographic glide strain and l the instantaneous length of the crystal.2 If e is the (small) elongation parallel to F produced by dg then e = dl/l, and so Equation 7.30 gives: e = cos φ 0 cos λ 0 dγ

(7.31)

The relative translation of the parts of the crystal parallel to b implies that as the crystal gets longer its two ends move with respect to one another in a direction transverse to the applied force F. This effect is not important for very small strains, but when minerals are deformed large amounts in compression (usually under hydrostatic pressure), or metal crystals extended by large amounts in tension, it must be taken into account. In compression, the ends of the crystal may be prevented from moving sideways by friction, and in tension, crystals are usually gripped at the ends. Consider the tensile case, and suppose that there is no lateral constraint. The crystal will take up the form shown in Figure 7.17. If, however, due to the lateral constraints the point A′ is forced to lie above O at O′, then if there is glide solely on the system shown, the 2

The identity of the geometrical factors in Equations 7.28 and 7.30 is worth noting in passing. This arises because, of course, if a given applied force produces no resolved shear stress on a given glide system, because cos f0 or cos l0 is zero, then it does no work if that glide system operates. Certain orientations of an applied force F will give zero values for t in Equation 7.28 or for dl in Equation 7.30 if the crystal does not possess five independent slip systems.

Kelly_c07.indd 222

11/30/2011 8:24:56 AM

Glide and Texture

223

f

n

l

O′

b A′ l0

A l

n N

f0

l0

b O

Figure 7.17

crystal lattice will be rotated with respect to the direction OO′. From Figure 7.17 the elongation of the crystal e equals (l − l0)/l0, so from the triangle OAA′: sin λ 0 l =1+ e = l0 sin λ

(7.32)

l cos φ 0 = l0 cos φ

(7.33)

and from triangles NAO, NA′O:

where l0 and f0 are the initial values of l and f. The crystallographic glide strain g is given by AA′/(l0 cosf0 ) and AA′ = l cos l − l0 cos l0, so: γ =

Kelly_c07.indd 223

l cos λ − l0 cos λ 0 cos λ cos λ 0 = − l0 cos φ 0 cos φ cos φ 0

(7.34)

11/30/2011 8:24:59 AM

224

Crystallography and Crystal Defects

At a particular instance during glide, the resolved shear stress t [=(F/A) cos f cos l], where A is the cross-sectional area of the ellipse whose centre is A′, is: sin 2 λ 0 ⎞ F cos φ ⎛ 1− τ= ⎜ ⎟ A ⎝ (1 + e)2 ⎠

1/ 2

(7.35)

It can be seen from Figure 7.17 that the area of the glide plane remains constant during deformation (except for negligibly small changes due to the formation of slip steps). Therefore, the quantity A/cos f does not alter, and so Equation 7.35 can be written as: F cos φ 0 τ= A0

1/ 2

⎡ ⎛l ⎞2 ⎤ ⎢1 − ⎜ 0 ⎟ sin 2 λ 0 ⎥ ⎢⎣ ⎝ l ⎠ ⎥⎦

(7.36)

where A0 is the original cross-sectional area of the specimen prior to tensile testing. As deformation proceeds, the value of l decreases, and so for a given force F the resolved shear stress increases. We can also derive Equations 7.32–7.34 directly from Equation 7.7 and Figure 7.8. It is useful to do this because the vector formulae make the compression case easy to deal with. From Figure 7.8, a vector r is changed by glide of amount g to the vector r′, where: r ′ = r + γ (r ⋅ n ) β

(see Equation 7.7). We take r parallel to the tensile axis when g = 0, and then r′ represents the tensile axis after a crystallographic glide strain g : r′ l = (1 + e) = l0 r

(7.37)

The quantity n is a unit vector normal to the glide plane, so: cos φ =

l cos φ 0 (r ′ ⋅ n ) 1 = [(r ⋅ n) + γ (r ⋅ n)(β ⋅ n)] = 0 r′ r′ l

(7.38)

since cos f0 = (r ◊ n)/ uru and b ◊ n = 0. Thus we have Equation 7.33. Also: r ′ × β = r ′ sin λ

(7.39)

since b is a unit vector. From Equation 7.7: r′ × β = r × β,

since β × β = 0

(7.40)

and so: l sin λ 0 = l0 sin λ

Kelly_c07.indd 224

(7.41)

11/30/2011 8:25:03 AM

Glide and Texture (b)

225

[101] [111]

(a)

[101] 111

[112] 9

7

8 7 6 5

6 5 4 3 2 1 0

10

11 12

4 3 2 1

011 001

Al–Cu

[001]

Cu–Zn

[011]

Figure 7.18 Changes in orientation of c.c.p. metal crystals during glide. The numbers indicate successive determinations of the crystal orientation. ((a) is based on a diagram in Figure 6 of [42]; (b) is based on Figure 16 of [43], redrawn as Figure 69 of [44].)

which is Equation 7.32. Finally, if we form the dot product of both sides of Equation 7.7 with b, we obtain: l cos λ = l0 cos λ 0 + γ l0 cos φ 0

(7.42)

Thus, using Equation 7.33 we have: γ =

cos λ cos λ 0 − cos φ cos φ 0

which is Equation 7.34. When a long, thin crystal is used in an experiment, such as that illustrated in Figure 7.12, the change in orientation of the tensile axis with respect to the crystal axes (which is easier to consider than what is the same thing, the change of the crystal axes with respect to the tensile direction) can be measured and plotted on a stereogram. Since the change of orientation is such that the tensile axis rotates towards the slip direction, this can be used to determine the direction of glide. An actual example for a c.c.p. metal crystal is given in Figure 7.18a [42]. When the orientation of the tensile axis in Figure 7.18a reaches the great – circle joining the (0 01) and (1 11) poles, which is a mirror plane, the resolved shear stresses on two-slip systems are equal and slip might occur on both systems simultaneously. When two slip systems operate simultaneously, double slip or duplex slip is said to occur. In many cases in c.c.p. cubic metals, a crystal continues to slip on the primary system after the orientation has reached the mirror plane. In this case the orientation of the tensile axis ‘overshoots’ into the neighbouring unit triangle, so that slip is not proceeding on the nominally most highly stressed system. An example is shown in Figure 7.18b. After a certain

Kelly_c07.indd 225

11/30/2011 8:25:13 AM

226

Crystallography and Crystal Defects

amount of this additional primary slip the conjugate system suddenly operates and further slip occurs on this system, sometimes followed by ‘overshooting’ on the conjugate system, – as in Figure 7.18b. When the tensile axis reaches a k112l pole – [112] in the example shown – in Figure 7.18b, the vector sum of the two slip directions [101] and [011] – no further orientation change should occur, provided each slip system contributes equally to the deformation. There is also a change of orientation of the lattice of a crystal during a compression test. To deal with this case it is simplest to use vector formulae. We first use Equation 7.7 to find how a given plane of normal m is altered by glide. Let r1, r2 be any two nonparallel unit vectors in the given plane. Write m = r1 × r2. Now transform each of r1 and r2 according to Equation 7.7 to give r′1 and r′2. Then the new vector m′ representing m after a crystallographic glide strain of amount g is: m ′ = r1′ × r2′

(7.43)

Substituting for r′1 and r′2 from Equation 7.7, we have: m ′ = [r1 × r2 ] + γ (r1 ⋅ n)β × r2 − γ (r2 ⋅ n)β × r1 = m + γ β × [(r1 ⋅ n)r2 − (r2 ⋅ n)r1 ] (7.44) Using the formula for the vector triple product (Appendix 1), this is seen to be: m ′ = m + γ β × n × [r2 × r1 ]

(7.45)

m ′ = m − γ β × [n × m]

(7.46)

That is:

and again using the formula for the vector triple product: m′ = m − γ (( β ⋅ m)n − ( β ⋅ n)m)

(7.47)

m ′ = m − γ (β ⋅ m)n

(7.48)

or:

since (b ◊ n) = 0. It is evident from Equations 7.46 and 7.48 that any plane moves to its final position in such a way that its normal always lies in the plane containing the initial position of the normal and n, the normal to the glide plane. If we now consider the case of compression of a thin crystal between flat plates, as in Figure 7.19, we take the constraint to be that the plane initially normal to the stress axis must be maintained in this orientation with respect to the stress axis as the crystal deforms. To maintain positive values of g during compression, we suppose slip to occur so that (b ◊ m) is negative (Figure 7.19). Equation 7.48 then reads: m′ = m + γ ( β ⋅ m)n

(7.49)

From Equation 7.49, the normal to the glide plane then approaches the normal to the compression plates by rotating about an axis which is parallel to the line of intersection of the

Kelly_c07.indd 226

11/30/2011 8:25:15 AM

Glide and Texture F

(a)

F

(b) n

m m′

n b

227

h0

h

n

n b

F

Figure 7.19

F

Compression of a single crystal between plates

glide plane and the compression plates (Figure 7.19b). The initial thickness of the crystal is h0, which will be reduced during compression to a height h such that: h0 m′ = h m

(7.50)

because the volume of the crystal must be conserved. With the constraint that we have assumed, the change of orientation of the crystal lattice will be such that the normal to the slip plane rotates towards the axis of compression. If the initial and final angles, after a shear strain g, between the direction of compression and the normal to the slip plane are f0, f, and l and l0 are the corresponding obtuse values of the angle between the compression axis and the slip direction, then we have, from Equation 7.49: m′ ⋅ β = m ⋅ β

(7.51)

since: n⋅β = 0 Therefore: h0 cos λ 0 = h cos λ

(7.52)

m′ × n = m × n

(7.53)

h0 sin φ 0 = h sin φ

(7.54)

and also, from Equation 7.49:

Thus:

Kelly_c07.indd 227

11/30/2011 8:25:24 AM

228

Crystallography and Crystal Defects

Finding the modulus of each side of Equation 7.49, we have: 2

2

2

2

m ′ = m + 2γ m cos φ 0 cos λ 0 + γ 2 m cos2 λ 0

(7.55)

and using Equation 7.50: 2

⎛ h0 ⎞ 2 2 ⎜⎝ h ⎟⎠ = 1 + 2γ cos φ 0 cos λ 0 + γ cos λ 0

(7.56)

Since l0 is obtuse, because we have specified that (b ◊ m) is negative, it is apparent from this equation that h0 < h. Forming m′ ◊ n = m ◊ n + g (b ◊ m) and using Equations 7.50 and 7.52: γ =

cos φ cos φ 0 − cos λ cos λ 0

(7.57)

The resolved shear stress t is given by: 1/ 2

⎡ ⎛ h ⎞2 ⎤ F F⎛ h⎞ τ = cos φ cos λ = ⎜ ⎟ cos λ 0 ⎢1 − ⎜ ⎟ sin 2 φ 0 ⎥ A A ⎝ h0 ⎠ ⎢ ⎝ h0 ⎠ ⎥ ⎣ ⎦

(7.58)

Since A0h0 = Ah, Equation 7.58 may be written as: 1/ 2

2 ⎡ ⎛ h ⎞2 ⎤ F ⎛ h⎞ ⎢ τ= cos λ sin 2 φ 0 ⎥ 0 1− ⎜ ⎜ ⎟ ⎟ A0 ⎝ h0 ⎠ ⎢ ⎝ h0 ⎠ ⎥ ⎣ ⎦

(7.59)

In compression, the normal to the glide plane approaches the direction of compression, so that, for example, in Figure 7.13, F0 would approach the (111) pole until it meets the boundary between [001] and [011]; thereafter, systems B IV and A III would be equally stressed and the stable orientation of the normal to the glide plane would be (011), the plane midway between A and B lying in the same zone as A and B. Formulae for the change in orientation of the crystal lattice with respect to the direction of an applied force have been given for duplex slip in both compression and tension by Bowen and Christian [45]. During double glide there is a change in orientation of the lattice of the crystal with respect to the direction of a tensile force until the applied force is symmetrically related to the two slip systems. Thus, as we have seen, in tension of c.c.p. metals, k112l directions represent stable orientations lying midway between two k110l directions.

7.6 Texture Because large strains can cause a reorientation of the lattice of a crystal, it follows that, in a polycrystalline material, continued plastic flow, such as that which occurs during the working of metals, tends to develop a texture or a preferred orientation of the lattice within

Kelly_c07.indd 228

11/30/2011 8:25:32 AM

Glide and Texture

229

the grains, as well as a preferred change of shape of the grains. Working involves very large plastic strains, often hundreds of per cent. The development of a texture changes the crystallographic properties of the material significantly. A fine-grained material in which the grains have random lattice orientations will have isotropic properties, provided that other crystal defects such as inclusions and boundaries are uniformly distributed. However, a specimen with a preferred orientation will have anisotropic properties, which may be desirable or undesirable, depending upon the intended use of the material. The final texture that develops may resemble a single orientation or may comprise crystals distributed between two or more preferred orientations. During plastic flow the process of reorientation is gradual. In theory, the orientation change proceeds until a texture is reached that is stable against indefinitely continued flow of a given type. The theoretical end distribution of orientations and the manner in which it develops are a characteristic of the material, its crystal structure, its microstructure and the nature of the forces arising from the deformation process. Whether a material actually reaches its stable orientation depends upon many variables, such as the rate of working and the temperature at which it is carried out. Textural changes may correspond with marked changes in the ductility of a material. Thus there is an interplay between the role of deformation in creating texture and the role of texture in facilitating deformation. While the basic principles underlying texture development for single crystals have been presented in Section 7.4, the prediction of actual textures during forming processes is necessarily very complicated [46–48]. The various processes of texture development have been categorized according to their final state and to the kind of working involved, for example wire and fibre textures, compression textures, sheet and rolling textures, torsion textures and deep drawing textures. Some examples of ideal end textures are presented in Table 7.5. In addition to deformation textures, anisotropic properties of a polycrystalline material can also arise as a result of recrystallization following working (see Chapter 11, Footnote 1) or as a result of material fabrication processes that do not involve plastic deformation. For example, the vapour deposition of layers on substrates often results in a layer having a polycrystalline texture with a preferred orientation in the growth direction and random orientations perpendicular to the growth direction. Some examples of deposition textures are included in Table 7.5. There is usually a statistical distribution of orientations of the various crystals in a sample. This distribution can be measured and represented on a pole figure, such as in Figure 7.20. A pole figure is similar to a stereographic projection. On it is presented the statistical distribution of the orientations of the plane normals from a particular set of planes. A pole figure is usually obtained using diffraction from X-rays, neutrons or electrons.3 In the typical case of X-ray diffraction in the laboratory, the detector position is fixed to collect the diffraction from one particular set of planes. The sample is rotated about two axes so as to scan over all possible orientations. The corresponding pole figure is usually presented as a contour map, where the contours are labelled according to the relative strength of the diffraction signal. For example, Figure 7.20 is a pole figure showing the relative intensities of the reflections from {111} planes in a cold-rolled copper sample. The relative populations of planes in the various 3

For X-ray and neutron diffraction, the experiment obtains an average texture over volumes of the order of cubic millimetres. Using electron diffraction, textures from different regions of the sample can be discriminated, giving rise to the terms microtexture and mesotexture used in the study of textural variations within a sample.

Kelly_c07.indd 229

11/30/2011 8:25:38 AM

Kelly_c07.indd 230

11/30/2011 8:25:38 AM

b.c.c.

Rolling texture {plane}/kaxisl

c.c.p.

Rolling texture {plane}/kaxisl Tension (fibre) texture kaxisl

Deposition texture kgrowth directionl

Compression texture kaxisl

Tension (fibre) texture kaxisl

Description

Crystal structure

Fe single crystal and polycrystalline Mo, Nb, Ta, V, W, ferrosilicon, b-brass

– Between {001} k110l and {112} k11 0l; – {111} k112l k110l

k111l

Range from k110l to k311l; some k111l

k211l k111l Range from k110l to k311l

Some single crystals Single crystal and polycrystalline Al α-brass (70Cu / 30Zn) Au on cleaved NaCl by thermal evaporation

k111l and k100l

– {110} k112l and {110} k001l

– {111} k112l {001} k110l – – {110} k11 2l – and {112} k111 – l {123} k412l + {146} k211 l

– – {110} k11 2l then {112} k111 l

Texture

Al, Cu, Au, Ag, Ni

α-brass (70Cu / 30Zn)

Cu

Al single crystals

Al

Example material

Some common end or final textures

Table 7.5

Often both components together Occasionally

Random orientation in the plane of growth

Known as ‘pure metal’ texture at high temperatures and large deformations Up to 90% reduction After 90% reduction Orientations between these extremes or spread around these ideal end textures Known as ‘alloy’ or ‘brass’ texture; changes to ‘pure metal’ texture at high temperatures Relative proportions dependent upon temperature, strain rate, percentage reduction, stacking fault energy and twinning Except for starting orientation k111l For starting orientation k111l Tendency to rotate away from k111l and k100l Tendency to rotate away from k100l

Comments

[50]

[49]

[52]

[51]

[50] [51] [50]

[51]

[49]

[49]

[50]

[49]

Ref.

Kelly_c07.indd 231

11/30/2011 8:25:38 AM

h.c.p.

Compression texture kaxisl Deposition texture kgrowth directionl

Tension (fibre) texture kaxisl

Rolling texture {plane}/kaxisl

Compression texture kaxisl Deposition texture kgrowth directonl

Ti on oxidized Si (001) by magnetron sputtering

Zr, Ti Mg

Zn

Mg

[55]

Random in-plane orientation

k0001l

[51] [51] [51]

High temperatures Small reductions Large reductions

[51]

– k2110l k0001l 70°–from k0001l spiral texture k1010l k0001l

– k1010l

[51] [51]

Zn, Cd Zr, Ti

Deviation is in the transverse sense, i.e. about the rolling direction Low temperatures

[51]

– 20–25° off {0001} k112 –0l 30–40° off {0001} k1010l

Low growth rates and low substrate temperatures Some in-plane texture in both cases

k110l – {0001} k1120l

[53,54]

High growth rates

k111l

Mo on (001) Si by magnetron sputtering

Mg

[50]

k111l, some k100l

Fe

232

Crystallography and Crystal Defects RD

0.5 1 2 3 4 5 8 12 0.5 1

2 3 5 8 12 15

0.5

1 2 3

CD 4 5

Near (123) [412] Near (146) [211] (110) [112] (112) [111] (110) [001]

Figure 7.20 The {111} pole figure of electrolytic copper rolled to 96.6% reduction at room temperature, where RD is the rolling direction and CD is the cross direction. The numbers represent relative intensities of the diffraction signal [56]

orientations are proportional to the numbers against the contour lines. The pole figure is interpreted in terms of an ideal end orientation. In uniaxial textures, such as those obtained in tension, compression and wire- and rod-forming processes, it is often sufficient to specify which crystallographic direction (or directions) lies parallel to the unique axis. For sheet textures, ideal orientations are given by a plane or planes lying parallel to the plane of the sheet and a direction or directions in the plane lying parallel to a significant direction in the sheet, such as the rolling direction (RD). For example, to identify {110} – k001l and {110} k11 2l textures the procedures illustrated in Figure 7.21 might be followed. First, identify the orientations of the {111} poles relative to the {110} plane and the k001l and k112l directions. A stereographic projection is shown in Figure 7.21a with the (110) plane normal perpendicular to the plane of the paper. All of the {111} poles are shown, along with those k001l and k112l directions that are in the (110) plane and thus could lie parallel to the RD. The orientations of the {111} poles when the RD corresponds to k001l and k112l

Kelly_c07.indd 232

11/30/2011 8:25:38 AM

Glide and Texture (b) (a)

233

Rolling direction

001 112

112

111

111 111 110 111

111

111 112

112 001

(c)

(d) Rolling direction

Rolling direction +

Figure 7.21 (a) Standard stereographic projection in the (110) orientation showing the poles for the {001}, {112} and {111} plane normals. Orientations of the {111} plane normals for – (b) the (110)k001l rolling texture, (c) the (110)k11 2l rolling texture and (d) a combination of (b) and (c)

are shown in Figures 7.21b and c, respectively. Note that there are two possible k112l orientations, which results in there being 12 {111} pole positions. The case where the end texture – contains both {110} k001l and {110} k11 2l orientations is illustrated in Figure 7.21d. A pole figure from an ideal end texture will have the appearance of a pole plot from one or a few single crystals, depending upon how many orientations comprise the end texture. A real textured material will show a broader distribution of intensities about the ideal orientation. How close the actual texture is to the ideal texture is a qualitative judgement. Actual textures are described as varying from ‘weak’ (a small proportion of grains having

Kelly_c07.indd 233

11/30/2011 8:25:38 AM

234

Crystallography and Crystal Defects f1 F

45º f2

90º

90º

– 45º

Figure 7.22 Spatial representation of the half-maximum density of the ODF relevant for both heavily cold-rolled heavily rolled a-brass and heavily rolled silver [46,47,57] ND F [001]

[100] Nodal direction

f2

RD f1 [010]

Figure 7.23 Definition of the orientation of a crystallite in rolled sheet by means of three Euler angles, f1, F and f2 (after [47]). The nodal direction is parallel to the vector product of ND and the crystallite [001] direction. RD is the rolling direction and ND is the sheet normal

rotated to the endpoint) to ‘strong’ (a large volume fraction of grains having rotated to or close to the endpoint). A more computationally intensive, but more representative, measure of texture is in the orientation distribution function (ODF). Using data from pole figures taken for several reflections, the orientations of three primary axes of the crystallites are plotted with respect to three standard axes. ODFs can be displayed as three-dimensional plots or as a series of two-dimensional sections. An ODF relevant for both heavily rolled α-brass and heavily rolled silver is shown in Figure 7.22, where f1, F and f2 are the angles between principal directions in the crystallites and significant directions in the forming process and are known as the Euler angles. In this diagram the surface shown represents the half-maximum density – of the orientation distribution corresponding to a [011](211) texture.

Kelly_c07.indd 234

11/30/2011 8:25:38 AM

Glide and Texture

235

Typical Euler angles for rolled sheet are illustrated in Figure 7.23; F is the angle between the crystallite [001] direction and the sheet normal (ND), f2 is the angle between the crystallite [100] direction and the nodal direction, and f1 is the angle between the nodal direction and RD. The nodal direction lies perpendicular to ND and the crystallite [001] direction and is parallel to the direction defined by the vector product of these two directions. We see in Figure 7.22 that the spread in f1 is about 10º, the spread in F is about 10º and the spread in f2 is about 20º, indicating a pronounced texture with only a small spread in orientation. Using the mathematical analysis of the ODF, a near-quantitative description of texture is possible.

Problems – 7.1 a-ZnS has the point group 4 3m. (a) Does it possess a centre of symmetry? Assume that the slip planes are {111} and – the slip directions k110l. – – (b) Is slip in the [11 0] direction crystallographically equivalent to that in [110]? 7.2 During the process of glide the displacements imposed upon the surfaces of a crystal are centrosymmetric. Use this notion and Figure 7.5 to deduce the rules (1)–(4) given in Section 7.2. 7.3 Enumerate the number of physically distinct glide systems for a cubic crystal (e.g. a – – c.c.p. metal) of point group m3m which slips on {111} in k110l directions. Along which directions should such a crystal be stressed in uniaxial tension if the resolved shear stress is to be the same on (a) eight systems, (b) six systems and (c) four systems? Show that for a given tensile axis [uvw], the Schmid factor cos f cos l for the slip system which operates must satisfy the condition: 2 3 3

≤ cos φ cos λ ≤ 0.5

Hence or otherwise, determine the individual values of f and l when cos f cos l = 0.5. 7.4 Establish the number of independent slip systems possessed by CsBr, which is cubic – (Pm3m) and slips on {110} in k001l. How many independent systems does such a crystal possess if pencil glide occurs with the same glide directions? – 7.5 Consider an amount of glide g to occur on the (011) plane in the [011 ] direction of a cubic crystal. Take axes parallel to the cubic axes. (a) Write down the components of the pure strain tensor. (b) Write down the components of the pure strain tensor if glide of amount g ′ occurs – on (100) in the same direction, [011], as before. (c) How many components of the pure strain tensor can be altered independently of one another by glide on these two systems? (d) If g ′ was always equal to a constant fraction of g so that g ′ = kg, what would be the answer to (c)?

Kelly_c07.indd 235

11/30/2011 8:25:39 AM

236

Crystallography and Crystal Defects

(e) Use the above results to prove generally that if pencil glide occurs in a crystal then slip with a given slip direction can provide two independent components of the pure strain tensor. 7.6 Can you think of three slip directions which operating together would provide a contradiction of the statement, ‘When pencil glide occurs a crystal need only possess in general three noncoplanar slip directions in order for a general strain to be possible’? – – 7.7 Copper is cubic (Fm3m) and slips on {111} k11 0l. Sketch a stereogram of a crystal showing the components of the slip systems. Which slip system(s) are expected to operate if the tensile axis is (a) [123], (b) [113] and (c) [122]? – – 7.8 Rock salt is cubic (Fm3m) and slips on {110} k11 0l. Sketch a stereogram showing the components of the slip systems. Which slip system(s) are expected to operate if the tensile axis is (a) [123], (b) [213] and (c) [013]? – 7.9 Magnesium oxide is cubic with the NaCl structure and slips on {110} in k11 0l. (a) List the directions along which a tensile or compressive force applied to the crystal cannot produce glide. (b) Can the crystal be twisted plastically about [100]? (c) List the same directions as in (a) for graphite. (The glide elements for graphite are listed in Table 7.1.) 7.10 The analysis of strain in Chapter 6 requires that the strain be infinitesimal. Explain why this restriction does not invalidate the analysis of Section 7.3 (which shows that five independent glide systems are necessary for a general deformation) because, when glide takes place, large strains occur in some volumes of the crystal. 7.11 A tetragonal crystal is subject to a tensile stress of magnitude s along [100] and to a shear stress t on (100) in [010]. (a) Write down the components of the stress tensor referred to the crystal axes. – (b) Find the shear stress on (110) in the [11 0] direction by altering the axes of reference of the stress tensor. (c) Find, by the same procedure, the tensile stress normal to (110). 7.12 Prove Equation 7.30. –

7.13 A single crystal of zinc which slips on (0001) in k1120l directions is stressed in tension and is oriented so that the tensile axis makes an angle of 45° with [112ˉ0] and is at 60° to the normal to (0001). (a) Along which direction will slip first occur? (b) If slip starts when the tensile stress on the crystal is 2.1 MPa, calculate the critical resolved shear stress necessary to produce slip in zinc. – 7.14 Copper slips on {111} in k11 0l. A cylindrical single crystal 10 cm long is stressed in – tension. The tensile axis is [123]. (a) Which is the slip system with the highest resolved shear stress? The specimen is strained in tension until the tensile axis reaches a symmetry position where two slip systems have equal resolved shear stresses.

Kelly_c07.indd 236

11/30/2011 8:25:40 AM

Glide and Texture

237

(b) Which are the two systems? (c) What is the orientation of the tensile axis at this stage? (d) What is the new length of the specimen? 7.15 Discuss the following statement. ‘A general small homogeneous change of shape of a body can be described by a pure strain and a rotation. If the volume of the body is conserved the pure strain tensor has five independent components and the pure rotation tensor has three. Therefore, eight quantities must be specified to describe the change of shape of a single crystal within a polycrystalline body. It follows from this that eight slip systems must in general operate in all grains of a polycrystal which is subject to a general change of shape.’

Suggestions for Further Reading H.-J. Bunge (1982) Texture Analysis in Materials Science, Mathematical Methods, Butterworths, London. G.Y. Chin, R.N. Thurston and E.A. Nesbitt (1966) Finite plastic deformation due to crystallographic slip, Trans. Am. Inst. Min. Metall. Petrol. Engrs, 236, 69–76. G.E. Dieter (1988) Mechanical Metallurgy (SI metric edition adapted by D.J. Bacon), McGraw-Hill, London. G.W. Groves and A. Kelly (1963) Independent slip systems in crystals, Phil. Mag., 8, 877–887. W.J. McGregor Tegart (1966) Elements of Mechanical Metallurgy, Macmillan, New York. E. Schmid and W. Boas (1950) Plasticity of Crystals, F.A. Hughes and Co. Ltd, London.

References [1] E. Reusch (1867) Ueber eine besondere Gattung von Durchgängen im Steinsalz und Kalkspath, Poggendorff’s Annalen der Physik und Chemie, 132, 441–451. [2] J.A. Ewing and W. Rosenhain (1899) Experiments in micro-metallurgy:— Effects of Strain. Preliminary notice, Proc. Roy. Soc. Lond. A, 65, 85–90. [3] J.A. Ewing and W. Rosenhain (1900) The crystalline structure of metals, Phil. Trans. Roy. Soc. Lond. A, 193, 353–375. [4] G.W. Groves and A. Kelly (1963) Independent slip systems in crystals, Phil. Mag., 8, 877–887. [5] J.P. Hirth and J. Lothe (1982) Theory of Dislocations, 2nd Edition, John Wiley and Sons, New York. [6] F.R.N. Nabarro (1987) Theory of Crystal Dislocations, Dover Publications, New York. [7] D.J. Bacon and V. Vitek (2002) Atomic scale modelling of dislocations and related properties in the hexagonal-close-packed metals, Metall. Mater. Trans A, 33, 721–733. [8] A. Kelly and D.J. Rowcliffe (1966) Slip in titanium carbide, Phys. Stat. Sol., 14, K29–K33. [9] B.L. Eyre and A.F. Bartlett (1966) Determination of the Burgers vector of dislocations in deformed uranium carbide, Phil. Mag., 13, 641–643. [10] W. Skrotzki, R. Tamm, C.-G. Oertel, J. Röseberg and H.-G. Brokmeier (2000) Microstructure and texture formation in extruded lead sulfide (galena), J. Struct. Geol., 22, 1621–1632. [11] W.A. Rachinger (1956) Glide in lead telluride, Acta Metall., 4, 647–649. [12] J.F. Byron (1968) The yield and flow of single crystals of uranium oxide, J. Nucl. Mater., 28, 110–114. [13] T.E. Mitchell (1979) Application of transmission electron microscopy to the study of deformation in ceramic oxides, J. Am. Ceram. Soc., 62, 254–267. [14] T.E. Mitchell (1999) Dislocations and mechanical properties of MgO–Al2O3 single crystals, J. Am. Ceram. Soc., 82, 3305–3316. [15] K.-H. Yang, N.-J. Ho and H.-Y. Lu (1999) Deformation microstructure in (001) single crystal strontium titanate by Vickers indentation, J. Am. Ceram. Soc., 92, 2345–2353.

Kelly_c07.indd 237

11/30/2011 8:25:40 AM

238

Crystallography and Crystal Defects

[16] C. Levade, J.-J. Couderc, I. Dudouit and J. Garigue (1986) The plastic behaviour of natural sphalerite crystals between 473 and 873 K, Phil. Mag. A, 54, 259–279. [17] B. Kedjar, L. Thilly, J.-L. Demenet and J. Rabier (2010) Plasticity of indium antimonide between −176 °C and 400 °C under hydrostatic pressure. Part II: Microscopic aspects of the deformation, Acta Mater., 58, 1426–1440. [18] Y. Androussi, G. Vanderschaeve and A. Lefebvre (1989) Slip and twinning in high-stressdeformed GaAs and the influence of doping, Phil. Mag. A, 59, 1189–1204. [19] S. Amelinckx and P. Delavignette (1960) Electron optical study of basal dislocations in graphite, J. Appl. Phys., 31, 2126–2135. [20] F. Yang and J.C.M. Li (2007) Deformation behavior of tin and some tin alloys, J. Mater. Sci.: Mater. Electron., 18, 191–210. [21] K.H.G. Ashbee and R.E. Smallman (1963) The plastic deformation of titanium dioxide single crystals, Proc. Roy. Soc. Lond. A, 274, 195–205. [22] K. Suzuki, M. Ichihara and S. Takeuchi (1991) High-resolution electron microscopy of lattice defects in TiO2 and SnO2, Phil. Mag. A, 63, 657–665. [23] M. Georgieff and E. Schmid (1926) Über die Festigkeit und Plastizität von Wismutkristallen, Z. Phys., 36, 759–774. [24] R.E. Slonaker, M. Smutz, H. Jensen and E.H. Olson (1965) Factors affecting the growth and the mechanical and physical properties of bismuth single crystals, J. Less-Common Metals, 8, 327– 338. [25] C. Steegmuller and J.S. Daniel (1972) Slip in bismuth, J. Less-Common Metals, 27, 81–85. [26] J.G. Rider and F. Heckscher (1966) Slip in single crystals of mercury, Phil. Mag., 13, 687–692. [27] J.D. Snow and A.H. Heuer (1973) Slip systems in Al2O3, J. Am. Ceram. Soc., 56, 153–157. [28] R.J. Stokes, T.L. Johnston and C.H. Li (1961) Mechanical properties of tellurium single crystals, Acta Metall., 9, 415–427. [29] F.J. Spooner and C.G. Wilson (1966) Slip and twinning in gallium, J. Less-Common Metals, 10, 169–184. [30] J.S. Daniel, B. Lesage and P. Lacombe (1971) The influence of temperature on slip and twinning in uranium, Acta Metall., 19, 163–173. [31] V. Vitek (1992) Structure of dislocation cores in metallic materials and its impact on their plastic behaviour, Prog. Mater. Sci., 36, 1–27. [32] W.G. Tyson (1969) Slip modes of thallium, Acta Metall., 17, 863–868. [33] T.G. Carnahan and T.E. Scott (1973) Deformation modes of hcp yttrium at 77, 298, and 497 K, Metall. Trans., 4, 27–32. [34] R.E. von Mises (1928) Mechanik der plastischen Formänderung von Kristallen, Zeitschrift für Angewandte Mathematik und Mechanik, 8, 161–185. [35] E. Schmid (1925) Neuere Untersuchungen an Metallkristallen, Proc. 1st. International Congress for Applied Mechanics, Delft, 1924 (edited by C.B. Biezeno and J.M. Burgers), Technische Boekhandel en Drukkerij J. Waltman, Jr., Delft, pp. 342–353. [36] G.Y. Chin (1972) Competition among {110}, {112} and {123} slip modes in bcc metals, Metall. Trans., 3, 2213–2216. [37] B. Orlans-Joliet, B. Bacroix, F. Montheillet, J.H. Driver and J.J. Jonas (1988) Yield surfaces of b.c.c. crystals for slip on the {110} and {112} systems, Acta Metall., 36, 1365– 1380. [38] E. Schmid and W. Boas (1950) Plasticity of Crystals, F.A. Hughes and Co. Ltd, London. [Originally published as Kristallplastizität mit besonderer Berücksichtigung der Metalle, Julius Springer, Berlin in 1935.] [39] G.I. Taylor and C.F. Elam (1925) The plastic extension and fracture of aluminium crystals, Proc. Roy. Soc. Lond. A, 108, 28–51. [40] J. Diehl, personal communication to A. Seeger, acknowledged on p. 24 of A. Seeger (1958) Kristallplastizität, Handbuch der Physik, Band VII.2: Kristallphysik II (edited by S. Flügge), Springer-Verlag, Berlin, pp. 1–210. [41] I.M. Hutchings (1993) Quick non-graphical method for deducing slip systems in cubic close packed metals in tension or compression, Mater. Sci. Tech., 9, 929–930.

Kelly_c07.indd 238

11/30/2011 8:25:40 AM

Glide and Texture

239

[42] R.J. Price and A. Kelly (1964) Deformation of age-hardened aluminium alloy crystals–I. Plastic flow, Acta Metall., 12, 159–169. [43] Freiherr von Göler and G. Sachs (1929) Zugversuche an Kristallen aus Kupfer und α-Messing, Z. Phys., 55, 581–620. [44] A. Seeger (1958) Kristallplastizität, Handbuch der Physik, Band VII.2: Kristallphysik II (edited by S. Flügge), Springer-Verlag, Berlin pp. 1–210. [45] D.K. Bowen and J.W. Christian (1965) The calculation of shear stress and shear strain for double glide in tension and compression, Phil. Mag., 12, 369–378. [46] H.-J. Bunge (1982) Texture Analysis in Materials Science, Mathematical Methods, Butterworths, London. [47] R.W. Cahn (1991) Measurement and control of texture, in Volume 15, Materials Science and Technology (series editors R.W. Cahn, P. Haasen and E.J. Kramer), Processing of Metals and Alloys (edited by R.W. Cahn), Wiley–VCH, Chichester and Weinheim, Chapter 10: pp. 429–480. [48] U.F. Kocks, C.N Tomé and H.-R. Wenk (1998) Texture and Anisotropy: Preferred Orientations in Polycrystals and their Effect on Materials Properties, Cambridge University Press, Cambridge. [49] I.L. Dillamore and W.T. Roberts (1965) Preferred orientation in wrought and annealed metals, Metall. Rev., 10, 271–380. [50] H. Hu, R.S. Cline and S.R. Goodman (1965) Deformation textures in metals, in Recrystallization, Grain Growth and Textures, American Society for Metals, Metals Park, OH, pp. 295–367. [51] C.S. Barrett and T.B. Massalski (1980) Structure of Metals: Crystallographic Methods, Principles and Data, Pergamon, Oxford, pp. 541–583. [52] K.E. Harris and A.H. King (1994) Localized texture formation and its detection in polycrystalline thin films of gold, in Mechanisms of Thin Film Evolution, Volume 317 (editors S.M. Yalisove, C.V. Thompson and D.J. Eaglesham), Materials Research Society, Pennsylvania, pp. 425–430. [53] M. Vill, S.G. Malhotra, Z. Rek, S.M. Yalisove and J.C. Bilello (1994) White-beam transmission characterization of texture in Mo thin films and Mo/W multilayers, in Mechanisms of Thin Film Evolution, Volume 317 (editors S.M. Yalisove, C.V. Thompson and D.J. Eaglesham), Materials Research Society, Pennsylvania, pp. 413–418. [54] O.P. Karpenko, M. Vill, S.G. Malhotra, J.C. Bilello and S.M. Yalisove (1994) Texture in sputtered Mo films, in Mechanisms of Thin Film Evolution, Volume 317 (editors S.M. Yalisove, C.V. Thompson and D.J. Eaglesham), Materials Research Society, Pennsylvania, pp. 467–472. [55] R. Ahuja and H.L. Fraser (1994) Structural transitions in titanium-aluminum thin film multilayers, Mechanisms of Thin Film Evolution, Volume 317 (editors S.M. Yalisove, C.V. Thompson and D.J. Eaglesham), Materials Research Society, Pennsylvania, pp. 479–484. [56] H. Hu and S.R. Goodman (1963) Texture transition in copper, Trans. Met. Soc. AIME, 227, 627–639. [57] H. J. Bunge (1987) Three-dimensional texture analysis, Int. Mater. Rev., 32, 265–291.

Kelly_c07.indd 239

11/30/2011 8:25:40 AM

8 Dislocations 8.1

Introduction

In Chapter 7 the geometry of glide was studied on a macroscopic scale. The geometrical results on this scale are adequately described by the model of blocks of crystal sliding over one another rigidly. However, when glide occurs in a real crystal, all the atoms above the slip plane do not move simultaneously over those below. At any given time some of the atoms have moved into their new positions while others have not yet done so, and the displacement of the upper block of crystal relative to the lower varies from one region of the slip plane to another. Lines in the slip plane separating regions where slip has occurred from those where it has not are called dislocations. This is the simplest way in which to introduce the idea of dislocations; we shall see later that they can be formed in other ways. For ease of illustration and simplicity we will consider slip in a crystal with the primitive cubic lattice and one atom associated with each lattice point. A block of such a crystal cut with faces parallel to {100} planes is shown in Figure 8.1. A (001) slip plane, PQRT, is shown, and slip in the [010] direction has occurred over only the region PQSS′. It is evident that the crystal lattice is distorted, especially close to the dislocation which lies along SS′. The distortion decreases as the amount of slip over PQSS′ is reduced. In Figure 8.1 the displacement over PQSS′ is equal to [010],1 which is the smallest displacement that can be made without producing a fault in the crystal structure at the plane PQSS′. The displacement is a constant vector quantity over the whole region PQSS′ (except within a few atoms of the dislocation line SS′), and it is this quantity that characterizes the dislocation. As a dislocation moves through the crystal, the displacement associated with it does not change. This characteristic quantity is called the Burgers vector of the dislocation.

1 A specific displacement is written in terms of its components along the crystal axes (Section 1.2). In cubic crystals the lattice parameter a is often included in the notation, although it is superfluous.

Crystallography and Crystal Defects, Second Edition. Anthony Kelly and Kevin M. Knowles. © 2012 John Wiley & Sons, Ltd. Published 2012 by John Wiley & Sons, Ltd.

Kelly_c08.indd 241

11/30/2011 8:49:27 AM

242

Crystallography and Crystal Defects

T S′

P

R S

Q

[001] [010] [100]

Figure 8.1 A screw dislocation in a primitive cubic lattice

T

R P

Q

Figure 8.2

As the dislocation SS′ in Figure 8.1 moves from right to left, the slipped region of the crystal increases. When the dislocation reaches the surface at RT, the whole crystal has been slipped by [010], as shown in Figure 8.2. A dislocation may turn into a new orientation; this does not change its Burgers vector. The result of rotating SS′ in the slip plane through a right angle is shown in Figure 8.3. The dislocation which results, EE′, has the same [010] displacement vector associated with it, the crystal now having slipped by this amount over

Kelly_c08.indd 242

11/30/2011 8:49:27 AM

Dislocations

243

T

E R

P

E′ Q

Figure 8.3 An edge dislocation in a primitive cubic lattice

T

P R D

D′ Q

Figure 8.4 A mixed dislocation, DD′, in a primitive cubic lattice

QREE′ and not having slipped over PTEE′. A length of dislocation which lies normal to its Burgers vector, such as EE′, is called an edge dislocation; one like SS′ which lies parallel to its Burgers vector is called a screw dislocation. In general, a dislocation may lie at any angle to its Burgers vector or may be curved like the dislocation DD′ in Figure 8.4. At D′ the dislocation is in edge orientation and at D in screw orientation. Elsewhere the dislocation has both edge and screw components and is referred to as mixed. The reason for the names ‘edge’ and ‘screw’ becomes clear when we look at the positions of the atoms around the dislocation. The positions close to the dislocation cannot be calculated exactly without a detailed knowledge of the laws of force between the atoms,

Kelly_c08.indd 243

11/30/2011 8:49:28 AM

244

Crystallography and Crystal Defects K

E

Figure 8.5 Atom positions around an edge dislocation (according to Equation 8.21) (a) q 4

3

S1

S

S2

x1

1

2

(b)

S1′ 4 3 2 1 4 3 2 1 S1

Figure 8.6 Screw dislocation in a simple cubic crystal (a) looking along the dislocation and (b) looking normal to the dislocation which lies along S1S1′

although in some cases they can be observed at the surface of a crystal at atomic resolution with scanning tunnelling microscopes and atom probes, and within thin crystals using high-resolution transmission electron microscopy. For the present, it is enough to recognize that there is a small amount of arbitrariness in the location of the atoms shown in Figures 8.5 and 8.6. The arrangement of atoms in a plane normal to the edge dislocation EE′ of Figure 8.3 is shown in Figure 8.5. There is an extra incomplete plane of atoms KE above the slip plane. The edge of the extra plane coincides with the dislocation and gives it

Kelly_c08.indd 244

11/30/2011 8:49:28 AM

Dislocations

245

its name. A similar view of a plane normal to a screw dislocation does not show the distortion of the lattice, because the displacements of the atoms are parallel to the dislocation in this case (Figure 8.6a). A view of the atom positions in the atom planes immediately above and below the slip plane is given by Figure 8.6b. The term ‘screw’ arises because the successive planes of atoms normal to the dislocation are converted by the presence of the dislocation into a single screw surface, or spiral ramp. This can be visualized from Figure 8.1 by imagining oneself to be walking around the dislocation on these planes. Successive intersections of such a tour with the plane of Figure 8.6 occur at 1, 2, 3, 4 and so on. Crystals normally contain a great number of dislocations, even before they are plastically deformed. The total length of dislocation line in 1 m3 of a metallic crystal (the dislocation density) may typically be 1012 m, although a wide variation over orders of magnitude is possible, depending on the degree to which the metal has been either annealed or cold worked. So far we have considered only dislocations occurring as a result of slip and lying in a slip plane. This is an unnecessary restriction, and dislocations can, in fact, be produced in other ways than by glide, as we shall see in Section 8.2. A general method is therefore needed for describing the Burgers vector – that characteristic discontinuity of displacement which defines a dislocation in a crystal. The following method is often used. First, a closed circuit is made around the suspected dislocation, called a Burgers circuit. This is a circuit made by jumping from one lattice point to a neighbouring lattice point until the starting point is reached again. The circuit must be made in ‘good’ material – that is, in regions of the crystal in which, even though they may be strained, each jump is recognizably associated with a jump in a perfect crystal of the same structure. With this vital condition fulfilled, a corresponding set of jumps can then be traced in the perfect crystal; if it fails to close, the circuit in the real crystal does indeed surround a dislocation. A little thought will show that if the circuit fails to close then it must do so by a lattice vector. The lattice vector that is needed to complete the circuit in the ideal crystal is defined as the Burgers vector of the dislocation. A dislocation that can be dealt with by this procedure must have a Burgers vector equal to a translation vector of the Bravais lattice; such a dislocation is called a perfect dislocation. This method of defining the Burgers vector is illustrated in Figure 8.7. The circuit of 17 successive jumps in the real crystal has a corresponding set of jumps in the perfect crystal which fails to close. The vector [010] is needed to complete the circuit in the ideal crystal; this is the Burgers vector. Some sign convention is needed to define the sense of the Burgers vector. The FS/RH convention works as follows. First, a sense is arbitrarily attached to the dislocation line. This permits a choice of Burgers circuit with a right-hand screw relationship to the line (the RH of the notation). In Figure 8.7 the line is taken to run into the paper. The Burgers vector is then taken to run from the finish to the start of the path in the perfect crystal (the FS of the notation); for example, from F to S in Figure 8.7.2 If the sense of the line is reversed, the Burgers vector is also reversed, so that some consistency in choosing a line sense is desirable.

2

The opposite convention, SF/RH, is used by some authors. For an account of where one convention has been used, and where the other, see de Wit [1].

Kelly_c08.indd 245

11/30/2011 8:49:28 AM

246

Crystallography and Crystal Defects

S

F

[010]

Figure 8.7 A Burgers circuit around an edge dislocation (a)

(b) a E2 E1 E1

E2

Figure 8.8

As an example, consider a closed loop of dislocation lying in a slip plane (Figure 8.8a). Suppose that within the loop the top half of the crystal has slipped by [010] with respect to the bottom half, as shown by the arrow. Then the positions of the atoms in the (100) plane (the plane a in Figure 8.8a) are as shown in Figure 8.8b. Since the edge dislocations at E1 and E2 would annihilate one another if they glided together (their extra planes would join), they are commonly referred to as edge dislocations of opposite sign. The Burgers vector at E2 is in the opposite direction to that at E1 if the direction assigned to the line at E2 is the same as that assigned to the line at E1, such as into the page. This would be perfectly fine if the dislocation lines at E1 and E2 were actually parallel lines. If the whole loop is being considered, however, it is more logical to make the sense of the line continuous around the loop. Then if the direction of the line at E1 is into the page, the direction of the line at E2 must be out of the page, and when the Burgers circuits round E1 and E2 are each taken in the RH sense, the same sense of Burgers vector is obtained at E1 as at E2 This second way of stating the Burgers vector emphasizes the fact that the displacement discontinuity, which the Burgers vector measures, remains constant along a given dislocation line. This follows because if we move the Burgers circuit along the dislocation line it must remain in good material.

Kelly_c08.indd 246

11/30/2011 8:49:28 AM

Dislocations (a)

247

(b) l

n D′

d

B′

l

P

B

d

A′ Q A D

Figure 8.9

The principle of the conservation of the Burgers vector is a general one, and from it, it follows that a dislocation line cannot end inside a crystal. It must end at a surface, form a closed loop or meet other dislocations. A point at which dislocation lines meet is called a node. The conservation of the Burgers vector in this case can be stated in the following way. If the directions of all the dislocation lines are taken to run out from the node then the sum of the Burgers vectors of all the dislocations is zero. This is the dislocation analogue of Kirchhoff’s law of the conservation of electric current in a network of conductors.

8.2

Dislocation Motion

We have seen that the motion of a dislocation on a slip plane changes the area over which slip has occurred. In this section the effect of dislocation motion in general will be discussed. Consider two neighbouring atoms, P and Q, lying at lattice points in a plane which is threaded by a dislocation DD′ (Figure 8.9a). Suppose the dislocation passes between P and Q so as to move inside a Burgers circuit, part of which is the step from P to Q. The corresponding circuit in the ideal crystal then acquires a closure failure equal to the Burgers vector, b. This must be attributed to a displacement of P relative to Q of b in the real crystal (it cannot be attributed to the relative displacement of the members of any other neighbouring pair of atoms in the Burgers circuit since it is possible to draw Burgers circuits through these that do not contain the dislocation either before or after its movement). The determination of the sense of the relative displacement requires some care. Define a positive direction QP by the cross product l × d (Figure 8.9b); that is, l, d and QP are related as a right-handed set of axes x, y, z. Here l is the vector parallel to the dislocation line used in defining the Burgers vector b by the FS/RH convention; d is a vector in the direction of motion of the dislocation. With this definition, the displacement of the atom on the positive side, P, relative to that on the negative, Q, is +b when the dislocation passes between P and Q, as shown. We shall use this result to study the relative displacement of material on either side of the surface that a dislocation sweeps out during its motion. Suppose a segment of a dislocation line AB moves to A′B′, sweeping out a plane surface whose unit normal is n. The sense of n is defined in accordance with the previous paragraph as the sense of l × d (Figure 8.9b). The atoms above ABB′A′ are displaced by b relative to those below.

Kelly_c08.indd 247

11/30/2011 8:49:28 AM

248

Crystallography and Crystal Defects (a)

b

(b)

b

Figure 8.10 The dislocation loop shown in (a) can glide so that its area projected normal to the Burgers vector does not change. It moves in the surface of a cylinder. (b) This shows that a screw segment can leave the surface of this cylinder without changing the projected area

If b · n is positive, the atoms above move away from those below, creating a void, whose volume is b · n per unit area swept out. Motion for which b · n < 0 requires the disposal of extra material of volume b · n per unit area. When b · n ≠ 0 the dislocation motion is normally accompanied by diffusion, which brings in atoms to fill the void when b · n > 0 and disperses the extra atoms when b · n < 0. Dislocation motion of this type is called ‘climb’. The origin of this name can be seen from Figure 8.5. If the atoms on the edge of the extra plane are removed, the edge dislocation in Figure 8.5 will climb up out of its slip plane. Climb downwards could be accomplished by adding atoms to the extra plane. Dislocation glide is motion that does not involve the addition or removal of material; that is, motion for which b · n = 0. The glide surface is defined accordingly as that surface which contains the dislocation line and whose normal is everywhere perpendicular to the Burgers vector. For a straight-edge dislocation, this defines a single plane, which is the slip plane. For a screw dislocation any plane passing through the dislocation fulfils the condition b · n = 0. For a closed loop of dislocation a cylinder is defined as the glide surface. The surface of the cylinder is generated by lines parallel to the Burgers vector passing through all points on the dislocation (Figure 8.10a). The glide of the loop is not confined to the surface of its glide cylinder, because if it has any screw parts they can glide on any plane; however, the area of the loop in projection on a plane normal to the axis of the cylinder remains constant (Figure 8.10b). This area is zero for a loop on a slip plane (Figure 8.8a). When the area is not zero, the loop is called ‘prismatic’. A special case is a pure-edge dislocation loop. This could be produced by prismatic punching, as shown in Figure 8.11, in which case its structure corresponds to a penny-shaped disc of extra atoms in the plane of the loop. With a Burgers vector of opposite sense, its structure corresponds to a disc of missing atoms. In the latter case, the loop could be formed by collecting together a disc of vacant lattice sites. When a dislocation glides, there is no problem of acquiring or disposing of extra atoms. This is in sharp distinction to climb, and it leads us to suppose that a dislocation will be able

Kelly_c08.indd 248

11/30/2011 8:49:29 AM

Dislocations

249

(a)

(b)

E

E′ E

E′

Figure 8.11 (a) Production of a prismatic dislocation loop by punching. (b) Section normal to the plane of the loop and passing through E and E′

to glide much more quickly than it can climb. The ease of gliding may be quite different for different crystallographic surfaces, and may be so much easier for one crystallographic plane that slip is effectively confined to that plane.

8.3 The Force on a Dislocation In Section 8.1 we found that when a dislocation moved on a slip plane, the area of the slip plane across which slip had occurred was increased or decreased, according to the direction of motion. As a result, work may be done by the forces applied to the crystal. For example, suppose forces acting in the slip direction are applied to the top and bottom surfaces of the crystal in Figure 8.1, in the directions SS′ on the top surface and S′S on the bottom. When the dislocation, of unit length say, moves to the left and sweeps out an area 1.dx of slip plane, applied forces of magnitude s dx move through the slip distance b, if the applied forces are of strength s per unit area of the top and bottom surfaces. The work done is then: dw = σ b dx

(8.1)

We can use this result to define a force3 acting on a unit length of the dislocation in the direction Ox: F=−

dE dx

(8.2)

where E is the energy of the system, which comprises the crystal and the device applying the forces to it. If we examine the work done by the forces acting on the surfaces at the slip plane, which are displaced relative to one another when the dislocation moves a distance dx, we see that it has the same magnitude sb dx as the work done by the externally applied forces, but is opposite in sign. This work done at the slip plane is dissipated, like the work 3

Defining a ‘force’ exerted on a dislocation line is a way of describing the tendency of the configuration which constitutes the dislocation to move through the crystal. There is no physical force on a dislocation line in the sense in which there is a force on a rod when a string attached to it is pulled, for example.

Kelly_c08.indd 249

11/30/2011 8:49:29 AM

250

Crystallography and Crystal Defects

done at sliding surfaces in a friction problem. The dissipated energy is supplied by the device applying the forces to the crystal, which therefore loses energy: − dE = dw = σ b dx

(8.3)

Substituting Equation 8.2 in Equation 8.3 gives: F = σb

(8.4)

This definition of the force per unit length acting on a dislocation can be extended to the general case of a dislocation moving in any direction in a crystal which is stressed internally or by external forces. To do this we use the result of the preceding section, that when a segment of dislocation line sweeps out an area of internal surface, the material on the positive side of that surface is displaced by b relative to the material on the negative side. The crystal is conceived to be cut at this surface. The force acting on one of the surfaces of the cut is calculated from the stress in the crystal, and the work done by this force on the crystal during the displacement is then calculated, the other surface being held fixed. The dislocation will be driven in such a direction that this work is negative. In the absence of external forces the energy of the crystal will then decrease (its self-stress will be reduced), and the magnitude of the force on the dislocation is defined by the decrease in the energy of the crystal when the dislocation moves a unit distance. If the dislocation is being driven by externally applied forces, this energy loss is made up by the work done on the crystal by the applied forces; the energy of the crystal itself does not change. The decrease in energy of a larger system which includes the device applying the force can then be considered to define the force acting on the dislocation, and identical equations are obtained. Using the sign convention of the preceding section, the force F acting on a unit area of the surface bounding the negative side of the cut is given by (see Section 6.3): Fi = σ ij n j

(8.5)

F =s ·n

(8.6)

or, in vector notation:

This force is exerted by the material on the positive side of the swept-out surface. The stress is s and n is a unit vector normal to the swept-out surface. The sense of n is given by l × d, where l is a unit vector parallel to the dislocation line and d is a unit vector in the direction of motion (Figure 8.9). Without loss of generality, we can take d perpendicular to l, since any motion of the dislocation parallel to itself sweeps out no area. Therefore: n = l×d

(8.7)

The movement of the dislocation displaces the surface bounding the negative side of the cut by −b if the opposite surface remains at rest, so that the work done on the crystal is: w = − (σ ⋅ n) ⋅ b

Kelly_c08.indd 250

(8.8)

11/30/2011 8:49:29 AM

Dislocations

251

which, because s is a symmetrical tensor, can be written in suffix notation (Appendix 1) as: w = − σ ij n j bi = − σ ji bi n j That is, in vector notation: w = − (σ ⋅ b) ⋅ n

(8.9)

The decrease in energy, −w, is given by the negative of this, so: − w = (σ ⋅ b) ⋅ (l × d) or: − w = (σ ⋅ b) × l ⋅ d

(8.10)

using the theorems on the scalar triple product of vectors (Appendix 1). We now have the work done by the crystal when a unit length of dislocation moves a unit distance in the form: −w = F⋅d

(8.11)

where d is a unit vector in the direction of motion. F is therefore the force per unit length acting on the dislocation, so: F = (σ ⋅ b) × l

(8.12)

The expression s · b represents the force per unit length acting on a plane normal to the Burgers vector, of area b. Since l is a unit vector parallel to the dislocation, we see that the force is always normal to the dislocation line. As an example of the application of this formula, consider the edge dislocation of Figure 8.12 in a region of general stress s. The stress may be the result of forces applied to the exterior of the crystal, or it may be a local self-stress.4 Suppose that the dislocation runs along the x2-axis and that its Burgers vector is in the direction −x1. It is evident that the glide plane is the plane containing these two directions. The traction on the surface whose outward normal is b is the result of components due to s11, s12 and s13 (Figure 8.12). The component of (s · b) due to s12 is parallel to l and so makes no contribution to (s · b) × l. The component s11 produces a traction in the direction of b and a component of force on the dislocation of magnitude s11b acting downwards, perpendicular to the glide plane. If s11 is negative, the force on the dislocation is directed upwards. This confirms the intuition that a compression along the x1-axis will tend to squeeze the extra plane out of the crystal, and that a tensile stress will tend to draw it downwards. The component of the force normal to the glide plane is called the climb force. The glide force acts in the glide plane, and in this case it is given by the shear component s13, which produces a force per unit length of magnitude s13b directed along Ox1. This is completely consistent with glide arising through volume-conserving shear 4

A self-stress, sometimes called an internal stress, is a stress that exists within a crystal that is free from externally applied forces.

Kelly_c08.indd 251

11/30/2011 8:49:29 AM

252

Crystallography and Crystal Defects

x3

l x2 s11

b

s12 s13

x1

Figure 8.12

processes (Chapter 7). Sometimes it is only important to know the glide force; that is, the component of force in the slip plane. As can be seen from Equation 8.8, the glide force on any dislocation is simply b times the component of the traction on the slip plane that acts in the slip direction. When an edge dislocation climbs under the influence of a stress, void or extra material is created, and it is intuitively clear that the climb will be brought to a halt if the extra material is allowed to accumulate, or if the void is not filled in. This leads to the idea of a ‘chemical’ force on a dislocation, due, for instance, to the absence of atoms on some of the sites in the surrounding lattice. To understand this force we must anticipate somewhat. It is shown in Chapter 10 that a crystal in equilibrium contains a certain number of empty atomic sites, called vacancies. To define the chemical force in this instance we write down the equilibrium concentration of vacancies in the presence of an edge dislocation under stress. When the concentration has this equilibrium value the dislocation has no tendency to create or annihilate vacancies by climbing, and so we define a chemical force equal and opposite to the climb force exerted by the stress. Suppose that when a vacancy is created by adding a lattice atom to the edge of the extra plane of an edge dislocation, a length ab of dislocation climbs by bb. Here a and b are constants of order unity which depend upon the structure of the crystal. Then when a vacancy is created, a stress that exerts a climb force F per unit length does work W 5 given by: W = Fαβ b2

(8.13)

Consequently, the equilibrium concentration of vacancies is increased from its value C0 in the absence of the climbing force6 to: ⎛ Fαβ b2 ⎞ C = C0 exp ⎜ ⎟ ⎝ kT ⎠

(8.14)

5 Here we are neglecting work that will be done by the hydrostatic component of the stress if the volume of the crystal changes when an atom is removed from an interior site. For the effect of this, see Weertman [2]. 6 See Section 10.1.

Kelly_c08.indd 252

11/30/2011 8:49:29 AM

Dislocations

253

where k is Boltzmann’s constant and T is absolute temperature. We define a chemical (or osmotic) force equal and opposite to F as being exerted by the concentration C of vacancies through the equation: −F = −

kT αβ b2

ln

C C0

(8.15)

In the absence of stress, a concentration C which is not equal to its equilibrium value C0 gives a chemical force that is not balanced by a force due to stress. The magnitude of this force is given by Equation 8.15. The dislocation will then climb upwards in Figure 8.12 if C/C0 > 1; that is, in the presence of a ‘supersaturation’ of vacancies. It is interesting to compare the magnitude of the ‘chemical stress’ F/b with the magnitude of a typical mechanical stress. Setting a = b = 1, mb3 ~5 eV,7 where m is the rigidity modulus and kT ≈ 0.025 eV at room temperature, we obtain: F C μ ~ ln b 200 C0

(8.16)

Many crystals cannot support so large an applied stress as m/200, so quite trifling supersaturations (C/C0 ~ 3) produce a force larger than that arising from any applied stress. Larger supersaturations, such as may be produced by quenching from close to the melting point, can cause small prismatic dislocation loops to be produced. These have been observed, for example, in aluminium [3,4].

8.4 The Distortion in a Dislocated Crystal It is important to know exactly how the structure of a crystal is distorted by a dislocation. This information is needed in tackling such problems as how dislocations interact with each other and with other lattice defects. An obvious way to approach the problem is to investigate an elastic continuum containing a dislocation. If a satisfactory solution is found for the dislocated continuum, the atoms in a crystal can then be assigned the displacements that are suffered by the corresponding points in the continuum. As a first approximation, isotropic elasticity can be assumed. For a screw dislocation in an isotropic continuum, the problem is simple enough for an intuitive approach to give the correct solution. We expect the displacement at any point to be parallel to the direction of the line of the dislocation. Further, because of the radial symmetry of the situation, a total displacement b must be spread out evenly over a circular path around the dislocation. This suggests a displacement uz given by: uz =

7

bθ 2π

(8.17)

The eV (electron volt) is a unit of energy equal to 1.602 × 10−19 J.

Kelly_c08.indd 253

11/30/2011 8:49:29 AM

254

Crystallography and Crystal Defects b

q

g

r

2πr

b

z

Figure 8.13

Strain due to a screw dislocation lying along the z-axis

If a path at a radial distance r from the dislocation is imagined to be straightened out, as in Figure 8.13, the shear strain is seen to be: γ zθ =

b 2π r

(8.18)

The non-zero stress component is the corresponding shear stress, given by Hooke’s law, Equation 6.85, as: σ zθ = σ θ z =

μb

2π r

(8.19)

where m is the shear modulus defined in Equation 6.82. It remains only to check that the stresses given by Equation 8.19 are such that every part of the body containing the dislocation is in equilibrium. Because the stress szq does not change with z or q, the opposite faces of all small elements, like the one shown in Figure 8.14, centred at a distance r away from the z-axis, are acted on by equal and opposite forces, so that the element is in equilibrium. Further, since szr, sq r and srr are everywhere zero, the surface of a cylinder around the dislocation is free of force. A difficulty with the shear strain given by Equation 8.18 is that it becomes infinite as r approaches zero. Since Hooke’s law applies only to small strains, it is usual to cut off the solution at a radius where the strains become large, say r ~ 5b. The material within a cylindrical surface of this radius is called the dislocation core. The core surface is in effect a boundary of the elastic body. The forces that would be exerted from point to point on this boundary by the core material are not known, but it is known that no net force can be exerted in any direction, nor any couple. This condition is satisfied by Equation 8.19, which gives a cylindrical surface that is entirely free of force. Equations 8.17 and 8.19 therefore give satisfactory displacements and stresses at distances greater than about 5b from a screw dislocation in an infinitely long isotropic cylinder. For a finite cylinder with free ends, the

Kelly_c08.indd 254

11/30/2011 8:49:29 AM

Dislocations

255

dz szq dr

szq

dq

z

Figure 8.14 Stress due to a screw dislocation along the z-axis acting on a small element of volume rdrdqdz at a distance r away from the z-axis

solution needs to be modified in order to remove the effect of the couple on the end surfaces that is produced by the stress szq. The problem of finding the displacements around other dislocations can be approached in the same way.8 A displacement function is sought that gives the required discontinuity of displacement in a circuit around the dislocation and in addition satisfies the equations of equilibrium. Expressed in Cartesian coordinates, with the dislocation lying along the x3-axis, the equations of equilibrium are the three equations: ∂σ i1 ∂x1

+

∂σ i 2 ∂x2

=0

(i = 1, 2, 3)

(8.20)

The stress sij can be expressed in terms of the derivatives of the components of displacement u1, u2 and u3 through Hooke’s law (Section 6.5). Because the stress and strain given by any displacement having the required discontinuity become infinite at the dislocation, it is further necessary to ensure that a cylinder of material containing the dislocation is in equilibrium, or in other words, that the force exerted on the core surface vanishes. The solution for an edge dislocation in an isotropic medium is more complicated than that for a screw. If the dislocation lies along the x3-axis with its Burgers vector parallel to x1, the displacements can be written in the forms [5]: u1 =

8

b 2π

⎡ −1 x2 ⎛ λ + μ ⎞ x1 x2 ⎤ + ⎢ tan ⎥ x1 ⎜⎝ λ + 2 μ ⎟⎠ x12 + x22 ⎦⎥ ⎣⎢

(8.21a)

The remainder of this section is somewhat advanced and can be omitted at a first reading.

Kelly_c08.indd 255

11/30/2011 8:49:30 AM

256

Crystallography and Crystal Defects

u2 =

b 2π

⎡ ⎛ λ + μ ⎞ x22 ⎤ μ ln x12 + x22 + ⎜ ⎢− ⎥ ⎝ λ + 2 μ ⎠⎟ x12 + x22 ⎥⎦ ⎢⎣ 2(λ + 2 μ )

(

)

(8.21b)

where l is the Lamé constant (Section 6.5). The first term in Equation 8.21a has the same form as the solution for a screw dislocation, and provides the necessary cyclic discontinuity in u1 equal to the Burgers vector b. The first term in u2, the displacement normal to the slip plane, is needed in order that the equations of Equilibrium 8.20 are satisfied. The second terms in Equations 8.21a and b are needed to make the core force vanish. The pattern produced when these displacements are imposed on a square array of points in the x1x2-plane is shown in Figure 8.5. The elastic constants used in Equations 8.21 to obtain Figure 8.5 were those of tungsten, which happens to be elastically isotropic, to a good approximation. A consideration of the relevant equations leading to Equations 8.21 shows that there is an element of choice in the constant of integration in the equations relating the displacements to the elastic strains. Results quoted elsewhere for these displacements [6–10] are the same, apart from differences in the choice of the constant of integration. The stresses which follow from the displacements given by Equations 8.21 are: σ 11 = − σ 22 =

μb

x2 (3 x12 + x22 )

2π (1 − ν ) ( x12 + x22 )2 μb

x2 ( x12 − x22 )

2π (1 − ν ) ( x12 + x22 )2

σ 33 = ν (σ 11 + σ 22 ) σ 12 =

μb

(8.22)

x1 ( x12 − x22 )

2π (1 − ν ) ( x12 + x22 )2

where n is Poisson’s ratio. The stresses and strains due to a mixed dislocation in an isotropic medium whose line makes an angle q with its Burgers vector can be obtained by simply adding the stresses and strains due to a screw dislocation of the Burgers vector b cos q to those due to an edge dislocation of the Burgers vector b sin q. This is because the terms in the stress fields of the screw and edge components are independent of one another. Tungsten, together with aluminium, is an exceptional crystal in being, elastically, almost isotropic. For most crystals, obtaining accurate values for the positions of atoms outside the core of a dislocation requires the use of the true elastic constants of the crystal, rather than the averaged values, which describe the isotropic behaviour of a polycrystal of the material. This means that the correct form of Hooke’s law must be used in converting Equations of Equilibrium 8.20 into equations in the displacements. In the general case, this introduces all nine terms of the type ∂2ui/∂xa∂xb into Equations of Equilibrium 8.20 (i = 1, 2, 3; a, b = 1, 2). The resultant mathematics is highly complex, requiring the solution of a sixth-order polynomial [10–12]. The cases that have been solved analytically are ones in which this number of terms is reduced because of symmetry. This requires not only that the crystal structure be of high symmetry but also that the dislocation lies in some special direction in

Kelly_c08.indd 256

11/30/2011 8:49:30 AM

Dislocations

257

x2 – [110]

r

θ x1

O

[001]

Figure 8.15

the crystal, such as along a two-fold axis of symmetry. For example, full solutions have been published for an edge dislocation along 〈001〉 in a cubic crystal, a screw normal to a mirror plane and a dislocation lying in the basal plane of a hexagonal crystal [13,14]. Yin et al. [15] have recently compared a number of approaches for numerical efficiency and accuracy to compute stresses, displacements and forces on finite lengths of arbitrarily oriented dislocations in anisotropic media. The simplest case is that of a screw dislocation lying normal to a mirror plane [13]. Then, if the x3-axis is chosen to be parallel to the dislocation, the elastic constants c′14, c′15, c′24, c′25, c′34, c′35, c′46 and c′56 vanish (see Table 6.2; primed elastic constants are constants referred to axes that are not chosen with a conventional relationship to the crystal axes) [10]. The displacement can be written in the form [10]: u3 = −

(c ′ c ′ − c45 ′ 2 )1/ 2 x2 b tan −1 44 55 2π c44 ′ x1 − c45 ′ x2

(8.23)

For a screw dislocation along 〈110〉 in a c.c.p. crystal, Equation 8.23 reduces to: u3 = −

A1/2 x2 b tan −1 2π x1

(8.24)

where the x1- and x2- axes are shown in Figure 8.15 and A is the anisotropy factor given by Equation 6.77: A=

2c44 c11 − c12

The anisotropy factor destroys the radial symmetry of the displacement, which is otherwise of the same form as in an isotropic medium. When A > 1, as it is for c.c.p. metals, the shear strain is greatest on the {110} plane; when A < 1, as it is for some alkali halides and some

Kelly_c08.indd 257

11/30/2011 8:49:30 AM

258

Crystallography and Crystal Defects

b.c.c. metals, the shear strain is greatest on the {100} plane. Because the shear modulus varies with orientation, a shear stress szr is introduced: σ zr =

c44 b(1 − A)sin θ cos θ 2π A1/ 2 r (cos2 θ + A sin 2 θ )

(8.25)

in addition to the shear stress szq, which has the same form as in the isotropic case, namely [13]: σ zθ =

c44 b 2π A1/ 2 r

(8.26)

8.5 Atom Positions Close to a Dislocation Although the solutions for dislocations in an elastic continuum can be used to assign displacements to the atoms around a dislocation in a crystal, these displacements are unlikely to be correct for atoms close to the dislocation, because the elastic continuum solutions may not be valid in this region of high strain. To determine the displacements in this core region of the dislocation, a detailed knowledge of the forces acting between atoms is needed. Atomistic simulations now enable these displacements to be determined using suitable interatomic potentials. Comprehensive reviews of progress in this area over the years can be found in the Dislocations in Solids series [16–18]. However, to convey the essential physical aspects of such displacements without recourse to such detailed simulations, our discussion here will be less rigorous. As a starting point, consider a simple cubic lattice and take the displacements for a screw dislocation given by Equation 8.17, treating it as an isotropic continuum: uz =

bθ 2π

If the position of the dislocation line is taken to be as in Figure 8.6 and q is taken as the angle measured anticlockwise from Sx1, which can be considered to be the trace of a plane on which the screw glides, the displacements of the atoms numbered 1 to 4, for example, are: b 3b 5b 7b , , , 8 8 8 8 respectively. The displacement across the slip plane Sx1 is: Δu = b −

bθ

(8.27)

π

No displacement has occurred across the slip plane to the far left of the dislocation (q = p), while the relative displacement is b to the far right (q = 0). Equation 8.27 can be written as: Δu = b −

Kelly_c08.indd 258

b π

tan −1

b b = b− π 2 x1

⎛π −1 2 x1 ⎞ ⎜⎝ 2 − tan b ⎟⎠

11/30/2011 8:49:30 AM

Dislocations

259

Δu b

–2

–1

0

Figure 8.16

1

2

x1 /b

Plot of Equation 8.28

or: Δu =

2x b b + tan −1 1 2 π b

(8.28)

This function is plotted in Figure 8.16. The distance on the slip plane over which the displacement lies between 14 and 34 of its extreme values is defined as the width of the dislocation on that plane. The width of the dislocation in Figure 8.16 is b, slightly more than the width of 0.75 b determined for the width of a screw dislocation core in aluminium in recent atomistic simulations [19]. Suppose now that we double the width of the dislocation by making Δu change with x1 according to the equation: Δu =

x b b + tan −1 1 2 π b

(8.29)

This is equivalent to giving the atoms the displacements that they would have, according to the symmetrical solution (8.17), if they were arranged on a tetragonal lattice with a spacing across the slip plane twice that within the plane. The displacements of the atoms 1 to 4 become approximately: b b 2b 5b , , , 6 3 3 6 The widened dislocation is shown in Figure 8.17. The shear strain in bonds 1–4 and 2–3 is twice that in the bonds 1–2 and 3–4. A similar situation would be expected in a real crystal if the bonds between the slip planes were weaker than those between atoms within a slip plane. A model which gives special consideration to the bonds across the slip plane is the Peierls dislocation [20]. In this model the crystal is supposed to be divided into two blocks at the slip plane, each of which is an elastic continuum. The atomic structure is taken into account only at the slip plane, where the two blocks join. A periodic force law is allowed to act between the rows of atoms immediately above the slip plane and those immediately below. For simplicity, a sine law is chosen:

Kelly_c08.indd 259

11/30/2011 8:49:30 AM

260

Crystallography and Crystal Defects S′ 4

3 2

1 4

3 2

l S

Figure 8.17 A screw dislocation of twice the width of the one shown in Figure 8.6

σ=

bμ 2π Δ u sin 2π a b

(8.30)

The spacing between the slip planes is a, so that Δu/a is the shear in the bond between two rows of atoms across the slip plane, while b is the atomic spacing within a slip plane. Equation 8.30 reduces to Hooke’s law at small strains; that is, at small values of Δu. A dislocation is made by straining the elastic blocks and then joining them at the slip plane. The restoring force acting between sheared rows of atoms according to Equation 8.30 tends to narrow the dislocation. The forces due to the elastic strains within the blocks tend to widen it. A balance is reached with a certain distribution of displacements. Either an edge or a screw dislocation can be made, although the model is more attractive for an edge dislocation, where there are large shear strains on a unique slip plane. The displacements across the slip plane of a Peierls screw are identical to those predicted by the elastic continuum solution (8.28). That is: Δu =

2x b b + tan −1 1 π 2 a

(8.31)

The displacements for a Peierls edge differ from those for an elastic edge dislocation and give: Δu =

2 x (1 − ν ) b b + tan −1 1 2 π a

(8.32)

The Peierls edge is wider than the screw by the factor 1/(1 − n), where n is Poisson’s ratio. As n increases towards its greatest possible value of 0.5, the resistance of the material to elastic shear decreases relative to its resistance to dilatation. An increase in the width of an edge dislocation as n increases therefore accords with the qualitative idea that if the atoms are hard, but shear over one another easily, as for metallic materials, then squeezing in the extra plane of atoms will spread the dislocation out over its slip plane. On the other hand, if there are strong directed bonds across the slip plane, their resistance to shear will lead to a narrow dislocation. Such directed bonds occur in covalent crystals like silicon.

Kelly_c08.indd 260

11/30/2011 8:49:30 AM

Dislocations

261

An important property which is controlled by the atom positions in the dislocation core is the force needed to start a straight dislocation moving in an otherwise perfect lattice. As the dislocation moves, the displacements around it will change, and in general the energy stored in the core will change slightly. Consequently, a force is exerted on the dislocation, given by: Fx = −

dE dx

(8.33)

where E is the energy due to the dislocation. The maximum value of this force is called the Peierls force, because it was first investigated by Peierls using a model of an edge dislocation [20]. The method can be briefly illustrated with the help of Figure 8.6, taking the dislocation S to be a Peierls screw. For any position of S on the plane Sx1 (Figure 8.6a), Equation 8.31 can be used to assign displacements to the atoms. The energy stored in the bonds across the slip planes, 2–3, 1–4 and so on, can then be summed as a function of the position of the dislocation. The energy sum E′ turns out to be a minimum for position S1 and a maximum for position S2 (Figure 8.6a), where the highly strained 1–4 bond makes a large contribution. At an intermediate position, dE′/dx1 can be shown to have a maximum value of the form: dE ′ ⎛ πa⎞ = Fp ≈ μ exp ⎜ − ⎟ ⎝ b⎠ dx1

(8.34)

This result has no quantitative significance because of the unrealistic nature of the model, and indeed it gives far too large a value for the force needed to move a dislocation in, say, a c.c.p. metal. The decrease in Fp with the parameter a, which on this model is equivalent to the width of the dislocation, is physically reasonable. As a dislocation becomes narrower, the change in displacement as it moves is distributed among fewer atoms. When the width is very small, a few core atoms have to make large jumps, for which there may be a substantial energy barrier, in order to move the dislocation by one atomic spacing.

8.6 The Interaction of Dislocations with One Another When a crystal is plastically deformed, some of its dislocations are lost as they glide to the surfaces of the crystal. However, dislocations must also be replenished during plastic flow, because a strain of 10% typically increases their density by 1012–1013m−2 (dislocation density is defined in Section 8.1). As the density of dislocations increases, their interaction with one another becomes important. For example, the stress needed to deform the crystal plastically increases and becomes controlled by the forces that dislocations exert on one another, rather than by the stress needed to move an isolated dislocation. A simple mechanism by which dislocations can multiply was suggested by Frank and Read [21]. Its operation requires only that a dislocation in a slip plane be pinned at two points. In Figure 8.18 the dislocation is pinned at the points x′y′ where it changes its plane. It is apparent from Figures 8.18a and b that this configuration could occur if a screw segment xy glided off its original slip plane to the position x′y′. This manoeuvre is called

Kelly_c08.indd 261

11/30/2011 8:49:30 AM

262

Crystallography and Crystal Defects (b) x′

(a)

x

x

y′ y

y

b

(d) (c) x′ x

x′ x

y′ y

y′ y

Figure 8.18

Dislocation multiplication

cross-slip. When the segment x′y′ changes back to a plane parallel to the original slip plane, it is easy to see that it can generate any number of expanding loops, using x′ and y′ as pivots. This variant of the Frank–Read mechanism is due to Koehler [22]. It allows slip to spread out sideways from a single active slip plane and so it can account for the commonly observed slip band, which is a set of very closely spaced parallel planes on which slip has occurred (see Figure 7.3). When slip occurs in bands, or even when it occurs more diffusely, dislocations on nearby parallel slip planes must on occasion come close to one another. Then the stress due to the one dislocation will exert a force on the other dislocation, according to Equation 8.12, where we substitute for s the stress due to one dislocation at the position of the other. Two special cases, parallel screws and parallel edges, will be briefly reviewed, assuming isotropic elasticity. Parallel screw dislocations a distance r apart experience a simple central force: F=

μb2

(8.35) 2π r The force per unit length, F, is repulsive when the screws are identical, so that their stress fields reinforce one another, and attractive when they are of opposite sign, so that their stress fields cancel as they come together. There is no position of equilibrium. Parallel edge dislocations, on the other hand, have two positions of equilibrium in respect of the component of force which lies in the slip plane. Since an edge dislocation would have to climb to move out of its slip plane, this is the only component of force that can cause an edge dislocation to move at low temperature. Its magnitude per unit length can be derived from Equations 8.22. It is convenient to write it in terms of polar coordinates as follows: Fg =

Kelly_c08.indd 262

μb 2

2π (1 − ν )r

cos θ (cos2 θ − sin 2 θ )

(8.36)

11/30/2011 8:49:30 AM

Dislocations

yo

263

r q x

0.3 Fg

0.2 0.1 0

1

2

3

4

5

6 x /y

o

– 0.1 – 0.2

Figure 8.19 Force between parallel edge dislocations on slip planes a distance y0 apart. The force is given in units of mb 2/2p(1 − n)y

The angle q is defined in Figure 8.19, in which Equation 8.36 is illustrated for edges of opposite sign. There is an unstable equilibrium at q = p/2 and a stable one at q = p/4, 3p/4. The force per unit length, Fm, which would be needed to push the parallel edges past one another on slip planes a distance y apart is: Fm =

μb2

8π (1 − ν ) y

(8.37)

Since yield stresses are typically in the range 10−3–10−4 m, edge dislocations of opposite sign are likely to become stuck against one another if they lie on slip planes which are a few hundred Å or less apart. Close pairs of dislocations of opposite sign are in fact commonly observed in deformed crystals; they are called dislocation dipoles. The forces acting between like edges are equal in magnitude but opposite in sign to those acting between unlike edges. The stable equilibrium therefore occurs at q = p /2. Two like edge dislocations are less likely to trap one another during glide than two unlike ones, because the applied stress moves them both in the same direction. However, the equilibrium configuration at q = p /2 becomes prominent when climb can occur. The component of force normal to the slip plane, the climb force, is given by: Fc =

μb2

2π (1 − ν )r

sin θ (1 + 2 cos2 θ )

(8.38)

This force is one of attraction between unlike edges and repulsion between like edges, for all q. If the temperature is high enough to allow climb, unlike edges from different slip planes annihilate one another, while any excess edges of the same sign which are left over arrange themselves in walls perpendicular to the slip plane. This is known as polygonization and occurs during the process of recovery when metals are annealed.

Kelly_c08.indd 263

11/30/2011 8:49:31 AM

264

Crystallography and Crystal Defects

P

r

d

b1 b2

Figure 8.20

Orthogonal screw dislocations, a perpendicular distance d apart

The elastic interaction of two dislocations in an anisotropic medium can differ quite significantly from the corresponding interaction in an isotropic medium. In copper, for example, two parallel screws lying along 〈110〉 in the same {111} slip plane exert forces on one another which are directed out of the slip plane, because of the shear stress srz given by Equation 8.25. Substitution of the appropriate constants into Equation 8.25 shows that the component of force normal to the slip plane is no less than 60% of the component of attraction or repulsion in the slip plane, which would be the sole component if the crystal of copper were elastically isotropic. Dislocations on intersecting slip planes also exert forces on one another due to their stress fields. For example, the stress field of a screw in an isotropic medium exerts a force on an orthogonal screw, given by: F=

μb1b2 d

2π r 2

(8.39)

where F is the force per unit length at the point P on the orthogonal screw, defined in Figure 8.20. The direction of F is normal to both dislocations. Its sign can be checked by comparing the shear stresses due to each screw at the midpoint of the shortest line joining them (the line of length d in Figure 8.20). The screws attract if the two stresses cancel one another and repel if they reinforce one another. Dislocations on intersecting slip planes interact in a second way, when they cut through one another. Because the material on one side of the surface swept out by a moving dislocation is displaced by the Burgers vector relative to the material on the other side, each dislocation acquires an extra length of line, equal in magnitude and direction to the Burgers vector of the other dislocation. If the extra length of line happens to lie on the plane on which the remainder of the dislocation is already gliding, it is called a kink. A kink can be eliminated immediately by glide. When the extra length of line does not lie on this plane, it is called a jog. When two orthogonal screws intersect, each acquires a jog which is a segment of edge dislocation. A jog of this type is shown in Figure 8.21, where the sign of the screw is indicated by means of the step that it produces on the surface of the crystal. If the jogged dislocation PQRS moves as a whole towards AD, the jog QR is forced to climb. Careful inspection of Figure 8.21 will show that a void is produced of volume QR times b times the distance moved. This void will take the form of a trail of vacant lattice sites. If PQRS moves in the opposite direction, towards BC, a trail of interstitial defects will be produced.

Kelly_c08.indd 264

11/30/2011 8:49:31 AM

Dislocations C

265

S R

B

D

Q P A

Figure 8.21

A third way in which two intersecting dislocations may interact with one another is that in certain circumstances they can come together and combine to form a new dislocation. This process is discussed in detail in the next chapter.

Problems 8.1 A screw dislocation of Burgers vector b passes straight through a crystal, meeting the front and back surfaces at 90°. Keeping this orientation, it moves so that its ends trace out circular paths and the dislocation line sweeps out a cylindrical surface. Describe the deformation produced by n revolutions of the dislocation. 8.2 Show how a pure edge dislocation loop, like that in Figure 8.11, can develop screw segments by gliding into a new shape. Hence show that it is geometrically possible for an edge dislocation loop to become a source for glide on any plane containing its Burgers vector. 8.3 An edge dislocation in a crystal of NaCl lies along [001] and its Burgers vector is 1 110 ] . If the dislocation is to be moved through a distance of 1 μm in the [100] direc2[ tion, calculate the volume of material that must be added to or subtracted from the edge of its extra plane, per metre of dislocation. 8.4 An edge dislocation in a crystal of NaCl lies along [001] and its Burgers vector is 1 110 ] . Calculate the glide force acting upon the dislocation under the action of a ten2[ sile stress s (a) when the tensile axis is [100] and (b) when the tensile axis is [111]. 8.5 A screw dislocation in a crystal of AgCl has the Burgers vector 12 [110 ] . If the dislocation could glide with equal ease on any plane, on which plane would it glide when under the action of a tensile stress (a) when the tensile axis is [100] and (b) when the tensile axis is [111]? 8.6 A screw dislocation lies along the axis of an isotropic cylinder of radius R. If the stress field were given by Equation 8.19, there would be forces acting on the end faces of the cylinder. Obtain an expression for the couple which would then be acting on the cylinder. (In a free cylinder the stress field would not be exactly given by Equation 8.19 but

Kelly_c08.indd 265

11/30/2011 8:49:31 AM

266

Crystallography and Crystal Defects

would contain an additional term, unimportant near the dislocation line, corresponding to a twisting of the cylinder, which neutralizes the couple implied by Equation 8.19 alone.) 8.7 From either Equations 8.21 or Equations 8.22 and 6.87, obtain the strain at a point directly above or below an edge dislocation (x1 = 0). Calculate the dilatations at points 5b above and 5b below an edge dislocation in aluminium. 8.8 Prepare a diagram of a plane which is normal to an edge dislocation in an isotropic medium, showing the lines in the plane on which one of the stress components s11, s22 and s12 vanishes (the dislocation lies along the x3-axis with its Burgers vector parallel to Ox1). Show the signs of the stresses in the various regions of the diagram. 8.9 Consider a screw dislocation in a c.c.p. crystal lying along [110]. Show (from Equation 8.24) that at equal distances from the dislocation, the shear strain on the – (11 0) plane that passes through the dislocation is A times the shear strain on the (001) plane that passes through the dislocation, where A = 2c44/(c11 − c12). 8.10 Obtain an expression for the width on the (001) plane of a screw dislocation lying along [110] in a sodium chloride crystal. Assume that the elastic continuum solution for the displacements (Equation 8.24) applies to all the atoms around the dislocation. 8.11 A cubic crystal is being stretched in a [100] direction. Its deformation is being pro– duced by edge dislocations lying parallel to [001] and gliding on (110) and (11 0) planes. If the density of these dislocations is r, the magnitude of the Burgers vector – of each one is b and their average velocity is V , determine the rate of increase of tensile strain of the crystal (= (1/l)(dl/dt), l = length of crystal). 8.12 Analyse the interaction between two edge dislocations whose lines are parallel to one another but whose Burgers vectors are orthogonal. Determine all positions of equilibrium with respect to glide forces and divide these into cases of stable, unstable and neutral equilibrium. 8.13 Find the total force experienced by an infinitely long screw dislocation of the Burgers vector b1 due to the presence of an infinitely long orthogonal screw dislocation of the Burgers vector b2. 8.14 In a crystal of sodium chloride, two orthogonal screw dislocations, of Burgers vectors – 1 110 ] and 12 [110] respectively, are being driven towards one another by a tensile stress 2[ along [100]. Demonstrate that each dislocation acquires a jog which produces interstitial defects if the dislocations continue to move under the action of the applied stress. 8.15 What is the minimum number of dislocations each with Burgers vector equal to the smallest lattice translation vector that can meet at a node in the following crystals: (a) b.c.c. iron, (b) diamond, (c) zinc and (d) caesium chloride? Under what conditions will the node be glissile?

Suggestions for Further Reading A.H. Cottrell (1953) Dislocations and Plastic Flow in Crystals, Oxford University Press, Oxford. J.P. Hirth and J. Lothe (1982) Theory of Dislocations, 2nd Edition, John Wiley and Sons, New York.

Kelly_c08.indd 266

11/30/2011 8:49:31 AM

Dislocations

267

D. Hull and D.J. Bacon (2011) Introduction to Dislocations, 5th Edition, Butterworth-Heinemann, Oxford. F.R.N. Nabarro (1987) Theory of Crystal Dislocations, Dover Press, Mineola, New York. W.T. Read (1953) Dislocations in Crystals, McGraw-Hill, New York. J.W. Steeds (1973) Introduction to Anisotropic Elastic Theory of Dislocations, Clarendon Press, Oxford. J. Weertman and J.R. Weertman (1992) Elementary Dislocation Theory, Oxford University Press, Oxford.

References [1] R. de Wit (1965) The direction of the force on a dislocation and the sign of the Burgers vector, Acta Metall., 13, 1210–1211. [2] J. Weertman (1965) The Peach–Koehler equation for the force on a dislocation modified for hydrostatic pressure, Phil. Mag., 11, 1217–1223. [3] P.B. Hirsch, J. Silcox, R.E. Smallman and K.H. Westmacott (1958) Dislocation loops in quenched aluminium, Phil. Mag., 3, 897–908. [4] J. Silcox and M.J. Whelan (1960) Direct observations of the annealing of prismatic dislocation loops and of climb of dislocations in quenched aluminium, Phil. Mag., 5, 1–23. [5] J.M. Burgers (1939) Some considerations on the fields of stress connected with dislocations in a regular crystal lattice. I., Proc. Konin. Ned. Akad. Wet., 42, 293–325. [6] J.S. Koehler (1941) On the dislocation theory of plastic deformation, Phys. Rev., 60, 397–410. [7] F.R.N. Nabarro (1952) Mathematical theory of stationary dislocations, Adv. Phys., 1, 269–394. [8] W.T. Read (1953) Dislocations in Crystals, McGraw-Hill, New York. [9] A.M. Kosevich (1979) Crystal dislocations and the theory of elasticity, in Dislocations in Solids, Volume 1 (edited by F.R.N. Nabarro), North-Holland, Amsterdam, pp. 33–141. [10] J.P. Hirth and J. Lothe (1982) Theory of Dislocations, 2nd Edition, John Wiley and Sons, New York. [11] J.W. Steeds (1973) Introduction to Anisotropic Elastic Theory of Dislocations, Clarendon Press, Oxford. [12] J.W. Steeds and J.R. Willis (1979) Dislocations in anisotropic media, in Dislocations in Solids, Volume 1 (edited by F.R.N. Nabarro) North-Holland, Amsterdam, pp. 143–165. [13] J.D. Eshelby, W.T. Read and W. Shockley (1953) Anisotropic elasticity with applications to dislocation theory, Acta Metall., 1, 251–259. [14] Y.T. Chou and J.D. Eshelby (1962) The energy and line tension of a dislocation in a hexagonal crystal, J. Mech. Phys. Solids, 10, 27–34. [15] J. Yin, D.M. Barnett and W. Cai (2010) Efficient computation of forces on dislocation segments in anisotropic elasticity, Modelling Simul. Mater. Sci. Eng., 18, art. 045013. [16] R. Bullough and V.K. Tewary (1979) Lattice theories of dislocations, in Dislocations in Solids, Volume 2 (edited by F.R.N. Nabarro), North-Holland, Amsterdam, pp. 1–65. [17] M.S. Duesbery (1989) The dislocation core and plasticity, in Dislocations in Solids, Volume 8 (edited by F.R.N. Nabarro) North-Holland, Amsterdam, pp. 67–173. [18] W. Cai, V.V. Bulatov, J. Chang, J. Li and S. Yip (2004) Dislocation core effects on mobility, in Dislocations in Solids, Volume 12 (edited by F.R.N. Nabarro and J.P. Hirth), Elsevier, Amsterdam, pp. 1–80. [19] G. Lu, N. Kioussis, V.V. Bulatov and E. Kaxiras (2001) Dislocation core properties of aluminium: a first-principles study, Mater. Sci. Eng. A, 309–310, 142–147. [20] R. Peierls (1940) The size of a dislocation, Proc. Phys. Soc., 52, 34–37. [21] F.C. Frank and W.T. Read (1950) Multiplication processes for slow moving dislocations, Phys. Rev., 79, 722–723. [22] J.S. Koehler (1952) The nature of work-hardening, Phys. Rev., 86, 52–59.

Kelly_c08.indd 267

11/30/2011 8:49:31 AM

9 Dislocations in Crystals 9.1 The Strain Energy of a Dislocation A considerable amount of strain energy is stored in the elastically distorted region around a dislocation line. The magnitude of the energy stored in an elastically strained region is always of the form 12 × (elastic modulus) × (strain)2, per unit volume (see Equation 6.60). Since the strain at a given point is proportional to the magnitude of the Burgers vector of the dislocation b, the total strain energy will be proportional to b2. To find the absolute magnitude of the energy stored, it is necessary to make a more detailed calculation. This can be done in two ways. In the first method, the energy stored in a small element of volume is found and an integration is performed. For a screw dislocation the appropriate element is a thin cylindrical shell of radius r, thickness dr, because the shear strain g within such a thin shell is constant (Equation 8.18): b 2π r

γ =

An elastically isotropic medium is assumed. The strain energy per unit length of shell is then: μb2 dE = ( 1 μγ 2 ) 2π r dr = dr 2 4π r

(9.1)

and so the energy per unit length of dislocation in the region from the core, radius r0, out to a radius R is: E=

∫

R

r0

μb2

4π r

dr

or: Crystallography and Crystal Defects, Second Edition. Anthony Kelly and Kevin M. Knowles. © 2012 John Wiley & Sons, Ltd. Published 2012 by John Wiley & Sons, Ltd.

Kelly_c09.indd 269

11/30/2011 6:17:38 PM

270

Crystallography and Crystal Defects

b

x2

x1

Figure 9.1

E=

⎛ R⎞ ln ⎜ ⎟ 4π r ⎝ r0 ⎠

μb2

(9.2)

To be exact, Equation 9.2 should be corrected to allow for the relaxation of stress at the free end surfaces of the cylinder. However, any uncertainty in the value of r0 makes this correction unimportant. The strain energy due to an edge dislocation is more easily calculated by a second method. Suppose that the dislocation is formed in initially unstrained material by making a cut from the surface of the material up to the site of the dislocation line, and then applying forces to the faces of the cut so as to give them a relative displacement of b. Then the work done by these forces equals the elastic energy stored around the completed dislocation. As the faces of the cut are displaced, the Burgers vector increases smoothly from zero to b. The work done in increasing the Burgers vector of unit length of dislocation from b to b + db is: dW = F ( β ) dβ

(9.3)

where F(b) is the force acting on one of the faces of the cut in the direction of b. This force is given by the stress field of the dislocation at the cut surface. For an edge dislocation which is made by cutting along the slip plane in a cylinder of radius R (Figure 9.1): F=

∫

R

r0

σ 12 dx1

(9.4)

The fact that only the stress on a single plane is involved gives this method an advantage over volume integration, when the stress field is complicated. From the forms of Equations 8.22, with x2 = 0 and the Burgers vector = b:

Kelly_c09.indd 270

11/30/2011 6:17:44 PM

Dislocations in Crystals

σ 12 =

μβ

2π (1 − ν )x1

271

(9.5)

and therefore: ⎛ R⎞ ln ⎜ ⎟ 2π (1 − ν ) ⎝ r0 ⎠ μβ

F=

(9.6)

The strain energy per unit length is then: E=W =

∫

b 0

F dβ =

⎛ R⎞ ln ⎜ ⎟ 4π (1 − ν ) ⎝ r0 ⎠ μb 2

(9.7)

In an isotropic medium, an edge dislocation has more elastic strain energy than a screw, in the ratio of 1:(1−n). For aluminium, n = 0.34 and so per unit length the edge dislocation has 1.5 times as much energy as the screw; for tungsten, n = 0.17 and the ratio is only 1.2. The strain due to a mixed dislocation, with a Burgers vector at an angle q to the dislocation line, is equal to the sum of the strains due to parallel edge and screw dislocations of Burgers vectors b sin q and b cos q, respectively. Therefore, the energy of a mixed dislocation is given by: E=

Kb2 ⎛ R ⎞ ln ⎜ ⎟ 4π ⎝ r0 ⎠

(9.8)

sin 2 θ + μ cos2 θ

(9.9)

where: K=

μ

1−ν

To estimate the absolute magnitude of the strain energy per unit length of dislocation line, it is sufficient to consider Equation 9.2: E=

⎛ R⎞ ln ⎜ ⎟ 4π ⎝ r0 ⎠

μb2

The difficulty in applying this equation is that the strain energy increases without limit as R increases. In a real crystal, either the surfaces of the crystal, or more probably other dislocations, will limit R. Fortunately, because of its logarithmic dependence on R, the magnitude of E is not very sensitive to the particular value of R which is assumed. For aluminium, which is approximately isotropic elastically, with m = 28 GPa, b = 2.86 × 10−10 m and an assumed r0 = b [1], the energy per unit length is 1.49 × 10−9 J m−1 when R is set at 1 μm, and 2.75 × 10−9 J m−1 when R is set at 1 mm. A value of 2 × 10−9 J m−1 corresponds to an energy per Å length of dislocation of 1.25 eV. This energy is large enough to ensure that a crystal containing a single dislocation is never in thermodynamic equilibrium. (Even at high temperatures the entropy introduced by a dislocation subtracts only a relatively

Kelly_c09.indd 271

11/30/2011 6:17:48 PM

272

Crystallography and Crystal Defects

b1

b3

b2

b1

q b2 b3

Figure 9.2

small amount from its energy, so that the free energy of a dislocated crystal of ordinary size is always greater than that of a perfect crystal.) To obtain the total energy of a dislocation, the energy stored within the dislocation core must be added to the energy given by Equation 9.8. The core energy can be roughly estimated in various ways, which agree in giving its order of magnitude as mb2/4p J m−1 [1,2]. For aluminium, this amounts to 0.1 eV per Å, considerably less than the energy stored outside the core. In a real crystal, the importance of the core energy lies less in its magnitude than in the variation of this magnitude as the dislocation glides through the crystal. If the core energy increases sharply as the dislocation moves from its position of minimum energy, its motion is strongly resisted (Section 8.5). It is always geometrically possible for two dislocations to combine to form a single dislocation, as shown in Figure 9.2. When this happens, the Burgers vector of the resultant dislocation, b3, is simply the vector sum of the Burgers vectors of the combining dislocations: b3 = b1 + b2

(9.10)

To determine whether such a reaction is energetically favourable, we must compare the energy of a crystal containing a dislocation of the Burgers vector b3 with that of a crystal containing two widely separated dislocations of the Burgers vectors b1 and b2. The former can be written as K3b32 and the latter as K1b12 + K2b22. Although it is evident from Equation 9.8 that the constants K1, K2 and K3 depend on the angles between the dislocation lines and their Burgers vectors, the difference between K3b32 and K1b12 + K2b22 is usually so large that the sign of K3b32 − (K1b12 + K2b22) is not affected by setting K1 = K2 = K3. Consequently, the sign of b32 − (b12 + b22) is a useful criterion for determining whether the reaction of two dislocations to form a third leads to a reduction in energy. Using this, a reduction will occur if: b32 < b12 + b22

Kelly_c09.indd 272

(9.11)

11/30/2011 6:17:55 PM

Dislocations in Crystals

273

This rapid test for deciding whether two dislocations will react is known as Frank’s rule [3]. It can also be expressed in terms of the angle q between b1 and b2 (Figure 9.2). If q < 90°, the dislocations will not react; if q > 90° they will attract and react with one another. The same rule can be applied in reverse to decide whether a dislocation of the Burgers vector b3 is stable. If two lattice vectors summing to b3 and making an angle q < 90° with each other are available, the dislocation will dissociate into two dislocations with these vectors as Burgers vectors. The rule is obviously most reliable when q is far from 90°. It follows from Frank’s rule that most dislocations other than those with the shortest lattice vector as the Burgers vector are unstable. For example, a dislocation with a Burgers vector 12 211 in a c.c.p. crystal would decompose into two 12 011 dislocations: 1 [211] → 1 [110] + 1 [101] 2 2 2

(9.12)

However, it sometimes happens that a dislocation whose Burgers vector is greater than the least lattice vector cannot decompose spontaneously. An example is the [100] dislocation in a b.c.c. crystal. Although the 12 111 dislocation has a smaller energy, Frank’s rule predicts that the decomposition: [100] → 1 [11 1] + 1 [111] 2 2

(9.13)

will not occur, and that no other geometrically possible decomposition is favourable energetically. The Burgers vectors that are definitely stable in various lattices are listed in Table 9.1. Doubtful cases in which the vector is the sum of two orthogonal vectors (q = 90°) are omitted. The fact that the dislocation with the smallest Burgers vector has the least elastic energy fits in well with the observation that the slip direction is almost always that of the shortest lattice translation vector in the crystal (Table 7.1). It is natural to enquire whether the observed slip planes are those on which a dislocation of minimum Burgers vector has the smallest elastic energy, when the elastic anisotropy of the crystal is taken into account. The elastic energy per unit length for an undissociated dislocation in an anisotropic medium is given by: E=

K ′b2 ⎛ R ⎞ ln ⎜ ⎟ 4π ⎝ r0 ⎠

(9.14)

where K′ depends on the elastic constants. Foreman has computed the energy factor K′ in a number of cases [4]. In copper, for example, an edge dislocation of the 12 110 Burgers vector has a lower elastic energy when it lies in a {110} plane (K′ = 64.5 GPa) than when it lies in a {111} plane (K′ = 74.5 GPa). Since the observed slip plane is {111}, it appears that the elastic energy alone does not determine which slip plane operates. In order to understand the choice of slip plane it is evidently necessary to take account of the atomic structure of the crystal (see also Section 7.1).

Kelly_c09.indd 273

11/30/2011 6:17:57 PM

274

Crystallography and Crystal Defects

Table 9.1

Definitely stable dislocations in some Bravais lattices

Lattice

Burgers vector

Number of equivalent vectors

Square of Burgers vector

Simple cubic

〈100〉

6

a2

B.c.c.

1 111 2 〈100〉

8

3a2/4

6

a2

C.c.p. Hexagonal

1 110 2 1 1120 3 〈0001〉

12

a2/2

6

a2

2

c2

6

a2

〈100〉 – 〈110〉 – 〈111〉

6

4a2 sin2 a/2

6

a2(1 + 4 sin2 a/2)

〈100〉

6

a2

〈110〉

6

4a2 cos2 a/2

〈111〉

2

9a2(1− 4 sin2 α / 2)

Simple tetragonal

〈100〉

4

a2

2

c2

Body-centred tetragonal

〈001〉 1 111 2

8

a2/2 + c2/4

〈100〉

4

a2

〈001〉

2

c2

1 111 2 〈100〉

8

a2/2 + c2/4

4

a2

Rhombohedral a < 90° Rhombohedral a > 90°

c/a < 2

Body-centred tetragonal c/a > 2

3

The fact that a dislocation line has a certain amount of energy per unit length associated with it causes it to try to shorten itself, or in other words, it gives it a line tension. It is not easy to define this line tension precisely because the energy is not concentrated at the line itself but is contained in its far-reaching strain field. Let us consider the tendency of a circular dislocation loop of radius r to shrink. To prevent it from shrinking, a radial force Fr per unit length must be applied, given by the condition that the energy change accompanying an infinitesimal contraction of the loop must vanish. Therefore: Fr 2π r dr = E 2π dr

(9.15)

or: Fr =

Kelly_c09.indd 274

E r

11/30/2011 6:18:06 PM

Dislocations in Crystals

275

T

Fr rdq π dq 2 2

r

dq T

Figure 9.3

where E is the energy per unit length of the dislocation loop. Since the strains due to the opposite sides of the loop cancel one another at distances that are large compared to r, we can determine E approximately by setting R = r in Equation 9.2: E≈

⎛r⎞ ln ⎜ ⎟ 4π ⎝ r0 ⎠

μb2

(9.16)

If we consider a small segment of the loop, shown in Figure 9.3, subtending an angle dq at the centre of the loop, we see that to keep this segment in equilibrium its ends must experience a tension T given by setting the sum of radial forces equal to zero: 2T sin

dθ = Fr r dθ 2

(9.17)

Since dq is very small, we therefore have from Equations 9.15 and 9.17: T =E

(9.18)

We may extend this result with the aid of Equation 9.16 to say that the line tension of a dislocation bowed to a radius of curvature r is approximately: T≈

⎛ ρ⎞ ln ⎜ ⎟ 4π ⎝ r0 ⎠

μb2

(9.19)

With r ≈ 500r0, substitution into Equation 9.19 gives the value of T ≈ 0.5 μb2, which is often used as the value of the line tension of a dislocation in rough calculations. A diagram which helps in the calculation of the stress needed to extrude a dislocation between obstacles a distance l apart is shown in Figure 9.4. The radial force on the dislocation is supplied by a shear stress t on the slip plane, parallel to the Burgers vector. From Equation 8.4: Fr = τ b

Kelly_c09.indd 275

(9.20)

11/30/2011 6:18:17 PM

276

Crystallography and Crystal Defects

Fr

l

r

Figure 9.4

Using Equations 9.15 and 9.18, if the radius of curvature of the dislocation line is r: τ=

T bρ

(9.21)

or, setting T = 0.5 mb2: τ=

0.5 μb

ρ

(9.22)

Since the minimum value of r is 0.51, occurring when the dislocation has been bowed out to a semicircle, the stress required to force the dislocation between the obstacles is given by: τ≈

μb l

(9.23)

It is apparent from this equation that this is also the shear stress needed to operate a Frank– Read source whose pinning points are a distance l apart. An interesting improvement to Equation 9.19 can easily be made by allowing for the fact that the strain energy of a dislocation varies with the angle q between its line and its Burgers vector. (For an isotropic medium, this variation is given by Equation 9.9.) As a consequence, if the equilibrium of an isolated segment of dislocation is considered, not only must a force E be applied to its ends to stop it shrinking, but also a couple Γ per unit length must be applied to it to stop it turning into an orientation of lower energy. The value of Γ is found by considering an infinitesimal rotation dq of the segment from its equilibrium position. Setting the energy change equal to zero: Γ dθ − dE = 0

or: Γ=

dE dθ

(9.24)

As the dislocation curves through the infinitesimal angle dq, the couple per unit length acting upon it changes by (d2E/dq 2)dq. This results in unbalanced radial forces acting on

Kelly_c09.indd 276

11/30/2011 6:18:24 PM

Dislocations in Crystals

277

dE – d2E dq dq dq 2 2

Fr dS

E dS r

E

dE + d2E dq dq dq 2 2

dq

q

Figure 9.5

the ends of a curved segment of length dS, as shown by Figure 9.5. The total radial force per unit length needed to keep the dislocation bowed out is now given by: Fr dS = E dθ +

d2 E dθ 2

dθ

or: Fr =

E ρ

+

1 d2 E ρ dθ 2

(9.25)

If the line tension T is defined by the equation: Fr =

T ρ

(9.26)

then, from Equation 9.25, T is given by: T=E+

d2 E dθ 2

(9.27)

Substitution of Equation 9.9 into Equation 9.27 shows that a screw dislocation in an isotropic material is much stiffer than an edge, even though the edge has the greater elastic energy. Physically, this is because in order to bend a screw dislocation, it must be given some edge character, of relatively high energy. In aluminium, which as we have already noted is approximately isotropic elastically, n = 0.34, so that the screw dislocation is four times as stiff as the edge.

9.2

Stacking Faults and Partial Dislocations

So far, it has been assumed that the smallest Burgers vector that a crystal dislocation may possess is the shortest lattice vector. Although such a dislocation could reduce the elastic strain energy by dissociating into two dislocations with smaller Burgers vectors, this would

Kelly_c09.indd 277

11/30/2011 6:18:30 PM

278

Crystallography and Crystal Defects

create a fault in the crystal structure, which, in general, would have a high energy. In certain special cases, however, the fault has a rather small energy. When this is so, the dislocation does indeed dissociate into two dislocations, called partial dislocations or, briefly, partials, which leave a planar fault between them as they move apart. The mutual repulsion of the partials due to their stress fields decreases as the partials separate, but the attractive force exerted by the surface tension of the fault remains constant. An equilibrium separation is therefore reached at which the forces of repulsion and attraction balance. It is now well established that 〈110〉 dislocations in c.c.p. metals dissociate into partials on the {111} slip plane. The fault that lies between the partials is a fault in the stacking sequence of the {111} planes, which does not change the relative positions of atoms that are nearest neighbours of one another. The production of this stacking fault can best be visualized with the aid of sheets of closely packed balls, stacked one on top of another (Section 3.2). By sliding an upper block of sheets through a/6 〈211〉 over those underneath, the so-called intrinsic stacking fault is produced (Figure 9.6). For example, if the second ABC block in the sequence ABC ABC is slid over the first, the sequence becomes ABCBCA… The sheets at the fault are now in the sequence BCBC, which, if continued, produces a close-packed hexagonal structure. Such a fault occurs when the 12 110 dislocation dissociates into 61 211 dislocations, which are called Shockley partials or Heidenreich–Shockley partials [5]: − − − 1 [011] → 1 [112] + 1 [1 21] 2 6 6

(9.28)

for dissociation of the 12 [01 1] dislocation on the (111) plane. The pattern of atoms at the (111) slip plane around a 12 [01 1] 60° dislocation that has dissociated into Shockley partials is shown in Figure 9.6. (For simplicity in drawing, the partials are shown to be very narrow; in a real crystal they would be wider.) The separation of the Shockley partials is determined by the energy per unit area, g , of the stacking fault between them. The fault draws the partials together with a force g per unit length, so that the equilibrium separation r is given by: G =γ r

(9.29)

where the elastic repulsion factor G can be calculated. Assuming isotropic elasticity, the screw component of the first partial, b1 cos q1, gives a shear stress on the slip plane: σ 23 =

μb1 cos θ1

2π r

(9.30)

where Ox2 is normal to the slip plane, Ox3 is parallel to the dislocations and q1 is the angle between the partial dislocation line and its Burgers vector. From Equations 8.22, the edge component gives the stress: σ 12 =

Kelly_c09.indd 278

μb1 sin θ1 2π (1 − v)r

(9.31)

11/30/2011 6:18:35 PM

Dislocations in Crystals

B

B

B

B

C

B

B

B

1 [121] 6 1 [211] 6

1 2 [011]

l

Figure 9.6 partials

B

B

B

C

C

C

B

C

C

B

B

279

1 b1 = 6 [112]

l

b2 = 16 [121]

Dislocation on a (111) plane of a c.c.p. metal which has split into two Shockley

The component of the traction on the slip plane in the direction of the Burgers vector of the second partial is given by:1 τ = σ 23 cos θ 2 + σ 12 sin θ 2

(9.32)

Since, by Section 8.3, G = t b2, it follows that: G=

μb1b2 ⎛ sin θ1 sin θ 2 ⎞ cos θ1 cos θ 2 + ⎜ ⎟⎠ 2π ⎝ 1−ν

(9.33)

The substitution of typical values for the constants in Equation 9.33 shows that a relatively wide separation of the partials of the order of 100 Å occurs only when the stacking fault energy is as low as 10 mJ m−2. Most c.c.p. metals and alloys have a higher stacking fault energy than this, so the separation of partials will only be seen in the transmission electron microscope using weak beam imaging conditions [6]. The remaining sections of this chapter are devoted to the study of dislocations in specific crystal structures.

1 Care must be taken to measure q1 and q2, the angles between the partial dislocation lines and their Burgers vectors, in the same sense.

Kelly_c09.indd 279

11/30/2011 6:18:44 PM

280

Crystallography and Crystal Defects

9.3

Dislocations in C.C.P. Metals

The 〈110〉 slip direction of c.c.p. metals is easy to understand, because 12 110 is the shortest lattice vector. The {111} slip plane is the plane on which a ‘perfect’ dislocation with a 1 110 Burgers vector may split into two Shockley partial dislocations, as described in 2 Section 9.2. The equilibrium separation of the two partials is determined by the energy of the stacking fault between them. The lower the stacking fault energy, the wider the split and the more rigorously should slip be confined to a particular {111} plane. The stacking fault energy is therefore a property of great physical importance as it determines the propensity of materials to twin and to cross-slip; unfortunately, it is also very difficult to measure accurately. Various values are listed in Table 9.2. The production of a stacking fault during slip is effectively illustrated by a rigid ball model, such as that shown in Figure 9.6. In this model, the slip path that requires the least ‘riding up’ of the balls follows a zigzag route along the valleys in the {111} surface, in two alternating 〈112〉 directions. The displacements along 〈112〉 alternately create and remove a stacking fault. From inspection of this model, one might wrongly conclude that only one type of stacking fault could occur on {111}. In particular, the stacking fault that would be obtained by interchanging the positions of the two partials in Figure 9.6 appears at first to be impossible, since it seems to involve A–A stacking, with a large ride-up of the balls when the leading dislocation advances. However, this conclusion can be modified if the necessary displacements are spread over two successive {111} planes. For example, at the position of the dislocation on the left of Figure 9.6, starting with a perfect crystal, a displacement 61 [211] of all the balls above the bottom {111} layer to the right of this position, followed by a displacement 61 [121] of all the balls above the next {111} layer, produces a net 61 [1 1 2] displacement without violating nearest-neighbour relationships. Formally, the partial dislocation then consists of two Shockley partials, 61 [2 1 1] and 61 [1 21] , on adjacent planes, but except at its core the dislocation cannot be distinguished from a single 1 [112] Shockley partial. 6 Therefore, by spreading the displacements over two planes, the 61 [112] Shockley partial can be made the leading partial for glide from left to right in Figure 9.6. When an interchange of the order of the partials is accomplished in this way, they are separated by a ‘double’ stacking fault, which is called an extrinsic fault. The energy of this fault is expected to be slightly higher than that of the intrinsic (single) fault. Consequently, the form of splitting shown in Figure 9.6 is believed to be the usual one. The distinction between the structures of intrinsic and extrinsic stacking faults can be neatly displayed by a notation due to Frank [12]. When a close-packed plane is stacked upon the plane beneath according to a pair in the sequence ABC…, the stacking of that plane is depicted by a triangle Δ. When a plane is stacked so that its relation to the plane beneath it is a pair in the reverse sequence BAC…, its stacking is then depicted by an inverted triangle ∇ (pronounced nabla). These symbols are derived from the stacking of balls – they represent the orientation of the triangles of balls onto which the balls in the next layer are stacked. The c.c.p. structure is then shown as ΔΔΔΔ and the h.c.p. structure as Δ∇Δ∇ … The intrinsic stacking fault is ΔΔ∇ΔΔΔ, while the extrinsic stacking fault is

Kelly_c09.indd 280

11/30/2011 6:18:47 PM

Dislocations in Crystals

281

Table 9.2 The stacking fault energies of c.c.p. metals Metal Ag Al Au Cu Ni

(a)

Stacking fault energy (mJ m−2)

Ref.

16 135 32 41 120–130

[7] [8] [9] [7,10] [11]

(b) C

C

B

B

A C B

A B

B A C B

A

A

A

C

C

C

B A C A B A C

Figure 9.7 (a) Faulted vacancy loop in a c.c.p. metal, showing traces of the (111) planes in a plane normal to the loop. (b) Extra atom loop

ΔΔ∇∇ΔΔ, emphasizing that the extrinsic fault is equivalent to two intrinsic faults on adjacent planes. It is possible to produce stacking faults by means other than slip on the close-packed plane. An intrinsic stacking fault is produced by removing part of a {111} layer of atoms, as shown in Figure 9.7a, provided that the gap is then closed directly, without any shear parallel to the {111} plane. Physically, this may happen when excess vacancies collect together on a {111} plane. Squeezing in a piece of an extra {111} layer creates an extrinsic fault, as shown in Figure 9.7b. The faults shown in Figure 9.7 are both bounded by partial dislocations whose Burgers vectors are normal to the {111} plane and are of the magnitude of the spacing of these planes; that is, 13 111 . In distinction from Shockley partials, these partials could glide only on surfaces that are normal to the usual {111} slip plane; if they did so they would leave a high-energy stacking fault behind them. They are called Frank partials or, because of their immobility, Frank sessiles. Although a stacking fault must be bounded by a partial dislocation, or end at a surface, it is now clear that the Burgers vector of the partial is not uniquely determined by the type of fault. In a given case, any lattice vector may be added to the Burgers vector of the partial without affecting the fault. For example, an intrinsic fault on (111) bounded by a

Kelly_c09.indd 281

11/30/2011 6:18:57 PM

282

Crystallography and Crystal Defects (a)

[001]

D

(b)

A C

D

b A

C B

[010]

d g

a [100]

D

B

D

Figure 9.8 Thompson’s tetrahedron. (After Thompson [13]. Reproduced by permission of the Institute of Physics and Physical Society.)

1 [11 2] 6 1 [2 11] 6

Shockley partial might equally well be bounded by two other Shockley partials, or 61 [121] . Thus: − 1 [ −211] = 1 [112] + 6 6 − − 1 [121] = 1 [112] + 6 6

− 1 [101] 2 − 1 [011] 2

(9.34) (9.35)

or, by the Frank partial with the Burgers vector 13 [1− −− 1 1] : −− − 1 1 [1 1 −− 3 1 1] = 6 [112] + 2 [1 1 0]

(9.36)

Before going on to consider reactions between dislocations in c.c.p. metal crystals, it will be helpful to introduce a device known as Thompson’s tetrahedron [13]. This gives a picture of various Burgers vectors in relation to the four {111} planes, which can be chosen to form the four faces of a tetrahedron. This tetrahedron and its relation to the crystal structure is shown in Figure 9.8a; the four faces of the tetrahedron, when they are opened out from the vertex D, are shown in Figure 9.8b. The lettering of the various points is conventional and follows Thompson’s original paper.2 An edge of the tetrahedron, such as CB, represents the Burgers vector of a perfect dislocation, 12 110 . Vectors given by Greek–Roman letter combinations such as d C represent Shockley partials, except when the Greek and Roman letters are in the same position in their respective alphabets, such as g C, which indicates a Frank partial.

2

Kelly_c09.indd 282

An alternative convention would be to letter the tetrahedron as the mirror image of Figure 9.8a.

11/30/2011 6:18:59 PM

Dislocations in Crystals

283

D

1 – [110] 2 Perfect

1 – [111] 3 Frank

d

1 – [112] 6 Shockley

B

Figure 9.9

The reaction between a Frank partial, a Shockley partial and a perfect dislocation given by Equation 9.36 becomes, in Thompson’s notation: δ D = δ B + BD

The relationship between these three Burgers vectors is shown in Figure 9.9. This reaction has some interesting applications. The stacking fault within the ‘vacancy loop’ of Figure 9.7a can be removed if the Frank dislocation decomposes according to Equation 9.36 and if then its Shockley component shrinks to nothing by gliding in the plane of the loop. This removes the stacking fault at the expense of an increase in elastic energy due to the − −− increase in the Burgers vector of the loop from 13 [1 1 1] to 12 [1 1 0] . In comparing the energies of faulted and unfaulted loops, allowance must be made for the shortening of the –– unfaulted loop when it glides into a (1 1 0) orientation normal to its Burgers vector. The unfaulted loop is favoured when the stacking fault energy is high and also when the loop is large, because the energy gained by destroying the fault is proportional to the area of the unfaulted region, whereas the extra elastic energy is approximately proportional to its perimeter. Another application is to the possible dissociation of a perfect dislocation into a Shockley partial and a Frank partial: BD → Bδ + δ D For example: 1 [1 10] → 1 [1 12] + 1 [1 1 1] 2 3 6

Kelly_c09.indd 283

(9.37)

11/30/2011 6:19:08 PM

284

Crystallography and Crystal Defects

l

l

Cd

dB

Figure 9.10

Since the Burgers vectors of these two partials are orthogonal, and since a stacking fault would have to be created between them, this dissociation does not ordinarily occur. It may occur in special cases, as when the Shockley components from the two members of a perfect dislocation dipole can annihilate one another, leaving behind a Frank dipole. This reaction is simply the reverse of the unfaulting of a prismatic loop described above. In order to define the sense of the Burgers vector of a dislocation, when it is written in Thompson’s notation it is necessary to introduce a convention that will assign a sense to the slip displacement signified by the symbol d C, for instance. The following convention can be used. The sense of the slip displacement signified by d C is defined as follows. The observer looks at the slip plane ABC from outside the tetrahedron; that is, with the apex D pointing away from him or her (Figure 9.8a). Then the atoms above the slip plane ABC closest to the observer are displaced by d C. Referring to the crystal structure, it is clear that the displacements dA, d B and d C produce an intrinsic stacking fault, whereas Ad, Bd and Cd produce an extrinsic fault. The dissociation of the perfect dislocation CB into Shockley partials on ABC can be written as: CB → Cδ + δ B

(9.38)

The Burgers vectors of the partials in the Thompson notation are then as shown in Figure 9.10, according to the FS/RH convention. (The line vectors have been chosen to run down the page, so that the observer looks in the negative line direction, in order to match the figure with the logical form of Equation 9.38.) Reversing the order of the partials would produce an extrinsic fault between them. The order of the Shockley partials is an important factor in dislocation reactions. The only reaction between perfect dislocations that definitely leads to a reduction in energy is of the type: CB + BA → CA

Kelly_c09.indd 284

(9.39)

11/30/2011 6:19:15 PM

Dislocations in Crystals (a)

p CB

BA q

(b)

(c) BA

CB

BA

CB

r

CA

CB

BA

BA

CB

CB BA

s

285

BA

CB

Figure 9.11 Reaction of two dislocations on a common slip plane. The dislocations are assumed to be pinned at the points p, q, r and s

Bd

dB

dA

Cd

Cd

l

dA

dB

Bd dA

Figure 9.12

Cd

Same reaction as Figure 9.11 but showing splitting into partials

If the dislocations of Burgers vectors BA and CB meet on their common slip plane, they will react over a certain length, forming two nodes (Figure 9.11). It is apparent from a consideration of Figure 9.12 that the nodes will have different structures, because of the sequence of the Shockley partials (it is assumed that only intrinsic faults occur). Alternate expanded and contracted nodes have been seen, in stainless steel, for example [14]. The same reaction (9.39) can also occur when the dislocations are on different slip planes. For example, suppose that dislocations CB and BA lie on the planes opposite vertices A and C respectively, and let their lines lie parallel to the intersection of these planes, BD, as they glide towards one another. This event is likely to occur during the later stages of the tensile deformation of a crystal, because it corresponds to the intersection of primary and conjugate slip (Section 7.4). If the two dislocations on the {111} planes are dissociated into Shockley partials, as shown in Figure 9.13, and if they come together in such a way that just before they meet their stacking faults make an acute angle (cos−1(1/3) = 70.53°) with one another, the leading partials aB and Bg will react to form a new partial along BD:

Kelly_c09.indd 285

11/30/2011 6:19:17 PM

286

Crystallography and Crystal Defects (a)

(b)

D

plane CBD

plane ABD

Ca

gA

b A

C d g

a D

Ca 1

aB

B

D

gA Bg

1

ag

Figure 9.13 Lomer–Cottrell lock

α B + Bγ → αγ

1 [1 2 1] + 1 [2 1 1] → 1 [1 1 0] 6 6 6

(9.40)

The edge dislocation ag is called a stair-rod, a name suggested to Thompson by Nabarro (quoted by Thompson in a footnote in [13]), from the way in which it joins two stacking faults at a bend rather like a stair rod holding down a stair carpet. The whole configuration is called either a Lomer–Cottrell lock or a Cottrell–Lomer lock [15,16]; here, we shall adopt the former terminology. Since it cannot glide, it is an important obstacle to other dislocations. The stair-rod dislocation of the type ag can also be produced by the dissociation of a Frank partial: α A → αγ + γ A

1 [1 11] → 1 [1 1 0] + 1 [1 1 2] 3 6 6

(9.41)

This reaction makes it possible to understand the small tetrahedra of stacking faults that can be produced experimentally by quenching gold from near its melting point to room temperature, and then ageing at 100 °C [17].3 Imagine that the excess vacancies which are trapped by the quench first form a Frank loop similar to that shown in Figure 9.7a. Let the loop be a triangle, with sides along the 〈110〉 directions AB, BC, CA. Each side can then dissociate on a different {111} plane, as shown in Figure 9.14. The Shockley dislocations produced by the dissociations attract one another and react at the intersections of the {111} planes to form stair-rod dislocations. The final product is a tetrahedron whose faces are intrinsic stacking faults and whose edges are stair-rod dislocations. Each edge of the tetrahedron is exactly like the corner of a Lomer–Cottrell lock. The formation of the tetrahedron decreases the elastic energy at the expense of additional stacking fault energy.

3 Ageing means holding at a constant temperature for a period of time, usually in order to allow some change in the structure of the material to occur.

Kelly_c09.indd 286

11/30/2011 6:19:18 PM

Dislocations in Crystals (a)

(b)

D

287

D

ag bγ gD

B aD

B A

bD

da

l

db

C

Figure 9.14

A

ab

da db

l

dg

dg

C

Formation of a stacking fault tetrahedron from a Frank vacancy loop

Ba

Ab ab/ DC

Figure 9.15

Hirth lock

The 61 110 dislocation is one of four possible stable stair rods. Other dislocations at an acute-angle bend can be derived by adding lattice vectors to 61 [110] . The only resultant which is stable, according to Frank’s rule, is 13 [1 1 0] , formed by adding 12 [1 1 0] . One of the interesting occurrences that would produce an obtuse-angle stacking fault bend is the reaction of the leading partials of the dislocations BD on the plane opposite the vertex A and AC on the plane opposite the vertex B: BD → Bα + α D AC → Aβ + β C

(9.42)

1 [2 1 1] + 1 [2 11] → 1 [0 1 0] 3 6 6

(9.43)

The resulting configuration, shown in Figure 9.15, is called the Hirth lock [18,19], even though, as Nabarro [20] notes in his book on p. 220, it appears in a tabulation given by Friedel [21]. In Thompson’s notation, Equation 9.43 may be written as: α D + β C → αβ /DC

Kelly_c09.indd 287

(9.44)

11/30/2011 6:19:20 PM

288

Crystallography and Crystal Defects Table 9.3

Dislocations in c.c.p. metals Burgers vector b

Name of dislocation Indices

Relative b2

Thompson notation

Perfect

1 110 2

AB

1

Shockley

1 211 6

Ad

1 3

Frank

1 110 3

Aa

2 3

Thompson stair-rod

1 6 1 3 1 3 1 6

110

ad

110

—

100

da/CB

310

—

1 9 4 9 2 9 5 9

Acute stair-rod Obtuse stair-rod Obtuse stair-rod

The 13 0 1 0 vector denoted by ab/DC is in the direction of the line joining the point bisecting ab to the point bisecting DC and has twice the magnitude of this line. Some of the properties of dislocations in c.c.p. metals are summarized in Table 9.3.

9.4

Dislocations in the Rock Salt Structure

The dislocations that have been identified in crystals of the rock salt (NaCl) structure have a 12 110 Burgers vector, as would be expected (Table 9.1). The slip plane is usually {110}, but not always (Table 7.1). When slip on {110} is examined, it is impossible to find a stacking fault that looks as though it might have a low energy and could serve as the halfway stage of an indirect 1 110 displacement. Therefore, the 12 110 dislocation is not expected to split into 2 – partials on {110}. The fact that only perfect dislocations need be considered greatly simplifies the analysis of dislocation reactions. The relationship between the 〈110〉 Burgers – vectors and the {11 0} slip planes is shown in Figure 9.16, which may be compared with Thompson’s tetrahedron. A consideration of this figure confirms that, as expected from the crystallography, each Burgers vector lies in only one slip plane (e.g. AC lies in OAC only) and each slip plane contains only one Burgers vector (OAC contains only AC). This one-toone correspondence contrasts with the slip systems of the c.c.p. metals, and still further simplifies the study of dislocation interactions. In fact, there is only one dislocation reaction to consider – that between dislocations on planes at 60° to one another: AB + BC → AC ⎫⎪ 1 [101] + 1 [011] → 1 [110] ⎬ ⎪⎭ 2 2 2

Kelly_c09.indd 288

(9.45)

11/30/2011 6:19:29 PM

Dislocations in Crystals

289

B

E G

O

D H

A F

C

– – Figure 9.16 Relation between slip planes and directions in {110}〈110〉 or {110}〈111〉 slip. The point O lies at the centre of the tetrahedron ABCD whose edges are parallel to 〈110〉. The planes OAB, OAC and so on are {110} and the directions OA, OB, OC, OD are 〈111〉

If the reacting dislocations AB and BC are confined to their slip planes, (101) and (011) respectively, the resultant AC is laid down along the line of intersection of the slip planes, – OB, [111]. Hence, the glide plane of the resultant AC is (112), and for this reason it is very immobile at low temperatures. In LiF at room temperature, the dislocations on one plane will block slip on another which intersects it at 60° so efficiently that, after 1% shear strain in single slip, a resolved shear stress of about 15 times that which was needed to activate the first system must be put upon the intersecting system in order to bring it into operation [22]. Although less complex in their interactions than dislocations in c.c.p. metals, dislocations in crystals with the rock salt structure do have a property of special interest – they can carry an electric charge. The edge dislocation on {110} has an ‘extra plane’ consisting of a sheet of Na+ ions and a sheet of Cl− ions (Figure 9.17). This sheet of NaCl ‘molecules’ has been isolated in Figure 9.18. Its edge defines the dislocation line, which has a number of jogs in it. At A, an extra anion defines two jogs. The section BC has a net charge of + e; therefore the jogs at B and C are each assigned a charge of + e/2. The ‘whole’ jog at D is uncharged. This is the type of jog which is produced by intersection with an orthogonal screw dislocation; charged jogs of types B and C may be called half-jogs or, because they are produced when a single ion jumps on to or off the edge of the extra plane, diffusional jogs. It is apparent that the line as a whole can be charged, up to a maximum of e/2 per atom length. Physically, a line may become charged by acting as a source or sink for vacancies (Section 10.1). For example, because the energy needed to make a single cation vacancy is less than that needed to make an anion vacancy in NaCl, either a surface or an edge dislocation raised to a high temperature will generate excess cation vacancies which can diffuse into the crystal until their emission is throttled by the electric field that is built up as a consequence of the resultant space charge [23,24]. Relative to the adjacent crystal, the dislocation or surface acquires a positive charge, which is balanced by the nearby vacant

Kelly_c09.indd 289

11/30/2011 6:19:50 PM

290

Crystallography and Crystal Defects

+

+

+ –

–

–

–

+

+

+

–

–

–

–

+

+ –

+

–

[110] –

+

[110]

+ –

–

–

Figure 9.17 Edge dislocation in NaCl. The slip plane and the two sheets of ions constituting the extra plane are shown dotted

– +

+ –

– + – A

+ –

–

+

–

+

+

–

+

–

+

–

+

B

C

–

+

–

+

–

+

+

–

+

–

[001] D

[110]

Figure 9.18

cation sites in the crystal. On the other hand, a dislocation in an impure crystal of NaCl can acquire a negative charge in order to compensate, partly, for the extra positive charge carried by divalent impurity cations, such as Ca2+, by acting as a sink at which excess cation vacancies caused by the impurity cations can condense [23,24]. At low temperatures the effect of relatively low p.p.m. levels of impurities will predominate over the equilibrium properties that the dislocation would have in a pure crystal.

9.5

Dislocations in Hexagonal Metals

By analogy with c.c.p. metals, the slip plane of hexagonal metals should be the closestpacked basal plane (0001), the Burgers vector of a slip dislocation should be the a vector of the hexagonal lattice, 13 [112 0] , and, furthermore, this dislocation may be expected to split into two 13 10 10 partials, the analogues of Shockley partials. However, the analogy is certainly incomplete, because other slip planes, and another slip direction, sometimes operate (Table 7.2). With this reservation in mind, we will first examine dislocations on the basal plane, produced by slip and by the aggregation of point defects. – Since the three 〈112 0〉 slip vectors are coplanar, reaction between slip dislocations can only form a network of dislocations in the basal plane. Written in the notation of Figure 9.19, the reaction is:

Kelly_c09.indd 290

11/30/2011 6:19:50 PM

Dislocations in Crystals (a)

291

(b) – – a2 [1210]

S C s

B

A

a3 –– [1120]

C

B S

A –– a1 [2110] In plane

Above plane

Figure 9.19 Atoms and lattice vectors in a hexagonal metal

AB + BC → AC ⎫⎪ 1 [12 10] + 1 [1 120] → 1 [2110] ⎬ ⎪⎭ 3 3 3

(9.46)

The splitting of a perfect dislocation can also be shown on Figure 9.19: AB → Aσ + σ B ⎫⎪ 1 [12 10] → 1 [1100] + 1 [01 10] ⎬ ⎪⎭ 3 3 3

(9.47)

Between the partials As and s B, which are analogous to Shockley partials, there is a small layer of c.c.p. stacking. The sequence ABABABA becomes ABACBCB, or in Frank’s notation, Δ∇Δ∇Δ∇ is changed to Δ∇∇∇Δ∇. The order of the partials on successive basal planes must alternate; that is, if it is As − s B on one plane it must be s B − As on the next. This is in contrast to the splitting of perfect dislocations in a c.c.p. metal, where the order of the Shockley partials must always be the same if the same type of stacking fault is to be produced. In metals of small c/a ratio, the 13 2110 dislocation slips quite easily on a prism plane, – {1010}, indicating that it is not widely split on the basal plane. Zirconium and titanium, for example, slip much more easily on prism planes than on the basal plane. It is interesting to note that the reaction AB + BC → AC between prism plane dislocations cannot produce a strong barrier, because the product, formed along the intersection of two of the prism planes, is always oriented so that it can glide on the third. The experimentally determined stacking fault energy of Co is relatively low, 27 ± 4 mJ m−2 at room temperature [25]. (Cobalt transforms to a c.c.p. structure at 420 °C – see

Kelly_c09.indd 291

11/30/2011 6:19:53 PM

292

Crystallography and Crystal Defects

(a) A

(b)

B

B

A B

A

A

A

C

B

B

B

A

C

A B

C

A B A

A

A

B

B

A B

A

A

A

C A

A B A

Figure 9.20 Two possible structures for a vacancy loop in a hexagonal metal

Section 12.3.) Stacking fault energies in other h.c.p. metals are generally regarded as being much higher (see for example [25–27]), consistent with 13 2110 dislocations not being widely split on the basal plane. As with c.c.p. metals, stacking faults can arise as a result of point defect condensation. Such a fault is different from the fault produced by the splitting of a 13 1120 dislocation. When a disc of vacancies collects on a basal plane, a prismatic dislocation loop forms at its perimeter. If the disc is one vacancy thick, and if A–A stacking is to be avoided, the loop may be faulted in one of two ways. Either a single basal layer or the whole crystal on one side of the loop must be sheared over by a vector of the As type. These alternatives are shown in Figure 9.20. In case (a), the single layer can be shifted from an A into a C position by passing As partials of opposite sign on either side of it. The Burgers vector of the prismatic dislocation remains 12 [0001] , s S in Figure 9.19b, at the cost of a stacking fault which is triple, in terms of the number of next-nearest-neighbour stacking violations. In case (b), a single As partial is passed, so that the loop encloses a single stacking fault, but its Burgers vector increases to AS, as follows: Aσ + σ S = AS ⎫⎪ 1 [1100] + 1 [0001] → 1 [2203] ⎬ ⎪⎭ 3 2 6

(9.48)

Similar reasoning applies to faulted loops produced by discs of extra atoms. There is clear experimental evidence for these vacancy loops in zinc [28]; such stacking faults should have a slightly smaller energy than the double fault produced by the splitting of a perfect slip dislocation. –– – A more surprising slip system is the {112 2} 〈112 3〉, called second-order pyramidal glide. This occurs in a number of h.c.p. metals, such as Zn, Cd, Mg and Be [29]. The remarkable feature is the large size of the slip vector, 13 1123 ; that is, c + a. Even more puzzling is the fact that this system operates, second only to basal slip, in zinc and cadmium, which have the largest c/a ratios. A slip plane and its slip vectors are shown in the hexagonal cell in Figure 9.21. Each slip plane contains one slip vector and each slip vector lies in one slip plane.

Kelly_c09.indd 292

11/30/2011 6:19:57 PM

Dislocations in Crystals

293

B s C A

– [1123]

–– (1122)

B′

–– – Figure 9.21 A {112 2} 〈1123〉 slip system

The relationship between the six slip planes and six Burgers vectors, by means of a surface analogous to that used to illustrate the rock salt slip systems (Figure 9.16), is shown in Figure 9.22. The slip vectors are A′B, A′C, B′C, B′A, C′A, C′B and their antiparallel counterparts; the six slip planes are represented by A′BσA′ for the slip vector A′B, and so on. In a review of deformation modes in h.c.p. metals, Yoo et al. [30] noted that little is known about the dislocation cores of the c + a dislocations apart from results obtained through atomistic simulation: there is a distinct lack of detailed experimental observations on dislocation interactions and their role in pyramidal slip. More recent work has confirmed this trend – while there have been improvements in the choice of atom potential to model c + a dislocations in h.c.p. metals [31], experimental observations of the pyramidal glide system in h.c.p. metals still remain few in number. In addition, as Hull and Bacon note [32], there seems to be a close relationship between the occurrence of –– – {112 2}〈112 3〉 slip and twinning (Chapter 11) in h.c.p. metals, which serves to complicate the situation. –– Possible dislocation reactions between c + a dislocations on {112 2} planes in this system can be dealt with easily by decomposing each 13 1123 vector into its c and a components. The c components either add or cancel; provided c > a, there is an increase in energy when they add and a decrease when they cancel, whatever the a components may be. There are three reactions, then, corresponding to the three possible combinations of the a components when the c components cancel. The reaction is least favourable energetically when the a components are alike:

Kelly_c09.indd 293

11/30/2011 6:20:03 PM

294

Crystallography and Crystal Defects C s

B

A

A′ C′′ B′

B′′ A′′ C′

Figure 9.22

–– – Relation between slip planes and directions in {112 2} 〈1123〉 slip

C ′ A + AB′ → C ′ B′ ⎫⎪ 1 [1 1 23] + 1 [1 123] → 2 [1 120] ⎬ ⎪⎭ 3 3 3

(9.49)

The product C′B′ is formed along the line As in the basal plane common to the two slip planes C′AσC′ and B′AσB′ and can immediately split into two perfect 13 [1 12 0] dislocations. The most favourable reaction is: C ′ A + BC ′ → BA ⎫⎪ 1 [1 123] + 1 [2 1 1 3] → 1 [1210] ⎬ ⎪⎭ 3 3 3

(9.50)

A consideration of Figure 9.22 shows that the product BA is formed along the line C′s common to C′AσC′ and C′BσC′, so that it is likely to be immobile and an obstacle to other dislocations. The result of the third reaction is less easy to see from Figure 9.22. The reaction is: C ′ A + BA ′ → C ′C ′′ ⎫⎪ 1 [1 123] + 1 [2113] → 1 [3030] ⎬ ⎪⎭ 3 3 3

(9.51)

The product C′C″ should split into two a dislocations, AC + BC, but since its line does not lie in the basal plane, these dislocations are also likely to be immobile. – It is also conceivable in principle that the 〈112 3〉 dislocation might itself split into partials of the type AS (Figure 9.19):

Kelly_c09.indd 294

11/30/2011 6:20:05 PM

Dislocations in Crystals

1 [1123] → 1 [0 2 2 3] + 1 [2 0 2 3] 3 6 6

295

(9.52)

However, there is no reason to assign a low energy to the fault, which would have to form – on {112 2}. Furthermore, 13 [112 3] screw dislocations in zinc and cadmium are observed to cross-slip frequently, which is evidence against such splitting. There are two reactions between a basal-plane dislocation and a second-order pyramidal dislocation. The first is simply a rearrangement of Reaction 9.50: C ′ A + AB → C ′ B ⎫⎪ 1 [1 123] + 1 [12 10] → 1 [2113] ⎬ ⎪⎭ 3 3 3

(9.53)

The product lies along As, out of its pyramidal slip plane C′ sB. Therefore it can act as a barrier. The second reaction is simply the annihilation of the a component of the pyramidal: C ′ A + A ′′C ′ → A ′′A ⎫⎪ 1 [1 123] + 1 [1120] → [0001] ⎬ ⎪⎭ 3 3

(9.54)

The extra plane of the product A″A consists of two basal layers of atoms. These may be thought of as tending to wedge open the basal plane, which is also a cleavage plane. In this respect the reaction is like that which produces the 〈100〉 dislocation in b.c.c. metals (Section 9.6).

9.6

Dislocations in B.C.C. Crystals

It is now well established that a slip dislocation in a b.c.c. metal has the expected Burgers vector 12 111 . The plane on which this dislocation prefers to glide is far less certain (Table 7.1). We shall first assume that slip occurs somewhat more easily on {110} than on – other planes in the 〈111〉 zone. The relationship between the 12 111 Burgers vectors and the {110} slip planes can be shown on the same diagram that was used for rock salt structures (Figure 9.16). It is evident from Figure 9.16 that any two different Burgers vectors meet either at 70.53° or at 109.47°. In the latter case the dislocations will react: OA + OC → EF ⎫⎪ 1 [111] + 1 [111] → [100] ⎬ ⎪⎭ 2 2

(9.55)

The character of the product dislocation depends on the slip planes of the reactants, because these determine the direction in which its line lies. If the reacting dislocations are on the same slip plane then the glide plane of the product will of course be this plane also. If they are on planes such as AOB and AOC, which intersect at 60° along a 〈111〉, then the product, formed along this line, will still be able to glide in a {110} plane. However, if the reacting

Kelly_c09.indd 295

11/30/2011 6:20:09 PM

296

Crystallography and Crystal Defects

dislocations are on orthogonal planes, such as AOD and COB, their product will lie along a 〈001〉 like GH in Figure 9.16. It is then an edge dislocation with a {100} glide plane. The extra plane of this dislocation is parallel to the usual cleavage plane of a b.c.c. crystal, and it has been suggested that the crystal may be cracked open for a short distance beneath the extra plane [33]. The fact that slip is not very rigorously confined to any one plane is strong evidence that the 12 111 dislocation is not split widely into partials, and that therefore stacking faults have a high energy. Nevertheless, it is possible to find plausible-looking stacking faults in a rigid-ball model of the structure. A ball model of the {110} planes is shown in Figure 9.23. The arrows starting at P point out the natural path in which to slide the balls of the upper layer over the lower. This corresponds to the dissociation: 1 [111] → 1 [011] + 1 [211] + 1 [011] 2 8 4 8

(9.56)

The fault which is formed on both sides of the 14 [211] dislocation occurs quite naturally in a rigid-ball structure, because it leads to closer packing (for this reason it may be important in the martensitic transformation of a b.c.c. to a h.c.p. structure – see Section 12.10). Thus, the 81 [011] which produces the fault drops the ball P from a saddle position into a valley. However, nearest-neighbour relationships are violated and the fault must ordinarily have a rather high energy, since it has never been detected in b.c.c. metals. Computer calculations using atomistic simulations have confirmed the high energy of faults in the b.c.c. crystal structure. For example, the early work of Vitek [34] using a simple central force potential and limited computer power showed that there are no stable intrinsic faults on either the {110} or the {112} planes in b.c.c. crystals. As Ventelon and Willaime [35] have recently noted, atomistic simulations of screw dislocations in b.c.c.

[011]

[100]

1 [111] 2

P

Figure 9.23

Kelly_c09.indd 296

11/30/2011 6:20:18 PM

Dislocations in Crystals

297

metals do not show splitting into well-defined partials and stacking faults, but instead reveal core configurations that are able to spread into the three {110} planes containing the zone axis of the screw dislocation. The power of such calculations highlights the limitations of further hard-sphere models showing splitting of 12 111 dislocations into partials separated by stacking faults on {110} and {211} planes, such as those considered in the first edition of this book [36]: such models are purely geometric in nature and therefore cannot predict the energies of the postulated stacking faults. By comparison, atomistic simulations are becoming increasingly sophisticated in terms of the choice of potential, even when they apply only to rigid dislocations at absolute zero; as Duesbery and Vitek argue [37], it is expected that results of such calculations will carry through, at least qualitatively, to conditions at finite temperature.

9.7

Dislocations in Some Covalent Solids

In crystals of diamond, Ge and Si, the atoms are held together by strong, directional covalent bonds (Figure 3.12). Dislocations in these crystals are immobile at low temperatures. This is because the Peierls stress is high; that is to say, the energy of the dislocation varies sharply with its position in the crystal. Extensive slip occurs only at elevated temperatures – above about 60% of the absolute melting temperature in Ge and Si. The slip plane – is then {111} and the slip direction 〈110〉. One can imagine the way in which glide might occur. The dislocation will lie, as much as it can, in a position of low energy, probably along some prominent crystallographic direction. It advances when, aided by thermal activation, a small length of line surmounts its energy barrier and spills over into the next energy trough (Figure 9.24). The connecting segment which is stranded on the energy hill is called a kink, distinguished from a jog by the fact that it lies wholly in the slip plane (Section 8.6). The kinks can glide apart relatively easily and, as they do so, the dislocation is advanced by the trough separation. The dislocation lying on a {111} plane at 60° to its Burgers vector, 12 1 10 , happens to – be easy to draw in projection on to a {101} plane normal to the dislocation; it is shown in this way in Figure 9.25. In this figure, which serves equally well for the sphalerite (zincblende) structure and for the diamond crystal structure, the small black dots represent a column of one atom species (e.g. Zn) and the encircled dots a second atom species (e.g. S); these two species are identical in the diamond crystal structure. Here, the dislocation line

Figure 9.24 Double kink in a dislocation line. The dotted lines represent positions of high energy for the dislocation

Kelly_c09.indd 297

11/30/2011 6:20:23 PM

298

Crystallography and Crystal Defects – [111]

[111] Type l Type ll

Figure 9.25 A 60° dislocation in sphalerite. The structure of a 60° dislocation in the diamond structure is identical, except that all the atoms are then the same

– – is along the vector common to (111) and (11 11) – that is, [101] – while the Burgers vector of the dislocation is 12 [01 1] . There are two possible {111} slip planes, type I and type II. The 60° dislocation in Figure 9.25 is shown with its extra plane ending at a type II plane, where it breaks the lower number of bonds. The one bond per atom which is broken is described as a dangling bond. Intuitively, it might seem that slip should occur at the widely spaced type II planes, by the glide of dislocations like that of Figure 9.25. However, this is before the possibility of splitting into partials is examined. There can be stacking faults on the {111} plane that do not violate tetrahedral bonding and are exactly analogous to intrinsic and extrinsic faults in c.c.p. metals. The stacking sequence of the perfect crystal can be written as a ab bc ga a… (see Sections 3.4 and 3.5). In this sequence, the diatom a − a can be treated as a unit, denoted by A. Type I planes separate sheets of diatoms packed in the c.c.p. sequence ABCA… An intrinsic fault is formed by passing a Shockley partial, 61 211 , over a type I plane; passing two different Shockley partials over successive type I planes produces the extrinsic fault. The 12 110 dislocation can split into partials on a type I plane: 1 [01 1] = 1 [112] + 1 [12 1] 2 6 6

(9.57)

so that one dislocation is a 30° partial and the other a 90° partial. Experimental evidence shows that moving dislocations are indeed split into partials in this way [38], with the 90° partials being more mobile than the 30° partials [39]. This set of partials is known as the

Kelly_c09.indd 298

11/30/2011 6:20:25 PM

Dislocations in Crystals

299

S [110] R

P Q

– [110]

O – [001]

Figure 9.26 Stacking fault in a silicon film. Point O lies at the bottom surface of the film and points P, Q, R and S at the top surface. OP, OQ, OR and OS are stair-rod dislocations

‘glide set’ of dislocations [2]. Partials dissociating on the alternative type II planes are termed the ‘shuffle set’ [2]; these have a more complicated geometry and are believed to be less mobile [2], although they may play an important role in low-temperature deformation [40]. A rich variety of stacking faults is found in Si films grown epitaxially from the vapour phase [41]. Faults originating at irregularities in the substrate grow along with the film, sometimes joined together as pieces of polyhedra. A schematic of a piece of an octahedral stacking fault in a film, which is parallel to {100}, is shown in Figure 9.26. The faces of the halfoctahedron are alternate intrinsic and extrinsic faults, joined by a 61 110 stair-rod dislocation. The configuration at a corner can be derived from the Lomer–Cottrell lock (Figure 9.13) by gliding one of the Shockleys of the lock to the other side of the stair-rod dislocation. An alternative tetrahedrally bonded structure is that of wurtzite, in which ZnS units are stacked in the hexagonal sequence ABA… Stacking faults in sphalerite consist of thin layers of the wurtzite structure. Similarly, stacking faults in wurtzite can occur which are thin layers of the sphalerite structure and are exactly analogous to stacking faults in a hexagonal metal. Dislocations in AlN, which has this structure, are widely split, the fault energy being only about 4 mJ m−2 [42]. Neither wurtzite nor sphalerite possesses a centre of symmetry, with the interesting consequence that the core structures of dislocations of opposite sign can be distinguished from one another in these structures. Suppose that an undissociated 60° dislocation in, say, GaAs, which has the sphalerite structure, always lies on a type II plane (Figure 9.25). Its extra plane then ends either on a Ga atom or on an As atom, according to whether it comes in from the top or the bottom of the crystal. Dislocations of opposite sign can therefore be labelled Ga and As dislocations, and because of their different core structures they may have quite different Peierls stresses. In this context, it is of interest to note that the set of (111) planes on which dislocations reside and move has been a topic of controversy since the 1960s in crystals with the sphalerite and diamond structures [40]. Tetrahedrally bounded crystals contain a three-dimensional network of strong bonds, but in many crystals the atoms are bonded together strongly only within layers which are themselves connected by relatively weak forces. Graphite is such a crystal. The dislocations and stacking faults on the basal plane of graphite are exactly analogous to those on the basal

Kelly_c09.indd 299

11/30/2011 6:20:30 PM

300

Crystallography and Crystal Defects – – [1210]

–– [1120]

C

B s

A –– [2110]

Figure 9.27 Atoms and lattice vectors in the basal plane of graphite

plane of a hexagonal metal. Figure 9.19b is applicable; its relationship to the structure of graphite is shown in Figure 9.27. Because of the weak interlayer bonding, the energies of the three basic types of stacking fault described in Section 9.5 are very small. One of these faults is produced by the dissociation of a perfect dislocation, as follows: AC → σ C + Aσ ⎫⎪ 1 [2110] → 1 [1010] + 1 [1100] ⎬ ⎪⎭ 3 3 3

(9.58)

By direct measurement of the separation of the 13 [10 10] partials, which are 1500 Å apart in the edge orientation and 800 Å apart in the screw orientation [43], the energy of the fault has been found to be only 0.5 mJ m−2. A schematic side view of a split 60° dislocation can be seen in Figure 9.28, showing the layer of rhombohedral stacking at the fault. Although slip dislocations are strictly confined to the basal planes in graphite, their reactions with one another are a little more complex than might at first be expected. The complexities are a result of the wide separation of the partials and of the fact that, because of this wide separation, the individual partials on nearby planes can, in effect, react with one another. As an example, consider a reaction between the dislocations AB and AC, which would simply repel one another if they were not split. Suppose that they lie on adjacent planes, so that if AB splits in the order A s + s B then AC must split in the order of s C + As. If the split dislocations are caused to approach, AB from the left and AC from the right, the partials s B and s C will come over one another and react: σ B + σ C → Aσ

(9.59)

The result is a stable double ribbon, shown in Figure 9.29.

Kelly_c09.indd 300

11/30/2011 6:20:31 PM

Dislocations in Crystals b

c

b

301

[0001] b

a

a

b

c

b

a

a

a

b

b

b

a

a

– [1100]

a

In plane Above plane

Figure 9.28

b

c

a

b

b a b

As

c a b

a sC sB

b

c b

a As

b

a

a

b

b

As

As

As

Figure 9.29

9.8

Dislocations in Other Crystal Structures

The detailed analysis of the geometry of dislocations, which has been carried out up to this point for a number of specific crystal structures, could be repeated for many other crystal structures. It is hoped that the principles employed have now been demonstrated sufficiently that the reader is able to deal with any case that may be encountered in metals, ceramics, semiconductors, mesomorphic phases, quasicrystals and superlattice structures.

Problems –– 9.1 In a b.c.c. metal, two dislocations of the Burgers vector [111] and [11 1] respectively have reacted over a certain length (as in Figure 9.11). If the reacting dislocations are pinned at points p, q, r and s, which lie at the corners of a square of side L, make an estimate of the length of the product dislocation (neglect the variation of the energy of a dislocation with the orientation of its line).

Kelly_c09.indd 301

11/30/2011 6:20:35 PM

302

Crystallography and Crystal Defects

9.2 A dislocation is being extruded between small precipitate particles which lie in a row, each particle being a distance l from its neighbours. Determine the force acting on each particle as a function of the shear stress s applied on the slip plane of the dislocation parallel to the Burgers vector b and estimate the maximum force that can be exerted on each particle. 9.3 Using Frank’s rule, make a study of reactions between stable perfect dislocations in a body-centred tetragonal crystal. Consider the effect of the value of the c/a ratio on the reactions. 9.4 Compare the number of atoms that are improperly surrounded by nearest neighbours (i.e. as an atom in the h.c.p. structure instead of as in the c.c.p. structure) at intrinsic and in extrinsic faults in c.c.p. metals. What structure is formed if both the Shockley partials in a Lomer–Cottrell lock are forced to glide to the opposite side of the stairrod dislocation? 9.5 Using a dislocation corresponding to one particular slip plane and slip direction as one of the reacting dislocations forming a Lomer–Cottrell lock, how many different – locks can be formed? For the slip system (111) [101], give the Burgers vector of each partial dislocation in all of the possible Lomer–Cottrell locks. 9.6 If the concentration of vacancies in aluminium at its melting point is 9.4 × 10−4 and if after quenching the aluminium from its melting point the vacancies condense into discs on the close-packed plane and form Frank loops, determine the density of dislocations introduced (a) when the loops are 50 Å in radius and (b) when the loops are 500 Å in radius. 9.7 Assuming isotropic elasticity, calculate the separation of the Shockley partials of a screw dislocation in Ag, Al and Au. Use the stacking fault energies given in Table 9.2. For Ag take m = 28 GPa, n = 0.38; for Al take m = 26 GPa, n = 0.34; for Au take m = 28 GPa, n = 0.42. 9.8 For the first four lattices listed in Table 9.1, find the Burgers vectors of any dislocations whose stability, according to Frank’s rule, is doubtful; that is, dislocations that might dissociate into two perfect dislocations whose Burgers vectors are at 90° to one another. 9.9 Lead sulphide, PbS, has the same crystal structure as NaCl, but the usual slip system – is {100}〈011〉 instead of {011}〈011〉. (a) Compare dislocation reactions that may occur as a result of slip in PbS with those occurring in NaCl. (b) Sketch the structure of the edge of the extra plane of an edge dislocation in PbS. 9.10 Describe the dislocation loops that might be produced in zinc by the aggregation of interstitial atoms into discs of atoms parallel to the basal plane. Also describe the dislocation loops that might be produced in graphite by the aggregation of vacant sites into discs parallel to the basal plane. – 9.11 Project the structure of silicon on to a (101) plane and show, in this projection, the structure of an intrinsic stacking fault and the structure of an extrinsic stacking fault in silicon.

Kelly_c09.indd 302

11/30/2011 6:20:36 PM

Dislocations in Crystals

303

9.12 Show how, in graphite, two dislocation ribbons (i.e. dislocations that are split into widely separated partials) that are on next-nearest-neighbour basal planes can interact to form a three-fold ribbon. 9.13 An alloy of 50 at% Cu–50 at% Zn contains dislocations of Burgers vector 12 111 and 〈100〉. The alloy is then ordered to produce the B2 superlattice (Section 3.8). – Describe the effect of gliding the 12 111 dislocation on {110} and the 〈100〉 dislocation on {010} after ordering has occurred. From your result, how would you expect two identical 12 111 dislocations to interact in the ordered alloy?

Suggestions for Further Reading See the suggestions for Chapter 8 and the following: F.R.N. Nabarro, M.S. Duesbery, J.P. Hirth and L. Kubin (1979–2010) Dislocations in Solids, Volumes 1–16, Dislocations and Disclinations, Elsevier, Amsterdam. T. Suzuki, S. Takeuchi and H. Yoshinaga (1991) Dislocation Dynamics and Plasticity, Springer, Berlin (translated from the Japanese edition published by Shokabo in 1985).

References [1] G. Lu, N. Kioussis, V.V. Bulatov and E. Kaxiras (2001) Dislocation core properties of aluminum: a first-principles study, Mater. Sci. Eng. A, 309–310, 142–147. [2] J.P. Hirth and J. Lothe (1982) Theory of Dislocations, 2nd Edition, John Wiley and Sons, New York. [3] F.C. Frank (1949) written answer to a remark by E.N. da C. Andrade on the paper by N.F. Mott (1949) Mechanical properties of metals, Physica, 15, 119–128: Physica, 15, 131–133. [4] A.J.E. Foreman (1955) Dislocation energies in anisotropic crystals, Acta Metall., 3, 322–330. [5] R.D. Heidenreich and W. Shockley (1948) Study of slip in aluminum crystals by electron microscope and electron diffraction methods, Bristol Conference on the Strength of Solids, The Physical Society, London, pp. 57–75. [6] D.B. Williams and C.B. Carter (1996) Transmission Electron Microscopy: A Textbook for Materials Science, Plenum Press, New York. [7] D.J.H. Cockayne, M.L. Jenkins and I.L.F. Ray (1971) The measurement of stacking-fault energies of pure face-centred cubic metals, Phil. Mag., 24, 1383–1392. [8] P.S. Dobson, P.J. Goodhew and R.E. Smallman (1967) Climb kinetics of dislocation loops in aluminium, Phil. Mag., 16, 9–22. [9] M.L. Jenkins (1972) Measurement of the stacking-fault energy of gold using the weak-beam technique of electron microscopy, Phil. Mag., 26, 747–751. [10] W.M. Stobbs and C.H. Sworn (1971) The weak beam technique as applied to the determination of the stacking-fault energy of copper, Phil. Mag., 24, 1365–1381. [11] C.B. Carter and S.M. Holmes (1977) The stacking-fault energy of nickel, Phil. Mag., 35, 1161–1172. [12] F.C. Frank (1951) The growth of carborundum: dislocations and polytypism, Phil. Mag., 42, 1014–1021. [13] N. Thompson (1953) Dislocation nodes in face-centred cubic lattices, Proc. Phys. Soc. B, 66, 481–492. [14] M.J. Whelan (1959) Dislocation interactions in face-centred cubic metals, with particular reference to stainless steel, Proc. Roy. Soc. Lond. A, 249, 114–137.

Kelly_c09.indd 303

11/30/2011 6:20:36 PM

304

Crystallography and Crystal Defects

[15] W.M. Lomer (1951) A dislocation reaction in the face-centred cubic lattice, Phil. Mag., 42, 1327–1331. [16] A.H. Cottrell (1952) The formation of immobile dislocations during slip, Phil. Mag., 43, 645–647. [17] J. Silcox and P.B. Hirsch (1959) Direct observations of defects in quenched gold, Phil. Mag., 4, 72–89. [18] J.P. Hirth (1961) On dislocation interactions in the fcc lattice, J. Appl. Phys., 32, 700–706. [19] J.B. Bilde-Sørensen, T. Leffers and P. Barlow (1977) Dissociated structure of dislocation loops with Burgers vector a in electron-irradiated Cu–Ni, Phil. Mag., 36, 585–595. [20] F.R.N. Nabarro (1987) Theory of Crystal Dislocations, Dover Publications, New York. [21] J. Friedel (1955) On the linear work hardening rate of face-centred cubic single crystals, Phil. Mag., 46, 1169–1186. [22] T.H. Alden (1963) Extreme latent hardening in compressed lithium fluoride crystals, Acta Metall., 11, 1103–1105. [23] J.D. Eshelby, C.W.A. Newey, P.L. Pratt and A.B. Lidiard (1958) Charged dislocations and the strength of ionic crystals, Phil. Mag., 3, 75–89. [24] R.W. Whitworth (1975) Charged dislocations in ionic crystals, Adv. Phys., 24, 203–304. [25] A. Korner and H.P. Karnthaler (1983) Weak-beam study of glide dislocations in h.c.p. cobalt, Phil. Mag. A, 48, 469–477. [26] R.L. Fleischer (1986) Stacking fault energies of hcp metals, Scripta Metall., 22, 223–224. [27] L. Wen, P. Chen, Z.-F. Tong, B.-Y. Tang, L.-M. Peng and W.-J. Ding (2009) A systematic investigation of stacking faults in magnesium via first-principles calculation, Eur. Phys. J. B, 72, 397–403. [28] P.S. Dobson and R.E. Smallman (1966) The climb of dislocation loops in zinc, Proc. Roy. Soc. Lond. A, 293, 423–431. [29] M.H. Yoo (1981) Slip, twinning, and fracture in hexagonal close-packed metals, Metall. Trans. A, 12, 409–418. [30] M.H. Yoo, J.R. Morris, K.M. Ho and S.R. Agnew (2002) Nonbasal deformation modes of hcp metals and alloys: role of dislocation source and mobility, Metall. Trans. A, 33, 813–822. [31] T. Nogaret, W.A. Curtin, J.A. Yasi, L.G. Hector and D.R. Trinkle (2010) Atomistic study of edge and screw dislocations in magnesium, Acta Mater., 58, 4332–4343. [32] D. Hull and D.J. Bacon (2011) Introduction to Dislocations, 4th Edition, ButterworthHeinemann, Oxford. [33] A.H. Cottrell (1958) Theory of brittle fracture in steel and similar metals, Trans. Am. Inst. Min. Metall. Petrol. Engrs., 212, 192–203. [34] V. Vítek (1968) Intrinsic stacking faults in body-centred cubic crystals, Phil. Mag., 18, 773–786. [35] L. Ventelon and F. Willaime (2010) Generalized stacking-faults and screw-dislocation corestructure in bcc iron: a comparison between ab initio calculations and empirical potentials, Phil. Mag., 90, 1063–1074; corrigendum, 4071. [36] A. Kelly and G.W. Groves (1970) Crystallography and Crystal Defects, Longman Group Limited, London. [37] M.S. Duesbery and V. Vitek (1998) Plastic anisotropy in b.c.c. transition metals, Acta Mater., 46, 1481–1492. [38] A. Olsen and J.C.H. Spence (1981) Distinguishing dissociated glide and shuffle set dislocations by high resolution electron microscopy, Phil. Mag. A, 43, 945–965. [39] H.R. Kolar, J.C.H. Spence and H. Alexander (1996) Observation of moving dislocation kinks and unpinning, Phys. Rev. Lett., 77, 4031–4034. [40] W. Cai, V.V. Bulatov, J. Chang, J. Li and S. Yip (2004) Dislocation core effects on mobility, in Dislocations in Solids, Volume 12 (edited by F.R.N. Nabarro and J.P. Hirth), Elsevier, Amsterdam, pp. 1–80. [41] G.R. Booker (1964) Crystallographic imperfections in silicon, Disc. Faraday Soc., 38, 298–304. [42] P. Delavignette, H.B. Kirkpatrick and S. Amelinckx (1961) Dislocations and stacking faults in aluminum nitride, J. Appl. Phys., 32, 1098–1100. [43] C. Baker, Y.T. Chou and A. Kelly (1961) The stacking-fault energy of graphite, Phil. Mag., 6, 1305–1308.

Kelly_c09.indd 304

11/30/2011 6:20:39 PM

10 Point Defects 10.1

Introduction

Disturbances in a crystal which, apart from elastic strains associated with them, extend for no more than a few interatomic distances in any direction are called point defects. Although impurity atoms in solution can be classified as point defects, we shall be mainly concerned with structural point defects, of which there are two elementary types. The first is the vacancy, which consists of an atomic site from which the atom is missing. The second consists of a small region of crystal which contains an extra atom. This is called an interstitial defect, from the idea that the extra atom is squeezed into an interstice between the others. A point defect differs from a dislocation and from a two-dimensional defect such as a crystal boundary in two important respects. The first is that, even with modern transmission electron microscopes, scanning tunnelling microscopes and atom probe field-ion microscopes, point defects are relatively difficult to observe directly, so that in the main they can be detected and studied only through their effect upon some physical property of the crystal. The second distinction is that point defects may be present in appreciable concentrations when the crystal is in thermodynamic equilibrium. While dislocations and interfaces always raise the free energy of a crystal, adding a certain number of point defects to an otherwise perfect crystal reduces its free energy to a minimum value. This is because of a gain of entropy which arises from the many possible sets of places in the crystal where the point defects can be put. This configurational entropy is given by:

S = k ln W

(10.1)

where k is Boltzmann’s constant (1.38 × 10−23 J K−1 or 8.62 × 10−5 eV K−1) and W is the number of different arrangements of point defects. When n defects are distributed amongst

Crystallography and Crystal Defects, Second Edition. Anthony Kelly and Kevin M. Knowles. © 2012 John Wiley & Sons, Ltd. Published 2012 by John Wiley & Sons, Ltd.

Kelly_c10.indd 305

11/30/2011 9:59:11 AM

306

Crystallography and Crystal Defects

N sites, the number of arrangements is NPn = N(N − 1)…(N − n + 1) = N!/(N − n)! if each defect is distinct. In fact, all the defects are identical, and the n labels needed to distinguish them from one another can be distributed in n! ways. Therefore: W = N Cn =

N! ( N − n)! n !

(10.2)

Manipulating Equation 10.2 into a form suitable for the application of Stirling’s approximation (ln x! ≈ x ln x − x, for large x) gives: ln W = N ln N − ( N − n) ln( N − n) − n ln n

(10.3)

so that in Equation 10.1: S = k [ N ln N − ( N − n) ln ( N − n) − n ln n]

(10.4)

If the presence of one defect increases the internal energy of the crystal by Ef , the change in free energy of a crystal containing n identical defects, at a temperature of T K, is: ΔF = nEf − T (S + nS ′ )

(10.5)

Here it is assumed that n/N is so small that the defects do not interact with one another. The extra entropy term nS′ in Equation 10.5 represents the fact that each defect may add a certain entropy S′ to the crystal because of its effect on the vibration of the atoms in its neighbourhood. The number of defects producing the minimum free energy, ne , is found by setting dΔF/dn = 0, giving: ne ⎛ E ⎞ ⎛ S′⎞ = exp ⎜ ⎟ exp ⎜ − f ⎟ ⎝ k⎠ ⎝ kT ⎠ N − ne

(10.6)

If the defect in question is a vacancy then N − ne is simply the number of atoms in the crystal. Since in fact ne 0. Finally, comparing the Schmid factors for A III and D I, we have: A III : | cos φ cos λ | (× 6(u2 + v 2 + w 2 )) = w 2 + vu + vw − u2 D I : | cos φ cos λ | (× 6(u2 + v 2 + w 2 )) = w 2 + vu + uw − v 2 and since: n w + v 2 > uw + u2 for 0 < u < v < w, it follows that A III is the slip system with the greatest Schmid factor; that – is, the slip system (111) [101]. This is of course the slip system found using either Diehl’s rule or OILS rule for a pole within the 001–011–111 standard stereographic triangle in c.c.p. crystals. Thus, Diehl’s rule and OILS rule are both proved using this methodology. The extension of this analysis to other stereographic triangles can be achieved by suitable permutations of the indices defining the poles at the corners of the standard stereographic triangle. A simple extension of this methodology enables special cases, such as where u = v > 0, to be considered when two or more slip systems have the same Schmid factor.

References [1] J. Diehl, personal communication to A. Seeger, acknowledged on p. 24 of A. Seeger (1958) Kristallplastizität, Handbuch der Physik, Band VII.2: Kristallphysik II (edited by S. Flügge), Springer-Verlag, Berlin, pp. 1–210. [2] I.M. Hutchings (1993) Quick non-graphical method for deducing slip systems in cubic close packed metals in tension or compression, Materials Science and Technology, 9, 929–930.

Kelly_bapp05.indd 486

11/30/2011 2:48:47 PM

Appendix 6 Homogeneous Strain A body is said to be homogeneously strained if the distortion is the same everywhere. Under these circumstances, the eij in Equations 6.5 and 6.9 are constants, independent of position in the body. The equation: dui =

∂ui ∂x j

dx j = eij dxj

(A6.1)

can then be integrated immediately to obtain the displacements: ui = (u0 )i + eij x j

(i, j = 1, 2, 3)

(A6.2)

It is apparent from Equation A6.2 that in homogeneous strain, the displacements are linear functions of the position coordinates. The constants (u0)i represent the translation of the body as a whole, and are of no further interest. Subtracting this translation from the displacement, we obtain the residual displacement: xi′ − xi = eij x j

(A6.3)

where x'i are the new coordinates (referred to axes that have been translated by (u0)i but not rotated) of the point which was originally at xi. Equation A6.3 written out in full is: x1′ = (1 + e11 ) x1 + e12 x2 + e13 x3 x2′ = e21 x1 + (1 + e22 ) x2 + e23 x3 x3′ = e31 x1 + e32 x2 + (1 + e33 ) x3

Crystallography and Crystal Defects, Second Edition. Anthony Kelly and Kevin M. Knowles. © 2012 John Wiley & Sons, Ltd. Published 2012 by John Wiley & Sons, Ltd.

Kelly_bapp06.indd 487

11/30/2011 2:51:35 PM

488

Crystallography and Crystal Defects

The shape into which a line or surface whose general equation is: f ( x1 , x2 , x3 ) = 0

(A6.4)

is deformed can be determined by solving Equation A6.3 for x1, x2 and x3 in terms of x′1, x′2 and x′3, and substituting these values into Equation A6.4. In this way it can be shown that any homogeneous strain, large or small, has the following four properties: 1. Straight lines remain straight lines, and in general are rotated and stretched or contracted, all straight lines in the same direction being rotated through the same angle and stretched or contracted in the same ratio. Similarly, planes are deformed into planes. 2. A sphere is deformed into an ellipsoid. The ellipsoid into which a sphere of unit radius is deformed is called the strain ellipsoid. 3. The axes of the strain ellipsoid are derived from three mutually perpendicular diameters of the unit sphere, which are called the principal axes. These axes form the only set of three orthogonal directions which remain orthogonal after the strain. 4. In the unstrained state there is a particular ellipsoid, called the reciprocal strain ellipsoid, which deforms into the unit sphere. Its axes are the principal axes. In general, the principal axes are rotated by the strain. A deformation which leaves the principal axes unrotated is called a pure strain. A general homogeneous strain can be accomplished in two stages: a pure strain in which the principal axes receive their correct extensions, followed by a rotation in which they are brought to their final position. The above results are applied in the discussion of the geometry of martensitic transformations in Chapter 12. We shall now mention three very simple types of homogeneous strain.

A6.1 Simple Extension x1′ = kx1 , x 2′ = x2 , x3′ = x3 ,

⎛ e11 = k − 1 e12 = 0 e13 = 0 ⎞ ⎜e = 0 e22 = 0 e23 = 0⎟ ⎜ 21 ⎟ e32 = 0 e33 = 0⎠ ⎝ e31 = 0

(A6.5)

The principal axes Ox1, Ox2 and Ox3 are not rotated; therefore, simple extension is a pure strain.

A6.2

Simple Shear x1′ = x1 + gx2 , x2′ = x2 , x3′ = x3 ,

⎛ e11 = 0 e12 = g e13 = 0 ⎞ ⎜ ⎟ ⎜ e21 = 0 e22 = 0 e23 = 0 ⎟ ⎜e = 0 e = 0 e = 0⎟ 32 33 ⎝ 31 ⎠

(A6.6)

where g is the magnitude of the shear strain, as defined in Equation 6.2. A more detailed description of simple shear is developed in Chapters 7 and 11, where it is required for the description of slip and twinning. Simple shear is not a pure strain; its nonrotational part is described below.

Kelly_bapp06.indd 488

11/30/2011 2:51:41 PM

Homogeneous Strain

489

x 2° x2

P

Q

P⬘

x1

a a p –a 4 2 O

a = tan–1

x 1°

g 2

Figure A6.1

A6.3

Pure Shear x1′ = kx1 , −1

x2′ = k x2 , x3′ = x3 ,

e13 = 0 ⎞ ⎛ e11 = k − 1 e12 = 0 ⎜ ⎟ e22 = (1 / k ) − 1 e23 = 0 ⎟ ⎜ e21 = 0 ⎜e =0 e32 = 0 e33 = 0 ⎟⎠ ⎝ 31

(A6.7)

In this strain, the principal axes are Ox1, Ox2 and Ox3, and they are not rotated.

A6.4

The Relationship between Pure Shear and Simple Shear

The relationship between a pure shear and a simple shear is illustrated by the diagram in Figure A6.1. A simple shear of strength g, referred to axes Ox1°, Ox°, 2 distorts a circle into the ellipse shown in Figure A6.1. The same ellipse can be produced by a strain which is a pure shear, referred to axes Ox1, Ox2, with Ox1 at an angle of π / 4 − 12 tan −1 g / 2 to Ox1°, as shown in Figure A6.1. The required magnitude of the pure shear is given by:

(

k − 1/ k = g

)

(A6.8)

In order for the displacements produced by this pure shear to be identical to those produced by the simple shear, it must be preceded by a rotation of tan−1g/2. Thus point P, for example, is rotated to Q, and the pure shear then carries Q to P′. Alternatively, the displacements of the simple shear can be produced by a pure shear referred to axes at ±π / 4 + 12 tan − 1 g / 2 to Ox1°, followed by a rotation of tan−1g/2. These axes are principal axes of the simple shear; Ox1, Ox2 and Ox3 (which remains unchanged) are the principal axes of the simple shear in their final, rotated position. When the simple shear is of very small magnitude (g = g, where g 3 ; for practical values of c/a seen in h.c.p. metals (1.5 < c/a < 1.9), com– pression would be possible if the only twinning mode were (112 1) and elongation – would be possible if the only twinning mode were (112 2). 11.12 Yes. 11.14 4°. 11.15 10%.

Chapter 12 12.1 4, 2 (twins). Component of b normal to (111) must equal 2 a / 3 . 0 0⎞ ⎛ 1 12.3 12 〈110〉 vectors. Yes. ⎜ − 1 1 − 1 ⎟ . ⎜ 2 2 2⎟ ⎜⎝ 0 1 1 ⎟⎠ 12.5 1.57. 12.6 0.18°, 0.003. 12.7 2, 4, 6. ⎛ ⎞ 1 0 0 ⎜ ⎟ 12.10 ⎜ . 0 1 − 1⎟ 2 2⎟ ⎜ 1⎟ ⎜0 1 ⎝ 2 2⎠

Chapter 13 13.2 13.3 13.4 13.5 13.6

Kelly_both.indd 506

Step heights are 1, 3, 1 and 2 lattice plane spacings, respectively. g(0 0 1) = 0.894 g(2 1 0), g(1 1 1) = 0.775 g(2 1 0), g(1 1 0) = 0.949 g(2 1 0) (as in Figure 13.5).

1.16 J m−2, 15%. (a) Attract, (b) energy increases as b2 ln b. – Boundary plane: (a) {110}, (b) {110}, (c) {112 0}. Axis of tilt: (a) 〈001〉, (b) 〈211〉, a a a – (c) 〈1 100〉. Angle of tilt: (a) 2 sin −1 , (b) 2 sin −1 , (c) 2 sin −1 . 2d 2 2d 2 2d

11/30/2011 7:37:49 PM

Brief Solutions to Selected Problems

507

13.7 See E.J. Freise and A. Kelly (1961) Twinning in graphite, Proc. Roy. Soc. Lond. A, 264, 269–276. 13.9 The difference in angle in radians is of the order of the ratio of the twin boundary to the surface free energy. 13.11 Effective surface free energy = 0.96g. 13.12 3.75%. – 13.13 (a) (11 0), (b) 3.1 × 107 m−1, (d) about 8°. 13.15 Two.

Kelly_both.indd 507

11/30/2011 7:38:04 PM

Index Note: Page numbers in italics refer to Figures; those in bold to Tables aggregation of point defects, 309, 311 alkali halides, point defects, 309–10, 315, 320–1 alkali metals, crystal structure, 92, 369 allotropy (elements), 86, 110 alloys, metallic amorphous (noncrystalline), 124 phase transformations, 363–4, 374–83 quasicrystalline phases (i-phases), 136–7 strained layer epitaxy, 425 topological close-packing (TCP), 135 twinning frequency, 342–3, 353–4, 354 aluminium dislocation strain energies, 271–2 elastic isotropy, 256 vacancy generation, with heating, 318, 319 amorphous materials, 123–6 anelastic strain, 326–7, 329 anisotropy Hooke’s law application, dislocation strains, 256–8 of mesogenic molecules (liquid crystals), 126–7 and polycrystalline textures, 229 annealing, 322–4, 323, 325 twins, 336 antimony, crystal structure, 97–8, 98, 98 antiphase domain boundaries, 112, 113 antisymmetric tensors, 148–9 arsenic, crystal structure, 97–8, 98, 98

atactic polymers, 115 atomic radii, 110 austenite, 363, 379–82 axes of rotational symmetry, 15–16, 43, 44 permissible combinations, 21–6, 25 pure (proper rotation), 44, 44–5 axial angles, 6, 6, 8, 67 axial glide planes, 72 axial (c/a) ratios, 52 hexagonal close-packed metals, 90–1, 91 and slip planes, 205, 208, 291 and martensitic transformation, 374 wurtzite structure compounds, 101, 101 Bain correspondence, 379, 379–81, 383 barium titanate (BaTiO3) crystal structure, 105 phase transitions and ferroelectric properties, 384 binding energy, divacancies, 310–11 bismuth, crystal structure, 97–8, 98, 98 body-centred cubic (b.c.c.) structure dislocation geometry, 295–7, 296 glide systems, 205, 219–20, 221 lattice symmetry and unit cells, 36–7, 37, 92–3, 93 point defects interstitials, 314, 314–15 vacancies, 313, 316, 316 transformation to h.c.p. structure, 369, 369–70, 374, 375, 385–6 twinning (metals), 342–4, 343

Crystallography and Crystal Defects, Second Edition. Anthony Kelly and Kevin M. Knowles. © 2012 John Wiley & Sons, Ltd. Published 2012 by John Wiley & Sons, Ltd.

Kelly_bindex.indd 509

11/30/2011 3:17:12 PM

510

Index

Boltzmann’s constant, 253, 305 Born–Mayer potential, 312 boron nitride, hexagonal form, 97, 97 brass, texture, 234, 234 Bravais (space) lattices, 26–37, 28, 71–2 brittleness, 199, 396 bulk metallic glasses (BMGs), 124 Burgers circuit, 245, 246, 246, 247 Burgers vector general description methods, 245–7, 246 related to strain energy, 269–71, 272–3 as slip plane displacement, 241–5 stability of dislocations, 273, 274 c/a ratios see axial ratios caesium chloride crystal structure, 99, 100, 496 unit cell, 7, 7 calcite crystal structure, 109, 109–10 deformation twinning, 345, 345, 354 calcium fluoride (fluorite), crystal structure, 102–3, 103 carbon iron impurity atomic arrangement, 326, 327, 329 in steel, and martensitic transformation, 363, 380, 380–1 see also diamond; graphite cassiterite structure see rutile crystal structure cellular solid materials, 137, 138–9 centre of symmetry, 16, 45, 153–4, 177–8 centred rectangular cells, 19, 21 charged dislocations, 289–90, 290 chemical force, on dislocations, 252–3 cholesteric phases (liquid crystals), 127, 128, 129 chrysoberyl crystal structure, 107 cleavage planes, 295, 296, 396–7, 397 climb (dislocation motion), 244, 248, 251, 252–3 close packing (of spheres), 86–8, 87, 88 Bernal’s RCPS model, 124, 125 interstices, 89, 90, 104

Kelly_bindex.indd 510

plane stacking, 88, 89, 91 stacking faults, 278–9, 279, 281 Frank notation, 280–1 topological (TCP) structures, icosahedral packing, 135, 136 closed forms, 49–50 cobalt martensitic transformation, 366–9, 368, 420 stacking fault energy, 291–2 coherency strain, 421, 427 coincidence site lattices (CSL), 405–6, 406, 407 compliances (elastic constants), 182–4, 188, 190 composition plane, K1 (twinning), 335, 337, 339, 350–3, 354 compound (degenerate) twins, 340 compounds, simple inorganic (MX and MX2), 98–104, 494–8 compression, and crystal lattice deformation, 226–8, 227 conductivity (electrical) direction, referred to tensor principal axes, 149–52, 151 measurement, and point defect mobility, 318–21, 320, 321 tensor components, 141–2, 144–5 constancy of angle, law of, 8, 8 converse effect (piezoelectricity), 181 coordination number, 3–4, 86, 110 copper alloys, martensitic transformation, 382–3 point defects, mobility, 308–9 rolled, texture, 229, 232, 232 correspondence matrix, 370, 379 corundum see sapphire covalent bonding dislocation geometry, 297–300, 301 dislocation width (Peierls model), 260 in polymers, 115 critical resolved shear stress, law of, 219 cross-slip (dislocations), 261–2, 262 crowdions (Paneth), 314, 314–15, 316–17

11/30/2011 3:17:13 PM

Index

crystal structure descriptive methods, 85–6, 116–17, 119 growth, 417–18 crystal systems, 26, 26 elastic constants, 184–93, 188, 190 enantiomorphous, 68–9 Internet information sources, 499–500 of named elements, 491–4 noncentrosymmetric, piezoelectric moduli, 179–81 second-rank tensor limitations, 155, 156, 158–9 special forms, 67, 68 crystallographic glide strain definition, 202–3, 203 in displacement analysis, 210 and lattice orientation, in tension/ compression, 222, 223–4, 226 cubic close-packed (c.c.p.) structure, 86–9, 87, 88, 89, 90 coincidence lattices, 405, 406 dislocation geometry, 278–88, 279, 288 double slip, 225, 225–6 and icosahedral packing, 134, 135 point defects interstitials, 314, 314 vacancies, 312–13, 313, 316, 317, 317–18 slip system stereograms, 219, 220, 220–2, 222 transformation to h.c.p. structure, 366–9, 368, 385 twinning (metals), 335–7, 336, 337, 342 see also face-centred cubic (f.c.c.) structure cubic crystal system elastic constants, 186–7, 187, 189 glide systems, pure strain and rotation, 212–15, 213, 214 lattice symmetry and unit cells, 35, 35–7, 36, 37 planar spacing and interplanar angles, 471–2 point group symmetry elements, 53, 53–5 property representation quadric, 158

Kelly_bindex.indd 511

511

shear stress and piezoelectricity, 180, 180–1 stereogram, 453–5, 454 stereograms, 55, 55 tetragonal defect orientation, 329, 329 damping, 327 defect structures, 99 deformation twinning, 337–42, 339, 354–8 dendrites, 417, 418 density dislocation, 245, 261 of solid solutions, 111 deviatoric stress, 176 diad (two-fold) axis of symmetry, 18, 19–20, 30 diagonal glide planes, 72 diamond crystal structure, 95, 95, 96 dislocations, 297–8, 298 diamond glide planes, 72 Diehl’s rule, 221, 483–4, 485–6 diffraction patterns in crystal structure determination, 85, 464 Laue method, 69, 69 diffusion-based phase transformations, 364 dihedral angles, 420, 421 dilatation, 169–70, 170, 260 dipoles dislocation, 263, 284 electric, single crystal (piezoelectricity), 177, 180 directions closest-packed (lattice), 87–8, 88, 91 glide (slip), 201, 201–2, 204, 225, 273 indices, transformation for unit cell changes, 473–4 physical properties, tensor representation, 150–2, 151, 155–60 relative displacement, in dislocations, 247, 247 shear, in twinning (h), 338–9, 339, 350–1 specification of, 9, 9

11/30/2011 3:17:13 PM

512

Index

dislocation glide motion, 248, 248–9 dislocations Burgers vector, general description, 245–7, 246 core, atomic positions, 258–61 crystal distortion, 253–8 forces and crystal stress, 249–53, 398–9 geometry, for specific crystal structures, 301 body-centred cubic (b.c.c.) crystals, 295–7, 296 covalent solids, 297–301 cubic close-packed (c.c.p.) metals, 280–8, 288 hexagonal metals, 290–5, 291 rock salt, 288–90, 289 glide mechanisms, 205, 241–5 interactions and multiplication, 261–5, 262, 272 loop motion, 247–9, 248 partial, and stacking faults, 277–9, 279 pile-up, in deformation twinning, 355–6, 356 strain energy and stability, 269–77, 274 displacive phase transitions, 384 domains, in ordered crystals, 112, 113 double hexagonal close-packed structure, 92 double (duplex) slip, 72, 225, 228 ductility, 199, 229 dummy suffix notation (tensor components), 145–6 dyadic operators see second-rank tensors edge dislocations atomic positions, 243–5, 244 bonding and Peierls force, 261 and Burgers vector, 246, 246 description, for cubic lattice, 242–3, 243 distortion stresses and strains, 255–6 strain energy calculation, 270–1 electric charge (NaCl), 289–90, 290 parallel, 262–3, 263 stair rods, 286, 286–7, 299 stress and force components, 251–3, 252 Einstein summation convention, 145–6, 438

Kelly_bindex.indd 512

elastic twinning, 356 elasticity crystal deformation, compared with plastic glide, 200 dislocation elastic energy, 273, 277 elastic constants, in crystal classes, 184–9, 188, 190 in isotropic materials, 189, 192–3, 256 strain and stress relationships, 181–4 electric fields see space charge regions electrical conductivity see conductivity electron irradiation, 324–5, 325 ellipsoids as effect of homogeneous strain on spheres, 371, 371, 488 physical property representation, 157–60, 158, 159 emissary dislocations, 356, 356 enantiomorphs crystal classes, 68–9 related to symmetry, 43–4 engineering shear strain, 165–6, 166, 170 entropy, related to point defects, 305–6, 310 epitaxial growth, 423–4, 424, 424 equilibrium point defect concentration, 305, 307, 318, 319 Euler angles, 234, 234–5 Euler’s theorem, related to regular polyhedra, 131, 133 extension, 165, 166, 488 extrinsic (double) stacking faults, 279, 280–1, 284 extrusion (of dislocations), 275–7, 276, 277 F-centres (anion vacancies), 310 face-centred cubic (f.c.c.) structure Bravais lattice, 36, 36, 86 transformation to face-centred tetragonal (f.c.t.), 374–6 ferroelectric materials, 335, 384 ferrous oxide, point defects, 310 fibre composite materials, 139 field tensors, 142 fluorite crystal structure, 102–3, 103, 498 foams, 137–9, 138

11/30/2011 3:17:13 PM

Index

forces, on dislocations climb and glide components, 251–3, 252, 263 Peierls model, 259–61 work and energy relationships, 249–51, 396–7 Frank partials, 281–3, 286–7, 287 Frank–Read mechanism, dislocation source, 261–2, 276 Frank’s rule, 272, 272–3, 287 Frenkel defects, 306–7, 325 FS/RH convention (Burgers vector), 245–6, 246, 247, 284 garnets, crystal structure, 107–9, 108 glasses, 123, 124, 189 glide (slip) conditions and process, 199–200, 200 displacement tensor components analysis as pure strain and rotation, 211–12, 212 for different slip systems, 212–14, 213 in three dimensions, 210, 210–11 in two dimensions, 208–10, 209 fine structure, 200–1, 202, 202 independent slip systems, 215–17, 216, 481–3 large strains in single crystals glide system choice, 218–22 lattice orientation changes, 222–8 measurement of glide strain, 202–3, 203 plane symmetry elements, in space groups, 70–1, 72, 78 polycrystalline grain deformation, 217–18 system elements, 203–5, 204 for named crystal types, 205, 206–7 see also dislocations glide cylinder (dislocation motion), 248, 248 grain boundaries energy related to tilt angle, 398–400, 399 good fit and coincidence lattices, 405, 405–7, 407 interface junctions, 409–14 source lattice (dislocation array), 408, 408–9

Kelly_bindex.indd 513

513

see also phase boundaries; tilt boundaries grains lattice rotation, 217–18 polycrystal arrangement, froth analogy, 418–19, 419 preferred lattice orientation (texture), 228–9, 233–5 role in structure of crystalline solids, 397 graphene, unit cell definition, 3–6, 4 graphite basal plane dislocations, 299–300, 300, 301, 350 crystal structures, 95–7, 97 twinning, 346, 349–50, 350, 351 vacancies, 317 grossular (natural garnet), 108 group theory, 79 H-centres (anion interstitial defects), 315, 315 habit plane, 364–5, 371–4, 373 in steels, 381–2, 382 halite see sodium chloride Heidenreich–Shockley partials see Shockley partials Hermann–Mauguin notation, 78–9, 80 Herring’s construction, crystal shape, 415–16, 416 hexad (six-fold) axis of symmetry, 18, 20–1 hexagonal close-packed (h.c.p.) structure, 87, 89, 90–1, 91, 92 second-order pyramidal glide, 292–3, 293 at twin boundary, 336 hexagonal crystal system, 33, 34, 35, 35 dislocation geometry, 290–5, 291 elastic constants, 189, 191 orthohexagonal cell indices, 476–7, 477 planar spacing and interplanar angles, 471, 472 point group symmetry elements, 56, 56–9 twinning (metals), 346, 349 Hirth lock configuration, 287, 287–8 holosymmetric class (of crystal systems), 50

11/30/2011 3:17:13 PM

514

Index

homogeneous strain, 166, 200, 208–9, 328, 445 mathematical properties, 487–8 see also extension; shear Hooke’s law, 181–2, 445–6 anisotropic media, calculations, 256–8 dislocation stresses and strains, 254–5 for isotropic solids, 192–3 hydrostatic pressure, 175–6, 199 i-phases, 136–7 icosahedral packing, 134–5, 135, 136 ilmenite (FeTiO3), crystal structure, 106 improper rotations, 44 impurities, and point defects, 305, 310, 322, 326 incommensurate structures, 137 indium crystal structure, 93–4 thallium (In–Tl) alloys, martensitic transformation, 374–49, 376 inert gases crystal structure, 86 secondary bonding, 115 infinitesimal strain, 166 in three dimensions, 168–70, 170 in two dimensions, 166–8, 167, 168, 169 interatomic distances (in crystals), 110, 491–4 interface junctions, 409–14, 411, 412 internal friction, 327 International Tables for Crystallography arithmetic crystal classes and space groups, 71, 73, 74–6, 77 entry example, 3-D space group, 79–82, 80–1 conventional symbols, 48 interstices in amorphous solids, 124 body-centred cubic crystals, 92–3, 93 cubic close-packed crystals, 89, 90 filled, in compounds, 98, 100, 101, 104 hexagonal close-packed crystals, 91, 92, 92 interstitial defects, 305, 309 configurations, 313–15, 314, 315

Kelly_bindex.indd 514

mobility, 316 interstitial solid solutions, 110–11, 111 intrinsic (single) stacking faults, 280–1, 280–4 invariant planes, 365–6, 371–3 inverse matrices, 445–7 inverse spinel structure, 107 ionic radii, 110, 491–4 isomorphic groups, 79 isotactic polymers, 115 isotropic crystals, 158 elastic properties, 189, 192–3, 256 jogs, 264–5, 265, 289 Kevlar (PPTA), 126, 127 kinks, 264, 297, 297 Kronecker delta, 177, 186, 193, 440 Lamé constants, 192–3, 256 lamellae, twinned crystals, 337–8, 354–5, 355, 356, 357–8 twin boundary surface grooving, 413, 413 lattice parameters, 6, 8–9 derivation of interatomic distances, 110 ratio (axial ratios), 52 of steel (austenite/martensite) phases, 380, 380 lattice points, 5–6, 10 lattices Bravais (space), 26–37, 28, 71–2 cellular material structures, 138–9 definition, formal, 6 plane spacing and direction, 7–11, 9, 10, 442–3, 469–72 vectors and lattice planes, 11–14, 12, 440–2, 441, 475 see also symmetry elements Laue groups, 69, 69, 158, 185 line tension, dislocation loops, 274–7, 275 liquid crystals, 126–9, 128, 130 lithium niobate (LiNbO3), crystal structure, 106 Lomer–Cottrell lock configuration, 286, 286, 299 long-range order (solid solutions), 113, 387

11/30/2011 3:17:13 PM

Index

magnesioferrite (MgFe2O4), 420 martensite (quenched steel), 363, 379–82, 382 martensitic transformation in alloys, 374–83 crystallographic features, 364–6, 365, 367 in metal crystals, 366–74 in nonmetals, 384–5 nucleation and growth of plates, 385–7 massive transformation, 363–4 matrices applications for martensitic lattice transformations, 370 notation for piezoelectric moduli, 178–80 for stiffness and compliance, 184, 188 for twinning index transformations, 341–2 mathematical operations, 443–7 rotation, 21–2, 142, 448 matter tensors, 142, 142 mercury, crystal structure, 94, 94 meshes see nets, two-dimensional; porous solid materials mesogenic units, in polymers, 127 mesophase materials (liquid crystals), 126–9, 128, 130 metallic crystal structures, 86–95 reorientation, in metal working, 228–9, 230–1 Miller index notation, 10, 11, 52, 440, 471–2 Miller–Bravais indices, 56–7, 57, 61 three- to four-index transformation, 57–8, 58 twinning shear transformation, 341 mirror plane, 16, 16, 19, 19, 43–4 related to space groups, 78 related to twinning, 335–6 misfits (interface strain), 421–3, 422, 427–8, 428 mixed dislocations description, for cubic lattice, 243, 243 distortion stresses and strains, 256

Kelly_bindex.indd 515

515

strain energy calculation, 271 mobility, point defects, 308, 308–9, 315–17, 318–21 molecular beam epitaxy (MBE), 423, 424–5 monoclinic crystal system elastic constants, 185 lattice symmetry and unit cells, 27, 29, 29–30, 30 piezoelectric moduli, 179 planar spacing, 470 point group symmetry elements, 63, 63–5 property representation quadric, 159 twin boundary, 406, 407 Morse function, 312 multiplicity, 49–50 nematic phases (liquid crystals), 127–9, 128, 130 nets, two-dimensional consistent with crystal symmetry, 17, 18–19, 19–21 lattice point arrays, 5, 7–8 rectangular, 18–19, 21 stacking, 27, 27, 29, 29–30, 30 Neumann bands, 354 Neumann’s principle, 153–4, 177 nickel arsenide (niccolite), crystal structure, 101–2, 102, 497 titanium (Ni–Ti) alloys, martensitic transformation, 383 noble metals, crystal structure, 86 node, dislocation lines, 247, 285, 285 noncrystallographic symmetry, 136–7 nonprimitive unit cell, 21 nucleation, martensite, 385, 385–7 octahedral interstices, 89, 90, 91, 93 OILS rule (Hutchings), 221–2, 484–6 open forms, 49–50 ordering, in solid solutions, 111–13, 112, 114 orientation distribution function (ODF), 234, 234–5

11/30/2011 3:17:13 PM

516

Index

orthorhombic crystal system elastic constants, 185–6 example of space group description, 79–82, 80–1 lattice symmetry and unit cells, 30–3, 31, 32 piezoelectric moduli, 179 planar spacing and interplanar angles, 470, 472 point group symmetry elements, 49, 49–52, 51 property representation quadric, 158–9 PAA (para-azoxyanisole), 126, 126, 127 packing fraction, 86–7, 124, 126 partial dislocations, 277–9, 279, 343–4 Pearson symbol (crystal structure), 116–17, 119 Peierls dislocation model, 259–61 pencil glide, 205, 208, 215 perovskite crystal structure, 104–5, 105, 133–4, 135 phase boundaries, 420–4, 421, 421 phase transformations, 363–4, 384 see also martensitic transformation piezoelectricity, 177–81, 425 converse effect, 181 plagioclase feldspars, twin structures, 351 plane groups (2-D space groups), 73, 74–6, 77, 77–8 plastic deformation see glide Platonic solids, 131–4, 132 point defects aggregation, 310–11 configurations, 312–17 definition and types, 305 energy characteristics, 305–9 experimental production and studies, 317–21 in ionic crystals (alkali halides), 309–10 produced by radiation, 324–6 in quenched metals, 321–4 symmetry and anelasticity, 326–9 point groups, 43 general and special forms, 49–50 related to space groups, 71–2

Kelly_bindex.indd 516

symmetry elements, 44–8, 46–7 terminology for cubic systems, 53–4 Poisson’s ratio (n), 189, 192, 256 polarization, electrical, 177, 180 pole figures, 229, 232, 232 poles location on stereographic projections, 50–2, 51, 65, 451–5, 452 construction geometry, 458, 458–9, 459, 460 using Wulff net, 460–1, 462, 463 orientation and rolling texture, 232–3, 233 twin growth dislocation, 357, 357 polycrystalline materials, 137, 189, 397 glide deformation, 217–18 grain boundary tensions, 418, 418 texture development, during working, 228–35, 230–1 polyethylene, structure, 115, 116, 117 polygonization, 263 polyhedra, geometry of, 129, 131–4, 132 Voronoi construction, 124–6, 125 polymers, crystal structures, 113, 115, 118, 498 imperfections and amorphous regions, 115, 119 lyotropic and thermotropic liquid crystals, 126, 127 martensitic transformation, 384–5 unit cell, 115, 117 polymorphism (compounds), 86 porous solid materials, 137–8 primary glide plane, 220, 222 primitive unit cell, 6, 21, 440 principal axes and components, symmetric tensors, 149, 169, 170 prismatic dislocation loops, 248–9, 249, 253, 292 projections, geometry of, 451–5, 452, 453 pseudo-twins, in Fe–Be alloys, 353–4, 354 pseudomorphic strained layers, 425–8 pure shear related to simple shear, 489, 489 stresses, 174, 176

11/30/2011 3:17:13 PM

Index

pure strain tensors, 168–9, 169 and independent slip systems, 215–17, 216, 481–3 pyramidal glide, 292–3, 293, 294, 295 quasicrystals, 135–7 quaternion algebra, 22–3, 448–9 quenched metals, 321–4, 363–4 radiation damage, 308, 310, 324–6 radius–normal property, representation ellipsoid, 159, 159–60 random close-packed sphere model (RCPS), 124, 125 rare earth metals crystal structure, 90, 92 ion substitution, in garnets, 108–9 rational indices, law of, 10 rational line/plane, 10 reciprocal lattice vectors, 12, 440–3, 441, 469 reciprocal twins, 340–1 reconstructive transformation, 384 recrystallization, 229, 336 rectangular nets diad axes and mirror planes, 18–19, 21 stacking, and orthorhombic lattices, 31, 32 reflection symmetry, 16, 16, 18–19, 19 reflection (normal, type I) twins, 339–40, 340 relative displacement (strain) tensors, 167, 168–9, 210–11 relaxation time (elastic compliance), 3 27, 328 repeat units (distance), polymers, 115, 116 replacement collisions (point defects), 324 representation quadric, tensors and property measurement radius–normal property, 159, 159–60 representation surfaces, equations, 155–9, 158 representative volume elements, 139 resistivity, quenched metals, 322, 323

Kelly_bindex.indd 517

517

resolved shear stress evaluation, 218, 218–19 largest, associated glide systems, 219–22, 483–5 rhombus nets and unit cells, 31–3, 32 rigidity (shear) modulus, 192, 253, 254 rock salt see sodium chloride rolled metals, crystal orientation (texture), 229, 232, 232–5, 233, 234 rotation (parallel, type II) twins, 340, 340 rotational symmetry, 15–16, 444, 448 combinations, possible, 21–6, 25, 71 and crystallographic point groups, 44–8, 46–7 occurrence in crystal nets, 16–21, 17, 18 in quasicrystals, 135–6 rotoinversion axes, 44, 45, 48 rutile crystal structure, 103–4, 104, 133, 498 sapphire (corundum, a-Al2O3) conditions for glide, 199 crystal structure, 105–6, 106 scalar product mathematical operation, 436–8 scalar triple product, 438–9 and Weiss zone law, 13 Schläfli symbols, 131, 132 Schlegel diagrams, 131–3, 132 Schmid factor, 219, 221–2, 483–4, 485–6 Schoenflies notation, 78–9 Schottky defect, 309–10, 319–21 screw axes (symmetry elements), in space groups, 70, 70–2, 72 screw dislocations atomic positions, 243–4, 244, 245, 258–9 dislocation width, 259, 259, 260 description, for cubic lattice, 241–3, 242 distortion stresses and strains, 253–5, 254, 255 strain energy calculation, 269–70 orthogonal, 264, 264 parallel, 262, 264

11/30/2011 3:17:14 PM

518

Index

second-rank (dyadic) tensors definition and symmetry, 148–9 limitations imposed by crystal symmetry, 153–5, 156 representation surfaces, 155–9, 158 physical properties represented, 141–2, 142 referred to principal axes, 149–52, 150, 169, 173–4 vector components, transformation of, 144–5, 146–8 secondary bonding, in polymers, 115 self-accommodation, martensite variants, 374, 378, 378, 383 self-diffusion, 308–9, 322, 323, 324 semiconductors crystal growth and structure, 424–8 lattice parameters and stiffness constants, 427 shape-memory materials, 363, 383, 386 shear engineering shear strain (g), 165–6, 166, 170 forces, plastic yield (glide) responses, 199–203 modulus (rigidity), 192, 253, 254 pure strain tensor components, 168, 169, 169 resolved shear stress calculation, 218, 218–19 simple and pure, compared, 488–9, 489 stress components (s), 170, 172–3, 175, 176 and twinning mechanism, 336–9, 337, 338 shear magnitude, s, 338–9, 352–3 sheet textures, 232–5, 233, 234 Shockley partials compared with Frank partials, 281–3 separation and stacking fault energy, 278–9, 279, 280, 281 short-range order (solid solutions), 113 shuffle (atomic displacement), 346, 353 silicon stacking faults and dislocations, 297, 299, 299

Kelly_bindex.indd 518

states and properties, 124, 138 silver, rolled (crystal orientation), 234, 234 slip see glide slip lines (bands), observation of, 200–1, 202, 202, 262 smectic phases (liquid crystals), 127, 128, 129 soaps, 127 sodium chloride (rock salt, halite) crystal structure, 98–9, 99, 495–6 and discovery of glide, 200 dislocation geometry, 288–90, 289 glide planes and directions, 204–5 Schottky defects, 309–10, 319–21 vacancies, ionic displacement, 313, 313 solid solutions, 110–13, 111, 112, 114 see also alloys, metallic space charge regions, rock salt, 289–90, 290, 309 space groups, 69–78 three-dimensional, example, 79–82, 80–1 two-dimensional (plane) groups, 73, 74–6, 77, 77–8 space lattices see Bravais lattices sphalerite (zinc blende, a-ZnS) crystal structure, 100, 100–1, 497 dislocations, 297–8, 298, 299 piezoelectricity, 180 plane stacking sequence, 95, 96 twin structures, 344, 344–5 spheres see close packing spinel crystal structure, 106–7, 107 stacking faults, 278–9, 279, 336 see also dislocations stair rod dislocations, 286, 286–7, 299 steel, martensitic transformation, 363, 379–82, 380, 382 nucleation and growth of plates, 386–7 stereograms construction general diagrams and triclinic application, 65–7, 66 hexagonal system, 58–9, 59 monoclinic system, axis setting conventions, 63, 63–4, 64

11/30/2011 3:17:14 PM

Index

orthorhombic system example, 50–2, 51 pole opposites and angles, 458–60 small circle, 455–8, 456, 457 Wulff net graphical aid, 460–3 conventional symbols, 44–5, 45, 48 of crystallographic point groups, 46–7, 48 glide system depiction, 219–22, 220, 221 projection geometry, 451–5, 453 properties, proof of, 465–7, 466, 467 stiffness constants, 182–4, 188, 190 strain anelastic, 326–7, 329 definitions, 165–6, 166 elastic, produced by applied stress, 181, 182, 183 energy, stored in dislocation, 269–72, 270 homogeneous, 166, 200, 208–9, 328 infinitesimal, 166–70 in martensite plates and lattices, 365–6 combined with rotation, 372–4, 373, 375 pure and observed lattice strains, 370–2, 371, 372 in multiple twinning, 357 strained layer epitaxy, 424–8, 425 stress calculation, 172, 172–3 chemical (in dislocation), 252–3 components, definition and notation, 170–2, 171, 174, 175, 176 contracted notation, 178, 182–3 hydrostatic and deviatoric, 176 fields, on intersecting dislocations, 264, 278 homogeneous, 174 pure shear, 174–5, 175 related to strain (Hooke’s law), 181–2, 254–5 Strukturbericht designation (crystal structure), 116–17, 119 subgroups, 79 substitution of cations, in garnet structures, 108–9 of metals, in solid solutions, 110–11, 111

Kelly_bindex.indd 519

519

superconducting materials, crystal structures, 105 superelasticity, 378, 383 supergroups, 79 superlattices, 112–13, 114, 114 surface free energy, 394, 396 at interface junctions, 409–11, 410 measurement, 394–7, 395 related to equilibrium crystal shape (Wulff theorem), 414–16, 415 and twin boundaries, 413–14, 414 surfaces atomic bonding and energy plots, 392–4, 393, 394 interfacial simulation, 406–8 definition and alternative structures, 391–2, 392 growth rates, 417–18 outer, reconstruction, 391 see also grain boundaries symmetric tensors, 148–9, 154–5 symmetry elements crystals, macroscopic level, 3, 43–8 of defects, 328–9 groups, subgroups and supergroups, 79 limitations on crystal physical properties, 153–5, 156 notation and nomenclature, 78–9 operation types, 14–16, 43–4 restrictions, in crystals, 16–21, 17 slip system families, 203–5 space group descriptions, 69–78 syndiotactic polymers, 115 tactic polymers, 115 tensile strains, 169, 192, 326 tension dislocation line, 274–7, 275 and glide, in metal crystals, 222–6, 223, 225 tensors principal axes and components, 149 transformation operations, 142–5, 144–5 types and ranks, 141–2, 161, 167, 177 see also second-rank tensors

11/30/2011 3:17:14 PM

520

Index

tetrad (four-fold) axis of symmetry, 18, 20 tetragonal crystal system, 28, 30 elastic constants, 189 planar spacing, 471 point group symmetry elements, 52–3 tetrahedral interstices, 89, 90, 91, 92–3 texture, 228–9, 230–1, 232–5 thermal faceting, 416–17, 417 thermoelastic martensite, 386 Thompson’s tetrahedron, 282, 282–4, 288 tilt boundaries asymmetrical, 401–3, 402 rotated (twist), 403, 403–5 symmetrical, 397–401, 398, 401 tin (a- and b-Sn), crystal structures, 94–5 titanium dioxide (rutile), crystal structure, 103–4, 104, 133 martensitic transformation, metal and alloys, 369, 374, 375, 383 topologically close-packed (TCP) structures, 135, 136 torque terms, grain interface junctions, 410–11, 411, 413 transformation formula (tensor components), 148, 152, 154, 170 transformation toughening, 384 translation glide, 199–203, 200 translational symmetry, 6, 15, 43 combined with rotation/inversion (space groups), 69–78 triad (three-fold) axis of symmetry, 18, 20–1 triclinic crystal system, 27, 28 elastic constants, 184–5 planar spacing, 470 point group symmetry elements, 65–7, 66 property representation quadric, 159 trigonal crystal system lattice symmetry and unit cells, 26, 33, 33–5, 34 planar spacing, 471 point group symmetry elements, 59–62, 60 special forms, 62, 62

Kelly_bindex.indd 520

use of rhombohedral/hexagonal axes, 60–2, 71, 477–9, 478 tungsten, elastic isotropy, 256 twinned crystals crystal morphology, 354–8 geometric elements, 339, 339–42, 347–8, 350–4 martensitic lamellae, 376–8, 377 occurrence and causes, 335, 336–7 structure, examples of, 342–6, 349–50 twist boundaries, 403, 403–5 two-surface analysis, 201, 464–5, 465 unit cells, 3–7 of cellular solid materials, 139 conventional, in crystal systems, 26, 26 electron density, 85 of ordered solid solutions, 112, 112 rhombohedral and hexagonal, in trigonal crystals, 60, 60–2, 61, 71, 477–9 of tactic polymers, 115, 117 transformation of indices (directions and planes), 473–5 unit parallelogram, 5 unit quaternions, 22–3, 449 uranium, twinning, 340–1 vacancies, 305 binding energy, 310–11 configuration models, 312–13, 313, 313 and dislocation forces, 252–3 dislocation loops, in hexagonal metals, 292, 292 formation energy calculation, 307 positions and generation, 306–7, 307 related to electrical charge, 289–90, 290 vapour deposition, 229, 336, 423 vectors definition and components, 435–6, 436 director, in liquid crystal alignment, 127, 129 lattice translation, 15 related to crystal lattice planes, 11–14, 440–3, 441 scalar product, 436–8

11/30/2011 3:17:14 PM

Index

transformation of components, 142–4, 143, 146 dummy suffix notation, 145–6 vector product operations, 438–40, 439 triple product formula, 226, 439 von Mises condition, 217 Voronoi polyhedra, 124–6, 125 wavy glide, 205, 208, 215 Weaire–Phelan structure, 418, 419 Weiss zone law, 11–14, 62 white tin (b-Sn), crystal structure, 94–5 Wulff net, 460–1, 461, 462, 463 Wulff plot, crystal/grain shape, 414–17, 415 wurtzite (b-ZnS)

Kelly_bindex.indd 521

521

crystal structure, 100, 101, 101, 497 surfaces, 392, 392 stacking faults and dislocations, 299 Young’s modulus (E), 189, 192, 427 zeolites, 137, 138 zinc, twinning, 346, 349 zinc-blende see sphalerite zirconium martensitic transformations, 369–74, 375 oxide (zirconia), transformation toughening, 384 twinning, 346, 349 zone addition rule, 14, 51–2 zones, of crystal lattice planes, 12–14

11/30/2011 3:17:14 PM

Kelly_ffirs.indd i

11/29/2011 4:19:54 PM

Crystallography and Crystal Defects Second Edition

ANTHONY KELLY Fellow of Churchill College

and

KEVIN M. KNOWLES Fellow of Churchill College

Department of Materials Science and Metallurgy University of Cambridge

Kelly_ffirs.indd iii

11/29/2011 4:19:54 PM

This edition first published 2012 © 2012 John Wiley & Sons, Ltd Registered Office John Wiley & Sons, Ltd, The Atrium, Southern Gate, Chichester, West Sussex, PO19 8SQ, United Kingdom For details of our global editorial offices, for customer services and for information about how to apply for permission to reuse the copyright material in this book please see our website at www.wiley.com. The right of the author to be identified as the author of this work has been asserted in accordance with the Copyright, Designs and Patents Act 1988. All rights reserved. No part of this publication may be reproduced, stored in a retrieval system, or transmitted, in any form or by any means, electronic, mechanical, photocopying, recording or otherwise, except as permitted by the UK Copyright, Designs and Patents Act 1988, without the prior permission of the publisher. Wiley also publishes its books in a variety of electronic formats. Some content that appears in print may not be available in electronic books. Designations used by companies to distinguish their products are often claimed as trademarks. All brand names and product names used in this book are trade names, service marks, trademarks or registered trademarks of their respective owners. The publisher is not associated with any product or vendor mentioned in this book. This publication is designed to provide accurate and authoritative information in regard to the subject matter covered. It is sold on the understanding that the publisher is not engaged in rendering professional services. If professional advice or other expert assistance is required, the services of a competent professional should be sought. The publisher and the author make no representations or warranties with respect to the accuracy or completeness of the contents of this work and specifically disclaim all warranties, including without limitation any implied warranties of fitness for a particular purpose. This work is sold with the understanding that the publisher is not engaged in rendering professional services. The advice and strategies contained herein may not be suitable for every situation. In view of ongoing research, equipment modifications, changes in governmental regulations, and the constant flow of information relating to the use of experimental reagents, equipment, and devices, the reader is urged to review and evaluate the information provided in the package insert or instructions for each chemical, piece of equipment, reagent, or device for, among other things, any changes in the instructions or indication of usage and for added warnings and precautions. The fact that an organization or Website is referred to in this work as a citation and/or a potential source of further information does not mean that the author or the publisher endorses the information the organization or Website may provide or recommendations it may make. Further, readers should be aware that Internet Websites listed in this work may have changed or disappeared between when this work was written and when it is read. No warranty may be created or extended by any promotional statements for this work. Neither the publisher nor the author shall be liable for any damages arising herefrom. Library of Congress Cataloging-in-Publication Data Kelly, A. (Anthony) Crystallography and crystal defects / Anthony Kelly and Kevin M. Knowles. – 2nd ed. p. cm. Includes bibliographical references and index. ISBN 978-0-470-75015-5 (cloth) – ISBN 978-0-470-75014-8 (pbk.) 1. Crystallography. 2. Crystals–Defects. I. Knowles, Kevin M. II. Title. QD931.K4 2012 548′.8–dc23 2011034130 A catalogue record for this book is available from the British Library. HB ISBN: 9780470750155 PB ISBN: 9780470750148 Set in 10/12pt Times by SPi Publisher Services, Pondicherry, India

Kelly_ffirs.indd iv

11/29/2011 4:19:54 PM

Contents Preface to the Second Edition Part I

Perfect Crystals

xiii 1

1 Lattice Geometry 1.1 The Unit Cell 1.2 Lattice Planes and Directions 1.3 The Weiss Zone Law 1.4 Symmetry Elements 1.4.1 Translational Symmetry 1.4.2 Rotational Symmetry 1.4.3 Reflection Symmetry 1.5 Restrictions on Symmetry Elements 1.6 Possible Combinations of Rotational Symmetries 1.7 Crystal Systems 1.8 Space Lattices (Bravais Lattices) Problems Suggestions for Further Reading References

3 3 7 11 14 15 15 16 16 21 26 26 37 40 41

2 Point Groups and Space Groups 2.1 Macroscopic Symmetry Elements 2.2 Orthorhombic System 2.3 Tetragonal System 2.4 Cubic System 2.5 Hexagonal System 2.6 Trigonal System 2.7 Monoclinic System 2.8 Triclinic System 2.9 Special Forms in the Crystal Classes 2.10 Enantiomorphous Crystal Classes 2.11 Laue Groups 2.12 Space Groups 2.13 Nomenclature for Point Groups and Space Groups 2.14 Groups, Subgroups and Supergroups 2.15 An Example of a Three-Dimensional Space Group

43 43 49 52 53 56 59 63 65 67 68 69 69 78 79 79

Kelly_ftoc.indd v

11/14/2011 12:14:28 PM

vi

Contents

Problems Suggestions for Further Reading References

Kelly_ftoc.indd vi

82 84 84

3 Crystal Structures 3.1 Introduction 3.2 Common Metallic Structures – 3.2.1 Cubic Close-Packed (Fm3m) 3.2.2 Hexagonal Close-Packed (P63 /mmc) 3.2.3 Double Hexagonal Close-Packed (P63 /mmc) – 3.2.4 Body-Centred Cubic (Im3m) 3.3 Related Metallic Structures 3.3.1 Indium (I4/mmm) – 3.3.2 Mercury (R3m) 3.3.3 b-Sn (I41/amd) 3.4 Other Elements and Related Compounds – 3.4.1 Diamond (Fd3m) 3.4.2 Graphite (P63 /mmc) 3.4.3 Hexagonal Boron Nitride (P63 /mmc) – 3.4.4 Arsenic, Antimony and Bismuth (R3m) 3.5 Simple MX and MX2 Compounds – 3.5.1 Sodium Chloride, NaCl (Fm3m) – 3.5.2 Caesium Chloride, CsCl (Pm3m) – 3.5.3 Sphalerite, a-ZnS (F43m) 3.5.4 Wurtzite, b-ZnS (P63mc) 3.5.5 Nickel Arsenide, NiAs (P63/mmc) – 3.5.6 Calcium Fluoride, CaF2 (Fm3m) 3.5.7 Rutile, TiO2 (P42/mnm) 3.6 Other Inorganic Compounds – 3.6.1 Perovskite (Pm3m) – – 3.6.2 a-Al2O3 (R3c), FeTiO3 (R3) and LiNbO3 (R3c) – 3.6.3 Spinel (Fd3m), Inverse Spinel and Related Structures – 3.6.4 Garnet (Ia3d) – 3.6.5 Calcite, CaCO3 (R3c) 3.7 Interatomic Distances 3.8 Solid Solutions 3.9 Polymers 3.10 Additional Crystal Structures and their Designation Problems Suggestions for Further Reading References

85 85 86 86 90 92 92 93 93 94 94 95 95 95 97 97 98 98 99 100 101 101 102 103 104 104 105 106 107 109 110 110 113 116 119 121 122

4 Amorphous Materials and Special Types of Crystal–Solid Aggregates 4.1 Introduction 4.2 Amorphous Materials 4.3 Liquid Crystals

123 123 123 126

11/14/2011 12:14:28 PM

Contents

4.4 4.5 4.6 4.7 4.8

4.3.1 Nematic Phases 4.3.2 Cholesteric Phases 4.3.3 Smectic Phases Geometry of Polyhedra Icosahedral Packing Quasicrystals 4.6.1 A Little Recent History and a New Definition Incommensurate Structures Foams, Porous Materials and Cellular Materials Problems Suggestions for Further Reading References

vii

127 129 129 129 134 135 136 137 137 139 139 140

5 Tensors 5.1 Nature of a Tensor 5.2 Transformation of Components of a Vector 5.3 Dummy Suffix Notation 5.4 Transformation of Components of a Second-Rank Tensor 5.5 Definition of a Tensor of the Second Rank 5.6 Tensor of the Second Rank Referred to Principal Axes 5.7 Limitations Imposed by Crystal Symmetry for Second-Rank Tensors 5.8 Representation Quadric 5.9 Radius–Normal Property of the Representation Quadric 5.10 Third- and Fourth-Rank Tensors Problems Suggestions for Further Reading References

141 141 142 145 146 148 149 153 155 159 161 161 163 163

6 Strain, Stress, Piezoelectricity and Elasticity 6.1 Strain: Introduction 6.2 Infinitesimal Strain 6.3 Stress 6.4 Piezoelectricity 6.4.1 Class 2 6.4.2 Class 222 6.4.3 Class 23 6.4.4 Class 432 6.4.5 The Converse Effect 6.5 Elasticity of Crystals – 6.5.1 Class 1 6.5.2 Class 2 6.5.3 Class 222 6.5.4 Class 23 Problems Suggestions for Further Reading References

165 165 166 170 177 179 179 180 180 181 181 184 185 185 186 193 196 196

Kelly_ftoc.indd vii

11/14/2011 12:14:28 PM

viii

Contents

Part II

Imperfect Crystals

7 Glide and Texture 7.1 Translation Glide 7.2 Glide Elements 7.3 Independent Slip Systems 7.4 Large Strains of Single Crystals: The Choice of Glide System 7.5 Large Strains: The Change in the Orientation of the Lattice During Glide 7.6 Texture Problems Suggestions for Further Reading References

199 199 203 208 218

8 Dislocations 8.1 Introduction 8.2 Dislocation Motion 8.3 The Force on a Dislocation 8.4 The Distortion in a Dislocated Crystal 8.5 Atom Positions Close to a Dislocation 8.6 The Interaction of Dislocations with One Another Problems Suggestions for Further Reading References

241 241 247 249 253 258 261 265 266 267

9 Dislocations in Crystals 9.1 The Strain Energy of a Dislocation 9.2 Stacking Faults and Partial Dislocations 9.3 Dislocations in C.C.P. Metals 9.4 Dislocations in the Rock Salt Structure 9.5 Dislocations in Hexagonal Metals 9.6 Dislocations in B.C.C. Crystals 9.7 Dislocations in Some Covalent Solids 9.8 Dislocations in Other Crystal Structures Problems Suggestions for Further Reading References

269 269 277 280 288 290 295 297 301 301 303 303

10 Point Defects 10.1 Introduction 10.2 Point Defects in Ionic Crystals 10.3 Point Defect Aggregates 10.4 Point Defect Configurations 10.5 Experiments on Point Defects in Equilibrium 10.6 Experiments on Quenched Metals 10.7 Radiation Damage

Kelly_ftoc.indd viii

197

222 228 235 237 237

305 305 309 310 312 317 321 324

11/14/2011 12:14:28 PM

Contents

10.8

Anelasticity and Point Defect Symmetry Problems Suggestions for Further Reading References

ix

326 329 331 331

11

Twinning 11.1 Introduction 11.2 Description of Deformation Twinning 11.3 Examples of Twin Structures 11.3.1 C.C.P. Metals 11.3.2 B.C.C. Metals 11.3.3 Sphalerite (Zinc Blende) 11.3.4 Calcite 11.3.5 Hexagonal Metals 11.3.6 Graphite 11.4 Twinning Elements 11.5 The Morphology of Deformation Twinning Problems Suggestions for Further Reading References

335 335 337 342 342 342 344 345 346 346 350 354 358 360 360

12

Martensitic Transformations 12.1 Introduction 12.2 General Crystallographic Features 12.3 Transformation in Cobalt 12.4 Transformation in Zirconium 12.5 Transformation of Indium–Thallium Alloys 12.6 Transformations in Steels 12.7 Transformations in Copper Alloys 12.8 Transformations in Ni–Ti-Based Alloys 12.9 Transformations in Nonmetals 12.10 Crystallographic Aspects of Nucleation and Growth Problems Suggestions for Further Reading References

363 363 364 366 369 374 379 382 383 384 385 387 388 389

13

Crystal Interfaces 13.1 The Structure of Surfaces and Surface Free Energy 13.2 Structure and Energy of Grain Boundaries 13.3 Interface Junctions 13.4 The Shapes of Crystals and Grains 13.5 Boundaries between Different Phases 13.6 Strained Layer Epitaxy of Semiconductors Problems Suggestions for Further Reading References

391 391 397 409 414 420 424 429 431 431

Kelly_ftoc.indd ix

11/14/2011 12:14:28 PM

x

Kelly_ftoc.indd x

Contents

Appendix 1 Crystallographic Calculations A1.1 Vector Algebra A1.1.1 The Scalar Product A1.1.2 The Vector Product A1.2 The Reciprocal Lattice A1.3 Matrices A1.4 Rotation Matrices and Unit Quaternions References

435 435 436 438 440 443 448 449

Appendix 2 The Stereographic Projection A2.1 Principles A2.2 Constructions A2.2.1 To Construct a Small Circle A2.2.2 To Find the Opposite of a Pole A2.2.3 To Draw a Great Circle through Two Poles A2.2.4 To Find the Pole of a Great Circle A2.2.5 To Measure the Angle between two Poles on an inclined Great Circle A2.3 Constructions with the Wulff Net A2.3.1 Two-Surface Analysis A2.4 Proof of the Properties of the Stereographic Projection References

451 451 455 455 458 458 459

Appendix 3 Interplanar Spacings and Interplanar Angles A3.1 Interplanar Spacings A3.1.1 Triclinic A3.1.2 Monoclinic A3.1.3 Orthorhombic A3.1.4 Trigonal A3.1.5 Tetragonal A3.1.6 Hexagonal A3.1.7 Cubic A3.2 Interplanar Angles A3.2.1 Orthorhombic A3.2.2 Hexagonal A3.2.3 Cubic

469 469 470 470 470 471 471 471 471 472 472 472 472

Appendix 4 Transformation of Indices Following a Change of Unit Cell A4.1 Change of Indices of Directions A4.2 Change of Indices of Planes A4.3 Example 1: Interchange of Hexagonal and Orthorhombic Indices for Hexagonal Crystals A4.4 Example 2: Interchange of Rhombohedral and Hexagonal Indices

473 473 475

460 460 464 465 468

476 477

11/14/2011 12:14:29 PM

Contents

Appendix 5 Slip Systems in C.C.P. and B.C.C. Crystals A5.1 Independent Glide Systems in C.C.P. Metals – A5.1.1 Example: Slip Along [110] on the (111) Slip Plane A5.1.2 Number of Independent Glide Systems A5.2 Diehl’s Rule and the OILS Rule – A5.2.1 Use of Diehl’s Rule for {111} Slip (Such as C.C.P. Metals) – A5.2.2 Use of Diehl’s Rule for {110} Slip (Such as B.C.C. Metals) A5.2.3 The OILS Rule A5.3 Proof of Diehl’s Rule and the OILS Rule References

xi

481 481 481 482 483 484 484 484 485 486

Appendix 6 Homogeneous Strain A6.1 Simple Extension A6.2 Simple Shear A6.3 Pure Shear A6.4 The Relationship between Pure Shear and Simple Shear

487 488 488 489 489

Appendix 7 Crystal Structure Data A7.1 Crystal Structures of the Elements, Interatomic Distances and Six-Fold Coordination-Number Ionic Radii A7.2 Crystals with the Sodium Chloride Structure A7.3 Crystals with the Caesium Chloride Structure A7.4 Crystals with the Sphalerite Structure A7.5 Crystals with the Wurtzite Structure A7.6 Crystals with the Nickel Arsenide Structure A7.7 Crystals with the Fluorite Structure A7.8 Crystals with the Rutile Structure

491 491 495 496 497 497 497 498 498

Appendix 8 Further Resources A8.1 Useful Web Sites A8.2 Computer Software Packages

499 499 499

Brief Solutions to Selected Problems

501

Index

509

Kelly_ftoc.indd xi

11/14/2011 12:14:29 PM

Preface to the Second Edition This fully revised and updated edition has been prepared by a very active worker in the field, who has used previous editions extensively both in teaching and in research, together with one of the original authors. Since the first edition, written in the late 1960s, understanding of crystal defects such as dislocations, stacking faults, twin, grain and interphase boundaries and of their effect on the mechanical and electrical properties of materials has grown enormously and has been accompanied by a total change in style of the way in which both research and teaching are carried out through the use of the fast digital computer. This edition takes account of this change. It provides a fully updated account of basic crystallography and of structural imperfections in materials, while ensuring that it remains accessible to both undergraduate and postgraduate students and to others wishing to have a basic understanding of crystallography and why this subject is important when dealing with real (i.e. imperfect) materials. This edition has discussions of a number of new topics not covered in previous editions such as piezoelectricity, groups, subgroups and supergroups, liquid crystals, incommensurate materials and the structure of foamed and amorphous materials, and martensitic transformations in nickel–titanium shape memory alloys and zirconia ceramics. The topic of quasicrystalline materials, covered briefly in the revised edition published in 2000, has been rewritten and linked to discussions of icosahedral packing and the understanding of topologically close-packed structures. Constructions involving the stereographic projection have been moved to an appendix. It is now usual to produce stereographic projections via proprietary software packages. Accounts of three-dimensional coordinate geometry and spherical trigonometry have been rewritten using vector algebra, matrix algebra and quaternions. Such algebra is also amenable to the use of spreadsheets. Tables of data and references in previous editions have been meticulously checked and updated. Numbered references are listed in full at the end of each chapter, together with suggestions for further reading. The problems at the end of each chapter have been reviewed and updated. Brief solutions to these are given after the appendices. More detailed worked solutions are available on the password protected Wiley Web page accompanying this book at http://booksupport.wiley.com. Lists of websites and computer software packages relevant to the topics we have covered here are given in a new appendix. The authors are extremely grateful to those who have helped to foster our interest in crystallography. AK would like to thank in particular the late Geoffrey Groves, co-author of the first edition, as well as Patricia Kidd, co-author of the revised edition published in 2000; KMK would like to thank the late David Smith, his DPhil supervisor at Oxford, and also a former PhD student of AK.

Kelly_fpref.indd xiii

11/29/2011 3:40:26 PM

xiv

Preface

We are both grateful to James Elliott for his great help with preparing diagrams of polymer crystals and to other colleagues from both of our departments at Cambridge and at Churchill College, Cambridge for their advice and encouragement. In attempting to strike a balance between general background knowledge, specialist research knowledge and succinctness of description, we have inevitably had to make compromises in every chapter; each could have been a separate volume. We hope the reader whose understanding of crystallography and crystal defects goes well beyond what we have described here will nevertheless find parts where we have enriched his or her knowledge. Finally, we hope that all readers will enjoy reading this book as much as we have enjoyed both its writing and its revision. Anthony Kelly Kevin M. Knowles

Kelly_fpref.indd xiv

11/29/2011 3:40:27 PM

Part I Perfect Crystals

Kelly_p01.indd 1

11/29/2011 4:12:52 PM

1 Lattice Geometry

1.1 The Unit Cell Crystals are solid materials in which the atoms are regularly arranged with respect to one another. This regularity of arrangement can be described in terms of symmetry elements; these elements determine the symmetry of the physical properties of a crystal. For example, the symmetry elements show in which directions the electrical resistance of a crystal will be the same. Many naturally occurring crystals, such as halite (sodium chloride), quartz (silica) and calcite (calcium carbonate), have very well-developed external faces. These faces show regular arrangements at a macroscopic level, which indicate the regular arrangements of the atoms at an atomic level. Historically, such crystals are of great importance because the laws of crystal symmetry were deduced from measurements of the interfacial angles in them; measurements were first carried out in the seventeenth century. Even today, the study of such crystals still possesses some heuristic advantages in learning about symmetry. Nowadays the atomic pattern within a crystal can be studied directly by techniques such as high-resolution transmission electron microscopy. This atomic pattern is the fundamental pattern described by the symmetry elements and we shall begin with it. In a crystal of graphite the carbon atoms are joined together in sheets. These sheets are only loosely bound to one another by van der Waals forces. A single sheet of such atoms provides an example of a two-dimensional crystal; indeed, recent research has shown that such sheets can actually be isolated and their properties examined. These single sheets are now termed ‘graphene’. The arrangement of the atoms within a sheet of graphene is shown in Figure 1.1a. In this representation of the atomic pattern, the centre of each atom is represented by a small dot, and lines joining adjacent dots represent bonds between atoms. All of the atoms in this sheet are identical. Each atom possesses three nearest neighbours. Crystallography and Crystal Defects, Second Edition. Anthony Kelly and Kevin M. Knowles. © 2012 John Wiley & Sons, Ltd. Published 2012 by John Wiley & Sons, Ltd.

Kelly_c01.indd 3

11/30/2011 6:13:52 PM

4

Crystallography and Crystal Defects (a)

(b)

S R y

M

Y O´

O N

A

P

B

H

X Q

x

T

(c)

y b g a

x

Figure 1.1

We describe this by saying that the coordination number is 3. In this case the coordination number is the same for all the atoms. It is the same for the two atoms marked A and B. However, atoms A and B have different environments: the orientation of the neighbours is different at A and B. Atoms in a similar situation to those at A are found at N and Q; there is a similar situation to B at M and at P. It is obvious that we can describe the whole arrangement of atoms and interatomic bonds shown in Figure 1.1a by choosing a small unit such as OXAY, describing the arrangement of the atoms and bonds within it, then moving the unit so that it occupies the position NQXO and repeating the description and then moving it to ROYS and so on, until we have

Kelly_c01.indd 4

11/30/2011 6:13:53 PM

Lattice Geometry

5

filled all space with identical units and described the whole pattern. If the repetition of the unit is understood to occur automatically, then to describe the crystal we need only describe the arrangement of the atoms and interatomic bonds within one unit. The unit chosen we would call the ‘unit parallelogram’ in two dimensions (in three dimensions, the ‘unit cell’). In choosing the unit we always choose a parallelogram in two dimensions or a parallelepiped in three dimensions. The reason for this will become clear later. Having chosen the unit, we describe the positions of the atoms inside it by choosing an origin O and taking axes Ox and Oy parallel to the sides, so that the angle between Ox and Oy is ≥ 90°. We state the lengths of the sides a and b, taking a equal to the distance OX and b equal to the distance OY (Figure 1.1a), and we give the angle g between Ox and Oy. In this case a = b = 2.45 Å1 (at 25 °C) and g = 120°. To describe the positions of the atoms within the unit parallelogram, we note that there is one at each corner and one wholly inside the cell. The atoms at O, X, A, Y all have identical surroundings.2 In describing the positions of the atoms we take the sides of the parallelogram, a and b, as units of length. Then the coordinates of the atom at O are (0, 0); those at X (1, 0); those at Y (0, 1); and those at A (1, 1). The coordinates of the atom at O′ are obtained by drawing lines through O′ parallel to the axes Ox and Oy. The coordinates of O′ are therefore 13 , 23 . To describe the contents fully inside the unit parallelogram – that is, to describe the positions of the atoms – we need only give the coordinates of the atom at the origin, (0, 0), and those of the atom at O′. The reason is that the atoms at X, A and Y have identical surroundings to those at O and an atom such as O, X, A or Y is shared between the four cells meeting at these points. The number of atoms contained within the area OXAY is two. O′ is within the area, giving one atom. O, Y, A, X provide four atoms each shared between four unit cells, giving an additional 4 × 14 = 1. A second way of arriving at the same result is to move the origin of the unit cell slightly away from the centre of the atom at O so that the coordinate of the O atom is (ε1, ε2) and the coordinate of the O′ atom is 13 + ε1 , 23 + ε 2 , where 0 < ε1, ε2 90°. Close examination of the proposed structure shows that it has a monoclinic I lattice. Specify a more conventional description of the lattice type and describe the relationship of the sides of the unit cell for this new lattice type in terms of the monoclinic I unit cell.

Kelly_c01.indd 38

11/30/2011 6:15:23 PM

Lattice Geometry

39

1.5 The spinel MgAl2O4 has a = b = c = 8.11 Å and a = b = g = 90°. Crystals show – – – ––– the faces (111), (111), (111) and (111) and the faces parallel to these, namely (11 1), –– – – –– (111 ), (111) and (1 1 1 1). Such crystals look like regular or distorted octahedra. –– (a) Find the zone axis symbol (indices) of the zone containing (111) and (1 1 1). Which of the other faces listed above also lie in this zone? –– (b) Show that the zone containing (111) and (11 1) also contains (001) and (110). (c) Sketch the projection of the lattice on (001). Draw in the trace of the (110) lattice plane and the normal to the plane through the origin. Find the perpendicular distance of the first plane of this set from the origin in terms of the cell side. (d) Draw the section of the lattice through the origin which contains the normal to (110) and the normal to (001). Mark in on this section the traces of the (111), –– ––– – (11 1), (11 1) and (111) planes. Measure the angles between adjacent planes. 1.6 Find the angle between [111] and the normal to (111) in (a) a cubic crystal and (b) a tetragonal one with a = 5.67 Å, c = 12.70 Å. – 1.7 Show that the faces (111), (231) and (12 4) all lie in a zone. (a) Find the zone symbol (indices) of this zone and (b) calculate the angle between this zone and the zone [100] in the cubic system. –– 1.8 In a tetragonal crystal CuFeS2, the angle between (111) and (11 1) is 108.67°. Calculate (a) the ratio of the axial lengths and (b) the interzone angle [236]∧[001]. 1.9 Following the method of Section 1.6, determine the angles between the rotational axes in the axial combinations of (a) two triads and a diad and (b) a tetrad, a triad and a diad. Draw a sketch to show the arrangement of the symmetry elements in each case. 1.10 Show that (a) successive combinations of rotations about two different tetrad axes are unable to be expressed as a rotation about a single triad axis in crystals, and (b) successive combinations of rotations about two different triad axes are unable to be expressed as a rotation about a single tetrad axis in crystals. 1.11 The unit cell of a two-dimensional lattice has a = b, g = 120°. Dispose three atoms about each lattice point in different ways so that the two-dimensional crystal can show the following symmetries in turn: (a) a six-fold axis with mirror planes parallel to it, (b) a three-fold axis, (c) a diad axis at the intersection of two mirror planes, (d) a two-fold axis and (e) a one-fold axis. 1.12 CdI2 and CdCl2 both belong to the trigonal crystal system. The former has a primitive hexagonal lattice and the latter a rhombohedral lattice. The coordinates of the atoms associated with each lattice point are given below, using a hexagonal unit cell for both crystals: CdI 2 Cd: 0, 0, 0 I: ±

(

2 1 1 3 3 4

, ,

)

CdCl 2 Cd: 0, 0, 0 Cl: ±

( 23 , 13 , 121 )

Draw plans of the two structures on (001) and outline on your diagram for CdCl2 the projections of the cell edges of the true rhombohedral primitive unit cell.

Kelly_c01.indd 39

11/30/2011 6:15:32 PM

40

Crystallography and Crystal Defects

1.13 Show that there are three cubic lattices by following the procedure used in Section 1.8 and finding the conditions for which in Figure 1.28 triad axes lie normal to (010), (100) and (001) of the rhombohedral primitive unit cell. Hint: find the condition under which successive planes project along their normal so that the lattice points in one lie at the centroids of triangles of lattice points in that below it. 1.14 A two-dimensional crystal possesses four-fold rotational symmetry. Sketch the net. Position four atoms of an element at the net points so that the arrangement is consistent with (a) just four-fold symmetry and (b) four-fold symmetry with mirror planes parallel to the four-fold symmetry axis. Are two different arrangements of mirror planes possible in (b)? 1.15 Specify the directions of a*, b* and c* in a hexagonal crystal relative to the lattice vectors a, b and c. What is the angle between a* and b*? Determine the magnitudes of a*, b* and c* in terms of the lattice parameters a and c. Using the formula |t*hkℓ| = 1/dhkℓ, show that the interplanar spacing of the hkl planes in an hexagonal crystal is given by the formula: 1 dhk 2

= (h2 + k 2 + hk )

4 3a 2

+

l2 c2

Hence show that the planes (hkl), (h,−(h+k),l) and (k,−(h+k),l) have the same interplanar spacing. 1.16 Show that in a triclinic crystal the vector [uvw] is parallel to the normal to the plane (hkl) if: ⎛ h⎞ ⎛ a 2 ab cos γ ⎜ ⎟ ⎜ b2 ⎜ k ⎟ = ⎜ ab cos γ ⎜ ⎟ ⎜ ⎜⎝ l ⎟⎠ ⎝ ac cos β bc cos α

ac cos β ⎞ ⎟ bc cos α ⎟ c 2 ⎟⎠

⎛ u⎞ ⎜ ⎟ ⎜ v⎟ ⎜ ⎟ ⎜⎝ w⎟⎠

Determine u, v and w in terms of h, k, l, a, b and g . Hint: it is useful to define an orthonormal set of vectors with respect to which the basis vectors a, b and c of the triclinic crystal are defined. 1.17 Using the hint in Problem 1.16, or otherwise, confirm that the volume, V, of the unit cell of a triclinic crystal with cell dimensions a, b, c, a, b and γ is given by the formula: V = abc 1 − cos2 α − cos2 β − cos2 γ + 2 cos α cos β cos γ

Suggestions for Further Reading S.M. Allen and E.L. Thomas (1999) The Structure of Materials, John Wiley and Sons, New York. M.J. Buerger (1963) Elementary Crystallography, John Wiley and Sons, New York. M.J. Buerger (1970) Contemporary Crystallography, McGraw-Hill, New York.

Kelly_c01.indd 40

11/30/2011 6:15:33 PM

Lattice Geometry

41

C. Giacovazzo (ed.) (2011) Fundamentals of Crystallography (International Union of Crystallography Texts on Crystallography – 15), 3rd Edition, Oxford University Press, Oxford. C. Hammond (2009) The Basics of Crystallography and Diffraction (International Union of Crystallography Texts on Crystallography – 12), 3rd Edition, Oxford University Press, Oxford. F.C. Phillips (1971) Introduction to Crystallography, 4th Edition, Oliver & Boyd, Edinburgh. J.-J. Rousseau (1998) Basic Crystallography, John Wiley and Sons, Chichester.

References [1] M.J. Buerger (1963) Elementary Crystallography, John Wiley and Sons, New York, pp. 35–45. [2] M.J. Buerger (1970) Contemporary Crystallography, McGraw-Hill, New York, pp. 24–27. [3] H. Grimmer (1974) Disorientations and coincidence rotations for cubic lattices, Acta Crystall. A, 30, 685–688. [4] S.L. Altmann (1986) Rotations, Quaternions and Double Groups, Clarendon Press, Oxford. [5] J.B. Kuipers (1999) Quaternions and Rotation Sequences, Princeton University Press, Princeton. [6] T. Hahn and A. Looijenga-Vos (2002) International Tables for Crystallography (ed. Theo Hahn), 5th, Revised Edition, Vol. A: Space-Group Symmetry, published for the International Union of Crystallography by Kluwer Academic Publishers, Dordrecht, pp. 14–16.

Kelly_c01.indd 41

11/30/2011 6:15:37 PM

2 Point Groups and Space Groups 2.1

Macroscopic Symmetry Elements

The macroscopically measured properties of a crystal, such as electrical resistance, thermal expansion, optical properties, magnetic susceptibility and the elastic constants, show a symmetry which can be defined and understood without reference to the translational symmetry elements defined by the lattice. If the translational symmetry of the crystal is disregarded, the remaining symmetry elements (such as axes of rotational symmetry, mirror planes and any centre of inversion), themselves consistent with the translational symmetry of the lattice, can be arranged into 32 consistent groups. These are the 32 crystallographic point groups. They are so called because they are consistent with translational symmetry and because all of the symmetry elements in a group pass through a single point and the operation of these elements leaves just one point unmoved – the point through which they pass. Other point groups, such as the point group symmetry of the icosahedron, which we shall consider in Chapter 4 when discussing the point group symmetries exhibited by quasicrystals, are not compatible with translational symmetry. The axes of rotational symmetry, the mirror plane and the centre of inversion are all called macroscopic symmetry elements because their presence or absence in a given crystal can be decided in principle by macroscopic tests, such as etching of the crystal, the arrangement of the external faces or the symmetry of the physical properties, without any reference to the atomic structure of the crystal. The macroscopic symmetry elements are of two kinds. A symmetry operation of the first kind, such as a pure rotation axis, when operating on a righthanded object (say) produces a right-handed object from it, and all subsequent repetitions of this object are also right-handed. A symmetry operation of the second kind repeats an enantiomorphous object from an original object. The left and right hands of the ideal external form of the human body are enantiomorphously related. The operation of reflection illustrated in Figure 1.12 is an example of a symmetry operation of the second kind since a left-handed object is repeated from an original right-handed object. Subsequent operation of the same Crystallography and Crystal Defects, Second Edition. Anthony Kelly and Kevin M. Knowles. © 2012 John Wiley & Sons, Ltd. Published 2012 by John Wiley & Sons, Ltd.

Kelly_c02.indd 43

11/30/2011 7:32:17 PM

44

Crystallography and Crystal Defects

3⫻

2p 4

2⫻ 3

2p 4

2 4

1 2p 4⫻ 4

2p 4

Figure 2.1

1

2

3

4

6

Figure 2.2

symmetry element would produce a right-handed object again and then a left-handed object, and so forth. A symmetry operation of the second kind thus involves a reversal of sense in the operation of repetition. Inversion through a centre is also an operation of the second kind. In developing the 32 crystallographic point groups it is convenient to have all the macroscopic symmetry elements represented by axes and to do this we define what are called improper rotations. These produce repetition by a combination of a rotation and an operation of inversion. We shall use rotoinversion axes. These involve rotation coupled with inversion through a centre.1 A pure rotation axis is said to produce a proper rotation. The basic operation of repetition by a rotation axis is shown schematically in Figure 2.1. An n-fold axis repeats an object by successive rotations through an angle of 2p/n. In the example shown in Figure 2.1, the axis is one of four-fold symmetry. The operation of monad, diad, triad, tetrad and hexad pure rotation axes on a single initial pole is shown in Figure 2.2. These diagrams are stereograms (see Appendix 2) with the pole of the axis at 1 It is also possible to use rotoreflection axes [1], pp. 23–30, also termed alternating axes [2], p. 117, in developing the point groups. These repeat an object by rotation coupled with reflection in a plane normal to the axis. One-fold, two-fold, three-fold, ~ ~ ~ ~ ~ ~ four-fold and six-fold rotoreflection axes are possible, usually denoted 1 (pronounced ‘one tilde’), 2 , 3 , 4 and 6 respectively. 1 is clearly equivalent to a mirror plane.

Kelly_c02.indd 44

11/30/2011 7:32:18 PM

Point Groups and Space Groups (a)

(b)

m

45

(c)

m

Centre

Figure 2.3

Figure 2.4

1 (≡ centre)

2 (≡ m)

3 (≡ 3 plus centre)

4

6 (≡ 3 m)

Figure 2.5

the centre of the primitive circle. Dots are used to represent poles in the northern hemisphere of projection related to one another by the rotation axis. The numbers below the stereograms give the shorthand labels for the axes 1, 2, 3, 4 and 6, indicating a one-fold, two-fold, three-fold, four-fold and six-fold axis, respectively. The repetition of an object by a mirror plane, symbol m, and by a centre of symmetry (or centre of inversion) is shown in Figure 2.3. In Figure 2.3a the mirror plane lies normal to the primitive circle. It is denoted by a strong vertical line | coinciding with the mirror in the stereographic projection. In Figure 2.3b the mirror coincides with the primitive; the dot representing the pole in the northern hemisphere has as its mirror image the circle shown in the southern hemisphere. In Figure 2.3c the centre of inversion is at the centre of the sphere of projection. The one-fold inversion axis is a centre of symmetry. The operation of the other rotoinversion axes is explained in Figures 2.4 and 2.5. The twofold rotation–inversion axis 2¯ shown

Kelly_c02.indd 45

11/30/2011 7:32:18 PM

46

Crystallography and Crystal Defects The 32 three-dimensional point groups Triclinic

Monoclinic (1st setting)

Tetragonal

X 1

2

4

m ( = 2)

4

2 ⁄m

4 ⁄m

X (even)

X (even) plus centre and

X (odd)

1 Monoclinic (2nd setting)

Orthorhombic

2

222

422

m

2mm

4mm

X2

Xm

X2 (even) or

Xm (even)

42m

X2 or

Xm plus centre and

Xm (odd)

2 ⁄m

mmm

4 ⁄mmm

Figure 2.6 Stereograms of the poles of equivalent general directions and of the symmetry elements of each of the 32 point groups. The z-axis is normal to the paper. (Taken from the International Tables for X-ray Crystallography, Vol. 1 [4] and adapted to conform to current notation for the two centrosymmetric point groups in the cubic crystal system.)

Kelly_c02.indd 46

11/30/2011 7:32:19 PM

Point Groups and Space Groups Trigonal

Hexagonal

47

Cubic

X 3

6

23

X

(even)

6 X

(even) plus centre and

3

X

6 ⁄m

m3

(odd)

X2 32

622

432

Xm 3m

6mm X2

(even)

or Xm

6m2

43m

(even)

X2 or

Xm

plus centre and

3m

6 ⁄mmm

Figure 2.6

Kelly_c02.indd 47

m3m

Xm

(odd)

(continued)

11/30/2011 7:32:19 PM

48

Crystallography and Crystal Defects

in Figure 2.4 repeats an object by rotation through 180° (360°/2) to give the dotted circle, – followed by inversion to give the full circle. Similarly, the threefold inversion axis 3 involves rotation through 360°/3 = 120° coupled with an inversion. In general, an n-fold rotoinversion axis n– involves rotation through an angle of 2p/n coupled with inversion through a centre. The rotation and inversion are both part of the operation of repetition and must not be considered as separate operations. The operation of the various rotoinversion axes that can occur in crystals on a single initial pole is shown in Figure 2.5, with the pole of the rotoinversion axis at the centre of the primitive circle. The following symbols are – – – used: inversion monad, 1, symbol ; inversion diad, 2, symbol ; inversion triad, 3, – – symbol ; inversion tetrad, 4 , symbol ; inversion hexad, 6, symbol . Inspection of – – Figures 2.2–2.4 shows that 1 is identical to a centre of symmetry, 2 is identical to a mirror – plane normal to the inversion diad, 3 is identical to a triad axis plus a centre of symmetry – and 6 is identical to a triad axis normal to a mirror plane (symbol 3/m, the sign ‘/m’ indicat– ing a mirror plane normal to an axis of symmetry).2 Only 4 is unique. The operation of – repetition described by 4 cannot be reproduced by any combination of a proper rotation axis and a mirror plane or a centre of symmetry. – – – – The various different combinations of 1, 2, 3, 4 and 6 pure rotation axes and 1, 2, 3, 4 and – 6 rotoinversion axes constitute the 32 point groups or crystal classes. These 32 classes are grouped into systems according to the presence of defining symmetry elements (see Table 1.3). Stereograms of each of the 32 point groups or crystal classes are given in Figure 2.6, following the current conventions of the International Tables for Crystallography [3]. With the exception of the two triclinic point groups, each point group is depicted by two stereograms. The first stereogram shows how a single initial pole is repeated by the operations of the point group and the second stereogram shows all of the symmetry elements present. The nomenclature for describing the crystal classes is as follows. X indicates a rotation axis – and X an inversion axis. X/m is a rotation axis normal to a mirror plane, Xm a rotation axis with a mirror plane parallel to it and X2 a rotation axis with a diad normal to it. X/mm indi– cates a rotation axis with a mirror plane normal to it and another parallel to it. Xm is an inversion axis with a parallel plane of symmetry. A plane of symmetry is an alternative description of a mirror plane. We shall describe each of the classes in Sections 2.2–2.8. A derivation of the 32 classes follows by noting from Sections 1.5 and 1.6 that the rotation axes consistent with translational symmetry are 1, 2, 3, 4 and 6. Individually, these give in total five crystal classes. Their consistent combinations give another six (see Table 1.2): 222, 322, 422, 622, 332 and 432, thus totalling 11. All of these 11 involve only operations of the first kind. A lattice is inherently centrosymmetric (Section 1.4) and so each of the rotation axes could be replaced by the corresponding rotoinversion axis, thus giving another five – – – – – classes: 1, 2, 3, 4 and 6. The remaining sixteen can be described as combinations of the proper and improper rotation axes. It is convenient to begin first with the three crystal systems where the angles between the axes are all 90°, then to consider the hexagonal and trigonal crystal systems, before finally turning our attention to the monoclinic and triclinic systems.

2

Our symbols are identical to those used in the International Tables for Crystallography [3], with the exception of ‘ ’, which in the International Tables is always indicated by the symbol for a mirror plane.

Kelly_c02.indd 48

11/30/2011 7:32:19 PM

Point Groups and Space Groups

2.2

49

Orthorhombic System

A crystal in this system contains three diads, which must be at right angles to one another. In Figure 2.6 they are the crystal axes. From Table 1.3 and Figures 1.19d–g, the lattice parameters may be all unequal. The point group containing just three diad axes at right angles is shown in Figure 2.6 and is designated 222. In general, a pole in a crystal belonging to this point group is repeated four times. If the indices of the initial pole are (hkl), where there is no special relationship between h, k and l, the operation of all of the symmetry elements of the point group on this –– –– –– one initial pole produces three other poles. These are (h k l), (hk l ) and (h kl ) (Figure 2.7). The assemblage of crystal faces produced by repetition of an initial crystal face with indices (hkl) is called the form hkl and is given the symbol {hkl}.3 If the assemblage of faces encloses space, the form is said to be closed; otherwise it is open. In this case {hkl} is closed. The symbol {hkl} with curly brackets means all faces of the form hkl, in this case, –– –– – – for the point group 222, (hkl), (h k l), (hk l ) and (h kl ). The form {hkl} is said to show a multiplicity of four. Then {hkl} would be said to be a general form; that is, a form that bears no special relationship to the symmetry elements of the point group. Special forms in this crystal class would be {100}, {010} and {001}; each of these forms – gives just two faces: for {100}, these would be the faces (100) and (1 0 0) (Figure 2.7). These forms are all open ones. They are easily recognized as special forms since their mul– 100 – hk0

––

hk0

––

– – – h0l h0l

hkl

– 010

– 0kl

–– hkl

001

z

–– 0kl

0kl – 0kl

– 001

––

hkl

h0l

– h0l

– hk0

010

y

hkl

hk0 100 x

Figure 2.7 A stereogram of an orthorhombic crystal of point group 222 centred on 001. The diad axes are parallel to the x-, y- and z-axes. 3

All the individual faces of the form {hkl} are crystallographically identical. In a similar way, if a single direction is given, say [uvw], then all the directions produced if the repetition operations of the point group are carried out on the initial direction are called the family of directions of the type uvw and are given the symbol 〈uvw〉.

Kelly_c02.indd 49

11/30/2011 7:32:20 PM

50

Crystallography and Crystal Defects

tiplicity is less than that of the general form. Forms such as {hk0}, {h0l} and {0kl} which have one index zero and no special relationship between the other two would also be described as special, even though, as is evident from Figure 2.7, the multiplicity of each is four, as for the general form in this crystal class. One reason for this is that these poles lie normal to a diad axis. This is a special position with respect to this axis and has the result that if a crystal grew with faces parallel only to the planes of indices {hk0}, {h0l} and {0kl}, it would appear to show mirror symmetry as well as the three diad axes. A second reason is that each of the {hk0}, {h0l} and {0kl} forms is open, while the general {hkl} form is closed. Special forms usually correspond to poles lying normal to or on an axis of symmetry, and normal to or on mirror planes, and sometimes to poles lying midway between two axes of symmetry. However, the best definition of a special form is as follows: a form is special if the development of the complete form shows a symmetry of arrangement of the poles which is higher than the one the crystal actually possesses. Special forms in all of the crystal classes are listed later, in Table 2.1. The orthorhombic system also contains the classes 2mm and mmm (Figure 2.6). The former contains two mirror planes, which must be at right angles. Two mirror planes at right angles automatically show diad symmetry along the line of intersection (Figure 2.6). – –– Since m ≡ 2, this group could be designated 2 2 2, and this is why it appears in the orthorhombic system, which is defined as possessing three diad axes. This crystal class could simply be designated mm since the diad is automatically present. However, mm2 is usually used for the later development of space groups (see Section 2.12). A crystal containing three diad axes can also contain mirrors normal to all of these without an axis of higher symmetry. Such a point group is designated mmm, or could be designated 2/mm. As can be seen from Figure 2.6, the multiplicity of the general form is now eight. The special forms {hk0}, {h0l} and {0kl} now show a lower multiplicity than the general one. The point group mmm shows the highest symmetry in the orthorhombic system. The point group showing the highest symmetry in a particular crystal system is said to be the holosymmetric class. To plot a stereogram of an orthorhombic crystal centred on 001 if given the lattice parameters a, b and c, we proceed as shown in Figure 2.8. In Figure 2.8a the poles of the (001), (010) and (100) planes are immediately inserted at the centre of the primitive and where the x- and y-axes cut the primitive, respectively. A pole (hk0) can be inserted at an angle q along the primitive to (100), as shown in Figure 2.8a, by noting from Figure 2.8b (which is a section of the crystal parallel to (001) showing the intersection of the plane (hk0) with the crystal axes) that the pole of (100) lies along OM, that (hk0) makes intercepts on the crystal axes of a/h along the x axis and b/k along the y axis, and that q is the angle between the normal to (hk0) and the normal to (100). From Figure 2.8b we have: tan θ = cot (90° − θ ) =

a /h a k = b/k b h

That is: tan (100) ^ (hk 0) = ( a / b)(k / h)

Kelly_c02.indd 50

(2.1a)

11/30/2011 7:32:20 PM

Point Groups and Space Groups

51

(a)

(b) 90°–q 001

010

y

–b k

0

N

q

Trace of (hk0)

q

hk0 –a h

q

Normal to (hk0)

90°–q 100 x

M

(d)

(c)

001 h0l

0kl

010

001

011

010

hkl hk0 311

100

100

310

Figure 2.8

where (100)∧(hk0) means the angle between the (100) and (hk0) planes; that is, the angle between the pole of (100) and the pole of (hk0). Similarly, if the lattice parameters are given, we can locate (0kl) and (h0l), since: tan (001) ^ (0 kl ) = (c / b)(k / l )

(2.1b)

tan (001) ^ (h0l ) = (c / a)(h / l )

(2.1c)

and:

These relations can be seen immediately by drawing diagrams similar to Figure 2.8b but looking along the x- and y-axes, respectively. When poles such as (h0l), (0kl) and (hk0) have been inserted on the stereogram, we can insert a pole such as (hkl) immediately by use of the zone addition rule, given in Section 1.3, Equation 1.20. If two poles (h1k1l1), (h2k2l2) both lie in the same zone with the indices [uvw] then so does the pole of the plane (mh1 + nh2, mk1 + nk2, ml1 + nl2); that is, any plane whose indices can

Kelly_c02.indd 51

11/30/2011 7:32:23 PM

52

Crystallography and Crystal Defects

be formed by taking linear combinations of the indices of two planes in a given zone can provide the indices of a further plane in that same zone (Section 1.3). In general, m and n can be positive or negative, but if m and n are both positive then the pole of the plane under consideration must lie on the great circle between the poles of (h1k1l1) and (h2k2l2): this simple result can be extremely useful when locating poles on stereographic projections such as Figure 2.7. In Figure 2.8c, after (001), (010), (100) and (hk0), (h0l), (0kl) are plotted, then to plot, say, (hkl), we note that (hkl) must lie in the zone containing (001) and (hk0), since if we multiply (001) by the number l and add the indices (00l) and (hk0) we obtain (hkl). It then follows that (hkl) lies somewhere on the great circle between (001) and (hk0). Similarly, (hkl) lies in the zone containing (0kl) and (100), since h times (100) gives (h00) and this added to (0kl) gives (hkl). Again, it is true that (hkl) lies somewhere on the great circle between (0kl) and (100), but we can now rationalise that (hkl) must lie at the intersection of the two great circles we have considered. We then draw the great circle (or zone) containing (001) and (hk0) and that containing (001) and (0kl) and we know that (hkl) is situated where these intersect. A particular example may make the procedure clear. Suppose we wish to locate (311) after plotting (001), (010) and (100) (Figure 2.8d). One way to proceed would be to locate (011) using Equation 2.1b, setting k = 1 and l = 1 and using the known lattice parameters. We then find (310), on the primitive, by finding the angle between (100) and (310) from Equation 2.1a, setting h = 3 and k = 1. Finally, we note that (311) lies in the zone containing (001) and (310), since (001) plus (310) yields (311). Also, (311) lies in the zone containing (100) and (011) since three times (100) plus (011) yields (311). The pole of (311) is then immediately located by drawing the great circle through (001) and (310) and that through (011) and (100); (311) is located where these great circles meet. Using the above procedure for locating poles is usually the quickest way to draw an accurate stereogram when key poles have been located either by calculation or through the use of a computer software package. It must be strongly emphasized that, although we have chosen the orthorhombic system as an example, the use of Equation 1.20 to locate poles applies to any crystal system and does not depend on the crystal axes being at any particular angle to one another. The utility of Equation 1.20 is one of the great advantages of the Miller index for denoting crystal planes, and arises naturally from the properties of a space lattice. Equations such as Equation (2.1) can of course be used to find the ratio of the lattice parameters – the axial ratios – from measurements of the angles between poles.

2.3 Tetragonal System The tetrad axis is always taken parallel to the z-axis. The lattice parameters a and b are equal. The holosymmetric point group is 4/mmm, showing three mutually perpendicular mirror planes with a tetrad normal to one of them (Figure 2.6). If a single pole is repeated according to the presence of these symmetry elements it will be found that diad axes are necessarily present normal to the mirrors and that, in addition, a second pair of diad axes also

Kelly_c02.indd 52

11/30/2011 7:32:25 PM

Point Groups and Space Groups

53

normal to mirror planes automatically arises. One of the pairs of mutually perpendicular diads is chosen as defining the directions of the x- and y-axes. The general form is {hkl}, with a multiplicity of 16. Special forms are {001}, {100}, {110}, {hk0}, {h0l} and {hhl}. The last of these, {hhl}, indicates a face making equal intercepts on the x- and y-axes. The point group 422 could be specified simply as 42 since if 4 and 2 are present at right angles a second pair of diad axes arises and one of these pairs is chosen to define the x- and – – y-axes. The group 4 2m can be developed as 4 m. It is then found that diad axes automatically arise at 45° to the two, mutually perpendicular, mirror planes. The pair of diad axes is taken – to define the x- and y-axes. The four other tetragonal point groups, 4, 4 , 4/m and 4mm, are straightforward and no diad axes arise. The angles between poles on a stereogram and the ratio of the lattice parameters (i.e. the ratio a : c in this crystal system) are easily related by using equations such as Equation 2.1 with a = b.

2.4

Cubic System

Cubic crystals possess four triad axes as a minimum symmetry requirement. These are arranged as in Figure 1.30 and are always taken to lie along the type directions of the unit cell, which is a cube, so a = b = c. This is the only crystal system in which the direction [uvw] necessarily coincides with the normal to the plane (uvw) for all u, v, w. If we put four triad axes to coincide with the 〈111〉 directions on a stereogram and allow these to operate on a single pole, as in Figure 2.9, we find that diad axes automatically arise along the crystal axes. The presence of the diads also follows from Table 1.2, with the row starting 233. The point group symbol used to describe the combination of a diad and two triads, shown in Table 1.2, is just 23. This is the cubic point group of lowest symmetry. The multiplicity of the general form for this point group is 12 (Figure 2.9). A feature of the – symbols for describing point groups in the cubic system is that the symbol 3 or 3, even though it indicates the defining axis for the system, is never placed first because the triads,

Figure 2.9

Kelly_c02.indd 53

11/30/2011 7:32:26 PM

54

Crystallography and Crystal Defects (a)

(b) m

m m

Figure 2.10

or inverse triads, are always at 54.74° (cos −1 (1/ 3)) to the crystal axes. (In all other systems the defining axis comes first in the symbol – the presence of the diads or inverse diads parallel to at least two axes must be stated to distinguish orthorhombic point groups from monoclinic point groups.) – The figure 3 (or 3) always occurs second in the symbol for cubic point groups, and this enables a point group in the cubic system to be distinguished from those in all other crystal systems. In a cubic crystal mirror planes can run either parallel to {1 0 0} planes, as in Figure 2.10a, or else parallel to {1 1 0} planes, as in Figure 2.10b. The first alternative is – – described by putting the symbol m before 3 (to give m3) and the second by placing m after – – – the 3 (or 3) to give X3m or X3m, where X is an axis other than 3 or 3. If we add mirror planes parallel to {100} to the class 23 we obtain 2/m3, conventionally – denoted m3. (Prior to the most recent revision of the International Tables for Crystallography in 1995 this point group was denoted m3; older textbooks will use this terminology as well.) As is evident from Figure 2.6, this contains a centre of symmetry in addition to the three diads at the intersection of three mutually perpendicular mirror planes – and the four triads. The triads therefore become inversion triads, 3. The multiplicity of the general form {hkl} is 24. It is worth noting from Table 2.3 (see below) that when there are no diads along 〈110〉 nor mirrors parallel to {110}, {hk0} and {kh0} are separate special – forms. This occurs in the classes 23 and m3. Replacement of the diads in 23 by tetrads gives 43. Here we notice that diads automatically arise along the 〈110〉 directions, as tabulated in Table 1.2. This class is denoted 432 to indicate the diads because of later development of space groups (see Section 2.11). However, 43 is sufficient to identify it. – Replacement of 2 by 4 in 23 will be found to produce mirror planes automatically parallel to the {110} planes, and hence passing through the triads. Correspondingly, if mirrors – parallel to {110} are added to 23 then the diad axes along the directions become 4 axes. If we have mirror planes passing through the triad axes then parallel to the crystal – – – axes we can have either 4 or 4. The first of these classes is 4 3m and the second m3m. (This latter point group was known as m3m conventionally prior to the 1995 revision of the International Tables for Crystallography.) In 4¯ 3m there is no centre of symmetry and there are no additional symmetry elements, other than those indicated in the symbol.

Kelly_c02.indd 54

11/30/2011 7:32:26 PM

Point Groups and Space Groups

55

100 210

]

210

[0

12

[02

[0 2 1

1]

12

[0

]

]

110

110 321

[1 02 ]

132

[20

312

312 201

] 321

[111

0]

121

111

231

221 211 [1 10 ] [ 1 321 11]

[21

0]

120

110

0]

1]

[01

[12

110

[12

212

101

122

]

211

112

]

01

[1

132

[111

221

212

]

111

231

11

]

213

213

010

[100]

[0

02

[1

102

112

122

121

1]

021

011

123

123

132

[10

132

012

001

121

122 123

012

011

[1 [111] 10 ]

112

102

123

021

1]

213

213

[010]

]

0]

112

122

120

231

111

212

212

111

[201

[21

221

101

121

120

211 312

312

231

010

201

211

221 120

321

210

210 100

Figure 2.11

Stereogram of a cubic crystal. (From [5], p. 82. Copyright 1959.)

– – The multiplicity of the general form is 24. In 4 3m (as in 23), {111} and {111} are separate special forms: each shows four planes parallel to the surfaces of a regular tetrahedron. – Class m3m has mirror planes parallel to {100} and to {110}; thus nine are present in all. There are six diads, three tetrads, a centre and of course the four triads. All of these can be produced by putting mirrors parallel to both {110} and {100}, coupled with the four triads. – Hence the symbol m3m is used to describe this point group, which is the cubic holosym– metric class. In full notation this would be 4/m 3 2/m, to denote the point group symmetry – elements as 4/m along the directions, 3 along the directions and 2/m along the directions. The general form has 48 faces. A stereogram of a cubic crystal with the poles of a number of faces indicated, along with the zones in which they lie, is shown in Figure 2.11. Additional poles are easily located on a stereogram, such as that in Figure 2.11, by use of the zone addition rule explained in Section 1.3 (Equation 1.20 and following) and used to plot poles in Section 2.2.

Kelly_c02.indd 55

11/30/2011 7:32:27 PM

56

2.5

Crystallography and Crystal Defects

Hexagonal System

Crystals possessing a hexad axis have a Bravais lattice, as illustrated in Figure 1.19j in Section 1.8. The x- and y-axes are at 120° to one another and perpendicular to the hexagonal axis along z. The holosymmetric class of this system, 6/mmm, possesses a hexad at the intersection of two sets of three vertical planes of symmetry, two sets of three diad axes normal to these, a plane of symmetry normal to the hexad axis and a centre of symmetry (Figure 2.6). These symmetry elements are shown in Figure 2.12a. Diad axes at 120° to one another are taken as the crystal axes. If this is done, the indices of a number of faces are as marked in Figure 2.12b. The plane of index (100) is repeated by the hexad axis to give – – – – (010), (110), (100), (010), (110). All of these are identical crystallographic planes and yet – their Miller indices appear different: note (010) and (110). To avoid the possibility of confusion from having planes of the same form with quite different indices, it is customary in materials science and metallurgy to employ Miller–Bravais indices for the hexagonal system. To do this, we choose a third crystal axis u normal to the hexagonal axis and at 120° to both the x- and the y-axes. The lattice repeat distance u along u is equal to a (= b) from Figure 1.19j. To state the Miller–Bravais indices of a plane we then take the intercepts along all three axes, x, y and u, express these in terms of the lattice parameters and proceed exactly as in Section 1.2. The result is that a plane always has four indices (hkil), where i is the intercept along the u-axis. It is obvious that there is a necessary relationship between h, k and i since the u-axis is a redundant third axis normal to the hexagonal axis. This can be deduced from Figure 2.13 and is: i = − (h + k ) (a)

(2.2)

u

(b)

110 1120

100 1010

210 2110

010 0110

y

110 1100 001

120 1210

120 1210

0001

110 1100

y

010 0110

210 2110

x

100 1010

110 1120

x

Figure 2.12

Kelly_c02.indd 56

11/30/2011 7:32:28 PM

Point Groups and Space Groups

57

i.e. the third index is always the negative of the sum of the first two. The indices of a number of poles are given in both Miller–Bravais and Miller indices in Figure 2.12b. The hexagonal symmetry is then apparent in the former from the indices of planes of the same form. A Miller–Bravais system is also used to specify directions in hexagonal crystals so that the index appears as [uvtw] instead of [uvw]. When this is done, a little care is needed in relating the results to those obtained using a three-index notation. To enable directions of a given family to have indices of similar appearance, the directions are specified by taking steps along all three axes and arranging it so that the step along the u-axis is of such length that the number of unit repeat vectors moved along this direction, t, is equal to the negative of (u + v). –– The direction corresponding to the x-axis in Figure 2.14 is then [21 1 0] in the four-index –– notation and [100] in the three-index system; the magnitude of [21 10] is three times that of [100], so therefore [100] in the three-index system is equivalent in magnitude to the fourindex vector 13 [2 1 1 0] . Likewise, [010] in the three-index system is equivalent in magnitude to the four-index vector 13 [1 2 1 0] and [110] to 13 [1 1 2 0] . It should be noted that the Miller–Bravais index cannot easily be immediately written down from the first two indices of the three-index triplet, as is the case for a plane, although knowing the four-index vectors equivalent in magnitude and direction to the three-index vectors [100] and [010] enables more general three-index vectors [uvw] to be transformed into their four-index equivalent vectors relatively easily prior to the clearing of fractions to specify four-index zones or directions. Some indices of direction specified in both ways are given in Figure 2.14. In relating planes and zone axes using Equation 1.6, it is usually best to work entirely in the three-index

u

O

a k

B

y

Trace of (hkil )

a 120° h –a i X A

x

Figure 2.13

Kelly_c02.indd 57

11/30/2011 7:32:29 PM

58

Crystallography and Crystal Defects [011] [1213]

[001] [0001]

u

y

2 [0110] [120] –1 –1 [2110] [100]

[1120] [110]

x

Figure 2.14

notation for both planes and directions and to translate the three-index notation for a direction into the four-index system at the end of the calculation. It is also useful to note that the condition needed for a four-index vector [uvtw] to lie in a four-index plane (hkil) is: hu + kv + it + lw = 0

(2.3)

Other point groups besides 6/mmm in the hexagonal system are shown in Figure 2.6. We – note that 6 (≡ 3/m) is placed in this system because of the use of rotoinversion axes to – describe symmetry operations of the second sort; 6, 6, 6/m and 6mm show no diad axes, just like their counterparts in the tetragonal system. The crystal axes for 6mm are usually cho– sen to be perpendicular to one set of mirrors (they then lie in the other set) and 6 m2 could – be developed as 6 m (≡ 3/mm). The diads automatically arise and are chosen as crystallographic axes. Of course, 622 contains diads. It could be developed as 62, since the second set of diads arises automatically (e.g. see Table 1.2). The axes are chosen parallel to one set of diads. Only 6/m and 6/mmm are centrosymmetric in this system. It is apparent from the stereogram in Figure 2.12b that stereograms with 0001 at the centre showing {hki0} poles are straightforward to plot. To plot more general poles on a stereogram with 0001 at the centre, it is apparent that the c/a ratio has to be used. Thus, for

Kelly_c02.indd 58

11/30/2011 7:32:33 PM

Point Groups and Space Groups

59

Normal to (0001)

Normal to (hh2hl)

c l q a h

a h

y

a 2h 90º 30º

x

Figure 2.15

example, this has to be used to determine the angle between faces such as (0001) and – (hh2hl), for example (1121). It is convenient to choose a (hh2hl) plane because such a plane is equally inclined to the x- and the y-axes. From Figure 2.15, the angle q between the (0001) pole and the (hh2hl) pole is seen to be given by: tan θ =

c 2h a l

(2.4)

– Similarly, the angle q between (0001) and (h0h l) is: tan θ =

c 2h a 3l

(2.5)

– – An example of a stereogram centred at (0001) with poles of the forms {1121}, {1011} and – {1231} indicated for a hexagonal cell is shown in Section 2.6 in connection with crystals of the trigonal system. The special forms in the various classes of the hexagonal system are listed in Table 2.1.

2.6 Trigonal System This crystal system is defined by the possession of a single triad axis. It is closely related to the hexagonal system. The possession of a single triad axis by a crystal does not, by itself, indicate whether the lattice considered as a set of points is truly hexagonal, or

Kelly_c02.indd 59

11/30/2011 7:32:34 PM

60

Crystallography and Crystal Defects 211 101

110

214

112

241

z

001

010

124

011

121

100

111

010

y 142

011

001 100

121 120

421

x

210

412

112 102

201

110

101 211

– Figure 2.16 A stereogram of a trigonal crystal of class 3m with a rhombohedral unit cell. When poles in the upper and lower hemispheres coincide in projection, the indices shown refer to the poles in the upper hemisphere

whether it is based on the staggered stacking of triequiangular nets. When the lattice is rhombohedral, a cell of the shape of Figure 1.19k can be used. The cell in Figure 1.19k is a rhombohedron and the angle a (< 120°) is characteristic of the substance. When the lattice of a trigonal crystal is hexagonal, it is not appropriate to use a rhombohedral unit cell. – The symmetry elements in the holosymmetric class 3m are shown in Figure 2.6 and the repetition of a single pole in accordance with this symmetry is also demonstrated. In this – class, three diad axes arise automatically from the presence of 3 and the three mirrors lying – parallel to 3. These diad axes, which intersect in the inverse triad axis, do not lie in the mirror planes. If the rhombohedral cell is used for such a crystal then the axes cannot be chosen parallel to prominent axes of symmetry. A stereogram of a trigonal crystal indexed according to a rhombohedral unit cell is shown in Figure 2.16. The value of a is 98°. The x-, y- and z-axes are taken to lie in the mirror planes and the inverse triad is a body diagonal of the cell, therefore lying along the direction [111], which, from the geometry of the rhombohedral unit cell, is also parallel to the normal to the (111) plane. It is clear that the x-, y- and z-axes – that is, the directions [100], [010] and [001] – do not lie normal to the (100), (010) and (001) planes, respectively. However, these directions are easily located. For example, the z-axis, [001], is the pole of the zone – – containing (110), (010), (100) and (110), shown as a great circle in Figure 2.16. Likewise,

Kelly_c02.indd 60

11/30/2011 7:32:37 PM

Point Groups and Space Groups u

1010 2110

1120

2111 1011

1121

0110

1100

1101

0111 1211

1210

0001

1211

3211

1011 1121

2111 3121

y

1231

0110

2131

2110 x

1210

0111

1101

1100

61

1120 1010

Figure 2.17 The same crystal as in Figure 2.16 indexed using a hexagonal cell. When poles in the upper and lower hemispheres superpose in projection, the indices refer to poles in the upper hemisphere

– – the y-axis is the pole of the zone containing (101), (100), (001) and (101), and the x-axis is – – the pole of the zone containing (011), (001), (010) and (011). In plotting a stereogram of a trigonal crystal with a rhombohedral unit cell from a given value of the angle a, it is useful to note that the angle g between any of the crystal axes and the unique triad axis is given by: sin γ =

2 3

sin α /2

(2.6)

(see Problem 2.2). For many purposes it is more convenient to use a hexagonal cell when dealing with trigonal crystals, irrespective of whether the lattice of the trigonal crystal is primitive hexagonal or rhombohedral. The shape of the cell chosen is the same as for hexagonal crystals (Figure 1.19j) and, since it is chosen without reference to the lattice, may or may not be primitive. The value c/a is characteristic of the substance. – A stereogram of a trigonal crystal of the point group 3m with planes indexed according to the Miller–Bravais scheme is shown in Figure 2.17. This is the same crystal as that in Figure 2.16 (c/a = 1.02). When using the hexagonal cell, the x-, y- and u-axes are chosen – parallel to the diads in 3m.

Kelly_c02.indd 61

11/30/2011 7:32:37 PM

62

Crystallography and Crystal Defects

The relationship between the indices in the two stereograms can be easily worked out using the zone addition rule and the Weiss zone law, Equation 1.6, from the orientation relationship of the rhombohedral and hexagonal cells. In Figures 2.16 and 2.17 this is – – –– (0001)⏐⏐(111)4 and (1011)⏐⏐(100). The plane (1010) in Figure 2.17 then has indices (211 ) –– –– in Figure 2.16. The indices (211 ) could be deduced by noting that the plane (211 ) contains –– the [111] direction (and so the pole of (211) must lie on the primitive if [111] is at the centre of the stereogram), is equally inclined to the y- and z-axes, and lies in the zone containing (111) and (100). The plotting of a stereogram and the determination of axial ratios for a trigonal crystal referred to hexagonal axes then proceed as for the hexagonal system.5 – In the class 3m, special forms lie (i) normal to the triad: {0001}, (ii) parallel to the triad: – {hki0}, (iii) normal to mirror planes: {h0h l}, and (iv) equally inclined to two diads: – – {hh2hl}. The six faces in the form {h0h l} make a rhombohedron; {1012} would be an – – – – – – – –– example, consisting of the planes (1012), (1102), (0112), (1012), (1102) and (011 2). This form is similar in appearance to {0hh¯l}, which is also a rhombohedron, rotated 60° with respect to the first one. – – – The relationship between {h0h l} and {0hh l} (or, equivalently, {0kk l}) is shown in Figure 2.18. They are actually quite separate forms and each one is a special form. We – – therefore need to add {0hh l} to the list of special forms, in addition to {h0h l}. It is apparent – – from Figure 2.16 that when using the rhombohedral cell the two forms {1011} and {0111} – have different indices, since the face above (001) in the projection in Figure 2.16 would – have indices (221). – The other trigonal point groups are shown in Figure 2.6. In 3 and in 3 there are neither mirrors nor diads. The class 3m has three mirrors intersecting in the triad axis; the x-, y- and u-axes of the hexagonal cell are taken to lie perpendicular to the mirror planes. The point group 32 contains diads normal to 3 (consistent with the geometry for permissible combinations of rotational symmetry operations in Table 1.2), which are taken as the crystallo– graphic axes. If three mirror planes intersect in an inversion triad, as in 3m, then diads automatically arise normal to the mirror planes; the diads are chosen as the x-, y- and u-axes. Finally, we note that the class 3/m is not specified as a point group in the trigonal system: it is placed in the hexagonal system because it is equivalent to 6¯.

(1011)

y

(1101)

y

(1011)

(0111)

Figure 2.18 The symbol ⏐⏐ means ‘parallel to’. The relationship between the two cells used in Figures 2.16 and 2.17 is shown in Figure A4.2a, where general methods of transforming the indices of planes and directions, when different unit cells are chosen for the same crystal, are considered. 4 5

Kelly_c02.indd 62

11/30/2011 7:32:39 PM

Point Groups and Space Groups

2.7

63

Monoclinic System

Crystals in the monoclinic system possess a single two-fold axis. Since a mirror plane is – equivalent to an inverse diad, the class m (≡ 2) is put into this system. Two settings are shown in Figure 2.6 for the monoclinic point groups, depending on whether the stereogram is centred on the two-fold axis (the 1st setting) or whether the two-fold axis is lying in the equatorial plane of the stereogram (the 2nd setting). With respect to the convention for choosing x-, y- and z-axes for stereograms centred on the normal to the 001 planes for orthorhombic, tetragonal and cubic crystals, the two-fold axis is along the z-axis in the 1st setting, so that the angle g between the x- and y-axes is obtuse (as for hexagonal crystals, where g is fixed to be 120°), while a = b = 90°. In the 2nd setting, the two-fold axis is along the y-axis, so that the angle b between the x- and z-axes is obtuse, while a = g = 90°. Somewhat confusingly, both conventions are used in the scientific literature to describe the unit cells of monoclinic crystals, but it is much more common in materials science and metallurgy for the 2nd setting to be used, as we have chosen to do in Table 1.3 and Figures 1.19b and c. Irrespective of the choice of 1st or 2nd setting, the sides of the unit cells of crystals belonging to the monoclinic system are in general all unequal to one another. The symmetry elements in the holosymmetric point group 2/m are shown in Figure 2.19 for the 2nd setting. The pole of (010) and the y-axis coincide on the stereogram. In this m 100

hk0

hk0

x h0l hkl

hkl

0kl

0kl z

010

010

b – 90° 001

0kl

hkl

y

0kl

f

hkl h0l

hk0

+x

hk0

b – 90° 100 m

Figure 2.19

Kelly_c02.indd 63

Monoclinic stereogram centred on [001] for the 2nd setting

11/30/2011 7:32:39 PM

64

Crystallography and Crystal Defects z

(hk0)

b

b k

90° f

Normal to 010

b – 90° 90° a h

y

Normal to hk0

x

Figure 2.20 A diagram from which the angle f in Figure 2.19 between 010 and hk0 can be derived

figure, [001], the z-axis, is chosen to be at the centre of the primitive and so (100) lies on the primitive 90° from (010). The x-axis, the direction [100], which makes the obtuse angle b with [001], is necessarily in the lower hemisphere. The angle between [001] and (001) is (b − 90°), which is of course equal to the angle between (100) and [100]. Poles such as {hk0} lie around the primitive because [100] lies in {hk0} planes (Weiss zone law, Equation 1.6). A pole such as (hk0) lies at angle j to (010), given by: cot ϕ =

(a / h) sin β (b / k )

(2.7a)

(see Figure 2.20), or equivalently (Section A3.2): cos ϕ =

Kelly_c02.indd 64

k b ⎛ h2 k2 ⎞ ⎜ a 2 sin 2 β + b2 ⎟ ⎝ ⎠

1/2

(2.7b)

11/30/2011 7:32:39 PM

Point Groups and Space Groups

65

The factor sin b arises because the normals to (hk0) and (010) and the x-axis do not lie in the same plane. In the point group 2/m the only special form besides {010} is {h0l}, with – – a multiplicity of two – the planes (h0l) and (h 0l ). It is apparent that the two faces in this latter form are parallel, both lying normal to the mirror plane and parallel to the diad axis. The general form is {hkl}, with a multiplicity of four (see Figure 2.19). {hk0} and {0kl} are also general forms. The remaining point groups in the monoclinic system are 2 and m. Again, {h0l} is a special form in both and so is {010}. However, 2 does not possess a centre and so for this – point group {010} and {010} must each be listed as separate special forms.

2.8 Triclinic System There are no special forms in either of the point groups in this system. The unit cell is a general parallelepiped and the geometry is more complicated than even for the monoclinic system. The drawing of a stereogram whose centre is taken to be the z-axis, [001], can be carried out with the aid of Figures 2.21a and b. The two diagrams here are completely general and can be specialized to apply to any crystal system more symmetric than the triclinic by setting one or more of the axial angles to particular values and by setting two or more of the lattice parameters to be equal. The choice of the centre of the stereogram as the z-axis in Figure 2.21a means that all planes of the general form (hk0) lie on the primitive of the stereogram, just as for the monoclinic stereogram in Figure 2.19. However, for triclinic crystals there is no good reason to have the 010 pole located on the right-hand side of the horizontal axis of the stereogram, and so here it is deliberately rotated around the primitive away from this position. The great circle passing through 001 and 010 is the [100] zone, containing planes of the general form (0kl). Therefore, the angle between this zone and the primitive must be the angle between [100] and [001], b, as shown in Figure 2.21a. This is because the stereographic projection is a conformal projection (see Appendix 2); that is, one for which angles are faithfully reproduced. Similarly, a and g can be specified on Figure 2.21a from the triclinic system geometry. Angles between poles can be determined using Equation A3.18. Once the position of the 010 pole (or any other pole of the form hk0) has been chosen, geometry determines the positions of the remaining poles on the stereogram. Thus, for example, the position of the 001 pole is fixed knowing that it lies in the [100] zone, which has to make an angle of b with the primitive, and that 001 is a given angle from 010, determined for example using Equation A3.4. Likewise, the position of a pole 0kl lying in the [100] zone can be determined, as can the positions of the poles 100, h0l, hk0 and hkl. While stereographic projections can now be produced routinely via proprietary software packages, it is still instructive to consider further aspects of the geometry of the part of the triclinic stereogram shown in Figure 2.21a in order to gain a full appreciation of the richness of information displayed on stereograms. An (hkl) plane of a triclinic crystal is shown in Figure 2.21b. The six angles f1–f6 in Figure 2.21b are the same as those marked in Figure 2.21a. Thus, for example, f1 in Figure 2.21b is an angle lying in the (001) plane. It is the angle – between the y-axis and the vector [k h0] common to (hkl) and (001); that is, the angle

Kelly_c02.indd 65

11/30/2011 7:32:42 PM

66

Crystallography and Crystal Defects (a) b

z

010 f3

001 y

0kl

f2

f1

f4

hkl h0l hk0

f6 a

f5

100 z

(b)

f5 f4 (010)

a

b g f3 f2

a h

(100)

c l

f6

b k f1

y

hkl (001)

x

Figure 2.21 Diagrams relevant to drawing stereograms of triclinic crystals. The centre of the stereogram in (a) is the z-axis, [001]

between the zone containing (001), (h0l) and (100) and the zone containing (001), (hkl) and (hk0). We can therefore mark f1 on the stereogram. Similarly, f5 in Figure 2.21b is an angle – lying in the (100) plane. It is the angle between the z-axis and the vector [0 l k] common to (hkl) and (100); that is, the angle between the zone containing (100), (hk0) and (010) and the zone containing (100), (hkl) and (0kl). f5 can therefore also be marked on the

Kelly_c02.indd 66

11/30/2011 7:32:42 PM

Point Groups and Space Groups

67

stereogram. Proceeding in this way, we can identify all of the angles f1–f6. We have, from the geometry in Figure 2.21b:

α + φ5 + φ6 = 180° β + φ3 + φ4 = 180° γ + φ1 + φ 2 = 180°

(2.8)

Furthermore, from the triangle on the (001) face in Figure 2.21b we have, using the sine rule: a/h b/k = sin φ1 sin φ2

(2.9)

a / h sin φ1 = b / k sin φ2

(2.10a)

c / l sin φ6 = b / k sin φ5

(2.10b)

a / h sin φ4 = c / l sin φ3

(2.10c)

Therefore:

and similarly:

and:

As an aside, we note that Equations 2.10a–c are also of use in finding axial ratios and axial angles from measured angles between planes on single crystal specimens of crystals belonging to the triclinic crystal system; such crystals tend to be minerals or organic materials, rather than metals, the crystal structures of which rarely tend to belong to either the monoclinic or the triclinic systems.

2.9

Special Forms in the Crystal Classes

A summary of the special forms in the various crystal classes for the various crystal systems is given in Table 2.1. The orientation of the axes is that used in this chapter. Monoclinic crystals are in the 2nd setting of Figure 2.6 and trigonal crystals are referred to hexagonal axes. There are no special forms in the triclinic system.

Kelly_c02.indd 67

11/30/2011 7:32:42 PM

68

Crystallography and Crystal Defects

Table 2.1

Special forms in the crystal classes

2

32

6mm

– {0 1 0}, {0 1 0}, {h 0 l}

– {0 –0 –0 1}, {1 0 –1 0}, {2 1 1 0}, {1 1 –2 0}, {h k i 0}, {h 0 h l}, {0 k k l}, {h h 2h l}, {2h h h l}

– – {0 0 0 1}, {0 0 0 1}, {1 0 1 0}, – {1 1 2 0}, {h k i 0}, {h 0 h l}, {h h 2h l}

m and 2/m

4

{0 1 0}, {h 0 l}

– {0 0 1}, {0 0 1}, {h k 0}

mm2

– 4 and 4/m

– {0 0 1}, {0 0 1}, {1 0 0}, {0 1 0}, {h k 0}, {h 0 l}, {0 k l}

{0 0 1}, {h k 0}

622 and 6/mmm – – {0 0 0 1}, {1 0 1 0}, {1 1 2 0}, {h k i 0}, {h 0 h l}, {h h 2h l}

222 and mmm

4mm

23

– {0 0 1}, {0 0 1}, {1 0 0}, {1 1 0}, {h k 0}, {h 0 l}, {h h l} – 4 2m

{1 0 0}, {1 1 – 0}, {h k 0}, {k– h 0}, {1 1 1}, {1 1 1}, {h l l}, {h l l}, {h h l}, {h h l} – m3

{0 0 1}, {1 0 0}, {1 1 0}, {h k 0}, {h 0 l}, {h h l}, {h h l}

{1 0 0}, {1 1 0}, {h k 0}, {k h 0}, {1 1 1}, {h l l}, {h h l}

42 and 4/mmm

432

{0 0 0 1}, {h k i 0}

{0 0 1}, {1 0 0}, {1 1 0}, {h k 0}, {h 0 l}, {h h l}

3m

6

{1 0 0}, {1 1 0}, {h k 0}, {1 1 1}, {h l l}, {h h l} – 4 3m

– – {0 0 0 – 1}, {0 0 0– 1}, {1 0 1 0}, {0 1 1 0}, {1 1 2 0}, {h k i 0}, {h 0 h l} {0 k k l}, {h h 2h l} – 3m – – {0 0 0 1}, {1 0 1 0}, {1 1 2 0}, {h k i 0}, {h 0 h l}, {0 k k l}, {h h 2h l}

– {0 0 0 1}, {0 0 0 1}, {h k i 0}

{1 0 0}, {0 1 0}, {0 0 1}, {h k 0}, {h 0 l}, {0 k l} 3 – {0 0 0 1}, {0 0 0 1}, {h k i 0} – 3

2.10

– 6 and 6/m {0 0 0 1}, {h k i 0}

– 6 m2 – – {0 0 0 – 1}, {1 0 1 0}, {0 1 1 0}, {1 1 2 0}, {h k i 0}, {h 0 h l}, {0 k k l}, {h h 2h l}

{1 0 – 0}, {1 1 0}, {h– k 0}, {1 1 1}, {1 1 1}, {h l l}, {h l l}, {h h l}, {h h l} – m3m {1 0 0}, {1 1 0}, {h k 0}, {1 1 1}, {h l l}, {h h l}

Enantiomorphous Crystal Classes

In some crystal classes the possibility exists of crystals being found in either a right-handed or a left-handed modification with the two not being superposable, in the sense that the right hand of the body cannot be superposed upon the left hand. This occurs if the crystal only

Kelly_c02.indd 68

11/30/2011 7:32:48 PM

Point Groups and Space Groups Table 2.2

69

Laue groups

System Cubic Hexagonal Tetragonal Trigonal Orthorhombic Monoclinic Triclinic

Class – – 432, 4–3m, m3m 23, m3 ¯ 622, – 6mm, 6m2, 6/mmm 6, 6, 6/m – 422, – 4mm, 4 m2, 4/mmm 4, 4 , 4/m– 32,– 3m, 3m 3, 3 222, 2mm, mmm 2, m, – 2/m 1, 1

Laue group – m3 –m m3 6/mmm 6/m 4/mmm 4/m – 3 –m 3 mmm 2/m – 1

possesses simple rotation symmetry operations; that is, no symmetry operation of the second kind. Therefore, mirror planes and rotoinversion axes of any degree do not appear in such crystal classes. There are 11 such classes: 1, 2, 3, 4, 6, 23, 222, 32, 422, 622 and 432.

2.11

Laue Groups

Some physical methods of examination of crystals cannot determine whether or not there is a centre of symmetry present, such as, for example, when stationary single crystals are illuminated by a continuous distribution of X-ray wavelengths (known as ‘white radiation’) to produce Laue diffraction patterns. This is known as the Laue method. Such diffraction patterns are used for symmetry determination and for the accurate alignment of crystals; they are also useful for time-resolved macromolecular crystallography using synchrotron radiation. The Laue group is the crystal class to which a particular crystal belongs if a centre of symmetry is added to the symmetry elements already present. The 11 Laue groups are shown in Table 2.2. The loss of symmetry information in time-resolved macromolecular crystallography is more than compensated for by the ability to capture structural information over subnanosecond timescales in fast chemical reactions such as enzyme reactions.

2.12

Space Groups

We showed in Section 1.4 that repetition of an object (e.g. an atom or group of atoms) in a crystal is carried out by operations of rotation, reflection (or inversion) and translation. We have also described in this chapter the consistent combinations of rotations and inversions that can occur in crystals, and in Section 1.8 we described the possible translations that can occur in crystals to produce the 14 Bravais lattices, or space lattices. However, we have so far not made any attempt to combine the operations of rotation (and inversion) with translation, except briefly in Section 1.5, where it was shown that only one-, two-, three-, four- and six-fold rotation axes are compatible with translational symmetry. A full description of the symmetry of a crystal involves a description of the way in

Kelly_c02.indd 69

11/30/2011 7:32:48 PM

70

Crystallography and Crystal Defects (a)

(b)

(c)

t 2 180º

t 2

180º

t 2

180º 180º

2

21

Figure 2.22 (a) A two-fold rotation axis. (b) A 21 screw axis. (c) A glide plane normal to the surface of the paper

which all of the symmetry elements are distributed in space. This is called the space group. There are 230 different crystallographic space groups and each one gives the fullest description of the symmetry elements present in a crystal possessing that group. The rotation axes and rotoinversion axes possible in crystals were discussed in Section 2.1 and the possible translations in Section 1.8. An enumeration of the way these axes can be consistently combined with the translation is therefore an enumeration of the possible space groups. Space groups are most important in the solution of crystal structures. They are also very useful when establishing symmetry hierarchies in phase transitions in perovskites [6–8]. When an attempt is made to combine the operations of rotation and translation, the possibility arises naturally of what is called a screw axis. This involves repetition by rotation about an axis, together with translation parallel to that axis. Similarly, a repetition by reflection in a mirror plane may be combined with a translational component parallel to that plane to produce a glide plane. If, for example, a two-fold rotational axis occurs in a crystal, then this means some structural unit or motif is arranged about this direction so that it is repeated by a rotation of 180° about the axis. The repetition shown in Figure 2.22a corresponds to a pure rotational diad axis. However, the rotation of 180° could be coupled with a translation of one-half of the lattice repeat distance, t, in the direction of the axis to give the screw diad axis shown in Figure 2.22b, denoted by the symbol 21. The translation t/2 will be of a length of the order of the lattice parameters of the crystal and hence of the order of a few Ångstrom units (1 Å = 10−10 m), and so quite undetected by the naked eye. The operation of glide plane repetition is shown in Figure 2.22c. Again, the magnitude of the translation will be of the

Kelly_c02.indd 70

11/30/2011 7:32:48 PM

Point Groups and Space Groups

71

order of the lattice parameters. Macroscopically, the crystal containing a 21 axis would then show diad symmetry about that axis in the symmetry of its external faces or of its physical properties. Similarly, the glide plane in Figure 2.22c would show itself macroscopically as a mirror plane. Although the presence of a screw axis, say a screw diad as in Figure 2.22b, indicates the presence of identical atomic motifs arranged about it so that they are related by a rotation plus translation, the screw axis must not be thought of as translating the translation vectors of the lattice. A screw axis and a pure rotation axis of the same order n repeat a translation in the same way. It follows that the rotational components of screw axes can only be 2p/1, 2p/2, 2p/3, 2p/4, 2p/6 and that an n-fold screw and an n-fold pure rotation axis must have similar locations with respect to a similar set of translations. The angles between screws and between screws and rotations must therefore be the same as the permissible combinations listed in Table 1.2. When we combine the operations of rotation with translation and look for the possible consistent combinations we can start with the point group and associate its symmetry elements with each lattice point of the lattices consistent with it. From the number of Bravais lattices and number of point groups detailed in Figures 1.19 and 2.6 it might be expected that 66 space groups could be obtained (2 triclinic, 6 monoclinic, 12 orthorhombic, 14 tetragonal, 5 trigonal with a rhombohedral lattice, 5 trigonal with a hexagonal lattice, 7 hexagonal and 15 cubic). Seven additional ones arise because of cases in which the glide planes or screw axes automatically arising are different for different orientations of the – – point group with respect to the lattice; for example, in the tetragonal system I4 m2 and I4 2m are distinct space groups. The 14 space groups for which this consideration is relevant are – – – – – – Cmm2, Amm2 (≡ C2mm), P4 2m, P4 m2, I4 2m, I4 m2, P6 m2, P6 2m, P312, P321, P3m1, – – P31m, P3m1 and P31m. Therefore, there are 73 such space groups, referred to as arithmetic crystal classes in Section 8.2.3 of the fifth edition of the International Tables for Crystallography [3]. When the possibilities of introducing screw axes to replace pure rotational axes and glide planes to replace mirror planes are taken into consideration, the result is to produce a total of 230 different space groups [3]. Of particular note are the space groups in the trigonal crystal system. Of the 25 trigonal space groups, only seven have a – – – rhombohedral unit cell (R3, R3, R32, R3m, R3c, R3m, R3c); the majority have a primitive hexagonal unit cell. Buerger [1] argues that ‘to refer one crystal of the trigonal class to rhombohedral axes, and another to hexagonal axes, because the lattice types are R and P respectively, leads to confusion’ (p. 106) and discourages the use of rhombohedral axes for this reason. It is certainly the case in the scientific literature that the use of rhombohedral axes for crystals where the space group is one of the seven rhombohedral space groups is markedly less prevalent than the use of hexagonal axes. The various kinds of screw axis possible are shown in Table 2.3. An nN-fold screw axis involves repetition by rotation through 360°/n with a translation of tN/n, where t is a lattice repeat vector parallel to the axis. There are five types of screw hexad; for example, 61 involves rotation through 60° and translation of t/6, while 65 involves rotation through 60° and translation of 5t/6. By drawing a diagram showing the repetition of objects by these axes, it is easily seen that 61 is a screw of opposite hand to 65, 41 to 43, and 62 to 64. A diagram to show this for 31 and 32 is given in Figure 2.23. In this figure, A and A′ are lattice points. The operation of 31 is straightforward, as shown in Figure 2.23a. When repeating an object according to 32, note that the object at height 43 must also occur at height 13 , since

Kelly_c02.indd 71

11/30/2011 7:32:49 PM

72

Crystallography and Crystal Defects

Table 2.3

Screw axes in crystals

Name

Symbol

Screw diad

21

Screw triads

31 32

Screw tetrads

41 42 43

Screw hexads

61 62 63 64 65

Graphical symbol

Right-handed screw translation along the axis in units of the lattice parameter 1 2 1 3 2 3 1 4 2 1 4=2 3 4 1 6 2 1 6=3 3= 6 4 6= 5 6

1 2 2 3

A and A′ are both lattice points and the pattern is infinitely long parallel to AA′. It should also be noted that axes 42 and 63 include the pure rotation axes 2 and 3 respectively in the lattice. 62 and 64 also contain two-fold rotation axes. Glide planes are described as axial glide planes if the translation parallel to the mirror is parallel to a single axis of the unit cell and equal to one-half of the lattice parameter in that direction. Such glide planes are given the symbols a, b or c, corresponding to the directions of the glide translations. A diagonal glide plane involves a translation of one-half of a face diagonal or one-half of a body diagonal (the latter in the tetragonal and cubic systems), given the symbol n, and a diamond glide plane involves a translation of one-quarter of a face diagonal, given the symbol d. The diamond glide plane involves a translation of one-quarter of a body diagonal in the tetragonal and cubic systems. In centred cells, the possibility of a ‘double’ glide plane arises, given the symbol e. In this symmetry operation, recognised officially in the most recent edition of the International Tables for Crystallography and incorporated into the conventional space group symbols of five space groups [3], two glide reflections occur through the plane under consideration, with glide vectors perpendicular to one another. The conventional space group symbol shows that the space groups have been built up by placing a point group at each of the lattice points of the appropriate Bravais lattice. Thus, – – for example, Fm3m (in full, F 4/m 3 2/m) means the cubic face-centred lattice with the – point group m3m associated with each lattice point and P63/mmc (in full, P 63/m 2/m 2/c) is a hexagonal primitive lattice derived from P6/mmm by replacing the six-fold rotation axis

Kelly_c02.indd 72

11/30/2011 7:32:49 PM

Point Groups and Space Groups (a)

73

(b)

A⬘

A⬘

2t 3

A

t 3

120º 31

A

120º

120º 32

Figure 2.23 Screw axes 31 and 32: these are screw axes of opposite hand, as shown by the symbols at the top

by 63 and one of the mirror planes by a c-axis glide plane. P63/mmc and P6/mmm share the same point group symmetry. The point group symmetry of any crystal is derived immediately from the space group symbol by replacing screw axes by the appropriate rotational axes and glide planes by mirror planes in the space group symbol. The arrangements of all of the symmetry elements in the 230 space groups are listed in the various editions of the International Tables for Crystallography. Of particular interest to most materials scientists are the coordinates of general and special positions within each unit cell and diagrams showing the symmetry elements. More recent editions have extensive descriptions of space groups, which also include listings of maximal subgroups and minimal supergroups; these concepts will be discussed in general terms in Sections 2.14 and 2.15. For our purposes in this section, the essential elements of how the assignment of a crystal structure to a particular space group imposes restrictions on the possible general and special positions of atoms or ions within a particular unit cell can be illustrated by considering the 17 two-dimensional space groups (or plane groups). These space groups are shown in Figure 2.24 in the same way they are depicted in the International Tables for

Kelly_c02.indd 73

11/30/2011 7:32:50 PM

No. 1 p1

1 Parallelogram

Origin on 1 Coordinates of equivalent positions 1 1 x, y

No. 3 pm ,

m Rectangular ,

,

No. 2 p2

2 Parallelogram

Origin at 2 Coordinates of equivalent positions 2 1 x, y ; x–, y– 1 2 21– , 12– 1 2 12– , 0 1 1 2 0, 2– 1 2 0, 0 m Rectangular No. 4 pg ,

,

,

Origin on m Coordinates of equivalent positions – y 2 1 x, y ; x, 1, 1 m 2 y 1 m 0, y

Origin on g Coordinates of equivalent positions 2 1 x, y ; x–, 1–2 + y

No. 5 cm ,

No. 6 pmm , ,

m Rectangular ,

mm Rectangular , ,

, ,

,

, ,

Origin on m Coordinates of equivalent positions (0, 0 ) +; ( 1–2, 1–2 ) + 4 1 x, y ; x–, y 2 m 0, y

, ,

Origin at 2mm Coordinates of equivalent positions 4 1 x, y ; x–, y ; x–, y– ; x, y– 2 m –12 , y ; 12–, y– 2 m 0, y ; 0, y– m x, –12 ; x–, 12– 2 m x, 0; x–, 0 2 1 mm 21– , 12– 1 mm 12– , 0 1 mm 0, 1–2 1 mm 0, 0

Figure 2.24 The 17 two-dimensional space groups arranged following the International Tables for Crystallography [3]. The headings for each figure read, from left to right, Number, Short Symbol (see Table 2.4), Point Group, Net. Below each figure the columns give the number of equivalent positions, the point group symmetry at those positions and the coordinates of the equivalent positions. The coordinates of positions x, y are expressed in units equal to the cell edge length in these two directions.

Kelly_c02.indd 74

11/30/2011 7:32:50 PM

No. 7 pmg

No. 8 pgg

mm Rectangular

,

mm Rectangular

,

,

,

,

,

Origin at 2 Coordinates of equivalent positions 4 1 x, y; x, y; 1–2 + x, y; 12– – x, y 2 m 1–4, y; –43, y

Origin at 2 Coordinates of equivalent positions 4 1 x, y; x–, –y; 1–2 + x, 1–2 – y; 21– – x, 2 2 12–, 0; 0, 12–

2 2

2

0, 21–; 12–, 1–2 0, 0; 21–, 0

2 2

No. 9 cmm

+y

1– 2

No. 10 p4

mm Rectangular

,

1

0, 0; 2–,

2

1– 2

4 Square

,

,

, , , ,

,

,

,

Origin at 2mm Coordinates of equivalent positions (0, 0) +; (12–, 1–2 ( + 8 1 x, y; x, y; x, y; x, y m 0, y; 0, y 4 m x, 0; x, 0 4 4 2 14–, 1–4; 14–, 3–4 2 mm 0, 1–2 2 mm 0, 0

Origin at 4 Coordinates of equivalent positions 4 1 x, y; x, y; y, x; y, x 2 2 1–2, 0; 0, 12– 1 4 1–2, 1–2 1 4 0, 0

No. 11 p4m , , , ,

No. 12 p4g

4 mm Square , , , ,

4 mm Square

,

, , , ,

, ,

, ,

, ,

Origin at 4mm Coordinates of equivalent positions 8 1 x, y; x, y; y, x; y, x; x, y; x, y; y, x; y, x m x, x; x, x; x, x; x, x 4 1 1 1 m x, –2; x; –2; –2, x; –12, x 4 m x, 0; x; 0; 0, x; 0, x 4 1 1 mm 2–, 0; 0, 2– 2 1– 1– 1 4mm 2, 2 1 4mm 0, 0

Figure 2.24

Kelly_c02.indd 75

,

Origin at 4 Coordinates of equivalent positions 1 1 1 1 8 1 x, y; y, x; –2 – x, –2 + y; –2 – y, –2 – x; 1– 1– 1– 1– x, y; y, x; 2 + x, 2 – y; 2 + y, 2 + x m x, 1–2 + x; x, 1–2 – x; 1–2 + x, x, 1–2 – x, x 4 2 mm 2

4

1– 2,

0; 0, 1–2

0, 0; 1–2 ,

1– 2

(continued)

11/30/2011 7:32:50 PM

No. 13 p3

No. 14 p3m1

3 Triequiangular

3 m Triequiangular

,

, ,

,

,

,

, ,

,

,

,

,

Origin at 3 Coordinates of equivalent positions 3 1 x, y; y, x − y; y − x, x 1 3 3–2, 13– 1 3 13– , 23– 1 3 0, 0

Origin at 3m Coordinates of equivalent positions 6 1 x, y; y, x − y; y − x, x; x, x − y; y − x, y; y, x m x, x; x, 2x; 2x, x 3 1 3m –32, 13– 1 3m 1–3, 2–3 1 3m 0, 0

No. 15 p31m

No. 16 p6

3 m Triequiangular

,

6 Triequiangular

,

, ,

,

,

,

, ,

,

,

,

Origin at 31m Coordinates of equivalent positions 6 1 x, y; y, x – y; y − x, x; y, x; x, y − x; x − y, y 3 m x, 0; 0, x; x, x 2 3 13–, –23; –23, 13– 1 3m 0, 0

Origin at 6 Coordinates of equivalent positions 6 1 x, y; y, x – y; y − x, x; x, y; y, y – x; x – y, x 3 2 –12 , 0; 0, –12; –12, –12 2 3 13– , –32; –23, 1–3 1 6 0, 0

No. 17 p6m 6 mm Triequiangular , , , , , , , , , , , ,

,

, ,

,

, , ,

,

, ,

, ,

Origin at 6mm Coordinates of equivalent positions 1 x, y; y, x – y; y – x, x–; y, x; x–, y – x; 12 x – y, y– ; x–, y– ; y, y – x ; x – y, x ; y– , x–; x, x – y; y – x, y m x, x–; x, 2x; 2x–, x– ; x–, x; x–, 2x–; 2x, x 6 m x, 0; 0, x; x–, x–; x–, 0; 0, x–; x, x 6 3 mm 12– , 0; 0, 12– ; 12– , 12– 3m –13, –32; –23, 1–3 2 1 6mm 0, 0

Figure 2.24 (continued)

Kelly_c02.indd 76

11/30/2011 7:32:51 PM

Point Groups and Space Groups

77

Table 2.4 Two-dimensional lattices, point groups and space groups System and lattice symbol

Parallelogram p (primitive) Rectangular p and c (centred)

Point group

1 2 m 2mm

Square p

4 4mm

Triequiangular (hexagonal) p

3 3m 6 6mm

Space group symbols Full

Short

p1 p211 p1m1 p1g1 c1m1 p2mm p2mg p2gg c2mm p4 p4mm p4gm p3 p3m1 p31m p6 p6mm

p1 p2 pm pg cm pmm pmg pgg cmm p4 p4m p4g p3 p3m1 p31m p6 p6m

Space group number

1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17

Note: The two distinct space groups p3m1 and p31m correspond to different orientations of the point group relative to the lattice. This does not lead to distinct groups in any other case.

Crystallography [3]. If the plane groups are understood, the essential elements of the threedimensional space group tables in the International Tables can be understood without difficulty. Space groups are obtained by the application of point group symmetry to finite lattices, the possibility of translation symmetry being taken into account. There are five lattices or nets in two dimensions, shown in Figure 1.14. Following the convention in the International Tables for Crystallography, we shall give them the symbol p for primitive and c for centred. The symbols for two-fold, three-fold, four-fold and six-fold axes and for the mirror plane are as in Section 2.1. The only additional symmetry element in two dimensions is the glide reflection line: symbol g and denoted by a dashed line in Figure 2.24. It involves reflection and a translation of one-half of the repeat distance parallel to the line. The two-dimensional lattices and the two-dimensional point groups are combined in Table 2.4 to show the space groups that can arise, which are shown in Figure 2.24. In all the diagrams, the x-axis runs down the page and the y-axis runs across the page, the positive y-direction being towards the right. In each of the diagrams the left-hand one shows the equivalent general positions of the space group; that is, the complete set of positions produced by the operation of the symmetry elements of the space group upon one initial position chosen at random. The total number of general positions is the number falling within the cell, but surrounding positions are also shown to illustrate the symmetry. The righthand diagram is that of the group of spatially distributed symmetry operators; that is, the true space (plane) group.

Kelly_c02.indd 77

11/30/2011 7:32:51 PM

78

Crystallography and Crystal Defects

Below each of the diagrams in Figure 2.24, the equivalent general positions and special positions are also indicated. Special positions are positions located on at least one symmetry operator so that repetition of an initial point produces fewer equivalent positions than in the general case. The symmetry at each special position is also given. The group p1 is obtained by combining the parallelogram net and a one-fold axis of rotational symmetry. There are no special positions in the cell. The group p2 arises by combining the parallelogram net and a diad. A mirror plane requires the rectangular net (Section 1.5) and if this net is combined with a single mirror, the space group pm, No. 3, results. Points , are in mirror relationship to one another. If the mirror in pm is replaced by a glide and reflection line, the space group pg results. In No. 4 the glide reflection line runs normal to the x-axis. The centred rectangular lattice necessarily shows a glide reflection line as in cm, No. 5, but only one of these need be present, corresponding to the plane point group m. Since, in this case, the net is multiply primitive, the motif associated with the lattice point at ( 12 , 12 ) is the same as that at (0, 0). Hence the coordinates of equivalent positions, if added to ( 12 , 12 ) , give additional equivalent positions. If two mirror planes at right angles (point group mm) are combined with the rectangular lattice we get diads at the intersections of the mirrors as in pmm, No. 6. If one or both of the mirrors is replaced by g, the diads no longer lie at the intersections (see pmg, No. 7 and pgg, No. 8). The group cmm, No. 9, necessarily involves the presence of two sets of glide reflection lines, while p4, No. 10, denotes the square lattice and point group 4, which together necessarily involve the presence of diads. However, mirror planes are not required. If 4 lies at the intersection of two sets of mirrors we have p4m, No. 11, the diagonal glide reflection line necessarily being present. However, 4 can also lie at the intersection of two sets of glide reflection lines, in which case again two sets of mirrors arise but the mirrors intersect in diads, giving point group symmetry mm at these points (No. 12). The triequiangular net and point group 3 give the space group p3 (No. 13). If mirror planes are combined with the triad axis – the combination of the point group 3m and the triequiangular net – it is found that the mirrors can be arranged in two different ways with respect to the points of the net, yielding p31m and p3m1 (Nos. 14 and 15). With the hexagonal point group 6mm, which necessarily has two sets of mirrors, this duality does not arise and the two space groups are p6 and p6mm (Nos. 16 and 17).

2.13

Nomenclature for Point Groups and Space Groups

The nomenclature we have introduced in this chapter to describe point groups and space groups conforms to a notation known as the Hermann–Mauguin notation arising from the work of Carl Hermann [9] and Charles-Victor Mauguin [10] and used in the Internationale Tabellen zur Bestimmung von Kristallstrukturen, edited by Hermann and published in 1935. However, another notation for describing point group and space group symmetry is also in common use. This second notation, known as the Schoenflies notation, is named after Arthur Moritz Schoenflies [11]. This latter notation is used in particular in physical chemistry in connection with molecular symmetry and molecular spectroscopy [12], and it is also useful when considering group theoretical aspects of point groups and space groups [13]. The equivalence between the Hermann–Mauguin notation and the Schoenflies notation is discussed in detail by Hans Burzlaff and Helmut Zimmerman in Chapter 12 of

Kelly_c02.indd 78

11/30/2011 7:32:51 PM

Point Groups and Space Groups

79

International Tables for Crystallography [3]. The reason why the Hermann–Mauguin notation might be preferred over the Schoenflies notation is neatly summarized by Phillips [2]: ‘each space group symbol [in the Hermann–Mauguin notation] conveys all the essential information, whereas we must always have a catalogue at hand to follow an arbitrary serial numbering such as that of Schoenflies’ (p. 340).

2.14

Groups, Subgroups and Supergroups

It is evident from the discussion in this chapter on point groups and space groups that each point group and space group consists of a self-consistent finite set of symmetry operations. Therefore, point groups and space groups can be described in the formalism of group theory [13–15]. A group G is a set of elements g1, g2, g3 … gn which conform to the following four conditions [15]: 1. The product gigj of any two group elements must be another element within the group. 2. Group multiplication is associative: (gigj)gk = gi(gjgk). 3. There is a unique group element I called the identity element belonging to G so that its operation on a member of the group gi is such that Igi = giI = gi. 4. Each element within the group has a unique inverse; that is, for each gi there is a unique element gi−1 so that gigi−1 = gi−1 gi = I. Thus, for example, following the example of the point group mmm used by de Jong [5], p. 20, the eight group elements within this point group are: the identity, I; three 180° rotations about the x-, y- and z-axes; three reflections in the (100), (010) and (001) planes; and a centre of symmetry. A subgroup of these symmetry elements is found in 2mm: the identity, a 180° rotation about the x-axis and two reflections in the (010) and (001) planes. – Other subgroups are the point groups 222, 2/m, m, 2, 1 and 1. Conversely, the point group mmm is clearly a supergroup for 2mm and 222. Similar principles apply to subgroups and supergroups of space groups. Thus, for example, following Hans Wondratschek in Chapter 8 of International Tables for Crystallography – [3], the space group P6 2m is one member of the group whose minimal nonisomorphic – supergroup is P63/mcm; it has as maximal nonisomorphous subgroups P6 , P321, P31m and Pm2m. (Groups are termed isomorphic if they have an equivalent group multiplication structure but differ in the nature of the elements constituting them [15]. Thus, for example, the point groups 2/m, 222 and 2mm are isomorphic: all three have four elements within the group and the same multiplication structure within them.)

2.15 An Example of a Three-Dimensional Space Group To illustrate the principles we have outlined in Sections 2.12–2.14, an example of an entry in the most recent edition of the International Tables for Crystallography is shown in Figure 2.25. It is apparent from the Hermann–Mauguin notation of this space group, Pnma, No. 62, that crystals with this space group symmetry belong to the orthorhombic crystal 16 system, point group mmm. The Schoenflies notation D2h indicates that the space group is dihedral (or two-sided; from the ‘D’), that it has a 2-fold rotation axis (from the ‘2’), that

Kelly_c02.indd 79

11/30/2011 7:32:54 PM

Crystallography and Crystal Defects

80

D16 2h

Pnma No. 62

Orthorhombic

mmm

Patterson symmetry P m m m

P 21/n 21/m 21/a 21 21 21 P– – –a nm 1 4

1 4

1 4

1 4

2 21 21 P n–1 – – am

1 4

1 4

1 4

2 2 2 P –1 –1 –1 b n m

21 21 21 Pm – –n –b

1 4

1 4

1 4

2 2 2 P –1 –1 –1 cm n 1 4

1 4

1 4

1 4 –

,

–

2 2 2 P –1 –1 –1 mc n

+

+

–

,

,

+

, 1+ 1 +

1+ 2

2

2

, 1–

, 1 – 1– 2 2 –

,

– +

1 4

1 4

2

+

–

,

,

+

1 4

– Origin at 1 on 1211 Asymmetric unit 0 ≤ x ≤ 12 ; 0 ≤ y ≤ 14 ; 0 ≤ z ≤1 Symmetry operations (2) 2 (0,0, 12 )

(1) 1 –

(5) 1 0,0,0

(6) a x,y, 14

1 4 ,0,z

(3) 2(0, 12 ,0) 0,y,0

(4) 2( 12,0,0) x,41 , 41

(7) m x, 14, z

(8) n(0, 12 , 12 ) 14 ,y,z

Figure 2.25 An example of a space group. (Taken from [3].)

there is in addition a mirror plane perpendicular to this 2-fold axis (from the ‘h’ subscript) 1 28 and that it is the 16th of 28 such space groups D2h … D2h (space groups 47–74 inclusive), all of which are space groups derived from the mmm point group. The full Hermann–Mauguin notation for this space group is P21/n 21/m 21/a, showing that there are three mutually perpendicular sets of screw diads in addition to the mirror, m, and the diagonal, n, and axial, a, glide planes. The diagrams of the symmetry elements of the group follow the principles in Figure 2.24, with the use of standard graphical symbols for n (parallel to (100) ) and a (parallel to (001) ). The projections in the top left-hand corner and the bottom right-hand corner are both down [001], the one in the top right-hand corner down [010] and the one in the bottom left-hand corner down [100]. The asymmetric unit is ‘a (simply) connected smallest part of space from which, by application of all symmetry operations of the space group, the whole of space is filled

Kelly_c02.indd 80

11/30/2011 7:32:54 PM

Point Groups and Space Groups CONTINUED

No. 62

81

Pnma

Generators selected (1); t(1,0,0); t(0,1,0); t(0,0,1); (2); (3); ( 5) Positions Multiplicity, Wyckoff letter, Site symmetry 8

4 4 4

d

c b a

1

Coordinates

Reﬂection conditions General:

(1) x, y, z

– z + –1 (2) x– + –12 , y, 2

– y + –1 , z– (3) x, 2

y + –12 , –z + –12 (4) x + –12 , –

– –y, –z (5) x,

–12 ,

y, –z + –12

(7) x, –y + –12 , z

(8) x– + –12 , y + –12 , z + –12

(6) x +

m

x, –14 , z

x– + –12 , –34 , z + –12

– 1 – 1

0, 0, –12

–12 , 0, 0

0, 0, 0

–12 ,

0, –12

Symmetry of special projections Along [001] p2gm a' = –12 a b' = b Origin at 0, 0, z Maximal non-isomorphic subgroups I

[2] Pn21a (Pna21, 33) [2] Pnm21 (Pmn21, 31) [2] P21ma (Pmc21, 26) [2] P212121 (19) [2] P1 1 21/a (P21/c, 14) [2] P21/n11 (P21/c, 14) [2] P121/m1 (P21/m, 11)

IIa IIb

none none

– –3 , –z x, 4

x + –12 , –14 , –z + –12

0kl : k + l = 2n hk0 : h = 2n h00 : h = 2n 0k0 : k = 2n 00l : l = 2n Special: as above, plus no extra conditions

1 – 1 0, – 2, 2

–12 , –12 , 0

hkl : h + l, k = 2n

1 0, –2 ,

–12 , –12 , –12

hkl : h + l, k = 2n

0

Along [010] p2gg a' = c b' = a Origin at 0, y, 0

Along [100] c2mm a' = b b' = c Origin at x, –14 , –14

1; 3; 6; 8 1; 2; 7; 8 1; 4; 6; 7 1; 2; 3; 4 1; 2; 5; 6 1; 4; 5; 8 1; 3; 5; 7

Maximal isomorphic subgroups of lowest index IIc [3] Pnma (a' = 3a) (62); [3] Pnma (b' = 3b) (62) ;[3] Pnma (c' = 3c) (62) Minimal non-isomorphic supergroups I none [2] Amma (Cmcm, 63); [2] Bbmm (Cmcm, 63); [2] Ccme (Cmce, 64); [2] Imma (74); [2] Pcma (b' = –12 b) (Pbam, 55); II [2] Pbma (c' = –12 c) (Pbcm, 57); [2] Pnmm (a' = –12 a) (Pmmn, 59)

Figure 2.25

(continued)

exactly’ [3]. The listing under the heading ‘Symmetry Operations’ in Figure 2.25 is a summary of the various geometric descriptions of each of the eight symmetry operations in the

(

1

)

1

space group, numbered (1)–(8). Thus, for example, here the second of these, 2 0,0, 2 4 , 0, z, 1 defines the screw diad parallel to [001] intersecting the x–y plane at ( 4 , 0). The ‘Generators Selected’ define the order in which the coordinates of the symmetrically equivalent positions are produced; for example, the coordinates related by symmetry to the general position x, y, z in the space group. (1) is the identity operation, showing that in this case integral lattice translations produce the equivalent point in adjacent unit cells. After the ‘Positions’, which follow the protocol described in Section 2.12, and the ‘Symmetry of

Kelly_c02.indd 81

11/30/2011 7:32:54 PM

82

Crystallography and Crystal Defects

Special Projections’, which are self-explanatory, a summary is given of subgroups and supergroups related to the space group under consideration, following the methodology set out in Chapter 2 of International Tables for Crystallography [3]. Finally, the reflection conditions listed under ‘Positions’ specify the systematic absences which occur under kinematical diffraction conditions, such as X-ray diffraction.

Problems Material in Appendices 1 and 2 may be useful; in Problem 2.12 the material in Appendix 4 may also be useful. 2.1 Using Figure 2.13, confirm that in the four-index notation for a plane with indices (hkil): i = −(h + k ) (Equation 2.2.) Confirm also that the condition for a four-index vector [uvtw] to lie in a four-index plane (hkil) is: hu + kv + it + lw = 0 2.2 Show that the angle g between any of the crystal axes and the unique triad axis in a trigonal crystal is given by: sin γ =

2 sin α /2 3

2.3 The corners of a wooden model of a cube are cut off to make equal faces of the form – – – – {111}. The first four new faces are cut in positions (111), (111), (1 11) and (111 ), in that order. Draw sketch stereograms to show the symmetry elements shown by the model after each new face is formed. What is the crystal system of the model in each case? 2.4 (a) Sketch stereograms showing the operation of the undermentioned symmetry elements on two distinct poles, each in a general position, and insert the symmetry elements themselves, except the centre of symmetry: centre of symmetry vertical plane of symmetry horizontal plane of symmetry vertical axes 2, 3, 4, 6 – – – – vertical inversion axes 2, 3, 4 , 6 horizontal axes 2, 4 – horizontal inversion axis 4 . – (b) The symbol X /m is not used in conventional point group notation. Draw sketch stereograms of the poles of one general form for each possible value of X and hence derive the conventional symbols that are actually used. – – 2.5 (a) In which of the trigonal classes 3, 3, 3m, 32, 3m does a rhombohedron occur as a special form? In what class is the rhombohedron the general form? – – (b) Which of the tetragonal classes 4, 4 , 4/m, 422, 4mm, 4 2m, 4/mmm have closed forms as their general forms?

Kelly_c02.indd 82

11/30/2011 7:32:58 PM

Point Groups and Space Groups

83

– – – (c) To which of the cubic classes 23, m3, 432, 4 3m and m3m could a crystal belong which had the shape of (i) an octahedron, (ii) a tetrahedron or (iii) an icositetrahedron? (The icositetrahedron is the name given to the {112} form with 24 faces.) 2.6 In a holosymmetric cubic crystal the angle between (110) and a face P which lies in the zone [010] is 53.97°. Find the indices of P and calculate the angle between P and – the face P′ related to P by the mirror plane parallel to (110). Determine the indices – [uvw] of the zone containing P and P′ and calculate the interzone angle [uvw]∧[110]. – 2.7 (a) Calculate the angle between [0001] and [1123] in beryllium (hexagonal, a = 2.28 Å, – – c = 3.57 Å). What face lies at the intersection of the zones [1123] and [2113]? (b) In a crystal of calcite (trigonal; c/a = 0.8543), a face lies in the zone – – – between (1011) and (1101) at an angle of 16.50° from (1011). Determine the indices of this face. 2.8 In an orthorhombic crystal (topaz) with axial ratios a:b:c = 0.529:1:0.477, the following angles were measured to the face P of the general form: (100)∧P = 67.85°, (010)∧P = 66.5°. Determine the indices of P. 2.9 Calculate the axial ratios a : b : c and the axial angle b for a monoclinic crystal – – – (gypsum) given that (110)∧(110) = 68.5°, (001)∧(110) = 82.3° and (001)∧(101) = 33.1°. – – 2.10 (a) In a hexagonal zeolite crystal the angle (1010)∧(1011) is found to be 37.2°. Calculate the axial ratio c/a and specify the indices of the zone containing both faces in (i) conventional three-dimensional indices and (ii) the Miller–Bravais 4-index notation. – (b) Show that (0001)∧(1122) = 48.8°. Hence, construct a stereogram centred on 0001 – – – – showing all the poles of the form {1010}, {1011}, {1120} and {1122} for this zeolite. 2.11 a-sulphur forms orthorhombic holosymmetric crystals with a = 10.48 Å, b = 12.92 Å and c = 24.55 Å. (a) Draw a sketch stereogram showing the symmetry elements shown by a-sulphur. (b) Calculate the angles (001)∧(011) and (100)∧(110). Insert these poles on a stereogram. (c) Hence, draw an accurate stereogram of sulphur showing all the faces of the forms {100}, {010}, {001}, {101}, {110}, {111}, {011} and {113}. Index all the faces in the upper hemisphere. Which of these are general and which are special forms? 2.12 In dealing with some imperfect crystals with a cubic face-centred lattice it is convenient to use a hexagonal unit cell. The cubic face-centred lattice can be referred to a hexagonal cell where the z-axis is parallel to [111] and of magnitude 3a , where a is the lattice parameter of the conventional cubic unit cell and the x- and y-axes are parallel to the 〈1 0 1〉 directions perpendicular to [111] and of magnitude a / 2 . (a) Draw a diagram showing the relation between the two unit cells. (b) Write the hexagonal lattice vectors in terms of the cubic lattice vectors. Hence, derive the matrix for transforming the indices of lattice planes.

Kelly_c02.indd 83

11/30/2011 7:33:01 PM

84

Crystallography and Crystal Defects

(c) Find the ratio of the volumes of the two unit cells by the matrix method and check by direct calculation. How many lattice points does each contain? – (d) Obtain the hexagonal indices of the planes with indices (112), (100) and (110) referred to the conventional cubic cell.

Suggestions for Further Reading See the suggestions for Chapter 1 as well as the following: T. Janssen (1973) Crystallographic Groups, North-Holland, Amsterdam. W.A. Wooster (1973) Tensors and Group Theory for the Physical Properties of Crystals, Clarendon Press, Oxford.

References [1] M.J. Buerger (1963) Elementary Crystallography, John Wiley and Sons, New York. [2] F.C. Phillips (1971) Introduction to Crystallography, 4th Edition, Oliver & Boyd, Edinburgh. [3] T. Hahn (ed.) (2002) International Tables for Crystallography, 5th, Revised Edition, Vol. A: Space-Group Symmetry, published for the International Union of Crystallography by Kluwer Academic Publishers, Dordrecht. [4] N.F.M. Henry and K. Lonsdale (eds.) (1952) International Tables for X-Ray Crystallography, Volume I, International Union for Crystallography–Kynoch Press, Birmingham, England. [5] W.F. de Jong (1959) General Crystallography: A Brief Compendium, W.H. Freeman, New York. [6] M.A. Carpenter and C.J. Howard (2009) Symmetry rules and strain/order-parameter relationships for coupling between octahedral tilting and cooperative Jahn–Teller transitions in ABX3 perovskites. I. Theory, Acta Crystall. B, 65, 134–146. [7] M.A. Carpenter and C.J. Howard (2009) Symmetry rules and strain/order-parameter relationships for coupling between octahedral tilting and cooperative Jahn–Teller transitions in ABX3 perovskites. II. Application, Acta Crystall. B, 65, 147–159. [8] C.J. Howard and M.A. Carpenter (2010) Octahedral tilting in cation-ordered Jahn–Teller distorted perovskites – a group-theoretical analysis, Acta Crystall. B, 66, 40–50. [9] C. Hermann (1928) Zur systematischen Strukturtheorie I. Eine neue Raumgruppensymbolik, Z. Kristall., 68, 257–287. [10] C. Mauguin (1931) Sur le symbolisme des groupes de répétition ou de symétrie des assemblages cristallins, Z. Kristall., 76, 542–558. [11] A. Schoenflies (1891) Krystallsysteme und Krystallstructur, B.G. Teubner, Leipzig. [12] P.W. Atkins and J. De Paula (2009) Atkins’ Physical Chemistry, 9th Edition, Oxford University Press, Oxford. [13] G. Burns and A.M. Glazer (1990) Space Groups for Solid State Scientists, 2nd Edition, Academic Press, New York. [14] J. Mathews and R.L. Walker (1970) Mathematical Methods of Physics, 2nd Edition, Addison-Wesley, Reading, MA. [15] K.F. Riley, M.P. Hobson and S.J. Bence (2006) Mathematical Methods for Physics and Engineering, 3rd Edition, Cambridge University Press, Cambridge.

Kelly_c02.indd 84

11/30/2011 7:33:04 PM

3 Crystal Structures 3.1

Introduction

The relative positions of the atoms in crystals can be deduced from measurements of the relative intensities of the diffraction spectra using X-rays, electrons or neutrons. X-rays are most useful in this regard because the intensities of the diffracted waves are not as affected by crystalline perfection as are those obtained with electrons. Neutron diffraction is a more specialised technique than X-ray diffraction or electron diffraction, but has distinct advantages when determining the crystal structures of low-atomic-number materials and when locating the atomic positions of elements such as hydrogen in a material. Careful measurements of the spectra enable the electron density to be found throughout the unit cell of a crystal. Since only the outermost electrons are involved in binding the atoms together in a crystal, most of the electrons in the crystal reside in orbits that are the same as those in an isolated atom. The crystal structure can therefore be described by stating the relative positions of atoms within the unit cell. In many crystals of both elements and compounds the charge distribution of the outermost electrons, which are not involved in the chemical binding, are more or less spherically symmetric and therefore the crystal structure is sometimes regarded as being composed of spheres of the same size (if the crystal structure of an element is being considered) or of different sizes (corresponding to the different atoms in a chemical compound) packed together. The crystal structures of the stable elements and of most simple compounds are now well established. These are listed in the Suggestions for Further Reading given at the end of this chapter. We shall now describe a number of the structures, emphasizing the geometrical features of the relative arrangement of the atoms. The imperfections in these crystals, such as point defects, dislocations and grain boundaries, will be described in Part II. When describing each crystal structure we shall state the space group in the style given in the International Tables for Crystallography [1] because from this symbol the Bravais lattice

Crystallography and Crystal Defects, Second Edition. Anthony Kelly and Kevin M. Knowles. © 2012 John Wiley & Sons, Ltd. Published 2012 by John Wiley & Sons, Ltd.

Kelly_c03.indd 85

11/30/2011 4:07:02 PM

86

Crystallography and Crystal Defects

and the point group of the crystal are immediately known (see Section 2.12). Other ways of describing crystal structures are described in Section 3.10. We shall first describe the structures of some of the elements and then those of simple compounds. In many cases a given element or compound possesses more than one crystal structure, each being the thermodynamically stable form in a given regime of temperature and pressure. When this is the case, an element is said to show allotropy and a compound is spoken of as polymorphous. In describing the crystal structures of some compounds we shall sometimes refer to the chemical formulae as being of the type MX, M denoting a metal ion or atom and X an electro-negative element, such as O, F, Cl and so on. Crystal structures can be described by stating the lattice and the coordinates of the atoms in terms of the cell sides as units of length, referred to the lattice point at the origin. In multiply primitive unit cells the same arrangement of atoms must, of course, occur around every lattice point.

3.2

Common Metallic Structures

The vast majority of the elements are metallic. With notable exceptions such as manganese (Mn), gallium (Ga), indium (In), tin (Sn), mercury (Hg), polonium (Po), protoactinium (Pa), uranium (U) and plutonium (Pu) (see Appendix 7), the metallic elements all possess one of four structures: either the cubic close-packed (c.c.p.), hexagonal close-packed (h.c.p.), double hexagonal close-packed (double h.c.p.) or body-centred cubic (b.c.c.). The c.c.p. structure is also frequently referred to as face-centred cubic (f.c.c.); however, we will use the designation c.c.p. here to distinguish clearly between the face-centred cubic1 Bravais lattice and the c.c.p. crystal structure. 3.2.1

– Cubic Close-Packed (Fm3m)

The noble metals (Cu, Ag, Au), the metals of higher valence (Al and Pb), the later transition metals (Ni, Rh, Pd, Ir, Pt) and the inert gases (Ne, Ar, Kr, Xe) when in the solid state all possess this structure (see Appendix 7), as does Fe between 912 and 1394 °C and Co above 420 °C. The lattice is face-centred cubic and there is one atom associated with each lattice point. A conventional unit cell of the structure with lattice parameter a is shown in Figure 3.1a. The conventional unit cell has four lattice points, and therefore four atoms, per unit cell. The relationship of this unit cell to the primitive rhombohedral unit cell for this crystal structure is shown in Figure 3.1b. The coordinates of the atoms in the conventional unit cell are therefore (0, 0, 0), ( 12 , 12 , 0) ,

( 12 , 0, 12 ) and (0, 12 , 12 ) . Each atom possesses 12 nearest neighbours at a distance of a /

2 . The coordination number is thus 12. This structure is the one obtained if equal spheres are placed in contact at the lattice points of a face-centred cubic lattice. A diagram illustrating this is shown in Figure 3.2a. An alternative packing arrangement of equal spheres which produces the hexagonal close-packed structure is shown in Figure 3.2b (Section 3.2.2). If the radius of the spheres is R then R = a / (2 2). The proportion of space filled by the spheres in the c.c.p.

1

Kelly_c03.indd 86

Also known as a cubic face-centred lattice; the two terms are identical.

11/30/2011 4:07:03 PM

Crystal Structures (a)

87

(b)

a

Figure 3.1 (a) The conventional unit cell of the c.c.p. crystal structure. (b) The primitive unit cell of the c.c.p. crystal structure shown within the conventional unit cell (a)

(b)

Figure 3.2 Close packing of equal spheres. (a) Cubic close-packed (c.c.p.). The close-packed layers are parallel to the darker balls. (b) Hexagonal close-packed (h.c.p.). The close-packed layers are horizontal. (After Bragg and Claringbull [9].)

crystal structure is π / (3 2) or 74%. This is described by saying that the packing fraction is 0.74. A packing fraction of 0.74 is the closest packing of equal spheres that can be achieved [2–8], and is the closest packing that can be achieved with equal spheres at the lattice points of a Bravais lattice (see Section 3.6). Rows of spheres are in contact along the line joining their centres. These lines are 〈1 1 0〉 directions in the lattice. Such directions are the closest packed and are termed close-packed directions. There are 12 such directions in all, if account is taken of change in sign. Taking the atomic centres to be at the lattice points, it is apparent from Figure 1.27 that in the {1 1 1} planes, which lie normal to triad axes, the atom centres form a triequiangular net of points. If the atoms are spheres of radius a /2 2 , the appearance of a {1 1 1} plane is

Kelly_c03.indd 87

11/30/2011 4:07:09 PM

88

Crystallography and Crystal Defects

A

A C

C

B A

1] a [121] 6

B A

C

C

a [01 2

B

B A

a [112] 6

A

A C

B

B A

A

B A

Figure 3.3

shown by the full circles in Figure 3.3. Each sphere is in contact with six equidistant spheres with centres in the plane. Since the arrangement shown in Figure 3.3 is the closest packing of circles in a plane, the {111} planes are spoken of as being closest packed, or close-packed. There are eight such planes in the lattice if distinction is drawn between parallel normals of – – – opposite sense (so that, for example, (11 1) and (1 11) are counted separately) and each contains six close-packed directions. The spacing of the {111} planes is a / 3 = 2 2/3 R and so is equal to 2/3 of the atomic spacing in the {111} planes. The centres of the atoms in a particular (111) plane occupy points such as A in Figure 3.3. If the positions of the centres of the atoms in adjacent (111) planes are projected on to this (111) plane, they occupy positions such as those marked B or C in Figure 3.3. The projections of the spheres centred on points B are shown dotted in the figure. A given crystal can be considered to be made up by stacking, one above the other, successive planar rafts of closest-packed spheres so that proceeding in the [111] direction the centres of the atoms in adjacent rafts follow the sequence ABCABCABC… (Figure 3.4a). The same crystal structure, but in a different orientation, would be described by the sequence of rafts ACBACBACB… Any atom in a c.c.p. crystal has 12 nearest neighbours along < 110 > directions at a distance of a / 2 (= 2R), 6 second-nearest along < 100 > directions at a (= 2 2 R) , 24 third-nearest along < 211 > directions at 3/2 a(= 2 3 R) and 12 fourth-nearest along < 110 > directions at

Kelly_c03.indd 88

2 a( = 2 4 R ) .

11/30/2011 4:07:12 PM

Crystal Structures

89

A

(a) A

A A

(b)

C

A

A

C C

A B

B B B

B B

A

A A

A

A A

Figure 3.4 The stacking of closest-packed planes in (a) the c.c.p. structure and (b) the h.c.p. structure

When the c.c.p. crystal structure is regarded as being made up of spheres in contact, the size of the interstices between spheres is important, because many other crystal structures contain at least one set of atoms in either a c.c.p. arrangement or a very close approxima-

tion to it. The largest interstice occurs at positions in the unit cell with coordinates ( 12 , 12 , 12 ) and equivalent positions ( i.e. 0, 12 , 0; 0, 0, 12 and 12 0, 0 ). There are four of these interstice s per unit cell and, hence, one per lattice point; one is illustrated in Figure 3.5. The largest sphere which can be placed in this position without disturbing the arrangement of spheres at the lattice points has radius r = ( 2 − 1) R = 0.414 R. This sphere would have octahedral coordination with six nearest neighbours (Figure 3.5); for this reason these interstices are commonly referred to as octahedral interstices. The sites of these octahedral interstices by themselves form a face-centred cubic lattice.

The second largest interstice occurs at points with coordinates ( 14 , 14 , 14 ) and equivalent positions (Figure 3.6). The largest sphere which can be placed here has radius r = ( 3/2 − 1) R = 0.225 R and possesses tetrahedral coordination; for this reason these interstices are commonly referred to as tetrahedral interstices. There are eight such points in the unit cell and hence two per lattice point. If the atoms in the c.c.p. crystal structure are ignored, the sites of the tetrahedral interstices can be seen to lie on a primitive cubic lattice.

Kelly_c03.indd 89

11/30/2011 4:07:19 PM

90

Crystallography and Crystal Defects

x

Figure 3.5 The largest interstice in the c.c.p. structure: the octahedral interstice

x

Figure 3.6 The second largest interstice in the c.c.p. structure: the tetrahedral interstice

3.2.2

Hexagonal Close-Packed (P63 /mmc)

This structure is exhibited by the early transition metals Sc, Ti, Y and Zr, by the divalent metals Be, Mg, Zn and Cd, and by a number of the rare earth metals (see Appendix 7). The hexagonal primitive unit cell contains two atoms with coordinates (0, 0, 0) and ( 23 , 13 , 21 ) (Figure 3.7). Hence, there are two atoms associated with each lattice point. There is no pure rotational hexagonal axis, but instead 63 axes located at 00z; that is, at the origin of the unit cell (and equivalent sites) running parallel to the z-axis. This structure can be produced by packing together equal spheres, as shown in Figure 3.2b. If each sphere has 12 nearest neighbours equally far away from it, the axial ratio c/a must equal 8/3 = 1.633 . The packing fraction is then 0.74, as in the c.c.p. structure.

Kelly_c03.indd 90

11/30/2011 4:07:25 PM

Crystal Structures

91

c

y

x

a

Figure 3.7 The unit cell of the h.c.p. structure Table 3.1 Axial ratios at room temperature of some metals with an h.c.p. crystal structure Metal Cd Zn Co Mg Re

c/a

Metal

c/a

1.886 1.857 1.625 1.624 1.615

Sc Zr Ti Y Be

1.597 1.593 1.587 1.571 1.568

Values of the axial ratio for a number of metals with this structure are given in Table 3.1. Cobalt has an axial ratio very close to the ideal. It is noteworthy that there are significant departures from the ideal axial ratio: Ti and Zn, for example. If the atomic centres are projected on to a plane parallel to (0001), the basal plane, the structure can be regarded as being made up by stacking rafts of spheres in the sequence ABABAB or ACACAC (Figures 3.3 and 3.4b). If c/a is equal to or greater than the ideal value for sphere packing, there are six – directions of the type 〈1 1 2 0〉 in the basal plane along which atoms touch, and these are the only close-packed directions. If c/a is less than the ideal value, spheres will not touch along these directions, but will be sufficiently close to one another that they can to all intents be regarded as close-packed directions. Octahedral interstices in the h.c.p. crystal structure have coordinates ( 13 , 23 , 14 ) and ( 13 , 23 , 43 ) (Figure 3.8a). There are two such interstices per unit cell and hence one per atom. If c/a = 8/3 then the largest sphere that can be inserted without disturbing the spheres of radius R packed in contact has radius r = 0.414R, just as in the c.c.p. crystal structure. The second-largest interstices, the tetrahedral interstices, lie at 0, 0, 83 , 0, 0, 85 , ( 23 , 13 , 81 ) and ( 23 , 13 , 87 ) (Figure 3.8b). There are four such interstices per cell and hence two per

(

atom. If c/a =

Kelly_c03.indd 91

) (

)

8/3 these have r/R = 0.225, again, just as in the c.c.p. crystal structure.

11/30/2011 4:07:28 PM

92

Crystallography and Crystal Defects (a)

(b)

X

X y

y

x

x

Figure 3.8 Interstices in the h.c.p. arrangement. The octahedral interstices in (a) are denoted by X and the tetrahedral interstices in (b) by open circles

3.2.3

Double Hexagonal Close-Packed (P63 /mmc)

In the eight rare earth metals La, Pr, Nd, Pm, Am, Cm, Bk and Cf, the hexagonal close packing is a four-layer repeat, ABAC. This crystal structure is often referred to as the double h.c.p. structure. The axial ratios characteristic of these metals vary between 3.192 for Pm and 3.262 for Cf, so that in each case they are just below the ideal value of 2 8/3 = 3.266. There are four atoms per unit cell, one octahedral interstice per atom and two tetrahedral interstices per atom. 3.2.4

– Body-Centred Cubic (Im3m)

This structure is shown by the alkali metals Li, Na, K, Rb and Cs, and by the transition metals V, Cr, Fe, Nb, Mo, Ta and W. It is also shown by Ti and Zr at high temperature. The lattice is b.c.c. with one atom at each lattice point, so the atomic coordinates are (0, 0, 0) and ( 12 , 12 , 12 ) (Figure 3.9). Each atom has eight nearest neighbours along 〈111〉 directions at a separation of 3a /2, where a is the lattice parameter. These eight 〈111〉 directions are close-packed directions. Unlike in the c.c.p. and h.c.p. structures, none of the nearest neighbours of one particular atom are nearest neighbours of each other. If the b.c.c structure is presumed to be made up with spheres of equal size, these each have radius R = 3a /4. The packing fraction is π 3 /8 = 0.68. The second-nearest neighbours of an atom are closer than in the c.c.p. structure. There are six second-nearest neighbours along directions at a distance 4 R / 3 = 2.309R (in c.c.p., second-nearest neighbours are at 2 2R = 2.828R) and 12 third-nearest along directions at 4 2 R / 3. There are no closest-packed planes of atoms in this structure. This structure has its largest interstices at coordinates ( 12 , 14 , 0 ) and equivalent positions (Figure 3.10). There are 12 such positions per cell: six per lattice point, and therefore six per atom. The largest sphere fitting in such an interstice has radius r = 5/3 − 1 R = 0.291R. This interstice is therefore significantly smaller than the largest one in c.c.p. It has four nearest neighbours equidistant from it, and so it is a tetrahedral interstice, but the tetrahedron

(

Kelly_c03.indd 92

)

11/30/2011 4:07:41 PM

Crystal Structures

93

a

Figure 3.9 The b.c.c crystal structure

X

O

O = 1, 1, 0 2 2 X = 12 , 14 , 0

Figure 3.10 Tetrahedral (X) and octahedral (O) interstices in the b.c.c crystal structure

that these neighbours form is not regular. The second-largest interstice is at ( 12 , 12 , 0) and equivalent positions (Figure 3.10). There are six such sites per cell ( 6 × 12 at the centres of cube faces and 12 × 14 at the midpoints of cube edges) and so three per lattice point. Each can accommodate a sphere of radius r = (2/ 3 − 1) R = 0.155R; such a sphere is at the centre of a distorted octahedron, and so these interstices are distorted octahedral interstices.

3.3 3.3.1

Related Metallic Structures Indium (I4 /mmm)

The crystal structure of indium is very similar to the c.c.p. structure. It is body-centred tetragonal with c/a = 1.521. This axial ratio is such that, if referred to a face-centred tetragonal lattice instead of the conventional body-centred one, the axial ratio c/a = 1.076.

Kelly_c03.indd 93

11/30/2011 4:07:55 PM

94

Crystallography and Crystal Defects

Therefore, the structure can be described as face-centred tetragonal (F4/mmm), with one atom at each lattice point and an axial ratio of 1.076. 3.3.2

– Mercury (R3m)

Mercury also has a structure that can be described as distorted c.c.p. The primitive unit cell has a rhombohedral lattice with one atom at each lattice point (Figure 3.11). The axial angle a is 70.74° and a = 2.992 Å at 78 K. The primitive unit cell of a c.c.p. crystal has a = 60° (Figure 3.1b). Thus the mercury structure can be derived from the c.c.p. crystal structure by compressing it along a body diagonal of the cell. The atoms in the (111) planes of mercury are therefore arranged to form a triequiangular net but the spacing of these planes is too small to allow closest packing of spherical atoms. The nearest neighbours of any one atom are in adjacent (111) planes. The closest-packed directions are 〈100〉 of the primitive rhombohedral cell of side a (Figure 3.11). There are six nearest neighbours at a distance a. Mercury can, of course, also be referred to a rhombohedral face-centred cell containing four atoms to emphasize the relationship to the conventional cell of an c.c.p. crystal. This larger cell for Hg has a′ = 4.577 Å and axial angle a ′ = 98.36° at 78 K (see Problem 3.4). 3.3.3

b-Sn (I41/amd)

b-Sn, also known as white tin, is the form of tin that is stable at room temperature. It has a body-centred tetragonal lattice with two atoms associated with each lattice point: one at the lattice point and the other at 0, 12 , 14 . The value of c/a at room temperature is 0.546. Each atom has four nearest neighbours at the vertices of an irregular tetrahedron and two more at a slightly greater distance (see Problem 3.5). The structure is a distorted form

(

)

a

a

Figure 3.11 The crystal structure of mercury, showing the primitive rhombohedral unit cell

Kelly_c03.indd 94

11/30/2011 4:08:00 PM

Crystal Structures

95

of the diamond structure (Section 3.4.), which is taken by the form of tin stable below room temperature known as a-Sn or grey tin.

3.4 3.4.1

Other Elements and Related Compounds – Diamond (Fd3m)

The elements Si, Ge, a-Sn (the low-temperature allotrope of tin) and crystalline carbon stable at high temperature and pressure (diamond) all have the structure shown in Figure 3.12. The Bravais lattice is face-centred cubic and there are two atoms associated with each lattice point. The coordinates of these atoms can be taken to be (0, 0, 0) and ( 14 , 14 , 14 ) , or, if the origin is taken to be at a centre of symmetry, ± 81 , 81 , 81 . The coordination number is 4, with the nearest neighbours at a distance 3a /4 arranged at the corners of a regular tetrahedron, outlined in Figure 3.12. The atom centres lie at the corners of triequiangular nets in {111} planes. If these are projected on to (111) the stacking sequence of successive (111) planes can be described as CA AB BC CA AB BC. Successive planes are not equally separated from one another (Figure 3.13). The structure is very loosely packed. If equal spheres in contact have their centres at the atom centres, the packing fraction is only π 3 /16 = 0.34. The diamond crystal structure can be regarded as a special case of the sphalerite crystal structure (sub-section 3.5.3), in which the atoms at (0, 0, 0) and ( 14 , 14 , 14 ) are of different types. For this reason, Figure 3.13 can also be used to show the stacking sequence of the sphalerite crystal structure. In – sphalerite, there are no longer centres of symmetry, so the space group symmetry is F43m (Section 3.5).

(

3.4.2

)

Graphite (P63 /mmc)

The thermodynamically stable crystal structure of carbon at room temperature is graphite, shown in Figure 3.14a. The lattice is hexagonal with four atoms per unit cell, with coordinates

y x

a

Figure 3.12 The crystal structure of diamond

Kelly_c03.indd 95

11/30/2011 4:08:01 PM

96

Crystallography and Crystal Defects

[111]

[112] C b

C B a 4 3

B A

B a

A C

A g

C B

C b

B A

a 3

A C

B a A g

Figure 3.13 The stacking of (111) planes in the diamond and sphalerite structures. The atomic positions are projected onto (110). In diamond, the filled and open circles represent the same type of atom. The sequence of triequiangular nets is described for diamond on the left-hand side and for sphalerite (zinc blende) on the right-hand side

(

)(

)

2 1 1 1 2 , , 0 and ( , , ) . At room temperature a = 2.46 Å and c = 6.71 Å; (0, 0, 0), 0, 0, 12 3 3 2 3 3 thus c/a = 2.72 is large. The atoms in one (0001) plane are arranged at the corners of regular hexagons. The x- and y-axes of the unit cell are shown in Figure 1.1. The structure can be built up by stacking successive hexagonal sheets of atoms one above the other along the z-axis so that the hexagons are in the same orientation, but with half the corners of the hexagons in one plane lying in the centres of the hexagons in adjacent planes (Figure 3.14a). If the atomic centres are all projected on to (0001), the stacking sequence can be described as ABABAB or ACACAC, where it must be remembered that the letters A, B and C refer to sheets of atoms arranged at the corners of hexagons, rather than at the vertices of equilateral triangles, as in the h.c.p. crystal structure, for example. Each atom has three nearest neighbours at a separation of a / 3 in the basal plane. Half of the atoms in any one hexagonal layer have atoms directly above and below them at a distance of c/2. The separation of the nearest neighbours in the (0001) planes is only 1.42 Å (compared with 1.54 Å in diamond) and this is much smaller than the separation of the hexagonal sheets – 3.35 Å. Graphite is therefore said to possess a layer structure because the atoms are strongly bonded within a sheet, and the sheets are only weakly bound to one another through van der Waals forces. If graphite crystals are ground or otherwise severely deformed at low temperature, another form of graphite can be detected in which the atomic hexagons are arranged in the sequence ABCABCABC or alternatively CBACBACBA. This crystal structure has a rhom– bohedral Bravais lattice (space group R3m). The primitive rhombohedral cell has a = 3.635 Å

Kelly_c03.indd 96

11/30/2011 4:08:08 PM

Crystal Structures (a)

97

(b)

y

x Graphite

BN

Figure 3.14 (a) The crystal structure of graphite. (b) The crystal structure of hexagonal boron nitride

and a = 39.5° at room temperature. There are two atoms per unit cell with coordinates ±(u, u, u) where u = 61 (= 0.167). 3.4.3

Hexagonal Boron Nitride (P63 /mmc)

The structure of hexagonal boron nitride thermodynamically stable at room temperature is closely related to that of graphite (Figure 3.14b). The atoms occur in hexagonal sheets, but the sheets are stacked directly above one another along [0001] so that the stacking sequence is described as AAAAA…, with unlike atoms above one another in consecutive layers (see Figure 3.14b). In any one sheet there are equal numbers of B and N atoms arranged so that B and N alternate around any one atomic hexagon. At room temperature the B–N separation in the sheets is 1.45 Å and the separation of the sheets is 3.33 Å. – 3.4.4 Arsenic, Antimony and Bismuth (R3m) The structures of As, Sb and Bi are also based on a primitive rhombohedral Bravais lattice, with two atoms associated with each lattice point. The structure is shown in Figure 3.15. The coordinates of the atoms in the rhombohedral unit cell are ±(u, u, u); u is a little less than 14 and a somewhat less than 60° (see Table 3.2). The structure is easily visualized as being made up of sheets of atoms lying perpendicular to [111]. Within each sheet the atoms are arranged at the corners of triequiangular nets. Referring to Figure 3.15 and noting the values of u, the stacking sequence of these nets along [111] is BA CB AC BA… If u is 14 , the spacing of adjacent nets will be regular. In fact, each atom in any one sheet has three nearest neighbours in the closest adjacent sheet at d1 (see Table 3.2) and three at a slightly greater distance in the sheet on the other side at d2. The possession of three nearest neighbours fits with the positions of As, Sb and Bi in the periodic table, since each atom is

Kelly_c03.indd 97

11/30/2011 4:08:12 PM

98

Crystallography and Crystal Defects

A C A C C

C

B C B

B

B A B

A

Figure 3.15 The crystal structure of As, Sb and Bi Table 3.2

As Sb Bi

Cell dimensions of As, Sb and Bi

a (Å)

a (deg)

u

d1 (Å)

d2 (Å)

4.132 4.507 4.746

54.13 57.11 57.23

0.227 0.233 0.234

2.517 2.908 3.071

3.120 3.355 3.529

expected to form three covalent bonds. If a = 60° and u = 14 in this structure, each atom has six closest neighbours and the arrangement of the atoms is at the points of a simple cubic lattice.

3.5

Simple MX and MX2 Compounds – Sodium Chloride, NaCl (Fm3m)

3.5.1

One-third of all compounds of the type MX crystallize in the sodium chloride (halite) – structure (Fm3m), shown in Figure 3.16. In such compounds the metal atom or ion M is usually smaller than the electronegative element, X. The lattice is face-centred cubic with two different atoms associated with each lattice point: one, say X, at (0, 0, 0) and the other, M, at 0, 0, 12 . Each of the two types of atom, considered in isolation, lies upon a facecentred cubic lattice, and each lies at the largest interstice of the other’s face-centred cubic lattice. From the diagram in Figure 3.5 and from inspection of Figure 3.16, it is then clear that each atom has a coordination number of 6, the neighbours being at the vertices of a regular octahedron. There are four formula units per conventional unit cell but there is clearly no trace of the formation of a molecule of MX in this structure.

(

Kelly_c03.indd 98

)

11/30/2011 4:08:16 PM

Crystal Structures

99

Figure 3.16 The crystal structure of sodium chloride, NaCl

Each {111} lattice plane specifies a double sheet of atoms, each of the sheets consisting entirely of atoms of one kind arranged at the points of a triequiangular net. If we denote sheets of atoms of one kind with a Greek letter and those of the other with a Roman letter, then the stacking sequence along a [111] direction can be described as A g B a C b A g B a C b … The spacing of the sheets of atoms denoted by letters from the same alphabet is a / 3 , where a is the lattice parameter. All of the alkali halides, with the exception of CsCl, CsBr and CsI, crystallize with this crystal structure, as do many of the sulfides, selenides and tellurides of Mg, Ca, Sr, Ba, Pb and Mn, as well as the oxides of formula MO of Mg, Ca, Sr, Ba, Cd, Ti, Zr, Mn, Fe, Co, Ni and U and some transition metal carbides and nitrides such as TiC, TiN, TaC, ZrC, ZrN, UN and UC (see Section A7.2 in Appendix 7). When the metallic ion is of variable valence, crystals with this structure often form with some ion positions unoccupied. For example, FeO crystals would be perfect if they contained only divalent iron, Fe2+. If some Fe3+ ions are present then for every two Fe3+ ions, one of the sites on the iron sublattice must be empty. Such a structure is called a defect structure (see Section 10.1). 3.5.2

– Caesium Chloride, CsCl (Pm3m)

CsCl, CsBr, CsI, as well as many intermetallic compounds such as CuBe, CuZn, AgCd, AgMg – and FeAl (see Section A7.3 in Appendix 7), show the caesium chloride structure (Pm3m), which has a primitive cubic lattice with one atom of each kind associated with each lattice point, one, say X, at (0, 0, 0) and the other, M, at ( 12 , 12 , 12 ) (Figure 3.17). The coordination number is 8 for each atom, the nearest neighbours being at

Kelly_c03.indd 99

3a /2 , where a is the lattice parameter.

11/30/2011 4:08:19 PM

Crystallography and Crystal Defects

100

a 90°

90°

90°

a

a

Figure 3.17 The crystal structure of caesium chloride, CsCl

(a)

(b)

c

y a

a x

Figure 3.18 The crystal structures of (a) sphalerite (a-ZnS) and (b) wurtzite (b-ZnS)

3.5.3

– Sphalerite, a-ZnS (F43m)

– The cubic form of ZnS, designated a-ZnS, shows the sphalerite structure2 (F43m) shown in Figure 3.18. This is also exhibited by the sulphides, selenides and tellurides of Be, Zn, Cd and Hg and the halides of Cu and AgI: see Section A7.4 of Appendix 7 for a tabulation of selected crystals with the sphalerite structure. The lattice is face-centred cubic with one atom of each kind associated with each lattice point, one at (0, 0, 0) and the other at ( 14 , 14 , 14 ) , so the relationship to the structure of diamond (Section 3.4) is very close (Figure 3.13). Each type of atom considered in isolation from the other lies at the lattice points of a face-centred cubic lattice and each lies in the second largest interstice of the close-packed crystal structure

2

Kelly_c03.indd 100

Sometimes called zinc blende.

11/30/2011 4:08:23 PM

Crystal Structures

101

Table 3.3 Axial ratios at room temperature of some materials with the wurtzite crystal structure Material NH4F a-AgI BeO ZnO b-ZnS

c/a

Material

c/a

1.61 1.63 1.63 1.60 1.63

b-CdS CdSe AlN SiC TaN

1.62 1.63 1.60 1.65 1.62

of the other. The coordination number is 4, the nearest neighbours being atoms of the other kind at a distance 3a /4 arranged at the vertices of a regular tetrahedron. The sequence of (111) planes is stacked at the same intervals as in diamond (Figure 3.12), but alternate planes are occupied by atoms of different chemical species. Thus, following the same nomenclature as for NaCl, the stacking sequence is g A a B b C g A … (Figure 3.13). 3.5.4 Wurtzite, b-ZnS (P63mc) The sphalerite structure is derived from the c.c.p. structure by placing atoms of a different kind to those at the lattice points at every other tetrahedrally coordinated interstice. A related structure, also shown by ZnS, is obtained by filling alternate tetrahedrally coordinated interstices in the h.c.p. structure. This is the b-ZnS or wurtzite structure (P63mc). The lattice is hexagonal with atoms of one kind at (0, 0, 0) and ( 23 , 13 , 21 ) and those of the other kind at (0, 0, u) and 23 , 13 , 21 + u (Figure 3.18b). The value of u is very close to 0.375, i.e. 83 ; however, it is not constrained by symmetry to be exactly 0.375. From Figure 3.8b the relationship to the h.c.p. structure is obvious. Each atom is, of course, tetrahedrally coordinated with four of the opposite kind. The stacking of planes of atoms parallel to (0001) using the same nomenclature as for NaCl and a-ZnS is then A a B b A a B… or equivalently A a C g A a C g A … This structure is shown by a number of compounds (Table 3.3). The axial ratios shown in Table 3.3 and Section A7.5 of Appendix 7 are quite close to the ideal, 1.633, for hexagonal close packing of one type of ion with the other in the tetrahedral interstices.

(

3.5.5

)

Nickel Arsenide, NiAs (P63/mmc)

We described the sodium chloride structure as being derived from the c.c.p. structure by placing a second set of atoms in the octahedrally coordinated largest interstices of the structure. It is not surprising therefore that a structure exists in which atoms of a different kind are placed in the octahedral interstices of the h.c.p. structure. This is the nickel arsenide (nickeline)3 structure (P63/mmc) (Figure 3.19). The lattice is hexagonal, with atoms of one kind at (0,0,0) and 0, 0, 12 and those of the other kind at ( 23 , 13 , 14 ) and ( 13 , 23 , 34 ). For both kinds of atom the coordination number is 6, but while the sites occupied by one kind of atom, those denoted by open circles in Figure 3.19, lie in positions corresponding to a

(

3

)

Also known as niccolite.

Kelly_c03.indd 101

11/30/2011 4:08:24 PM

102

Crystallography and Crystal Defects

= As = Ni c

y a x

Figure 3.19 The crystal structure of nickel arsenide, NiAs

Table 3.4 Axial ratios at room temperature of some materials with the nickel arsenide structure Material NiAs CrS FeS

c/a

Material

c/a

1.40 1.64 1.66

CoS NiS

1.52 1.55

close-packed hexagonal arrangement (As), the others (Ni) lie at the lattice points of a primitive hexagonal lattice (if the As atoms are ignored), with a repeat distance in the c direction half that of the lattice parameter of the NiAs crystal structure. This difference in stacking of the M and X atoms is obvious from Figure 3.8a and also by stating the stacking sequence of the planes of atoms along [0001] following the procedure for NaCl. The stacking sequence is A b A g A b A g … The atoms denoted by Greek letters lie in the centre of a trigonal prism of atoms denoted by Roman letters, while the atoms denoted by Roman letters are octahedrally coordinated. The axial ratios of some crystals of sulphides with this structure are listed in Table 3.4; the selenides, tellurides and antimonides of the metals listed often have the same structure: see Section A7.6 of Appendix 7. The values of c/a at room temperature depart from the ideal for hexagonal close packing of one type of ion. Usually the metal atom is situated in the type of site occupied by Ni in NiAs, but in PtB the ‘anti-NiAs’ structure is shown. 3.5.6

– Calcium Fluoride, CaF2 (Fm3m)

If all of the tetrahedral interstices in the c.c.p. crystal structure are filled with atoms of a different kind from those in the c.c.p. crystal structure, we obtain the calcium fluoride – (CaF2) or fluorite structure (Fm3m) (Figure 3.20). The lattice is face-centred cubic with

Kelly_c03.indd 102

11/30/2011 4:08:33 PM

Crystal Structures

103

=F = Ca

a

Figure 3.20 The crystal structure of calcium fluoride, CaF2

atoms of one kind, for example Ca, at (0, 0, 0) and equivalent positions, and with F atoms at ( 14 , 14 , 14 ) and ( 14 , 43 , 14 ) and equivalent positions. There are clearly four formula units per unit cell. The coordination number of Ca is 8, with the nearest neighbours being atoms of F arranged at the corners of a cube. If the calcium atoms are ignored, it is apparent that the fluorine atoms lie at the lattice points of a primitive cubic lattice. Each F atom has tetrahedral coordination with four Ca atoms. The centres of atoms of one kind all form triequiangular nets of points parallel to {111} lattice planes. The separation of the atoms in these places is the same for the two types of atom. The stacking sequence of these planes along [111] can therefore be described as … aBg bCa g Ab aBg bCa … The planes of atoms denoted by successive Roman letters are regularly spaced from one another; the same is true of the planes of atoms denoted by Greek letters. This structure is shown by the fluorides of Ca, Sr and Ba and by the oxides of Zr, Th, Hf and U. Oxides and sulfides of alkali metals also show this structure; in these cases it is sometimes called the antifluorite structure. A tabulation of crystals with the flourite structure is given in Section A7.7 of Appendix 7. 3.5.7

Rutile, TiO2 (P42/mnm)

A common structure of compounds with the formula AX2, besides that of fluorite, is the rutile (TiO2) structure (P42/mnm) (Figure 3.21a). It is also sometimes called the cassiterite (SnO2) structure. A number of dioxides and fluorides have this crystals structure, such as those tabulated in Section A7.8 of Appendix 7. The lattice is primitive tetragonal with c/a about 0.65. There are titanium atoms at (0, 0, 0) and ( 12 , 12 , 12 ) and oxygen atoms at ± (u, u, 0) and ± (u + 12 , 12 − u, 12 ) , where u is close to 0.30 in all examples of the structure. Thus, there are two formula units per cell. A plan of the structure is shown in Figure 3.21b, projected down [001]. Each Ti atom is surrounded by six O atoms, but the octahedron of O atoms is not a regular octahedron. It is apparent that the crystal structure of rutile can be described in terms of how these Ti octahedra pack together. This leads conceptually to the more general geometry of the packing of polyhedra, which will be

Kelly_c03.indd 103

11/30/2011 4:08:33 PM

104

Crystallography and Crystal Defects

(a)

(b) y Ti 0

Ti 0 0.5 0

O 0.5 Ti

c

O

0

O

a

0 Ti

TiO2

= Ti

0.5

O

0 Ti

x

=O

Figure 3.21 (a) The crystal structure of rutile, TiO2. (b) The rutile crystal structure projected down [001]. The numbers indicate the z-coordinates of the atoms

discussed in Section 4.4 in the context of the packing of atoms or ions within very complicated crystal structures.

3.6

Other Inorganic Compounds

As we have seen in the descriptions of simple crystal structures in Sections 3.2–3.5, the concept of the packing of spheres into arrangements that are close-packed is of great practical use. It is also useful for circumstances where there are departures from the most close-packed ideal arrangement shown by c.c.p. crystal structures or h.c.p. crystal structures where c/a = 8 / 3, so that a ‘close-packed’ arrangement of one type of atom or ion (not necessarily in contact) occurs, with the interstices filled or partly filled with smaller atoms (or ions). Simple examples of such structures have already been considered in Section 3.5. In this section we consider other examples where the chemistry is less simple, or where the packing departs significantly from the ideal close-packed arrangement. 3.6.1

– Perovskite (Pm3m)

This primitive cubic crystal structure is a very common structure of crystals of compounds of the type MM′X3. It is named after the mineral perovskite, CaTiO3, which has this crystal structure above 900 °C; at room temperature, CaTiO3 has an orthorhombic crystal structure belonging to the space group Pnma (see Section 2.15).4 In this crystal structure, the calcium (M) and oxygen (X) ions taken together form a c.c.p. arrangement with the titanium (M′) ions in the octahedral voids (Figure 3.22). The coordination number of Ca is 12, that of 4

Kelly_c03.indd 104

SrTiO3 has this crystal structure at room temperature.

11/30/2011 4:08:38 PM

Crystal Structures

O

Ca

105

Ti

– Figure 3.22 The crystal structure of perovskite, Pm3m

Ti is 6 and that of O is 2. The atomic coordinates in the primitive unit cell are Ti ( 12 , 12 , 12 ) , Ca (0, 0, 0) and O 12 , 12 ,0 , 0, 12 , 12 , 12 , 0, 12 . The description of the perovskite crystal structure in terms of the packing of titanium octahedra will be deferred to Section 4.4. There are many slightly distorted forms of the perovskite structure that are important in solid-state devices. At room temperature, barium titanate, BaTiO3 (P4mm), has a crystal – structure that is a tetragonally distorted form of the Pm3m high-temperature structure. At lower temperatures, further distortions convert this into an orthorhombic crystal structure (Amm2) and a rhombohedral crystal structure (R3m) [10]. Pb(Zr1−xTix)O3, in which the Zr and Ti ions both occupy the M′ position, has two different rhombohedral (R3m and R3c) crystal structures [11] and a tetragonal (P4mm) form at room temperature, dependent on the value of x. The high-temperature superconducting oxide YBa2Cu3O7−d , where d is a small fraction 0 ⎝ ⎠

(4.8)

Hence, it follows that if m = n, they can both only take the value 3; integers 4 or greater would not satisfy this inequality. If m = 3, possible values of n which satisfy Equation 4.7 for integer E are 3, 4 and 5, giving E = 6, 12 or 30: the tetrahedron, the cube and the dodecahedron, respectively. If n = 3, solutions for m are 3, 4 or 5, giving the tetrahedron, the octahedron and the icosahedron, respectively. Many examples where use was made of the first three Platonic solids are discussed in Chapter 3 in order to describe a crystal structure; for example, the tetrahedron was used for the diamond structure and the cube for the sodium chloride structure. The description of crystal structures given in Chapter 3 is useful, but its formality, based as it is on the Bravais lattice, often fails to indicate the way in which the solid crystal is bound by the forces between the component atoms. For this reason, it is often useful to describe crystal structures in terms of an assemblage of polyhedra linked in various ways. This approach can help to simplify the description of the structures and bring out the crystal chemistry or explain why a crystal possesses a desirable physical property. Thus, for example, the rutile structure, MX2 (sub-Section 3.5.7), can be described either as a complex assemblage of oxygen ions, with the titanium ions occupying one-half of the octahedral cavities, or alternatively, and more powerfully, as an assemblage of slightly distorted TiO6 octahedra linked by their corners and edges. The perovskite structure, MM′X3 (sub-Section 3.6.1), can be regarded as a framework of M′X6 octahedra linked by their corners, each X being shared by two octahedra. The result is a three-dimensional assemblage of

Kelly_c04.indd 133

11/29/2011 7:06:00 PM

134

Crystallography and Crystal Defects

octahedra whose tetragonal axes coincide with those of the unit cell. When the relative dimensions of the octahedra of M′ ions are incompatible with this configuration, the structure becomes slightly distorted, causing a lowering in symmetry. –– The regular dodecahedron, the fourth Platonic solid, has m3 5 point group symmetry. It has 12 five-fold axes, 20 triads and 30 diads and mirror planes. The 12 five-fold axes are at an angle to one another of tan−1 2 = 63.43°. Seen in projection looking down one of the five-fold axes, the other five adjacent five-fold axes are all at 72° to one another. Sets of rods (or fibres) aligned normal to the faces of a regular dodecahedron can produce an elastically isotropic solid; this requires that the cross-sections of the rods have specific shapes and that these be arranged to meet each other in specified ways [12].

4.5

Icosahedral Packing

Regular dodecahedral packing has not so far been shown to be of great use in the description and understanding of complicated crystal structures, in contrast to the icosahedron. This also –– has m3 5 point group symmetry, with 12 five-fold rotation axes, 20 triads and 30 diads and mirror planes. The importance of the icosahedron arises because of its close relationship with cubic close packing. In the cubic close-packed (c.c.p) assembly of equal spheres, each sphere is surrounded by a first coordination polyhedron of 12 identical spheres (Section 3.2). Each neighbouring sphere is situated at a vertex of a cubo-octahedron (see Figure 13.28a). This 14-sided figure has eight hexagonal faces and six square faces and can be formed by suitably truncating a cube with planar slices at the eight vertices to form the eight equilateral triangular faces. At each new vertex produced, exactly halfway along the edges of the original cube, two hexagonal faces and two square faces meet. A second layer of spheres packed similarly over the first layer will be found to require 42 spheres to complete it. In general, it may be shown that if the structure of spheres is continued, the nth layer will consist of (10n2 + 2) spheres [13]. The cubo-octahedron can be transformed into a regular icosahedron by compression of some 5% along the line joining the vertices to the centre and allowing the square faces to become rhombs, and each to split into two triangular faces. This movement is easily illustrated on a stereogram (Problem 4.5). When an icosahedron of 12 spheres about a central sphere is surrounded by a second icosahedral sphere, the second shell will also contain 42 spheres. The second shell will lie over the first, so that spheres will be in contact along the six five-fold axes of symmetry. These spheres will not be close-packed. The packing density of such an icosahedral shell packing is less than that of the c.c.p. structure, 0.74, but nonetheless can be quite high; close to 0.69, which is a higher packing fraction than is found in body-centred cubic (b.c.c.) (0.68) [13]. The packing fraction in this icosahedron shell packing can be calculated by noting that within the solid icosahedron the unit that is repeated is a distorted tetrahedron; 20 of these make up the solid icosahedron. An icosahedral packing of equal spheres is shown in Figure 4.6. On each triangular face, the layers of spheres succeed each other, just as in the c.c.p. sequence. Each of these spheres touches just six neighbours, three above and three below, and is separated by a distance of 5% of its radius from its six neighbours in the plane of the icosahedron. Icosahedral packing is extremely useful for describing structures containing many types of atom of very different sizes. The polyhedra within a given structure can have various

Kelly_c04.indd 134

11/29/2011 7:06:02 PM

Amorphous Materials and Special Types of Crystal–Solid Aggregates

135

Figure 4.6 Packing of equal-sized spheres into an icosahedral arrangement. The diagram shows the third layer of spheres. (After Mackay [13].)

shapes in order to accommodate atoms or ions of different sizes. They are often referred to as topologically close-packed (TCP) structures or Frank–Kasper phases [14,15]. TCP structures enable a closer packing of atoms to arise than is found in the geometrically closepacked structures (c.c.p. and hexagonal close-packed, h.c.p.). There are many examples in the literature of metallic alloys with TCP structures containing three or more types of atom. In general, TCP structures are made up of clusters of polyhedra, with the symmetry of the whole crystal being less than that of the individual clusters. Icosahedral coordination frequently occurs in TCP structures, as do clusters containing 55 or more atoms. Examples of icosahedral coordination can be found in compounds such as MoAl12 (Figure 4.7), WAl12 – and Mn0.5Cr0.5Al12 [16]. The space group of these compounds is now designated Im3. Some of the triads and diads from the icosahedral arrangement of the Al atoms are retained in the crystal, but the five-fold rotational axes of the individual MoAl12 units are lost.

4.6

Quasicrystals

The perovskite example is one where, in order to maintain the essential packing of the ions, the deviation from ideal symmetry is towards a lower symmetry (Sections 3.6 and 4.4). In some cases, particularly where the packing is based on clumps of atoms with nearly close packing, the point symmetry may be greatly increased, so that it exceeds that compatible with repetition at the points of a Bravais lattice. The famous first report of five-fold rotational symmetry in a solid occurred in 1984, in a paper whose title amply describes the effect: ‘Metallic phase with long-range orientational order and no translational symmetry’ [17]. For this discovery, the first author of the paper, Daniel Shechtman, was awarded the 2011 Nobel Prize for Chemistry. The compositions of

Kelly_c04.indd 135

11/29/2011 7:06:03 PM

136

Crystallography and Crystal Defects

Figure 4.7 The crystal structure of MoAl12. This figure is derived from Figure 1 of [16]. Molybdenum (Mo) atoms (heavily shaded) are found at the corners and centre of the unit cell. Each Mo is surrounded by 12 aluminium atoms (lightly shaded) arranged at the 12 vertices of a regular icosahedron

the alloys investigated were relatively simple: Al with 10–14 wt% of Mn, Fe or Cr. Since these initial observations, many examples have been found in related alloy systems of metallic phases without translational symmetry in two or three dimensions. These can show a number of ‘forbidden’ rotational symmetries (e.g. 5-, 8-, 10- or 12-fold symmetry), which are completely incompatible with the possession of a Bravais lattice as defined so far in this book. Such structures are best described in terms of the regular or slightly irregular (distorted) polyhedra, often icosahedra. Phases with icosahedral symmetry are often referred to as i-phases. Useful reviews of quasicrystals can be found in [18] and [19]. The first quasicrystals were produced by rapid cooling from the melt. Although this is still a common way of producing quasicrystalline phases, quasicrystalline phases of suitable compositions can now be produced in centimetre sizes by conventional crystal growth methods, such as in i-Al–Mn–Pd. It is common for i-phases to be formed over a range of compositions, such as in i-Mg–Al–Zn alloys [18]. There is often a quasicrystalline phase and a crystalline phase of the same composition in the same alloy. Three typical alloys readily showing both crystal and quasicrystal behaviour are α-Al–Mn–Si, Mg32(Al,Zn)49 and Al5.6Li2.9Cu. In such alloys, it is usual for the crystalline phase to have a relatively large unit cell, and to be referred to as an approximant (of the quasicrystal). A notable feature of quasicrystals is that they can be almost free of defects: this can be deduced directly from the contrast seen in transmission electron microscopy of individual icosahedral grains, but also from the extreme sharpness of the X-ray diffraction peaks – which are often as sharp as those found from very carefully prepared silicon crystals. 4.6.1 A Little Recent History and a New Definition As we have noted above, the history of quasicrystals began in 1984 with their discovery by Shechtman and his coauthors. Since then, hundreds of quasicrystals have been discovered. Very recently, evidence has been produced that quasicrystals might form naturally in Al–Cu–Fe minerals, producing the Al65Cu24Fe13 phase [20]. Following these many discoveries, the International Union of Crystallography has amended its definition of a

Kelly_c04.indd 136

11/29/2011 7:06:03 PM

Amorphous Materials and Special Types of Crystal–Solid Aggregates

137

crystal so as to include ordering of the atoms in either a periodic or an aperiodic manner. Nowadays those symmetries compatible with translational symmetry are defined as crystallographic. This leaves room for ‘noncrystallographic symmetries’. Hence crystals can be divided into two main classes: those with crystallographic point group symmetry, to which all of the structures described in this book other than in this section belong, and those with noncrystallographic symmetry, to which the quasicrystals described in this section and the incommensurate structures described in Section 4.7 belong.

4.7

Incommensurate Structures

In addition to quasicrystals, there are other types of aperiodic structures. The first incommensurate phases were discovered in the 1970s [21]. A good example of an incommensurate phase is a magnetic system in which the magnetization has a helical structure with a pitch that does not have a rational relation to the underlying lattice [21,22]. Expressed mathematically, two periodicities q1 and q2 in the same direction in a lattice are incommensurate if their ratio cannot be expressed as a ratio of two integers M and N. That is: q1 M ≠ M , N = 1,2,3… q2 N Many materials are now known which display two or more periodicities that are incommensurate with each other. A well-known example of an incommensurate structure is the modulated structure which appears over a narrow 1.3 K temperature range in the high ↔ low phase transition in quartz [23]. A second example can be found in the mineral calaverite [24].

4.8

Foams, Porous Materials and Cellular Materials

While the emphasis in this book is on the arrangements of atoms in single crystals, there are a number of sections, such as those concerned with crystalline textures and interfaces, in which we note that most materials are usually arranged in polycrystalline aggregates. The interfaces between the individual crystals, known as grain boundaries or interphase boundaries (Chapter 13), are usually just a few atoms wide. These boundaries form a continuous skeleton within which the individual crystals are contained. If we imagine a solid metal or ceramic consisting only of these intercrystalline regions, with the material of the individual crystals removed, we should have a material with the geometry of a foam. An example of the microstructure of a solid foam is shown in Figure 4.8 [25,26]. The foam is an important type of porous solid, which itself is a class of cellular solids [27]. Polymer foams such as those of polyurethane and polystyrene have been known for many years, and there are natural cellular materials, such as zeolites and sponges – the term ‘sponge’ usually denotes a very flexible foam. Recent technical advances in techniques for foaming metal and ceramic have led to intense research into such materials. The nomenclature for describing the architecture of foams and other forms of porous solids is not completely consistent. The terms ‘three-dimensional meshes’ and ‘lattice structures’ are also used to describe foamed materials. The International Union of Pure and Applied Chemistry (IUPAC) recommendations for the characterization of porous solids [28] describe pore diameters of less than 2 nm as micro; between 2 and 50 nm as meso and

Kelly_c04.indd 137

11/29/2011 7:06:03 PM

138

Crystallography and Crystal Defects

5 mm

Figure 4.8 The microstructure of a foam made from an Al −9 wt% Si alloy containing 10 vol% of silicon carbide particulates [25,26]. Pretreated titanium dihydride, TiH2, was used as the foaming agent

greater than 50 nm as macro, but these definitions are not consistently maintained. These authors of the IUPAC recommendations had in mind catalysts, absorbents and membranes primarily. They define materials as constitutively porous if their final structure depends mainly on the original structure, such as pores in zeolites or amorphous carbon. Materials made porous by a subtractive processing route have material removed from them: chemically etched porous silicon is an example of such a material. The volume fraction of porosity is the fraction of the total volume occupied by pores; that is, Vp/V, where Vp is the total volume of pores and V the total volume of specimen. Pores are open if accessible by the particular probe used, and closed if they are not: the definition depends on the type of probe employed. Open pores are interconnected; the same range of sizes micro, meso and macro may be used to define the diameter of the connecting channels. It is also possible to have mesopores with micro-connectivity or mesopores with meso-connectivity. The term porous metal or porous ceramic usually suggests a porosity range of 15–75%. This range of porosity is shown by metals used in filtration, fluid flow control, self-lubricating bearings and battery electrodes. True foams have high porosities, such as 80–90%, and it is these that provide a distinct advantage for energy and sound absorption, vibration suppression and thermal management. A special form of closed-cell foam is a syntactic foam consisting of small spheres, which are stuck together (Greek: συνταξις – arrangement). If the pores are hollow and the interstices are completely filled, the maximum porosity is about 65%. To a first approximation, most porous structures can be regarded as equiaxed, although it is possible to obtain porous metals and ceramics with elongated structures, the so-called lotus structures; anodized aluminium is a particularly good example. The properties of porous materials are governed by three main factors: 1. The properties of the solid forming the walls of the foam. 2. The topology (connectivity) and shape of the faces and edges of the individual cells. 3. The relative density rf /rs of the foam, where rf is the overall density of the foam, and rs that of the solid material within it. When estimating the mechanical properties of cellular materials, reference is often made to lattice structures, which in this case refers to a connected set of struts, rather than the term used elsewhere in this book. In this context, a lattice, truss or space frame means an array of struts pin-jointed or rigidly bonded at their connections. Foams are like the trusses and frames of space structures, and so are made up of a connected array of struts or plates. They

Kelly_c04.indd 138

11/29/2011 7:06:04 PM

Amorphous Materials and Special Types of Crystal–Solid Aggregates

139

are characterized by a typical ‘unit cell’ with symmetry elements, even though most foams do not show translational symmetry. However, these lattices, cellular materials and foams differ from the lattices of the engineer in one very important regard: that of scale of size. The unit cell of a cellular material is one on the scale of micrometres–millimetres, or sometimes less, so allowing it to be viewed both as structure and as material. Although a foam may not show translational symmetry, the identification of a typical (or average) ‘unit cell’ is very important for describing the overall symmetry of the physical properties, such as elastic properties. This same procedure is used with composite materials – the best known of which, and presently the most useful, are the fibre composites, consisting of stiff fibres arranged in a soft and yielding matrix. Here, the ‘unit cell’ is termed the representative volume element. We shall revisit similar structures in Chapter 13.

Problems 4.1 Determine the shape of the polyhedron which represents the Voronoi polyhedron for a c.c.p. arrangement of spheres. What is the name of this polyhedron? 4.2 Construct the Schlegel figure for the rhombic dodecahedron. 4.3 Describe a solid having five vertices and six triangular faces. 4.4 Draw a stereogram of each of the Platonic solids and insert all of the symmetry elements; make the primitive of the stereogram parallel to the chosen plane of the relevant Schlegel diagram. 4.5 By placing a triad axis of the cubo-octahedron at the centre of the primitive, draw a stereogram to illustrate the distortion of a cubo-octahedron, so as to form a regular icosahedron. 4.6 Show that in c.c.p., the nth layer packed over the layers below is the surface of a cubooctahedron on which there are (n + 1) spheres along each of its edges. Hence show that the nth layer consists of (10n2 + 2) spheres. Explain why in an icosahedrally-packed assembly of equal spheres the nth layer packed over the layers must also consist of (10n2 + 2) spheres. 4.7 Giving your reasons, explain whether MoAl12 has crystallographic point group symmetry or noncrystallographic point group symmetry. 4.8 Give a logical reason why the porosity limit of a syntactic foam is very close to Bernal’s packing fraction for a liquid.

Suggestions for Further Reading S.M. Allen and E.L. Thomas (1999) The Structure of Materials, John Wiley and Sons, New York. A.M. Donald, A.H. Windle and S. Hanna (2006) Liquid Crystalline Polymers, 2nd Edition, Cambridge University Press, Cambridge. L.J. Gibson and M.F. Ashby (1997) Cellular Solids: Structure and properties, 2nd Edition, Cambridge University Press, Cambridge. C. Janot (1994) Quasicrystals: A Primer, 2nd Edition, Clarendon Press, Oxford. F.R.N. Nabarro (ed.) (1992) Dislocations in Solids, Vol. 9. Dislocations and Disclinations, North Holland, Amsterdam.

Kelly_c04.indd 139

11/29/2011 7:06:04 PM

140

Crystallography and Crystal Defects

References [1] J.D. Bernal (1959) A geometrical approach to the structure of liquids, Nature, 183, 141–147. [2] J.A. Elliott, A. Kelly and A.H. Windle (2002) Recursive packing of dense particle mixtures, J. Mater. Sci. Lett., 21, 1249–1251. [3] G.F. Voronoï (1908) Nouvelles applications des paramètres continus à la théorie des formes quadratiques. Deuxième mémoire. Recherches sur les parallélloèdres primitifs, J. reine angew. Math. (Crelle’s Journal), 134, 198–287. [4] B. Valenti and M.L. Sartirana (1984) Mesophase formation in lyotropic polymers, Il Nuovo Cimento, 3, 104–120. [5] F. Reinitzer (1888) Beiträge zur Kenntniss des Cholesterins, Monatshefte für Chemie, 9, 421–441. [6] O. Lehmann (1889) Über fliessende Krystalle, Z. Phys. Chem., 4, 462–472. [7] G. Friedel (1922) Les états mésomorphes de la matière, Ann. Physique, 18, 273–474. [8] F.R.N. Nabarro (1987) Theory of Crystal Dislocations, Dover Publications, New York. [9] F.C. Frank (1958) On the theory of liquid crystals, Disc. Faraday Soc., 25, 19–28. [10] H.S.M. Coxeter (1961) Introduction to Geometry, John Wiley and Sons, New York. [11] V. Schlegel (1883) Theorie der homogen zusammengesetzten Raumgebilde, Nova Acta Academiae Caesareae Leopoldino-Carolinae Germanicae Naturae Curiosorum, 44, 343–459. [12] J.G. Parkhouse and A. Kelly (1998) The regular packing of fibres in three dimensions, Proc. Roy. Soc. Lond. A, 454, 1889–1909. [13] A.L. Mackay (1962) A dense non-crystallographic packing of equal spheres, Acta Crystall., 15, 916–918. [14] F.C. Frank and J.S. Kasper (1958) Complex alloy structures regarded as sphere packings. I. Definitions and basic principles, Acta Crystall., 11, 184–190. [15] F.C. Frank and J.S. Kasper (1959) Complex alloy structures regarded as sphere packings. II. Analysis and classification of representative structures, Acta Crystall., 12, 483–499. [16] J. Adam and J.B. Rich (1954) The crystal structure of WAl12, MoAl12 and (Mn, Cr)Al12, Acta Crystall., 7, 813–816. [17] D. Shechtman, I. Blech, D. Gratias and J.W. Cahn (1984) Metallic phase with long-range orientational order and no translational symmetry, Phys. Rev. Lett., 53, 1951–1953. [18] A.I. Goldman and K.F. Kelton (1993) Quasicrystals and crystalline approximants, Rev. Mod. Phys., 65, 213–230; erratum 579. [19] W. Steurer (2004) Twenty years of structure research on quasicrystals. Part I. Pentagonal, octagonal, decagonal and dodecagonal quasicrystals, Z. Kristall., 219, 391–446. [20] L. Bindi, P.J. Steinhardt, N. Yao and P.J. Lu (2009) Natural quasicrystals, Science, 324, 1306–1309. [21] P. Bak (1982) Commensurate phases, incommensurate phases and the devil’s staircase, Rep. Prog. Phys., 45, 587–629. [22] M. Habenschuss, C. Stassis, S.K. Sinha, H.W. Deckman and F.H. Spedding (1974) Neutron diffraction study of the magnetic structure of erbium, Phys. Rev. B, 10, 1020–1026. [23] A. Putnis (1992) Introduction to Mineral Sciences, Section 12.3, Cambridge University Press, Cambridge. [24] W.J. Schutte and J.L. de Boer (1988) Valence fluctuations in the incommensurately modulated structure of calaverite AuTe2, Acta Crystall. B, 44, 486–494. [25] V. Gergely, D.C. Curran and T.W. Clyne (2003) The FOAMCARP process: foaming of aluminium MMCs by the chalk-aluminium reaction in precursors, Comp. Sci. Tech., 63, 2301–2310. [26] V. Gergely and T.W. Clyne (2000) The FORMGRIP process: foaming of reinforced metals by gas release in precursors, Adv. Engng. Mater., 2, 175–178. [27] L.J. Gibson and M.F. Ashby (1997) Cellular Solids: Structure and properties, 2nd Edition, Cambridge University Press, Cambridge. [28] J. Rouquerol, D. Avnir, C.W. Fairbridge, D.H. Everett, J.H. Haynes, N. Pernicone, J.D.F. Ramsay, K.S.W. Sing and K.K. Unger (1994) Recommendations for the characterization of porous solids, Pure & Appl. Chem., 66, 1739–1758.

Kelly_c04.indd 140

11/29/2011 7:06:04 PM

5 Tensors 5.1

Nature of a Tensor

There are a number of ways to introduce tensors. We shall begin by considering tensors of zero, first and second rank, before extending our discussion to tensors of third and fourth rank. Scalar quantities are examples of tensors of zero rank; these simply have magnitude. Vectors are tensors of the first rank. These have both direction and magnitude and represent a definite physical quantity. Tensors of the second rank are quantities that relate two vectors. Suppose we wish to know the relationship between the electric field in a crystal, represented by the vector E, and the current density (i.e. current per unit area of cross-section perpendicular to the current), represented by the vector J.1 In general, in a crystal the components of J referred to three mutually perpendicular axes (Ox1, Ox2, Ox3), which we can call J1, J2 and J3, will be related to the components of E, referred to the same set of axes in such a way that they each depend linearly on all three of the components E1, E2 and E3. It is usual to write this in the following way: J1 = σ 11 E1 + σ 12 E2 + σ 13 E3 J 2 = σ 21 E1 + σ 22 E2 + σ 23 E3 J 3 = σ 31 E1 + σ 32 E2 + σ 33 E3

(5.1)

The nine quantities s11, s12, s13, s21, s22, s23, s31, s32, s33 are called the components of the conductivity tensor. The electrical conductivity tensor relates the vectors J and E. If we write all of the relations (5.1) in the shorthand form: J=σ E

(5.2)

1

It is conventional to denote current density by j, as in Section A1.3 and in [1]. However, j is used in this chapter to denote a unit vector along Ox2.

Crystallography and Crystal Defects, Second Edition. Anthony Kelly and Kevin M. Knowles. © 2012 John Wiley & Sons, Ltd. Published 2012 by John Wiley & Sons, Ltd.

Kelly_c05.indd 141

11/30/2011 7:18:26 PM

142

Crystallography and Crystal Defects

Table 5.1

Properties represented by second-rank tensors

Tensor Electrical conductivity Thermal conductivity Diffusivity Permittivity Dielectric susceptibility Permeability Magnetic susceptibility

Vectors related Electric field Thermal gradient (negative) Concentration gradient (negative) Electric field Electric field Magnetic field Magnetic field

Current density Thermal current density Flux of atoms Dielectric displacement Dielectric polarization Magnetic induction Intensity of magnetization

we see that s is a quantity that multiplies the vector E in order to obtain the vector J. When a tensor relates two vectors in this way it is called a tensor of the second rank or second order. Many physical properties are represented by tensors like the electrical conductivity tensor. Such tensors are called matter tensors. Some examples are given in Table 5.1. In addition there are field tensors, of which two second-rank tensors are very important, namely stress and strain. The stress tensor relates the vector traction (force per unit area) and the orientation of an element of area in a stressed body. The strain tensor relates the displacement of a point in a strained body and the position of the point (see Chapter 6).

5.2 Transformation of Components of a Vector If we know the components of a vector, say p, referred to a set of orthogonal axes (Ox1, Ox2, Ox3), each of unit length – that is, orthonormal axes (Appendix 1) – it is often necessary to know the components of the same vector referred to a different set of axes (Ox′1, Ox′2, Ox′3), which are again orthonormal and have the same origin as Ox1, Ox2 and Ox3 (Figure 5.1). We must first define how the two sets of axes are related to one another. We do this by setting down a table of the cosines of the angles between each new axis and the three of the old set. The table will appear as: x1 New

x1′ a11 x2′ a21 x3′ a31

Old x2 x3 a12 a22 a32

a13 a23 a33

(5.3)

Here, a32, for example, is the cosine of the angle between the new axis 3 and the old axis 2; that is, the angle x′3Ox2 in Figure 5.1. Similarly, a11 is the cosine of the angle between Ox′1 and Ox1, and so on. In an array of the type of Equation 5.3 it should be noted that the sum of the squares of any row or column of the array is equal to one, because both sets of axes are orthonormal. Therefore, for example, a112+ a212+ a312 = 1 and a212+ a222+ a232 = 1, and so on. It is evident that the elements aij constitute the elements of a rotation matrix (Section A1.4). If we call this matrix A, the inverse of this matrix, A−1, is equal to its transpose, Ã (Section A1.4).

Kelly_c05.indd 142

11/30/2011 7:18:30 PM

Tensors

143

x3 x2′ x3′

cos–1 a21

P

cos–1 a23

k¢ k O

i

cos–1 a22

j¢ j

x2

i¢

x1 x1′

Figure 5.1

Now let p have components p1, p2, p3 along the old axes so that: p = p1i + p2 j + p3 k

(5.4)

where i, j, k are unit vectors along Ox1, Ox2, Ox3, respectively. The component of p along the new axis Ox′1 can be found by resolving the three old components, p1i, p2 j and p3k, along the new axis Ox′1 and adding up the projections, thus obtaining: p1′ = a11 p1 + a12 p2 + a13 p3

(5.5a)

Similarly, we find the new components of p along Ox′2 and Ox′3, p′2 and p′3 respectively, to be: p2′ = a21 p1 + a22 p2 + a23 p3

(5.5b)

p3′ = a31 p1 + a32 p2 + a33 p3

(5.5c)

and

The vector p has the same magnitude and direction referred to any set of axes. If i′, j′, k′ are unit vectors along Ox′1, Ox′2, Ox′3 then: p1i + p2 j + p3 k = p1′ i′ + p2′ j′ + p3′ k ′

(5.6)

From Equation 5.3 we can also write:

Kelly_c05.indd 143

11/30/2011 7:18:31 PM

144

Crystallography and Crystal Defects

i′ = a11i + a12 j + a13 k j′ = a21i + a22 j + a23 k k ′ = a31i + a32 j + a32 k

(5.7)

and, conversely, since the elements aij constitute the elements of a rotation matrix: i = a11i′ + a21 j′ + a31k ′ j = a12 i′ + a22 j′ + a32 k ′ k = a13 i′ + a23 j′ + a33 k ′

(5.8)

Equations 5.5a–c could also be deduced by using Equation 5.8 to express i, j and k each in terms of i′, j′ and k′ and then substituting in Equation 5.4, noting that p′1 is the coefficient of the unit vector i′, and so on. It is a useful exercise to write out the substitution in full. Proceeding in the same way, we can also obtain expressions for the old components of the vector p, [p1, p2, p3], in terms of the new components by substituting for i′, j′, k′ in terms of i, j, k (using Equations 5.7) on the right-hand side of Equation 5.6 and subsequently comparing terms on the two sides of the equation. Doing this, we find: p1 = a11 p1′ + a21 p2′ + a31 p3′ p2 = a12 p1′ + a22 p2′ + a32 p3′ p3 = a13 p1′ + a23 p2′ + a33 p3′

(5.9)

Relations (5.9) are the converse of Equations 5.5a–c. We are now in a position to relate these results on the transformation of the components of a vector to a relation such as Equation 5.2. A tensor of the second rank is a quantity that multiplies one vector to give another, generally nonparallel, vector of a different magnitude. If we return to our example of electrical conductivity in Section 5.1, we note that we could state Equations 5.1 in the following way:

J1i = (σ 11 E1 + σ 12 E2 + σ 13 E3 ) i J 2 j = (σ 21 E1 + σ 22 E2 + σ 23 E3 ) j J 3 k = (σ 31 E1 + σ 32 E2 + σ 33 E3 ) k

(5.10)

Having done this, let us add up these three equations and express the right-hand side in a new form so that the equation reads: J1i + J 2 j + J 3 k = [σ 11ii + σ 12 ij + σ 13 ik + σ 21 ji + σ 22 jj + σ 23 jk + σ 31ki + σ 32 kj + σ 33 kk ] .( E1i + E2 j + E3 k )

(5.11)

The quantity in square brackets is to be regarded as an operator, which operates on vector E in order to obtain the vector J from E. The form in which the operator is written here is the one that is appropriate to the orthogonal axes defined by the unit vectors i, j and k.2 We let the operator inside the square brackets ‘multiply’ the vector 2

Kelly_c05.indd 144

Note that inside the square brackets we do not have i . i (which equals one), but ii.

11/30/2011 7:18:37 PM

Tensors

145

E (= E1i + E2 j + E3k), as if we were forming the scalar (or dot) product of vector multiplication (Appendix 1). To understand Equation 5.11, it is best to write out the right-hand side term by term. The first term is s11ii · E1i = s11E1ii · i = s11E1i, since i · i = 1. The next term is s11ii · E2j = 0, since i · j = 0 because the i and j axes are orthogonal. Similarly, s11ii · E3k = 0 and s12ij · E1i = 0, but the fifth term is s12ij · E2j = s12E2i, since j · j = 1. If all terms are written out and similar ones collected, we finally obtain just Equations 5.10, which can also be represented as in Equations 5.1. Equation 5.11 is the expanded form of Equation 5.2, or, put another way, the most succinct expression of Equation 5.11 is Equation 5.2. Equation 5.11 contains the components of the conductivity tensor s11, s12, s13, …, s33 referred to the axes (Ox1, Ox2, Ox3), defined by the unit vectors i, j and k. We have seen how to transform the components of a vector, so we can also transform the components of this second-rank tensor. If we take new axes represented by the unit vectors i′, j′, k′, the components of the conductivity tensor s will be different and we can find what they are by substituting for i, j, k in Equation 5.11 the values of i′, j′, k′ referred to the new axes, using Equations 5.7. We would also have to substitute for E1, E2, E3 the components of E along the new axes – E′1, E′2, E′3 – so that the new components of the tensor s11′ , s12′ , s13′ ,…, s 33 ′ , multiplied by the new components of E in a form such as Equation 5.9, yield the components of the vector J, also referred to the new set of axes. This is very lengthy to write out and so we shall first introduce a convenient short notation.

5.3

Dummy Suffix Notation

The tensor T relates the vector p with components p1, p2 and p3 to the vector q with components q1, q2 and q3 so that: p1 = T11q1 + T12 q2 + T13q3 p2 = T21q1 + T22 q2 + T23q3 p3 = T31q1 + T32 q2 + T33q3

(5.12)

These three equations can be written as: j =3

p1 = ∑ T1 j q j , j =1

j =3

p2 = ∑ T2 j q j , j =1

j =3

p3 = ∑ T3 j q j

(5.13)

j =1

or, even more succinctly, as: j =3

pi = ∑ Ti j q j j =1

( i = 1, 2 , 3)

(5.14)

We now leave out the summation sign and introduce the Einstein summation convention [2]: if a suffix occurs twice in the same term, summation with respect to that suffix is

Kelly_c05.indd 145

11/30/2011 7:18:43 PM

146

Crystallography and Crystal Defects

automatically implied. In what follows, the summation will always run over the values 1, 2 and 3 for both i and j. Equations 5.12 can then be written as: pi = Tij q j

(5.15)

Here j is called a dummy suffix, because it does not matter which letter except i is taken to represent it. Equation 5.11 could equally well read: pi = Tik qk using k as the dummy suffix. If we apply this notation to Equations 5.5a–c, all three are contained in the single expression: pi′ = aij p j

(5.16)

Note that the dummy suffix occurs in neighbouring places in Equation 5.16. If we apply the same notation to Equations 5.9 we obtain: pi = (a −1 )ij p′j = (a )ij p′j = a ji p′j

(5.17)

so that when writing the ‘old’ components in terms of the ‘new’, the dummy suffixes are separated because, as we have noted in Section 5.2, the elements aij constitute the elements of a rotation matrix, and so the elements of the inverse of this matrix, [a−1]ij, are simply the transpose of this matrix. When first learning this notation it is best to write out the sums term by term. Thus p′i = aij pj gives, on expansion: p1′ = a1 j p j p2′ = a2 j p j p3′ = a3 j p j

(5.18)

These three sums can then be expanded without fear of making an error.

5.4 Transformation of Components of a Second-Rank Tensor Let two vectors p = [p1 p2 p3] and q = [q1 q2 q3] be related by the tensor Tij for a specific choice of the axes i, j, k. The components of Tij relate the components of q to those of p according to Equation 5.12, or, more succinctly, according to Equation 5.15: pi = Tij q j Now, the components of the two vectors depend upon the choice of axes, because this choice determines the values [p1 p2 p3] and [q1 q2 q3]. The vectors p and q themselves do not change. When the axes are changed, and hence the components of p and q change, the components Tij will also change. If now we choose new axes i′, j′, k′ so that: pi′ = Tij′q′j

Kelly_c05.indd 146

(5.19)

11/30/2011 7:18:47 PM

Tensors

147

we will wish to find the relation between the nine components Tij′ and the nine components Tij. We can find these directly by writing Equation 5.15 in the operational form of Equation 5.11: p1i + p2 j + p3 k = [T11ii + T12 ij + T13 ik + T21 ji + T22 jj + T23 jk + T31ki + T32 kj + T33 kk ] ⋅ (q1i + q2 j + q3 k )

(5.20)

We can now substitute for i, j and k in this equation the values of these quantities in terms of i′, j′ and k′ according to Equations 5.8. The substitution in the left-hand side yields p′1i′ + p′2 j′ + p′3k′, directly from Equation 5.6. Likewise, the term in round brackets on the right-hand side of Equation 5.20 becomes q′1i′ + q′2 j′ + q′3k′. The tensor operator in square brackets is treated in the same way and substitution is made for i, j and k in terms of i′, j′ and k′ from Equations 5.8. There will be 81 terms in total in this square bracket, but these can be grouped together in nine separate new terms. If all those containing (say) the vectors j′k′ are collected, there will be nine of these and the coefficient of j′k′ will be the new component T 23′ . If we write out the expression for T 23 ′ , it is: T23′ = (a21a31T11 + a21a32T12 + a21a33T13 + a22 a31T21 + a22 a32T22 + a22 a33T23 + a23 a31T31 + a23 a32T32 + a23 a33T33 )

(5.21)

Using the summation convention, this can be written succinctly in the form: ′ = a2 k a3l Tkl T23

(5.22)

Similarly, the other eight components of T ij′ may be found by collecting the terms in i′i′, i′j′, i′ k′, j′i′, j′ j′, k′ i′, k′ j′ and k′k′, respectively. Using the summation convention, the full relationship can be written in the form: Tij′ = aik a jl Tkl

(5.23)

For each value of i and j, the sum is to be taken over both k and l. To confirm Equation 5.23 is correct, it is helpful to write out the expansion summing over each of these separately. For example, if i = 2 and j = 3, Equation 5.21 is the expanded version of Equation 5.23. An alternative, and more elegant, method to establish the relationship between Tij′ and Tij is to perform the following mathematical operations with suitable dummy suffices to determine the nine components of T′ij: 1. Write p′ in terms of p: p′i = aik pk (using Equation 5.16). 2. Write p in terms of q: pk = Tkl ql (using Equation 5.15). 3. Write q in terms of q′: ql = ajl q′j (using Equation 5.17). When we combine these three operations we have: pi′ = aik pk = aik Tkl ql = aik Tkl a jl q′j

Kelly_c05.indd 147

(5.24)

11/30/2011 7:18:55 PM

148

Crystallography and Crystal Defects

or: pi′ = aik Tkl a jl q′j

(5.25)

This is of the form of Equation 5.19. Therefore, by comparing Equations 5.19 and 5.26, we have the important result: Tij′ = aik Tkl a jl

(5.26)

which is Equation 5.23, because the order in which a product is written on the right-hand side of this equation does not matter when the dummy suffix notation is used. The relationship between T′ij and Tij is most easy to remember in the form: Tij′ = aik a jl Tkl

(5.27)

The reverse transformation to Equation 5.27 – that is, the transformation giving the components of the tensor Tij in terms of those of the new components T′ij – can be accomplished in exactly the same way. This will lead to: Tij = aki alj Tkl′

(5.28)

It is a useful exercise to prove this.

5.5

Definition of a Tensor of the Second Rank

If the operator T relates two vectors p and q, so that T may be written in the form of the operator given in Equation 5.20, then T is known as a dyadic or tensor of the second rank. Alternatively, we can define a tensor of the second rank as a physical quantity which, with respect to a set of axes xi, has nine components which transform according to Equation 5.27 when the axes of reference are changed.3 A tensor of the second rank, Tij, is said to be symmetric if Tij = Tji, and to be skew symmetric or antisymmetric if Tij = −Tji. Thus the tensor with components: ⎡ 9 −4 ⎢ −4 7 ⎢ ⎣⎢ 1 2

1⎤ 2 ⎥⎥ 6 ⎥⎦

(5.29)

is symmetric. An antisymmetric tensor necessarily has all the diagonal terms Tij equal to zero, such as the tensor:

Generalizing this definition, a scalar is a tensor of zero rank, because it transforms according to the law r′ = r when the axes are changed. A vector is a tensor of the first rank, because when the axes are changed, its components transform according to the rule pi′ = aij pj (Equation 5.16). Sometimes, the word ‘order’ is used instead of rank to describe the number of suffixes appropriate to a tensor quantity. 3

Kelly_c05.indd 148

11/30/2011 7:19:01 PM

Tensors

β⎤ ⎡ 0 −γ ⎢ γ 0 −α ⎥⎥ ⎢ ⎢⎣ − β α 0 ⎥⎦

149

(5.30)

Whether or not a tensor is symmetric or antisymmetric is independent of the choice of axes. The condition for two tensors to be equal is that each component of one be equal to the corresponding component of the other. Any second-rank tensor may be expressed as the sum of a symmetric tensor and of an antisymmetric tensor. This is because any component Tij can always be written as: Tij = 12 (Tij + T ji ) + 12 (Tij − T ji )

(5.31)

The first term then gives the component of a symmetric second-rank tensor and the second term that of an antisymmetric second-rank tensor. Any symmetric tensor Sij can be transformed by a suitable choice of axes so that it takes on the simple form: 0 0⎤ ⎡ S11 ⎢ 0 S 0 ⎥⎥ 22 ⎢ ⎢⎣ 0 0 S33 ⎥⎦

(5.32)

That is, all Sij = 0 unless i = j. Such a tensor when expressed in this form is said to be referred to its principal axes. When referred to its principal axes, the components S11, S22, S33 are called the principal components and are often written simply as S1, S2, S3, respectively. This second-rank tensor can be written in the form: S1ii + S2 jj + S3 kk

(5.33)

We shall not prove any of the above statements. Proofs can be found in the books listed at the end of this chapter.

5.6 Tensor of the Second Rank Referred to Principal Axes When referred to its principal axes, the symmetric tensor Sij relating vectors p and q only has its diagonal components S11, S22 and S33 as possible non-zero components. Under these circumstances, the equations: pi = Sij q j

(5.34)

p1 = S11q1 , p2 = S22 q2 , p3 = S33q3

(5.35)

reduce to:

Now let us return to the simple example of electrical conductivity. The conductivity tensor sij is symmetric. When referred to its principal axes, all the sij are zero except s11, s22 and s33.

Kelly_c05.indd 149

11/30/2011 7:19:07 PM

150

Crystallography and Crystal Defects x2

J J2 E2

O

E

x1

E1 J1

Figure 5.2

If the crystal under consideration is orthorhombic, monoclinic or triclinic, there is no symmetry requirement that two or more of s11, s22 and s33 have to be equal. For our purposes here we shall assume that none of s11, s22 and s33 are equal. Suppose we apply an electrical field E in the x1–x2 plane with components [E1, E2, 0] along these principal axes. Then: J1 = σ 11 E1 + σ 12 E2 + σ 13 E3 = σ 11 E1

(5.36)

because s12 and s13 are both zero. Similarly, J2 = s22E2. However, J3 = 0 because E3 = 0. We can represent this relationship between J and E on a diagram such as Figure 5.2. This diagram can be constructed by drawing E, finding E1 and E2, and multiplying E1 by s11 to get J1 and E2 by s22 to get J2. We then construct J from its components along the axes; that is, J1 and J2. It should be noted carefully that, in general, J and E are not parallel. If E were directed along Ox1, we would have J1 = s11E1 because then both J2 and J3 would be zero. Likewise, if E were directed along Ox2, J would be parallel to E; J will only be parallel to E if E is directed along a principal axis. When we speak of the conductivity in a particular direction, what we actually mean in practice is that if E is applied in that direction and the current density is measured in the same direction, to give a value Jǁ, the conductivity in this direction is Jǁ divided by the magnitude of E; that is, Jǁ/uEu. We can find an expression for this by resolving J parallel to E. Suppose E is applied in a direction so that its direction cosines with respect to the principal axes of the conductivity tensor are cosa, cosb and cosg. Then we have:

Kelly_c05.indd 150

11/30/2011 7:19:14 PM

Tensors

151

x2 J||

E cos b

22

a os 2

Ec

11

s

s

s22 E cos b

Ec os 2

b

E

O

E cos a

x1

s11 E cos a

Figure 5.3 Derivation of the magnitude of the conductivity in a particular direction. The figure is drawn for s11 = 250 and s22 = 75 (ohm−1 m)−1, so that s22 = 0.3s11

J1 = σ 11 E1 = σ 11 E cosα J 2 = σ 22 E2 = σ 22 E cosβ J 3 = σ 33 E3 = σ 33 E cosγ

(5.37)

where E is the magnitude of E (i.e. uEu). Then, a unit vector nˆ parallel to E is simply the vector [cosa, cosb, cosg ], since cos2a + cos2b + cos2g = 1. Resolving J parallel to E produces a vector parallel to E of magnitude Jǁ = J.nˆ . Hence: J|| = J1 cos α + J 2 cos β + J 3 cos γ = E (σ 11 cos2 α + σ 22 cos2 β + σ 33 cos2 γ ) (5.38) Therefore the conductivity in the direction parallel to E is: σ = J|| / E = σ 11 cos2 α + σ 22 cos2 β + σ 33 cos2 γ

(5.39)

The steps in deriving Equation 5.39 are illustrated diagrammatically in Figure 5.3 for the simple case where E is normal to the principal axis Ox3 of the conductivity tensor, so that cosg = 0. It is instructive to derive the result given in Equation 5.39 in a different way. Suppose we consider the meaning of the component s 11 ′ of the conductivity tensor irrespective of whether it is referred to principal axes. The component s 11 ′ relates the electric field along axis Ox′1 to the component of the current along the same axis Ox′1. If, therefore, we wish to find the value of the conductivity in a particular direction, having been given the components of the conductivity tensor referred to its principal axes, we can proceed as follows: Choose a new set of axes such that Ox′1 is along the direction of interest. Then the component s 11′ of the conductivity tensor referred to this new set of axes gives us the

Kelly_c05.indd 151

11/30/2011 7:19:16 PM

152

Crystallography and Crystal Defects

conductivity along this particular direction – the Jǁ/E. We are only interested in s11′ , so in writing out the array of the aij for this transformation we only need to know the values of the cosines of the angles between Ox′1 and the principal axes of the conductivity tensor, Ox1, Ox2 and Ox3. Following the scheme of the expressions in Equation 5.3, we therefore only need to know a11, a12 and a13. These quantities are cosa, cosb and cosg, respectively. Using the transformation formula in Equation 5.27, we have: σ ij′ = aik a jl σ kl

(5.40)

σ11 ′ = a1k a1l σ kl

(5.41)

and so when i = 1 and j = 1:

Since sij is defined relative to its principal axes, the only non-zero terms within this conductivity tensor are s11, s22 and s33. Therefore: σ11 ′ = a11a11σ 11 + a12 a12σ 22 + a13 a13σ 33

(5.42)

Substituting for a11, a12, a13, we obtain: 2 2 2 σ 11 ′ = σ 11 cos α + σ 22 cos β + σ 33 cos γ

(5.43)

in agreement with Equation 5.39. It is clear that we could have proceeded in exactly the same way to find the conductivity in a particular direction even if the values of the components of sij, the conductivity tensor, had not been given to us referred to principal axes. In that case there would have been, in general, nine terms in the expansion of Equation 5.40. This transformation formula clearly holds irrespective of whether the sij are referred to principal axes. Therefore, we can state that to find the value of a property of a crystal in a particular direction we proceed as follows: Let the components of the tensor representing this property be given as Tij referred to axes (Ox1, Ox2, Ox3). Choose an axis along the direction of interest and call this Ox 1′. Let this axis have direction cosines referred to (Ox1, Ox2, Ox3) of a11, a12, a13, respectively. Then the value of the property T11′ in the direction we are interested in is given by: T11′ = a1i a1 j Tij

(5.44)

This relation holds for all second-rank tensors, whether or not they are symmetrical. This equation can be written in a convenient shorthand notation by removing the dash and the ‘1’ subscripts in Equation 5.44, so that the property T along the direction of interest is: T = li l j Tij

(5.45)

where the relevant direction cosines are now defined as l1, l2 and l3 to conform to the notation used by Nye [1].

Kelly_c05.indd 152

11/30/2011 7:19:20 PM

Tensors

5.7

153

Limitations Imposed by Crystal Symmetry for Second-Rank Tensors

The discussion in this section applies to tensors used to represent physical properties of crystals, and strictly only to perfect single crystals; that is, ones without defects. Suppose two vector quantities p and q are related by the tensor Tij in a crystal so that this tensor represents a property of the crystal. The crystal then determines the relationship between components of p and those of q and we choose to represent this relationship by means of the tensor Tij. We state the components of Tij with respect to certain axes. If we now take a different set of axes in the crystal, the components of p and of q along these new axes will in general be different and, furthermore, the relationship between the components of p and those of q along the new axes will alter because the tensor T′ij referred to these new axes will in general be different from Tij. However, if we select new axes in the crystal which are related to the old ones by some symmetry operation, the values of the components of p and of q with respect to the new set of axes will be different from the values of those referred to the old ones, but the relationship between the components of p and those of q will be the same, so that: Tij′ = Tij This is because the properties of the crystal are the same along the new axes as along the old ones. In order for this to be true for particular symmetry elements, limitations are imposed upon the components of Tij when representing a property of a crystal. The same general type of argument will also impose restrictions upon the components of tensors of the third and higher orders; examples occur in Sections 6.4 and 6.5. The fact that physical properties of crystals should remain the same when the system of coordinates to which the properties are referred are rotated to a new set of coordinates by a symmetry operation was first appreciated by Franz Neumann, who applied this principle to elastic coefficients of crystals in a course in elasticity at the University of Königsberg in 1873/4 [3,4]. While this is one way [5] of defining what has now come to be known as Neumann’s principle, it is nowadays more usual to state the principle in the form: The symmetry elements of a physical property of a crystal must include the symmetry elements of the point group of the crystal [1(p. 20),6,7].

It is important to appreciate that the principle does not state that the symmetry of the physical property is the same as that of the point group: the symmetry of physical properties is often higher than that of the point group. Physical properties characterized by a second-order tensor are necessarily invariant with respect to the operation of a centre of symmetry. This is implicit in the linear relations: pi = Tij q j because if we substitute −pi for pi and −qj for qj (i.e. we reverse the directions of p and of q), the relation is still satisfied by the same values of Tij. In terms of applying Neumann’s principle, this means that physical properties represented by second-order tensors for all

Kelly_c05.indd 153

11/30/2011 7:19:27 PM

154

Crystallography and Crystal Defects

crystals must include the symmetry of 1¯; this will be true even for crystals belonging to noncentrosymmetric point groups. It will assist in understanding what follows if we look at the centre-of-symmetry statement in another way. Suppose that for one set of axes (Ox1, Ox2, Ox3) the relation between the pi and the qj is given by Tij. If we now reverse the axes of reference, leaving p and q the same as before, this corresponds to choosing a new set of axes such that the array of the aij relating the axes is:

x1 New

Old x2 x3

x1′ −1 0 x2′ 0 −1 x3′ 0 0

0 0

(5.46)

−1

Here, all aij are equal to zero unless i = j. We now apply the transformation formula, Equation 5.27: Tij′ = aik a jl Tkl Therefore: Tij′ = aii a jj Tij = Tij since a11 = a22 = a33 = −1

(5.47)

What we have done here is to leave the measured quantities p and q the same and to imagine the crystal inverted through a centre-of-symmetry operation. We have obtained the same result as if we had reversed the directions of p and q. Now suppose the crystal contains a diad axis of symmetry. If we measure a certain property along a certain direction with respect to this axis, and then rotate the crystal 180° about this axis and remeasure the property, we will get the same value as before by Neumann’s principle. This imposes restrictions on the values of the components of any symmetric second-rank tensor Sij which represents this property. In this context, it is relevant that the tensors of the second rank in which we will be interested will all be symmetric. To see what these restrictions are, take axes (Ox1, Ox2, Ox3) and suppose there is a diad axis along Ox2, such as might arise in a material with monoclinic symmetry. Initially, we assume the tensor Sij is symmetric, so that it has six independent components. Now, if we take new axes related to the old by a rotation of 180° about Ox2, the physical property must remain the same as before. The new axes are related to the old by the array of aij as: Old x1 x2 x3 New

Kelly_c05.indd 154

x1′ −1 0 0 x2′ 0 1 0 x3′ 0 0 −1

(5.48)

11/30/2011 7:19:30 PM

Tensors

155

The components of the tensor with respect to the new axes, S′ij, are given in terms of the old components, Sij, by: Sij′ = aik a jl Skl

(5.49)

and we must have S′ij = Sij for all i and j. If we work out the components S′ij one by one, we find: ′ = a11a11S11 = S11 , S11 ′ = a33 a33 S33 = S33 , S33

′ = a22 a22 S22 = S22 , S22 ′ = a11a33 S13 = S13 S13

(5.50)

but: ′ = a22 a33 S23 = −S23 S23

and

′ = a11a22 S12 = −S12 S12

(5.51)

However, we must also have S′23 = S23 and S′12 = S12. Therefore, S23 = S12 = 0. Hence, a symmetrical second-rank tensor representing a physical property of a crystal with a twofold axis of rotational symmetry must have the components S23 and S12 equal to zero when referred to axes so that Ox2 corresponds to the diad axis. The limitations on the components of a symmetrical second-rank tensor representing a physical property of a crystal are summarized in Table 5.2 for each of the seven crystal systems. The derivation of this table is dealt with in Section 5.8 by a rapid method. However, we could deduce part of it using the procedure we have just outlined for a diad axis and applying this to the defining symmetry elements of each of the crystal classes. The constraints listed in Table 5.2 apply to any of the physical properties of a crystal listed in Table 5.1 (see Footnote 4 in this chapter).

5.8

Representation Quadric

The discussion in Section 5.6 demonstrated that the measured value of a property that can be represented by a second-order tensor will vary with the direction of measurement and that this variation can be found by the procedure of that section, leading to Equation 5.45, which is: T = li l j Tij If we expand this equation, we obtain: T = li (l1Ti1 + l2Ti 2 + l3Ti 3 ) (5.52) = l12T11 + l1l2T12 + l1l3T13 + l2l1T21 + l22T22 + l2l3T23 + l3l1T31 + l3l2T32 + l32T33 Here, l1, l2 and l3 are the direction cosines of the direction we are considering with respect to the same axes to which Tij is referred. We shall now restrict our discussion to symmetrical second-rank tensors, so that Tij = Tji. When second-order tensors are used to represent physical properties, in nearly every case the tensor can be shown to be symmetrical (a proof

Kelly_c05.indd 155

11/30/2011 7:19:34 PM

156

Crystallography and Crystal Defects

Table 5.2 Number of independent components of physical properties represented by second-rank (order) tensors Crystal system

Orientation of principal axes with respect to the crystal axes

Form of tensor

Number of independent components

Cubic

Any; representation quadric is a sphere

⎡ S 0 0⎤ ⎢0 S 0 ⎥ ⎢ ⎥ ⎣0 0 S ⎦

1

Tetragonal Hexagonal Trigonala

x3 parallel to 4, 6, 3 or 3¯

⎡ S1 0 0 ⎤ ⎢ ⎥ ⎢ 0 S1 0 ⎥ ⎢⎣ 0 0 S3 ⎥⎦

2

Orthorhombic

x1, x2, x3 parallel to the diads along the x-, y- and z-axes

⎡ S1 0 0 ⎤ ⎢0 S 0 ⎥ 2 ⎢ ⎥ ⎣⎢ 0 0 S3 ⎦⎥

3

Monoclinic

x2 parallel to the diad along the y-axis

⎡ S11 0 S13 ⎤ ⎢0 S 0 ⎥ 22 ⎢ ⎥ ⎢⎣ S13 0 S33 ⎥⎦

4

Triclinic

Not fixed

⎡ S11 S12 S13 ⎤ ⎢S S S ⎥ ⎢ 12 22 23 ⎥ ⎣⎢ S13 S23 S33 ⎥⎦

6

a

A hexagonal cell is used here for trigonal crystals.

always involves thermodynamic considerations).4 We shall show in Chapter 6 that when second-rank tensors are used to represent stresses and small strains, they too are always symmetric. When the tensor is symmetric, terms such as a1a2T12 and a2a1T21 are clearly equal. If we denote the tensor now by Sij, S being chosen to remind ourselves that it is symmetric, we have, from Equation 5.52: S = l12 S11 + l22 S22 + l32 S33 + 2l1l2 S12 + 2l1l3 S13 + 2l2 l3 S23

(5.53)

If Sij were referred to principal axes as well as being symmetric, Equation 5.52 would reduce to: 4 All of the properties listed in Table 5.1 can be shown to be represented by symmetric second-rank tensors [1]. However, in the case of the transport properties in materials, such as electrical or thermal conductivity and diffusion, appeal to experiment is necessary to complete the proof. In some cases, the tensor is definitely not symmetric; examples are the tracer mixing tensor and the antisymmetric stirring tensor, both of which are used in models of ocean circulation behaviour [8].

Kelly_c05.indd 156

11/30/2011 7:19:40 PM

Tensors

S = S1l12 + S2 l22 + S3l32

157

(5.54)

because S12 = S13 = S23 = 0. In Equation 5.54 we have also chosen to use an abbreviated notation, so that the principal axis coefficients are written S1, S2 and S3, rather than S11, S22 and S33. Equation 5.53 is of the same form as the equation to the general surface of the second degree (called a quadric) written in polar coordinates and referred to its centre as the origin. The general equation of a quadric is: 1 r2

= A cos2 α + B cos2 β + C cos2 γ + 2 D cos α cos β + 2 E cos α cos γ + 2 F cos β cos γ

(5.55)

where r is the radius vector and cosa, cosb and cosg are the direction cosines of r with respect to a set of orthogonal axes. When the general surface of the second degree is referred to its principal axes, it takes the form: 1 r2

= A cos2 α + B cos2 β + C cos2 γ

(5.56)

which is of the same form as Equation 5.54. When the axes, to which a general surface of the second degree is referred, are altered, the coefficients in Equation 5.55 transform in the same way as do the components of a symmetrical second-rank tensor. Because of this, the variation of a given property of a crystal with direction, given by Equations 5.53 and 5.54, can be represented by a figure in three-dimensional space, which gives the variation of the property S with direction. The general surface of the second degree can be an ellipsoid or a hyperboloid of one or two sheets. To explain the procedure for representing the variation of the property S with direction in a crystal, we shall confine ourselves to the case where the values of S1, S2 and S3 in Equation 5.54 and A, B and C in Equation 5.56 are all positive. In this case, the second-degree surface, which we shall call the representation quadric, is an ellipsoid.5 Fixing attention on Equations 5.54 and 5.56, we see that if we construct an ellipsoid of semiprincipal axes 1/ S1 , 1/ S2 , 1/ S3 , as in Figure 5.4, so that a general point on the ellipsoid satisfies the equation: S1 x12 + S2 x22 + S3 x32 = 1

(5.57)

then the length r of any radius vector of the ellipsoid (representation quadric) is equal to the reciprocal of the square root of the magnitude of the property S in that direction. Thus, if we return to the example of electrical conductivity, and we know the values s1, s2 and s3 of the components of the electrical conductivity referred to principal axes, then we can construct the conductivity quadric (which, if the sii are all positive, will be an ellipsoid). If now a field E is applied in any direction, the magnitude of the conductivity in that 5 If two of the coefficients S1, S2, S3 are positive and the other one is negative, the quadric is a hyperboloid of one sheet; if two are negative and the other is positive, it is a hyperboloid of two sheets. If all three values are negative, the quadric is an imaginary ellipsoid [1].

Kelly_c05.indd 157

11/30/2011 7:19:48 PM

158

Crystallography and Crystal Defects x3

1 √S3

1 √s3 r

g b

O a 1 √S1

1 √s2

1 √s11′

1 √S2

1 √s1

x2

x1

Figure 5.4 The representation ellipsoid

direction can be found by drawing a radius vector r in the direction of E, measuring the value of r and taking the reciprocal of the square root of r to find the conductivity in that direction. We are now in a position to deal rapidly with the limitations imposed by crystal symmetry on any physical property of a crystal which can be described by a symmetric second-rank tensor. The number of independent coefficients in the equation of the representation surface (Equation 5.55) equals the number of independent components of the tensor representing the physical property (Equation 5.53). If we look for the symmetry of the representation quadric of a property of a crystal belonging to each of the Laue groups,6 we find that the symmetry of the representation quadric for a symmetrical second-rank tensor is governed only by the symmetry of the crystal system. The results are collected in Table 5.2. A cubic crystal must possess four triad axes. The representation quadric is then a sphere, and so the axes, to which the symmetrical second-rank tensor representing any of the properties shown in Table 5.1 is referred, are then of no consequence. The crystal is isotropic with regard to this property. Hexagonal, trigonal and tetragonal crystals have two independent components for the properties indicated in Table 5.1. This is because the representation quadric must be a surface of revolution about the hexad, triad or tetrad, respectively. A general quadric shows three mutually perpendicular diad axes. In the orthorhombic system these must lie along the crystal diads. There are then just three independent 6 The Laue groups are important here because we showed in Section 5.7 that all properties represented by a second-rank tensor are necessarily invariant upon the operation of a centre of symmetry.

Kelly_c05.indd 158

11/30/2011 7:19:54 PM

Tensors

159

p

q Q O

Figure 5.5 The radius–normal property of a representation ellipsoid

components of the tensor necessary to describe the physical property. In the monoclinic system, one of the diad axes of the quadric must lie parallel to the crystallographic diad. There are four independent components of the symmetrical second-rank tensor describing a property. These can be thought of as three necessary to specify the length of the semi-axes of the quadric and one to fix the angle in the plane, normal to the crystal diad, between a crystal axis and a principal axis of the quadric. In the triclinic system there are six independent components possible for any property that may be represented by a symmetrical second-rank tensor – a symmetrical second-rank tensor has to be invariant upon a centrosymmetric operation and the holosymmetric class in this system, 1¯, possesses just a centre of symmetry.

5.9

Radius–Normal Property of the Representation Quadric

The representation ellipsoid has a further very useful property known as the radius–normal property. It can be stated as follows: if Sij are the components of a symmetrical second-rank tensor relating the vectors p and q so that pi = Sijqj then the direction of p for a given q can be found by drawing a radius vector OQ of the representation quadric parallel to q and finding the normal to the quadric at Q. This is shown in two dimensions in Figure 5.5. A proof of this property can be undertaken straightforwardly using the principles of vector calculus applied to surfaces [9]. From Equation 5.57, the equation of the ellipsoid with respect to the principal axes of Sij takes the form: S1 x12 + S2 x22 + S3 x32 = 1, Suppose a unit vector parallel to q has direction cosines l1, l2 and l3 with respect to the three mutually perpendicular principal axes (Ox1, Ox2, Ox3). The vector p in Figure 5.5 will be parallel to the vector [S1l1, S2l2, S3l3]. We wish to determine the normal to the representation ellipsoid at a point such as Q, so that OQ is in the direction of q and is the vector y = [x1, x2, x3] = [rl1, rl2, rl3], where the reciprocal of the square root of r is the property of the tensor Sij in that direction (Section 5.8).

Kelly_c05.indd 159

11/30/2011 7:19:54 PM

160

Crystallography and Crystal Defects

In general from Equation 5.57 we can solve for x3 so that: x3 =

1 − S1 x12 − S2 x22 S3

(5.58)

and: ⎡ y = ⎢ x1 , x2, ⎢⎣

1 − S1 x12 − S2 x22 ⎤ ⎥ S3 ⎥⎦

(5.59)

We can now determine the gradients ∂y/∂x1 and ∂y/∂x2. Since the surface of the representation ellipsoid is smooth, these two gradients define the tangent plane at the point of interest [9]. A vector normal to this tangent plane will be parallel to the vector: n=

∂y ∂x1

×

∂y ∂x2

(5.60)

It is evident from Equation 5.59 that: ⎡ ⎤ ⎡ S1 x1 Sx ⎤ ⎥ = ⎢1, 0, − 1 1 ⎥ = ⎢1, 0, − ∂x1 ⎢ S3 x3 ⎦ S3 1 − S1 x12 − S2 x22 ⎥⎦ ⎣ ⎣ ⎡ ⎤ ⎡ S2 x 2 S x ⎤ ∂y ⎥ = ⎢1, 0, − 2 2 ⎥ = ⎢0, 1, − 2 2 ∂x2 ⎢ S3 x3 ⎦ S3 1 − S1 x1 − S2 x2 ⎥⎦ ⎣ ⎣ ∂y

(5.61)

so that:

i

j

k ⎡S x S x ⎤ Sx n = 1 0 − 1 1 = ⎢ 1 1 , 2 2 , 1⎥ S3 x3 ⎣ S3 x3 S3 x3 ⎦ S x 0 1 − 2 2 S3 x3

(5.62)

That is, n is parallel to the vector: n = [ S1 x1 , S2 x2 , S3 x3 ] = r [ S1l1 , S2 l2 , S3l3 ]

(5.63)

Hence, n is parallel to the vector p. Finally, we note that we could have solved Equation ∂y ∂y 5.57 for either x1 or x2, rather than x3, and then defined n by either n = or × ∂ ∂ x x3 ∂y ∂y 2 n= × as appropriate; we would still have obtained the same result for n. ∂x3 ∂x1

Kelly_c05.indd 160

11/30/2011 7:19:57 PM

Tensors

161

5.10 Third- and Fourth-Rank Tensors Just as a second-rank tensor relates two vectors, so a third-rank tensor relates a second-rank tensor and a vector, and a fourth-rank tensor relates two second-rank tensors, and so on. Thus, for a tensor of the third rank, Tijk, we can envisage a relationship between a secondrank tensor sjk and a vector pi so that, for example: pi = Tijk s jk

(5.64)

Equally, relationships could be of the general form: sij = Tijk pk

(5.65)

where we require the tensor of the third rank to transform as: T ′ijk = ail a jm aknTlmn

(5.66)

generalizing the result in Section 5.4 for a tensor of the second rank. Likewise, a tensor of the fourth rank, Tijkl, can relate two tensors of the second rank, sij and gkl, through an equation of the form: sij = Tijkl gkl

(5.67)

T ′ijkl = aim a jn akp alqTmnpq

(5.68)

where Tijkl transforms as:

We shall consider third- and fourth-rank tensors in more detail in Chapter 6, once we have introduced the two important field tensors of stress and strain.

Problems 5.1 Define a tensor of the second rank. Write down two physical properties of crystals that can be represented by a second-rank tensor, and for each state the two physical quantities that are related by the tensor. For one of your examples, write down in full the equations relating the components of the two physical quantities and explain your notation. Explain the physical significance of the tensor component D12, where D is the diffusivity tensor. 5.2 Explain why the array of the aij in Equation 5.3 does not represent the components of a second-rank tensor. 5.3 Express the following tensor as the sum of a symmetric tensor and an antisymmetric tensor: ⎛ 12 6 0⎞ ⎜ 4 7 0⎟ ⎜ ⎟ ⎝ 0 0 3⎠

Kelly_c05.indd 161

11/30/2011 7:20:06 PM

162

Crystallography and Crystal Defects

5.4 If s is a symmetric dyadic and n and b are vectors, show that: (σ ⋅ n) ⋅ b = (σ ⋅ b) ⋅ n 5.5 A crystal possesses a single four-fold rotational axis of symmetry parallel to the z-axis. Find the necessary relations between the components of a second-rank tensor representing a physical property of the crystal when the tensor is referred to axes parallel to the crystal axes. How can this result be reconciled with the entry for tetragonal crystals in Table 5.2? 5.6 Prove that whether a tensor is symmetric or antisymmetric is independent of the choice of axes. Hint: show that if Tij = Tji then T′ij = T′ji. 5.7 The electrical conductivity of an orthorhombic crystal, with lattice parameters a = 10.2 Å, b = 7.8 Å and c = 6.3 Å, is found in general to be anisotropic. However, in a (hk0) plane whose normal is 52° to the [010] axis, the electrical conductivity is isotropic. In a separate experiment on the same crystal, it was found that the magnitude of the electrical conductivity in the [001] direction was 4 × 107 Ω−1m−1 and that the electrical conductivity in the [010] direction was three times that in the [100] direction. (a) Determine the electrical conductivity tensor of the crystal with respect to the crystallographic axes of the orthorhombic crystal. (b) Determine the electrical conductivity in the [110] direction. 5.8 (a) The electrical conductivity tensor of a crystal has the components: ⎛ 18.25 − 3 × 2.25 0⎞ ⎜ ⎟ σ ij = ⎜ − 3 × 2.25 22.75 0⎟ × 108 Ω −1m −1 ⎜ 0 0 9⎟⎠ ⎝ Take new axes rotated 60° about x3 in a clockwise direction looking along negative x3 and write down a table of the direction cosines between the new and old axes as in Section 5.2. Check that the sum of the squares of the aij in each row and column equals 1. (b) Write down the components of the conductivity tensor referred to the new axes. Check that sij has not altered. The tensor is now referred to principal axes. (c) Draw a section of the representation quadric (i.e. the conductivity ellipsoid in this case) in the plane x′3 = 0. Draw radius vectors of the resulting ellipse at angles of 30° and 60° to x′1 and hence find the conductivity in these directions. (d) Check your results in (c) by direct calculations. (e) Suppose an electric field E of 100 Vm−1 is established in a direction at 60° to x′1 in the plane x′3 = 0. Write down the components of this electric field along x′1 and x′2 and hence find the electric current densities in these two directions. Finally, find the component of the resultant current density along E and hence the electrical conductivity in this direction. (f) Find the direction of the resultant current vector J in (e). (g) Draw the direction of the resultant current density vector on your diagram prepared in (c) and confirm that J is parallel to the normal to the surface of the representation quadric at the point where a vector from the origin parallel to E meets the representation quadric.

Kelly_c05.indd 162

11/30/2011 7:20:13 PM

Tensors

163

Suggestions for Further Reading D.R. Lovett (1999) Tensor Properties of Crystals, 2nd Edition, Adam Hilger, Bristol and Philadelphia. J.F. Nye (1985) Physical Properties of Crystals, Clarendon Press, Oxford. D.E. Sands (1982) Vectors and Tensors in Crystallography, Addison-Wesley, Reading, Massachusetts and London. W.A. Wooster (1973) Tensors and Group Theory for the Physical Properties of Crystals, Clarendon Press, Oxford.

References [1] J.F. Nye (1985) Physical Properties of Crystals, Clarendon Press, Oxford. [2] A. Einstein (1916) Die Grundlage der allgemeinen Relativitätstheorie, Annalen der Physik, 49, 769–822. [3] F. Neumann (1885) Elasticität krystallinischer Stoffe, Chapter 12 in O.E. Meyer and B.G. Teubner (eds) Vorlesungen über die Theorie der Elasticität der festen Körper und des Lichtäthers, Leipzig, pp. 164–202. [4] S. Katzir (2004) The emergence of the principle of symmetry in physics, Historical Studies in the Physical and Biological Sciences, 35, 35–65. [5] W.A. Wooster (1973) Tensors and Group Theory for the Physical Properties of Crystals, Clarendon Press, Oxford, p. 15. [6] P. Gay (1972) The Crystalline State, Oliver and Boyd, Edinburgh, p. 259. [7] D.R. Lovett (1999) Tensor Properties of Crystals, 2nd Edition, Adam Hilger, Bristol and Philadelphia, p. 31. [8] S.M. Griffies (1998) The Gent–McWilliams skew flux, J. Phys. Oceanogr., 28, 831–841. [9] K.F. Riley, M.P. Hobson and S.J. Bence (2006) Mathematical Methods for Physics and Engineering, 3rd Edition, Cambridge University Press, Cambridge, pp. 345–347.

Kelly_c05.indd 163

11/30/2011 7:20:16 PM

6 Strain, Stress, Piezoelectricity and Elasticity 6.1

Strain: Introduction

When forces are applied to crystals or when imperfections are formed inside them the atoms change their relative positions. This change in the relative positions is called strain, and in this section we describe a way of specifying it. The basic ideas of strain are those of extension and shear. The first is easily understood. Consider a very thin rod of length l (Figure 6.1a). Let the rod be stretched so that l′ is its length in the strained state. Then the extension, e, is defined as: e=

l′ − l l

(6.1)

That is: l ′ = l (1 + e) Thus e is the ratio of the change in length to the original length. It is positive in tension and negative in compression. Shear is a measure of the change in angle between two lines in a body when the body is distorted. It is defined as follows (Figure 6.1b). If OP, OR are two perpendicular straight lines in the unstrained state and O′P′, O′R′ are the positions of the corresponding lines in the strained state then the (engineering) shear strain g associated with these two directions at the point O is defined as: γ = tan

⎛ π − θ⎞ ⎝2 ⎠

(6.2)

Crystallography and Crystal Defects, Second Edition. Anthony Kelly and Kevin M. Knowles. © 2012 John Wiley & Sons, Ltd. Published 2012 by John Wiley & Sons, Ltd.

Kelly_c06.indd 165

11/30/2011 7:08:07 PM

166

Crystallography and Crystal Defects (a)

(b) P

l

P′

tan–1γ

l′ θ

R′

O′

l′ l

O

Figure 6.1

R

(a) Definition of extension. (b) Definition of shear

where q is the angle between O′P′ and O′R′ in the strained state. The description of general distortions, involving both extensions and shears, can be very complicated. We shall consider two important special cases: 1. Infinitesimal strain, where it is assumed that the quantities e and g are so small that their squares and products can be neglected. For elastic strains within a crystal, this assumption is a good one, except at points which are only a very few atomic distances from a defect. 2. Homogeneous strain, where every part of the strained region suffers the same distortion. Large homogeneous strains will be encountered in Chapters 7, 11 and 12. In this chapter we will restrict our attention to infinitesimal strains, because these are relevant for a description of how elastic strains affect perfect crystals when considering piezoelectricity and elasticity. Homogeneous strains are considered in Appendix 6. The discussion of homogeneous strains in the context of slip, twinning and martensitic transformations will be deferred to the relevant chapters later in the book.

6.2

Infinitesimal Strain

The distortion of a body can be described by giving the displacement of each point from its location in the undistorted state. Any displacements which do not correspond to a translation or rotation of the body as a whole will produce a strain. We now confine ourselves to two dimensions and choose an origin fixed in space such as O in Figure 6.2. Let P be a point with coordinates (x1, x2) in the unstrained state, which after distortion of the body moves to the point P′. (Then the displacement of the point P is the vector PP′.) Let the coordinates of P′ be (x1 + u1, x2 + u2). Now consider a point Q with coordinates (x1 + dx1, x2 + dx2) lying infinitesimally close to P in the unstrained state. After deformation, Q moves to Q′. Now, in a strained body, the displacement of Q will not be exactly the same as that of P. The displacement of Q to Q′ has components (u1 + du1, u2 + du2). We can write: du1 =

Kelly_c06.indd 166

∂u1 ∂x1

dx1 +

∂u1 ∂x2

dx2

(6.3)

11/30/2011 7:08:08 PM

Strain, Stress, Piezoelectricity and Elasticity

167

Q′

x2 P′

Q P

x1

O

Figure 6.2

and: ∂u2

du2 =

dx1 +

∂x1

∂u2 ∂x2

dx2

(6.4)

Defining the four quantities at the point P: e11 =

∂u1 ∂x1

,

e12 =

∂u1 ∂x2

e22 =

,

∂u2 ∂x2

,

e21 =

∂u2 ∂x2

,

(6.5)

Equations 6.3 and 6.4 can be compactly written as: dui = eij dx j

( j = 1,2)

(6.6)

Since dui and dxj are vectors, according to the definition given in Chapter 5, eij is a tensor, which we can term the relative displacement tensor. We shall now demonstrate the physical meaning of the various eij when each is very small compared to unity. Let us take two special positions of the vector PQ: first parallel to Ox1 (PQ1) and then parallel to Ox2 (PQ2), and find out how a rectangular element at P is distorted (Figure 6.3). For PQ1 we put dx2 = 0 and obtain: du1 = du2 =

∂u1 ∂x1 ∂u2 ∂x1

dx1 = e11 dx1

(6.7)

dx1 = e21 dx1

(6.8)

From Figure 6.3 it is clear that e11 measures the extension per unit length of PQ1 resolved along Ox1, while e21 measures the anticlockwise rotation of PQ1, provided that e11 and e21 are small. Similarly, e22 measures the change in length per unit length of PQ2, resolved along Ox2, and e12 measures the small clockwise rotation of PQ2. This relative displacement tensor eij is not completely satisfactory as a measure of strain, because it is possible to have non-zero components of eij without there being any distortion of the body. Thus, consider a rigid-body rotation through a small angle w, illustrated in

Kelly_c06.indd 167

11/30/2011 7:08:08 PM

168

Crystallography and Crystal Defects x2

Q′2

Q′1

Q2 P′

dx1

P

du2 dx1 + du1

Q1 x1

O

Figure 6.3

x2

Q'2

Q2 w Q'1 P

w Q1

O

x1

Figure 6.4

Figure 6.4. Evidently we have e11 = e22 = 0, but e12 = −w and e21 = w (since for small angles, tan w = w − O(w3) ≅ w, neglecting the higher-order terms because we are considering infinitesimal relative displacements). To remove the component of rotation from a general eij we express it as the sum of a symmetrical tensor, eij, and an antisymmetrical tensor, wij, so that: eij = ε ij + ω ij = 1 (eij + e ji ) + 1 (eij − e ji ) 2

ε ij =

1 2

2

(eij + e ji ) is then defined as the pure strain and ω ij =

1 2

(6.9)

(eij − e ji ) measures the rota-

tion (as in Figure 6.4). The geometrical interpretation of Equation 6.9 is shown in Figure 6.5. It should be noted that the change in angle between the two lines originally at right angles in Figure 6.5 is 2e12. Therefore, the shear component of the pure strain tensor e12 is half the engineering shear strain g defined in Equation 6.2. In specifying infinitesimal strain in three dimensions, the method is the same as for two dimensions. The variation of displacement u (= u1, u2, u3) with variation in position x (= x1, x2, x3) is used to define nine components of a relative displacement tensor eij:

Kelly_c06.indd 168

11/30/2011 7:08:08 PM

Strain, Stress, Piezoelectricity and Elasticity 1 2

e12

1 2

(e12+e21)

=

169

(e12–e21)

+

e21 e12

e12

=

+

w12

Figure 6.5

eij =

∂ui

(i, j = 1, 2, 3)

∂x j

(6.10)

The strain tensor eij is then defined as the symmetrical part of eij: ε ij = 1 (eij + e ji )

2

(6.11)

In full: ⎡ ε11 ⎢ ⎢ ε12 ⎢⎣ ε13

ε12 ε 22 ε 23

1 (e + e ) 1 (e + e ) ⎤ ⎡ e11 21 31 2 12 2 13 ⎢ ⎥ ⎥ 1 (e + e ) ⎥ e22 ε 23 ⎥ = ⎢ 1 (e21 + e12 ) 32 ⎥ 2 23 ⎢2 ε 33 ⎥⎦ ⎢ 1 ⎥ 1 (e + e13 ) (e + e23 ) e33 2 32 ⎣⎢ 2 31 ⎦⎥ ε13 ⎤

(6.12)

The diagonal components of eij are the changes in length per unit length of lines parallel to the axes and are called the tensile strains. The off-diagonal components measure shear strains so that, for instance, e13 is one-half the change in angle between two lines originally parallel to the Ox1 and Ox3 axes. Since pure strain is a symmetrical second-rank tensor, it can be referred to principal axes (Chapter 5). Under these circumstances, the shear components vanish and we have: ⎡ ε1 ε = ⎢⎢ 0 ⎢⎣ 0

0 ε2

0

0⎤ 0 ⎥⎥ ε 3 ⎥⎦

(6.13)

The geometrical meanings of the principal strains e1, e2 and e3 are shown in Figure 6.6, which shows that a unit cube whose edges are parallel to the principal axes is changed into a rectangular-sided figure with edges (1 + e1), (1 + e2) and (1 + e3). The change in volume per unit volume is called the dilatation, and is given by: Δ = (1 + ε1 ) (1 + ε 2 ) (1 + ε 3 ) − 1 = ε1 + ε 2 + ε 3

(6.14)

where terms such as e1e2 and e1e2e3 have been neglected, since the strains are infinitesimal. When the strain is referred to any other axes, the dilatation is always given by the invariant

Kelly_c06.indd 169

11/30/2011 7:08:09 PM

170

Crystallography and Crystal Defects (l + e ) 1

x2

l l

(l + e2)

l

(l +

O

e 3)

x1

x3

Figure 6.6

sum of the trace of the strain matrix, (e11 + e22 + e33). (This is a general result for symmetrical tensors of the second rank, the proof of which follows from the properties of similarity transformations and can be found in references [1–4] of Appendix 1.) The components of either eij or eij can be transformed to new axes by means of the standard transformation rule for second-rank tensors (Chapter 5). In a number of books on elasticity, the strain is described by the quantities: ⎡ εx ⎢ ⎢γ xy ⎢ ⎣⎢γ zx

γ xy

γ zx ⎤

εy

γ yz ⎥

γ yz

⎥

⎥ ε z ⎦⎥

(6.15)

We then see that, for instance, gxy ≡ 2e12. The g values are usually called shear strains or engineering shear strains, and it should be noted that they are equal to twice the corresponding tensor shear strains defined in this book. This array of the values of e and g does not form a tensor.

6.3

Stress

When atoms in a crystal are displaced relative to one another, forces act on them, tending to restore their normal spatial relationship. If a plane is passed through a strained region of crystal, it will be found that the atoms on one side of the plane are exerting forces upon the atoms on the other side. At any point on the plane, the force acting per unit area of plane is defined as the traction on the plane at that point. The force is customarily resolved into components normal and parallel to the plane, fn and fs, respectively, and corresponding normal and shear stress components, sn and t, are defined as follows: fn σ n = δ Lt (6.16) A→ 0 δA τ = δ Lt A→ 0

fs δA

(6.17)

The area d A is shown in Figure 6.7; it surrounds the point P, so that by finding the limit of the series of average stresses f/d A as d A decreases, the stress at the point itself can be

Kelly_c06.indd 170

11/30/2011 7:08:09 PM

Strain, Stress, Piezoelectricity and Elasticity ƒn

171

ƒ

ƒs

P dA

Figure 6.7 x3 (z)

(a)

s31 (τzx)

s33 (z)

s13 (τxz)

(x)

(x)

s12 (τxy)

s21 (τyx)

sz

z

szr

szq s32 (τzy) srq

s23 (τyz)

s11 x1

(b)

sq r

sr

sq

srz

s22 (sy)

sq z x2 (y)

q

Figure 6.8 Definition of stress components (a) in Cartesian coordinates and (b) in cylindrical polar coordinates

defined. For this definition to be meaningful, the force at P must not be changing too sharply on an atomic scale. The procedure outlined above could be repeated for any plane passing through the point P. To define the stress at P completely, it is sufficient to specify the stresses acting on three mutually perpendicular planes passing through P. It is then possible to calculate the stress acting on any other plane by means of a force balance. The stresses acting on the faces of an infinitesimal cube located at P are shown in Figure 6.8a, using two alternative notations. In the numerical suffix notation, the stress component sij is the component in the direction of the xj-axis of the traction acting on the face whose normal is parallel to xi.1 The sign convention is that a stress is positive if the force component and the outward-going 1 Nye [1] and Lovett [2] use a notation where sij is the component in the direction of the xi-axis of the traction acting on the face whose normal is parallel to xj. The notation we have chosen is that used elsewhere, such as [3–6], but, irrespective of which notation is used, sij = sji in equilibrium. There is no single ‘correct’ notation.

Kelly_c06.indd 171

11/30/2011 7:08:09 PM

172

Crystallography and Crystal Defects x3 C P s11

B

x2

s21 s22 O s 23

s31 s33 A

Figure 6.9

x1

Calculation of the stress acting on the plane ABC

normal of the face on which it acts have the same sense, relative to the axes to which they are respectively parallel. The letter suffix notation follows the same pattern, except that shear stresses are distinguished by the letter t. It is sometimes convenient to work with cylindrical polar coordinates instead of Cartesian coordinates, and the stress components for this case are shown in Figure 6.8b. As the cube in Figure 6.8a is supposed to be infinitesimally small, the forces acting on opposite faces must be equal and opposite. If the cube were of side d, the shear stresses txy and tyx would produce a couple (txy − tyx) d 3, tending to rotate the cube about the z-axis. Since the moment of inertia of the cube varies as d 5, it vanishes as d → 0 more rapidly than does the couple (txy − tyx) d 3, so that, to avoid an infinite angular acceleration: τ xy = τ yx

and in general in equilibrium: σ ij = σ ji

(6.18)

In order to calculate the stress acting upon any given plane at P, an infinitesimal body is constructed having one face, ABC, parallel to the given plane and all its other faces parallel to the cube faces (Figure 6.9). A balance of the forces acting on the tetrahedron ABCO then determines the required stress. Let P = [P1P2P3] be the traction exerted on the face ABC by the material outside the tetrahedron. Setting the sum of forces in the Ox1 direction equal to zero: P1 ( ABC ) = σ 11 ( BOC ) + σ 21 ( AOC ) + σ 31 ( AOB)

(6.19)

Now, the volume of a tetrahedron is (area of base × perpendicular height)/3. If we specify the perpendicular from O to ABC to be d then evidently: d. (ABC ) = OA.( BOC ) = OB.( AOC ) = OC.( AOB)

Kelly_c06.indd 172

(6.20)

11/30/2011 7:08:10 PM

Strain, Stress, Piezoelectricity and Elasticity

173

and so: d d d ( BOC ) ( AOC ) ( AOB) = = l1 ; = = l2 ; = = l3 ( ABC ) OA ( ABC ) OB ( ABC ) OC

(6.21)

where l1 is the cosine of the angle between the normal to ABC and Ox1, and so on for l2 and l3. Hence: P1 = σ 11l1 + σ 21l2 + σ 31l3

(6.22)

where li are the direction cosines of the normal to the plane ABC. We obtain similar equations for P2 and P3, and all three equations can be written compactly as: Pi = σ ji l j

(6.23)2

Resolving P into two components, one normal and one parallel to ABC, we can obtain the normal stress sn and shear stress t, where sn is given by the sum of the components Pi, each resolved normal to ABC: σ n = Pl i i

Therefore, from Equation 6.23: σ n = σ ji l j li

(6.24)

By resolving the forces: τ = ⎡⎣ P 2 − σ n2 ⎤⎦

1/2

(6.25)

where P is the magnitude of P. It is apparent from Equation 6.23 that the components of the vector P representing the traction on a plane are linearly related to those of the unit vector which is normal to that plane. It follows that the relating coefficients sij form a tensor of the second rank. When the axes of reference are rotated, the components of a given stress transform according to the general transformation law: σ ij = aik a jl σ kl

(6.26)

where aij is the cosine of the angle between the new Oxi-axis and the old Oxj-axis (Chapter 5). Because the stress tensor is symmetrical (sij = sji), it is always possible to find a set of axes, the principal axes, so that a cube with its edges parallel to them has no shear stresses acting upon its faces. Referred to the principal axes, the stress takes the form: ⎛ σ1 0 ⎜0 σ 2 ⎜ ⎝0 0

2

0⎞ 0⎟ ⎟ σ3 ⎠

(6.27)

It is evident that this equation is written Pi = sijlj in the notation used by Nye [1] and Lovett [2].

Kelly_c06.indd 173

11/30/2011 7:08:10 PM

174

Crystallography and Crystal Defects

where s1, s2 and s3 are called the principal stresses. In very special cases, a body may be under a homogeneous stress; that is, the stress may be the same at every point. If the stress is homogeneous, parallel cubes of any size and at any location have the same tractions on their faces. Such a condition obtains in the tensile test of a uniform rod, the stress at every point being: ⎛ F/A 0 0⎞ ⎜ ⎟ 0 0⎟ ⎜ 0 ⎜ 0 0 0 ⎟⎠ ⎝

(6.28)

where F is the tensile force and A is the cross-sectional area of the rod, and the tensile axis is parallel to Ox1. More generally, the stress in a body varies from point to point. However, the different components of stress cannot vary in an entirely arbitrary way, independently of one another. The variations in the different stress components must be related in such a way that there is a balance of the forces acting on any internal body (assuming that the body as a whole is in static equilibrium). One face of a cube of side 2d in a varying stress field is shown in Figure 6.10. By setting the sum of forces in the Ox1 direction equal to zero, we obtain: ∂σ 11 ∂x1

+

∂σ 21 ∂x2

+

∂σ 31 ∂x3

+ f1 = 0

(6.29)

where f1 is the component of body force per unit volume (e.g. due to gravity) acting in the Ox1 direction. Two similar equations are obtained with respect to the Ox2 and Ox3 directions, and all three equations of equilibrium can be written compactly as: ∂σ ij ∂xi

+ fj = 0

(6.30)

The repetition of the suffix i in Equation 6.30 implies the summation of the differential coefficients obtained by setting i = 1, 2 and 3 in turn. We shall now mention some important types of stress. A pure shear stress is of the form s12 = S, with all other sij zero, or: ⎛ 0 S 0⎞ ⎜ ⎟ ⎜S 0 0⎟ ⎜ 0 0 0⎟ ⎝ ⎠

(6.31)

When the axes of reference are rotated through 45° about Ox3, in an anticlockwise sense, the stress components transform to: ⎛S 0 0⎞ ⎜ ⎟ ⎜ 0 −S 0 ⎟ ⎜ 0 0 0⎟ ⎝ ⎠

Kelly_c06.indd 174

(6.32)

11/30/2011 7:08:10 PM

Strain, Stress, Piezoelectricity and Elasticity (s22 +

⭸s22 d) ⭸x2

(s12 +

(s11

⭸s12 d) ⭸x2

(s12 +

⭸s11 d) ⭸x1 P (s12

⭸s12 d) ⭸x1

(s11 +

⭸s12 d) ⭸x1

(s12

175

⭸s11 d) ⭸x1

⭸s12 d) ⭸x2 (s22

⭸s22 d) ⭸ x2

Figure 6.10

S

S

S S

P

P

Figure 6.11 A shear stress at the point P

The principal stresses of a pure shear are therefore equal tensile and compressive stresses acting on planes at 45° to those on which the shear stress acts alone (Figure 6.11). In a general state of stress, shear stress components exist on all planes other than those normal to the principal axes. It can be shown that the largest shear stress occurs on the plane which bisects the angle between the planes on which the greatest and least of the principal stresses act (Figure 6.12). If s1 < s2 < s3, the magnitude of the largest shear stress is 12 (σ 3 − σ 1 ) . A hydrostatic pressure p takes the form: 0 ⎞ ⎛−p 0 ⎜ ⎟ 0 − p 0 ⎟ ⎜ ⎜ 0 0 − p ⎟⎠ ⎝

Kelly_c06.indd 175

(6.33)

11/30/2011 7:08:10 PM

176

Crystallography and Crystal Defects s3 tmax

tmax

s1

Figure 6.12 If σ3 is the largest principal stress and σ1 is the smallest, the largest shear stress acts in the direction shown, on a plane that is normal to the plane of the figure

which remains the same no matter what axes of reference are chosen. In other words, a hydrostatic pressure produces no shear stress anywhere. It is possible to produce any state of stress by superimposing a hydrostatic pressure or tension upon three pure shear stresses. To prove this, we note that a general stress can be written as the sum of a hydrostatic component and a component called the deviatoric stress. Referred to principal axes, the stress can be written as: ⎛ σ1 0 ⎜0 σ 2 ⎜ 0 0 ⎝

0⎞ ⎛ σ ii 1⎜ ⎟ 0 = 0 ⎟ 3⎜ σ3 ⎠ ⎝ 0

0 σ ii

0

⎛σ − 1 σ 0 ⎞ ⎜ 1 3 ii 0⎟ +⎜ 0 ⎟ ⎜ σ ii ⎠ ⎜ 0 ⎝

0

⎞ ⎟ ⎟ 0 ⎟ (6.34) 1 σ 3 − σ ii ⎟⎠ 3 0

σ 2 − 1 σ ii

3

0

where sii = s1 + s2 + s3. The hydrostatic component 13 σ ii is invariant, because the sum (s11 + s22 + s33) remains the same whatever axes of reference are chosen, since, just like strain tensors (Section 6.2), stress tensors are symmetrical second-rank tensors. The deviatoric stress can be expressed as the sum of three pure shear stresses, as follows: ⎛ σ 1 − 1 σ ii 3 ⎜ ⎜ 0 ⎜ ⎜ 0 ⎝ ⎛ σ1 − σ 3 1 + ⎜ 0 3⎜ ⎝ 0

Kelly_c06.indd 176

0 σ 2 − 1 σ ii 3

0

⎞ ⎛ σ1 − σ 2 ⎟ 1⎜ ⎟ 0 = 0 ⎟ 3⎜ 0 ⎝ σ 3 − 1 σ ii ⎟⎠ 3 0

0 σ 2 − σ1 0

0 0 ⎞ 0 0 ⎞ ⎛0 1 0 0 ⎟ + ⎜ 0 σ2 − σ3 0 ⎟ ⎟ 3⎜ ⎟ 0 σ 3 − σ1 ⎠ 0 σ3 − σ2 ⎠ ⎝0

0⎞ 0⎟ ⎟ 0⎠ (6.35)

11/30/2011 7:08:10 PM

Strain, Stress, Piezoelectricity and Elasticity 3

177

1'

2' 2

1

3' 'New' set of axes

'Old' set of axes

Figure 6.13

6.4

Piezoelectricity

When some single crystals are stressed in uniaxial tension, an electric polarization, P, can occur within the crystal, the magnitude of which increases linearly with the magnitude of the stress. This manifests itself through the development of electrical charges on the surfaces of the crystals. P is a vector describing the electric dipole moment per unit volume, or equivalently, the surface charge developed per unit area [1,7]. Conversely, the application of an electric field, E, to these single crystals produces a strain within the crystals, and again there is a linear relationship between the magnitude of the electric field and the magnitude of the strain produced. This phenomenon is known as piezoelectricity and was first discovered by Pierre and Jacques Curie in 1880 [7]. The piezoelectric tensor, dijk, is a tensor of the third rank which relates the stress applied, sjk, to the polarization produced, Pi: Pi = dijk σ jk

(6.36)

Reversing the sign of sjk reverses the sign of Pi. As we will now demonstrate, it is straightforward to show that this means that centrosymmetric crystals cannot exhibit piezoelectricity using Neumann’s principle (Section 5.7). From Equation 5.66, tensors of the third rank transform as: T ′ijk = ail a jm aknTlmn If a crystal has a centre of symmetry at the origin, the direction [uvw] maps exactly on to –] for all u, v and w. We can examine what happens to the d specified the direction [u– –v w ijk relative to an ‘old’ orthonormal set 1, 2 and 3 if we then choose new orthonormal axes 1′, 2′ and 3′ related to 1, 2 and 3 by the centre of symmetry (Figure 6.13). Under these circumstances, aij = − dij, where dij is the Kronecker delta, since the angle between the ith ‘old’ axis and the jth ‘new’ axis is either 90 or 180°. Hence, the elements of the tensor dijk produce transformed moduli so that: dijk ′ = ail a jm akn dlmn = − δ il δ jm δ kn dlmn = − dijk

(6.37)

However, if the crystal has a centre of symmetry, and we have performed this centre-ofsymmetry operation, the transformed modulus d′ijk defined with respect to the ‘new’ axis set must be equal to the modulus dijk defined with respect to the ‘old’ axis set. That is, we require:

Kelly_c06.indd 177

11/30/2011 7:08:11 PM

178

Crystallography and Crystal Defects

′ = dijk dijk

(6.38)

for all i, j and k. For Equations 6.37 and 6.38 to be compatible, it follows that dijk = 0 for all i, j and k, so that we can conclude that materials with a centre of symmetry have zero piezoelectric moduli, and are not therefore piezoelectric. Of the 32 crystal classes, 21 are noncentrosymmetric (Chapter 2); a necessary (but not sufficient) condition for a crystal to exhibit piezoelectricity is that it belongs to a noncentrosymmetric crystal class. In principle, we might expect the tensor dijk to have 27 independent components. However, the fact that for a shear stress, skj = sjk, irrespective of body torques being present [8], means in turn that dikj = dijk and so there are actually at most 18 independent coefficients of dijk. At this stage, it becomes possible to introduce a contracted notation in which two suffixes are replaced by one, both in sjk and in dijk. The notation for the stress sij is contracted as follows: ⎛ σ 11 σ 12 ⎜σ σ 22 ⎜ 12 ⎝ σ 13 σ 23

σ 13 ⎞

⎛ σ1

σ 23 ⎟ → ⎜ σ 6

⎟ σ 33 ⎠

⎜ ⎝σ5

σ6 σ2 σ4

σ5 ⎞

σ4 ⎟

⎟ σ3 ⎠

(6.39)

A similar procedure applies to dijk, but in this case it is necessary to introduce factors of into the contracted form of dijk: dijk → dmn for n = 1, 2 and 3 dijk →

1 dmn for n = 4, 5 and 6 2

1 2

(6.40a) (6.40b)

The new dmn form a 3 × 6 matrix of 3 rows and 6 columns, but are not tensors. It is instructive to see why the factors of 12 arise by examining one component of Equation 6.36. For example, when i = 2: P2 = d211σ 11 + d212σ 12 + d213σ 13 + d221σ 21 + d222σ 22 + d223σ 23 + d231σ 31 + d232σ 32 + d233σ 33 from which it is evident that the two terms d212s12 and d221s21 in the full notation become together d26s6 in the contracted notation only if the factor of 12 is included. Similar considerations apply to the other terms for n = 5 and 6 in this equation. The zero and non-zero dij for a particular crystal class can be represented conveniently using a matrix notation introduced by van Dyke in 1950 [9]. In this notation, and the variation used by Nye [1], non-zero dij are represented by large filled dots, •, zero dij are represented by either small dots or a space, numerically equivalent dij are joined by lines, and rings denote values which are the negative of •. A complete presentation of the piezoelectric moduli in this form for each crystal class is given in Appendix E of Nye [1]. Here, we will restrict our attention to consideration of determining the non-zero dij of a few noncentrosymmetic crystal classes.

Kelly_c06.indd 178

11/30/2011 7:08:11 PM

Strain, Stress, Piezoelectricity and Elasticity

179

3 1'

2

2'

1 3' 'Old' set of axes

Figure 6.14

6.4.1

'New' set of axes

180° rotation about [010]

Class 2

In this crystal class there is a single 180° rotation axis. Let this be about x2 in a crystal. ‘Old’ and ‘new’ axes can be defined as in Figure 6.14. The only non-zero aij are a11 = −1, a22 = 1 and a33 = −1. Hence, for example: d113' = a11a11a33 d113 = − d113 ; d112' = a11a11a22 d112 = d112

(6.41)

However, because of the diad axis, d113 ′ must be equal to d113 and d112 ′ must be equal to d112. Hence, we conclude that d113 = 0 but d112 ≠ 0. Thus, if in the transformation from dijk to d′ijk the sign is +1, the modulus is non-zero, but if the sign is −1, the modulus is zero. Clearly, only those dijk with either a single ‘2’ or three ‘2’s survive. Hence the non-zero moduli are the eight in bold in the array: d111

d112 d122

d113 d123 d133

d 211

d212 d 222

d 213 d223 d 233

d311

d312 d322

d313 d323 d333

(6.42)

which then become the eight dots in the corresponding matrix representation: ⎛ ⋅ ⋅ ⋅ • ⋅ •⎞ ⎜ ⎟ ⎜• • • ⋅ • ⋅ ⎟ ⎜ ⋅ ⋅ ⋅ • ⋅ •⎟ ⎝ ⎠ 6.4.2

(6.43)

Class 222

Here, the occurrence of two mutually perpendicular diads forces the third one to occur (Section 1.6). Of the eight non-zero dij in Class 2, only d14, d25 and d36 are non-zero for Class 222 (Problem 6.9), so that the matrix representation is the following: ⎛⋅ ⋅ ⋅ • ⋅ ⋅ ⎞ ⎜ ⎟ ⎜⋅ ⋅ ⋅ ⋅ • ⋅ ⎟ ⎜⋅ ⋅ ⋅ ⋅ ⋅ •⎟ ⎝ ⎠

Kelly_c06.indd 179

(6.44)

11/30/2011 7:08:11 PM

Crystallography and Crystal Defects

180

3

2'

2

3'

1 'Old' set of axes

Figure 6.15

6.4.3

1'

'New' set of axes

120° rotation about [111]

Class 23

Crystal Class 23 has three mutually perpendicular diads and four triad axes along and belongs to the cubic crystal system. Clearly, from the above consideration of Class 222, we know that there are at most three independent dij in Class 23 before we consider the effect of the triad axes. Suppose we examine the effect of a 120° anticlockwise rotation about [111]. In terms of the ‘old’ axes, this is 1 → 2, 2 → 3 and 3 → 1 (Figure 6.15). The only non-zero aij are a12 = 1, a23 = 1 and a31 = 1. Thus, for example: d123′ = a11a22 a33 d123 + a11a23 a32 d132 + a12 a21a33 d213 + a12 a23 a31d231 + a13 a21a32 d312 + a13 a22 a31d321 reduces to: d123′ = a12 a23 a31d231 = d231

(6.45)

and likewise d231′ = d312 and d312′ = d123. Thus, in the dij terminology, d14 = d25 = d36. That is:

(6.46)

Further rotations of 120° about the three other triad axes leave this result unchanged. This result is also true for class 4¯3m: the effect of a shear stress s12 acting in the (001) plane of – a crystal such as sphalerite is to produce a polarization, P3, in the [001] direction by displacing tetrahedrally coordinated zinc ions relative to the centre of mass of the four surrounding sulphur ions (Problem 6.12). (By convention, the direction of polarization of a vector from the centre of the negative charge to the centre of the positive charge determines the sense of a dipole.) 6.4.4

Class 432

Here we have 90° symmetry operations to superimpose upon the ‘basic’ symmetry elements of Class 23. Consider the effect of a 90° anticlockwise symmetry operation about x3 on the surviving moduli of Class 23; that is, d123 = d213 = d312. The non-zero aij are a12 = 1,

Kelly_c06.indd 180

11/30/2011 7:08:11 PM

Strain, Stress, Piezoelectricity and Elasticity

181

a21 = −1 and a33 = 1. Hence, d213′ = a21a12a33d123 = −d123, d123′ = a12a21a33d213 = − d213 and d321′ = a33a21a12d312 = −d312. However, since we must also have d123 = d213 = d312, it follows that d123 = d213 = d312 = 0, and so for Class 432 all the piezoelectric moduli vanish. Thus, even though 432 is not centrosymmetric, crystals belonging to Class 432 are not piezoelectric. This is the only noncentrosymmetic class for which all the piezoelectric moduli vanish; the remaining 20 crystal classes have at least one nonvanishing piezoelectric modulus [1]. 6.4.5 The Converse Effect In the converse piezeoelectric effect, the relevant tensor equation is: ejk = dijkEi

(6.47)

where the dijk are the same as in Equation 6.36 [1]. When Equation 6.47 is expressed in the contracted form: ej = dijEi

(6.48)

the ejk transform as: ⎛ ε11 ⎜ ε12 ⎜⎝ ε 13

ε12 ε 22 ε 23

⎛ ε1 ε13 ⎞ ⎜ ε 23 ⎟ → ⎜ 1 ε 6 2 ⎜1 ε 33 ⎟⎠ ⎜⎝ ε 5 2

1ε 2 6 ε2

1ε 2 4

1ε ⎞ 2 5 1 ε ⎟⎟ 2 4 ⎟ ε 3 ⎟⎠

(6.49)

(Problem 6.13). Note that the contracted shear strains e4, e5 and e6 are engineering shear strains (g ), as defined in Section 6.2, and not tensor shear strains.

6.5

Elasticity of Crystals

In a strained crystal, the stress at any point is linearly related to the strain at that point, provided that the strain is very small. This relationship is known as Hooke’s law. The physical basis for Hooke’s law is merely that at small strains the relative displacements of the atoms are small, so that the interatomic force–separation relationship operates over such a small range as to be sensibly linear. In most solids, strains do in fact remain small (e.g. 2 / 3 that on the {110} planes, slip only on the [111] – (101) slip system would occur for all initial crystal orientations within this stereographic triangle [36,37]. From Table 7.1, it is worth noting that, in crystals of the NaCl structure slipping on – {110} k110l, at least two slip systems are always equally stressed. C.c.p. metal crystals have been very intensively studied. Even for crystals with the position of F near to the centre of the unit triangle, small amounts of glide on systems other than the most highly stressed one are observed. Since the slip plane of a glide system is easily observed, these slip systems are usually identified by reference to the glide plane alone. The slip plane of the most highly stressed system is called the primary glide plane; the names given to this and the others are shown in Figure 7.16.

Kelly_c07.indd 220

11/30/2011 8:24:53 AM

Glide and Texture

221

[0001]

I

I

[1100]

[1010]

[2110]

Figure 7.14 A unit triangle of the standard stereogram of a hexagonal crystal of point group – 6/mmm which glides on (0001) in k1120l, showing the slip direction of maximum resolved shear stress

111

[111] (211) [111] (101) [111] (112) 001

011

– Figure 7.15 The 001–011–111 stereographic triangle for a b.c.c. metal crystal which glides – – on {11 0} in k111l and on {112 } in k111l, showing the regions within this triangle where the resolved shear stresses on the various slip systems are greatest for a situation where the – – critically resolved shear stress is the same on the {11 0} and {112 } planes. The dashed line is – – the boundary between the two possible k111l {112} systems if slip did not occur on {110}

– In cubic crystals slipping on {111} k11 0l, a simple rule has been given by Diehl [40] to identify the primary glide system when the direction of F lies in any of the unit triangles shown in Figure 7.13. This states: ‘Reflect the k110l pole of the triangle in question in the opposite side of the triangle to find the glide direction, and reflect the {111} pole of the triangle in the opposite side to find the glide plane normal.’ An equivalent rule to this is the OILS rule devised by Hutchings [41] as a nongraphical method for deducing the slip

Kelly_c07.indd 221

11/30/2011 8:24:56 AM

222

Crystallography and Crystal Defects [101] (111) Critical

(111) Conjugate

F (001)

[011]

(111) Primary

(111) Cross

Figure 7.16

system with the highest Schmid factor. A mathematical proof of the validity of these two rules is given in Appendix 5.

7.5 Large Strains: The Change in the Orientation of the Lattice During Glide Returning to Figure 7.12, if a small amount of glide, dg, occurs on the slip system shown, the crystal will increase in length by dl in the direction of F where: dl = l cos φ 0 cos λ 0 dγ

(7.30)

where dg is the increment of crystallographic glide strain and l the instantaneous length of the crystal.2 If e is the (small) elongation parallel to F produced by dg then e = dl/l, and so Equation 7.30 gives: e = cos φ 0 cos λ 0 dγ

(7.31)

The relative translation of the parts of the crystal parallel to b implies that as the crystal gets longer its two ends move with respect to one another in a direction transverse to the applied force F. This effect is not important for very small strains, but when minerals are deformed large amounts in compression (usually under hydrostatic pressure), or metal crystals extended by large amounts in tension, it must be taken into account. In compression, the ends of the crystal may be prevented from moving sideways by friction, and in tension, crystals are usually gripped at the ends. Consider the tensile case, and suppose that there is no lateral constraint. The crystal will take up the form shown in Figure 7.17. If, however, due to the lateral constraints the point A′ is forced to lie above O at O′, then if there is glide solely on the system shown, the 2

The identity of the geometrical factors in Equations 7.28 and 7.30 is worth noting in passing. This arises because, of course, if a given applied force produces no resolved shear stress on a given glide system, because cos f0 or cos l0 is zero, then it does no work if that glide system operates. Certain orientations of an applied force F will give zero values for t in Equation 7.28 or for dl in Equation 7.30 if the crystal does not possess five independent slip systems.

Kelly_c07.indd 222

11/30/2011 8:24:56 AM

Glide and Texture

223

f

n

l

O′

b A′ l0

A l

n N

f0

l0

b O

Figure 7.17

crystal lattice will be rotated with respect to the direction OO′. From Figure 7.17 the elongation of the crystal e equals (l − l0)/l0, so from the triangle OAA′: sin λ 0 l =1+ e = l0 sin λ

(7.32)

l cos φ 0 = l0 cos φ

(7.33)

and from triangles NAO, NA′O:

where l0 and f0 are the initial values of l and f. The crystallographic glide strain g is given by AA′/(l0 cosf0 ) and AA′ = l cos l − l0 cos l0, so: γ =

Kelly_c07.indd 223

l cos λ − l0 cos λ 0 cos λ cos λ 0 = − l0 cos φ 0 cos φ cos φ 0

(7.34)

11/30/2011 8:24:59 AM

224

Crystallography and Crystal Defects

At a particular instance during glide, the resolved shear stress t [=(F/A) cos f cos l], where A is the cross-sectional area of the ellipse whose centre is A′, is: sin 2 λ 0 ⎞ F cos φ ⎛ 1− τ= ⎜ ⎟ A ⎝ (1 + e)2 ⎠

1/ 2

(7.35)

It can be seen from Figure 7.17 that the area of the glide plane remains constant during deformation (except for negligibly small changes due to the formation of slip steps). Therefore, the quantity A/cos f does not alter, and so Equation 7.35 can be written as: F cos φ 0 τ= A0

1/ 2

⎡ ⎛l ⎞2 ⎤ ⎢1 − ⎜ 0 ⎟ sin 2 λ 0 ⎥ ⎢⎣ ⎝ l ⎠ ⎥⎦

(7.36)

where A0 is the original cross-sectional area of the specimen prior to tensile testing. As deformation proceeds, the value of l decreases, and so for a given force F the resolved shear stress increases. We can also derive Equations 7.32–7.34 directly from Equation 7.7 and Figure 7.8. It is useful to do this because the vector formulae make the compression case easy to deal with. From Figure 7.8, a vector r is changed by glide of amount g to the vector r′, where: r ′ = r + γ (r ⋅ n ) β

(see Equation 7.7). We take r parallel to the tensile axis when g = 0, and then r′ represents the tensile axis after a crystallographic glide strain g : r′ l = (1 + e) = l0 r

(7.37)

The quantity n is a unit vector normal to the glide plane, so: cos φ =

l cos φ 0 (r ′ ⋅ n ) 1 = [(r ⋅ n) + γ (r ⋅ n)(β ⋅ n)] = 0 r′ r′ l

(7.38)

since cos f0 = (r ◊ n)/ uru and b ◊ n = 0. Thus we have Equation 7.33. Also: r ′ × β = r ′ sin λ

(7.39)

since b is a unit vector. From Equation 7.7: r′ × β = r × β,

since β × β = 0

(7.40)

and so: l sin λ 0 = l0 sin λ

Kelly_c07.indd 224

(7.41)

11/30/2011 8:25:03 AM

Glide and Texture (b)

225

[101] [111]

(a)

[101] 111

[112] 9

7

8 7 6 5

6 5 4 3 2 1 0

10

11 12

4 3 2 1

011 001

Al–Cu

[001]

Cu–Zn

[011]

Figure 7.18 Changes in orientation of c.c.p. metal crystals during glide. The numbers indicate successive determinations of the crystal orientation. ((a) is based on a diagram in Figure 6 of [42]; (b) is based on Figure 16 of [43], redrawn as Figure 69 of [44].)

which is Equation 7.32. Finally, if we form the dot product of both sides of Equation 7.7 with b, we obtain: l cos λ = l0 cos λ 0 + γ l0 cos φ 0

(7.42)

Thus, using Equation 7.33 we have: γ =

cos λ cos λ 0 − cos φ cos φ 0

which is Equation 7.34. When a long, thin crystal is used in an experiment, such as that illustrated in Figure 7.12, the change in orientation of the tensile axis with respect to the crystal axes (which is easier to consider than what is the same thing, the change of the crystal axes with respect to the tensile direction) can be measured and plotted on a stereogram. Since the change of orientation is such that the tensile axis rotates towards the slip direction, this can be used to determine the direction of glide. An actual example for a c.c.p. metal crystal is given in Figure 7.18a [42]. When the orientation of the tensile axis in Figure 7.18a reaches the great – circle joining the (0 01) and (1 11) poles, which is a mirror plane, the resolved shear stresses on two-slip systems are equal and slip might occur on both systems simultaneously. When two slip systems operate simultaneously, double slip or duplex slip is said to occur. In many cases in c.c.p. cubic metals, a crystal continues to slip on the primary system after the orientation has reached the mirror plane. In this case the orientation of the tensile axis ‘overshoots’ into the neighbouring unit triangle, so that slip is not proceeding on the nominally most highly stressed system. An example is shown in Figure 7.18b. After a certain

Kelly_c07.indd 225

11/30/2011 8:25:13 AM

226

Crystallography and Crystal Defects

amount of this additional primary slip the conjugate system suddenly operates and further slip occurs on this system, sometimes followed by ‘overshooting’ on the conjugate system, – as in Figure 7.18b. When the tensile axis reaches a k112l pole – [112] in the example shown – in Figure 7.18b, the vector sum of the two slip directions [101] and [011] – no further orientation change should occur, provided each slip system contributes equally to the deformation. There is also a change of orientation of the lattice of a crystal during a compression test. To deal with this case it is simplest to use vector formulae. We first use Equation 7.7 to find how a given plane of normal m is altered by glide. Let r1, r2 be any two nonparallel unit vectors in the given plane. Write m = r1 × r2. Now transform each of r1 and r2 according to Equation 7.7 to give r′1 and r′2. Then the new vector m′ representing m after a crystallographic glide strain of amount g is: m ′ = r1′ × r2′

(7.43)

Substituting for r′1 and r′2 from Equation 7.7, we have: m ′ = [r1 × r2 ] + γ (r1 ⋅ n)β × r2 − γ (r2 ⋅ n)β × r1 = m + γ β × [(r1 ⋅ n)r2 − (r2 ⋅ n)r1 ] (7.44) Using the formula for the vector triple product (Appendix 1), this is seen to be: m ′ = m + γ β × n × [r2 × r1 ]

(7.45)

m ′ = m − γ β × [n × m]

(7.46)

That is:

and again using the formula for the vector triple product: m′ = m − γ (( β ⋅ m)n − ( β ⋅ n)m)

(7.47)

m ′ = m − γ (β ⋅ m)n

(7.48)

or:

since (b ◊ n) = 0. It is evident from Equations 7.46 and 7.48 that any plane moves to its final position in such a way that its normal always lies in the plane containing the initial position of the normal and n, the normal to the glide plane. If we now consider the case of compression of a thin crystal between flat plates, as in Figure 7.19, we take the constraint to be that the plane initially normal to the stress axis must be maintained in this orientation with respect to the stress axis as the crystal deforms. To maintain positive values of g during compression, we suppose slip to occur so that (b ◊ m) is negative (Figure 7.19). Equation 7.48 then reads: m′ = m + γ ( β ⋅ m)n

(7.49)

From Equation 7.49, the normal to the glide plane then approaches the normal to the compression plates by rotating about an axis which is parallel to the line of intersection of the

Kelly_c07.indd 226

11/30/2011 8:25:15 AM

Glide and Texture F

(a)

F

(b) n

m m′

n b

227

h0

h

n

n b

F

Figure 7.19

F

Compression of a single crystal between plates

glide plane and the compression plates (Figure 7.19b). The initial thickness of the crystal is h0, which will be reduced during compression to a height h such that: h0 m′ = h m

(7.50)

because the volume of the crystal must be conserved. With the constraint that we have assumed, the change of orientation of the crystal lattice will be such that the normal to the slip plane rotates towards the axis of compression. If the initial and final angles, after a shear strain g, between the direction of compression and the normal to the slip plane are f0, f, and l and l0 are the corresponding obtuse values of the angle between the compression axis and the slip direction, then we have, from Equation 7.49: m′ ⋅ β = m ⋅ β

(7.51)

since: n⋅β = 0 Therefore: h0 cos λ 0 = h cos λ

(7.52)

m′ × n = m × n

(7.53)

h0 sin φ 0 = h sin φ

(7.54)

and also, from Equation 7.49:

Thus:

Kelly_c07.indd 227

11/30/2011 8:25:24 AM

228

Crystallography and Crystal Defects

Finding the modulus of each side of Equation 7.49, we have: 2

2

2

2

m ′ = m + 2γ m cos φ 0 cos λ 0 + γ 2 m cos2 λ 0

(7.55)

and using Equation 7.50: 2

⎛ h0 ⎞ 2 2 ⎜⎝ h ⎟⎠ = 1 + 2γ cos φ 0 cos λ 0 + γ cos λ 0

(7.56)

Since l0 is obtuse, because we have specified that (b ◊ m) is negative, it is apparent from this equation that h0 < h. Forming m′ ◊ n = m ◊ n + g (b ◊ m) and using Equations 7.50 and 7.52: γ =

cos φ cos φ 0 − cos λ cos λ 0

(7.57)

The resolved shear stress t is given by: 1/ 2

⎡ ⎛ h ⎞2 ⎤ F F⎛ h⎞ τ = cos φ cos λ = ⎜ ⎟ cos λ 0 ⎢1 − ⎜ ⎟ sin 2 φ 0 ⎥ A A ⎝ h0 ⎠ ⎢ ⎝ h0 ⎠ ⎥ ⎣ ⎦

(7.58)

Since A0h0 = Ah, Equation 7.58 may be written as: 1/ 2

2 ⎡ ⎛ h ⎞2 ⎤ F ⎛ h⎞ ⎢ τ= cos λ sin 2 φ 0 ⎥ 0 1− ⎜ ⎜ ⎟ ⎟ A0 ⎝ h0 ⎠ ⎢ ⎝ h0 ⎠ ⎥ ⎣ ⎦

(7.59)

In compression, the normal to the glide plane approaches the direction of compression, so that, for example, in Figure 7.13, F0 would approach the (111) pole until it meets the boundary between [001] and [011]; thereafter, systems B IV and A III would be equally stressed and the stable orientation of the normal to the glide plane would be (011), the plane midway between A and B lying in the same zone as A and B. Formulae for the change in orientation of the crystal lattice with respect to the direction of an applied force have been given for duplex slip in both compression and tension by Bowen and Christian [45]. During double glide there is a change in orientation of the lattice of the crystal with respect to the direction of a tensile force until the applied force is symmetrically related to the two slip systems. Thus, as we have seen, in tension of c.c.p. metals, k112l directions represent stable orientations lying midway between two k110l directions.

7.6 Texture Because large strains can cause a reorientation of the lattice of a crystal, it follows that, in a polycrystalline material, continued plastic flow, such as that which occurs during the working of metals, tends to develop a texture or a preferred orientation of the lattice within

Kelly_c07.indd 228

11/30/2011 8:25:32 AM

Glide and Texture

229

the grains, as well as a preferred change of shape of the grains. Working involves very large plastic strains, often hundreds of per cent. The development of a texture changes the crystallographic properties of the material significantly. A fine-grained material in which the grains have random lattice orientations will have isotropic properties, provided that other crystal defects such as inclusions and boundaries are uniformly distributed. However, a specimen with a preferred orientation will have anisotropic properties, which may be desirable or undesirable, depending upon the intended use of the material. The final texture that develops may resemble a single orientation or may comprise crystals distributed between two or more preferred orientations. During plastic flow the process of reorientation is gradual. In theory, the orientation change proceeds until a texture is reached that is stable against indefinitely continued flow of a given type. The theoretical end distribution of orientations and the manner in which it develops are a characteristic of the material, its crystal structure, its microstructure and the nature of the forces arising from the deformation process. Whether a material actually reaches its stable orientation depends upon many variables, such as the rate of working and the temperature at which it is carried out. Textural changes may correspond with marked changes in the ductility of a material. Thus there is an interplay between the role of deformation in creating texture and the role of texture in facilitating deformation. While the basic principles underlying texture development for single crystals have been presented in Section 7.4, the prediction of actual textures during forming processes is necessarily very complicated [46–48]. The various processes of texture development have been categorized according to their final state and to the kind of working involved, for example wire and fibre textures, compression textures, sheet and rolling textures, torsion textures and deep drawing textures. Some examples of ideal end textures are presented in Table 7.5. In addition to deformation textures, anisotropic properties of a polycrystalline material can also arise as a result of recrystallization following working (see Chapter 11, Footnote 1) or as a result of material fabrication processes that do not involve plastic deformation. For example, the vapour deposition of layers on substrates often results in a layer having a polycrystalline texture with a preferred orientation in the growth direction and random orientations perpendicular to the growth direction. Some examples of deposition textures are included in Table 7.5. There is usually a statistical distribution of orientations of the various crystals in a sample. This distribution can be measured and represented on a pole figure, such as in Figure 7.20. A pole figure is similar to a stereographic projection. On it is presented the statistical distribution of the orientations of the plane normals from a particular set of planes. A pole figure is usually obtained using diffraction from X-rays, neutrons or electrons.3 In the typical case of X-ray diffraction in the laboratory, the detector position is fixed to collect the diffraction from one particular set of planes. The sample is rotated about two axes so as to scan over all possible orientations. The corresponding pole figure is usually presented as a contour map, where the contours are labelled according to the relative strength of the diffraction signal. For example, Figure 7.20 is a pole figure showing the relative intensities of the reflections from {111} planes in a cold-rolled copper sample. The relative populations of planes in the various 3

For X-ray and neutron diffraction, the experiment obtains an average texture over volumes of the order of cubic millimetres. Using electron diffraction, textures from different regions of the sample can be discriminated, giving rise to the terms microtexture and mesotexture used in the study of textural variations within a sample.

Kelly_c07.indd 229

11/30/2011 8:25:38 AM

Kelly_c07.indd 230

11/30/2011 8:25:38 AM

b.c.c.

Rolling texture {plane}/kaxisl

c.c.p.

Rolling texture {plane}/kaxisl Tension (fibre) texture kaxisl

Deposition texture kgrowth directionl

Compression texture kaxisl

Tension (fibre) texture kaxisl

Description

Crystal structure

Fe single crystal and polycrystalline Mo, Nb, Ta, V, W, ferrosilicon, b-brass

– Between {001} k110l and {112} k11 0l; – {111} k112l k110l

k111l

Range from k110l to k311l; some k111l

k211l k111l Range from k110l to k311l

Some single crystals Single crystal and polycrystalline Al α-brass (70Cu / 30Zn) Au on cleaved NaCl by thermal evaporation

k111l and k100l

– {110} k112l and {110} k001l

– {111} k112l {001} k110l – – {110} k11 2l – and {112} k111 – l {123} k412l + {146} k211 l

– – {110} k11 2l then {112} k111 l

Texture

Al, Cu, Au, Ag, Ni

α-brass (70Cu / 30Zn)

Cu

Al single crystals

Al

Example material

Some common end or final textures

Table 7.5

Often both components together Occasionally

Random orientation in the plane of growth

Known as ‘pure metal’ texture at high temperatures and large deformations Up to 90% reduction After 90% reduction Orientations between these extremes or spread around these ideal end textures Known as ‘alloy’ or ‘brass’ texture; changes to ‘pure metal’ texture at high temperatures Relative proportions dependent upon temperature, strain rate, percentage reduction, stacking fault energy and twinning Except for starting orientation k111l For starting orientation k111l Tendency to rotate away from k111l and k100l Tendency to rotate away from k100l

Comments

[50]

[49]

[52]

[51]

[50] [51] [50]

[51]

[49]

[49]

[50]

[49]

Ref.

Kelly_c07.indd 231

11/30/2011 8:25:38 AM

h.c.p.

Compression texture kaxisl Deposition texture kgrowth directionl

Tension (fibre) texture kaxisl

Rolling texture {plane}/kaxisl

Compression texture kaxisl Deposition texture kgrowth directonl

Ti on oxidized Si (001) by magnetron sputtering

Zr, Ti Mg

Zn

Mg

[55]

Random in-plane orientation

k0001l

[51] [51] [51]

High temperatures Small reductions Large reductions

[51]

– k2110l k0001l 70°–from k0001l spiral texture k1010l k0001l

– k1010l

[51] [51]

Zn, Cd Zr, Ti

Deviation is in the transverse sense, i.e. about the rolling direction Low temperatures

[51]

– 20–25° off {0001} k112 –0l 30–40° off {0001} k1010l

Low growth rates and low substrate temperatures Some in-plane texture in both cases

k110l – {0001} k1120l

[53,54]

High growth rates

k111l

Mo on (001) Si by magnetron sputtering

Mg

[50]

k111l, some k100l

Fe

232

Crystallography and Crystal Defects RD

0.5 1 2 3 4 5 8 12 0.5 1

2 3 5 8 12 15

0.5

1 2 3

CD 4 5

Near (123) [412] Near (146) [211] (110) [112] (112) [111] (110) [001]

Figure 7.20 The {111} pole figure of electrolytic copper rolled to 96.6% reduction at room temperature, where RD is the rolling direction and CD is the cross direction. The numbers represent relative intensities of the diffraction signal [56]

orientations are proportional to the numbers against the contour lines. The pole figure is interpreted in terms of an ideal end orientation. In uniaxial textures, such as those obtained in tension, compression and wire- and rod-forming processes, it is often sufficient to specify which crystallographic direction (or directions) lies parallel to the unique axis. For sheet textures, ideal orientations are given by a plane or planes lying parallel to the plane of the sheet and a direction or directions in the plane lying parallel to a significant direction in the sheet, such as the rolling direction (RD). For example, to identify {110} – k001l and {110} k11 2l textures the procedures illustrated in Figure 7.21 might be followed. First, identify the orientations of the {111} poles relative to the {110} plane and the k001l and k112l directions. A stereographic projection is shown in Figure 7.21a with the (110) plane normal perpendicular to the plane of the paper. All of the {111} poles are shown, along with those k001l and k112l directions that are in the (110) plane and thus could lie parallel to the RD. The orientations of the {111} poles when the RD corresponds to k001l and k112l

Kelly_c07.indd 232

11/30/2011 8:25:38 AM

Glide and Texture (b) (a)

233

Rolling direction

001 112

112

111

111 111 110 111

111

111 112

112 001

(c)

(d) Rolling direction

Rolling direction +

Figure 7.21 (a) Standard stereographic projection in the (110) orientation showing the poles for the {001}, {112} and {111} plane normals. Orientations of the {111} plane normals for – (b) the (110)k001l rolling texture, (c) the (110)k11 2l rolling texture and (d) a combination of (b) and (c)

are shown in Figures 7.21b and c, respectively. Note that there are two possible k112l orientations, which results in there being 12 {111} pole positions. The case where the end texture – contains both {110} k001l and {110} k11 2l orientations is illustrated in Figure 7.21d. A pole figure from an ideal end texture will have the appearance of a pole plot from one or a few single crystals, depending upon how many orientations comprise the end texture. A real textured material will show a broader distribution of intensities about the ideal orientation. How close the actual texture is to the ideal texture is a qualitative judgement. Actual textures are described as varying from ‘weak’ (a small proportion of grains having

Kelly_c07.indd 233

11/30/2011 8:25:38 AM

234

Crystallography and Crystal Defects f1 F

45º f2

90º

90º

– 45º

Figure 7.22 Spatial representation of the half-maximum density of the ODF relevant for both heavily cold-rolled heavily rolled a-brass and heavily rolled silver [46,47,57] ND F [001]

[100] Nodal direction

f2

RD f1 [010]

Figure 7.23 Definition of the orientation of a crystallite in rolled sheet by means of three Euler angles, f1, F and f2 (after [47]). The nodal direction is parallel to the vector product of ND and the crystallite [001] direction. RD is the rolling direction and ND is the sheet normal

rotated to the endpoint) to ‘strong’ (a large volume fraction of grains having rotated to or close to the endpoint). A more computationally intensive, but more representative, measure of texture is in the orientation distribution function (ODF). Using data from pole figures taken for several reflections, the orientations of three primary axes of the crystallites are plotted with respect to three standard axes. ODFs can be displayed as three-dimensional plots or as a series of two-dimensional sections. An ODF relevant for both heavily rolled α-brass and heavily rolled silver is shown in Figure 7.22, where f1, F and f2 are the angles between principal directions in the crystallites and significant directions in the forming process and are known as the Euler angles. In this diagram the surface shown represents the half-maximum density – of the orientation distribution corresponding to a [011](211) texture.

Kelly_c07.indd 234

11/30/2011 8:25:38 AM

Glide and Texture

235

Typical Euler angles for rolled sheet are illustrated in Figure 7.23; F is the angle between the crystallite [001] direction and the sheet normal (ND), f2 is the angle between the crystallite [100] direction and the nodal direction, and f1 is the angle between the nodal direction and RD. The nodal direction lies perpendicular to ND and the crystallite [001] direction and is parallel to the direction defined by the vector product of these two directions. We see in Figure 7.22 that the spread in f1 is about 10º, the spread in F is about 10º and the spread in f2 is about 20º, indicating a pronounced texture with only a small spread in orientation. Using the mathematical analysis of the ODF, a near-quantitative description of texture is possible.

Problems – 7.1 a-ZnS has the point group 4 3m. (a) Does it possess a centre of symmetry? Assume that the slip planes are {111} and – the slip directions k110l. – – (b) Is slip in the [11 0] direction crystallographically equivalent to that in [110]? 7.2 During the process of glide the displacements imposed upon the surfaces of a crystal are centrosymmetric. Use this notion and Figure 7.5 to deduce the rules (1)–(4) given in Section 7.2. 7.3 Enumerate the number of physically distinct glide systems for a cubic crystal (e.g. a – – c.c.p. metal) of point group m3m which slips on {111} in k110l directions. Along which directions should such a crystal be stressed in uniaxial tension if the resolved shear stress is to be the same on (a) eight systems, (b) six systems and (c) four systems? Show that for a given tensile axis [uvw], the Schmid factor cos f cos l for the slip system which operates must satisfy the condition: 2 3 3

≤ cos φ cos λ ≤ 0.5

Hence or otherwise, determine the individual values of f and l when cos f cos l = 0.5. 7.4 Establish the number of independent slip systems possessed by CsBr, which is cubic – (Pm3m) and slips on {110} in k001l. How many independent systems does such a crystal possess if pencil glide occurs with the same glide directions? – 7.5 Consider an amount of glide g to occur on the (011) plane in the [011 ] direction of a cubic crystal. Take axes parallel to the cubic axes. (a) Write down the components of the pure strain tensor. (b) Write down the components of the pure strain tensor if glide of amount g ′ occurs – on (100) in the same direction, [011], as before. (c) How many components of the pure strain tensor can be altered independently of one another by glide on these two systems? (d) If g ′ was always equal to a constant fraction of g so that g ′ = kg, what would be the answer to (c)?

Kelly_c07.indd 235

11/30/2011 8:25:39 AM

236

Crystallography and Crystal Defects

(e) Use the above results to prove generally that if pencil glide occurs in a crystal then slip with a given slip direction can provide two independent components of the pure strain tensor. 7.6 Can you think of three slip directions which operating together would provide a contradiction of the statement, ‘When pencil glide occurs a crystal need only possess in general three noncoplanar slip directions in order for a general strain to be possible’? – – 7.7 Copper is cubic (Fm3m) and slips on {111} k11 0l. Sketch a stereogram of a crystal showing the components of the slip systems. Which slip system(s) are expected to operate if the tensile axis is (a) [123], (b) [113] and (c) [122]? – – 7.8 Rock salt is cubic (Fm3m) and slips on {110} k11 0l. Sketch a stereogram showing the components of the slip systems. Which slip system(s) are expected to operate if the tensile axis is (a) [123], (b) [213] and (c) [013]? – 7.9 Magnesium oxide is cubic with the NaCl structure and slips on {110} in k11 0l. (a) List the directions along which a tensile or compressive force applied to the crystal cannot produce glide. (b) Can the crystal be twisted plastically about [100]? (c) List the same directions as in (a) for graphite. (The glide elements for graphite are listed in Table 7.1.) 7.10 The analysis of strain in Chapter 6 requires that the strain be infinitesimal. Explain why this restriction does not invalidate the analysis of Section 7.3 (which shows that five independent glide systems are necessary for a general deformation) because, when glide takes place, large strains occur in some volumes of the crystal. 7.11 A tetragonal crystal is subject to a tensile stress of magnitude s along [100] and to a shear stress t on (100) in [010]. (a) Write down the components of the stress tensor referred to the crystal axes. – (b) Find the shear stress on (110) in the [11 0] direction by altering the axes of reference of the stress tensor. (c) Find, by the same procedure, the tensile stress normal to (110). 7.12 Prove Equation 7.30. –

7.13 A single crystal of zinc which slips on (0001) in k1120l directions is stressed in tension and is oriented so that the tensile axis makes an angle of 45° with [112ˉ0] and is at 60° to the normal to (0001). (a) Along which direction will slip first occur? (b) If slip starts when the tensile stress on the crystal is 2.1 MPa, calculate the critical resolved shear stress necessary to produce slip in zinc. – 7.14 Copper slips on {111} in k11 0l. A cylindrical single crystal 10 cm long is stressed in – tension. The tensile axis is [123]. (a) Which is the slip system with the highest resolved shear stress? The specimen is strained in tension until the tensile axis reaches a symmetry position where two slip systems have equal resolved shear stresses.

Kelly_c07.indd 236

11/30/2011 8:25:40 AM

Glide and Texture

237

(b) Which are the two systems? (c) What is the orientation of the tensile axis at this stage? (d) What is the new length of the specimen? 7.15 Discuss the following statement. ‘A general small homogeneous change of shape of a body can be described by a pure strain and a rotation. If the volume of the body is conserved the pure strain tensor has five independent components and the pure rotation tensor has three. Therefore, eight quantities must be specified to describe the change of shape of a single crystal within a polycrystalline body. It follows from this that eight slip systems must in general operate in all grains of a polycrystal which is subject to a general change of shape.’

Suggestions for Further Reading H.-J. Bunge (1982) Texture Analysis in Materials Science, Mathematical Methods, Butterworths, London. G.Y. Chin, R.N. Thurston and E.A. Nesbitt (1966) Finite plastic deformation due to crystallographic slip, Trans. Am. Inst. Min. Metall. Petrol. Engrs, 236, 69–76. G.E. Dieter (1988) Mechanical Metallurgy (SI metric edition adapted by D.J. Bacon), McGraw-Hill, London. G.W. Groves and A. Kelly (1963) Independent slip systems in crystals, Phil. Mag., 8, 877–887. W.J. McGregor Tegart (1966) Elements of Mechanical Metallurgy, Macmillan, New York. E. Schmid and W. Boas (1950) Plasticity of Crystals, F.A. Hughes and Co. Ltd, London.

References [1] E. Reusch (1867) Ueber eine besondere Gattung von Durchgängen im Steinsalz und Kalkspath, Poggendorff’s Annalen der Physik und Chemie, 132, 441–451. [2] J.A. Ewing and W. Rosenhain (1899) Experiments in micro-metallurgy:— Effects of Strain. Preliminary notice, Proc. Roy. Soc. Lond. A, 65, 85–90. [3] J.A. Ewing and W. Rosenhain (1900) The crystalline structure of metals, Phil. Trans. Roy. Soc. Lond. A, 193, 353–375. [4] G.W. Groves and A. Kelly (1963) Independent slip systems in crystals, Phil. Mag., 8, 877–887. [5] J.P. Hirth and J. Lothe (1982) Theory of Dislocations, 2nd Edition, John Wiley and Sons, New York. [6] F.R.N. Nabarro (1987) Theory of Crystal Dislocations, Dover Publications, New York. [7] D.J. Bacon and V. Vitek (2002) Atomic scale modelling of dislocations and related properties in the hexagonal-close-packed metals, Metall. Mater. Trans A, 33, 721–733. [8] A. Kelly and D.J. Rowcliffe (1966) Slip in titanium carbide, Phys. Stat. Sol., 14, K29–K33. [9] B.L. Eyre and A.F. Bartlett (1966) Determination of the Burgers vector of dislocations in deformed uranium carbide, Phil. Mag., 13, 641–643. [10] W. Skrotzki, R. Tamm, C.-G. Oertel, J. Röseberg and H.-G. Brokmeier (2000) Microstructure and texture formation in extruded lead sulfide (galena), J. Struct. Geol., 22, 1621–1632. [11] W.A. Rachinger (1956) Glide in lead telluride, Acta Metall., 4, 647–649. [12] J.F. Byron (1968) The yield and flow of single crystals of uranium oxide, J. Nucl. Mater., 28, 110–114. [13] T.E. Mitchell (1979) Application of transmission electron microscopy to the study of deformation in ceramic oxides, J. Am. Ceram. Soc., 62, 254–267. [14] T.E. Mitchell (1999) Dislocations and mechanical properties of MgO–Al2O3 single crystals, J. Am. Ceram. Soc., 82, 3305–3316. [15] K.-H. Yang, N.-J. Ho and H.-Y. Lu (1999) Deformation microstructure in (001) single crystal strontium titanate by Vickers indentation, J. Am. Ceram. Soc., 92, 2345–2353.

Kelly_c07.indd 237

11/30/2011 8:25:40 AM

238

Crystallography and Crystal Defects

[16] C. Levade, J.-J. Couderc, I. Dudouit and J. Garigue (1986) The plastic behaviour of natural sphalerite crystals between 473 and 873 K, Phil. Mag. A, 54, 259–279. [17] B. Kedjar, L. Thilly, J.-L. Demenet and J. Rabier (2010) Plasticity of indium antimonide between −176 °C and 400 °C under hydrostatic pressure. Part II: Microscopic aspects of the deformation, Acta Mater., 58, 1426–1440. [18] Y. Androussi, G. Vanderschaeve and A. Lefebvre (1989) Slip and twinning in high-stressdeformed GaAs and the influence of doping, Phil. Mag. A, 59, 1189–1204. [19] S. Amelinckx and P. Delavignette (1960) Electron optical study of basal dislocations in graphite, J. Appl. Phys., 31, 2126–2135. [20] F. Yang and J.C.M. Li (2007) Deformation behavior of tin and some tin alloys, J. Mater. Sci.: Mater. Electron., 18, 191–210. [21] K.H.G. Ashbee and R.E. Smallman (1963) The plastic deformation of titanium dioxide single crystals, Proc. Roy. Soc. Lond. A, 274, 195–205. [22] K. Suzuki, M. Ichihara and S. Takeuchi (1991) High-resolution electron microscopy of lattice defects in TiO2 and SnO2, Phil. Mag. A, 63, 657–665. [23] M. Georgieff and E. Schmid (1926) Über die Festigkeit und Plastizität von Wismutkristallen, Z. Phys., 36, 759–774. [24] R.E. Slonaker, M. Smutz, H. Jensen and E.H. Olson (1965) Factors affecting the growth and the mechanical and physical properties of bismuth single crystals, J. Less-Common Metals, 8, 327– 338. [25] C. Steegmuller and J.S. Daniel (1972) Slip in bismuth, J. Less-Common Metals, 27, 81–85. [26] J.G. Rider and F. Heckscher (1966) Slip in single crystals of mercury, Phil. Mag., 13, 687–692. [27] J.D. Snow and A.H. Heuer (1973) Slip systems in Al2O3, J. Am. Ceram. Soc., 56, 153–157. [28] R.J. Stokes, T.L. Johnston and C.H. Li (1961) Mechanical properties of tellurium single crystals, Acta Metall., 9, 415–427. [29] F.J. Spooner and C.G. Wilson (1966) Slip and twinning in gallium, J. Less-Common Metals, 10, 169–184. [30] J.S. Daniel, B. Lesage and P. Lacombe (1971) The influence of temperature on slip and twinning in uranium, Acta Metall., 19, 163–173. [31] V. Vitek (1992) Structure of dislocation cores in metallic materials and its impact on their plastic behaviour, Prog. Mater. Sci., 36, 1–27. [32] W.G. Tyson (1969) Slip modes of thallium, Acta Metall., 17, 863–868. [33] T.G. Carnahan and T.E. Scott (1973) Deformation modes of hcp yttrium at 77, 298, and 497 K, Metall. Trans., 4, 27–32. [34] R.E. von Mises (1928) Mechanik der plastischen Formänderung von Kristallen, Zeitschrift für Angewandte Mathematik und Mechanik, 8, 161–185. [35] E. Schmid (1925) Neuere Untersuchungen an Metallkristallen, Proc. 1st. International Congress for Applied Mechanics, Delft, 1924 (edited by C.B. Biezeno and J.M. Burgers), Technische Boekhandel en Drukkerij J. Waltman, Jr., Delft, pp. 342–353. [36] G.Y. Chin (1972) Competition among {110}, {112} and {123} slip modes in bcc metals, Metall. Trans., 3, 2213–2216. [37] B. Orlans-Joliet, B. Bacroix, F. Montheillet, J.H. Driver and J.J. Jonas (1988) Yield surfaces of b.c.c. crystals for slip on the {110} and {112} systems, Acta Metall., 36, 1365– 1380. [38] E. Schmid and W. Boas (1950) Plasticity of Crystals, F.A. Hughes and Co. Ltd, London. [Originally published as Kristallplastizität mit besonderer Berücksichtigung der Metalle, Julius Springer, Berlin in 1935.] [39] G.I. Taylor and C.F. Elam (1925) The plastic extension and fracture of aluminium crystals, Proc. Roy. Soc. Lond. A, 108, 28–51. [40] J. Diehl, personal communication to A. Seeger, acknowledged on p. 24 of A. Seeger (1958) Kristallplastizität, Handbuch der Physik, Band VII.2: Kristallphysik II (edited by S. Flügge), Springer-Verlag, Berlin, pp. 1–210. [41] I.M. Hutchings (1993) Quick non-graphical method for deducing slip systems in cubic close packed metals in tension or compression, Mater. Sci. Tech., 9, 929–930.

Kelly_c07.indd 238

11/30/2011 8:25:40 AM

Glide and Texture

239

[42] R.J. Price and A. Kelly (1964) Deformation of age-hardened aluminium alloy crystals–I. Plastic flow, Acta Metall., 12, 159–169. [43] Freiherr von Göler and G. Sachs (1929) Zugversuche an Kristallen aus Kupfer und α-Messing, Z. Phys., 55, 581–620. [44] A. Seeger (1958) Kristallplastizität, Handbuch der Physik, Band VII.2: Kristallphysik II (edited by S. Flügge), Springer-Verlag, Berlin pp. 1–210. [45] D.K. Bowen and J.W. Christian (1965) The calculation of shear stress and shear strain for double glide in tension and compression, Phil. Mag., 12, 369–378. [46] H.-J. Bunge (1982) Texture Analysis in Materials Science, Mathematical Methods, Butterworths, London. [47] R.W. Cahn (1991) Measurement and control of texture, in Volume 15, Materials Science and Technology (series editors R.W. Cahn, P. Haasen and E.J. Kramer), Processing of Metals and Alloys (edited by R.W. Cahn), Wiley–VCH, Chichester and Weinheim, Chapter 10: pp. 429–480. [48] U.F. Kocks, C.N Tomé and H.-R. Wenk (1998) Texture and Anisotropy: Preferred Orientations in Polycrystals and their Effect on Materials Properties, Cambridge University Press, Cambridge. [49] I.L. Dillamore and W.T. Roberts (1965) Preferred orientation in wrought and annealed metals, Metall. Rev., 10, 271–380. [50] H. Hu, R.S. Cline and S.R. Goodman (1965) Deformation textures in metals, in Recrystallization, Grain Growth and Textures, American Society for Metals, Metals Park, OH, pp. 295–367. [51] C.S. Barrett and T.B. Massalski (1980) Structure of Metals: Crystallographic Methods, Principles and Data, Pergamon, Oxford, pp. 541–583. [52] K.E. Harris and A.H. King (1994) Localized texture formation and its detection in polycrystalline thin films of gold, in Mechanisms of Thin Film Evolution, Volume 317 (editors S.M. Yalisove, C.V. Thompson and D.J. Eaglesham), Materials Research Society, Pennsylvania, pp. 425–430. [53] M. Vill, S.G. Malhotra, Z. Rek, S.M. Yalisove and J.C. Bilello (1994) White-beam transmission characterization of texture in Mo thin films and Mo/W multilayers, in Mechanisms of Thin Film Evolution, Volume 317 (editors S.M. Yalisove, C.V. Thompson and D.J. Eaglesham), Materials Research Society, Pennsylvania, pp. 413–418. [54] O.P. Karpenko, M. Vill, S.G. Malhotra, J.C. Bilello and S.M. Yalisove (1994) Texture in sputtered Mo films, in Mechanisms of Thin Film Evolution, Volume 317 (editors S.M. Yalisove, C.V. Thompson and D.J. Eaglesham), Materials Research Society, Pennsylvania, pp. 467–472. [55] R. Ahuja and H.L. Fraser (1994) Structural transitions in titanium-aluminum thin film multilayers, Mechanisms of Thin Film Evolution, Volume 317 (editors S.M. Yalisove, C.V. Thompson and D.J. Eaglesham), Materials Research Society, Pennsylvania, pp. 479–484. [56] H. Hu and S.R. Goodman (1963) Texture transition in copper, Trans. Met. Soc. AIME, 227, 627–639. [57] H. J. Bunge (1987) Three-dimensional texture analysis, Int. Mater. Rev., 32, 265–291.

Kelly_c07.indd 239

11/30/2011 8:25:40 AM

8 Dislocations 8.1

Introduction

In Chapter 7 the geometry of glide was studied on a macroscopic scale. The geometrical results on this scale are adequately described by the model of blocks of crystal sliding over one another rigidly. However, when glide occurs in a real crystal, all the atoms above the slip plane do not move simultaneously over those below. At any given time some of the atoms have moved into their new positions while others have not yet done so, and the displacement of the upper block of crystal relative to the lower varies from one region of the slip plane to another. Lines in the slip plane separating regions where slip has occurred from those where it has not are called dislocations. This is the simplest way in which to introduce the idea of dislocations; we shall see later that they can be formed in other ways. For ease of illustration and simplicity we will consider slip in a crystal with the primitive cubic lattice and one atom associated with each lattice point. A block of such a crystal cut with faces parallel to {100} planes is shown in Figure 8.1. A (001) slip plane, PQRT, is shown, and slip in the [010] direction has occurred over only the region PQSS′. It is evident that the crystal lattice is distorted, especially close to the dislocation which lies along SS′. The distortion decreases as the amount of slip over PQSS′ is reduced. In Figure 8.1 the displacement over PQSS′ is equal to [010],1 which is the smallest displacement that can be made without producing a fault in the crystal structure at the plane PQSS′. The displacement is a constant vector quantity over the whole region PQSS′ (except within a few atoms of the dislocation line SS′), and it is this quantity that characterizes the dislocation. As a dislocation moves through the crystal, the displacement associated with it does not change. This characteristic quantity is called the Burgers vector of the dislocation.

1 A specific displacement is written in terms of its components along the crystal axes (Section 1.2). In cubic crystals the lattice parameter a is often included in the notation, although it is superfluous.

Crystallography and Crystal Defects, Second Edition. Anthony Kelly and Kevin M. Knowles. © 2012 John Wiley & Sons, Ltd. Published 2012 by John Wiley & Sons, Ltd.

Kelly_c08.indd 241

11/30/2011 8:49:27 AM

242

Crystallography and Crystal Defects

T S′

P

R S

Q

[001] [010] [100]

Figure 8.1 A screw dislocation in a primitive cubic lattice

T

R P

Q

Figure 8.2

As the dislocation SS′ in Figure 8.1 moves from right to left, the slipped region of the crystal increases. When the dislocation reaches the surface at RT, the whole crystal has been slipped by [010], as shown in Figure 8.2. A dislocation may turn into a new orientation; this does not change its Burgers vector. The result of rotating SS′ in the slip plane through a right angle is shown in Figure 8.3. The dislocation which results, EE′, has the same [010] displacement vector associated with it, the crystal now having slipped by this amount over

Kelly_c08.indd 242

11/30/2011 8:49:27 AM

Dislocations

243

T

E R

P

E′ Q

Figure 8.3 An edge dislocation in a primitive cubic lattice

T

P R D

D′ Q

Figure 8.4 A mixed dislocation, DD′, in a primitive cubic lattice

QREE′ and not having slipped over PTEE′. A length of dislocation which lies normal to its Burgers vector, such as EE′, is called an edge dislocation; one like SS′ which lies parallel to its Burgers vector is called a screw dislocation. In general, a dislocation may lie at any angle to its Burgers vector or may be curved like the dislocation DD′ in Figure 8.4. At D′ the dislocation is in edge orientation and at D in screw orientation. Elsewhere the dislocation has both edge and screw components and is referred to as mixed. The reason for the names ‘edge’ and ‘screw’ becomes clear when we look at the positions of the atoms around the dislocation. The positions close to the dislocation cannot be calculated exactly without a detailed knowledge of the laws of force between the atoms,

Kelly_c08.indd 243

11/30/2011 8:49:28 AM

244

Crystallography and Crystal Defects K

E

Figure 8.5 Atom positions around an edge dislocation (according to Equation 8.21) (a) q 4

3

S1

S

S2

x1

1

2

(b)

S1′ 4 3 2 1 4 3 2 1 S1

Figure 8.6 Screw dislocation in a simple cubic crystal (a) looking along the dislocation and (b) looking normal to the dislocation which lies along S1S1′

although in some cases they can be observed at the surface of a crystal at atomic resolution with scanning tunnelling microscopes and atom probes, and within thin crystals using high-resolution transmission electron microscopy. For the present, it is enough to recognize that there is a small amount of arbitrariness in the location of the atoms shown in Figures 8.5 and 8.6. The arrangement of atoms in a plane normal to the edge dislocation EE′ of Figure 8.3 is shown in Figure 8.5. There is an extra incomplete plane of atoms KE above the slip plane. The edge of the extra plane coincides with the dislocation and gives it

Kelly_c08.indd 244

11/30/2011 8:49:28 AM

Dislocations

245

its name. A similar view of a plane normal to a screw dislocation does not show the distortion of the lattice, because the displacements of the atoms are parallel to the dislocation in this case (Figure 8.6a). A view of the atom positions in the atom planes immediately above and below the slip plane is given by Figure 8.6b. The term ‘screw’ arises because the successive planes of atoms normal to the dislocation are converted by the presence of the dislocation into a single screw surface, or spiral ramp. This can be visualized from Figure 8.1 by imagining oneself to be walking around the dislocation on these planes. Successive intersections of such a tour with the plane of Figure 8.6 occur at 1, 2, 3, 4 and so on. Crystals normally contain a great number of dislocations, even before they are plastically deformed. The total length of dislocation line in 1 m3 of a metallic crystal (the dislocation density) may typically be 1012 m, although a wide variation over orders of magnitude is possible, depending on the degree to which the metal has been either annealed or cold worked. So far we have considered only dislocations occurring as a result of slip and lying in a slip plane. This is an unnecessary restriction, and dislocations can, in fact, be produced in other ways than by glide, as we shall see in Section 8.2. A general method is therefore needed for describing the Burgers vector – that characteristic discontinuity of displacement which defines a dislocation in a crystal. The following method is often used. First, a closed circuit is made around the suspected dislocation, called a Burgers circuit. This is a circuit made by jumping from one lattice point to a neighbouring lattice point until the starting point is reached again. The circuit must be made in ‘good’ material – that is, in regions of the crystal in which, even though they may be strained, each jump is recognizably associated with a jump in a perfect crystal of the same structure. With this vital condition fulfilled, a corresponding set of jumps can then be traced in the perfect crystal; if it fails to close, the circuit in the real crystal does indeed surround a dislocation. A little thought will show that if the circuit fails to close then it must do so by a lattice vector. The lattice vector that is needed to complete the circuit in the ideal crystal is defined as the Burgers vector of the dislocation. A dislocation that can be dealt with by this procedure must have a Burgers vector equal to a translation vector of the Bravais lattice; such a dislocation is called a perfect dislocation. This method of defining the Burgers vector is illustrated in Figure 8.7. The circuit of 17 successive jumps in the real crystal has a corresponding set of jumps in the perfect crystal which fails to close. The vector [010] is needed to complete the circuit in the ideal crystal; this is the Burgers vector. Some sign convention is needed to define the sense of the Burgers vector. The FS/RH convention works as follows. First, a sense is arbitrarily attached to the dislocation line. This permits a choice of Burgers circuit with a right-hand screw relationship to the line (the RH of the notation). In Figure 8.7 the line is taken to run into the paper. The Burgers vector is then taken to run from the finish to the start of the path in the perfect crystal (the FS of the notation); for example, from F to S in Figure 8.7.2 If the sense of the line is reversed, the Burgers vector is also reversed, so that some consistency in choosing a line sense is desirable.

2

The opposite convention, SF/RH, is used by some authors. For an account of where one convention has been used, and where the other, see de Wit [1].

Kelly_c08.indd 245

11/30/2011 8:49:28 AM

246

Crystallography and Crystal Defects

S

F

[010]

Figure 8.7 A Burgers circuit around an edge dislocation (a)

(b) a E2 E1 E1

E2

Figure 8.8

As an example, consider a closed loop of dislocation lying in a slip plane (Figure 8.8a). Suppose that within the loop the top half of the crystal has slipped by [010] with respect to the bottom half, as shown by the arrow. Then the positions of the atoms in the (100) plane (the plane a in Figure 8.8a) are as shown in Figure 8.8b. Since the edge dislocations at E1 and E2 would annihilate one another if they glided together (their extra planes would join), they are commonly referred to as edge dislocations of opposite sign. The Burgers vector at E2 is in the opposite direction to that at E1 if the direction assigned to the line at E2 is the same as that assigned to the line at E1, such as into the page. This would be perfectly fine if the dislocation lines at E1 and E2 were actually parallel lines. If the whole loop is being considered, however, it is more logical to make the sense of the line continuous around the loop. Then if the direction of the line at E1 is into the page, the direction of the line at E2 must be out of the page, and when the Burgers circuits round E1 and E2 are each taken in the RH sense, the same sense of Burgers vector is obtained at E1 as at E2 This second way of stating the Burgers vector emphasizes the fact that the displacement discontinuity, which the Burgers vector measures, remains constant along a given dislocation line. This follows because if we move the Burgers circuit along the dislocation line it must remain in good material.

Kelly_c08.indd 246

11/30/2011 8:49:28 AM

Dislocations (a)

247

(b) l

n D′

d

B′

l

P

B

d

A′ Q A D

Figure 8.9

The principle of the conservation of the Burgers vector is a general one, and from it, it follows that a dislocation line cannot end inside a crystal. It must end at a surface, form a closed loop or meet other dislocations. A point at which dislocation lines meet is called a node. The conservation of the Burgers vector in this case can be stated in the following way. If the directions of all the dislocation lines are taken to run out from the node then the sum of the Burgers vectors of all the dislocations is zero. This is the dislocation analogue of Kirchhoff’s law of the conservation of electric current in a network of conductors.

8.2

Dislocation Motion

We have seen that the motion of a dislocation on a slip plane changes the area over which slip has occurred. In this section the effect of dislocation motion in general will be discussed. Consider two neighbouring atoms, P and Q, lying at lattice points in a plane which is threaded by a dislocation DD′ (Figure 8.9a). Suppose the dislocation passes between P and Q so as to move inside a Burgers circuit, part of which is the step from P to Q. The corresponding circuit in the ideal crystal then acquires a closure failure equal to the Burgers vector, b. This must be attributed to a displacement of P relative to Q of b in the real crystal (it cannot be attributed to the relative displacement of the members of any other neighbouring pair of atoms in the Burgers circuit since it is possible to draw Burgers circuits through these that do not contain the dislocation either before or after its movement). The determination of the sense of the relative displacement requires some care. Define a positive direction QP by the cross product l × d (Figure 8.9b); that is, l, d and QP are related as a right-handed set of axes x, y, z. Here l is the vector parallel to the dislocation line used in defining the Burgers vector b by the FS/RH convention; d is a vector in the direction of motion of the dislocation. With this definition, the displacement of the atom on the positive side, P, relative to that on the negative, Q, is +b when the dislocation passes between P and Q, as shown. We shall use this result to study the relative displacement of material on either side of the surface that a dislocation sweeps out during its motion. Suppose a segment of a dislocation line AB moves to A′B′, sweeping out a plane surface whose unit normal is n. The sense of n is defined in accordance with the previous paragraph as the sense of l × d (Figure 8.9b). The atoms above ABB′A′ are displaced by b relative to those below.

Kelly_c08.indd 247

11/30/2011 8:49:28 AM

248

Crystallography and Crystal Defects (a)

b

(b)

b

Figure 8.10 The dislocation loop shown in (a) can glide so that its area projected normal to the Burgers vector does not change. It moves in the surface of a cylinder. (b) This shows that a screw segment can leave the surface of this cylinder without changing the projected area

If b · n is positive, the atoms above move away from those below, creating a void, whose volume is b · n per unit area swept out. Motion for which b · n < 0 requires the disposal of extra material of volume b · n per unit area. When b · n ≠ 0 the dislocation motion is normally accompanied by diffusion, which brings in atoms to fill the void when b · n > 0 and disperses the extra atoms when b · n < 0. Dislocation motion of this type is called ‘climb’. The origin of this name can be seen from Figure 8.5. If the atoms on the edge of the extra plane are removed, the edge dislocation in Figure 8.5 will climb up out of its slip plane. Climb downwards could be accomplished by adding atoms to the extra plane. Dislocation glide is motion that does not involve the addition or removal of material; that is, motion for which b · n = 0. The glide surface is defined accordingly as that surface which contains the dislocation line and whose normal is everywhere perpendicular to the Burgers vector. For a straight-edge dislocation, this defines a single plane, which is the slip plane. For a screw dislocation any plane passing through the dislocation fulfils the condition b · n = 0. For a closed loop of dislocation a cylinder is defined as the glide surface. The surface of the cylinder is generated by lines parallel to the Burgers vector passing through all points on the dislocation (Figure 8.10a). The glide of the loop is not confined to the surface of its glide cylinder, because if it has any screw parts they can glide on any plane; however, the area of the loop in projection on a plane normal to the axis of the cylinder remains constant (Figure 8.10b). This area is zero for a loop on a slip plane (Figure 8.8a). When the area is not zero, the loop is called ‘prismatic’. A special case is a pure-edge dislocation loop. This could be produced by prismatic punching, as shown in Figure 8.11, in which case its structure corresponds to a penny-shaped disc of extra atoms in the plane of the loop. With a Burgers vector of opposite sense, its structure corresponds to a disc of missing atoms. In the latter case, the loop could be formed by collecting together a disc of vacant lattice sites. When a dislocation glides, there is no problem of acquiring or disposing of extra atoms. This is in sharp distinction to climb, and it leads us to suppose that a dislocation will be able

Kelly_c08.indd 248

11/30/2011 8:49:29 AM

Dislocations

249

(a)

(b)

E

E′ E

E′

Figure 8.11 (a) Production of a prismatic dislocation loop by punching. (b) Section normal to the plane of the loop and passing through E and E′

to glide much more quickly than it can climb. The ease of gliding may be quite different for different crystallographic surfaces, and may be so much easier for one crystallographic plane that slip is effectively confined to that plane.

8.3 The Force on a Dislocation In Section 8.1 we found that when a dislocation moved on a slip plane, the area of the slip plane across which slip had occurred was increased or decreased, according to the direction of motion. As a result, work may be done by the forces applied to the crystal. For example, suppose forces acting in the slip direction are applied to the top and bottom surfaces of the crystal in Figure 8.1, in the directions SS′ on the top surface and S′S on the bottom. When the dislocation, of unit length say, moves to the left and sweeps out an area 1.dx of slip plane, applied forces of magnitude s dx move through the slip distance b, if the applied forces are of strength s per unit area of the top and bottom surfaces. The work done is then: dw = σ b dx

(8.1)

We can use this result to define a force3 acting on a unit length of the dislocation in the direction Ox: F=−

dE dx

(8.2)

where E is the energy of the system, which comprises the crystal and the device applying the forces to it. If we examine the work done by the forces acting on the surfaces at the slip plane, which are displaced relative to one another when the dislocation moves a distance dx, we see that it has the same magnitude sb dx as the work done by the externally applied forces, but is opposite in sign. This work done at the slip plane is dissipated, like the work 3

Defining a ‘force’ exerted on a dislocation line is a way of describing the tendency of the configuration which constitutes the dislocation to move through the crystal. There is no physical force on a dislocation line in the sense in which there is a force on a rod when a string attached to it is pulled, for example.

Kelly_c08.indd 249

11/30/2011 8:49:29 AM

250

Crystallography and Crystal Defects

done at sliding surfaces in a friction problem. The dissipated energy is supplied by the device applying the forces to the crystal, which therefore loses energy: − dE = dw = σ b dx

(8.3)

Substituting Equation 8.2 in Equation 8.3 gives: F = σb

(8.4)

This definition of the force per unit length acting on a dislocation can be extended to the general case of a dislocation moving in any direction in a crystal which is stressed internally or by external forces. To do this we use the result of the preceding section, that when a segment of dislocation line sweeps out an area of internal surface, the material on the positive side of that surface is displaced by b relative to the material on the negative side. The crystal is conceived to be cut at this surface. The force acting on one of the surfaces of the cut is calculated from the stress in the crystal, and the work done by this force on the crystal during the displacement is then calculated, the other surface being held fixed. The dislocation will be driven in such a direction that this work is negative. In the absence of external forces the energy of the crystal will then decrease (its self-stress will be reduced), and the magnitude of the force on the dislocation is defined by the decrease in the energy of the crystal when the dislocation moves a unit distance. If the dislocation is being driven by externally applied forces, this energy loss is made up by the work done on the crystal by the applied forces; the energy of the crystal itself does not change. The decrease in energy of a larger system which includes the device applying the force can then be considered to define the force acting on the dislocation, and identical equations are obtained. Using the sign convention of the preceding section, the force F acting on a unit area of the surface bounding the negative side of the cut is given by (see Section 6.3): Fi = σ ij n j

(8.5)

F =s ·n

(8.6)

or, in vector notation:

This force is exerted by the material on the positive side of the swept-out surface. The stress is s and n is a unit vector normal to the swept-out surface. The sense of n is given by l × d, where l is a unit vector parallel to the dislocation line and d is a unit vector in the direction of motion (Figure 8.9). Without loss of generality, we can take d perpendicular to l, since any motion of the dislocation parallel to itself sweeps out no area. Therefore: n = l×d

(8.7)

The movement of the dislocation displaces the surface bounding the negative side of the cut by −b if the opposite surface remains at rest, so that the work done on the crystal is: w = − (σ ⋅ n) ⋅ b

Kelly_c08.indd 250

(8.8)

11/30/2011 8:49:29 AM

Dislocations

251

which, because s is a symmetrical tensor, can be written in suffix notation (Appendix 1) as: w = − σ ij n j bi = − σ ji bi n j That is, in vector notation: w = − (σ ⋅ b) ⋅ n

(8.9)

The decrease in energy, −w, is given by the negative of this, so: − w = (σ ⋅ b) ⋅ (l × d) or: − w = (σ ⋅ b) × l ⋅ d

(8.10)

using the theorems on the scalar triple product of vectors (Appendix 1). We now have the work done by the crystal when a unit length of dislocation moves a unit distance in the form: −w = F⋅d

(8.11)

where d is a unit vector in the direction of motion. F is therefore the force per unit length acting on the dislocation, so: F = (σ ⋅ b) × l

(8.12)

The expression s · b represents the force per unit length acting on a plane normal to the Burgers vector, of area b. Since l is a unit vector parallel to the dislocation, we see that the force is always normal to the dislocation line. As an example of the application of this formula, consider the edge dislocation of Figure 8.12 in a region of general stress s. The stress may be the result of forces applied to the exterior of the crystal, or it may be a local self-stress.4 Suppose that the dislocation runs along the x2-axis and that its Burgers vector is in the direction −x1. It is evident that the glide plane is the plane containing these two directions. The traction on the surface whose outward normal is b is the result of components due to s11, s12 and s13 (Figure 8.12). The component of (s · b) due to s12 is parallel to l and so makes no contribution to (s · b) × l. The component s11 produces a traction in the direction of b and a component of force on the dislocation of magnitude s11b acting downwards, perpendicular to the glide plane. If s11 is negative, the force on the dislocation is directed upwards. This confirms the intuition that a compression along the x1-axis will tend to squeeze the extra plane out of the crystal, and that a tensile stress will tend to draw it downwards. The component of the force normal to the glide plane is called the climb force. The glide force acts in the glide plane, and in this case it is given by the shear component s13, which produces a force per unit length of magnitude s13b directed along Ox1. This is completely consistent with glide arising through volume-conserving shear 4

A self-stress, sometimes called an internal stress, is a stress that exists within a crystal that is free from externally applied forces.

Kelly_c08.indd 251

11/30/2011 8:49:29 AM

252

Crystallography and Crystal Defects

x3

l x2 s11

b

s12 s13

x1

Figure 8.12

processes (Chapter 7). Sometimes it is only important to know the glide force; that is, the component of force in the slip plane. As can be seen from Equation 8.8, the glide force on any dislocation is simply b times the component of the traction on the slip plane that acts in the slip direction. When an edge dislocation climbs under the influence of a stress, void or extra material is created, and it is intuitively clear that the climb will be brought to a halt if the extra material is allowed to accumulate, or if the void is not filled in. This leads to the idea of a ‘chemical’ force on a dislocation, due, for instance, to the absence of atoms on some of the sites in the surrounding lattice. To understand this force we must anticipate somewhat. It is shown in Chapter 10 that a crystal in equilibrium contains a certain number of empty atomic sites, called vacancies. To define the chemical force in this instance we write down the equilibrium concentration of vacancies in the presence of an edge dislocation under stress. When the concentration has this equilibrium value the dislocation has no tendency to create or annihilate vacancies by climbing, and so we define a chemical force equal and opposite to the climb force exerted by the stress. Suppose that when a vacancy is created by adding a lattice atom to the edge of the extra plane of an edge dislocation, a length ab of dislocation climbs by bb. Here a and b are constants of order unity which depend upon the structure of the crystal. Then when a vacancy is created, a stress that exerts a climb force F per unit length does work W 5 given by: W = Fαβ b2

(8.13)

Consequently, the equilibrium concentration of vacancies is increased from its value C0 in the absence of the climbing force6 to: ⎛ Fαβ b2 ⎞ C = C0 exp ⎜ ⎟ ⎝ kT ⎠

(8.14)

5 Here we are neglecting work that will be done by the hydrostatic component of the stress if the volume of the crystal changes when an atom is removed from an interior site. For the effect of this, see Weertman [2]. 6 See Section 10.1.

Kelly_c08.indd 252

11/30/2011 8:49:29 AM

Dislocations

253

where k is Boltzmann’s constant and T is absolute temperature. We define a chemical (or osmotic) force equal and opposite to F as being exerted by the concentration C of vacancies through the equation: −F = −

kT αβ b2

ln

C C0

(8.15)

In the absence of stress, a concentration C which is not equal to its equilibrium value C0 gives a chemical force that is not balanced by a force due to stress. The magnitude of this force is given by Equation 8.15. The dislocation will then climb upwards in Figure 8.12 if C/C0 > 1; that is, in the presence of a ‘supersaturation’ of vacancies. It is interesting to compare the magnitude of the ‘chemical stress’ F/b with the magnitude of a typical mechanical stress. Setting a = b = 1, mb3 ~5 eV,7 where m is the rigidity modulus and kT ≈ 0.025 eV at room temperature, we obtain: F C μ ~ ln b 200 C0

(8.16)

Many crystals cannot support so large an applied stress as m/200, so quite trifling supersaturations (C/C0 ~ 3) produce a force larger than that arising from any applied stress. Larger supersaturations, such as may be produced by quenching from close to the melting point, can cause small prismatic dislocation loops to be produced. These have been observed, for example, in aluminium [3,4].

8.4 The Distortion in a Dislocated Crystal It is important to know exactly how the structure of a crystal is distorted by a dislocation. This information is needed in tackling such problems as how dislocations interact with each other and with other lattice defects. An obvious way to approach the problem is to investigate an elastic continuum containing a dislocation. If a satisfactory solution is found for the dislocated continuum, the atoms in a crystal can then be assigned the displacements that are suffered by the corresponding points in the continuum. As a first approximation, isotropic elasticity can be assumed. For a screw dislocation in an isotropic continuum, the problem is simple enough for an intuitive approach to give the correct solution. We expect the displacement at any point to be parallel to the direction of the line of the dislocation. Further, because of the radial symmetry of the situation, a total displacement b must be spread out evenly over a circular path around the dislocation. This suggests a displacement uz given by: uz =

7

bθ 2π

(8.17)

The eV (electron volt) is a unit of energy equal to 1.602 × 10−19 J.

Kelly_c08.indd 253

11/30/2011 8:49:29 AM

254

Crystallography and Crystal Defects b

q

g

r

2πr

b

z

Figure 8.13

Strain due to a screw dislocation lying along the z-axis

If a path at a radial distance r from the dislocation is imagined to be straightened out, as in Figure 8.13, the shear strain is seen to be: γ zθ =

b 2π r

(8.18)

The non-zero stress component is the corresponding shear stress, given by Hooke’s law, Equation 6.85, as: σ zθ = σ θ z =

μb

2π r

(8.19)

where m is the shear modulus defined in Equation 6.82. It remains only to check that the stresses given by Equation 8.19 are such that every part of the body containing the dislocation is in equilibrium. Because the stress szq does not change with z or q, the opposite faces of all small elements, like the one shown in Figure 8.14, centred at a distance r away from the z-axis, are acted on by equal and opposite forces, so that the element is in equilibrium. Further, since szr, sq r and srr are everywhere zero, the surface of a cylinder around the dislocation is free of force. A difficulty with the shear strain given by Equation 8.18 is that it becomes infinite as r approaches zero. Since Hooke’s law applies only to small strains, it is usual to cut off the solution at a radius where the strains become large, say r ~ 5b. The material within a cylindrical surface of this radius is called the dislocation core. The core surface is in effect a boundary of the elastic body. The forces that would be exerted from point to point on this boundary by the core material are not known, but it is known that no net force can be exerted in any direction, nor any couple. This condition is satisfied by Equation 8.19, which gives a cylindrical surface that is entirely free of force. Equations 8.17 and 8.19 therefore give satisfactory displacements and stresses at distances greater than about 5b from a screw dislocation in an infinitely long isotropic cylinder. For a finite cylinder with free ends, the

Kelly_c08.indd 254

11/30/2011 8:49:29 AM

Dislocations

255

dz szq dr

szq

dq

z

Figure 8.14 Stress due to a screw dislocation along the z-axis acting on a small element of volume rdrdqdz at a distance r away from the z-axis

solution needs to be modified in order to remove the effect of the couple on the end surfaces that is produced by the stress szq. The problem of finding the displacements around other dislocations can be approached in the same way.8 A displacement function is sought that gives the required discontinuity of displacement in a circuit around the dislocation and in addition satisfies the equations of equilibrium. Expressed in Cartesian coordinates, with the dislocation lying along the x3-axis, the equations of equilibrium are the three equations: ∂σ i1 ∂x1

+

∂σ i 2 ∂x2

=0

(i = 1, 2, 3)

(8.20)

The stress sij can be expressed in terms of the derivatives of the components of displacement u1, u2 and u3 through Hooke’s law (Section 6.5). Because the stress and strain given by any displacement having the required discontinuity become infinite at the dislocation, it is further necessary to ensure that a cylinder of material containing the dislocation is in equilibrium, or in other words, that the force exerted on the core surface vanishes. The solution for an edge dislocation in an isotropic medium is more complicated than that for a screw. If the dislocation lies along the x3-axis with its Burgers vector parallel to x1, the displacements can be written in the forms [5]: u1 =

8

b 2π

⎡ −1 x2 ⎛ λ + μ ⎞ x1 x2 ⎤ + ⎢ tan ⎥ x1 ⎜⎝ λ + 2 μ ⎟⎠ x12 + x22 ⎦⎥ ⎣⎢

(8.21a)

The remainder of this section is somewhat advanced and can be omitted at a first reading.

Kelly_c08.indd 255

11/30/2011 8:49:30 AM

256

Crystallography and Crystal Defects

u2 =

b 2π

⎡ ⎛ λ + μ ⎞ x22 ⎤ μ ln x12 + x22 + ⎜ ⎢− ⎥ ⎝ λ + 2 μ ⎠⎟ x12 + x22 ⎥⎦ ⎢⎣ 2(λ + 2 μ )

(

)

(8.21b)

where l is the Lamé constant (Section 6.5). The first term in Equation 8.21a has the same form as the solution for a screw dislocation, and provides the necessary cyclic discontinuity in u1 equal to the Burgers vector b. The first term in u2, the displacement normal to the slip plane, is needed in order that the equations of Equilibrium 8.20 are satisfied. The second terms in Equations 8.21a and b are needed to make the core force vanish. The pattern produced when these displacements are imposed on a square array of points in the x1x2-plane is shown in Figure 8.5. The elastic constants used in Equations 8.21 to obtain Figure 8.5 were those of tungsten, which happens to be elastically isotropic, to a good approximation. A consideration of the relevant equations leading to Equations 8.21 shows that there is an element of choice in the constant of integration in the equations relating the displacements to the elastic strains. Results quoted elsewhere for these displacements [6–10] are the same, apart from differences in the choice of the constant of integration. The stresses which follow from the displacements given by Equations 8.21 are: σ 11 = − σ 22 =

μb

x2 (3 x12 + x22 )

2π (1 − ν ) ( x12 + x22 )2 μb

x2 ( x12 − x22 )

2π (1 − ν ) ( x12 + x22 )2

σ 33 = ν (σ 11 + σ 22 ) σ 12 =

μb

(8.22)

x1 ( x12 − x22 )

2π (1 − ν ) ( x12 + x22 )2

where n is Poisson’s ratio. The stresses and strains due to a mixed dislocation in an isotropic medium whose line makes an angle q with its Burgers vector can be obtained by simply adding the stresses and strains due to a screw dislocation of the Burgers vector b cos q to those due to an edge dislocation of the Burgers vector b sin q. This is because the terms in the stress fields of the screw and edge components are independent of one another. Tungsten, together with aluminium, is an exceptional crystal in being, elastically, almost isotropic. For most crystals, obtaining accurate values for the positions of atoms outside the core of a dislocation requires the use of the true elastic constants of the crystal, rather than the averaged values, which describe the isotropic behaviour of a polycrystal of the material. This means that the correct form of Hooke’s law must be used in converting Equations of Equilibrium 8.20 into equations in the displacements. In the general case, this introduces all nine terms of the type ∂2ui/∂xa∂xb into Equations of Equilibrium 8.20 (i = 1, 2, 3; a, b = 1, 2). The resultant mathematics is highly complex, requiring the solution of a sixth-order polynomial [10–12]. The cases that have been solved analytically are ones in which this number of terms is reduced because of symmetry. This requires not only that the crystal structure be of high symmetry but also that the dislocation lies in some special direction in

Kelly_c08.indd 256

11/30/2011 8:49:30 AM

Dislocations

257

x2 – [110]

r

θ x1

O

[001]

Figure 8.15

the crystal, such as along a two-fold axis of symmetry. For example, full solutions have been published for an edge dislocation along 〈001〉 in a cubic crystal, a screw normal to a mirror plane and a dislocation lying in the basal plane of a hexagonal crystal [13,14]. Yin et al. [15] have recently compared a number of approaches for numerical efficiency and accuracy to compute stresses, displacements and forces on finite lengths of arbitrarily oriented dislocations in anisotropic media. The simplest case is that of a screw dislocation lying normal to a mirror plane [13]. Then, if the x3-axis is chosen to be parallel to the dislocation, the elastic constants c′14, c′15, c′24, c′25, c′34, c′35, c′46 and c′56 vanish (see Table 6.2; primed elastic constants are constants referred to axes that are not chosen with a conventional relationship to the crystal axes) [10]. The displacement can be written in the form [10]: u3 = −

(c ′ c ′ − c45 ′ 2 )1/ 2 x2 b tan −1 44 55 2π c44 ′ x1 − c45 ′ x2

(8.23)

For a screw dislocation along 〈110〉 in a c.c.p. crystal, Equation 8.23 reduces to: u3 = −

A1/2 x2 b tan −1 2π x1

(8.24)

where the x1- and x2- axes are shown in Figure 8.15 and A is the anisotropy factor given by Equation 6.77: A=

2c44 c11 − c12

The anisotropy factor destroys the radial symmetry of the displacement, which is otherwise of the same form as in an isotropic medium. When A > 1, as it is for c.c.p. metals, the shear strain is greatest on the {110} plane; when A < 1, as it is for some alkali halides and some

Kelly_c08.indd 257

11/30/2011 8:49:30 AM

258

Crystallography and Crystal Defects

b.c.c. metals, the shear strain is greatest on the {100} plane. Because the shear modulus varies with orientation, a shear stress szr is introduced: σ zr =

c44 b(1 − A)sin θ cos θ 2π A1/ 2 r (cos2 θ + A sin 2 θ )

(8.25)

in addition to the shear stress szq, which has the same form as in the isotropic case, namely [13]: σ zθ =

c44 b 2π A1/ 2 r

(8.26)

8.5 Atom Positions Close to a Dislocation Although the solutions for dislocations in an elastic continuum can be used to assign displacements to the atoms around a dislocation in a crystal, these displacements are unlikely to be correct for atoms close to the dislocation, because the elastic continuum solutions may not be valid in this region of high strain. To determine the displacements in this core region of the dislocation, a detailed knowledge of the forces acting between atoms is needed. Atomistic simulations now enable these displacements to be determined using suitable interatomic potentials. Comprehensive reviews of progress in this area over the years can be found in the Dislocations in Solids series [16–18]. However, to convey the essential physical aspects of such displacements without recourse to such detailed simulations, our discussion here will be less rigorous. As a starting point, consider a simple cubic lattice and take the displacements for a screw dislocation given by Equation 8.17, treating it as an isotropic continuum: uz =

bθ 2π

If the position of the dislocation line is taken to be as in Figure 8.6 and q is taken as the angle measured anticlockwise from Sx1, which can be considered to be the trace of a plane on which the screw glides, the displacements of the atoms numbered 1 to 4, for example, are: b 3b 5b 7b , , , 8 8 8 8 respectively. The displacement across the slip plane Sx1 is: Δu = b −

bθ

(8.27)

π

No displacement has occurred across the slip plane to the far left of the dislocation (q = p), while the relative displacement is b to the far right (q = 0). Equation 8.27 can be written as: Δu = b −

Kelly_c08.indd 258

b π

tan −1

b b = b− π 2 x1

⎛π −1 2 x1 ⎞ ⎜⎝ 2 − tan b ⎟⎠

11/30/2011 8:49:30 AM

Dislocations

259

Δu b

–2

–1

0

Figure 8.16

1

2

x1 /b

Plot of Equation 8.28

or: Δu =

2x b b + tan −1 1 2 π b

(8.28)

This function is plotted in Figure 8.16. The distance on the slip plane over which the displacement lies between 14 and 34 of its extreme values is defined as the width of the dislocation on that plane. The width of the dislocation in Figure 8.16 is b, slightly more than the width of 0.75 b determined for the width of a screw dislocation core in aluminium in recent atomistic simulations [19]. Suppose now that we double the width of the dislocation by making Δu change with x1 according to the equation: Δu =

x b b + tan −1 1 2 π b

(8.29)

This is equivalent to giving the atoms the displacements that they would have, according to the symmetrical solution (8.17), if they were arranged on a tetragonal lattice with a spacing across the slip plane twice that within the plane. The displacements of the atoms 1 to 4 become approximately: b b 2b 5b , , , 6 3 3 6 The widened dislocation is shown in Figure 8.17. The shear strain in bonds 1–4 and 2–3 is twice that in the bonds 1–2 and 3–4. A similar situation would be expected in a real crystal if the bonds between the slip planes were weaker than those between atoms within a slip plane. A model which gives special consideration to the bonds across the slip plane is the Peierls dislocation [20]. In this model the crystal is supposed to be divided into two blocks at the slip plane, each of which is an elastic continuum. The atomic structure is taken into account only at the slip plane, where the two blocks join. A periodic force law is allowed to act between the rows of atoms immediately above the slip plane and those immediately below. For simplicity, a sine law is chosen:

Kelly_c08.indd 259

11/30/2011 8:49:30 AM

260

Crystallography and Crystal Defects S′ 4

3 2

1 4

3 2

l S

Figure 8.17 A screw dislocation of twice the width of the one shown in Figure 8.6

σ=

bμ 2π Δ u sin 2π a b

(8.30)

The spacing between the slip planes is a, so that Δu/a is the shear in the bond between two rows of atoms across the slip plane, while b is the atomic spacing within a slip plane. Equation 8.30 reduces to Hooke’s law at small strains; that is, at small values of Δu. A dislocation is made by straining the elastic blocks and then joining them at the slip plane. The restoring force acting between sheared rows of atoms according to Equation 8.30 tends to narrow the dislocation. The forces due to the elastic strains within the blocks tend to widen it. A balance is reached with a certain distribution of displacements. Either an edge or a screw dislocation can be made, although the model is more attractive for an edge dislocation, where there are large shear strains on a unique slip plane. The displacements across the slip plane of a Peierls screw are identical to those predicted by the elastic continuum solution (8.28). That is: Δu =

2x b b + tan −1 1 π 2 a

(8.31)

The displacements for a Peierls edge differ from those for an elastic edge dislocation and give: Δu =

2 x (1 − ν ) b b + tan −1 1 2 π a

(8.32)

The Peierls edge is wider than the screw by the factor 1/(1 − n), where n is Poisson’s ratio. As n increases towards its greatest possible value of 0.5, the resistance of the material to elastic shear decreases relative to its resistance to dilatation. An increase in the width of an edge dislocation as n increases therefore accords with the qualitative idea that if the atoms are hard, but shear over one another easily, as for metallic materials, then squeezing in the extra plane of atoms will spread the dislocation out over its slip plane. On the other hand, if there are strong directed bonds across the slip plane, their resistance to shear will lead to a narrow dislocation. Such directed bonds occur in covalent crystals like silicon.

Kelly_c08.indd 260

11/30/2011 8:49:30 AM

Dislocations

261

An important property which is controlled by the atom positions in the dislocation core is the force needed to start a straight dislocation moving in an otherwise perfect lattice. As the dislocation moves, the displacements around it will change, and in general the energy stored in the core will change slightly. Consequently, a force is exerted on the dislocation, given by: Fx = −

dE dx

(8.33)

where E is the energy due to the dislocation. The maximum value of this force is called the Peierls force, because it was first investigated by Peierls using a model of an edge dislocation [20]. The method can be briefly illustrated with the help of Figure 8.6, taking the dislocation S to be a Peierls screw. For any position of S on the plane Sx1 (Figure 8.6a), Equation 8.31 can be used to assign displacements to the atoms. The energy stored in the bonds across the slip planes, 2–3, 1–4 and so on, can then be summed as a function of the position of the dislocation. The energy sum E′ turns out to be a minimum for position S1 and a maximum for position S2 (Figure 8.6a), where the highly strained 1–4 bond makes a large contribution. At an intermediate position, dE′/dx1 can be shown to have a maximum value of the form: dE ′ ⎛ πa⎞ = Fp ≈ μ exp ⎜ − ⎟ ⎝ b⎠ dx1

(8.34)

This result has no quantitative significance because of the unrealistic nature of the model, and indeed it gives far too large a value for the force needed to move a dislocation in, say, a c.c.p. metal. The decrease in Fp with the parameter a, which on this model is equivalent to the width of the dislocation, is physically reasonable. As a dislocation becomes narrower, the change in displacement as it moves is distributed among fewer atoms. When the width is very small, a few core atoms have to make large jumps, for which there may be a substantial energy barrier, in order to move the dislocation by one atomic spacing.

8.6 The Interaction of Dislocations with One Another When a crystal is plastically deformed, some of its dislocations are lost as they glide to the surfaces of the crystal. However, dislocations must also be replenished during plastic flow, because a strain of 10% typically increases their density by 1012–1013m−2 (dislocation density is defined in Section 8.1). As the density of dislocations increases, their interaction with one another becomes important. For example, the stress needed to deform the crystal plastically increases and becomes controlled by the forces that dislocations exert on one another, rather than by the stress needed to move an isolated dislocation. A simple mechanism by which dislocations can multiply was suggested by Frank and Read [21]. Its operation requires only that a dislocation in a slip plane be pinned at two points. In Figure 8.18 the dislocation is pinned at the points x′y′ where it changes its plane. It is apparent from Figures 8.18a and b that this configuration could occur if a screw segment xy glided off its original slip plane to the position x′y′. This manoeuvre is called

Kelly_c08.indd 261

11/30/2011 8:49:30 AM

262

Crystallography and Crystal Defects (b) x′

(a)

x

x

y′ y

y

b

(d) (c) x′ x

x′ x

y′ y

y′ y

Figure 8.18

Dislocation multiplication

cross-slip. When the segment x′y′ changes back to a plane parallel to the original slip plane, it is easy to see that it can generate any number of expanding loops, using x′ and y′ as pivots. This variant of the Frank–Read mechanism is due to Koehler [22]. It allows slip to spread out sideways from a single active slip plane and so it can account for the commonly observed slip band, which is a set of very closely spaced parallel planes on which slip has occurred (see Figure 7.3). When slip occurs in bands, or even when it occurs more diffusely, dislocations on nearby parallel slip planes must on occasion come close to one another. Then the stress due to the one dislocation will exert a force on the other dislocation, according to Equation 8.12, where we substitute for s the stress due to one dislocation at the position of the other. Two special cases, parallel screws and parallel edges, will be briefly reviewed, assuming isotropic elasticity. Parallel screw dislocations a distance r apart experience a simple central force: F=

μb2

(8.35) 2π r The force per unit length, F, is repulsive when the screws are identical, so that their stress fields reinforce one another, and attractive when they are of opposite sign, so that their stress fields cancel as they come together. There is no position of equilibrium. Parallel edge dislocations, on the other hand, have two positions of equilibrium in respect of the component of force which lies in the slip plane. Since an edge dislocation would have to climb to move out of its slip plane, this is the only component of force that can cause an edge dislocation to move at low temperature. Its magnitude per unit length can be derived from Equations 8.22. It is convenient to write it in terms of polar coordinates as follows: Fg =

Kelly_c08.indd 262

μb 2

2π (1 − ν )r

cos θ (cos2 θ − sin 2 θ )

(8.36)

11/30/2011 8:49:30 AM

Dislocations

yo

263

r q x

0.3 Fg

0.2 0.1 0

1

2

3

4

5

6 x /y

o

– 0.1 – 0.2

Figure 8.19 Force between parallel edge dislocations on slip planes a distance y0 apart. The force is given in units of mb 2/2p(1 − n)y

The angle q is defined in Figure 8.19, in which Equation 8.36 is illustrated for edges of opposite sign. There is an unstable equilibrium at q = p/2 and a stable one at q = p/4, 3p/4. The force per unit length, Fm, which would be needed to push the parallel edges past one another on slip planes a distance y apart is: Fm =

μb2

8π (1 − ν ) y

(8.37)

Since yield stresses are typically in the range 10−3–10−4 m, edge dislocations of opposite sign are likely to become stuck against one another if they lie on slip planes which are a few hundred Å or less apart. Close pairs of dislocations of opposite sign are in fact commonly observed in deformed crystals; they are called dislocation dipoles. The forces acting between like edges are equal in magnitude but opposite in sign to those acting between unlike edges. The stable equilibrium therefore occurs at q = p /2. Two like edge dislocations are less likely to trap one another during glide than two unlike ones, because the applied stress moves them both in the same direction. However, the equilibrium configuration at q = p /2 becomes prominent when climb can occur. The component of force normal to the slip plane, the climb force, is given by: Fc =

μb2

2π (1 − ν )r

sin θ (1 + 2 cos2 θ )

(8.38)

This force is one of attraction between unlike edges and repulsion between like edges, for all q. If the temperature is high enough to allow climb, unlike edges from different slip planes annihilate one another, while any excess edges of the same sign which are left over arrange themselves in walls perpendicular to the slip plane. This is known as polygonization and occurs during the process of recovery when metals are annealed.

Kelly_c08.indd 263

11/30/2011 8:49:31 AM

264

Crystallography and Crystal Defects

P

r

d

b1 b2

Figure 8.20

Orthogonal screw dislocations, a perpendicular distance d apart

The elastic interaction of two dislocations in an anisotropic medium can differ quite significantly from the corresponding interaction in an isotropic medium. In copper, for example, two parallel screws lying along 〈110〉 in the same {111} slip plane exert forces on one another which are directed out of the slip plane, because of the shear stress srz given by Equation 8.25. Substitution of the appropriate constants into Equation 8.25 shows that the component of force normal to the slip plane is no less than 60% of the component of attraction or repulsion in the slip plane, which would be the sole component if the crystal of copper were elastically isotropic. Dislocations on intersecting slip planes also exert forces on one another due to their stress fields. For example, the stress field of a screw in an isotropic medium exerts a force on an orthogonal screw, given by: F=

μb1b2 d

2π r 2

(8.39)

where F is the force per unit length at the point P on the orthogonal screw, defined in Figure 8.20. The direction of F is normal to both dislocations. Its sign can be checked by comparing the shear stresses due to each screw at the midpoint of the shortest line joining them (the line of length d in Figure 8.20). The screws attract if the two stresses cancel one another and repel if they reinforce one another. Dislocations on intersecting slip planes interact in a second way, when they cut through one another. Because the material on one side of the surface swept out by a moving dislocation is displaced by the Burgers vector relative to the material on the other side, each dislocation acquires an extra length of line, equal in magnitude and direction to the Burgers vector of the other dislocation. If the extra length of line happens to lie on the plane on which the remainder of the dislocation is already gliding, it is called a kink. A kink can be eliminated immediately by glide. When the extra length of line does not lie on this plane, it is called a jog. When two orthogonal screws intersect, each acquires a jog which is a segment of edge dislocation. A jog of this type is shown in Figure 8.21, where the sign of the screw is indicated by means of the step that it produces on the surface of the crystal. If the jogged dislocation PQRS moves as a whole towards AD, the jog QR is forced to climb. Careful inspection of Figure 8.21 will show that a void is produced of volume QR times b times the distance moved. This void will take the form of a trail of vacant lattice sites. If PQRS moves in the opposite direction, towards BC, a trail of interstitial defects will be produced.

Kelly_c08.indd 264

11/30/2011 8:49:31 AM

Dislocations C

265

S R

B

D

Q P A

Figure 8.21

A third way in which two intersecting dislocations may interact with one another is that in certain circumstances they can come together and combine to form a new dislocation. This process is discussed in detail in the next chapter.

Problems 8.1 A screw dislocation of Burgers vector b passes straight through a crystal, meeting the front and back surfaces at 90°. Keeping this orientation, it moves so that its ends trace out circular paths and the dislocation line sweeps out a cylindrical surface. Describe the deformation produced by n revolutions of the dislocation. 8.2 Show how a pure edge dislocation loop, like that in Figure 8.11, can develop screw segments by gliding into a new shape. Hence show that it is geometrically possible for an edge dislocation loop to become a source for glide on any plane containing its Burgers vector. 8.3 An edge dislocation in a crystal of NaCl lies along [001] and its Burgers vector is 1 110 ] . If the dislocation is to be moved through a distance of 1 μm in the [100] direc2[ tion, calculate the volume of material that must be added to or subtracted from the edge of its extra plane, per metre of dislocation. 8.4 An edge dislocation in a crystal of NaCl lies along [001] and its Burgers vector is 1 110 ] . Calculate the glide force acting upon the dislocation under the action of a ten2[ sile stress s (a) when the tensile axis is [100] and (b) when the tensile axis is [111]. 8.5 A screw dislocation in a crystal of AgCl has the Burgers vector 12 [110 ] . If the dislocation could glide with equal ease on any plane, on which plane would it glide when under the action of a tensile stress (a) when the tensile axis is [100] and (b) when the tensile axis is [111]? 8.6 A screw dislocation lies along the axis of an isotropic cylinder of radius R. If the stress field were given by Equation 8.19, there would be forces acting on the end faces of the cylinder. Obtain an expression for the couple which would then be acting on the cylinder. (In a free cylinder the stress field would not be exactly given by Equation 8.19 but

Kelly_c08.indd 265

11/30/2011 8:49:31 AM

266

Crystallography and Crystal Defects

would contain an additional term, unimportant near the dislocation line, corresponding to a twisting of the cylinder, which neutralizes the couple implied by Equation 8.19 alone.) 8.7 From either Equations 8.21 or Equations 8.22 and 6.87, obtain the strain at a point directly above or below an edge dislocation (x1 = 0). Calculate the dilatations at points 5b above and 5b below an edge dislocation in aluminium. 8.8 Prepare a diagram of a plane which is normal to an edge dislocation in an isotropic medium, showing the lines in the plane on which one of the stress components s11, s22 and s12 vanishes (the dislocation lies along the x3-axis with its Burgers vector parallel to Ox1). Show the signs of the stresses in the various regions of the diagram. 8.9 Consider a screw dislocation in a c.c.p. crystal lying along [110]. Show (from Equation 8.24) that at equal distances from the dislocation, the shear strain on the – (11 0) plane that passes through the dislocation is A times the shear strain on the (001) plane that passes through the dislocation, where A = 2c44/(c11 − c12). 8.10 Obtain an expression for the width on the (001) plane of a screw dislocation lying along [110] in a sodium chloride crystal. Assume that the elastic continuum solution for the displacements (Equation 8.24) applies to all the atoms around the dislocation. 8.11 A cubic crystal is being stretched in a [100] direction. Its deformation is being pro– duced by edge dislocations lying parallel to [001] and gliding on (110) and (11 0) planes. If the density of these dislocations is r, the magnitude of the Burgers vector – of each one is b and their average velocity is V , determine the rate of increase of tensile strain of the crystal (= (1/l)(dl/dt), l = length of crystal). 8.12 Analyse the interaction between two edge dislocations whose lines are parallel to one another but whose Burgers vectors are orthogonal. Determine all positions of equilibrium with respect to glide forces and divide these into cases of stable, unstable and neutral equilibrium. 8.13 Find the total force experienced by an infinitely long screw dislocation of the Burgers vector b1 due to the presence of an infinitely long orthogonal screw dislocation of the Burgers vector b2. 8.14 In a crystal of sodium chloride, two orthogonal screw dislocations, of Burgers vectors – 1 110 ] and 12 [110] respectively, are being driven towards one another by a tensile stress 2[ along [100]. Demonstrate that each dislocation acquires a jog which produces interstitial defects if the dislocations continue to move under the action of the applied stress. 8.15 What is the minimum number of dislocations each with Burgers vector equal to the smallest lattice translation vector that can meet at a node in the following crystals: (a) b.c.c. iron, (b) diamond, (c) zinc and (d) caesium chloride? Under what conditions will the node be glissile?

Suggestions for Further Reading A.H. Cottrell (1953) Dislocations and Plastic Flow in Crystals, Oxford University Press, Oxford. J.P. Hirth and J. Lothe (1982) Theory of Dislocations, 2nd Edition, John Wiley and Sons, New York.

Kelly_c08.indd 266

11/30/2011 8:49:31 AM

Dislocations

267

D. Hull and D.J. Bacon (2011) Introduction to Dislocations, 5th Edition, Butterworth-Heinemann, Oxford. F.R.N. Nabarro (1987) Theory of Crystal Dislocations, Dover Press, Mineola, New York. W.T. Read (1953) Dislocations in Crystals, McGraw-Hill, New York. J.W. Steeds (1973) Introduction to Anisotropic Elastic Theory of Dislocations, Clarendon Press, Oxford. J. Weertman and J.R. Weertman (1992) Elementary Dislocation Theory, Oxford University Press, Oxford.

References [1] R. de Wit (1965) The direction of the force on a dislocation and the sign of the Burgers vector, Acta Metall., 13, 1210–1211. [2] J. Weertman (1965) The Peach–Koehler equation for the force on a dislocation modified for hydrostatic pressure, Phil. Mag., 11, 1217–1223. [3] P.B. Hirsch, J. Silcox, R.E. Smallman and K.H. Westmacott (1958) Dislocation loops in quenched aluminium, Phil. Mag., 3, 897–908. [4] J. Silcox and M.J. Whelan (1960) Direct observations of the annealing of prismatic dislocation loops and of climb of dislocations in quenched aluminium, Phil. Mag., 5, 1–23. [5] J.M. Burgers (1939) Some considerations on the fields of stress connected with dislocations in a regular crystal lattice. I., Proc. Konin. Ned. Akad. Wet., 42, 293–325. [6] J.S. Koehler (1941) On the dislocation theory of plastic deformation, Phys. Rev., 60, 397–410. [7] F.R.N. Nabarro (1952) Mathematical theory of stationary dislocations, Adv. Phys., 1, 269–394. [8] W.T. Read (1953) Dislocations in Crystals, McGraw-Hill, New York. [9] A.M. Kosevich (1979) Crystal dislocations and the theory of elasticity, in Dislocations in Solids, Volume 1 (edited by F.R.N. Nabarro), North-Holland, Amsterdam, pp. 33–141. [10] J.P. Hirth and J. Lothe (1982) Theory of Dislocations, 2nd Edition, John Wiley and Sons, New York. [11] J.W. Steeds (1973) Introduction to Anisotropic Elastic Theory of Dislocations, Clarendon Press, Oxford. [12] J.W. Steeds and J.R. Willis (1979) Dislocations in anisotropic media, in Dislocations in Solids, Volume 1 (edited by F.R.N. Nabarro) North-Holland, Amsterdam, pp. 143–165. [13] J.D. Eshelby, W.T. Read and W. Shockley (1953) Anisotropic elasticity with applications to dislocation theory, Acta Metall., 1, 251–259. [14] Y.T. Chou and J.D. Eshelby (1962) The energy and line tension of a dislocation in a hexagonal crystal, J. Mech. Phys. Solids, 10, 27–34. [15] J. Yin, D.M. Barnett and W. Cai (2010) Efficient computation of forces on dislocation segments in anisotropic elasticity, Modelling Simul. Mater. Sci. Eng., 18, art. 045013. [16] R. Bullough and V.K. Tewary (1979) Lattice theories of dislocations, in Dislocations in Solids, Volume 2 (edited by F.R.N. Nabarro), North-Holland, Amsterdam, pp. 1–65. [17] M.S. Duesbery (1989) The dislocation core and plasticity, in Dislocations in Solids, Volume 8 (edited by F.R.N. Nabarro) North-Holland, Amsterdam, pp. 67–173. [18] W. Cai, V.V. Bulatov, J. Chang, J. Li and S. Yip (2004) Dislocation core effects on mobility, in Dislocations in Solids, Volume 12 (edited by F.R.N. Nabarro and J.P. Hirth), Elsevier, Amsterdam, pp. 1–80. [19] G. Lu, N. Kioussis, V.V. Bulatov and E. Kaxiras (2001) Dislocation core properties of aluminium: a first-principles study, Mater. Sci. Eng. A, 309–310, 142–147. [20] R. Peierls (1940) The size of a dislocation, Proc. Phys. Soc., 52, 34–37. [21] F.C. Frank and W.T. Read (1950) Multiplication processes for slow moving dislocations, Phys. Rev., 79, 722–723. [22] J.S. Koehler (1952) The nature of work-hardening, Phys. Rev., 86, 52–59.

Kelly_c08.indd 267

11/30/2011 8:49:31 AM

9 Dislocations in Crystals 9.1 The Strain Energy of a Dislocation A considerable amount of strain energy is stored in the elastically distorted region around a dislocation line. The magnitude of the energy stored in an elastically strained region is always of the form 12 × (elastic modulus) × (strain)2, per unit volume (see Equation 6.60). Since the strain at a given point is proportional to the magnitude of the Burgers vector of the dislocation b, the total strain energy will be proportional to b2. To find the absolute magnitude of the energy stored, it is necessary to make a more detailed calculation. This can be done in two ways. In the first method, the energy stored in a small element of volume is found and an integration is performed. For a screw dislocation the appropriate element is a thin cylindrical shell of radius r, thickness dr, because the shear strain g within such a thin shell is constant (Equation 8.18): b 2π r

γ =

An elastically isotropic medium is assumed. The strain energy per unit length of shell is then: μb2 dE = ( 1 μγ 2 ) 2π r dr = dr 2 4π r

(9.1)

and so the energy per unit length of dislocation in the region from the core, radius r0, out to a radius R is: E=

∫

R

r0

μb2

4π r

dr

or: Crystallography and Crystal Defects, Second Edition. Anthony Kelly and Kevin M. Knowles. © 2012 John Wiley & Sons, Ltd. Published 2012 by John Wiley & Sons, Ltd.

Kelly_c09.indd 269

11/30/2011 6:17:38 PM

270

Crystallography and Crystal Defects

b

x2

x1

Figure 9.1

E=

⎛ R⎞ ln ⎜ ⎟ 4π r ⎝ r0 ⎠

μb2

(9.2)

To be exact, Equation 9.2 should be corrected to allow for the relaxation of stress at the free end surfaces of the cylinder. However, any uncertainty in the value of r0 makes this correction unimportant. The strain energy due to an edge dislocation is more easily calculated by a second method. Suppose that the dislocation is formed in initially unstrained material by making a cut from the surface of the material up to the site of the dislocation line, and then applying forces to the faces of the cut so as to give them a relative displacement of b. Then the work done by these forces equals the elastic energy stored around the completed dislocation. As the faces of the cut are displaced, the Burgers vector increases smoothly from zero to b. The work done in increasing the Burgers vector of unit length of dislocation from b to b + db is: dW = F ( β ) dβ

(9.3)

where F(b) is the force acting on one of the faces of the cut in the direction of b. This force is given by the stress field of the dislocation at the cut surface. For an edge dislocation which is made by cutting along the slip plane in a cylinder of radius R (Figure 9.1): F=

∫

R

r0

σ 12 dx1

(9.4)

The fact that only the stress on a single plane is involved gives this method an advantage over volume integration, when the stress field is complicated. From the forms of Equations 8.22, with x2 = 0 and the Burgers vector = b:

Kelly_c09.indd 270

11/30/2011 6:17:44 PM

Dislocations in Crystals

σ 12 =

μβ

2π (1 − ν )x1

271

(9.5)

and therefore: ⎛ R⎞ ln ⎜ ⎟ 2π (1 − ν ) ⎝ r0 ⎠ μβ

F=

(9.6)

The strain energy per unit length is then: E=W =

∫

b 0

F dβ =

⎛ R⎞ ln ⎜ ⎟ 4π (1 − ν ) ⎝ r0 ⎠ μb 2

(9.7)

In an isotropic medium, an edge dislocation has more elastic strain energy than a screw, in the ratio of 1:(1−n). For aluminium, n = 0.34 and so per unit length the edge dislocation has 1.5 times as much energy as the screw; for tungsten, n = 0.17 and the ratio is only 1.2. The strain due to a mixed dislocation, with a Burgers vector at an angle q to the dislocation line, is equal to the sum of the strains due to parallel edge and screw dislocations of Burgers vectors b sin q and b cos q, respectively. Therefore, the energy of a mixed dislocation is given by: E=

Kb2 ⎛ R ⎞ ln ⎜ ⎟ 4π ⎝ r0 ⎠

(9.8)

sin 2 θ + μ cos2 θ

(9.9)

where: K=

μ

1−ν

To estimate the absolute magnitude of the strain energy per unit length of dislocation line, it is sufficient to consider Equation 9.2: E=

⎛ R⎞ ln ⎜ ⎟ 4π ⎝ r0 ⎠

μb2

The difficulty in applying this equation is that the strain energy increases without limit as R increases. In a real crystal, either the surfaces of the crystal, or more probably other dislocations, will limit R. Fortunately, because of its logarithmic dependence on R, the magnitude of E is not very sensitive to the particular value of R which is assumed. For aluminium, which is approximately isotropic elastically, with m = 28 GPa, b = 2.86 × 10−10 m and an assumed r0 = b [1], the energy per unit length is 1.49 × 10−9 J m−1 when R is set at 1 μm, and 2.75 × 10−9 J m−1 when R is set at 1 mm. A value of 2 × 10−9 J m−1 corresponds to an energy per Å length of dislocation of 1.25 eV. This energy is large enough to ensure that a crystal containing a single dislocation is never in thermodynamic equilibrium. (Even at high temperatures the entropy introduced by a dislocation subtracts only a relatively

Kelly_c09.indd 271

11/30/2011 6:17:48 PM

272

Crystallography and Crystal Defects

b1

b3

b2

b1

q b2 b3

Figure 9.2

small amount from its energy, so that the free energy of a dislocated crystal of ordinary size is always greater than that of a perfect crystal.) To obtain the total energy of a dislocation, the energy stored within the dislocation core must be added to the energy given by Equation 9.8. The core energy can be roughly estimated in various ways, which agree in giving its order of magnitude as mb2/4p J m−1 [1,2]. For aluminium, this amounts to 0.1 eV per Å, considerably less than the energy stored outside the core. In a real crystal, the importance of the core energy lies less in its magnitude than in the variation of this magnitude as the dislocation glides through the crystal. If the core energy increases sharply as the dislocation moves from its position of minimum energy, its motion is strongly resisted (Section 8.5). It is always geometrically possible for two dislocations to combine to form a single dislocation, as shown in Figure 9.2. When this happens, the Burgers vector of the resultant dislocation, b3, is simply the vector sum of the Burgers vectors of the combining dislocations: b3 = b1 + b2

(9.10)

To determine whether such a reaction is energetically favourable, we must compare the energy of a crystal containing a dislocation of the Burgers vector b3 with that of a crystal containing two widely separated dislocations of the Burgers vectors b1 and b2. The former can be written as K3b32 and the latter as K1b12 + K2b22. Although it is evident from Equation 9.8 that the constants K1, K2 and K3 depend on the angles between the dislocation lines and their Burgers vectors, the difference between K3b32 and K1b12 + K2b22 is usually so large that the sign of K3b32 − (K1b12 + K2b22) is not affected by setting K1 = K2 = K3. Consequently, the sign of b32 − (b12 + b22) is a useful criterion for determining whether the reaction of two dislocations to form a third leads to a reduction in energy. Using this, a reduction will occur if: b32 < b12 + b22

Kelly_c09.indd 272

(9.11)

11/30/2011 6:17:55 PM

Dislocations in Crystals

273

This rapid test for deciding whether two dislocations will react is known as Frank’s rule [3]. It can also be expressed in terms of the angle q between b1 and b2 (Figure 9.2). If q < 90°, the dislocations will not react; if q > 90° they will attract and react with one another. The same rule can be applied in reverse to decide whether a dislocation of the Burgers vector b3 is stable. If two lattice vectors summing to b3 and making an angle q < 90° with each other are available, the dislocation will dissociate into two dislocations with these vectors as Burgers vectors. The rule is obviously most reliable when q is far from 90°. It follows from Frank’s rule that most dislocations other than those with the shortest lattice vector as the Burgers vector are unstable. For example, a dislocation with a Burgers vector 12 211 in a c.c.p. crystal would decompose into two 12 011 dislocations: 1 [211] → 1 [110] + 1 [101] 2 2 2

(9.12)

However, it sometimes happens that a dislocation whose Burgers vector is greater than the least lattice vector cannot decompose spontaneously. An example is the [100] dislocation in a b.c.c. crystal. Although the 12 111 dislocation has a smaller energy, Frank’s rule predicts that the decomposition: [100] → 1 [11 1] + 1 [111] 2 2

(9.13)

will not occur, and that no other geometrically possible decomposition is favourable energetically. The Burgers vectors that are definitely stable in various lattices are listed in Table 9.1. Doubtful cases in which the vector is the sum of two orthogonal vectors (q = 90°) are omitted. The fact that the dislocation with the smallest Burgers vector has the least elastic energy fits in well with the observation that the slip direction is almost always that of the shortest lattice translation vector in the crystal (Table 7.1). It is natural to enquire whether the observed slip planes are those on which a dislocation of minimum Burgers vector has the smallest elastic energy, when the elastic anisotropy of the crystal is taken into account. The elastic energy per unit length for an undissociated dislocation in an anisotropic medium is given by: E=

K ′b2 ⎛ R ⎞ ln ⎜ ⎟ 4π ⎝ r0 ⎠

(9.14)

where K′ depends on the elastic constants. Foreman has computed the energy factor K′ in a number of cases [4]. In copper, for example, an edge dislocation of the 12 110 Burgers vector has a lower elastic energy when it lies in a {110} plane (K′ = 64.5 GPa) than when it lies in a {111} plane (K′ = 74.5 GPa). Since the observed slip plane is {111}, it appears that the elastic energy alone does not determine which slip plane operates. In order to understand the choice of slip plane it is evidently necessary to take account of the atomic structure of the crystal (see also Section 7.1).

Kelly_c09.indd 273

11/30/2011 6:17:57 PM

274

Crystallography and Crystal Defects

Table 9.1

Definitely stable dislocations in some Bravais lattices

Lattice

Burgers vector

Number of equivalent vectors

Square of Burgers vector

Simple cubic

〈100〉

6

a2

B.c.c.

1 111 2 〈100〉

8

3a2/4

6

a2

C.c.p. Hexagonal

1 110 2 1 1120 3 〈0001〉

12

a2/2

6

a2

2

c2

6

a2

〈100〉 – 〈110〉 – 〈111〉

6

4a2 sin2 a/2

6

a2(1 + 4 sin2 a/2)

〈100〉

6

a2

〈110〉

6

4a2 cos2 a/2

〈111〉

2

9a2(1− 4 sin2 α / 2)

Simple tetragonal

〈100〉

4

a2

2

c2

Body-centred tetragonal

〈001〉 1 111 2

8

a2/2 + c2/4

〈100〉

4

a2

〈001〉

2

c2

1 111 2 〈100〉

8

a2/2 + c2/4

4

a2

Rhombohedral a < 90° Rhombohedral a > 90°

c/a < 2

Body-centred tetragonal c/a > 2

3

The fact that a dislocation line has a certain amount of energy per unit length associated with it causes it to try to shorten itself, or in other words, it gives it a line tension. It is not easy to define this line tension precisely because the energy is not concentrated at the line itself but is contained in its far-reaching strain field. Let us consider the tendency of a circular dislocation loop of radius r to shrink. To prevent it from shrinking, a radial force Fr per unit length must be applied, given by the condition that the energy change accompanying an infinitesimal contraction of the loop must vanish. Therefore: Fr 2π r dr = E 2π dr

(9.15)

or: Fr =

Kelly_c09.indd 274

E r

11/30/2011 6:18:06 PM

Dislocations in Crystals

275

T

Fr rdq π dq 2 2

r

dq T

Figure 9.3

where E is the energy per unit length of the dislocation loop. Since the strains due to the opposite sides of the loop cancel one another at distances that are large compared to r, we can determine E approximately by setting R = r in Equation 9.2: E≈

⎛r⎞ ln ⎜ ⎟ 4π ⎝ r0 ⎠

μb2

(9.16)

If we consider a small segment of the loop, shown in Figure 9.3, subtending an angle dq at the centre of the loop, we see that to keep this segment in equilibrium its ends must experience a tension T given by setting the sum of radial forces equal to zero: 2T sin

dθ = Fr r dθ 2

(9.17)

Since dq is very small, we therefore have from Equations 9.15 and 9.17: T =E

(9.18)

We may extend this result with the aid of Equation 9.16 to say that the line tension of a dislocation bowed to a radius of curvature r is approximately: T≈

⎛ ρ⎞ ln ⎜ ⎟ 4π ⎝ r0 ⎠

μb2

(9.19)

With r ≈ 500r0, substitution into Equation 9.19 gives the value of T ≈ 0.5 μb2, which is often used as the value of the line tension of a dislocation in rough calculations. A diagram which helps in the calculation of the stress needed to extrude a dislocation between obstacles a distance l apart is shown in Figure 9.4. The radial force on the dislocation is supplied by a shear stress t on the slip plane, parallel to the Burgers vector. From Equation 8.4: Fr = τ b

Kelly_c09.indd 275

(9.20)

11/30/2011 6:18:17 PM

276

Crystallography and Crystal Defects

Fr

l

r

Figure 9.4

Using Equations 9.15 and 9.18, if the radius of curvature of the dislocation line is r: τ=

T bρ

(9.21)

or, setting T = 0.5 mb2: τ=

0.5 μb

ρ

(9.22)

Since the minimum value of r is 0.51, occurring when the dislocation has been bowed out to a semicircle, the stress required to force the dislocation between the obstacles is given by: τ≈

μb l

(9.23)

It is apparent from this equation that this is also the shear stress needed to operate a Frank– Read source whose pinning points are a distance l apart. An interesting improvement to Equation 9.19 can easily be made by allowing for the fact that the strain energy of a dislocation varies with the angle q between its line and its Burgers vector. (For an isotropic medium, this variation is given by Equation 9.9.) As a consequence, if the equilibrium of an isolated segment of dislocation is considered, not only must a force E be applied to its ends to stop it shrinking, but also a couple Γ per unit length must be applied to it to stop it turning into an orientation of lower energy. The value of Γ is found by considering an infinitesimal rotation dq of the segment from its equilibrium position. Setting the energy change equal to zero: Γ dθ − dE = 0

or: Γ=

dE dθ

(9.24)

As the dislocation curves through the infinitesimal angle dq, the couple per unit length acting upon it changes by (d2E/dq 2)dq. This results in unbalanced radial forces acting on

Kelly_c09.indd 276

11/30/2011 6:18:24 PM

Dislocations in Crystals

277

dE – d2E dq dq dq 2 2

Fr dS

E dS r

E

dE + d2E dq dq dq 2 2

dq

q

Figure 9.5

the ends of a curved segment of length dS, as shown by Figure 9.5. The total radial force per unit length needed to keep the dislocation bowed out is now given by: Fr dS = E dθ +

d2 E dθ 2

dθ

or: Fr =

E ρ

+

1 d2 E ρ dθ 2

(9.25)

If the line tension T is defined by the equation: Fr =

T ρ

(9.26)

then, from Equation 9.25, T is given by: T=E+

d2 E dθ 2

(9.27)

Substitution of Equation 9.9 into Equation 9.27 shows that a screw dislocation in an isotropic material is much stiffer than an edge, even though the edge has the greater elastic energy. Physically, this is because in order to bend a screw dislocation, it must be given some edge character, of relatively high energy. In aluminium, which as we have already noted is approximately isotropic elastically, n = 0.34, so that the screw dislocation is four times as stiff as the edge.

9.2

Stacking Faults and Partial Dislocations

So far, it has been assumed that the smallest Burgers vector that a crystal dislocation may possess is the shortest lattice vector. Although such a dislocation could reduce the elastic strain energy by dissociating into two dislocations with smaller Burgers vectors, this would

Kelly_c09.indd 277

11/30/2011 6:18:30 PM

278

Crystallography and Crystal Defects

create a fault in the crystal structure, which, in general, would have a high energy. In certain special cases, however, the fault has a rather small energy. When this is so, the dislocation does indeed dissociate into two dislocations, called partial dislocations or, briefly, partials, which leave a planar fault between them as they move apart. The mutual repulsion of the partials due to their stress fields decreases as the partials separate, but the attractive force exerted by the surface tension of the fault remains constant. An equilibrium separation is therefore reached at which the forces of repulsion and attraction balance. It is now well established that 〈110〉 dislocations in c.c.p. metals dissociate into partials on the {111} slip plane. The fault that lies between the partials is a fault in the stacking sequence of the {111} planes, which does not change the relative positions of atoms that are nearest neighbours of one another. The production of this stacking fault can best be visualized with the aid of sheets of closely packed balls, stacked one on top of another (Section 3.2). By sliding an upper block of sheets through a/6 〈211〉 over those underneath, the so-called intrinsic stacking fault is produced (Figure 9.6). For example, if the second ABC block in the sequence ABC ABC is slid over the first, the sequence becomes ABCBCA… The sheets at the fault are now in the sequence BCBC, which, if continued, produces a close-packed hexagonal structure. Such a fault occurs when the 12 110 dislocation dissociates into 61 211 dislocations, which are called Shockley partials or Heidenreich–Shockley partials [5]: − − − 1 [011] → 1 [112] + 1 [1 21] 2 6 6

(9.28)

for dissociation of the 12 [01 1] dislocation on the (111) plane. The pattern of atoms at the (111) slip plane around a 12 [01 1] 60° dislocation that has dissociated into Shockley partials is shown in Figure 9.6. (For simplicity in drawing, the partials are shown to be very narrow; in a real crystal they would be wider.) The separation of the Shockley partials is determined by the energy per unit area, g , of the stacking fault between them. The fault draws the partials together with a force g per unit length, so that the equilibrium separation r is given by: G =γ r

(9.29)

where the elastic repulsion factor G can be calculated. Assuming isotropic elasticity, the screw component of the first partial, b1 cos q1, gives a shear stress on the slip plane: σ 23 =

μb1 cos θ1

2π r

(9.30)

where Ox2 is normal to the slip plane, Ox3 is parallel to the dislocations and q1 is the angle between the partial dislocation line and its Burgers vector. From Equations 8.22, the edge component gives the stress: σ 12 =

Kelly_c09.indd 278

μb1 sin θ1 2π (1 − v)r

(9.31)

11/30/2011 6:18:35 PM

Dislocations in Crystals

B

B

B

B

C

B

B

B

1 [121] 6 1 [211] 6

1 2 [011]

l

Figure 9.6 partials

B

B

B

C

C

C

B

C

C

B

B

279

1 b1 = 6 [112]

l

b2 = 16 [121]

Dislocation on a (111) plane of a c.c.p. metal which has split into two Shockley

The component of the traction on the slip plane in the direction of the Burgers vector of the second partial is given by:1 τ = σ 23 cos θ 2 + σ 12 sin θ 2

(9.32)

Since, by Section 8.3, G = t b2, it follows that: G=

μb1b2 ⎛ sin θ1 sin θ 2 ⎞ cos θ1 cos θ 2 + ⎜ ⎟⎠ 2π ⎝ 1−ν

(9.33)

The substitution of typical values for the constants in Equation 9.33 shows that a relatively wide separation of the partials of the order of 100 Å occurs only when the stacking fault energy is as low as 10 mJ m−2. Most c.c.p. metals and alloys have a higher stacking fault energy than this, so the separation of partials will only be seen in the transmission electron microscope using weak beam imaging conditions [6]. The remaining sections of this chapter are devoted to the study of dislocations in specific crystal structures.

1 Care must be taken to measure q1 and q2, the angles between the partial dislocation lines and their Burgers vectors, in the same sense.

Kelly_c09.indd 279

11/30/2011 6:18:44 PM

280

Crystallography and Crystal Defects

9.3

Dislocations in C.C.P. Metals

The 〈110〉 slip direction of c.c.p. metals is easy to understand, because 12 110 is the shortest lattice vector. The {111} slip plane is the plane on which a ‘perfect’ dislocation with a 1 110 Burgers vector may split into two Shockley partial dislocations, as described in 2 Section 9.2. The equilibrium separation of the two partials is determined by the energy of the stacking fault between them. The lower the stacking fault energy, the wider the split and the more rigorously should slip be confined to a particular {111} plane. The stacking fault energy is therefore a property of great physical importance as it determines the propensity of materials to twin and to cross-slip; unfortunately, it is also very difficult to measure accurately. Various values are listed in Table 9.2. The production of a stacking fault during slip is effectively illustrated by a rigid ball model, such as that shown in Figure 9.6. In this model, the slip path that requires the least ‘riding up’ of the balls follows a zigzag route along the valleys in the {111} surface, in two alternating 〈112〉 directions. The displacements along 〈112〉 alternately create and remove a stacking fault. From inspection of this model, one might wrongly conclude that only one type of stacking fault could occur on {111}. In particular, the stacking fault that would be obtained by interchanging the positions of the two partials in Figure 9.6 appears at first to be impossible, since it seems to involve A–A stacking, with a large ride-up of the balls when the leading dislocation advances. However, this conclusion can be modified if the necessary displacements are spread over two successive {111} planes. For example, at the position of the dislocation on the left of Figure 9.6, starting with a perfect crystal, a displacement 61 [211] of all the balls above the bottom {111} layer to the right of this position, followed by a displacement 61 [121] of all the balls above the next {111} layer, produces a net 61 [1 1 2] displacement without violating nearest-neighbour relationships. Formally, the partial dislocation then consists of two Shockley partials, 61 [2 1 1] and 61 [1 21] , on adjacent planes, but except at its core the dislocation cannot be distinguished from a single 1 [112] Shockley partial. 6 Therefore, by spreading the displacements over two planes, the 61 [112] Shockley partial can be made the leading partial for glide from left to right in Figure 9.6. When an interchange of the order of the partials is accomplished in this way, they are separated by a ‘double’ stacking fault, which is called an extrinsic fault. The energy of this fault is expected to be slightly higher than that of the intrinsic (single) fault. Consequently, the form of splitting shown in Figure 9.6 is believed to be the usual one. The distinction between the structures of intrinsic and extrinsic stacking faults can be neatly displayed by a notation due to Frank [12]. When a close-packed plane is stacked upon the plane beneath according to a pair in the sequence ABC…, the stacking of that plane is depicted by a triangle Δ. When a plane is stacked so that its relation to the plane beneath it is a pair in the reverse sequence BAC…, its stacking is then depicted by an inverted triangle ∇ (pronounced nabla). These symbols are derived from the stacking of balls – they represent the orientation of the triangles of balls onto which the balls in the next layer are stacked. The c.c.p. structure is then shown as ΔΔΔΔ and the h.c.p. structure as Δ∇Δ∇ … The intrinsic stacking fault is ΔΔ∇ΔΔΔ, while the extrinsic stacking fault is

Kelly_c09.indd 280

11/30/2011 6:18:47 PM

Dislocations in Crystals

281

Table 9.2 The stacking fault energies of c.c.p. metals Metal Ag Al Au Cu Ni

(a)

Stacking fault energy (mJ m−2)

Ref.

16 135 32 41 120–130

[7] [8] [9] [7,10] [11]

(b) C

C

B

B

A C B

A B

B A C B

A

A

A

C

C

C

B A C A B A C

Figure 9.7 (a) Faulted vacancy loop in a c.c.p. metal, showing traces of the (111) planes in a plane normal to the loop. (b) Extra atom loop

ΔΔ∇∇ΔΔ, emphasizing that the extrinsic fault is equivalent to two intrinsic faults on adjacent planes. It is possible to produce stacking faults by means other than slip on the close-packed plane. An intrinsic stacking fault is produced by removing part of a {111} layer of atoms, as shown in Figure 9.7a, provided that the gap is then closed directly, without any shear parallel to the {111} plane. Physically, this may happen when excess vacancies collect together on a {111} plane. Squeezing in a piece of an extra {111} layer creates an extrinsic fault, as shown in Figure 9.7b. The faults shown in Figure 9.7 are both bounded by partial dislocations whose Burgers vectors are normal to the {111} plane and are of the magnitude of the spacing of these planes; that is, 13 111 . In distinction from Shockley partials, these partials could glide only on surfaces that are normal to the usual {111} slip plane; if they did so they would leave a high-energy stacking fault behind them. They are called Frank partials or, because of their immobility, Frank sessiles. Although a stacking fault must be bounded by a partial dislocation, or end at a surface, it is now clear that the Burgers vector of the partial is not uniquely determined by the type of fault. In a given case, any lattice vector may be added to the Burgers vector of the partial without affecting the fault. For example, an intrinsic fault on (111) bounded by a

Kelly_c09.indd 281

11/30/2011 6:18:57 PM

282

Crystallography and Crystal Defects (a)

[001]

D

(b)

A C

D

b A

C B

[010]

d g

a [100]

D

B

D

Figure 9.8 Thompson’s tetrahedron. (After Thompson [13]. Reproduced by permission of the Institute of Physics and Physical Society.)

1 [11 2] 6 1 [2 11] 6

Shockley partial might equally well be bounded by two other Shockley partials, or 61 [121] . Thus: − 1 [ −211] = 1 [112] + 6 6 − − 1 [121] = 1 [112] + 6 6

− 1 [101] 2 − 1 [011] 2

(9.34) (9.35)

or, by the Frank partial with the Burgers vector 13 [1− −− 1 1] : −− − 1 1 [1 1 −− 3 1 1] = 6 [112] + 2 [1 1 0]

(9.36)

Before going on to consider reactions between dislocations in c.c.p. metal crystals, it will be helpful to introduce a device known as Thompson’s tetrahedron [13]. This gives a picture of various Burgers vectors in relation to the four {111} planes, which can be chosen to form the four faces of a tetrahedron. This tetrahedron and its relation to the crystal structure is shown in Figure 9.8a; the four faces of the tetrahedron, when they are opened out from the vertex D, are shown in Figure 9.8b. The lettering of the various points is conventional and follows Thompson’s original paper.2 An edge of the tetrahedron, such as CB, represents the Burgers vector of a perfect dislocation, 12 110 . Vectors given by Greek–Roman letter combinations such as d C represent Shockley partials, except when the Greek and Roman letters are in the same position in their respective alphabets, such as g C, which indicates a Frank partial.

2

Kelly_c09.indd 282

An alternative convention would be to letter the tetrahedron as the mirror image of Figure 9.8a.

11/30/2011 6:18:59 PM

Dislocations in Crystals

283

D

1 – [110] 2 Perfect

1 – [111] 3 Frank

d

1 – [112] 6 Shockley

B

Figure 9.9

The reaction between a Frank partial, a Shockley partial and a perfect dislocation given by Equation 9.36 becomes, in Thompson’s notation: δ D = δ B + BD

The relationship between these three Burgers vectors is shown in Figure 9.9. This reaction has some interesting applications. The stacking fault within the ‘vacancy loop’ of Figure 9.7a can be removed if the Frank dislocation decomposes according to Equation 9.36 and if then its Shockley component shrinks to nothing by gliding in the plane of the loop. This removes the stacking fault at the expense of an increase in elastic energy due to the − −− increase in the Burgers vector of the loop from 13 [1 1 1] to 12 [1 1 0] . In comparing the energies of faulted and unfaulted loops, allowance must be made for the shortening of the –– unfaulted loop when it glides into a (1 1 0) orientation normal to its Burgers vector. The unfaulted loop is favoured when the stacking fault energy is high and also when the loop is large, because the energy gained by destroying the fault is proportional to the area of the unfaulted region, whereas the extra elastic energy is approximately proportional to its perimeter. Another application is to the possible dissociation of a perfect dislocation into a Shockley partial and a Frank partial: BD → Bδ + δ D For example: 1 [1 10] → 1 [1 12] + 1 [1 1 1] 2 3 6

Kelly_c09.indd 283

(9.37)

11/30/2011 6:19:08 PM

284

Crystallography and Crystal Defects

l

l

Cd

dB

Figure 9.10

Since the Burgers vectors of these two partials are orthogonal, and since a stacking fault would have to be created between them, this dissociation does not ordinarily occur. It may occur in special cases, as when the Shockley components from the two members of a perfect dislocation dipole can annihilate one another, leaving behind a Frank dipole. This reaction is simply the reverse of the unfaulting of a prismatic loop described above. In order to define the sense of the Burgers vector of a dislocation, when it is written in Thompson’s notation it is necessary to introduce a convention that will assign a sense to the slip displacement signified by the symbol d C, for instance. The following convention can be used. The sense of the slip displacement signified by d C is defined as follows. The observer looks at the slip plane ABC from outside the tetrahedron; that is, with the apex D pointing away from him or her (Figure 9.8a). Then the atoms above the slip plane ABC closest to the observer are displaced by d C. Referring to the crystal structure, it is clear that the displacements dA, d B and d C produce an intrinsic stacking fault, whereas Ad, Bd and Cd produce an extrinsic fault. The dissociation of the perfect dislocation CB into Shockley partials on ABC can be written as: CB → Cδ + δ B

(9.38)

The Burgers vectors of the partials in the Thompson notation are then as shown in Figure 9.10, according to the FS/RH convention. (The line vectors have been chosen to run down the page, so that the observer looks in the negative line direction, in order to match the figure with the logical form of Equation 9.38.) Reversing the order of the partials would produce an extrinsic fault between them. The order of the Shockley partials is an important factor in dislocation reactions. The only reaction between perfect dislocations that definitely leads to a reduction in energy is of the type: CB + BA → CA

Kelly_c09.indd 284

(9.39)

11/30/2011 6:19:15 PM

Dislocations in Crystals (a)

p CB

BA q

(b)

(c) BA

CB

BA

CB

r

CA

CB

BA

BA

CB

CB BA

s

285

BA

CB

Figure 9.11 Reaction of two dislocations on a common slip plane. The dislocations are assumed to be pinned at the points p, q, r and s

Bd

dB

dA

Cd

Cd

l

dA

dB

Bd dA

Figure 9.12

Cd

Same reaction as Figure 9.11 but showing splitting into partials

If the dislocations of Burgers vectors BA and CB meet on their common slip plane, they will react over a certain length, forming two nodes (Figure 9.11). It is apparent from a consideration of Figure 9.12 that the nodes will have different structures, because of the sequence of the Shockley partials (it is assumed that only intrinsic faults occur). Alternate expanded and contracted nodes have been seen, in stainless steel, for example [14]. The same reaction (9.39) can also occur when the dislocations are on different slip planes. For example, suppose that dislocations CB and BA lie on the planes opposite vertices A and C respectively, and let their lines lie parallel to the intersection of these planes, BD, as they glide towards one another. This event is likely to occur during the later stages of the tensile deformation of a crystal, because it corresponds to the intersection of primary and conjugate slip (Section 7.4). If the two dislocations on the {111} planes are dissociated into Shockley partials, as shown in Figure 9.13, and if they come together in such a way that just before they meet their stacking faults make an acute angle (cos−1(1/3) = 70.53°) with one another, the leading partials aB and Bg will react to form a new partial along BD:

Kelly_c09.indd 285

11/30/2011 6:19:17 PM

286

Crystallography and Crystal Defects (a)

(b)

D

plane CBD

plane ABD

Ca

gA

b A

C d g

a D

Ca 1

aB

B

D

gA Bg

1

ag

Figure 9.13 Lomer–Cottrell lock

α B + Bγ → αγ

1 [1 2 1] + 1 [2 1 1] → 1 [1 1 0] 6 6 6

(9.40)

The edge dislocation ag is called a stair-rod, a name suggested to Thompson by Nabarro (quoted by Thompson in a footnote in [13]), from the way in which it joins two stacking faults at a bend rather like a stair rod holding down a stair carpet. The whole configuration is called either a Lomer–Cottrell lock or a Cottrell–Lomer lock [15,16]; here, we shall adopt the former terminology. Since it cannot glide, it is an important obstacle to other dislocations. The stair-rod dislocation of the type ag can also be produced by the dissociation of a Frank partial: α A → αγ + γ A

1 [1 11] → 1 [1 1 0] + 1 [1 1 2] 3 6 6

(9.41)

This reaction makes it possible to understand the small tetrahedra of stacking faults that can be produced experimentally by quenching gold from near its melting point to room temperature, and then ageing at 100 °C [17].3 Imagine that the excess vacancies which are trapped by the quench first form a Frank loop similar to that shown in Figure 9.7a. Let the loop be a triangle, with sides along the 〈110〉 directions AB, BC, CA. Each side can then dissociate on a different {111} plane, as shown in Figure 9.14. The Shockley dislocations produced by the dissociations attract one another and react at the intersections of the {111} planes to form stair-rod dislocations. The final product is a tetrahedron whose faces are intrinsic stacking faults and whose edges are stair-rod dislocations. Each edge of the tetrahedron is exactly like the corner of a Lomer–Cottrell lock. The formation of the tetrahedron decreases the elastic energy at the expense of additional stacking fault energy.

3 Ageing means holding at a constant temperature for a period of time, usually in order to allow some change in the structure of the material to occur.

Kelly_c09.indd 286

11/30/2011 6:19:18 PM

Dislocations in Crystals (a)

(b)

D

287

D

ag bγ gD

B aD

B A

bD

da

l

db

C

Figure 9.14

A

ab

da db

l

dg

dg

C

Formation of a stacking fault tetrahedron from a Frank vacancy loop

Ba

Ab ab/ DC

Figure 9.15

Hirth lock

The 61 110 dislocation is one of four possible stable stair rods. Other dislocations at an acute-angle bend can be derived by adding lattice vectors to 61 [110] . The only resultant which is stable, according to Frank’s rule, is 13 [1 1 0] , formed by adding 12 [1 1 0] . One of the interesting occurrences that would produce an obtuse-angle stacking fault bend is the reaction of the leading partials of the dislocations BD on the plane opposite the vertex A and AC on the plane opposite the vertex B: BD → Bα + α D AC → Aβ + β C

(9.42)

1 [2 1 1] + 1 [2 11] → 1 [0 1 0] 3 6 6

(9.43)

The resulting configuration, shown in Figure 9.15, is called the Hirth lock [18,19], even though, as Nabarro [20] notes in his book on p. 220, it appears in a tabulation given by Friedel [21]. In Thompson’s notation, Equation 9.43 may be written as: α D + β C → αβ /DC

Kelly_c09.indd 287

(9.44)

11/30/2011 6:19:20 PM

288

Crystallography and Crystal Defects Table 9.3

Dislocations in c.c.p. metals Burgers vector b

Name of dislocation Indices

Relative b2

Thompson notation

Perfect

1 110 2

AB

1

Shockley

1 211 6

Ad

1 3

Frank

1 110 3

Aa

2 3

Thompson stair-rod

1 6 1 3 1 3 1 6

110

ad

110

—

100

da/CB

310

—

1 9 4 9 2 9 5 9

Acute stair-rod Obtuse stair-rod Obtuse stair-rod

The 13 0 1 0 vector denoted by ab/DC is in the direction of the line joining the point bisecting ab to the point bisecting DC and has twice the magnitude of this line. Some of the properties of dislocations in c.c.p. metals are summarized in Table 9.3.

9.4

Dislocations in the Rock Salt Structure

The dislocations that have been identified in crystals of the rock salt (NaCl) structure have a 12 110 Burgers vector, as would be expected (Table 9.1). The slip plane is usually {110}, but not always (Table 7.1). When slip on {110} is examined, it is impossible to find a stacking fault that looks as though it might have a low energy and could serve as the halfway stage of an indirect 1 110 displacement. Therefore, the 12 110 dislocation is not expected to split into 2 – partials on {110}. The fact that only perfect dislocations need be considered greatly simplifies the analysis of dislocation reactions. The relationship between the 〈110〉 Burgers – vectors and the {11 0} slip planes is shown in Figure 9.16, which may be compared with Thompson’s tetrahedron. A consideration of this figure confirms that, as expected from the crystallography, each Burgers vector lies in only one slip plane (e.g. AC lies in OAC only) and each slip plane contains only one Burgers vector (OAC contains only AC). This one-toone correspondence contrasts with the slip systems of the c.c.p. metals, and still further simplifies the study of dislocation interactions. In fact, there is only one dislocation reaction to consider – that between dislocations on planes at 60° to one another: AB + BC → AC ⎫⎪ 1 [101] + 1 [011] → 1 [110] ⎬ ⎪⎭ 2 2 2

Kelly_c09.indd 288

(9.45)

11/30/2011 6:19:29 PM

Dislocations in Crystals

289

B

E G

O

D H

A F

C

– – Figure 9.16 Relation between slip planes and directions in {110}〈110〉 or {110}〈111〉 slip. The point O lies at the centre of the tetrahedron ABCD whose edges are parallel to 〈110〉. The planes OAB, OAC and so on are {110} and the directions OA, OB, OC, OD are 〈111〉

If the reacting dislocations AB and BC are confined to their slip planes, (101) and (011) respectively, the resultant AC is laid down along the line of intersection of the slip planes, – OB, [111]. Hence, the glide plane of the resultant AC is (112), and for this reason it is very immobile at low temperatures. In LiF at room temperature, the dislocations on one plane will block slip on another which intersects it at 60° so efficiently that, after 1% shear strain in single slip, a resolved shear stress of about 15 times that which was needed to activate the first system must be put upon the intersecting system in order to bring it into operation [22]. Although less complex in their interactions than dislocations in c.c.p. metals, dislocations in crystals with the rock salt structure do have a property of special interest – they can carry an electric charge. The edge dislocation on {110} has an ‘extra plane’ consisting of a sheet of Na+ ions and a sheet of Cl− ions (Figure 9.17). This sheet of NaCl ‘molecules’ has been isolated in Figure 9.18. Its edge defines the dislocation line, which has a number of jogs in it. At A, an extra anion defines two jogs. The section BC has a net charge of + e; therefore the jogs at B and C are each assigned a charge of + e/2. The ‘whole’ jog at D is uncharged. This is the type of jog which is produced by intersection with an orthogonal screw dislocation; charged jogs of types B and C may be called half-jogs or, because they are produced when a single ion jumps on to or off the edge of the extra plane, diffusional jogs. It is apparent that the line as a whole can be charged, up to a maximum of e/2 per atom length. Physically, a line may become charged by acting as a source or sink for vacancies (Section 10.1). For example, because the energy needed to make a single cation vacancy is less than that needed to make an anion vacancy in NaCl, either a surface or an edge dislocation raised to a high temperature will generate excess cation vacancies which can diffuse into the crystal until their emission is throttled by the electric field that is built up as a consequence of the resultant space charge [23,24]. Relative to the adjacent crystal, the dislocation or surface acquires a positive charge, which is balanced by the nearby vacant

Kelly_c09.indd 289

11/30/2011 6:19:50 PM

290

Crystallography and Crystal Defects

+

+

+ –

–

–

–

+

+

+

–

–

–

–

+

+ –

+

–

[110] –

+

[110]

+ –

–

–

Figure 9.17 Edge dislocation in NaCl. The slip plane and the two sheets of ions constituting the extra plane are shown dotted

– +

+ –

– + – A

+ –

–

+

–

+

+

–

+

–

+

–

+

B

C

–

+

–

+

–

+

+

–

+

–

[001] D

[110]

Figure 9.18

cation sites in the crystal. On the other hand, a dislocation in an impure crystal of NaCl can acquire a negative charge in order to compensate, partly, for the extra positive charge carried by divalent impurity cations, such as Ca2+, by acting as a sink at which excess cation vacancies caused by the impurity cations can condense [23,24]. At low temperatures the effect of relatively low p.p.m. levels of impurities will predominate over the equilibrium properties that the dislocation would have in a pure crystal.

9.5

Dislocations in Hexagonal Metals

By analogy with c.c.p. metals, the slip plane of hexagonal metals should be the closestpacked basal plane (0001), the Burgers vector of a slip dislocation should be the a vector of the hexagonal lattice, 13 [112 0] , and, furthermore, this dislocation may be expected to split into two 13 10 10 partials, the analogues of Shockley partials. However, the analogy is certainly incomplete, because other slip planes, and another slip direction, sometimes operate (Table 7.2). With this reservation in mind, we will first examine dislocations on the basal plane, produced by slip and by the aggregation of point defects. – Since the three 〈112 0〉 slip vectors are coplanar, reaction between slip dislocations can only form a network of dislocations in the basal plane. Written in the notation of Figure 9.19, the reaction is:

Kelly_c09.indd 290

11/30/2011 6:19:50 PM

Dislocations in Crystals (a)

291

(b) – – a2 [1210]

S C s

B

A

a3 –– [1120]

C

B S

A –– a1 [2110] In plane

Above plane

Figure 9.19 Atoms and lattice vectors in a hexagonal metal

AB + BC → AC ⎫⎪ 1 [12 10] + 1 [1 120] → 1 [2110] ⎬ ⎪⎭ 3 3 3

(9.46)

The splitting of a perfect dislocation can also be shown on Figure 9.19: AB → Aσ + σ B ⎫⎪ 1 [12 10] → 1 [1100] + 1 [01 10] ⎬ ⎪⎭ 3 3 3

(9.47)

Between the partials As and s B, which are analogous to Shockley partials, there is a small layer of c.c.p. stacking. The sequence ABABABA becomes ABACBCB, or in Frank’s notation, Δ∇Δ∇Δ∇ is changed to Δ∇∇∇Δ∇. The order of the partials on successive basal planes must alternate; that is, if it is As − s B on one plane it must be s B − As on the next. This is in contrast to the splitting of perfect dislocations in a c.c.p. metal, where the order of the Shockley partials must always be the same if the same type of stacking fault is to be produced. In metals of small c/a ratio, the 13 2110 dislocation slips quite easily on a prism plane, – {1010}, indicating that it is not widely split on the basal plane. Zirconium and titanium, for example, slip much more easily on prism planes than on the basal plane. It is interesting to note that the reaction AB + BC → AC between prism plane dislocations cannot produce a strong barrier, because the product, formed along the intersection of two of the prism planes, is always oriented so that it can glide on the third. The experimentally determined stacking fault energy of Co is relatively low, 27 ± 4 mJ m−2 at room temperature [25]. (Cobalt transforms to a c.c.p. structure at 420 °C – see

Kelly_c09.indd 291

11/30/2011 6:19:53 PM

292

Crystallography and Crystal Defects

(a) A

(b)

B

B

A B

A

A

A

C

B

B

B

A

C

A B

C

A B A

A

A

B

B

A B

A

A

A

C A

A B A

Figure 9.20 Two possible structures for a vacancy loop in a hexagonal metal

Section 12.3.) Stacking fault energies in other h.c.p. metals are generally regarded as being much higher (see for example [25–27]), consistent with 13 2110 dislocations not being widely split on the basal plane. As with c.c.p. metals, stacking faults can arise as a result of point defect condensation. Such a fault is different from the fault produced by the splitting of a 13 1120 dislocation. When a disc of vacancies collects on a basal plane, a prismatic dislocation loop forms at its perimeter. If the disc is one vacancy thick, and if A–A stacking is to be avoided, the loop may be faulted in one of two ways. Either a single basal layer or the whole crystal on one side of the loop must be sheared over by a vector of the As type. These alternatives are shown in Figure 9.20. In case (a), the single layer can be shifted from an A into a C position by passing As partials of opposite sign on either side of it. The Burgers vector of the prismatic dislocation remains 12 [0001] , s S in Figure 9.19b, at the cost of a stacking fault which is triple, in terms of the number of next-nearest-neighbour stacking violations. In case (b), a single As partial is passed, so that the loop encloses a single stacking fault, but its Burgers vector increases to AS, as follows: Aσ + σ S = AS ⎫⎪ 1 [1100] + 1 [0001] → 1 [2203] ⎬ ⎪⎭ 3 2 6

(9.48)

Similar reasoning applies to faulted loops produced by discs of extra atoms. There is clear experimental evidence for these vacancy loops in zinc [28]; such stacking faults should have a slightly smaller energy than the double fault produced by the splitting of a perfect slip dislocation. –– – A more surprising slip system is the {112 2} 〈112 3〉, called second-order pyramidal glide. This occurs in a number of h.c.p. metals, such as Zn, Cd, Mg and Be [29]. The remarkable feature is the large size of the slip vector, 13 1123 ; that is, c + a. Even more puzzling is the fact that this system operates, second only to basal slip, in zinc and cadmium, which have the largest c/a ratios. A slip plane and its slip vectors are shown in the hexagonal cell in Figure 9.21. Each slip plane contains one slip vector and each slip vector lies in one slip plane.

Kelly_c09.indd 292

11/30/2011 6:19:57 PM

Dislocations in Crystals

293

B s C A

– [1123]

–– (1122)

B′

–– – Figure 9.21 A {112 2} 〈1123〉 slip system

The relationship between the six slip planes and six Burgers vectors, by means of a surface analogous to that used to illustrate the rock salt slip systems (Figure 9.16), is shown in Figure 9.22. The slip vectors are A′B, A′C, B′C, B′A, C′A, C′B and their antiparallel counterparts; the six slip planes are represented by A′BσA′ for the slip vector A′B, and so on. In a review of deformation modes in h.c.p. metals, Yoo et al. [30] noted that little is known about the dislocation cores of the c + a dislocations apart from results obtained through atomistic simulation: there is a distinct lack of detailed experimental observations on dislocation interactions and their role in pyramidal slip. More recent work has confirmed this trend – while there have been improvements in the choice of atom potential to model c + a dislocations in h.c.p. metals [31], experimental observations of the pyramidal glide system in h.c.p. metals still remain few in number. In addition, as Hull and Bacon note [32], there seems to be a close relationship between the occurrence of –– – {112 2}〈112 3〉 slip and twinning (Chapter 11) in h.c.p. metals, which serves to complicate the situation. –– Possible dislocation reactions between c + a dislocations on {112 2} planes in this system can be dealt with easily by decomposing each 13 1123 vector into its c and a components. The c components either add or cancel; provided c > a, there is an increase in energy when they add and a decrease when they cancel, whatever the a components may be. There are three reactions, then, corresponding to the three possible combinations of the a components when the c components cancel. The reaction is least favourable energetically when the a components are alike:

Kelly_c09.indd 293

11/30/2011 6:20:03 PM

294

Crystallography and Crystal Defects C s

B

A

A′ C′′ B′

B′′ A′′ C′

Figure 9.22

–– – Relation between slip planes and directions in {112 2} 〈1123〉 slip

C ′ A + AB′ → C ′ B′ ⎫⎪ 1 [1 1 23] + 1 [1 123] → 2 [1 120] ⎬ ⎪⎭ 3 3 3

(9.49)

The product C′B′ is formed along the line As in the basal plane common to the two slip planes C′AσC′ and B′AσB′ and can immediately split into two perfect 13 [1 12 0] dislocations. The most favourable reaction is: C ′ A + BC ′ → BA ⎫⎪ 1 [1 123] + 1 [2 1 1 3] → 1 [1210] ⎬ ⎪⎭ 3 3 3

(9.50)

A consideration of Figure 9.22 shows that the product BA is formed along the line C′s common to C′AσC′ and C′BσC′, so that it is likely to be immobile and an obstacle to other dislocations. The result of the third reaction is less easy to see from Figure 9.22. The reaction is: C ′ A + BA ′ → C ′C ′′ ⎫⎪ 1 [1 123] + 1 [2113] → 1 [3030] ⎬ ⎪⎭ 3 3 3

(9.51)

The product C′C″ should split into two a dislocations, AC + BC, but since its line does not lie in the basal plane, these dislocations are also likely to be immobile. – It is also conceivable in principle that the 〈112 3〉 dislocation might itself split into partials of the type AS (Figure 9.19):

Kelly_c09.indd 294

11/30/2011 6:20:05 PM

Dislocations in Crystals

1 [1123] → 1 [0 2 2 3] + 1 [2 0 2 3] 3 6 6

295

(9.52)

However, there is no reason to assign a low energy to the fault, which would have to form – on {112 2}. Furthermore, 13 [112 3] screw dislocations in zinc and cadmium are observed to cross-slip frequently, which is evidence against such splitting. There are two reactions between a basal-plane dislocation and a second-order pyramidal dislocation. The first is simply a rearrangement of Reaction 9.50: C ′ A + AB → C ′ B ⎫⎪ 1 [1 123] + 1 [12 10] → 1 [2113] ⎬ ⎪⎭ 3 3 3

(9.53)

The product lies along As, out of its pyramidal slip plane C′ sB. Therefore it can act as a barrier. The second reaction is simply the annihilation of the a component of the pyramidal: C ′ A + A ′′C ′ → A ′′A ⎫⎪ 1 [1 123] + 1 [1120] → [0001] ⎬ ⎪⎭ 3 3

(9.54)

The extra plane of the product A″A consists of two basal layers of atoms. These may be thought of as tending to wedge open the basal plane, which is also a cleavage plane. In this respect the reaction is like that which produces the 〈100〉 dislocation in b.c.c. metals (Section 9.6).

9.6

Dislocations in B.C.C. Crystals

It is now well established that a slip dislocation in a b.c.c. metal has the expected Burgers vector 12 111 . The plane on which this dislocation prefers to glide is far less certain (Table 7.1). We shall first assume that slip occurs somewhat more easily on {110} than on – other planes in the 〈111〉 zone. The relationship between the 12 111 Burgers vectors and the {110} slip planes can be shown on the same diagram that was used for rock salt structures (Figure 9.16). It is evident from Figure 9.16 that any two different Burgers vectors meet either at 70.53° or at 109.47°. In the latter case the dislocations will react: OA + OC → EF ⎫⎪ 1 [111] + 1 [111] → [100] ⎬ ⎪⎭ 2 2

(9.55)

The character of the product dislocation depends on the slip planes of the reactants, because these determine the direction in which its line lies. If the reacting dislocations are on the same slip plane then the glide plane of the product will of course be this plane also. If they are on planes such as AOB and AOC, which intersect at 60° along a 〈111〉, then the product, formed along this line, will still be able to glide in a {110} plane. However, if the reacting

Kelly_c09.indd 295

11/30/2011 6:20:09 PM

296

Crystallography and Crystal Defects

dislocations are on orthogonal planes, such as AOD and COB, their product will lie along a 〈001〉 like GH in Figure 9.16. It is then an edge dislocation with a {100} glide plane. The extra plane of this dislocation is parallel to the usual cleavage plane of a b.c.c. crystal, and it has been suggested that the crystal may be cracked open for a short distance beneath the extra plane [33]. The fact that slip is not very rigorously confined to any one plane is strong evidence that the 12 111 dislocation is not split widely into partials, and that therefore stacking faults have a high energy. Nevertheless, it is possible to find plausible-looking stacking faults in a rigid-ball model of the structure. A ball model of the {110} planes is shown in Figure 9.23. The arrows starting at P point out the natural path in which to slide the balls of the upper layer over the lower. This corresponds to the dissociation: 1 [111] → 1 [011] + 1 [211] + 1 [011] 2 8 4 8

(9.56)

The fault which is formed on both sides of the 14 [211] dislocation occurs quite naturally in a rigid-ball structure, because it leads to closer packing (for this reason it may be important in the martensitic transformation of a b.c.c. to a h.c.p. structure – see Section 12.10). Thus, the 81 [011] which produces the fault drops the ball P from a saddle position into a valley. However, nearest-neighbour relationships are violated and the fault must ordinarily have a rather high energy, since it has never been detected in b.c.c. metals. Computer calculations using atomistic simulations have confirmed the high energy of faults in the b.c.c. crystal structure. For example, the early work of Vitek [34] using a simple central force potential and limited computer power showed that there are no stable intrinsic faults on either the {110} or the {112} planes in b.c.c. crystals. As Ventelon and Willaime [35] have recently noted, atomistic simulations of screw dislocations in b.c.c.

[011]

[100]

1 [111] 2

P

Figure 9.23

Kelly_c09.indd 296

11/30/2011 6:20:18 PM

Dislocations in Crystals

297

metals do not show splitting into well-defined partials and stacking faults, but instead reveal core configurations that are able to spread into the three {110} planes containing the zone axis of the screw dislocation. The power of such calculations highlights the limitations of further hard-sphere models showing splitting of 12 111 dislocations into partials separated by stacking faults on {110} and {211} planes, such as those considered in the first edition of this book [36]: such models are purely geometric in nature and therefore cannot predict the energies of the postulated stacking faults. By comparison, atomistic simulations are becoming increasingly sophisticated in terms of the choice of potential, even when they apply only to rigid dislocations at absolute zero; as Duesbery and Vitek argue [37], it is expected that results of such calculations will carry through, at least qualitatively, to conditions at finite temperature.

9.7

Dislocations in Some Covalent Solids

In crystals of diamond, Ge and Si, the atoms are held together by strong, directional covalent bonds (Figure 3.12). Dislocations in these crystals are immobile at low temperatures. This is because the Peierls stress is high; that is to say, the energy of the dislocation varies sharply with its position in the crystal. Extensive slip occurs only at elevated temperatures – above about 60% of the absolute melting temperature in Ge and Si. The slip plane – is then {111} and the slip direction 〈110〉. One can imagine the way in which glide might occur. The dislocation will lie, as much as it can, in a position of low energy, probably along some prominent crystallographic direction. It advances when, aided by thermal activation, a small length of line surmounts its energy barrier and spills over into the next energy trough (Figure 9.24). The connecting segment which is stranded on the energy hill is called a kink, distinguished from a jog by the fact that it lies wholly in the slip plane (Section 8.6). The kinks can glide apart relatively easily and, as they do so, the dislocation is advanced by the trough separation. The dislocation lying on a {111} plane at 60° to its Burgers vector, 12 1 10 , happens to – be easy to draw in projection on to a {101} plane normal to the dislocation; it is shown in this way in Figure 9.25. In this figure, which serves equally well for the sphalerite (zincblende) structure and for the diamond crystal structure, the small black dots represent a column of one atom species (e.g. Zn) and the encircled dots a second atom species (e.g. S); these two species are identical in the diamond crystal structure. Here, the dislocation line

Figure 9.24 Double kink in a dislocation line. The dotted lines represent positions of high energy for the dislocation

Kelly_c09.indd 297

11/30/2011 6:20:23 PM

298

Crystallography and Crystal Defects – [111]

[111] Type l Type ll

Figure 9.25 A 60° dislocation in sphalerite. The structure of a 60° dislocation in the diamond structure is identical, except that all the atoms are then the same

– – is along the vector common to (111) and (11 11) – that is, [101] – while the Burgers vector of the dislocation is 12 [01 1] . There are two possible {111} slip planes, type I and type II. The 60° dislocation in Figure 9.25 is shown with its extra plane ending at a type II plane, where it breaks the lower number of bonds. The one bond per atom which is broken is described as a dangling bond. Intuitively, it might seem that slip should occur at the widely spaced type II planes, by the glide of dislocations like that of Figure 9.25. However, this is before the possibility of splitting into partials is examined. There can be stacking faults on the {111} plane that do not violate tetrahedral bonding and are exactly analogous to intrinsic and extrinsic faults in c.c.p. metals. The stacking sequence of the perfect crystal can be written as a ab bc ga a… (see Sections 3.4 and 3.5). In this sequence, the diatom a − a can be treated as a unit, denoted by A. Type I planes separate sheets of diatoms packed in the c.c.p. sequence ABCA… An intrinsic fault is formed by passing a Shockley partial, 61 211 , over a type I plane; passing two different Shockley partials over successive type I planes produces the extrinsic fault. The 12 110 dislocation can split into partials on a type I plane: 1 [01 1] = 1 [112] + 1 [12 1] 2 6 6

(9.57)

so that one dislocation is a 30° partial and the other a 90° partial. Experimental evidence shows that moving dislocations are indeed split into partials in this way [38], with the 90° partials being more mobile than the 30° partials [39]. This set of partials is known as the

Kelly_c09.indd 298

11/30/2011 6:20:25 PM

Dislocations in Crystals

299

S [110] R

P Q

– [110]

O – [001]

Figure 9.26 Stacking fault in a silicon film. Point O lies at the bottom surface of the film and points P, Q, R and S at the top surface. OP, OQ, OR and OS are stair-rod dislocations

‘glide set’ of dislocations [2]. Partials dissociating on the alternative type II planes are termed the ‘shuffle set’ [2]; these have a more complicated geometry and are believed to be less mobile [2], although they may play an important role in low-temperature deformation [40]. A rich variety of stacking faults is found in Si films grown epitaxially from the vapour phase [41]. Faults originating at irregularities in the substrate grow along with the film, sometimes joined together as pieces of polyhedra. A schematic of a piece of an octahedral stacking fault in a film, which is parallel to {100}, is shown in Figure 9.26. The faces of the halfoctahedron are alternate intrinsic and extrinsic faults, joined by a 61 110 stair-rod dislocation. The configuration at a corner can be derived from the Lomer–Cottrell lock (Figure 9.13) by gliding one of the Shockleys of the lock to the other side of the stair-rod dislocation. An alternative tetrahedrally bonded structure is that of wurtzite, in which ZnS units are stacked in the hexagonal sequence ABA… Stacking faults in sphalerite consist of thin layers of the wurtzite structure. Similarly, stacking faults in wurtzite can occur which are thin layers of the sphalerite structure and are exactly analogous to stacking faults in a hexagonal metal. Dislocations in AlN, which has this structure, are widely split, the fault energy being only about 4 mJ m−2 [42]. Neither wurtzite nor sphalerite possesses a centre of symmetry, with the interesting consequence that the core structures of dislocations of opposite sign can be distinguished from one another in these structures. Suppose that an undissociated 60° dislocation in, say, GaAs, which has the sphalerite structure, always lies on a type II plane (Figure 9.25). Its extra plane then ends either on a Ga atom or on an As atom, according to whether it comes in from the top or the bottom of the crystal. Dislocations of opposite sign can therefore be labelled Ga and As dislocations, and because of their different core structures they may have quite different Peierls stresses. In this context, it is of interest to note that the set of (111) planes on which dislocations reside and move has been a topic of controversy since the 1960s in crystals with the sphalerite and diamond structures [40]. Tetrahedrally bounded crystals contain a three-dimensional network of strong bonds, but in many crystals the atoms are bonded together strongly only within layers which are themselves connected by relatively weak forces. Graphite is such a crystal. The dislocations and stacking faults on the basal plane of graphite are exactly analogous to those on the basal

Kelly_c09.indd 299

11/30/2011 6:20:30 PM

300

Crystallography and Crystal Defects – – [1210]

–– [1120]

C

B s

A –– [2110]

Figure 9.27 Atoms and lattice vectors in the basal plane of graphite

plane of a hexagonal metal. Figure 9.19b is applicable; its relationship to the structure of graphite is shown in Figure 9.27. Because of the weak interlayer bonding, the energies of the three basic types of stacking fault described in Section 9.5 are very small. One of these faults is produced by the dissociation of a perfect dislocation, as follows: AC → σ C + Aσ ⎫⎪ 1 [2110] → 1 [1010] + 1 [1100] ⎬ ⎪⎭ 3 3 3

(9.58)

By direct measurement of the separation of the 13 [10 10] partials, which are 1500 Å apart in the edge orientation and 800 Å apart in the screw orientation [43], the energy of the fault has been found to be only 0.5 mJ m−2. A schematic side view of a split 60° dislocation can be seen in Figure 9.28, showing the layer of rhombohedral stacking at the fault. Although slip dislocations are strictly confined to the basal planes in graphite, their reactions with one another are a little more complex than might at first be expected. The complexities are a result of the wide separation of the partials and of the fact that, because of this wide separation, the individual partials on nearby planes can, in effect, react with one another. As an example, consider a reaction between the dislocations AB and AC, which would simply repel one another if they were not split. Suppose that they lie on adjacent planes, so that if AB splits in the order A s + s B then AC must split in the order of s C + As. If the split dislocations are caused to approach, AB from the left and AC from the right, the partials s B and s C will come over one another and react: σ B + σ C → Aσ

(9.59)

The result is a stable double ribbon, shown in Figure 9.29.

Kelly_c09.indd 300

11/30/2011 6:20:31 PM

Dislocations in Crystals b

c

b

301

[0001] b

a

a

b

c

b

a

a

a

b

b

b

a

a

– [1100]

a

In plane Above plane

Figure 9.28

b

c

a

b

b a b

As

c a b

a sC sB

b

c b

a As

b

a

a

b

b

As

As

As

Figure 9.29

9.8

Dislocations in Other Crystal Structures

The detailed analysis of the geometry of dislocations, which has been carried out up to this point for a number of specific crystal structures, could be repeated for many other crystal structures. It is hoped that the principles employed have now been demonstrated sufficiently that the reader is able to deal with any case that may be encountered in metals, ceramics, semiconductors, mesomorphic phases, quasicrystals and superlattice structures.

Problems –– 9.1 In a b.c.c. metal, two dislocations of the Burgers vector [111] and [11 1] respectively have reacted over a certain length (as in Figure 9.11). If the reacting dislocations are pinned at points p, q, r and s, which lie at the corners of a square of side L, make an estimate of the length of the product dislocation (neglect the variation of the energy of a dislocation with the orientation of its line).

Kelly_c09.indd 301

11/30/2011 6:20:35 PM

302

Crystallography and Crystal Defects

9.2 A dislocation is being extruded between small precipitate particles which lie in a row, each particle being a distance l from its neighbours. Determine the force acting on each particle as a function of the shear stress s applied on the slip plane of the dislocation parallel to the Burgers vector b and estimate the maximum force that can be exerted on each particle. 9.3 Using Frank’s rule, make a study of reactions between stable perfect dislocations in a body-centred tetragonal crystal. Consider the effect of the value of the c/a ratio on the reactions. 9.4 Compare the number of atoms that are improperly surrounded by nearest neighbours (i.e. as an atom in the h.c.p. structure instead of as in the c.c.p. structure) at intrinsic and in extrinsic faults in c.c.p. metals. What structure is formed if both the Shockley partials in a Lomer–Cottrell lock are forced to glide to the opposite side of the stairrod dislocation? 9.5 Using a dislocation corresponding to one particular slip plane and slip direction as one of the reacting dislocations forming a Lomer–Cottrell lock, how many different – locks can be formed? For the slip system (111) [101], give the Burgers vector of each partial dislocation in all of the possible Lomer–Cottrell locks. 9.6 If the concentration of vacancies in aluminium at its melting point is 9.4 × 10−4 and if after quenching the aluminium from its melting point the vacancies condense into discs on the close-packed plane and form Frank loops, determine the density of dislocations introduced (a) when the loops are 50 Å in radius and (b) when the loops are 500 Å in radius. 9.7 Assuming isotropic elasticity, calculate the separation of the Shockley partials of a screw dislocation in Ag, Al and Au. Use the stacking fault energies given in Table 9.2. For Ag take m = 28 GPa, n = 0.38; for Al take m = 26 GPa, n = 0.34; for Au take m = 28 GPa, n = 0.42. 9.8 For the first four lattices listed in Table 9.1, find the Burgers vectors of any dislocations whose stability, according to Frank’s rule, is doubtful; that is, dislocations that might dissociate into two perfect dislocations whose Burgers vectors are at 90° to one another. 9.9 Lead sulphide, PbS, has the same crystal structure as NaCl, but the usual slip system – is {100}〈011〉 instead of {011}〈011〉. (a) Compare dislocation reactions that may occur as a result of slip in PbS with those occurring in NaCl. (b) Sketch the structure of the edge of the extra plane of an edge dislocation in PbS. 9.10 Describe the dislocation loops that might be produced in zinc by the aggregation of interstitial atoms into discs of atoms parallel to the basal plane. Also describe the dislocation loops that might be produced in graphite by the aggregation of vacant sites into discs parallel to the basal plane. – 9.11 Project the structure of silicon on to a (101) plane and show, in this projection, the structure of an intrinsic stacking fault and the structure of an extrinsic stacking fault in silicon.

Kelly_c09.indd 302

11/30/2011 6:20:36 PM

Dislocations in Crystals

303

9.12 Show how, in graphite, two dislocation ribbons (i.e. dislocations that are split into widely separated partials) that are on next-nearest-neighbour basal planes can interact to form a three-fold ribbon. 9.13 An alloy of 50 at% Cu–50 at% Zn contains dislocations of Burgers vector 12 111 and 〈100〉. The alloy is then ordered to produce the B2 superlattice (Section 3.8). – Describe the effect of gliding the 12 111 dislocation on {110} and the 〈100〉 dislocation on {010} after ordering has occurred. From your result, how would you expect two identical 12 111 dislocations to interact in the ordered alloy?

Suggestions for Further Reading See the suggestions for Chapter 8 and the following: F.R.N. Nabarro, M.S. Duesbery, J.P. Hirth and L. Kubin (1979–2010) Dislocations in Solids, Volumes 1–16, Dislocations and Disclinations, Elsevier, Amsterdam. T. Suzuki, S. Takeuchi and H. Yoshinaga (1991) Dislocation Dynamics and Plasticity, Springer, Berlin (translated from the Japanese edition published by Shokabo in 1985).

References [1] G. Lu, N. Kioussis, V.V. Bulatov and E. Kaxiras (2001) Dislocation core properties of aluminum: a first-principles study, Mater. Sci. Eng. A, 309–310, 142–147. [2] J.P. Hirth and J. Lothe (1982) Theory of Dislocations, 2nd Edition, John Wiley and Sons, New York. [3] F.C. Frank (1949) written answer to a remark by E.N. da C. Andrade on the paper by N.F. Mott (1949) Mechanical properties of metals, Physica, 15, 119–128: Physica, 15, 131–133. [4] A.J.E. Foreman (1955) Dislocation energies in anisotropic crystals, Acta Metall., 3, 322–330. [5] R.D. Heidenreich and W. Shockley (1948) Study of slip in aluminum crystals by electron microscope and electron diffraction methods, Bristol Conference on the Strength of Solids, The Physical Society, London, pp. 57–75. [6] D.B. Williams and C.B. Carter (1996) Transmission Electron Microscopy: A Textbook for Materials Science, Plenum Press, New York. [7] D.J.H. Cockayne, M.L. Jenkins and I.L.F. Ray (1971) The measurement of stacking-fault energies of pure face-centred cubic metals, Phil. Mag., 24, 1383–1392. [8] P.S. Dobson, P.J. Goodhew and R.E. Smallman (1967) Climb kinetics of dislocation loops in aluminium, Phil. Mag., 16, 9–22. [9] M.L. Jenkins (1972) Measurement of the stacking-fault energy of gold using the weak-beam technique of electron microscopy, Phil. Mag., 26, 747–751. [10] W.M. Stobbs and C.H. Sworn (1971) The weak beam technique as applied to the determination of the stacking-fault energy of copper, Phil. Mag., 24, 1365–1381. [11] C.B. Carter and S.M. Holmes (1977) The stacking-fault energy of nickel, Phil. Mag., 35, 1161–1172. [12] F.C. Frank (1951) The growth of carborundum: dislocations and polytypism, Phil. Mag., 42, 1014–1021. [13] N. Thompson (1953) Dislocation nodes in face-centred cubic lattices, Proc. Phys. Soc. B, 66, 481–492. [14] M.J. Whelan (1959) Dislocation interactions in face-centred cubic metals, with particular reference to stainless steel, Proc. Roy. Soc. Lond. A, 249, 114–137.

Kelly_c09.indd 303

11/30/2011 6:20:36 PM

304

Crystallography and Crystal Defects

[15] W.M. Lomer (1951) A dislocation reaction in the face-centred cubic lattice, Phil. Mag., 42, 1327–1331. [16] A.H. Cottrell (1952) The formation of immobile dislocations during slip, Phil. Mag., 43, 645–647. [17] J. Silcox and P.B. Hirsch (1959) Direct observations of defects in quenched gold, Phil. Mag., 4, 72–89. [18] J.P. Hirth (1961) On dislocation interactions in the fcc lattice, J. Appl. Phys., 32, 700–706. [19] J.B. Bilde-Sørensen, T. Leffers and P. Barlow (1977) Dissociated structure of dislocation loops with Burgers vector a in electron-irradiated Cu–Ni, Phil. Mag., 36, 585–595. [20] F.R.N. Nabarro (1987) Theory of Crystal Dislocations, Dover Publications, New York. [21] J. Friedel (1955) On the linear work hardening rate of face-centred cubic single crystals, Phil. Mag., 46, 1169–1186. [22] T.H. Alden (1963) Extreme latent hardening in compressed lithium fluoride crystals, Acta Metall., 11, 1103–1105. [23] J.D. Eshelby, C.W.A. Newey, P.L. Pratt and A.B. Lidiard (1958) Charged dislocations and the strength of ionic crystals, Phil. Mag., 3, 75–89. [24] R.W. Whitworth (1975) Charged dislocations in ionic crystals, Adv. Phys., 24, 203–304. [25] A. Korner and H.P. Karnthaler (1983) Weak-beam study of glide dislocations in h.c.p. cobalt, Phil. Mag. A, 48, 469–477. [26] R.L. Fleischer (1986) Stacking fault energies of hcp metals, Scripta Metall., 22, 223–224. [27] L. Wen, P. Chen, Z.-F. Tong, B.-Y. Tang, L.-M. Peng and W.-J. Ding (2009) A systematic investigation of stacking faults in magnesium via first-principles calculation, Eur. Phys. J. B, 72, 397–403. [28] P.S. Dobson and R.E. Smallman (1966) The climb of dislocation loops in zinc, Proc. Roy. Soc. Lond. A, 293, 423–431. [29] M.H. Yoo (1981) Slip, twinning, and fracture in hexagonal close-packed metals, Metall. Trans. A, 12, 409–418. [30] M.H. Yoo, J.R. Morris, K.M. Ho and S.R. Agnew (2002) Nonbasal deformation modes of hcp metals and alloys: role of dislocation source and mobility, Metall. Trans. A, 33, 813–822. [31] T. Nogaret, W.A. Curtin, J.A. Yasi, L.G. Hector and D.R. Trinkle (2010) Atomistic study of edge and screw dislocations in magnesium, Acta Mater., 58, 4332–4343. [32] D. Hull and D.J. Bacon (2011) Introduction to Dislocations, 4th Edition, ButterworthHeinemann, Oxford. [33] A.H. Cottrell (1958) Theory of brittle fracture in steel and similar metals, Trans. Am. Inst. Min. Metall. Petrol. Engrs., 212, 192–203. [34] V. Vítek (1968) Intrinsic stacking faults in body-centred cubic crystals, Phil. Mag., 18, 773–786. [35] L. Ventelon and F. Willaime (2010) Generalized stacking-faults and screw-dislocation corestructure in bcc iron: a comparison between ab initio calculations and empirical potentials, Phil. Mag., 90, 1063–1074; corrigendum, 4071. [36] A. Kelly and G.W. Groves (1970) Crystallography and Crystal Defects, Longman Group Limited, London. [37] M.S. Duesbery and V. Vitek (1998) Plastic anisotropy in b.c.c. transition metals, Acta Mater., 46, 1481–1492. [38] A. Olsen and J.C.H. Spence (1981) Distinguishing dissociated glide and shuffle set dislocations by high resolution electron microscopy, Phil. Mag. A, 43, 945–965. [39] H.R. Kolar, J.C.H. Spence and H. Alexander (1996) Observation of moving dislocation kinks and unpinning, Phys. Rev. Lett., 77, 4031–4034. [40] W. Cai, V.V. Bulatov, J. Chang, J. Li and S. Yip (2004) Dislocation core effects on mobility, in Dislocations in Solids, Volume 12 (edited by F.R.N. Nabarro and J.P. Hirth), Elsevier, Amsterdam, pp. 1–80. [41] G.R. Booker (1964) Crystallographic imperfections in silicon, Disc. Faraday Soc., 38, 298–304. [42] P. Delavignette, H.B. Kirkpatrick and S. Amelinckx (1961) Dislocations and stacking faults in aluminum nitride, J. Appl. Phys., 32, 1098–1100. [43] C. Baker, Y.T. Chou and A. Kelly (1961) The stacking-fault energy of graphite, Phil. Mag., 6, 1305–1308.

Kelly_c09.indd 304

11/30/2011 6:20:39 PM

10 Point Defects 10.1

Introduction

Disturbances in a crystal which, apart from elastic strains associated with them, extend for no more than a few interatomic distances in any direction are called point defects. Although impurity atoms in solution can be classified as point defects, we shall be mainly concerned with structural point defects, of which there are two elementary types. The first is the vacancy, which consists of an atomic site from which the atom is missing. The second consists of a small region of crystal which contains an extra atom. This is called an interstitial defect, from the idea that the extra atom is squeezed into an interstice between the others. A point defect differs from a dislocation and from a two-dimensional defect such as a crystal boundary in two important respects. The first is that, even with modern transmission electron microscopes, scanning tunnelling microscopes and atom probe field-ion microscopes, point defects are relatively difficult to observe directly, so that in the main they can be detected and studied only through their effect upon some physical property of the crystal. The second distinction is that point defects may be present in appreciable concentrations when the crystal is in thermodynamic equilibrium. While dislocations and interfaces always raise the free energy of a crystal, adding a certain number of point defects to an otherwise perfect crystal reduces its free energy to a minimum value. This is because of a gain of entropy which arises from the many possible sets of places in the crystal where the point defects can be put. This configurational entropy is given by:

S = k ln W

(10.1)

where k is Boltzmann’s constant (1.38 × 10−23 J K−1 or 8.62 × 10−5 eV K−1) and W is the number of different arrangements of point defects. When n defects are distributed amongst

Crystallography and Crystal Defects, Second Edition. Anthony Kelly and Kevin M. Knowles. © 2012 John Wiley & Sons, Ltd. Published 2012 by John Wiley & Sons, Ltd.

Kelly_c10.indd 305

11/30/2011 9:59:11 AM

306

Crystallography and Crystal Defects

N sites, the number of arrangements is NPn = N(N − 1)…(N − n + 1) = N!/(N − n)! if each defect is distinct. In fact, all the defects are identical, and the n labels needed to distinguish them from one another can be distributed in n! ways. Therefore: W = N Cn =

N! ( N − n)! n !

(10.2)

Manipulating Equation 10.2 into a form suitable for the application of Stirling’s approximation (ln x! ≈ x ln x − x, for large x) gives: ln W = N ln N − ( N − n) ln( N − n) − n ln n

(10.3)

so that in Equation 10.1: S = k [ N ln N − ( N − n) ln ( N − n) − n ln n]

(10.4)

If the presence of one defect increases the internal energy of the crystal by Ef , the change in free energy of a crystal containing n identical defects, at a temperature of T K, is: ΔF = nEf − T (S + nS ′ )

(10.5)

Here it is assumed that n/N is so small that the defects do not interact with one another. The extra entropy term nS′ in Equation 10.5 represents the fact that each defect may add a certain entropy S′ to the crystal because of its effect on the vibration of the atoms in its neighbourhood. The number of defects producing the minimum free energy, ne , is found by setting dΔF/dn = 0, giving: ne ⎛ E ⎞ ⎛ S′⎞ = exp ⎜ ⎟ exp ⎜ − f ⎟ ⎝ k⎠ ⎝ kT ⎠ N − ne

(10.6)

If the defect in question is a vacancy then N − ne is simply the number of atoms in the crystal. Since in fact ne 0. Finally, comparing the Schmid factors for A III and D I, we have: A III : | cos φ cos λ | (× 6(u2 + v 2 + w 2 )) = w 2 + vu + vw − u2 D I : | cos φ cos λ | (× 6(u2 + v 2 + w 2 )) = w 2 + vu + uw − v 2 and since: n w + v 2 > uw + u2 for 0 < u < v < w, it follows that A III is the slip system with the greatest Schmid factor; that – is, the slip system (111) [101]. This is of course the slip system found using either Diehl’s rule or OILS rule for a pole within the 001–011–111 standard stereographic triangle in c.c.p. crystals. Thus, Diehl’s rule and OILS rule are both proved using this methodology. The extension of this analysis to other stereographic triangles can be achieved by suitable permutations of the indices defining the poles at the corners of the standard stereographic triangle. A simple extension of this methodology enables special cases, such as where u = v > 0, to be considered when two or more slip systems have the same Schmid factor.

References [1] J. Diehl, personal communication to A. Seeger, acknowledged on p. 24 of A. Seeger (1958) Kristallplastizität, Handbuch der Physik, Band VII.2: Kristallphysik II (edited by S. Flügge), Springer-Verlag, Berlin, pp. 1–210. [2] I.M. Hutchings (1993) Quick non-graphical method for deducing slip systems in cubic close packed metals in tension or compression, Materials Science and Technology, 9, 929–930.

Kelly_bapp05.indd 486

11/30/2011 2:48:47 PM

Appendix 6 Homogeneous Strain A body is said to be homogeneously strained if the distortion is the same everywhere. Under these circumstances, the eij in Equations 6.5 and 6.9 are constants, independent of position in the body. The equation: dui =

∂ui ∂x j

dx j = eij dxj

(A6.1)

can then be integrated immediately to obtain the displacements: ui = (u0 )i + eij x j

(i, j = 1, 2, 3)

(A6.2)

It is apparent from Equation A6.2 that in homogeneous strain, the displacements are linear functions of the position coordinates. The constants (u0)i represent the translation of the body as a whole, and are of no further interest. Subtracting this translation from the displacement, we obtain the residual displacement: xi′ − xi = eij x j

(A6.3)

where x'i are the new coordinates (referred to axes that have been translated by (u0)i but not rotated) of the point which was originally at xi. Equation A6.3 written out in full is: x1′ = (1 + e11 ) x1 + e12 x2 + e13 x3 x2′ = e21 x1 + (1 + e22 ) x2 + e23 x3 x3′ = e31 x1 + e32 x2 + (1 + e33 ) x3

Crystallography and Crystal Defects, Second Edition. Anthony Kelly and Kevin M. Knowles. © 2012 John Wiley & Sons, Ltd. Published 2012 by John Wiley & Sons, Ltd.

Kelly_bapp06.indd 487

11/30/2011 2:51:35 PM

488

Crystallography and Crystal Defects

The shape into which a line or surface whose general equation is: f ( x1 , x2 , x3 ) = 0

(A6.4)

is deformed can be determined by solving Equation A6.3 for x1, x2 and x3 in terms of x′1, x′2 and x′3, and substituting these values into Equation A6.4. In this way it can be shown that any homogeneous strain, large or small, has the following four properties: 1. Straight lines remain straight lines, and in general are rotated and stretched or contracted, all straight lines in the same direction being rotated through the same angle and stretched or contracted in the same ratio. Similarly, planes are deformed into planes. 2. A sphere is deformed into an ellipsoid. The ellipsoid into which a sphere of unit radius is deformed is called the strain ellipsoid. 3. The axes of the strain ellipsoid are derived from three mutually perpendicular diameters of the unit sphere, which are called the principal axes. These axes form the only set of three orthogonal directions which remain orthogonal after the strain. 4. In the unstrained state there is a particular ellipsoid, called the reciprocal strain ellipsoid, which deforms into the unit sphere. Its axes are the principal axes. In general, the principal axes are rotated by the strain. A deformation which leaves the principal axes unrotated is called a pure strain. A general homogeneous strain can be accomplished in two stages: a pure strain in which the principal axes receive their correct extensions, followed by a rotation in which they are brought to their final position. The above results are applied in the discussion of the geometry of martensitic transformations in Chapter 12. We shall now mention three very simple types of homogeneous strain.

A6.1 Simple Extension x1′ = kx1 , x 2′ = x2 , x3′ = x3 ,

⎛ e11 = k − 1 e12 = 0 e13 = 0 ⎞ ⎜e = 0 e22 = 0 e23 = 0⎟ ⎜ 21 ⎟ e32 = 0 e33 = 0⎠ ⎝ e31 = 0

(A6.5)

The principal axes Ox1, Ox2 and Ox3 are not rotated; therefore, simple extension is a pure strain.

A6.2

Simple Shear x1′ = x1 + gx2 , x2′ = x2 , x3′ = x3 ,

⎛ e11 = 0 e12 = g e13 = 0 ⎞ ⎜ ⎟ ⎜ e21 = 0 e22 = 0 e23 = 0 ⎟ ⎜e = 0 e = 0 e = 0⎟ 32 33 ⎝ 31 ⎠

(A6.6)

where g is the magnitude of the shear strain, as defined in Equation 6.2. A more detailed description of simple shear is developed in Chapters 7 and 11, where it is required for the description of slip and twinning. Simple shear is not a pure strain; its nonrotational part is described below.

Kelly_bapp06.indd 488

11/30/2011 2:51:41 PM

Homogeneous Strain

489

x 2° x2

P

Q

P⬘

x1

a a p –a 4 2 O

a = tan–1

x 1°

g 2

Figure A6.1

A6.3

Pure Shear x1′ = kx1 , −1

x2′ = k x2 , x3′ = x3 ,

e13 = 0 ⎞ ⎛ e11 = k − 1 e12 = 0 ⎜ ⎟ e22 = (1 / k ) − 1 e23 = 0 ⎟ ⎜ e21 = 0 ⎜e =0 e32 = 0 e33 = 0 ⎟⎠ ⎝ 31

(A6.7)

In this strain, the principal axes are Ox1, Ox2 and Ox3, and they are not rotated.

A6.4

The Relationship between Pure Shear and Simple Shear

The relationship between a pure shear and a simple shear is illustrated by the diagram in Figure A6.1. A simple shear of strength g, referred to axes Ox1°, Ox°, 2 distorts a circle into the ellipse shown in Figure A6.1. The same ellipse can be produced by a strain which is a pure shear, referred to axes Ox1, Ox2, with Ox1 at an angle of π / 4 − 12 tan −1 g / 2 to Ox1°, as shown in Figure A6.1. The required magnitude of the pure shear is given by:

(

k − 1/ k = g

)

(A6.8)

In order for the displacements produced by this pure shear to be identical to those produced by the simple shear, it must be preceded by a rotation of tan−1g/2. Thus point P, for example, is rotated to Q, and the pure shear then carries Q to P′. Alternatively, the displacements of the simple shear can be produced by a pure shear referred to axes at ±π / 4 + 12 tan − 1 g / 2 to Ox1°, followed by a rotation of tan−1g/2. These axes are principal axes of the simple shear; Ox1, Ox2 and Ox3 (which remains unchanged) are the principal axes of the simple shear in their final, rotated position. When the simple shear is of very small magnitude (g = g, where g 3 ; for practical values of c/a seen in h.c.p. metals (1.5 < c/a < 1.9), com– pression would be possible if the only twinning mode were (112 1) and elongation – would be possible if the only twinning mode were (112 2). 11.12 Yes. 11.14 4°. 11.15 10%.

Chapter 12 12.1 4, 2 (twins). Component of b normal to (111) must equal 2 a / 3 . 0 0⎞ ⎛ 1 12.3 12 〈110〉 vectors. Yes. ⎜ − 1 1 − 1 ⎟ . ⎜ 2 2 2⎟ ⎜⎝ 0 1 1 ⎟⎠ 12.5 1.57. 12.6 0.18°, 0.003. 12.7 2, 4, 6. ⎛ ⎞ 1 0 0 ⎜ ⎟ 12.10 ⎜ . 0 1 − 1⎟ 2 2⎟ ⎜ 1⎟ ⎜0 1 ⎝ 2 2⎠

Chapter 13 13.2 13.3 13.4 13.5 13.6

Kelly_both.indd 506

Step heights are 1, 3, 1 and 2 lattice plane spacings, respectively. g(0 0 1) = 0.894 g(2 1 0), g(1 1 1) = 0.775 g(2 1 0), g(1 1 0) = 0.949 g(2 1 0) (as in Figure 13.5).

1.16 J m−2, 15%. (a) Attract, (b) energy increases as b2 ln b. – Boundary plane: (a) {110}, (b) {110}, (c) {112 0}. Axis of tilt: (a) 〈001〉, (b) 〈211〉, a a a – (c) 〈1 100〉. Angle of tilt: (a) 2 sin −1 , (b) 2 sin −1 , (c) 2 sin −1 . 2d 2 2d 2 2d

11/30/2011 7:37:49 PM

Brief Solutions to Selected Problems

507

13.7 See E.J. Freise and A. Kelly (1961) Twinning in graphite, Proc. Roy. Soc. Lond. A, 264, 269–276. 13.9 The difference in angle in radians is of the order of the ratio of the twin boundary to the surface free energy. 13.11 Effective surface free energy = 0.96g. 13.12 3.75%. – 13.13 (a) (11 0), (b) 3.1 × 107 m−1, (d) about 8°. 13.15 Two.

Kelly_both.indd 507

11/30/2011 7:38:04 PM

Index Note: Page numbers in italics refer to Figures; those in bold to Tables aggregation of point defects, 309, 311 alkali halides, point defects, 309–10, 315, 320–1 alkali metals, crystal structure, 92, 369 allotropy (elements), 86, 110 alloys, metallic amorphous (noncrystalline), 124 phase transformations, 363–4, 374–83 quasicrystalline phases (i-phases), 136–7 strained layer epitaxy, 425 topological close-packing (TCP), 135 twinning frequency, 342–3, 353–4, 354 aluminium dislocation strain energies, 271–2 elastic isotropy, 256 vacancy generation, with heating, 318, 319 amorphous materials, 123–6 anelastic strain, 326–7, 329 anisotropy Hooke’s law application, dislocation strains, 256–8 of mesogenic molecules (liquid crystals), 126–7 and polycrystalline textures, 229 annealing, 322–4, 323, 325 twins, 336 antimony, crystal structure, 97–8, 98, 98 antiphase domain boundaries, 112, 113 antisymmetric tensors, 148–9 arsenic, crystal structure, 97–8, 98, 98

atactic polymers, 115 atomic radii, 110 austenite, 363, 379–82 axes of rotational symmetry, 15–16, 43, 44 permissible combinations, 21–6, 25 pure (proper rotation), 44, 44–5 axial angles, 6, 6, 8, 67 axial glide planes, 72 axial (c/a) ratios, 52 hexagonal close-packed metals, 90–1, 91 and slip planes, 205, 208, 291 and martensitic transformation, 374 wurtzite structure compounds, 101, 101 Bain correspondence, 379, 379–81, 383 barium titanate (BaTiO3) crystal structure, 105 phase transitions and ferroelectric properties, 384 binding energy, divacancies, 310–11 bismuth, crystal structure, 97–8, 98, 98 body-centred cubic (b.c.c.) structure dislocation geometry, 295–7, 296 glide systems, 205, 219–20, 221 lattice symmetry and unit cells, 36–7, 37, 92–3, 93 point defects interstitials, 314, 314–15 vacancies, 313, 316, 316 transformation to h.c.p. structure, 369, 369–70, 374, 375, 385–6 twinning (metals), 342–4, 343

Crystallography and Crystal Defects, Second Edition. Anthony Kelly and Kevin M. Knowles. © 2012 John Wiley & Sons, Ltd. Published 2012 by John Wiley & Sons, Ltd.

Kelly_bindex.indd 509

11/30/2011 3:17:12 PM

510

Index

Boltzmann’s constant, 253, 305 Born–Mayer potential, 312 boron nitride, hexagonal form, 97, 97 brass, texture, 234, 234 Bravais (space) lattices, 26–37, 28, 71–2 brittleness, 199, 396 bulk metallic glasses (BMGs), 124 Burgers circuit, 245, 246, 246, 247 Burgers vector general description methods, 245–7, 246 related to strain energy, 269–71, 272–3 as slip plane displacement, 241–5 stability of dislocations, 273, 274 c/a ratios see axial ratios caesium chloride crystal structure, 99, 100, 496 unit cell, 7, 7 calcite crystal structure, 109, 109–10 deformation twinning, 345, 345, 354 calcium fluoride (fluorite), crystal structure, 102–3, 103 carbon iron impurity atomic arrangement, 326, 327, 329 in steel, and martensitic transformation, 363, 380, 380–1 see also diamond; graphite cassiterite structure see rutile crystal structure cellular solid materials, 137, 138–9 centre of symmetry, 16, 45, 153–4, 177–8 centred rectangular cells, 19, 21 charged dislocations, 289–90, 290 chemical force, on dislocations, 252–3 cholesteric phases (liquid crystals), 127, 128, 129 chrysoberyl crystal structure, 107 cleavage planes, 295, 296, 396–7, 397 climb (dislocation motion), 244, 248, 251, 252–3 close packing (of spheres), 86–8, 87, 88 Bernal’s RCPS model, 124, 125 interstices, 89, 90, 104

Kelly_bindex.indd 510

plane stacking, 88, 89, 91 stacking faults, 278–9, 279, 281 Frank notation, 280–1 topological (TCP) structures, icosahedral packing, 135, 136 closed forms, 49–50 cobalt martensitic transformation, 366–9, 368, 420 stacking fault energy, 291–2 coherency strain, 421, 427 coincidence site lattices (CSL), 405–6, 406, 407 compliances (elastic constants), 182–4, 188, 190 composition plane, K1 (twinning), 335, 337, 339, 350–3, 354 compound (degenerate) twins, 340 compounds, simple inorganic (MX and MX2), 98–104, 494–8 compression, and crystal lattice deformation, 226–8, 227 conductivity (electrical) direction, referred to tensor principal axes, 149–52, 151 measurement, and point defect mobility, 318–21, 320, 321 tensor components, 141–2, 144–5 constancy of angle, law of, 8, 8 converse effect (piezoelectricity), 181 coordination number, 3–4, 86, 110 copper alloys, martensitic transformation, 382–3 point defects, mobility, 308–9 rolled, texture, 229, 232, 232 correspondence matrix, 370, 379 corundum see sapphire covalent bonding dislocation geometry, 297–300, 301 dislocation width (Peierls model), 260 in polymers, 115 critical resolved shear stress, law of, 219 cross-slip (dislocations), 261–2, 262 crowdions (Paneth), 314, 314–15, 316–17

11/30/2011 3:17:13 PM

Index

crystal structure descriptive methods, 85–6, 116–17, 119 growth, 417–18 crystal systems, 26, 26 elastic constants, 184–93, 188, 190 enantiomorphous, 68–9 Internet information sources, 499–500 of named elements, 491–4 noncentrosymmetric, piezoelectric moduli, 179–81 second-rank tensor limitations, 155, 156, 158–9 special forms, 67, 68 crystallographic glide strain definition, 202–3, 203 in displacement analysis, 210 and lattice orientation, in tension/ compression, 222, 223–4, 226 cubic close-packed (c.c.p.) structure, 86–9, 87, 88, 89, 90 coincidence lattices, 405, 406 dislocation geometry, 278–88, 279, 288 double slip, 225, 225–6 and icosahedral packing, 134, 135 point defects interstitials, 314, 314 vacancies, 312–13, 313, 316, 317, 317–18 slip system stereograms, 219, 220, 220–2, 222 transformation to h.c.p. structure, 366–9, 368, 385 twinning (metals), 335–7, 336, 337, 342 see also face-centred cubic (f.c.c.) structure cubic crystal system elastic constants, 186–7, 187, 189 glide systems, pure strain and rotation, 212–15, 213, 214 lattice symmetry and unit cells, 35, 35–7, 36, 37 planar spacing and interplanar angles, 471–2 point group symmetry elements, 53, 53–5 property representation quadric, 158

Kelly_bindex.indd 511

511

shear stress and piezoelectricity, 180, 180–1 stereogram, 453–5, 454 stereograms, 55, 55 tetragonal defect orientation, 329, 329 damping, 327 defect structures, 99 deformation twinning, 337–42, 339, 354–8 dendrites, 417, 418 density dislocation, 245, 261 of solid solutions, 111 deviatoric stress, 176 diad (two-fold) axis of symmetry, 18, 19–20, 30 diagonal glide planes, 72 diamond crystal structure, 95, 95, 96 dislocations, 297–8, 298 diamond glide planes, 72 Diehl’s rule, 221, 483–4, 485–6 diffraction patterns in crystal structure determination, 85, 464 Laue method, 69, 69 diffusion-based phase transformations, 364 dihedral angles, 420, 421 dilatation, 169–70, 170, 260 dipoles dislocation, 263, 284 electric, single crystal (piezoelectricity), 177, 180 directions closest-packed (lattice), 87–8, 88, 91 glide (slip), 201, 201–2, 204, 225, 273 indices, transformation for unit cell changes, 473–4 physical properties, tensor representation, 150–2, 151, 155–60 relative displacement, in dislocations, 247, 247 shear, in twinning (h), 338–9, 339, 350–1 specification of, 9, 9

11/30/2011 3:17:13 PM

512

Index

dislocation glide motion, 248, 248–9 dislocations Burgers vector, general description, 245–7, 246 core, atomic positions, 258–61 crystal distortion, 253–8 forces and crystal stress, 249–53, 398–9 geometry, for specific crystal structures, 301 body-centred cubic (b.c.c.) crystals, 295–7, 296 covalent solids, 297–301 cubic close-packed (c.c.p.) metals, 280–8, 288 hexagonal metals, 290–5, 291 rock salt, 288–90, 289 glide mechanisms, 205, 241–5 interactions and multiplication, 261–5, 262, 272 loop motion, 247–9, 248 partial, and stacking faults, 277–9, 279 pile-up, in deformation twinning, 355–6, 356 strain energy and stability, 269–77, 274 displacive phase transitions, 384 domains, in ordered crystals, 112, 113 double hexagonal close-packed structure, 92 double (duplex) slip, 72, 225, 228 ductility, 199, 229 dummy suffix notation (tensor components), 145–6 dyadic operators see second-rank tensors edge dislocations atomic positions, 243–5, 244 bonding and Peierls force, 261 and Burgers vector, 246, 246 description, for cubic lattice, 242–3, 243 distortion stresses and strains, 255–6 strain energy calculation, 270–1 electric charge (NaCl), 289–90, 290 parallel, 262–3, 263 stair rods, 286, 286–7, 299 stress and force components, 251–3, 252 Einstein summation convention, 145–6, 438

Kelly_bindex.indd 512

elastic twinning, 356 elasticity crystal deformation, compared with plastic glide, 200 dislocation elastic energy, 273, 277 elastic constants, in crystal classes, 184–9, 188, 190 in isotropic materials, 189, 192–3, 256 strain and stress relationships, 181–4 electric fields see space charge regions electrical conductivity see conductivity electron irradiation, 324–5, 325 ellipsoids as effect of homogeneous strain on spheres, 371, 371, 488 physical property representation, 157–60, 158, 159 emissary dislocations, 356, 356 enantiomorphs crystal classes, 68–9 related to symmetry, 43–4 engineering shear strain, 165–6, 166, 170 entropy, related to point defects, 305–6, 310 epitaxial growth, 423–4, 424, 424 equilibrium point defect concentration, 305, 307, 318, 319 Euler angles, 234, 234–5 Euler’s theorem, related to regular polyhedra, 131, 133 extension, 165, 166, 488 extrinsic (double) stacking faults, 279, 280–1, 284 extrusion (of dislocations), 275–7, 276, 277 F-centres (anion vacancies), 310 face-centred cubic (f.c.c.) structure Bravais lattice, 36, 36, 86 transformation to face-centred tetragonal (f.c.t.), 374–6 ferroelectric materials, 335, 384 ferrous oxide, point defects, 310 fibre composite materials, 139 field tensors, 142 fluorite crystal structure, 102–3, 103, 498 foams, 137–9, 138

11/30/2011 3:17:13 PM

Index

forces, on dislocations climb and glide components, 251–3, 252, 263 Peierls model, 259–61 work and energy relationships, 249–51, 396–7 Frank partials, 281–3, 286–7, 287 Frank–Read mechanism, dislocation source, 261–2, 276 Frank’s rule, 272, 272–3, 287 Frenkel defects, 306–7, 325 FS/RH convention (Burgers vector), 245–6, 246, 247, 284 garnets, crystal structure, 107–9, 108 glasses, 123, 124, 189 glide (slip) conditions and process, 199–200, 200 displacement tensor components analysis as pure strain and rotation, 211–12, 212 for different slip systems, 212–14, 213 in three dimensions, 210, 210–11 in two dimensions, 208–10, 209 fine structure, 200–1, 202, 202 independent slip systems, 215–17, 216, 481–3 large strains in single crystals glide system choice, 218–22 lattice orientation changes, 222–8 measurement of glide strain, 202–3, 203 plane symmetry elements, in space groups, 70–1, 72, 78 polycrystalline grain deformation, 217–18 system elements, 203–5, 204 for named crystal types, 205, 206–7 see also dislocations glide cylinder (dislocation motion), 248, 248 grain boundaries energy related to tilt angle, 398–400, 399 good fit and coincidence lattices, 405, 405–7, 407 interface junctions, 409–14 source lattice (dislocation array), 408, 408–9

Kelly_bindex.indd 513

513

see also phase boundaries; tilt boundaries grains lattice rotation, 217–18 polycrystal arrangement, froth analogy, 418–19, 419 preferred lattice orientation (texture), 228–9, 233–5 role in structure of crystalline solids, 397 graphene, unit cell definition, 3–6, 4 graphite basal plane dislocations, 299–300, 300, 301, 350 crystal structures, 95–7, 97 twinning, 346, 349–50, 350, 351 vacancies, 317 grossular (natural garnet), 108 group theory, 79 H-centres (anion interstitial defects), 315, 315 habit plane, 364–5, 371–4, 373 in steels, 381–2, 382 halite see sodium chloride Heidenreich–Shockley partials see Shockley partials Hermann–Mauguin notation, 78–9, 80 Herring’s construction, crystal shape, 415–16, 416 hexad (six-fold) axis of symmetry, 18, 20–1 hexagonal close-packed (h.c.p.) structure, 87, 89, 90–1, 91, 92 second-order pyramidal glide, 292–3, 293 at twin boundary, 336 hexagonal crystal system, 33, 34, 35, 35 dislocation geometry, 290–5, 291 elastic constants, 189, 191 orthohexagonal cell indices, 476–7, 477 planar spacing and interplanar angles, 471, 472 point group symmetry elements, 56, 56–9 twinning (metals), 346, 349 Hirth lock configuration, 287, 287–8 holosymmetric class (of crystal systems), 50

11/30/2011 3:17:13 PM

514

Index

homogeneous strain, 166, 200, 208–9, 328, 445 mathematical properties, 487–8 see also extension; shear Hooke’s law, 181–2, 445–6 anisotropic media, calculations, 256–8 dislocation stresses and strains, 254–5 for isotropic solids, 192–3 hydrostatic pressure, 175–6, 199 i-phases, 136–7 icosahedral packing, 134–5, 135, 136 ilmenite (FeTiO3), crystal structure, 106 improper rotations, 44 impurities, and point defects, 305, 310, 322, 326 incommensurate structures, 137 indium crystal structure, 93–4 thallium (In–Tl) alloys, martensitic transformation, 374–49, 376 inert gases crystal structure, 86 secondary bonding, 115 infinitesimal strain, 166 in three dimensions, 168–70, 170 in two dimensions, 166–8, 167, 168, 169 interatomic distances (in crystals), 110, 491–4 interface junctions, 409–14, 411, 412 internal friction, 327 International Tables for Crystallography arithmetic crystal classes and space groups, 71, 73, 74–6, 77 entry example, 3-D space group, 79–82, 80–1 conventional symbols, 48 interstices in amorphous solids, 124 body-centred cubic crystals, 92–3, 93 cubic close-packed crystals, 89, 90 filled, in compounds, 98, 100, 101, 104 hexagonal close-packed crystals, 91, 92, 92 interstitial defects, 305, 309 configurations, 313–15, 314, 315

Kelly_bindex.indd 514

mobility, 316 interstitial solid solutions, 110–11, 111 intrinsic (single) stacking faults, 280–1, 280–4 invariant planes, 365–6, 371–3 inverse matrices, 445–7 inverse spinel structure, 107 ionic radii, 110, 491–4 isomorphic groups, 79 isotactic polymers, 115 isotropic crystals, 158 elastic properties, 189, 192–3, 256 jogs, 264–5, 265, 289 Kevlar (PPTA), 126, 127 kinks, 264, 297, 297 Kronecker delta, 177, 186, 193, 440 Lamé constants, 192–3, 256 lamellae, twinned crystals, 337–8, 354–5, 355, 356, 357–8 twin boundary surface grooving, 413, 413 lattice parameters, 6, 8–9 derivation of interatomic distances, 110 ratio (axial ratios), 52 of steel (austenite/martensite) phases, 380, 380 lattice points, 5–6, 10 lattices Bravais (space), 26–37, 28, 71–2 cellular material structures, 138–9 definition, formal, 6 plane spacing and direction, 7–11, 9, 10, 442–3, 469–72 vectors and lattice planes, 11–14, 12, 440–2, 441, 475 see also symmetry elements Laue groups, 69, 69, 158, 185 line tension, dislocation loops, 274–7, 275 liquid crystals, 126–9, 128, 130 lithium niobate (LiNbO3), crystal structure, 106 Lomer–Cottrell lock configuration, 286, 286, 299 long-range order (solid solutions), 113, 387

11/30/2011 3:17:13 PM

Index

magnesioferrite (MgFe2O4), 420 martensite (quenched steel), 363, 379–82, 382 martensitic transformation in alloys, 374–83 crystallographic features, 364–6, 365, 367 in metal crystals, 366–74 in nonmetals, 384–5 nucleation and growth of plates, 385–7 massive transformation, 363–4 matrices applications for martensitic lattice transformations, 370 notation for piezoelectric moduli, 178–80 for stiffness and compliance, 184, 188 for twinning index transformations, 341–2 mathematical operations, 443–7 rotation, 21–2, 142, 448 matter tensors, 142, 142 mercury, crystal structure, 94, 94 meshes see nets, two-dimensional; porous solid materials mesogenic units, in polymers, 127 mesophase materials (liquid crystals), 126–9, 128, 130 metallic crystal structures, 86–95 reorientation, in metal working, 228–9, 230–1 Miller index notation, 10, 11, 52, 440, 471–2 Miller–Bravais indices, 56–7, 57, 61 three- to four-index transformation, 57–8, 58 twinning shear transformation, 341 mirror plane, 16, 16, 19, 19, 43–4 related to space groups, 78 related to twinning, 335–6 misfits (interface strain), 421–3, 422, 427–8, 428 mixed dislocations description, for cubic lattice, 243, 243 distortion stresses and strains, 256

Kelly_bindex.indd 515

515

strain energy calculation, 271 mobility, point defects, 308, 308–9, 315–17, 318–21 molecular beam epitaxy (MBE), 423, 424–5 monoclinic crystal system elastic constants, 185 lattice symmetry and unit cells, 27, 29, 29–30, 30 piezoelectric moduli, 179 planar spacing, 470 point group symmetry elements, 63, 63–5 property representation quadric, 159 twin boundary, 406, 407 Morse function, 312 multiplicity, 49–50 nematic phases (liquid crystals), 127–9, 128, 130 nets, two-dimensional consistent with crystal symmetry, 17, 18–19, 19–21 lattice point arrays, 5, 7–8 rectangular, 18–19, 21 stacking, 27, 27, 29, 29–30, 30 Neumann bands, 354 Neumann’s principle, 153–4, 177 nickel arsenide (niccolite), crystal structure, 101–2, 102, 497 titanium (Ni–Ti) alloys, martensitic transformation, 383 noble metals, crystal structure, 86 node, dislocation lines, 247, 285, 285 noncrystallographic symmetry, 136–7 nonprimitive unit cell, 21 nucleation, martensite, 385, 385–7 octahedral interstices, 89, 90, 91, 93 OILS rule (Hutchings), 221–2, 484–6 open forms, 49–50 ordering, in solid solutions, 111–13, 112, 114 orientation distribution function (ODF), 234, 234–5

11/30/2011 3:17:13 PM

516

Index

orthorhombic crystal system elastic constants, 185–6 example of space group description, 79–82, 80–1 lattice symmetry and unit cells, 30–3, 31, 32 piezoelectric moduli, 179 planar spacing and interplanar angles, 470, 472 point group symmetry elements, 49, 49–52, 51 property representation quadric, 158–9 PAA (para-azoxyanisole), 126, 126, 127 packing fraction, 86–7, 124, 126 partial dislocations, 277–9, 279, 343–4 Pearson symbol (crystal structure), 116–17, 119 Peierls dislocation model, 259–61 pencil glide, 205, 208, 215 perovskite crystal structure, 104–5, 105, 133–4, 135 phase boundaries, 420–4, 421, 421 phase transformations, 363–4, 384 see also martensitic transformation piezoelectricity, 177–81, 425 converse effect, 181 plagioclase feldspars, twin structures, 351 plane groups (2-D space groups), 73, 74–6, 77, 77–8 plastic deformation see glide Platonic solids, 131–4, 132 point defects aggregation, 310–11 configurations, 312–17 definition and types, 305 energy characteristics, 305–9 experimental production and studies, 317–21 in ionic crystals (alkali halides), 309–10 produced by radiation, 324–6 in quenched metals, 321–4 symmetry and anelasticity, 326–9 point groups, 43 general and special forms, 49–50 related to space groups, 71–2

Kelly_bindex.indd 516

symmetry elements, 44–8, 46–7 terminology for cubic systems, 53–4 Poisson’s ratio (n), 189, 192, 256 polarization, electrical, 177, 180 pole figures, 229, 232, 232 poles location on stereographic projections, 50–2, 51, 65, 451–5, 452 construction geometry, 458, 458–9, 459, 460 using Wulff net, 460–1, 462, 463 orientation and rolling texture, 232–3, 233 twin growth dislocation, 357, 357 polycrystalline materials, 137, 189, 397 glide deformation, 217–18 grain boundary tensions, 418, 418 texture development, during working, 228–35, 230–1 polyethylene, structure, 115, 116, 117 polygonization, 263 polyhedra, geometry of, 129, 131–4, 132 Voronoi construction, 124–6, 125 polymers, crystal structures, 113, 115, 118, 498 imperfections and amorphous regions, 115, 119 lyotropic and thermotropic liquid crystals, 126, 127 martensitic transformation, 384–5 unit cell, 115, 117 polymorphism (compounds), 86 porous solid materials, 137–8 primary glide plane, 220, 222 primitive unit cell, 6, 21, 440 principal axes and components, symmetric tensors, 149, 169, 170 prismatic dislocation loops, 248–9, 249, 253, 292 projections, geometry of, 451–5, 452, 453 pseudo-twins, in Fe–Be alloys, 353–4, 354 pseudomorphic strained layers, 425–8 pure shear related to simple shear, 489, 489 stresses, 174, 176

11/30/2011 3:17:13 PM

Index

pure strain tensors, 168–9, 169 and independent slip systems, 215–17, 216, 481–3 pyramidal glide, 292–3, 293, 294, 295 quasicrystals, 135–7 quaternion algebra, 22–3, 448–9 quenched metals, 321–4, 363–4 radiation damage, 308, 310, 324–6 radius–normal property, representation ellipsoid, 159, 159–60 random close-packed sphere model (RCPS), 124, 125 rare earth metals crystal structure, 90, 92 ion substitution, in garnets, 108–9 rational indices, law of, 10 rational line/plane, 10 reciprocal lattice vectors, 12, 440–3, 441, 469 reciprocal twins, 340–1 reconstructive transformation, 384 recrystallization, 229, 336 rectangular nets diad axes and mirror planes, 18–19, 21 stacking, and orthorhombic lattices, 31, 32 reflection symmetry, 16, 16, 18–19, 19 reflection (normal, type I) twins, 339–40, 340 relative displacement (strain) tensors, 167, 168–9, 210–11 relaxation time (elastic compliance), 3 27, 328 repeat units (distance), polymers, 115, 116 replacement collisions (point defects), 324 representation quadric, tensors and property measurement radius–normal property, 159, 159–60 representation surfaces, equations, 155–9, 158 representative volume elements, 139 resistivity, quenched metals, 322, 323

Kelly_bindex.indd 517

517

resolved shear stress evaluation, 218, 218–19 largest, associated glide systems, 219–22, 483–5 rhombus nets and unit cells, 31–3, 32 rigidity (shear) modulus, 192, 253, 254 rock salt see sodium chloride rolled metals, crystal orientation (texture), 229, 232, 232–5, 233, 234 rotation (parallel, type II) twins, 340, 340 rotational symmetry, 15–16, 444, 448 combinations, possible, 21–6, 25, 71 and crystallographic point groups, 44–8, 46–7 occurrence in crystal nets, 16–21, 17, 18 in quasicrystals, 135–6 rotoinversion axes, 44, 45, 48 rutile crystal structure, 103–4, 104, 133, 498 sapphire (corundum, a-Al2O3) conditions for glide, 199 crystal structure, 105–6, 106 scalar product mathematical operation, 436–8 scalar triple product, 438–9 and Weiss zone law, 13 Schläfli symbols, 131, 132 Schlegel diagrams, 131–3, 132 Schmid factor, 219, 221–2, 483–4, 485–6 Schoenflies notation, 78–9 Schottky defect, 309–10, 319–21 screw axes (symmetry elements), in space groups, 70, 70–2, 72 screw dislocations atomic positions, 243–4, 244, 245, 258–9 dislocation width, 259, 259, 260 description, for cubic lattice, 241–3, 242 distortion stresses and strains, 253–5, 254, 255 strain energy calculation, 269–70 orthogonal, 264, 264 parallel, 262, 264

11/30/2011 3:17:14 PM

518

Index

second-rank (dyadic) tensors definition and symmetry, 148–9 limitations imposed by crystal symmetry, 153–5, 156 representation surfaces, 155–9, 158 physical properties represented, 141–2, 142 referred to principal axes, 149–52, 150, 169, 173–4 vector components, transformation of, 144–5, 146–8 secondary bonding, in polymers, 115 self-accommodation, martensite variants, 374, 378, 378, 383 self-diffusion, 308–9, 322, 323, 324 semiconductors crystal growth and structure, 424–8 lattice parameters and stiffness constants, 427 shape-memory materials, 363, 383, 386 shear engineering shear strain (g), 165–6, 166, 170 forces, plastic yield (glide) responses, 199–203 modulus (rigidity), 192, 253, 254 pure strain tensor components, 168, 169, 169 resolved shear stress calculation, 218, 218–19 simple and pure, compared, 488–9, 489 stress components (s), 170, 172–3, 175, 176 and twinning mechanism, 336–9, 337, 338 shear magnitude, s, 338–9, 352–3 sheet textures, 232–5, 233, 234 Shockley partials compared with Frank partials, 281–3 separation and stacking fault energy, 278–9, 279, 280, 281 short-range order (solid solutions), 113 shuffle (atomic displacement), 346, 353 silicon stacking faults and dislocations, 297, 299, 299

Kelly_bindex.indd 518

states and properties, 124, 138 silver, rolled (crystal orientation), 234, 234 slip see glide slip lines (bands), observation of, 200–1, 202, 202, 262 smectic phases (liquid crystals), 127, 128, 129 soaps, 127 sodium chloride (rock salt, halite) crystal structure, 98–9, 99, 495–6 and discovery of glide, 200 dislocation geometry, 288–90, 289 glide planes and directions, 204–5 Schottky defects, 309–10, 319–21 vacancies, ionic displacement, 313, 313 solid solutions, 110–13, 111, 112, 114 see also alloys, metallic space charge regions, rock salt, 289–90, 290, 309 space groups, 69–78 three-dimensional, example, 79–82, 80–1 two-dimensional (plane) groups, 73, 74–6, 77, 77–8 space lattices see Bravais lattices sphalerite (zinc blende, a-ZnS) crystal structure, 100, 100–1, 497 dislocations, 297–8, 298, 299 piezoelectricity, 180 plane stacking sequence, 95, 96 twin structures, 344, 344–5 spheres see close packing spinel crystal structure, 106–7, 107 stacking faults, 278–9, 279, 336 see also dislocations stair rod dislocations, 286, 286–7, 299 steel, martensitic transformation, 363, 379–82, 380, 382 nucleation and growth of plates, 386–7 stereograms construction general diagrams and triclinic application, 65–7, 66 hexagonal system, 58–9, 59 monoclinic system, axis setting conventions, 63, 63–4, 64

11/30/2011 3:17:14 PM

Index

orthorhombic system example, 50–2, 51 pole opposites and angles, 458–60 small circle, 455–8, 456, 457 Wulff net graphical aid, 460–3 conventional symbols, 44–5, 45, 48 of crystallographic point groups, 46–7, 48 glide system depiction, 219–22, 220, 221 projection geometry, 451–5, 453 properties, proof of, 465–7, 466, 467 stiffness constants, 182–4, 188, 190 strain anelastic, 326–7, 329 definitions, 165–6, 166 elastic, produced by applied stress, 181, 182, 183 energy, stored in dislocation, 269–72, 270 homogeneous, 166, 200, 208–9, 328 infinitesimal, 166–70 in martensite plates and lattices, 365–6 combined with rotation, 372–4, 373, 375 pure and observed lattice strains, 370–2, 371, 372 in multiple twinning, 357 strained layer epitaxy, 424–8, 425 stress calculation, 172, 172–3 chemical (in dislocation), 252–3 components, definition and notation, 170–2, 171, 174, 175, 176 contracted notation, 178, 182–3 hydrostatic and deviatoric, 176 fields, on intersecting dislocations, 264, 278 homogeneous, 174 pure shear, 174–5, 175 related to strain (Hooke’s law), 181–2, 254–5 Strukturbericht designation (crystal structure), 116–17, 119 subgroups, 79 substitution of cations, in garnet structures, 108–9 of metals, in solid solutions, 110–11, 111

Kelly_bindex.indd 519

519

superconducting materials, crystal structures, 105 superelasticity, 378, 383 supergroups, 79 superlattices, 112–13, 114, 114 surface free energy, 394, 396 at interface junctions, 409–11, 410 measurement, 394–7, 395 related to equilibrium crystal shape (Wulff theorem), 414–16, 415 and twin boundaries, 413–14, 414 surfaces atomic bonding and energy plots, 392–4, 393, 394 interfacial simulation, 406–8 definition and alternative structures, 391–2, 392 growth rates, 417–18 outer, reconstruction, 391 see also grain boundaries symmetric tensors, 148–9, 154–5 symmetry elements crystals, macroscopic level, 3, 43–8 of defects, 328–9 groups, subgroups and supergroups, 79 limitations on crystal physical properties, 153–5, 156 notation and nomenclature, 78–9 operation types, 14–16, 43–4 restrictions, in crystals, 16–21, 17 slip system families, 203–5 space group descriptions, 69–78 syndiotactic polymers, 115 tactic polymers, 115 tensile strains, 169, 192, 326 tension dislocation line, 274–7, 275 and glide, in metal crystals, 222–6, 223, 225 tensors principal axes and components, 149 transformation operations, 142–5, 144–5 types and ranks, 141–2, 161, 167, 177 see also second-rank tensors

11/30/2011 3:17:14 PM

520

Index

tetrad (four-fold) axis of symmetry, 18, 20 tetragonal crystal system, 28, 30 elastic constants, 189 planar spacing, 471 point group symmetry elements, 52–3 tetrahedral interstices, 89, 90, 91, 92–3 texture, 228–9, 230–1, 232–5 thermal faceting, 416–17, 417 thermoelastic martensite, 386 Thompson’s tetrahedron, 282, 282–4, 288 tilt boundaries asymmetrical, 401–3, 402 rotated (twist), 403, 403–5 symmetrical, 397–401, 398, 401 tin (a- and b-Sn), crystal structures, 94–5 titanium dioxide (rutile), crystal structure, 103–4, 104, 133 martensitic transformation, metal and alloys, 369, 374, 375, 383 topologically close-packed (TCP) structures, 135, 136 torque terms, grain interface junctions, 410–11, 411, 413 transformation formula (tensor components), 148, 152, 154, 170 transformation toughening, 384 translation glide, 199–203, 200 translational symmetry, 6, 15, 43 combined with rotation/inversion (space groups), 69–78 triad (three-fold) axis of symmetry, 18, 20–1 triclinic crystal system, 27, 28 elastic constants, 184–5 planar spacing, 470 point group symmetry elements, 65–7, 66 property representation quadric, 159 trigonal crystal system lattice symmetry and unit cells, 26, 33, 33–5, 34 planar spacing, 471 point group symmetry elements, 59–62, 60 special forms, 62, 62

Kelly_bindex.indd 520

use of rhombohedral/hexagonal axes, 60–2, 71, 477–9, 478 tungsten, elastic isotropy, 256 twinned crystals crystal morphology, 354–8 geometric elements, 339, 339–42, 347–8, 350–4 martensitic lamellae, 376–8, 377 occurrence and causes, 335, 336–7 structure, examples of, 342–6, 349–50 twist boundaries, 403, 403–5 two-surface analysis, 201, 464–5, 465 unit cells, 3–7 of cellular solid materials, 139 conventional, in crystal systems, 26, 26 electron density, 85 of ordered solid solutions, 112, 112 rhombohedral and hexagonal, in trigonal crystals, 60, 60–2, 61, 71, 477–9 of tactic polymers, 115, 117 transformation of indices (directions and planes), 473–5 unit parallelogram, 5 unit quaternions, 22–3, 449 uranium, twinning, 340–1 vacancies, 305 binding energy, 310–11 configuration models, 312–13, 313, 313 and dislocation forces, 252–3 dislocation loops, in hexagonal metals, 292, 292 formation energy calculation, 307 positions and generation, 306–7, 307 related to electrical charge, 289–90, 290 vapour deposition, 229, 336, 423 vectors definition and components, 435–6, 436 director, in liquid crystal alignment, 127, 129 lattice translation, 15 related to crystal lattice planes, 11–14, 440–3, 441 scalar product, 436–8

11/30/2011 3:17:14 PM

Index

transformation of components, 142–4, 143, 146 dummy suffix notation, 145–6 vector product operations, 438–40, 439 triple product formula, 226, 439 von Mises condition, 217 Voronoi polyhedra, 124–6, 125 wavy glide, 205, 208, 215 Weaire–Phelan structure, 418, 419 Weiss zone law, 11–14, 62 white tin (b-Sn), crystal structure, 94–5 Wulff net, 460–1, 461, 462, 463 Wulff plot, crystal/grain shape, 414–17, 415 wurtzite (b-ZnS)

Kelly_bindex.indd 521

521

crystal structure, 100, 101, 101, 497 surfaces, 392, 392 stacking faults and dislocations, 299 Young’s modulus (E), 189, 192, 427 zeolites, 137, 138 zinc, twinning, 346, 349 zinc-blende see sphalerite zirconium martensitic transformations, 369–74, 375 oxide (zirconia), transformation toughening, 384 twinning, 346, 349 zone addition rule, 14, 51–2 zones, of crystal lattice planes, 12–14

11/30/2011 3:17:14 PM

Our partners will collect data and use cookies for ad personalization and measurement. Learn how we and our ad partner Google, collect and use data. Agree & close